T
KINETICS OF MATERIALS
Samuel M. Allen
Robert W. Balluffi
W. Craig Carter
W i t h Editorial Assistance from Rach...
185 downloads
1463 Views
31MB Size
Report
This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!
Report copyright / DMCA form
T
KINETICS OF MATERIALS
Samuel M. Allen
Robert W. Balluffi
W. Craig Carter
W i t h Editorial Assistance from Rachel A. Kemper
Department of Materials Science and Engineering Massachusetts Institute of Tech nology Cambridge, Massachusetts
WILEYINTERSCIENCE A JOHN WILEY & SONS, INC., PUBLICATION
Copyright @ 2005 by John Wiley & Sons, Inc. All rights reserved. Published by John Wiley & Sons, Inc., Hoboken, New Jersey. Published simultaneously in Canada. No part of this publication may be reproduced, stored in a retrieval system, or transmitted in any form or by any means, electronic, mechanical, photocopying, recording, scanning, or otherwise, except as permitted under Section 107 or 108 of the 1976 United States Copyright Act, without either the prior written permission of t h e Publisher, or authorization through payment of the appropriate percopy fee to the Copyright Clearance Center, Inc., 222 Rosewood Drive, Danvers, MA 01923, (978) 7508400, fax (978) 6468600, or on the web a t www.copyright.com. Requests to t h e Publisher for permission should be addressed to the Permissions Department, John Wiley & Sons, Inc., 111 River Street, Hoboken, NJ 07030, (201) 7486011, fax (201) 7486008. Limit of Liability/Disclaimer of Warranty: While the publisher and author have used their best efforts in preparing this book, they make no representations or warranties with respect t o the accuracy or completeness of the contents of this book and specifically disclaim any implied warranties of merchantability or fitness for a particular purpose. N o warranty may be created ore extended by sales representatives or written sales materials. The advice and strategies contained herin may not be suitable for your situation. You should consult with a professional where appropriate. Neither the publisher nor author shall be liable for any loss of profit or any other commercial damages, including but not limited t o special, incidental, consequential, or other damages. For general information on our other products and services please contact our Customer Care Department with the U.S. a t 8777622974, outside t h e U.S. a t 3175723993 or fax 3175724002. Wiley also publishes its books in a variety of electronic formats. Some content that appears in print, however, may not be available in electronic format. Library of Congress CataloginginPublication Data: Balluffi, Robert W . , 1924Kinetics of Materials / Robert W . Balluffi, Samuel M. Allen, W . Craig Cart,er; edited by Rachel A. Kemper; p. cm. Includes bibliographical references and index. ISBN 13 9780471246893 ISBN10 0471246891 1.MaterialsMechanical Properties. 2 . Materials science
I. Allen, Samuel M. 11. Carter, W . Craig. 111. Kemper, Rachel A. IV. Title. TA404.8.B35 2005 620.1' 1292dc22 2005047793 Printed in the United States of America. 10 9 8 7 6 5 4 3 2
CONTENTS
Preface
xvii
Acknowledgments
xix
Notation
xx
SymbolsRoman
xxi
SymbolsGreek
xxv
1 Introduction 1.1 Thermodynamics and Kinetics 1.1.1 Classical Thermodynamics and Constructions of Kinetic Theories 1.1.2 Averaging 1.2 Irreversible Thermodynamics and Kinetics 1.3 Mathematical Background 1.3.1 Fields 1.3.2 Variations 1.3.3 Continuum Limits and Coarse Graining 1.3.4 Fluxes 1.3.5 Accumulation 1.3.6 Conserved and Nonconserved Quantities 1.3.7 Matrices, Tensors, and the Eigensystem Bibliography Exercises
1
2 2 4 5 7 7 7
8 10 11 12 13 16 16 V
Vi
CONTENTS
PART I
M O T I O N OF ATOMS A N D MOLECULES BY DIFFUSION
2 Irreversible Thermodynamics: Coupled Forces and Fluxes Entropy and Entropy Production 2.1.1 Entropy Production 2.1.2 Conjugate Forces and Fluxes 2.1.3 Basic Postulate of Irreversible Thermodynamics 2.2 Linear Irreversible Thermodynamics 2.2.1 General Coupling between Forces and Fluxes 2.2.2 ForceFlux Relations when Extensive Quantities are Constrained 2.2.3 Introduction of the Diffusion Potential 2.2.4 Onsager’s Symmetry Principle Bibliography Exercises
23 25 27 27 28 28
Driving Forces and Fluxes for Diffusion
41
3.1
41 42
2.1
3
23
Concentration Gradients and Diffusion 3.1.1 SelfDiffusion: Diffusion in the Absence of Chemical Effects 3.1.2 SelfDiffusion of Component i in a Chemically Homogeneous Binary Solution 3.1.3 Diffusion of Substitutional Particles in a Chemical Concentration Gradient 3.1.4 Diffusion of Interstitial Particles in a Chemical Concentration Gradient 3.1.5 On the Algebraic Signs of Diffusivities 3.1.6 Summary of Diffusivities 3.2 Electrical Potential Gradients and Diffusion 3.2.1 Charged Ions in Ionic Conductors 3.2.2 Electromigration in Metals 3.3 Thermal Gradients and Diffusion 3.4 Capillarity and Diffusion 3.4.1 The Flux Equation and Diffusion Equation 3.4.2 Boundary Conditions 3.5 Stress and Diffusion 3.5.1 Effect of Stress on Mobilities 3.5.2 Stress as a Driving Force for Diffusion: Formation of SoluteAtom Atmosphere around Dislocations 3.5.3 Influence of Stress on the Boundary Conditions for Diffusion: Diffusional Creep 3.5.4 Summary of Diffusion Potentials Bibliography
30 32 33 35 36
44 44 52 53 53 54 55 55 56 57 58 61 61 61 62 64 66 67
CONTENTS
Exercises 4 The Diffusion Equation
4.1
Fick’s Second Law 4.1.1 Linearization of the Diffusion Equation 4.1.2 Relation of Fick’s Second Law to the Heat Equation 4.1.3 Variational Interpretation of the Diffusion Equation 4.2 Constant Diffusivity 4.2.1 Geometrical Interpretation of the Diffusion Equation when Diffusivity is Constant 4.2.2 Scaling of the Diffusion Equation 4.2.3 Superposition 4.3 Diffusivity as a Function of Concentration 4.4 Diffusivity as a Function of Time 4.5 Diffusivity as a Function of Direction Bibliography Exercises
5 Solutions t o the Diffusion Equation 5.1
SteadyState Solutions 5.1.1 One Dimension 5.1.2 Cylindrical Shell 5.1.3 Spherical Shell 5.1.4 Variable Diffusivity 5.2 NonSteady St ate Diffusion 5.2.1 Instantaneous Localized Sources in Infinite Media 5.2.2 Solutions Involving the Error Function 5.2.3 Method of Superposition 5.2.4 Method of Separation of Variables: Diffusion on a Finite Domain 5.2.5 Method of Laplace Transforms 5.2.6 Estimating the Diffusion Depth and Time to Approach Steady State Bibliography Exercises
6 Diffusion in Multicomponent Systems 6.1 6.2
General Formulation Solving the Diffusion Equations 6.2.1 Constant Diffusivities 6.2.2 ConcentrationDependent Diffusivities
vii
68
77 77 78 79 80 81 81 81 83 85 87 88 91 91 99
100 100 101 102 102 103 103 105 107 107 110 113 114 114
131 131 134 135 139
viii
CONTENTS
6.3 Measurement of Diffusivities Bibliography Exercises
7 Atomic Models for Diffusion 7.1
Thermally Activated Atomic Jumping 7.1.1 OneParticle Model with Square PotentialEnergy Wells 7.1.2 OneParticle Model with Parabolic PotentialEnergy Wells 7.1.3 ManyBody Model 7.2 Diffusion as a Series of Discrete Jumps 7.2.1 Relation of Diffusivity to the MeanSquare Particle Displacement 7.2.2 Diffusion and Random Walks 7.2.3 Diffusion with Correlated Jumps Bibliography Exercises
8 Diffusion in Crystals
8.1
Atomic Mechanisms 8.1.1 Ring Mechanism 8.1.2 Vacancy Mechanism 8.1.3 Interstitialcy Mechanism 8.1.4 Interstitial Mechanism 8.1.5 Diffusion Mechanisms in Various Materials 8.2 Atomic Models for Diffusivities 8.2.1 Metals 8.2.2 Ionic Solids 8.3 Diffusional Anelasticity (Internal Friction) 8.3.1 Anelasticity due to Reorientation of Anisotropic Point Defects 8.3.2 Determination of Diffusivities Bibliography Exercises
9 Diffusion along Crystal Imperfections 9.1 9.2
The Diffusion Spectrum Grain Boundaries 9.2.1 Regimes of GrainBoundary Shortcircuit Diffusion in a Polycryst a1 9.2.2 Analysis of Diffusion in the A, B, and C Regimes 9.2.3 Mechanism of Fast GrainBoundary Diffusion
141 141 141
145
145 146 148 149 154 155 156 158 158 159
163 163 164 164 165 167 167 169 169 177 183 183 189 189 190
209 209 214 214 218 221
CONTENTS
9.3 Dislocations 9.4 Free Surfaces Bibliography Exercises 10 Diffusion in Noncrystalline Materials
10.1 FreeVolume Model for Liquids 10.2 Diffusion in Amorphous Metals 10.2.1 SelfDiffusion 10.2.2 Diffusion of Small Interstitial Solute Atoms 10.3 Small Atoms (Molecules) in Glassy Polymers 10.4 Alkali Ions in Network Oxide Glasses 10.5 Diffusion of Polymer Chains 10.5.1 Structure of Polymer Chains 10.5.2 Diffusion of Isolated Polymer Chains in Dilute Solutions 10.5.3 Diffusion of Densely Entangled Polymer Chains by Reptation Bibliography PART I1
ix
222 223 224 225 229
229 232 232 234 239 240 241 241 243 245 247
M O T I O N OF DISLOCATIONS A N D INTERFACES
11 Motion of Dislocations 11.1 Glide and Climb 11.2 Driving Forces on Dislocations 11.2.1 Mechanical Force 11.2.2 Osmotic Force 11.2.3 Curvature Force 11.2.4 Total Driving Force on a Dislocation 11.3 Dislocation Glide 11.3.1 Glide in Perfect Single Crystals 11.3.2 Glide in Imperfect Crystals Containing Various Obstacles 11.3.3 Some Experimental Observations 11.3.4 Supersonic Glide Motion 11.3.5 Contributions of Dislocation Motion to Anelastic Behavior 11.4 Dislocation Climb 11.4.1 DiffusionLimited vs. SourceLimited Climb Kinetics 11.4.2 Experimental Observations 11.4.3 Analyses of Two Climb Problems Bibliography Exercises 12 Motion of Crystalline Surfaces
12.1 Thermodynamics of Interface Motion
253
253 255 255 256 257 258 258 258 263 264 265 266 266 267 269 269 274 275 285
285
X
CONTENTS
12.2 Motion of Crystal/Vapor Interfaces 12.2.1 Structure of Crystal/Vapor Surfaces 12.2.2 Crystal Growth from a Supersaturated Vapor 12.2.3 Surfaces as Sinks for Supersaturated Lattice Vacancies 12.3 Interface Motion during Solidification 12.3.1 Structure of Crystal/Liquid Interfaces 12.3.2 Crystal Growth from an Undercooled Liquid Bibliography Exercises 13 Motion of Crystalline Interfaces
13.1 Thermodynamics of Crystalline Interface Motion 13.2 Conservative and Nonconservative Motion 13.3 Conservative Motion 13.3.1 Glissile Motion of Sharp Interfaces by Interfacial Dislocation Glide 13.3.2 Thermally Activated Motion of Sharp Interfaces by Glide and Climb of Interfacial Dislocations 13.3.3 Thermally Activated Motion of Sharp Interfaces by Atom Shuffling 13.3.4 Thermally Activated Motion of Diffuse Interfaces by SelfDiffusion 13.3.5 Impediments to Conservative Interface Motion 13.3.6 Observations of Thermally Activated GrainBoundary Motion 13.4 Nonconservative Motion 13.4.1 Source Action of Sharp Interfaces 13.4.2 DiffusionLimited Vs. SourceLimited Kinetics Bibliography Exercises PART Ill
286 287 288 291 292 292 292 294 295 303
303 304 305 305 308 311 312 312 315 317 317 321 324 325
MORPHOLOGICAL EVOLUTION D U E TO CAPILLARY A N D APPLIED MECHANICAL FORCES
14 Surface Evolution due to Capillary Forces
14.1 Isotropic Surfaces 14.1.1 Flattening of Free Surfaces by Surface Diffusion 14.1.2 Surface Evolution by Vapor Transport 14.1.3 Evolution of Perturbed Cylinder by Vapor Transport 14.1.4 Evolution of Perturbed Cylinder by Surface Diffusion 14.1.5 Thermodynamic and Kinetic Morphological Wavelengths 14.2 Anisotropic Surfaces
337
338 338 341 345 345 346 346
CONTENTS
14.2.1 Some Geometrical Aspects of Anisotropic Surfaces 14.2.2 Rate of Morphological Interface Evolution Bibliography Exercises 15 Coarsening due to Capillary Forces
15.1 Coarsening of Particle Distributions 15.1.1 Classical MeanField Theory of Coarsening 15.1.2 Beyond the Classical MeanField Theory of Coarsening 15.2 Grain Growth 15.2.1 Grain Growth in Two Dimensions 15.2.2 Grain Growth in Three Dimensions Bibliography Exercises 16 Morphological Evolution: Diffusional Creep, and Sintering
16.1 Morphological Evolution for Simple Geometries 16.1.1 Evolution of Bamboo Wire via GrainBoundary Diffusion 16.1.2 Evolution of a Bundle of Parallel Wires via GrainBoundary Diffusion 16.1.3 Evolution of Bamboo Wire by Bulk Diffusion 16.1.4 Neck Growth between Two Spherical Particles via Surface Diffusion 16.2 Diffusional Creep 16.2.1 Diffusional Creep of TwoDimensional Polycrystals 16.2.2 Diffusional Creep of ThreeDimensional Polycrystals 16.3 Sintering 16.3.1 Sintering Mechanisms 16.3.2 Sintering Microstructures 16.3.3 Model Sintering Experiments 16.3.4 Scaling Laws for Sintering 16.3.5 Sintering Mechanisms Maps Bibliography Exercises PART IV
346 350 353 354 363
363 363 371 373 373 379 382 384 387
388 389 39 1 392 394 395 395 398 400 400 40 1 403 403 405 406 408
PHASE TRANSFORMATIONS
17 General Features of Phase Transformations
17.1 Order 17.1.1 17.1.2 17.2 Molar
xi
Parameters OneComponent or Fixed Stoichiometry Systems TwoComponent Systems FreeEnergy Changes
419
420 420 423 428
xii
CONTENTS
17.3 Continuous and Discontinuous Transformations Bibliography
18 Spinodal and OrderDisorder Transformations 18.1 Interdiffusivity a t Unstable Compositions 18.2 Diffuse Interface Theory 18.2.1 Free Energy of an Inhomogeneous System 18.2.2 Structure and Energy of Diffuse Interfaces 18.2.3 Diffusion Potential for Transformation 18.3 Evolution Equations for Order Parameters 18.3.1 CahnHilliard Equation 18.3.2 AllenCahn Equation 18.3.3 Numerical Simulation and the PhaseField Method 18.4 Decomposition and OrderDisorder: Initial Stages 18.4.1 CahnHilliard: Critical and Kinetic Wavelengths 18.4.2 AllenCahn: Critical Wavelength 18.5 CoherencyStrain Effects 18.5.1 Generalizations of the CahnHilliard and AllenCahn Equations 18.5.2 Diffraction and the CahnHilliard Equation Bibliography Exercises 19 Nucleation
19.1 Homogeneous Nucleation 19.1.1 Classical Theory of Nucleation in a OneComponent System without Strain Energy 19.1.2 Classical Theory of Nucleation in a TwoComponent System without Strain Energy 19.1.3 Effect of Elastic Strain Energy 19.1.4 Nucleus Shape of Minimum Energy 19.1.5 More Complete Expressions for the Classical Nucleation Rate 19.1.6 Nonclassical Models for the Critical Nucleus 19.1.7 Discussion 19.2 Heterogeneous Nucleation 19.2.1 Nucleation on Grain Boundaries, Grain Edges, and Grain Corners 19.2.2 Nucleation on Dislocations Bibliography Exercises
430 431 433
433 435 436 437 439 440 440 44 1 441 443 443 444 445 448 450 45 1 452 459
460 460 468 468 473 474 476 476 477 477 48 1 484 485
CONTENTS
20 Growth of Phases in Concentration and Thermal Fields
20.1 Growth of Planar Layers 20.1.1 Heat ConductionLimited Growth 20.1.2 DiffusionLimited Growth 20.1.3 Growth Limited by Heat Conduction and Mass Diffusion Simultaneously 20.1.4 Interface SourceLimited Growth 20.2 Growth of articles 20.2.1 DiffusionLimited Growth 20.2.2 Interface SourceLimited Growth 20.3 Morphological Stability of Moving Interfaces 20.3.1 Stability of Liquid/Solid Interface during Solidification of a Unary System 20.3.2 Stability of a l p Interface during DiffusionLimited Particle Growth 20.3.3 Stability of Liquid/Solid Interface during Binary Alloy Solidification 20.3.4 Analyses of Interfacial Stability Bibliography Exercises 21 Concurrent Nucleation and Growth
21.1 Overall Rate of Discontinuous Transformation 21.1.1 TimeCone Analysis of Concurrent Nucleation and Growth 21.1.2 Transformations near the Edge of a Thin SemiInfinite Plate 21.2 TimeTemperatureTransformation (TTT) Diagrams Bibliography Exercises 22 Solidification
22.1 OneDimensional Solidification 22.1.1 Scheil Equation 22.1.2 Zone Melting and Zone Leveling 22.2 Cellular and Dendritic Solidification 22.2.1 Formation of Cells and Dendrites 22.2.2 Solute Segregation during Dendritic Solidification 22.3 Structure of Castings and Ingots Bibliography Exercises 23 Precipitation
xiii
501
502 502 504 508 510 512 512 514 515 516 518 518 519 524 526 533
533 534 537 538 540 540 543
543 543 546 547 547 548 549 550 550 555
xiv
CONTENTS
23.1 23.2 23.3 23.4
General Features Nucleus Morphology and Energy Coherency Loss during Growth Two Example Systems 23.4.1 CuCo System 23.4.2 A1Cu System Bibliography 24 Martensitic Transformations
24.1 General Features 24.2 Crystallography 24.2.1 Lattice Deformation 24.2.2 Undistorted Plane by Application of Additional LatticeInvariant Deformation 24.2.3 Invariant Plane by Addition of RigidBody Rotation 24.2.4 Tensor Analysis of the Crystallographic Problem 24.2.5 Further Aspects of the Crystallographic Model 24.3 Glissile Interface 24.4 Nucleation of Martensite 24.5 Examples of Martensitic Transformations 24.5.1 InT1 System 24.5.2 FeNi System 24.5.3 FeNiC System Bibliography Exercises Appendix A: Densities, Fractions, and Atomic Volumes of Components
A. 1 Concentration Variables A.1.1 Mass Density A.1.2 Mass Fraction A.1.3 Number Density or Concentration A.1.4 Number, Mole, or Atom Fraction A.1.5 Site Fraction A.2 Atomic Volume Appendix B: Structure of Crystalline Interfaces
B.l B.2 B.3 B.4 B.5
Geometrical Degrees of Freedom Sharp and Diffuse Interfaces Singular, Vicinal, and General Interfaces Homophase and Heterophase Interfaces Grain Boundaries
555 556 557 558 558 560 561 563 563 565 565 567 570 571 571 572 574 575 575 578 579 580 581 587
587 587 588 588 588 588 588 591 591 592 593 595 596
CONTENTS
B.6 Coherent, Semicoherent, and Incoherent Interfaces B.7 Line Defects in Crystal/Crystal Interfaces Bibliography
XV
597 599 600
Appendix C: Capillarity and Mathematics of Space Curves and Interfaces 601
C.l
Specification of Space Curves and Interfaces C . l . l Space Curves C.1.2 Interfaces C.2 Isotropic Interfaces and Mean Curvature C.2.1 Implications of Mean Curvature (3.3 Anisotropic Interfaces and Weighted Mean Curvature (3.3.1 Geometric Constructions for Anisotropic Surface Energies (2.3.2 Implications of Weighted Mean Curvature (2.4 Equilibrium at a Curved Interface C.4.1 GibbsThomson Equation C.4.2 Equilibrium Solubilities of Small DispersedPhase Particles Bibliography Illustration Credits Cited Author Index Figure Index Topic Index
601 60 1 603 605 605 608 608 610 611 611 612 615 617 620 623 639
PREFACE
This textbook has evolved from part of the firstyear graduate curriculum in the Department of Materials Science and Engineering at the Massachusetts Institute of Technology (MIT). This curriculum includes four required semesterlong subjects“Materials at Equilibrium,” “Mechanical Properties of Materials,” “Electrical, Optical, and Magnetic Properties of Materials,” and “Kinetic Processes in Materials.” Together, these subjects introduce the essential building blocks of materials science and engineering at the beginning of graduate work and establish a foundation for more specialized topics. Because the entire scope of kinetics of materials is far too great for a semesterlength class or a textbook of reasonable length, we cover a range of selected topics representing the basic processes which bring about changes in the size, shape, composition, and atomistic structures of materials. The subject matter was selected with the criterion that structure is allimportant in determining the properties (and applications) of materials. Topics concerned with fluid flow and kinetics, which are often important in the processing of materials, have not been included and may be found in standard texts such as those by Bird, Stewart, and Lightfoot [l]and Poirier and Geiger [2]. The major topics included in this book are:
I. Motion of atoms and molecules by diffusion 11. Motion of dislocations and interfaces 111. Morphological evolution due to capillary and applied mechanical forces IV. Phase transformations xvii
xviii
PREFACE
The various topics are generally introduced in order of increasing complexity. The text starts with diffusion, a description of the elementary manner in which atoms and molecules move around in solids and liquids. Next, the progressively more complex problems of describing the motion of dislocations and interfaces are addressed. Finally, treatments of still more complex kinetic phenomenasuch as morphological evolution and phase transformationsare given, based to a large extent on topics treated in the earlier parts of the text. The diffusional transport essential to many of these phenomena is driven by a wide variety of forces. The concept of a basic diffusion potential, which encompasses all of these forces, is therefore introduced early on and then used systematically in the analysis of the many kinetic processes that are considered. We have striven to develop the subject in a systematic manner designed to provide readers with an appreciation of its analytic foundations and, in many cases, the approximations commonly employed in the field. We provide many extensive derivations of important results to help remove any mystery about their origins. Most attention is paid throughout to kinetic phenomena in crystalline materials; this reflects the interests and biases of the authors. However, selected phenomena in noncrystalline materials are also discussed and, in many cases, the principles involved apply across the board. We hope that with the knowledge gained from this book, students will be equipped to tackle topics that we have not addressed. The book therefore fills a significant gap, as no other currently available text covers a similarly wide range of topics. The prerequisites for effective use of this book are a typical undergraduate knowledge of the structure of materials (including crystal imperfections), vector calculus and differential equations, elementary elasticity theory, and a somewhat deeper knowledge of classical thermodynamics and statistical mechanics. At MIT the latter prerequisite is met by requiring students to take “Materials at Equilibrium” before tackling “Kinetic Processes in Materials.” To facilitate acquisition of prerequisites, we have included important background material in abbreviated form in Appendices. We have provided a list of our most frequently used symbols, which we have tried to keep in correspondence with general usage in the field. Also included are many exercises (with solutions) that amplify and extend the text. Bibliography 1. B.R. Bird, W.E. Stewart, and N. Lightfoot. Transport Phenomena. John Wiley & Sons, New York, 2nd edition, 2002.
2. D.R. Poirier and G.H. Geiger. Transport Phenomena in Materials Processing. The Minerals, Metals and Materials Society, Warrendale, PA, 1994.
xix
ACKNOWLEDGMENTS
We wish to acknowledge generous assistance from many friends and colleagues, especially Dr. John W. Cahn, Dr. Rowland M. Cannon, Prof. Adrian P. Sutton, Prof. Kenneth C. Russell, Prof. Donald R. Sadoway, Dr. Dominique Chatain, Prof. David N. Seidman, and Prof. Krystyn J. Van Vliet. Prof. David T . Wu graciously provided an unpublished draft of his theoretical developments in threedimensional grain growth which we have incorporated into Chapter 15. We frequently consulted Prof. Paul Shewmon’s valuable textbooks on diffusion, and he kindly gave us permission to adapt and reprint Exercise 3.4. Scores of students have used draft versions of this book in their study of kinetics and many have provided thoughtful criticism that has been valuable in making improvements. Particular thanks are due Catherine M. Bishop, Valerie LeBlanc, Nicolas Mounet, Gilbert Nessim, Nathaniel J . Quitoriano, Joel C. Williams, and Yi Zhang for their careful reading and suggestions. Ellen J. Siem provided illustrations from her Surface Evolver calculations. Scanning electron microscopy expertise was contributed by Jorge Feuchtwanger. Professors Alex King and HansEckart Exner and Dr. Markus Doblinger furnished unpublished micrographs. Angela M. Locknar expended considerable effort securing hardtolocate bibliographic sources. Andrew Standeven’s care in drafting the bulk of the illustrations is appreciated. Jenna Picceri’s and Geraldine Sarno’s proofreading skills and work on gathering permissions are gratefully acknowledged. Finally, we wish to thank our editor, Rachel A. Kemper, for her invaluable assistance at all stages of the preparation of this work. We are fortunate to have so many friends and colleagues who donated their time to help us correct and clarify the text. Although we have striven to remove them all, the remaining errors are the responsibility of the authors. This textbook has evolved over eight years, during which our extended families have provided support, patience, indulgence, and sympathy. We thank you with all of our hearts.
xx
NOTAT I 0N
Not at ion ~
Definition ~~~
~
~
a'
Vector a, the column vector a'
d
Unit vector a
A, [Aajl A
Matrix A, matrix A in component form
a'. b'
Scalar, inner or dot product of a' and
ZXb'
Vector, outer or cross product of a' and
a'T,
AT
Tensor A of rank two or greater
Transpose of a' or
b' b'
A
A, A,a
Total amount of A, amount of A per mole or per atom as deduced from context, density of A
(a)
Average value of a
Va
Gradient of scalar field a
V.A'
Divergence of vector field
A'
V . V a 3 V 2 a Laplacian of scalar field a
#j
6ij
Kronecker delta, S i j = 1 for i = j ; dij = 0 if i
L{a} or d
Laplace transform of a
Car,
KrogerVink notation for Ca on Ksite with positive effective charge
vx,
KrogerVink notation for vacancy on Agsite with negative effective charge
s:
KrogerVink notation for S on Osite with zero effective charge
xxi
SY MBOLSROMAN
Symbol
Definition
Units
A
Area
m2
a , b, c
Lattice constants
m
g, b
Burgers vector, magnitude of Burgers vector
m
b’
Specific magnetic moment
A ml
C , Ci
Concentration of molecules or atoms, concentration of species i
m3, d = 3 m2, d = 2 ml, d = 1
D, D
Mass diffusivity, diffusivity tensor
m2 sl
DxL
Bulk diffusivity in crystalline material free of line or planar imperfections
m2 sl
DB
Boundary diffusivity
m2 sl
DD
Dislocation diffusivity
m2 sl
DL
Liquid diffusivity
m2 sl
DS
Surface diffusivity
m2 sl
D
Chemical interdiffusivity

~
m2 sl ~
*D
Selfdiffusivity in pure material
m2 sl
*Di
Selfdiffusivity of component i in mult icomponent system
m2 sl
Di
Intrinsic diffusivity of component i in multicomponent system
m2 sl
d
Spatial dimensionality

E
Activation energy
J atom’
E
Young’s elastic modulus
P a = J m3
I3
Electric field vector
f
V ml ~~~
Correlation factor for atomic jumps in diffusion
~

xxii
SYMBOLSROMAN
SYMBOLSROMAN
Symbol
Definition
Units
F ,F , f
Helmholtz energy, Helmholtz energy per mole (or particle), Helmholtz energy density
J, J moll, J m3
Force, force per unit length
N, Nml
6, G, g
Gibbs energy, Gibbs energy per mole (or particle), Gibbs energy density
J, J moll, J m3
7f, H , h
Enthalpy, enthalpy per mole (or particle), enthalpy density
J, Jmoll, Jm3
h
Planck constant
6.626 x 1034 J s
14,Ii
Current of electrical charge, current of species i
c s1,
Unit vectors parallel to Cartesian coordinates 2,y, z
m2
J
Flux, flux of species i Nucleation rate
K
Thermal conductivity
J
K
Rate constant
various
k
Boltzmann constant
1.38 x ~ o  ~ ~ J K  ~
Lap
Onsager coupling coefficient (or tensor)
m2
M,M
Mobility, mobility tensor
various
M ,O
Atomic or molecular weight of species i
kg N;'
m
Mass Number
$7
s
i, j , I
f,$
N
N
Total number of atoms or molecules in subsystem
Nc
Number of components in a solution
NO
Avogadro's number
,3
S
s1
1
sl sl
S
K1
'N'
kg 

6.023 x
SYMBOLSROMAN
xxiii
SYMBOLSROMAN
Symbol
Definition
Units
n
Number per unit volume (concentration)
m3
a
Unit normal vector at interface

nd
Instantaneous diffusionsource strength
m2, d = 3
P
Pressure
Pa = Jm3
P
Probability

p'
Momentum
kg m sl
Q
Heat
J
4
Electrical charge
C
R
Radius
m
r'
Position vector relative to origin
m
T , 8, z
Cylindrical coordinates

r , 8, q5
Spherical coordinates

S, S, s
Entropy, entropy per mole (or particle), entropy density
J Kl, J Klmol',
T
Absolute temperature
K
Tm
Absolute melting temperature
K
t
Time
S
U ,U , u
Internal energy, internal energy per mole (or particle), internal energy density
J , Jmoll, J m3
u'
Displacement field
m
ml, d = 2 number, d = 1
J K1m3
xxiv
SYMBOLSROMAN
SYMBOLSROMAN ~~
Symbol
Definition
Units
V
Volume
m3
5, v
Velocity, speed
m sl
21
Specific volume

w,w
Work, work per unit volume
J
XZ 2,Y,z
Composition variable: mole, atomic, or number fraction of component i

Cartesian orthogonal coordinates
m
X I , 22,23
General coordinates

2,Z C
Coordination number, effective coordination number for critical nucleus
z z

Partition function

Zeldovich factor

xxv
SYMBOLSGREEK Symbol
r', r
Definition
Units
~
~
Atomic or molecular jump frequency for a particular jump, total jump frequency
S1
Surface or interfacial tension, work t o produce unit interfacial area at constant stress and temperature at orientation
J m'
Activity coefficient of component
various
6
Effective thickness of grain boundary or surface layer; diameter of dislocation core
m
77
Diffusion scaling factor, z / m

Unit vector tangent t o dislocation

E, E, E , ~
Component of strain, strain tensor, strain tensor in component form
mml
K , ~ 1 K',
ml
KI
Mean curvature; principal curvatures Weighted mean curvature
K
Thermal diffusivity
m2 sl
x
Wavelength
m
A
Elasticenergy shape factor
y,
?(a)
?fa
i
t
J m3

~
P P,
Pi
pr,
,LLP
~
Elastic shear modulus
P a = Jm3
Chemical potential, chemical potential of species i Chemical potential of species i in phase a , chemical potential of species i in reference state
J
Frequency
S1
J
~~
U
xxvi
SYMBOLSGREEK
SYMBOLSGREEK ~
Symbol
Definition
Units
U
Poisson's ratio

Capillarity vector
J mP2
Density Electrical conductivity
kg mP3
0,m , c ~ i j
Stress, stress tensor, component of stress tensor
Pa
Ir
Rate of entropy production per unit volume
J m3 sl K'
7
Characteristic time
S
@i
Diffusion potential for species i
J
@
Electrical potential Site fraction
J Cl
z P
P
X
~
c vlml sl

0, Ri, (R)
Atomic volume, atomic volume of component i, average atomic volume
m3
W
Angular frequency
S1
= Jm3
CHAPTER 1
INTRODUCTI0N
Kinetics of Materials is the study of the rates at which various processes occur in materialsknowledge of which is fundamental to materials science and engineering. Many processes are of interest, including changes of size, shape, composition, and structure. In all cases, the system must be out of equilibrium during these processes if they are to occur at a finite rate. Because the departure from equilibrium may be large or small and because the range of phenomena is so broad, the study of kinetics is necessarily complex. This complexity is reduced by introducing approximations such as the assumption of local equilibrium in certain regions of a system, linear kinetics, or meanfield behavior. In much of this book we employ these approximations. Ultimately, a knowledge of kinetics is valuable because it leads to prediction of the rates of materials processes of practical importance. Analyses of the kinetics of such processes are included here as an alternative to a purely theoretical approach. Some examples of these processes with welldeveloped kinetic models are the rates of diffusion of a chemical species through a material, conduction of heat during casting, grain growth, vapor deposition, sintering of powders, solidification, and diffusional creep. The mechanisms by which materials change are of prime importance in determining the kinetics. Materials science and engineering emphasizes the role of a material’s microstructure. Structure and mechanisms are the yarn from which materials science is woven [l]. Understanding kinetic processes in, for example, crystalline materials relies as much on a thorough familiarity with vacancies, interstitials, grain Kinetics of Materials. By Robert W .Balluffi, Samuel M. Allen, and W. Craig Carter. Copyright @ 2005 John Wiley & Sons, Inc.
1
2
CHAPTER 1: INTRODUCTION
boundaries, and other crystal imperfections as it does on basic mathematics and physics. Extensive discussion of mechanisms is therefore a feature of this book. We stress rigorous analysis, where possible, and try to build a foundation for understanding kinetics in preparation for concepts and phenomena that fall beyond the scope of this book. Also, in laying a foundation, we have selected basic topics that we feel will be part of the materials science and engineering curriculum for many years, no matter how technical applications of materials change. A comprehensive reading of this book and an effort a t solving the exercises should provide the requisite tools for understanding most of the major aspects of kinetic processes in materials.
1.1 T H E R M O D Y N A M I C S A N D KINETICS In the study of materials science, two broad topics are traditionally distinguished: thermodynamics and kinetics. Thermodynamicsis the study of equilibrium states in which state variables of a system do not change with time, and kinetics is the study of the rates at which systems that are out of equilibrium change under the influence of various forces. The presence of the word dynamics in the term thermodynamics is therefore misleading but is retained for historical reasons. In many cases, the study of kinetics concerns itself with the paths and rates adopted by systems approaching equilibrium. Thermodynamics provides invaluable information about the final state of a system, thus providing a basic reference state for any kinetic theory. Kinetic processes in a large system are typically rapid over short length scales, so that equilibrium is nearly satisfied locally; at the same time, longerlengthscale kinetic processes result in a slower approach to global equilibrium. Therefore, much of the machinery of thermodynamics can be applied locally under an assumption of local equilibrium. It is clear, therefore, that the subject of thermodynamics is closely intertwined with kinetics. 1.1.1 Classical Thermodynamics and Constructions of Kinetic Theories
Thermodynamics grew out of studies of systems that exchange energy. Joule and Kelvin established the relationship between work and the flow of heat which resulted in a statement of the first law of thermodynamics. In Clausius’s treatise, The Mechanical Theory of Heat, the law of energy conservation was supplemented with a second law that defined entropy, a function that can only increase as an isolated system approaches equilibrium [2]. PoincarB coined the term thermodynamiques to refer to the new insights that developed from the first and second laws. Development of thermodynamics in the nineteenth century was devoted to practical considerations of work, energy supply, and efficiency of engines. At the end of the nineteenth century, J . Willard Gibbs transformed thermodynamics into the subject of phase stability, chemical equilibrium, and graphical constructions for analyzing equilibrium that is familiar to students of materials science. Gibbs used the first and second laws rigorously, but focused on the medium that stores energy during a work cycle. From Gibbs’s careful and rigorous derivations of equilibrium conditions of matter, the modern subjects of chemical and material thermodynamics were born [3]. Modern theories of statistical and continuum thermodynamics
1.1: THERMODYNAMICS AND KINETICS
3
which comprise the fundamental tools for the science of materials processesderive from Gibbs’s definitive works. Thermodynamics is precise, but is strictly applicable to phenomena that are unachievable in finite systems in finite amounts of time. It provides concise descriptions of systems at equilibrium by specifying constant values for a small number of intensive parameters. Two fundamental results from classical thermodynamics that form the basis for kinetic theories in materials are: 1. If an extensive quantity can be exchanged between two bodies, a condition necessary for equilibrium is that the conjugate potential, which is an intensive quantity, must have the same value throughout both bodies.
This can be generalized to adjoining regions in materials. The equilibrium condition, which disallows spatial variations in a potential (e.g., the gradient in chemical potential or pressure), cannot exist in the presence of active physical processes that allow the potential’s conjugate extensive density (composition or volume/mole) to change. This implies that a small set of homogeneous potentials can be specified for a heterogeneous system at equilibriumand therefore the number of parameters required to characterize an equilibrium system is relatively small. For a system that is not at equilibrium, any variation of potential is permitted. There are an infinite number of ways that a potential [e.g., ,ui(zy,, z ) ] can differ from its equilibrium value. Thus, the task of describing and analyzing nonequilibrium systemsthe subject of the kinetics of materialsis more complex than describing equilibrium systems. With this complexity, construction of applicable kinetic theories and techniques requires approximations that must strike a balance between oversimplification and physical reality. Students will benefit from a solid understanding of which approximations are being made, why they are being made, and the fundamental physical principles on which they are founded. 2. If a closed system is in equilibrium with reservoirs maintaining constant potentials (e.g., P and T ) ,that system has a freeenergy function [e.g., G ( P , T ) ] that is minimized at equilibrium. Therefore, a necessary condition for equilibrium is that any variation in G must be nonnegative: ( 6 G ) p ,2~0.
This leads to classical geometrical constructions of thermodynamics, including the commontangent construction illustrated in Figs. 1.1 and 1.2. For closed systems that are not at equilibrium, a function G(P,T ) exists for the entire systembut only as a limiting value for the asymptotic approach to equilibrium. Away from equilibrium, the various parts of a system generally have gradients in potentials and there is no guarantee of the existence of an integrable local freeenergy density. The total free energy must decrease to a minimum value at equilibrium. However, there is no recipe for calculating such a total free energy from the constituent parts of a nonequilibrium system. A quandary arises: general statements regarding the approach to equilibrium that are based on thermodynamic functions necessarily involve extrapolation away from equilibrium conditions. However, useful models and theories can be developed from approximate expressions for functions having minima that coincide with the equilibrium thermodynamic quantities and from assumptions of local equilibrium states. This approach is consistent
4
CHAPTER 1 INTRODUCTION
,________
t
u

(9
moles of B/(total moles A+B) (a)

tangent
(x>
moles of B/(total moles A+B)
(b)
Figure 1.1: (a) Curves of the mininium free energy of homogeneous cy and /3 phases as a furictioii of average (overall) composition, ( X ) ,at constant P and T . G is the free energy of 1 mole of solution. Under nonequililxium conditions, free energies may be larger than those given by the curves, as the vertical arrow indicates. (b) Cornniontangent construction showing a minimum freeenergy curve for a system that may contain cy phase, /3 phase, or both coexisting. The curve consists of a segnient on the left which extends to the first point of common tangency, CT1, a straight line segment between two points of common tangency, CTl and CT2, and a further segment to the right of CT2. The system a t equilibrium consists of a homogeneous ac phase up to composition CT1. a mixture of coexisting a and B phases between CTl and CT2, and a homogeneous /3 phase beyond CT2. As in ( a ) , an infinite number of higher freeenergy states is possible for the system under nonequilibriuni conditions. A subset of these correspond to linear mixtures of homogeneous a and p phases whose free energies are given by the lower dashed line in ( b ) , where X,and X, are the cy and @’ phase compositions, respectively. These free energies are plotted, and the energies that can be obtained from such mixtures are bound from ahove by the dashed line representing a mixture of pure A and pure B. However, in general, energies of the nonequilibrium system are not bound, as indicated in Fig. 1.2.
with the laws of thermodynamics and provides an insightful and organized theoretical foundation for kinetic theories. Another approach is to build kinetic theories empirically and thus guarantee agreement between theory and experiment. Such theories often can successfully be extended t o predict observations of new phenomena. Confidence in such predictions is increased by a thorough understanding of the atomic mechanisms of the system on which the primary observation is made and of the system to which predictions will be applied.
1.1.2 Averaging Although it may be possible to use computation to simulate atomic motions and atomistic evolution, successful implementation of such a scheme would eliminate the need for much of this book if the computation could be performed in a reasonable amount of time. It is possible to construct interatomic potentials and forces between atoms that approximate real systems in a limited number of atomic configurations. Applying Newton’s laws (or quantum mechanics, if required) to calculate the particle motions, the approximate behavior of large numbers of interacting par
1.2: IRREVERSIBLE THERMODYNAMICS AND KINETICS
5

(X) moles of B/(total moles A +B) Figure 1.2: Representation of all possible values of system molar free energy in Fig. 1.1. ( X )is the average mole fraction of component B.
ticles can be simulated. At the time of this writing, believable approximations that simulate tens of millions of particles for microseconds can be performed by patient researchers with access to stateoftheart computational facilities. Such calculations have been used to construct thermodynamic data as a foundation on which to build kinetic approximations. However, simulations for systems with sizes and time scales of technological interest do not appear feasible in any current and credible longrange forecast. Just as statistical mechanics overcomes difficulties arising from large numbers of interacting particles by constructing rigorous methods of averaging, kinetic theory also uses averaging. However, the application of these methods to kinetically evolving systems is precluded because many of the fundamental assumptions of statistical mechanics (e.g., the ergodic hypothesis) do not apply. Many theories developed in this book are expressed by equations or results involving continuous functions: for example, the spatially variable concentration .(?). Materials systems are fundamentally discrete and do not have an inherent continuous structure from which continuous functions can be constructed. Whereas the composition at a particular point can be understood both intuitively and as an abstract quantity, a rigorous mathematical definition of a suitable composition function is not straightforward. Moreover, using a continuous position vector r' in conjunction with a crystalline system having discrete atomic positions may lead to confusion. The abstract conception of a continuum and the mathematics required to describe it and its variations are discussed below. 1.2
IRREVERSIBLE T H E R M O D Y N A M I C S A N D KINETICS
Irreversible thermodynamics originated in 1931 when Onsager presented a unified approach to irreversible processes [4]. In this book we explore some of Onsager's ideas, but it is worth remarking that his theory applies to systems that are near equi1ibrium.l Perhaps zeroth and firstorder thermodynamics would be ' N e a r is unfortunately a rather vague word when applied t o the state of a system. Systems that are close t o detailed balance where forward processes are almost balanced by backward processes,
6
CHAPTER 1 INTRODUCTION
more descriptivebut it really doesn’t matter as long as the proper application of fundamental principles is retained. Consider a material or system that is not) at equilibrium. Its extensive state variables (total entropy: number of moles of chemical component, i: total magnetization; volume; etc.) will change consistent with the second law of thermodynamics (i.e.? with an increase of entropy of all affected systems). At equilibrium. the values of the intensive variables are specified; for instance, if a chemical component is free to move from one part of the material to another and there are no barriers to diffusion, the chemical potential, p r , for each chemical component, i, must be uniform throughout the entire materiaL2 So one way that a material can be out of equilibrium is if there are spatial variations in the chemical potential: pi(x%y ?z ) . However, a chemical potential of a component is the amount of reversible work needed to add an infinitesimal amount of that component to a system at equilibrium. Can a chemical potential be defined when the system is not at equilibrium? This cannot’ be done rigorously, but’ based on decades of development of kinetic models for processes, it is useful to extend the concept of the chemical potential to systems close to, but not a t , equilibrium. Temperature is another quantity defined under equilibrium conditions and for which some doubt may arise regarding its applicability to nonequilibrium systems. Consider a bar of material with ends at different temperatures, as in Fig. 1.3. Suppose that the system has reached a steady statethe amount of heat absorbed by the bar at the hot end is equal to the amount of heat given off at the cold end. The temperature can be thought of as a continuous function, T ( x ) which , is sketched above the bar in Fig. 1.3. An imaginary therniometer placed along the bar would be expected to indicate the plotted temperatures as it moves from point to point. The thermometer in this case is in local equilibrium with an infinitesimal region of the bar. What kind of thermometer could perform such a measurement? In order not to affect the measurement, it must have a negligible heat capacity and be unable to conduct any significant amount of heat from the bar. Physically. no such
I
L
I
Figure 1.3: Represeiitat ion of a onetiiniensional t herrrial gradient such as during diffusion, may be regarded as near equilibrium. Quantification of “nearness” has theoretical utility and is a topic of current research [ 5 ] . 2Uniform chemical potential a t equilibrium assumes that the component conveys no other work terms. such as charge in an electric field. If other other energystorage mechanisms are associated with a component, a generalized potential (the diffusion potential, developed in Section 2.2.3) will be uniform a t equilibrium.
1.3: MATHEMATICAL BACKGROUND
7
thermometer can existnor can a real material be divided infinitesimally. However, this does not mean that one's intuition about the existence of such a function T ( x ) is wrong; it is reasonable to take a continuum limit (see Section 1.3.3) of such an idealized measurement and refer to the temperature at a point. 1.3
MATHEMATICAL BACKGROUND
A few basic physical and mathematical concepts are essential to the study of kinetics, and several of these concepts are introduced below using a mathematical language suited to a discussion of kinetics. 1.3.1
Fields
A field, f(6,associates a physical quantity with a position, r'= (z, y , ~ ) A. ~field may be timedependent: for example, f(r',t). The simplest case is a scalar field where the physical quantity can be described with one value at each point. For example, T(F,t ) can represent the spatial and timedependent temperature and p(F, t ) the d e n ~ i t y . ~ A vector field, such as force, @(r',t)or flux, f(r',t), requires specification of a magnitude and a direction in reference to a fixed frame. A ranktwo tensor field such as stress, u ( F ,t ) , relates a vector field to another vector often attached to the + + material in question: for example, u = F ( r , t ) / A ,where F(;, t ) is the force exerted by the stress, u ,on a virtual area embedded in the material and represented by the vector A' = AA,where A is the unit normal to the area and A is the magnitude of the area. Every sufficiently smooth scalar field has an associated natural vector field, which is the gradient field giving the direction and the magnitude of the steepest rate of ascent of the physical quantity associated with the field.5
1.3.2 Variations Consider a stationary scalar field such as concentration, c(F) (see Fig. 1.4), and the rate at which the values of c change as the position is moved with velocity v' [suppose that an insect is walking on the surface of Fig. 1.4 with velocity v'(x, y ) ] . The value of c will change with time, t , according to c(r'+ v't):
c(r'+ v't) = c ( 6 + V c . v'lt=o t + . . .
(1.1)
where Vc, the gradient of c, is the threedimensional vector field defined by
O4.3 =
dc d c dc
dc
dc
a,)  id+x  j +dyk
dcdz
Vc points in the direction of maximum rate of increase of the scalar field c ( q ; the magnitude of the gradient vector is equal to this rate of increase. The instantaneous 3Here, Cartesian coordinates represent points. Other coordinate systems are employed when appropriate. 4However, the definition of each of these quantities depends on the choice of averaging of a physical quantity (e.g., kinetic energy or mass) a t a point F. 5The associated natural vector field exists as long as there is a definition of distance (a norm).
8
CHAPTER i INTRODUCTION
Figure 1.4: Reprcsent,at,ioiisof a twodimerisiorial scalar field are at t,lie left arid middle. A familiar cxample of a scalar field is the altit,ude of a point, as a fimtiori of its loiigitucle and latitude a topographical map, its in the middle figure. It is iiiitlrrstootl iii topogritpliical rnaps t,liat local averaging is performed. Det,ails in the figure oil t,he riglit may exist at "iriicroscopic" scales t,liat can be ignored for 'macroscopic" model applicat,ioiis.
rate of change of c with respect to t is therefore
(1.3) Equation 1.3can be generalized further by considering a t i m e  d e p e n d e n t field c(F, t ) : the instantaneous rate of change of c with velocity v'(3is then dc
=
dt
dc vc4+ 
at
Another type of derivative, the divergence of a vector field, is defined in Section 1.3.5.
1.3.3 Continuum Limits and Coarse Graining Within the small volume of material shown at r' in Fig. 1.5, a certain quantity of species i is expected. This specifies a concentration for that particular small box: this concentration will be in local equilibrium with some diffusion potential. However, materials are comprised of discrete atoms (molecules), which complicates the definition of local concentration when the volume sampled becomes comparable to the mean distance between atoms being counted. In Fig. 1.5. for the physzcnl
'* 0 Figure 1.5: Infinitesirrial volurrie. A V , with diirierisioris dx. d y . a i d d z located at position ?with respect t o the origiIi at 0.
1 3 MATHEMATICAL BACKGROUND
9
limit of small volume AV = d x d y d z , the expectation of finding N atoms of species i in that volume vanishes as AV goes to zero. Suppose that the atoms are distributed in space as in Fig. 1.5.6 Consider the behavior of the concentration of idefined by (number of atoms of type i)/(volume)as the volume shrinks toward the point where c ( q is evaluated as in Fig. 1.6. Apparently, the limiting value used intuitively to define the concentration c ( 3 is
I
Figure 1.6:
AV
Behavior of the concentration a t
t~
point
c ( 3 as the volume A V + 0.
not a welldefined limit of the function c(F, AV + 0). This conceptual difficulty can be removed by defining a local convolution function such as in Fig. 1.7. A continuum limit for the concentration of particles, c ( 3 , can be defined with a convolution function <(F;), which specifies, at a position F, the weight to assign to a particle located a t ?:
This definition has the correct global behavior for large volumes V because
where it is assumed that the interference of convolution with the boundary of the domain V is negligible. Furthermore, the definition, Eq. 1.5, has the correct local behavior: suppose that a volume AV (with spatial dimensions large compared to
* *
r' = r Figure 1.7:
located at F =
T h e convolution function [ ( F 
?.
+
r
7 )accomplishes coarse graining of a n object
'Nicolas Mounet contributed significantly to the development of coarse graining in this section.
10
CHAPTER 1: INTRODUCTION
the width of the convolution function) contains a single isolated particle (i.e., the particle in AV is "far" from all others). Also, let the particle's i index be 1, with its position ri at the center of AV; then
Defined by Eq. 1.5, c ( q becomes a coarsegrained representation of the discrete particle positions. In one dimension, an exemplary choice for a convolution function is <(x  xi) = exp[(z  z ~ ) ~ / where B ~ ] ,B is the characteristic coarsegrained length. With this choice, the coarsegrained onedimensional concentration is N e(zzi)z/Bz xi=1 C(X) = (1.8) J;iB Examples with different characteristic coarsegrain lengths are shown in Fig. 1.8. In this book, it is assumed that the continuum limits exist and coarsegrained functions can be obtained that do not depend significantly on the choice of 5. 1
A
B=l
C
0 .c !. c C a 0
s C
0
I
,
I
I
0
I
I
25
,
I
I
I
l
I
I
50 Position
I
,
I
,
75
,
,
,
I
100
Figure 1.8: Example of onedimensional coarsegrained concentrations of discrete data. Twentytwo atoms were placed randomly on a discrete lattice at positions xi,0 < xi < 100. The concentration curves are continuous and have areas that are approximately equal to the number of atoms in the random sample. Each atom contributes a unit area to the coarsegrained ~ ( x )Broader . convolution functions (higher values of B ) produce greater degrees of coarse graining.
1.3.4
Fluxes
x(3, describes
the rate at which i flows through a unit area fixed with respect to a specified coordinate system. Let AA' be an oriented area, equal t o liAA = ( A z ,A , , A , ) in a Cartesian systems7 If ldi is a smooth function that
A flux of i,
7AA
IAA'I and A = AA'/lAA'l
1 3 MATHEMATICAL BACKGROUND
defines the rate at which i flows through area
AA’:
The proportionality factor must be a vector field
kf%(AX)=
This defines the local flux
x:
x . AA
x(F)as the continuum limit of if?(AA) = $(F) . f i
(1.10)
(1.11)
AA
1.3.5
11
Accumulation
The amount of i that accumulates in a volume AV = d x d y d z (with outwardoriented normals) in a Cartesian system during the time interval 6t is
AM, = (z that flowed in during bt)  (i that flowed out during bt) + (i produced inside during bt)
(1.12)
An expression for the accumulation can be written wiih the aid of Fig. 1.9, generalized to include the y and z components of the flux J : 6 A f , =d(n:+d~/2,0,0).idydz6t+x(xd~/2,0,0).idydz6t  d ( 0 ,y 
+ dyl2.0) . j dz dx 6t + x ( 0 ,y  dy/2,0). j d z dx 6t
x(O,O,z
+ d ~ / 2.)k dx dy 6t + $(O,O,
+ p,(F) AV6t
z
 d ~ / 2 .)k dx dy bt
(1.13)
where &(?) is the rate of production of the density of i in AV. Expanding to first order in dx,dy, d z , subtracting. and using the continuum limit yields aci
at
=
+
V . J ,
+
pi
(1.14)
Figure 1.9: Accuniulation of an extensive quantity arising from a divergence of its flux J’= ( J z , J v , J z ) .
12
CHAPTER 1 INTRODUCTION
where the quantity V . 4 is the divergence of
&, which for a general flux f i s 
dJ, dJ, ++ax dy
dJ, 8.2
(1.15)
This is the rate at which the flux causes the density of the quantity comprising the flux to decrease. The rate of accumulation of the extensive quantity’s density is therefore minus the divergence of the fluxof that quantity plus the rate ofproduction. Alternatively, Eq. 1.14 could be derived directly from
where B ( A V ) is the oriented surface around AV and the divergence theorem (Gauss’s theorem), +
S,(A,,
J , f i d A=
Lv
V.fdV
(1.17)
has been applied. Note that the divergence theorem has a geometrical interpretation. If the volume is comprised of many neighboring cells, the total accumulation in the volume is the sum of accumulations in all the cells; see the righthand side of Eq. 1.17. Each cell’s accumulation arises from the flux at its surfaces. However, when cells share an interface, they have opposite normal vectors, and the flux terms, f.d, cancel. In a group of abutting cells, the fluxes across the interior interfaces cancel so that the only contribution is due to the exterior surfaces.
1.3.6 Conserved and Nonconserved Quantities A conserved quantity cannot be created or destroyed and therefore has no sources or sinks; for conserved quantities such as atomic species i or internal energy U , (1.18) dU _  V
at
*

J,
(1.19)
where u is the internal energy density.8 For nonconserved quantities such as entropy, S , (1.20) where u is the rate of entropy production per unit volume. Entropy flux and entropy production are examined in Chapter 2. sBarring processes such as nuclear decay, transmutation, or implantation by ion irradiation.
1.3: MATHEMATICAL BACKGROUND
13
1.3.7 Matrices, Tensors, and the Eigensystem In this section we provide a brief review of topics in linear algebra and tensor pr0pert.y relations that are used frequently throughout the book. Nye’s book on tensor properties contains a complete overview and is also a valuable resource [ 6 ] . A general set of linear equations for the quantities yi (i = 1 , 2 , 3 , .. . , n) in terms of variables x j ( j = 1 , 2 , 3 , .. . , rn) can be written as
92 =
+ M12~2 + + M21~1 + +. . . +
y3 =
...
91 =
Mllxl
’ ‘
Mlmxm
M2222
or
m
yi =
C ~~~x~
(1.21)
for i = 1 , 2 , .. . , n
(1.22)
j=1
The Mij are the elements of a matrix, hf, that multiplies a vector 2 and produces the result, y’ = MZ,or in component form,
(1.23)
In this book, vector quantities such as 2 and y’ above are normally column vectors. When necessary, row vectors are indicated by use of the transpose (e.g., p).If the components of 2 and refer t o coordinate axes [e.g., orthogonal coordinate axes (51, 5 2 , 53) aligned with a particular choice of “right,” “forward,” and “up” in a laboratory], the square matrix hf is a ranktwo t e n ~ o r .In ~ this book we denote tensors of rank two and higher using boldface symbols (i.e.?M ) . If 2 is an applied force and y’ is the material response to the force (such as a flux), M is a ranktwo materialproperty tensor. For example, the full anisotropic form of Ohm’s law gives in terms of an applied electric field I? as a charge flux
&
(1.24)
x
is the ranktwo conductivity tensor for a particular material. In Eq. 1.24, x is the material property that relates both the magnitude of “effect” to the “cause” 3 and their directions& is not necessarily parallel to l?.
&
9Mis rank two because it relates two different sets of vector components in a prescribed way: that is, the components of Z are mapped into components of y’by the tensor M . The vectors Z and y’ refer t o a single coordinate system and are called rankone tensors.
14
CHAPTER 1: INTRODUCTION
The physical law in Eq. 1.24 can be expressed as an inverse relationship:
(1.25)
where the resistivity tensor, p , is the inverse of the conductivity tensor (Le., p =
xl)?
Many materials properties are anisotropic: they vary with direction in the material. When anisotropic materials properties are characterized, the values used t o represent the properties must be specified with respect to particular coordinate axes. If the material remains fixed and the properties are specified with respect to some new set of coordinate axes, the properties themselves must remain invariant. The way in which the properties are described will change, but the properties themselves (i.e,, the material behavior) will not. The components of tensor quantities transform in specified ways with changes in coordinate axes; such transformation laws distinguish tensors from matrices [ 6 ] . For a particular material response or applied field, particular choices of coordinate axis orientations may be especially convenient (e.g., axes aligned with crystal lattice vectors). Linear transformationssuch as rotations, reflections, and affine distortions can be performed on vector forces and responses by matrix multiplication to describe forceresponse relations in different coordinate systems. For instance, a vector E’ can be transformed between “old” and “new” coordinate systems by a matrix 4: (1.26)
A simple proof will show that (1.27) i.e., g l d  + n e w is the inverse of , and vice versa. It is often convenient to select the coordinate system for which the only nonzero elements of the property tensor lie on its diagonal. This is the eigensystem. To find the eigensystem, the general rules for transformation of a tensor must be identified. The transformation of Ohm’s law (Eq. 1.24) illustrates the way in which the material and serves t o demonstrate the general properties tensor xoldtransforms t o xneW rule for transforming ranktwo tensors: in old coordinate system: in new coordinate system:
eld = xoldE‘old
=
xnewknew
(1.28)
“Indices appear as 1, 2, 3 in Eq. 1.24 and as z, y, z in Eq. 1.25. The numerical indices represent any threedimensional coordinate system (including Cartesian), and the indices in Eq. 1.25 are strictly Cartesian.
1.3:MATHEMATICAL BACKGROUND
15
The relationship between xoldand xneW can be found by applying the transformations in Eqs. 1.26 to the expressions for Ohm’s law in both coordinate systems. For the first equation in Eq. 1.28, using the transformations in Eqs. 1.26, Anewrold J4‘new  Xold#ewold@w
(1.29)
and for the second equation in Eq. 1.28, (1.30)
Aoldnew J’old 4 = XnewAoldnew*ld
Leftmultiplying by the inverse transformations, Aold+newAnewold +new  J;ew + J4 

= A o l d  + n e w old
X

newold*ew
A
and AnewOld

oldnewJ’old
A
4
(1.31)
 J’old  AnewoldXnewAoldnew*ld 4

Therefore, Aoldnew xnew= 
Xold Anewrold
and
(1.32)
old  AnewrOld
x 

X
new
oldrnew
A
This patterna rankone tensor is transformed by a single matrix multiplication and a ranktwo tensor is transformed by two matrix multiplicationsholds for tensors of any rank. If A is an orthogonal transformation, such as a rigid rotation or a rigid rotation combined with a reflection, its inverse is its transpose. For example, if B is a rotation, R,jRji = 6ij, where 6ij is the Kronecker delta, defined as 1 if i = j 6ij = (1.33) 0 if i # j
{
i.e., 6 i j is the index form of the identity matrix. Square matrices and tensors can be characterized by their eigenvalues and eigenvectors. If M is an n x n square matrix (or tensor), there is a set of n special vectors, Z,each with its own special scalar multiplier X for which matrix multiplication of a vector is equivalent to scalar multiplication of a vector: MZ=XZ
or
(1.34) +
(Mxz_)Z= 0
where 0’ is a vector of zeros that has the same number of entries, n,as Zand 2 is the n x n identity matrix (i.e., 2 has ones along its major diagonal and zeros elsewhere). The solutions X i and Zi are the eigenvalues and eigenvectors of M.In general, there are n unique X i : & pairs for any M.The eigenvectors of M can be interpreted geometrically as the set of vectors that do not change direction when multiplied by nilinstead, they are scaled by a constant A. The eigenvalues can be determined from the polynomial equation for A: d e t ( M  X) = 0
(1.35)
16
CHAPTER 1: INTRODUCTION
which is a requirement that the homogeneous equation, Eq. 1.34, has a nontrivial solution. After the eigenvalues have been determined, the directions of the eigenvectors Zcan be determined by solving Eq. 1.34. A ranktwo property tensor is diagonal in the coordinate system defined by its eigenvectors. Ranktwo tensors transform like 3 x 3 square matrices. The general rule for transformation of a square matrix into its diagonal form is
matrix
]
=
[
eigenvector column matrix
]
1
[
'quare matrix
][
eigenvector column matrix
]
(1.36)
where the ith member of the diagonal matrix is the eigenvalue corresponding to the eigenvector used for the ith column vector of the transformation matrix. Nearly all ranktwo property tensors can be represented by 3 x 3 symmetric matrices and necessarily have real eigenvalues. Bibliography 1.
S.M. Allen and E.L. Thomas. The Structure of Materials. John Wiley & Sons, New York, 1999.
2. R. Clausius. The Mechanical Theory of Heat: With Its Applications to the SteamEngine and to the Physical Properties of Bodies. Van Voorst, London, 1867. 3. J.W. Gibbs. On the equilibrium of heterogeneous substances (1876). In Collected Works,volume 1. Longmans, Green, and Co., New York, 1928. 4. L. Onsager. Reciprocal relations in irreversible processes. 11. Phys. Rev., 38( 12):22652279, 1931. 5. W.C. Carter, J.E. Taylor, and J.W. Cahn. Variational methods for microstructural evolution. JOM, 49(12):3036, 1997. 6. J.F. Nye. Physical Properties of Crystals. Oxford University Press, Oxford, 1985.
EXERCISES 1.1 The concentration at any point in space is given by
c = A (zy
+ yz + ZX)
(1.37)
where A = constant.
(a) Find the cosines of the direction in which c changes most rapidly with distance from the point (1,1,1). (b) Determine the maximum rate of change of concentration a t that point. Solution. (a) The direction o f maximum rate o f change is along the gradient vector V c given
by Therefore,
V c = A [(y
+ ~ )+ i( Z + ~ )+ j + y)2] (Z
+j + i ) l/G.
V c (1,1,1) = 2A (i
and the direction cosines are [l/&, l/&
(1.38) (1.39)
EXERCISES
17
(b) The maximum rate of change o f c is then
IVc(l,1, 1)1= 2 A h
(1.40)
1.2 Consider the radially symmetric flux field
 r '
J=
where r' = xi
r3
(1.41)
+ y j+zk.
(a) Show that the total flux through any closed surface that does not enclose the origin vanishes. (b) Show that the flux through any sphere centered at the origin is independent of the sphere radius. Solution. The problem is most easily solved using the divergence theorem:
LJ.iLdA =L V . fdV
(1.42)
Consider first the divergence o f radially symmetric vector fields of a general form, including the present field as a special case, i.e.,
(1.43) For such fields
(1.44) In this case, n = 3 and the divergence o f T i n Eq. 1.42 is zero if the singularity at r = 0 is avoided. Therefore, if the closed surface does not include the origin,
V . JdV =0 and the total flux through the surface,
(1.45)
s, f.AdA, is also zero.
When the closed surface does enclose the origin, the total flux through the surface does not vanish. For a sphere o f radius R ,
(1.46) Therefore the total flux is independent o f R and equal t o 47r.
1.3 Suppose that the flux of some substance i is given by the vector field = A (xi
+ vj)
(1.47)
where A = constant. Find the rate, Mi,at which i flows through the hemispherical surface of the unit sphere x2
+ y2 + z 2 = 1
(1.48)
18
CHAPTER 1: INTRODUCTION
which lies above the (x,y) plane where z 2 0. Solution. Mi =
J
J;.dA=/
hemi
For the hemisphere,
J:.AdA
(1.49)
hemi
A = xi
+yj+z i
(1.50)
Also, the integral may be converted t o an integral over the projection of the hemisphere on the (x, y) plane (denoted by P ) by noting that
k.AdA=dxdy
 dxdy JJ J,.A=A z
so that
(1.51)
JJ J Cx 2+Fy 2j p dxdy
M,=
P
(1.52)
P
Converting t o polar coordinates and integrating over P ,
(1.53)
1.4 The matrix
A is given by (1.54)
(a) Find the eigenvalues and corresponding eigenvectors of A.
(b) Find matrices p and p' such that
p'AP
is a diagonal matrix.
Note: The tedium of completing such exercises, as well as following many derivations in this book, is reduced by the use of symbolic mathematical software. We recommend that students gain a working familiarity with at least one package such as MathematicaB, M A T L A B @ ,Mathcadco, or the publicdomain package M A X I M A . Solution. (a) The characteristic equation of ,cl is given by Eq. 1.35 as
X3  16X2
+ 72X  68 = 0
(1.55)
The eigenvalues are solutions t o the characteristic equation, giving
X i = 8.36258
Xz = 6.35861
XB = 1.27881
The eigenvectors corresponding t o the eigenvalues are 01
=
[
1.27252 0.5:8613
]
212
=
[
0.871722 2.413084
]
w3
=
[
0.144238 0.03105511
(1.56)
] (1.57)
Note that these eigenvectors are of arbitrary length.
EXERCISES
19
(b) From Eq. 1.36 it is seen that the desired matrix is 3 x 3 and has the three eigenvectors as its columns: P=
[
1.27252 0.538613 1
0.871722 2.43084 1
may be calculated as
The inverse of
 [ P' =
0.832149 0.176139 0.65601
0.352221 0.491171 0.13895
B y substitution it is readily verified that
PlM
0.144238 0.0305511 1
X i = 8.36258 =
0.130788 0.0404117 0.909624
Eq. 1.36 is obeyed: 0
Xz = 6.35861
0
1 1
0 0 As = 1.27881
(1.58)
(1.59)
1
(1.60)
PART I
MOTION OF ATOMS AND MOLECULES BY DIFFUSION
There are two arenas for describing diffusion in materials, macroscopic and microscopic. Theories of macroscopic diffusion provide a framework to understand particle fluxes and concentration profiles in terms of phenomenological coefficients and driving forces. Microscopic diffusion theories provide a framework to understand the physical basis of the phenomenological coefficients in terms of atomic mechanisms and particle jump frequencies. We start with the macroscopic aspects of diffusion. The components in a system out of equilibrium will generally experience net forces that can generate corresponding fluxes of the components (diffusion fluxes) as the system tries to reach equilibrium. The first step (Chapter 2) is the derivation of the general coupling between these forces and fluxes using the methods of irreversible thermodynamics. From general results derived from irreversible thermodynamics, specific driving forces and fluxes in various systems of importance in materials science are obtained in Chapter 3. These forces and fluxes are used to derive the differential equations that govern the evolution of the concentration fields produced by these fluxes (Chapter 4). Mathematical methods to solve these equations in various systems under specified boundary and initial conditions are explored in greater depth in Chapter 5 . Finally, diffusion in multicomponent systems is treated in Chapter 6.
22
Microscopic and mechanistic aspects of diffusion are treated in Chapters 710. An expression for the basic jump rate of an atom (or molecule) in a condensed system is obtained and various aspects of the displacements of migrating particles are described (Chapter 7). Discussions are then given of atomistic models for diffusivities and diffusion in bulk crystalline materials (Chapter 8), along line and planar imperfections in crystalline materials (Chapter 9), and in bulk noncrystalline materials (Chapter 10).
CHAPTER 2
IRREVERSIBLE THERMODYNAMICS AND COUPLING BETWEEN FORCES AND FLUXES
The foundation of irreversible thermodynamics is the concept of entropy production. The consequences of entropy production in a dynamic system lead to a natural and general coupling of the driving forces and corresponding fluxes that are present in a nonequilibrium system. 2.1
E N T R O P Y A N D ENTROPY PRODUCTION
The existence of a conserved internal energy is a consequence of the first law of thermodynamics. Numerical values of a system’s energy are always specified with respect to a reference energy. The existence of the entropy state function is a consequence of the second law of thermodynamics. In classical thermodynamics, the value of a system’s entropy is not directly measurable but can be calculated by devising a reversible path from a reference state to the system’s state and integrating dS = 6q,,,/T along that path. For a nonequilibrium system, a reversible path is generally unavailable. In statistical mechanics, entropy is related to the number of microscopic states available at a fixed energy. Thus, a statecounting device would be required to compute entropy for a particular system, but no such device is generally available for the irreversible case. To obtain a local quantification of entropy in a nonequilibrium material, consider a continuous system that has gradients in temperature, chemical potential, and other intensive thermodynamic quantities. Fluxes of heat, mass, and other extensive quantities will develop as the system approaches equilibrium. Assume that Kinetics of Materials. By Robert W. Balluffi, Samuel M. Allen, and W. Craig Carter. Copyright @ 2005 John Wiley & Sons, Inc.
23
24
CHAPTER 2 : IRREVERSIBLE THERMODYNAMICS:COUPLED FORCES AND FLUXES
the system can be divided into small contiguous cells at which the temperature, chemical potential, and other thermodynamic potentials can be approximated by their average values. The local equilibrium assumption is that the thermodynamic state of each cell is specified and in equilibrium with the local values of thermodynamic potentials. If local equilibrium is assumed for each microscopic cell even though the entire system is out of equilibrium, then Gibbs’s fundamental relation, obtained by combining the first and second laws of thermodynamics,
can be used to calculate changes in the local equilibrium states as a result of evolution of the spatial distribution of thermodynamic potentials. U and S are the internal energy and entropy of a cell, dW is the work (other than chemical work) done by a cell, Ni is the number of particles of the ith component of the possible N, components, and pi is the chemical potential of the ith component. pi depends upon the energetics of the chemical interactions that occur when a particle of i is added to the system and can be expressed as a general function of the atomic fraction X i : pi = pp
+ kT ln(yiXi)
(2.2)
The activity coefficient yi generally depends on X , but, according to Raoult’s law, is approximately unity for Xi x 1. Dividing dLI through by a constant reference cell volume, V,,
where all extensive quantities are now on a per unit volume basis (i.e., densities).’ For example, v = V / V , is the cell volume relative to the reference volume, V,, and ci = Ni/Vois the concentration of component i. The work density, dw, includes all types of (nonchemical) work possible for the system. For instance, the elastic work aij d E i j (where density introduced by smallstrain deformation is dw = aij and ~ i are j the stress and strain tensors), which can be further separated into 6ij d z i j (where 5 and t hydrostatic and deviatoric terms as dw = P d v are the deviatoric stress and strain tensors, respectively). The elastic work density therefore includes a work of expansion Pdv. Other work terms can be included in Eq. 2.3, such as electrostatic potential work, dw =  4 d q (where 4 is the electric potential and q is the charge density); interfacial work, dw =  y d A , in systems containing extensible interfaces (where y is the interfacial energy density and A is the interfacial area; magnetization work, dw = d . d6 (where d is the magnetic field and b‘ is the total magnetic moment density, including the permeability of vacuum); and electric polarization work, dw = E ’ dp’ (where l? is the electric field given by E’ = V$ and p’ is the total polarization density, including the contribution from the vacuum). If the system can perform other types of work, there must
+ xix,
xix j
‘Use of the reference cell volume, V,, is necessary because it establishes a thermodynamic reference state.
2.1. ENTROPY AND ENTROPY PRODUCTION
25
be terms in Eq. 2.3 to account for them. To generalize:
where $ j represents a j t h generalized intensive quantity and jugate extensive quantity densitye2Therefore,
C$jd<j =  P d u + 4 d q +
<j
represents its con
+ y d A + d6+ E . dp’ + pi dci + . . + p ~ dCN, , + .. .
j
6 k i dgkl
(2.5)
*
The $ j may be scalar, vector, or, generally, tensor quantities; however, each product in Eq. 2.5 must be a scalar. Equation 2.4 can be used to define the continuum limit for the change in entropy in terms of measurable quantities. The differential terms are the firstorder approximations to the increase of the quantities at a point. Such changes may reflect how a quantity changes in time, t , at a fixed point, r‘; or at a fixed time for a variable location in a point’s neighborhood. The change in the total entropy in the system, S, can be calculated by summing the entropies in each of the cells by integrating 2.4, which is derived by combining the first and over the entire ~ y s t e r n .Equation ~ second laws, applies to reversible changes. However, because s , u,and the & are all state variables, the relation holds if all quantities refer t o a cell under the local equilibrium assumption. Taking s as the dependent variable, Eq. 2.4 shows how s varies with changes in the independent variables, u and 0. In equilibrium thermodynamics, entropy maximization for a system with fixed internal energy determines equilibrium. Entropy increase plays a large role in irreversible thermodynamics. If each of the reference cells were an isolated system, the righthand side of Eq. 2.4 could only increase in a kinetic process. However, because energy, heat, and mass may flow between cells during kinetic processes, they cannot be treated as isolated systems, and application of the second law must be generalized to the system of interacting cells. In a hypothetical system for modeling kinetics, the microscopic cells must be open systems. It is useful to consider entropy as a fluxlike quantity capable of flowing from one part of a system to another, just like energy, mass, and charge. is related to the heat flux. An expression that relates Entropy flux, denoted by to measurable fluxes is derived below. Mass, charge, and energy are conserved quantities and additional restrictions on the flux of conserved quantities apply. However, entropy is not conservedit can be created or destroyed locally. The consequences of entropy production are developed below.
i,
2.1.1
Entropy Production
The local rate of entropydensity creation is denoted by Cr. The total rate of entropy creation in a volume V is Jv d. d V . For an isolated system, dS/dt = Jv Cr d V . 2The generalized intensive and extensive quantities may be regarded as generalized potentials and displacements, respectively. 3Note that S is the entropy of a cell, S is the entropy of the entire system, and s is the entropy per unit volume of the cell in its reference state.
26
CHAPTER 2 : IRREVERSIBLE THERMODYNAMICS: COUPLED FORCES AND FLUXES
However, for a more general system, the total entropy increase will depend upon how much entropy is produced within it and upon how much entropy flows through its boundaries. From Eq. 2.4, the time derivative of entropy density in a cell is
d s  1_ du  1 _ dt
T dt
T
C$j%
Using conservation principles such as Eqs. 1.18 and 1.19 in Eq. 2.6,4
From the chain rule for a scalar field A and a vector
g,
Equation 2.7 can be written
Comparison with terms in Eq. 1.20 identifies the entropy flux and entropy production: (2.10) (2.11) The terms in Eq. 2.10 for the entropy flux can be interpreted using Eq. 2.4. The entropy flux is related to the sum of all potentials multiplying their conjugate fluxes. Each extensive quantity in Eq. 2.4 is replaced by its flux in Eq. 2.10. Equation 2.11 can be developed further by introducing the flux of heat, JQ. Applying the first law of thermodynamics to the cell yields (2.12) where Q is the amount of heat transferred to the cell. By comparison with Eq. 2.4 and with the assumption of local equilibrium, dQ/Vo= Tds and therefore
Tu = YQ k c$j&
(2.13)
i
Substituting Eq. 2.13 into Eq. 2.11 then yields (2.14) 4Here, all the extensive densities are treated as conserved quantities. This is not the general case. For example, polarization and magnetization density are not conserved. It can be shown that for nonconserved quantities, additional terms will appear on the righthand side of Eq. 2.11.
2.1: ENTROPY AND ENTROPY PRODUCTION
27
2.1.2 Conjugate Forces and Fluxes Multiplying Eq. 2.14 by T gives (2.15) Every term on the righthand side of Eq. 2.15 is the scalar product of a flux and a gradient. Furthermore, each term has the same units as energy dissipation density, J m3 s’, and is a flux multiplied by a thermodynamic potential gradient. Each term that multiplies a flux in Eq. 2.15 is therefore a force for that flux. The paired forces and fluxes in the entropy production rate can be identified in Eq. 2.15 and are termed conjugate forces and fluxes. These are listed in Table 2.1 for heat, component i, and electric charge. These forces and fluxes have been identified for unconstrained extensive quantities (i.e., the differential extensive quantities in Eq. 2.5 can vary independently). However, many systems have constraints relating changes in their extensive quantities, and these constrained cases are treated in Section 2.2.2. Throughout Chapters 13 we assume, for simplicity, that the material is isotropic and that forces and fluxes are parallel. This assumption is removed for anisotropic materials in Chapter 4. Table 2.1 presents corresponding wellknown empirical forceflux laws that apply under certain conditions. These are Fourier’s law of heat flow, a modified version of Fick’s law for mass diffusion at constant temperature, and Ohm’s law for the ~ mobility, Mi, is defined as electric current density at constant t e m p e r a t ~ r e .The the velocity of component i induced by a unit force. Table 2.1: Selected Conjugate Forces, Fluxes, and Empirical ForceFlux Laws for Systems with Unconstrained Components, i. Extensive Quantity Heat
Flux J;
Conjugate Force
+VT
Component i
x
Vp, = Vat
Charge
J:,
v4
Empirical ForceFlux Law*
J; =  K V T
Fourier’s Modified Fick’s
x = Mzc, V p z
Ohm’s
J’9  pv4
*K = thermal conductivity; Mi = mobility of i; p = electrical conductivity
2.1.3 Basic Postulate of Irreversible Thermodynamics The basic postulate of irreversible thermodynamics is that, near equilibrium, the local entropy production is nonnegative: (2.16) 5Under special circumstances, this form of Fick’s law reduces to the classical form where D , is the mass diffusivity (see Section 3.1 for further discussion).
& = D,
Vc,,
28
CHAPTER 2 : IRREVERSIBLETHERMODYNAMICS.COUPLED FORCES AND FLUXES
Using the empirical laws displayed in Table 2.1, the entropy production can be identified for a few special cases. For instance, if only heat flow is occurring, then, using Eq. 2.15 and Fourier’s heatflux law,
& = K
VT
(2.17)
results in (2.18) which predicts (because of Eq. 2.16) that the thermal conductivity will always be positive. If diffusion is the only operating process,
(2.19) i=l
implying that each mobility is always positive.
2.2
LINEAR IRREVERSIBLE THERMODYNAMICS
In many materials, a gradient in temperature will produce not only a flux of heat but also a gradient in electric potential. This coupled phenomenon is called the thermoelectric effect. Coupling from the thermoelectric effect works both ways: if heat can flow, the gradient in electrical potential will result in a heat flux. That a coupling between different kinds of forces and fluxes exists is not surprising; flows of mass (atoms), electricity (electrons), and heat (phonons) all involve particles possessing momentum, and interactions may therefore be expected as momentum is transferred between them. A formulation of these coupling effects can be obtained by generalization of the previous empirical forceflux equations. 2.2.1
General Coupling between Forces and Fluxes
In general, the fluxes may be expected to be a function of all the driving forces acting in the system, Fi; for instance, the heat flux JQ could be a function of other forces in addition to its conjugate force FQ;that is,
Assuming that the system is near equilibrium and the driving forces are small, each of the fluxes can be expanded in a Taylor series near the equilibrium point
2.2: LINEAR IRREVERSIBLE THERMODYNAMICS
29
FQ = Fq = F1 = . . . = FN, = 0. To first order:
or in abbreviated form, (2.21)
where (2.22)
is evaluated at equilibrium (Fp = 0, for all P).6 In this approximation, the fluxes vary linearly with the forces. In Eqs. 2.20 and 2.22, the diagonal terms; L,,, are called direct coeficients; they couple each flux to its conjugate driving force. The offdiagonal terms are called coupling coeficients and are responsible for the coupling effects (also called cross efSects) identified above. Combining Eqs. 2.15 and 2.21 results in a relation for the entropy production that applies near equilibrium:
T C=~ P
CL,~F,F~
(2.23)
a
The connection between the direct coefficients in Eq. 2.21 and the empirical forceflux laws discussed in Section 2.1.2 can be illustrated for heat flow. If a bar of pure material that is an electrical insulator has a constant thermal gradient imposed along it, and no other fields are present and no fluxes but heat exist, then according t o Eq. 2.21 and Table 2.1,
JG = LQQ(  T1V T )
(2.24)
Comparison with Eq. 2.17 shows that the thermal conductivity K is related to the direct coefficient LQQ by
K = LQQ T
(2.25)
6Note that the fluxes and forces are written a: scalars,+cons@te@ with the assumption that the F Q be written as ranktwo material is isotropic. Otherwise, terms like JQ = ( ~ J Q / ~ F Q )must tensors multiplying vectors, and the equations that result can be written as linear relations (see Section 4.5 for further discussion).
30
CHAPTER 2 : IRREVERSIBLE THERMODYNAMICS: COUPLED FORCES AND FLUXES
If the material is also electronically conducting, the general forceflux relationships are (2.26) JQ = LQQFQ+ LQqFq Jq
= LqQFQ
+LwFq
(2.27)
If a constant thermal gradient is imposed and no electrically conductive contacts are made at the ends of the specimen, the heat flow is in a steady state and the chargedensity current must vanish. Hence Jq = 0 and a force LqQFQ
F4 
(2.28)
LW
will arise. The existence of the force Fq indicates the presence of a gradient in the electrical potential, V4, along the bar. Therefore, using Eqs. 2.28 and 2.26,
LQQ
1 4,
LQqLqQ
pQ = 
[% 1
TL4,
VT= KVT
(2.29)
In such a material under these conditions, Fourier's law again pertains, but the thermal conductivity K depends on the direct coefficient LQQ,as in Eq. 2.25, as well as on the direct and coupling coefficients associated with electrical charge flow. In general, the empirical conductivity associated with a particular flux depends on the constraints applied to other possible fluxes. 2.2.2
ForceFlux Relations when Extensive Quantities are Constrained
In many cases, changes in one extensive quantity are coupled to changes in others. This occurs in the important case of substitutional components in a crystal devoid of sources or sinks for atoms, such as dislocations, as explained in Section 11.1. Here the components are constrained to lie on a fixed network of sites (i.e., the crystal structure), where each site is always occupied by one of the components of the system. Whenever one component leaves a site, it must be replaced. This is called a network constraint [l].For example, in the case of substitutional diffusion by a vacancyatom exchange mechanism (discussed in Section 8.1.2), the vacancies are one of the components of the system; every time a vacancy leaves a site, it is replaced by an atom. As a result of this replacement constraint, the fluxes of components are not independent of one another. This type of constraint will be absent in amorphous materials because any of the N , components can be added (or removed) anywhere in the material without exchanging with any other components. The dNi will also be independent for interstitial solutes in crystalline materials that lie in the interstices between larger substitutional atoms, as, for example, carbon atoms in bodycentered cubic (b.c.c.) Fe, as illustrated in Fig. 8.8. In such a system, carbon atoms can be added or removed independently in a dilute solution. When a network constraint is present, NC
Y d N ,= 0 u i=l
(2.30)
2.2: LINEAR IRREVERSIBLE THERMODYNAMICS
Solving Eq. 2.30 for
d N N C and
31
putting the result into Eq. 2.3 yields
Tds = du
+ dw  C (pi  P N , ) N,l
dci
(2.31)
i=l
Starting with Eq. 2.31 instead of Eq. 2.3 and repeating the procedure that led to Eq. 2.15, the conjugate force for the diffusion of component i in a networkconstrained crystal takes the new form
Fi = v (Pi P N , ) 4
(2.32)
The conjugate force for the diffusion of a networkconstrained component i therefore depends upon the gradient of the difference between the chemical potential of component i and N, rather than on the chemical potential gradient of component i alone. If in the case of substitutional diffusion by the vacancy exchange mechanism, the vacancies are taken as the component N,, the driving force for component i depends upon the gradient of the difference between the chemical potential of component i and that of the vacancies. The difference arises because, during migration, a site’s state changes from occupancy by an atom of type i to occupancy by a vacancy. This result has been derived and extended by Larch6 and Cahn, who investigated coherent thermomechanical equilibrium in multicomponent systems with elastic stress fields [l41. In the development above, the choice of the N,th component in a system under network constraint system is arbitrary. However, the flux of each component in Eq. 2.21 must be independent of this choice [3, 41. This independence imposes conditions on the Lap coefficients. To demonstrate, consider a threecomponent system at constant temperature in the absence of an electric field, where components A , B , and C correspond to i = 1, 2, and 3, respectively. If component C is the N,th component, Eqs. 2.21 and 2.32 yield  PC)  LABV(PB  PC)
f A = LAAv(PA
~
JB =  L B A v ( P A
fc
= LCAV(PA  ~
c)L B B v ( P B
c)L C B V ( P B
~
c ) ~ c )
(2.33)
On the other hand, if B is the N,th component,
JL =  L A A ~ ( PAP B )  L A C ~ ( PCP B ) J A =  L B A ~ ( PAP B )  L B C ~ ( PCP B ) + +
& = LCAV(PA Because $ must be the same as Eqs. 2.33 and 2.34 imply that
<
 P B )  ~ c c v ( pcP B )
and the gradient terms are not necessarily zero,
+ + +
(2.35)
Lij = 0
(2.36)
+ + +
LAA LAB LAC= 0 L B A LBB LBC= 0 LCA LCB L c C = 0 or generally,
(2.34)
c NC
j=1
32
CHAPTER 2 : IRREVERSIBLE THERMODYNAMICS: COUPLED FORCES AND FLUXES
If the lattice network defines the coordinate system in which the fluxes are measured, the network constraint requires that (2.37) i=l
and this imposes the further condition on the Lij that
C Lij 2=1
=0
(2.38)
In other words, the sum of the entries in any row or column of the matrix L,, is zero. The conjugate forces and fluxes that are obtained when the only constraint is a network constraint are listed in Table 2.2. However, there are many cases where further constraints between the extensive quantities exist. For example, suppose that component 1 is a nonuniformly distributed ionic species that has no network constraint. Each ion will experience an electrostatic force due to the local electric field, as well as a force due to the gradient in its chemical potential. This may be demonstrated in a formal manner with Eq. 2.5, noting that dq in this case is not independent of dcl but, instead, dq = q l d q , where q1 is the electrical charge per ion assuming that all electric current is carried by ions. Thus dq and dcl can be combined in Eq. 2.5 into a single term ( p 1 + q l @ ) d c l , and when this term is carried through the process leading to Eq. 2.15, the ion flux, A , is found to be conjugate t o an ionic force Fl = V(p1+ q14) (2.39) The potential that appears in the total force expression is the sum of the chemical potential and the electropotential of the charged ion. This total potential is generally called the electrochemical potential. Additional forces would be added to the chemical potential force if, for example, the particle possessed a magnetic moment and a magnetic field were present. As will be seen, many possibilities for total forces exist depending upon the types of components and fields present. Table 2.2: Conjugate Forces and Fluxes for Systems with NetworkConstrained Components, i Quantity
Heat Component i Charge
2.2.3
Flux
Conjugate Force
J;k
$VT V ( p z  p N , ) = vQ., V#
J:,
Introduction of the Diffusion Potential
Any potential that accounts for the storage of energy due to the addition of a component determines the driving force for the diffusion of that component. The
33
2 2 , LINEAR IRREVERSIBLE THERMODYNAMICS
sum of all such supplemental potentials, including the chemical potential, appears as the total conjugate force for a diffusing component and is called the diffusion potential for that component and is represented by the symbol @.’ The conjugate force for the flux of component 1 will always have the form
.
FI = Val
(2.40)
and thus for the special case leading to Eq. 2.39, a1
2.2.4
= p1
+ 414
(2.41)
Onsager’s Symmetry Principle
Three postulates were utilized to derive the relations between forces and fluxes: 0
0 0
The rate of entropy change and the local rate of entropy production can be inferred by invoking equilibrium thermodynamic variations and the assumption of local equilibrium. The entropy production is nonnegative. Each flux depends linearly on all the driving forces.
These postulates do not follow from statements of the first and second laws of thermodynamics. Onsager’s principle supplements these postulates and follows from the statistical theory of reversible fluctuations [5]. Onsager’s principle states that when the forces and fluxes are chosen so that they are conjugate, the coupling coefficients are symmetric: L a p = Lp, (2.42) which simplifies the coupled forceflux equations and has led to experimentally verifiable predictions [6]. Furthermore, Eq. 2.42 guarantees that all the eigenvalues of Eq. 2.21 will be real numbers. Also, the quadratic form in Eq. 2.23 together with Eq. 2.16 implies that the kinetic matrix ( L a p ) will be positive definite; all the eigenvalues are nonnegative .a Equation 2.42 can be rewritten (2.43)
This equation shows that the change in flux of some quantity caused b y changing the direct driving force for another is equal to the change an flux of the second quantity caused b y changing the driving force for the first. These equations resemble the Maxwell relations from thermodynamics. 7The potential is an aggregate of all reversible work terms that can be transported with the species i. Using Lagrange multipliers, Cahn and Larch6 derive a potential that is a sum of the diffusant’s elastic energy and its chemical potential [4].Cahn and Larch4 coined the term diffusion potential to describe this sum. Our use of the term is consistent with theirs. sPositive definite means that the matrix when left and rightmultiplied by an arbitrary vector will yield a nonnegative scalar. If the matrix multiplied by a vector composed of forces is proportional to a flux, it implies that the flux always has a positive projection on the force vector. Technically, one should say that Lap is nonnegative definite but the meaning is clear.
34
CHAPTER 2 IRREVERSIBLE THERMODYNAMICS COUPLED FORCES AND FLUXES
The statisticalmechanics derivation of Onsager's symmetry principle is based on microscopic reversibility for systems near equilibrium. That is, the time average of a correlation between a driving force of type Q and the fluctuations of quantity /3 is identical with respect to switching ct and /3 [6]. A demonstration of the role of microscopic reversibility in the symmetry of the coupling coefficients can be obtained for a system consisting of three isomers, A, B , and C [7,8]. Each isomer can be converted into either of the other two, without any change in composition. Assuming a closed system containing these molecules at constant temperature and pressure, the rate of conversion of one type into another is proportional to its number, with the constant of proportionality being a rate constant, K (Fig. 2.1). The rates at which the numbers of A, B , and C change are then
dNA    (KAC
+ K A B ) N A+ KBANB+ KCANC
dt
+ +
+
dNB = KABNA (KBC K B A ) N B KCBN c dt dNc =KACNA KBCNB (KCA KCB)NC dt
+
(2.44)
At equilibrium, the time derivatives in Eq. 2.44 vanish. Solving for equilibrium in a closed system ( N A NB NC = Ntot)yields
+
Neq = A
K , Ntot K,+K~+K,
where
+
K7Ntot Neq K,+K~+K~
Neq KpNtot K,+K~+K,
(2.45)
+ + +
K , E KBAKCA KBAKCB + KCAKBC Kp KCBKAB KCBKAC + KABKCA (2.46) K7 E KACKBC KACKBA + KBCKAB For the system near equilibrium, let YAbe the difference between the number of A and its equilibrium value, YA= NA  N:q. Introducing this relationship and similar ones for B and C into Eq. 2.44, d Y =A
dt
+ KBAYB+ KCAYC (KAc + KABIYA B
C
Figure 2.1: Schematic conversion diagram for type A , B , and C molecules.
(2.47)
2.2: LINEAR IRREVERSIBLE THERMODYNAMICS
35
with similar expressions for B and C . If Henry's law is obeyed, the activity coefficient is constant and expanding the chemical potential (Eq. 2.2) near equilibrium (small Y A / N yields ~~) (2.48) Substituting Eq. 2.48 into Eq. 2.47 and carrying out similar procedures for B and C,
These constitute a set of linear relationships between the potential differences pz p:q, which drive the Y , toward equilibrium and their corresponding rates, d Y , / d t . In terms of the Onsager coefficients, they have the form
+ + % = LBAFA+ LBBFB+ LBCFC = LAAFA LABFB LACFC
di
+ L C B F B + LCCFC
(2.50)
3 LCAFA
When microscopic reversibility is present in a complex system composed of many particles, every elementary process in a forward direction is balanced by one in the reverse direction. The balance of forward and backward rates is characteristic of the equilibrium state, and detailed balance exists throughout the system. Microscopic reversibility therefore requires that the forward and backward reaction fluxes in Fig. 2.1 be equal, so that
K B AN i p= Ka K A B NEq Kp eq KCB NB = Kp KBC Nzq K, KAC N~ = Kr KCA Nip Ka
+
+
KBAKCA KBAKCB KCAKBC KCBKAB+ KCBKAC+ KABKCA = KCBKAB + KCBKAC+ KABKCA KACKBC K A C K B A +KBCKAB = KACKBC + K A C K B A+ KBCKAB KBAKCA + K B A K C B+ KCAKBC
+
(2.51)
Comparison of Eq. 2.50 with Eqs. 2.49 and 2.51 shows that L,, = L,, and therefore demonstrates the role of microscopic reversibility in the symmetry of the Onsager coefficients. More demonstrations of the Onsager principle are described in Lifshitz and Pitaerskii [6] and in Yourgrau et al. [8]. Solving Exercise 2.5 shows that the products of the forces and reaction rates in Eq. 2.49 appear in the expression for the entropy production rate for the chemical reactions. The forces and reaction rates are therefore conjugate, as expected. Bibliography 1. F.C. Larch6 and J.W. Cahn. A linear theory of thermochemical equilibrium of solids under stress. Acta Metall., 21(8):10511063, 1973.
36
CHAPTER 2 : IRREVERSIBLE THERMODYNAMICS COUPLED FORCES AND FLUXES
2. F.C. Larch6 and J.W. Cahn. A nonlinear theory of thermomechanical equilibrium of solids under stress. Acta Metall., 26(1):5360, 1978. 3. J.W. Cahn and F.C. Larch& An invariant formulation of multicomponent diffusion in crystals. Scripta Metall., 17(7):927937, 1983.
4. F.C. Larch6 and J.W. Cahn. The interactions of composition and stress in crystalline solids. Acta Metall., 33(3):331367, 1984.
5. L. Onsager. Reciprocal relations in irreversible processes. 11. Phys. Rev., 38( 12):22652279, 1931. 6. E.M. Lifshitz and L.P. Pitaevskii. Statistical Physics, Part 1. Pergamon Press, New York, 3rd edition, 1980. See pages 365ff. 7. K. Denbigh. The Principles of Chemical Equilibrium. Cambridge University Press, New York, 3rd edition, 1971.
8. W. Yourgrau, A. ven der Merwe, and G. Raw. Treatise on Irreversible and Statistical Thermophysics. Dover Publications, New York, 1982.
EXERCISES
2.1 Using an argument based on entropy production, what can be concluded about the algebraic sign of the electrical conductivity? Solution. If electronic conduction is the only operative process in a material at constant T, then Eq. 2.15 reduces t o TU=&.Vc$ (2.52) Using Ohm's law, Because U
& = pV4,
TU = p 10c$l2
2 0 and lVc$12is positive,
(2.53)
p must be positive.
2.2 An isolated bar of a good electrical insulator contains a rapidly diffusing unconstrained solute (i.e., component 1). Impose a constant thermal gradient along the bar, and find an expression for its thermal conductivity when the system reaches a steady state. Assume that no solute enters or leaves the ends of the bar. Express your result in terms of any of the Lap coefficients in Eq. 2.21 that are required. Solution. Using a similar method as the development that led t o Eq. 2.29, the relevant linear forceflux relations are
+ Ji = L Q F Q + L i F i
JQ = LQQFQ L Q ~ F I
(2.54)
The cross effect between the thermal and diffusion currents causes a redistribution of the unconstrained solute until a steadystate distribution is reached. In this condition 51 = 0 and, therefore, F1 =  F Q ( L ~ Q / L ~Putting ~ ) . this result into Eq. 2.54 then vields
The expression for K is similar t o Eq. 2.29, where electrical charge rather than component 1 was forced into a steadystate distribution by the thermal flux.
2.3 A common device used to measure temperature differences is the thermocouple in Fig. 2.2. Wires of metals A and B are connected with their common
37
EXERCISES
junction at the temperature T + A T and the opposite ends connected t o the terminals of a potentiometer maintained at temperature T . The potentiometer measures a voltage, + A B , across terminals 1 and 2 under conditions where no electric current is flowing. This voltage is then a measure of A T . Explain this effect, known as the Seebeck effect, in terms of relevant forces and fluxes. 1
I
I I
Potentiometer
+Temperature
T
I I I
1
I
L
Figure 2.2:
I      ,Temperature
T+AT
Thermocouple composed of metals A and B with a junction at one end.
Solution. The appropriate forceflux equation for this case is
Jq
d4 + Lq,Fq =  L , Q1?dT; ~  L "dx
= L¶QFQ
(2.56)
where, t o a good approximation, 2 measures the distance along the wire. Setting Jq = 0,
d4
LYQ L,, T
dT
(2.57)
The potentials a t 1 and 2 relative t o the potential at the junction are determined by integrating Eq. 2.57 along each wire. They will difFer because the A and B wires possess is then the difference between different values o f the coefficients L,Q and L y q , ~ A B these t w o potentials.
2.4 Figure 2.3 depicts an apparatus at constant uniform temperature. The bat
tery drives an electrical current around the circuit. Heat is absorbed a t one AIB junction and emitted at the other. Explain this phenomenon, known as the Peltier effect, in terms of relevant forces and fluxes. A
Figure 2.3:
Peltier effect apparatus coiriposed of metnl wires A and H
38
CHAPTER 2: IRREVERSIBLE THERMODYNAMICS:COUPLED FORCES AND FLUXES
Solution. Both heat and electrical charge currents will be present in the wire, and the generalized linear relationships are therefore
+
1dT d4 T d x  L Q X, ~ 1 dT d4 LqqFq=  L q 4 T d x  L q qd x
JQ = LQQFQ LQ,F, 5, = L,QFQ
+
= LQQ
(2.58) (2.59)
where, t o a good approximation, z measures distance along the wires. Because d T / d z = 0, JQ = LQ4 Jq (2.60) Lqq
Equation 2.60 shows that the electrical current will drive a heat current along each wire by an amount dependent upon the coupling coefFicient LQ, and the direct coefficient L,,. These coefFicients will have different values in the A and B wires, and therefore heat will accumulate (and be emitted) a t one junction and be absorbed at the other.
2.5 Show that products of the "forces" [i.e., the quantities (p:"  p i ) ] , and the
rates of reaction (i.e., the d Y , / d t ) which are present in Eq. 2.49 appear in the expression for the rate at which entropy is produced by the corresponding reactions. These quantities are therefore conjugate to one another just as are the conjugate forces and fluxes in Table 2.1. Obtain a general expression for the rate at which entropy is produced: the reactions are taking place in a container maintained at constant temperature and pressure. 0
0
The surroundings may be regarded as a reservoir at constant temperature and pressure. It may be necessary to transfer a quantity of heat, dQ, from the reservoir into the system in order to maintain constant temperature in the system; the total entropy change of the system plus reservoir, dS', will then be
dQ T
dS' = dS  
(2.61)
where dS and dQ/T are the entropy changes of the system and surroundings, respectively. For the system, du = dQ  PdV, and therefore dS' = 0
TdS  02.4  PdV T
(2.62)
Note that 6 = U + PV  T S , and applying the constant temperature and pressure condition, (2.63)
0
+
Equation 2.63, Q = U PV  T S , and Eq. 2.1 can be combined in the expression for the rate of entropy production: (2.64) T,P
i
EXERCISES
39
Solution. From Eq. 2.64,
B u t dNi/dt = d Y i / d t , and therefore
Suppose that the system is a t equilibrium with all three species at their equilibrium chemical potentials. We then make small changes in their numbers subject to the conservation condition NA N B Nc = N~'' (2.67)
+
+
Since in general for a system a t constant T and P ,
dG = P A dNA
+
/.LBdNB
+ pc d N c
(2.68)
the change in free energy of the system a t equilibrium will be
dG = p: dNA +/.LzdNB+pL',4dNc = 0 Since Y , = Ni
(2.69)
 Nteq, py d Y A tp z d Y B f p z dYc = 0
(2.70)
and
(2.71) adding Eqs. 2.66 and 2.71 then produces (2.72)
CHAPTER 3
DRIVING FORCES AND FLUXES FOR DIFFUSION
Fluxes of chemical components may arise from several different types of driving forces. For example, a charged species tends to flow in response to an applied electrostatic field; a solute atom induces a local volume dilation and tends to flow toward regions of lower hydrostatic compression. Chemical components tend to flow toward regions with lower chemical potential. The last caseflux in response to a chemical potential gradientleads to Fick’s first law, which is an empirical relation between the flux of a chemical species, $, and its concentration gradient, V c i in the form $ = DVci, where the quantity D is termed the mass diffusivity. Because different driving forces can arise for a chemical species and because the mechanisms of diffusion comprising the microscopic basis for D are essentially independent of the driving force, all the driving forces can be collected and attributed to the generalized diffusion potential, CJ,introduced in Chapter 2. The flux of a component in a solution can be complicated because components cannot always diffuse independently. This complication necessitates the introduction of different types of diffusion coefficients defined in specified reference frames to distinguish different diffusion systems.
3.1 DIFFUSION I N PRESENCE OF A CONCENTRATION GRADIENT If a concentration gradient exists in a single phase at uniform temperature that is free of all other fields and any interfaces, that component’s diffusion potential is identical to its chemical potential. The gradient in this potential is the driving Kinetics of Materials. By Robert W . Balluffi, Samuel M. Allen, and W . Craig Carter. Copyright @ 2005 John Wiley & Sons, Inc.
41
42
CHAPTER 3 DRIVING FORCES AND FLUXES FOR DIFFUSION
force for diffusion. A diffusional flux proportional to the diffusion potential gradient will then arise, as discussed in Chapter 2. However, it is much easier to determine a concentration gradient by experiment than a diffusion potential gradient. It is therefore convenient to use a thermodynamic model of the solution to express the chemicalpotential gradient in terms of a concentration gradient. The result is a diffusional flux proportional to the concentration gradient. The factor coupling the flux and concentration gradient is termed a diffusivity (or diffusioncoefficient),D , so that Fick’s first law in the form
J’=
DVc
(3.1)
applies. The flux and corresponding diffusivity in this relationship must always be specified relative to a particular reference frame (coordinate system) [I, 21.
3.1.1
SelfDiffusion: Diffusion in the Absence of Chemical Effects
During selfdiffusion in a pure material, whether a gas, liquid, or solid, the components diffuse in a chemically homogeneous medium. The diffusion can be measured using radioactive tracer isotopes or marker atoms that have chemistry identical to that of their stable isotope. The tracer concentration is measured and the tracer diffusivity (selfdiffusivity) is inferred from the evolution of the concentration profile. Figure 3.1 shows a diffusion couple containing a concentration gradient of the tracer atoms that could be used for this purpose. For a crystal where selfdiffusion takes place by the vacancyexchange mechanism, the Fick’s law flux equation can be derived.l Such a crystal is networkconstrained and has three componentsinert atoms, radioactive atoms, and vacancies [3]. Planes of atoms provide a local reference frame to quantify the fluxes of these components by allowing the count of the number of atoms that cross a unit area of crystal plane per unit time. The crystal remains rigidly fixed during selfdiffusion, and therefore these planes constitute a convenient single reference frame, called the crystal frame, or Cframe, for measuring flux. At constant temperature, with vacancies chosen as the N,th
W
0
Distance

W
Figure 3.1: Diffusion couple for measuring selfdiffusion in pure material. A small coriceritratioii of a radioactive isotope of component 1. c4,, is present initially on the left side of the couple. During diffusion, the radioactive particles will diffuse in the chemically homogeneous couple and become inteririixed with the inert particles. ’The vacancy exchange mechanism is described in Section 8.1.2.
3 1 . CONCENTRATION GRADIENTS AND DIFFUSION
43
component, Eq. 2.21 combined with Eq. 2.32 takes the form (for onedimensional isotropic diffusion)
where the star indicates the radioactive species, and the superscript C indicates that the flux of i is measured in a CframeS2 These equations are derived from the vacancyexchange mechanism; every forward jump of an atom occurs via a backward jump of a vacancy. The vacancies are assumed to be in thermodynamic equilibrium throughout, and therefore p v = 0.3 c1 c.1 cv = A , where A is a constant and typical vacancy atomic fractions are less than The chemical potentials of species 1 and 1 are given by Eq. 2.2 with Raoultian behavior (i.e., y1 = y*1 = 1). Therefore, d p i / d x = kTdlnci/dx. Because of the assumption of uniform vacancy equilibrium, c1 c.1 = A  cv is also uniform. Equations 3.2 become
+ +
+
[,
dcq J$ =  IcT Lq*1  L*11 Finally, because J$ = 0 and JY
ax
(3.3)
+ JZ = 0,
Equation 3.4 shows that the selfdiffusion of the radioactive tracers obeys Fick's law with a selfdiffusivity designated by *D. 'The vector notation is dropped when there is only one spatial dimension. Unless indicated otherwise, the diffusion is assumed to be isotropic in this chapter. Anisotropic diffusion is treated in Section 4.5. 3The vacancy chemical potential is defined by pv = ( a G / a N v ) ~ , pthat , is, by the freeenergy increase of a large system when a vacancy is created at a source such as a dislocation or a grain boundary. Dislocations act as vacancy sources as they climb in one direction and as sinks (i.e., negative sources), as they climb in the other. Throughout this book we generally refer to vacancy sources with the understanding that source and sink behavior are complementary (see Section 11.4). When this freeenergy change is zero (i.e., pv = 0), the system will be in a minimum freeenergy state with respect t o vacancy formation. The vacancy concentration at the source is then in local equilibrium. Assuming that pv is uniformly zero in a system requires an adequate density of vacancy sources.
44
CHAPTER 3: DRIVING FORCES AND FLUXES FOR DIFFUSION
3.1.2 SelfDiffusion of Component
i
in a Chemically Homogeneous Binary
Solution
In Section 3.1.1, the selfdiffusivity was obtained for a diffusion couple composed of a chemically pure material but with gradients of an isotope of that material. In this section we discuss selfdiffusion of an isotopic species in a chemically homogeneous binary solution consisting of atoms of types 1 and 2 in the presence of a concentration gradient of the isotope. The selfdiffusion of component 1 in such a system is measured by studying the diffusion of a radioactive isotope tracer of component 1 (i.e., q)under the condition that while there is a gradient in the tracer's concentration, c*1, the sum (c1 c q ) and c2 are both uniform. A possible diffusion couple is shown in Fig. 3.2. Considering Eq. 2.21 in a case in which diffusion occurs in a crystal by the vacancy exchange mechanism, there are four components, c1, c*1, c2, and cv. Because the crystal remains fixed during the diffusion, the Cframe is again used for measuring the flux. The system is chemically homogeneous, so
+
Again, a Fick'slaw expression is obtained for the selfdiffusion of the radioactive component. The selfdiffusivity of component 1 in a binary system of uniform chemical composition is designated by *D1to distinguish it from the selfdiffusivity of a pure material, *D.
t m
0
W
Distance + Figure 3.2:
Diffusion couple for nietlsuring solute selfdiffusion in a binary systein. During diffusion, a c q gradient develops in the chemically homogeneous material.
3.1.3 Diffusion of Substitutional Particles in a Chemical Concentration Gradient
When a solute of type i diffuses on substitutional sites in an inhomogeneous binary solution, both the solute particles and host particles interdiffuse on the substitutional sites. If one species diffuses more quickly than the other, the region initially richer in that species loses net mass and contracts. On the other hand, the region initially richer in the more slowly diffusing species gains net mass and expands. This process, which establishes a mass flow in the system, is known as the Kirkendall efSect after E. Kirkendall, who along with A. Smigelskas first observed it in crystalline metals [4].
3 1 CONCENTRATION GRADIENTS AND DIFFUSION
45
Description of the Diffusion in a Local CFrame. Figure 3.3 illustrates a crystalline binary system in which interdiffusion occurs along x by a vacancy mechanism. The crystal is no longer fixed in structure as during selfdiffusion but is flowing due to the Kirkendall effect, and its local planes are moving with a velocity, ~ ( x )with . respect to the ends of the sample. Although no unique Cframe exists throughout the diffusing crystal, a local Cframe with a small inert marker particle to indicate its origin can be fixed to any plane as illustrated. The distribution of the fasterdiffusing solute (i = 1) is also shown in Fig. 3.3a. If the diffusion fluxes are measured at any point in the diffusion zone with respect to its local Cframe, the constraint condition associated with the vacancy mechanism requires that the fluxes satisfy
In the Kirkendall effect, the difference in the fluxes of the two substitutional species requires a net flux of vacancies. The net vacancy flux requires continuous net vacancy generation on one side of the markers and vacancy destruction on the other side (mechanisms of vacancy generation are discussed in Section 11.4). Vacancy creation and destruction can occur by means of dislocation climb and is illustrated in Fig. 3.3b for edge dislocations. Vacancy destruction occurs when atoms from the extra planes associated with these dislocations fill the incoming vacancies and the extra planes shrink (i.e.. the dislocations climb as on the left side in Fig. 3.3b toward which the marker is moving). Creation occurs by the reverse process, where the extra planes expand as atoms are added to them in order to form vacancies, as on the right side of Fig. 3.3b. This contraction and expansion causes a mass flow that is revealed by the motion of embedded inert markers. as indicated in Fig. 3.3 [4]. jii + Tc + j i i 2
v
= 0
Figure 3.3: Schematic illustration of the Kirkeridall effect in a binary crystalline material diffusing by the vacancy mechanism. The sketch illustrates dislocation motion at, some t,ime aft>erthe diffusion couple’s initial condition. (a) Concentration vs. distance profile in t,he diffusion zone. An embedded inert marker is present moving with the velocity. v. and fluxes in the local Cframe associated with t,he marker are iridica.ted. (b) Local arrarigemerit of at,om plaries across the diffusion zone near the marker. Arrows indicate clirrih movements of niiinerous edge dislocations that occur when there is a net diffusion of vacancies from right to left,.
46
CHAPTER 3: DRIVING FORCES AND FLUXES FOR DIFFUSION
In this process, the net flux of substitutional atoms across the interface plane results in local volume changes (i.e., as a crystal plane is removed by climb, the crystal contracts in a direction normal to the plane). However, free expansion in directions parallel to the interface plane is constrained by the specimen ends, where significant diffusion has not occurred, and by the coherence of the interface between the expanding and contracting regions. Therefore, dimensional changes parallel t o the interface (i.e., normal to the diffusion direction) are restricted, and inplane compatibility stresses are generated. No outofplane compatibility stresses develop because the diffusion couple can expand freely in the diffusion direction. In diffusion specimens that have a relatively narrow diffusion zone compared to the extent of the specimen in the diffusion direction, compatibility stresses are pure shear stresses, and if the stresses exceed the crystal's yield stress, the onset of plastic flow enables the cross section of the diffusion specimen to remain ~ o n s t a n t . ~ The substitutional binary alloy diffusion illustrated in Fig. 3.3 is discussed in a treatment pioneered by Darken [6] (see also Crank's book "71). The system has three components, species 1, species 2, and vacancies, and is assumed to be at constant pressure and temperature with sites that can only be created or destroyed at sources (i.e., the system is network constrained except at dislocations or interfaces). The fluxes are obtained from Eqs. 2.21 and 2.32:
JF = L i i F i
+
LizF2
= L11 8% LIZ d@2 = L11 d(P1  Pv)  L12d ( P 2  PV)
Jg
+
= L21
8%
+
dX
dX
dX
dX = ~ 5 2 1 ~ 1L22F2
3 3 2
 L22
dX
= L21
d(P1  P V ) dX
dX
 L22
d(P2
(3.7)
 Pv)
dX
and J$ =  ( J f J,C) by Eq. 3.6. Assumption of local equilibrium permits the GibbsDuhem relation to be written (3.8)
A net vacancy flux develops in a direction opposite that of the fastestdiffusing species (species 1 in Fig. 3.3). Nonequilibrium vacancy concentrations would develop in the diffusion zone if they were not eliminated by dislocation climb. However, under usual conditions it is expected that a sufficient density of dislocations will be present to maintain the vacancy concentration near equilibrium IS]. It can therefore be assumed, to a good approximation, that pv = 0, and therefore Vpv = 0 everywhere in the diffusion zone. Using Eqs. 3.7 and 3.8 with Vpv = 0 yields
(3.9)
4When the fasterdiffusing component is diffused from the vapor phase into a thin sheet, and the diffusion zone is relatively wide compared to the sheet thickness, the constraints on the expansion parallel t o the diffusion interface are greatly reduced. Large specimen expansions normal to the diffusion direction have then been observed [5].
3.1 CONCENTRATION GRADIENTS AND DIFFUSION
47
The chemical potential gradients can be related to concentration gradients using pi = p:
+ kTln(yi(R)ci)
(3.10)
which is obtained by combining Eq. 2.2 with Eq. A.12, giving the result
dX
(3.11)
The local volume expansion arising from the local change of composition contributes t o diffusion via the derivative of the average site volume (R).5 The derivative of 71 is the contribution associated with the nonideality of the solution. Putting Eq. 3.11 into Eq. 3.9 yields a flux that is proportional to the concentration gradient:
This is a form of Fick’s law for a chemically inhomogeneous material where the intrinsic diffusivity, designated by D1, measures the flux in the local Cframe. A similar procedure for component 2 yields an analogous Fick’slaw expression, J,C =  D z d c a / d ~ . The selfdiffusivity of species 1 in a chemically homogeneous solution of concentration c1, corresponding to *D1 in Eq. 3.5, can be compared with the intrinsic diffusivity of the same species in a chemically inhomogeneous solution at the same concentration, corresponding to D1 in Eq. 3.12. Typically, in addition to the approximation of a concentrationindependent average site volume (O), it is reasonable to assume that the coupling (offdiagonal) terms, Ll2/c2 and Ll*l/c*l in Eqs. 3.5 and 3.12, are small compared with the direct term Lll/cl. In this approximation, (3.13) The primary difference between D1 and *D1 is a thermodynamic factor involving the concentration dependence of the activity coefficient of component 1. The thermodynamic factor arises because mass diffusion has a chemical potential gradient as a driving force, but the diffusivity is measured proportional to a concentration gradient and is thus influenced by the nonideality of the solution. This effect is absent in selfdiffusion. At this point it has been shown that the fluxes of species 1 and 2 can be described by Fick’slaw expressions involving two different intrinsic diffusivities, D1 and 0 2 , in a local coordinate system (local Cframe) fixed to the lattice plane through which flux is measured. However, because of the Kirkendall effect, these planes (reference frames) move normal to one another at different rates in a nonuniform fashion, and this description is therefore not useful for describing the diffusion throughout the specimen. When there is no change in the total specimen volume, the overall diffusion that occurs during the Kirkendall effect can be described in terms of a single diffusivity (the interdiffusivity) measured in a single reference frame (a volumefixed) frame. 5This expansion can usually be described by Vegard’s law in the form e z j  e:j = Tz3(c  C O ) ; et3 is the strain due to a concentration change, and the six Tz3are the Vegard coefficients.
48
CHAPTER 3: DRIVING FORCES AND FLUXES FOR DIFFUSION
Diffusion in a VolumeFixed Frame (VFrame). To find the volumefixed Vframe, assume that a frame, designated an Rframe, exists that relates all local Cframes [9]. If wf is component i's velocity in this Rframe, w p its velocity in a local Cframe, and w," the local Cframe's velocity measured in the Rframe, then
ci w,p = ci (WF
+ w,")
(3.14)
Because the flux in a local Cframe is the concentration multiplied by its local velocity, J," = ci wf, and using Eq. 3.14, JC = ci (us w,")= Di
dCi
(3.15)
dX
Two equations representing the contributions of components 1 and 2 to the volume flux are obtained by multiplying Eq. 3.15 through by R1 and R2. The sum of these two equations, using Eqs. A.8 and A.lO, is6
w,"  [R1ClW,R+ R2C&]
=
dCl ( D l  D2) R1
(3.16)
dX
Using Eqs. 3.15 (for i = l),3.16, and A.8 yields c1
w1"  c1 [RlCl?J,R+ R2c2.,"]
=  [c2R2D1
+
dCl ClRlDZ] 
dX
(3.17)
The accumulation equation in the Rframe is (3.18) Assuming that R1 and R2 possess constant but generally different values, and thus that there are no changes in overall specimen volume during diffusion, two equations for the component contributions to volume accumulation are obtained by multiplying Eq. 3.18 through by Ri and setting i = 1,2.? The sum of these two equations is the local volume expansion rate in the Rframe. Using Eq. A.8, (3.19) The quantity
+ R ~ C ~ Wcan ; ] therefore be, at most, a function o f t , that is, R ~ c ~ v+ , RR ~ C Z V= , " R1J,R + RzJ,R = f ( t ) (3.20)
[Rlc1w,R
and is the flux of volume passing through a plane in the Rframe. There is a particular Rframe, called the Vframe, for which f ( t ) = 0. In this frame, according to Eq. 3.20,
RiJ,V+R2J,V=O
I[
(3.21)
6For the derivation of Eq. 3.16, cv has been assumed t o be negligible; the exact expression on the  D ~ f l v % . Since the distance over which the species righthand side is ( D l  D2)R1% and the vacancy concentrations vary are similar, the gradient of cv is negligible compared with the gradient of c1 as well. 7The assumption of constant but different R values is generally acceptable. When any small volume changes are taken into account, the analysis of the diffusion becomes more complicated, as discussed elsewhere [2, 7, lo].
[
1
49
3 1 CONCENTRATION GRADIENTS A N D DIFFUSION
and the flux of volume through any plane is zero: hence, the term volumefixed frame. Then. using JY = CJI," and Eqs. 3.16, 3.17, and 3.21,
(3.22) and =
21:.
dCl
(Dl  D2) R1
ax
(3.23)
Equation 3.23 for the velocity of a local Cframe with respect to the Vframe is therefore the velocity of any inert marker with respect to the Vframe. The assumptions that R1 and Q2 are each constant throughout the material. and thus that there are no changes in overall specimen volume during diffusion. permit the use of Eq. 3.19 to derive the unique choice of the Vframe. In Eq. 3.22, the flux of 1 in the Vframe obeys Fick's law and can be written
(3.24) where the binary solution znterdiffusivity,designated by 5. is related to the intrinsic diffusivities of components 1 and 2 (measured in a local Cframe) by the relation

D = ~ l R l D 2+ c ~ R J D ~ which is often approximated through
(3.25)
R1 = Q2 = ( 0 ) as
5 = X1D.2 + X2Dl
(3.26)
Using a similar procedure to find the flux of component 2 in the Vframe yields J" 2

D d C 2
ax
(3.27)
The only remaining task is now to relate the Vframe to a laboratory frame suitable for experimental purposes. This is provided by the laboratory frame (Lframe) illustrated in Fig. 3.4. Here, the ends of the specimen are unaffected by the diffusion and are stationary with respect to each other since there is no change in the overall specimen volume. The specimen ends therefore provide the anchoring points for the rigid laboratory frame fixed to the ends as illustrated. Specimen
f
',
Laboratoryframe
/
0 Distance
Figure 3.4:
x+
Diffiisiori ( oiiplr. specimen with superimposed laboratoryframe (Lframe).
50
CHAPTER 3: DRIVING FORCES AND FLUXES FOR DIFFUSION
We now show that the Lframe in Fig. 3.4 is identical to the Vframe. The fluxes in the two frames are related by
+C ~ U ;
J,” = JY
(3.28)
Using Eq. 3.28 with i = 1 and i = 2 to obtain two equations, multiplying them by R1 and Rz, respectively, then adding them, using Eq. A.8, and differentiating the result with respect to x yields
dJf
01 d X
dJ,v + R2dJ,L d X = 0 1+R2+dX
dJl
dx
dub
dx
(3.29)
However, with the use of Eq. A.lO, (3.30)
and therefore
d=Vt( R 1  + R 2 adJ,v Jr)
ax
dX
(3.31)
dX
which, integrated, gives
(
dub =  R1/
Jt,
x x=L
dJ,YiR2/x
x=L
d~;)
(3.32)
Because J:, and u; are zero at the specimen ends x = ikL, where L is large compared to the diffusion zone width, (3.33)
Therefore, with Eq. 3.21,
u; =  (R,J,v
+ R2J,V) = 0
(3.34)
The Lframe and Vframe are thus identical. Equation 3.23 gives the velocity of the local Cframe with respect to the Vframe (i.e., the velocity of local mass flow measured by the velocity of an embedded inert marker relative to the ends of a diffusion couple such as in Figs. 3.3 and 3.4). The measurement of v,“ and 5 at the same concentration in a diffusion experiment thus produces two relationships involving D1 and D2 and allows their determination. In the Vframe, the diffusional flux of each component is given by a simple Fick’slaw expression where the factor that multiplies the concentration gradient is the interdiffusivity 5. In this frame, the interdiffusion is specified completely by one diffusivity. Chemical interdiffusion on a substitutional lattice can therefore be considered from two viewpoints. In the Vframe, it is described by a single diffusivity (Lee,the interdiffusivity). In a local Cframe fixed with respect to the local bulk material, the material flows locally with the velocity u,“ relative to the Vframe and the description of the fluxes of the two components requires two diffusivities (i.e., the intrinsic diffusivities). These three diffusivities are related by Eq. 3.25, and each is generally a function of the local composition.
3.1 CONCENTRATION GRADIENTS AND DIFFUSION
51
The Kirkendall effect alters the structure of the diffusion zone in crystalline materials. In many cases, the small supersaturation of vacancies on the side losing mass by fast diffusion causes the excess vacancies to precipitate out in the form of small voids, and the region becomes porous [ l l ] . Also, the plastic flow maintains a constant cross section in the diffusion zone because of compatibility stresses. These stresses induce dislocation multiplication and the formation of cellular dislocation structures in the diffusion zone. Similar dislocation structures are associated with hightemperature plastic deformation in the absence of diffusion [12141. In 1946, the Kirkendall effect was observed with inert markers in polymersolvent systems where the large polymer molecules diffused more slowly than the small solvent molecules [15]. Figure 3.5 shows an analogous phenomenon involving interdiffusion of fluids t o help explain marker motion and plastic deformation in solids during the Kirkendall effect. Two fluids comprised of components A and B are encapsulated in a fixed volume and separated in two chambers by a fixed rigid membrane. Initially, there is no pressure difference across the membrane (Le., pAleft + pBleft = p Aright + Pgight), but there is a difference in partial pressures, > Piight. If the osmotic membrane allows rapid diffusion of A but not of B , the pressures and Piight will then relax to equilibrium values until there is no difference in chemical potential across the membrane. This results in a difference in total pressure across the membrane.
Ppft
Ppft
PA
pl¶
Diffusive membrane
(a) Figure 3.5: Interface motion arid cavitatioii during iiiterdifl'usion in Huids. (a)Initial p riglit, p riglit. . (b) Later Sitllstio,l: p;cft > p A r k h + ' , p i c f t < p;igiit,, pAlrft + ,pHlcft A YI t . But Picft< situatioii: Coinpoiient '4 diffuses through rnenilxaiie so that PA]Cft = Plig +
p;inht
pA]eft. + p i c f t
< p;ight
+ p;i&
Consider now the consequences of the pressure difference. If the membrane became free t o move, it would move to the left, compressing the left chamber and expanding the right t o equilibrate the pressure difference (Fig. 3.6a). However, if the membrane is constrained, the fluid may cavitate in the left chamber to relieve the low pressure, as in Fig. 3.6b. This is analogous to the formation of voids in the Kirkendall effect.
Membrane moves (0)
'Cavitation
'
Membrane fixed
(b)
Figure 3.6: Possible consequences of t,tie s i t u s t h i in Fig. 3.5b. (a)If ttie nienilrane is allowed to rriove to tlie left,. the total pressures oil the left and right will become equal. (b) If tlie membrane is held fixed) Cavitation niay occur on tlie left to relieve tlie low pressure.
52
CHAPTER 3: DRIVING FORCES AND FLUXES FOR DIFFUSION
3.1.4
Diffusion of Interstitial Particles in a Chemical Concentration Gradient
Another system obeying Fick’s law is one involving the diffusion of small interstitial solute atoms (component 1) among the interstices of a host crystal in the presence of an interstitialatom concentration gradient. The large solvent atoms (component 2) essentially remain in their substitutional sites and diffuse much more slowly than do the highly mobile solute atoms, which diffuse by the interstitial diffusion mechanism (described in Section 8.1.4). The solvent atoms may therefore be considered to be immobile. The system is isothermal, the diffusion is not network constrained, and a local Cframe coordinate system can be employed as in Section 3.1.3. Equation 2.21 then reduces to + + 5; = L11F1 = L11V@1 = L11Vp1 (3.35) Assuming a dilute solution, Henry’s law [16] applies, and because c1 X1 N c1/c2, an acceptable approximation, using Eq. 2.2, is p1
= py
+ k T In ( K l c l )
<< c2
and
(3.36)
where K1 is a constant. Therefore,
kT Vp1 = VC1 c1
(3.37)
and (3.38)
L11 can be evaluated by introducing the interstitial mobility M I , which is the average drift velocity, i71, gained by diffusing interstitials when a unit driving force is applied, that is, M i kT (3.39) .i” = M1Vp1=  c1 V C l An interstitial drift velocity causes an interstitial flux, (3.40)
so that
JI” =  M l k T V c l
(3.41)
Comparison of Eqs. 3.38 and 3.41 indicates that
L11 = MlCl
(3.42)
In a dilute solution, M I is expected to be independent of the interstitial concentration. Therefore, Eq. 3.41 predicts a diffusive flux which depends linearly on the gradient in concentration. Diffusion is motivated solely by a concentration gradient, consistent with Fick’s law (i.e., Eq. 3.1) involving an intrinsic diffusivity given by
kT D1 = M1kT = L11C1
(3.43)
Equation 3.43, which expresses the link between the mobility and the diffusivity in this case, is known as the NernstEinstein equation.
3.1: CONCENTRATION GRADIENTS AND DIFFUSION
53
The same diffusion can be described within a Vframe. The analysis is identical to that used to obtain Eqs. 3.23, 3.24, and 3.25 except that in this case, 0 2 = 0. The marker velocity is therefore (3.44) and
 dc1
J 1v = D
(3.45)
dX
with the interdiffusivity, 5, given by

D = czR2Dl In general, for dilute concentrations clR1 << 1, and therefore c2R2 3.1.5
(3.46) 1 and 6
D1.
On the Algebraic Signs of Diffusivities
If the rate of entropy production, 6 , is nonnegative, M1 is also nonnegative (see Section 2.1.3) and L11 must be nonnegative. For a Henrian solution, it can be inferred that the diffusivity D1 is also nonnegative. However, there are more complicated cases, such as the concentrated solutions discussed in Section 3.1.3. In cases where the derivative of the chemical potential with respect to the concentration is negative, the postulate of positive entropy production implies a negative diffusivity in Fick's law (an experimental observation of a negative diffusivity is presented in Exercise 3.3). A negative diffusivity leads to an illposed diffusion equation; so, formulations based on fluxes and their conjugate driving forces (e.g., gradients in chemical potentials) are then preferred to Fick's law and indeed are more physical.* 3.1.6
Summary of Diffusivities
Four different types of diffusivities are summarized in Table 3.1. These include the selfdiffusivity in a pure material, *D; the selfdiffusivity of solute i in a binary system, *Di; the intrinsic diffusivity of component i in a chemically inhomogeneous system, Di; and the interdiffusivity, D , in a chemically inhomogeneous system. These diffusivities are applicable only in certain reference frames which are also listed in Table 3.1. In the remainder of this book, the type of diffusivity under discussion will be identified by these symbols when this information is relevant. When a diffusivity is identified in this manner, it may be assumed that the diffusion under consideration is being described in the proper corresponding frame.

8Zllposed means that the solution is unbounded and not robust with respect to initial conditions. In other words, two initial conditions that are very close t o each other will give solutions that are very far apart a short time later.
54
CHAPTER 3: DRIVING FORCES AND FLUXES FOR DIFFUSION
Summary of Definitions and Relationships for Diffusivities Table 3.1: Described in Chapter 3 Symbol
Name ~~~
*D
~~
Relationships ~
~
Selfdiffusivity in a pure material
Reference Frame Cframe or Vframe

*D is the selfdiffusivity in a chemically homogeneous material comprised of only one species. It is usually determined by measuring the diffusion of a radioactive isotope that is chemically indistinguishable from the inert species. Because there is no mass flow, the Cframe is also a Vframe, and either may be used. *D,
Selfdiffusivity of component i in a binary system
D,
E (1
+ %)*D,
Cframe or Vframe
*D, is the selfdiffusivity of component i in a chemically homogeneous binary system. *D, is related to D , as indicated. *D, is usually determined using an isotope. Because there is no net mam flow, the Cframe is also a Vframe, and either may be used. D,
Intrinsic diffusivity
xv 57" D,VC, +
= D,Vc,
=
G ~ C ,
Local Cframe Vframe
D , is the compositiondependent intrinsic diffusivity of component i in a chemically inhomogeneous system. In a binary system, it relates the flux of component i to its corresponding concentration gradient via Fick's law in a local Cframe (which is fixed with respect to the local bulk material of the diffusing system) and is moving with a velocity w with respect to the corresponding Vframe. The D, are related to 5 as indicated.

D
Interdiffusivity
= DVci D = $' clRlD2 + c2R2D1
Vframe Vframe
6 is the compositiondependent interdiffusivity in a chemically inhomogeneous system. In a binary system, it relates the flux of either component 1 or 2 to its corresponding concentration gradient via Fick's law in a Vframe.
3.2 M A S S DIFFUSION IN A N ELECTRICAL P O T E N T I A L GRADIENT A gradient in electrostatic potential can produce a driving force for the mass diffusion of a species, as discussed in Section 2 . 2 . 2 . Two examples of this are the potentialgradientinduced diffusional transport of charged ions in ionic conductors such as those used in solidelectrolyte batteries and the electroncurrentinduced diffusion of interstitial atoms in metals.
55
3 2 ELECTRICAL POTENTIAL GRADIENTS AND DIFFUSION
3.2.1 Charged Ions in tonic Conductors Consider an ionic material that contains a dilute concentration of positively charged ions that diffuse interstitially (interstitial diffusion is described in Section 8.1.4). 5 is the interdiffusivity of these ions in the absence of any field. As shown in Sections 2.2.2 and 2.2.3, if an electric field, E' = V@, is applied, the diffusion potential will be the electrochemical potential given by Eq. 2.41. According to Eq. 2.21, the flux of charged interstitials is (3.47) Using Eqs. 3.36 and 3.43, Eq. 3.47 takes the form (3.48) In the absence of a significant concentration gradient, the corresponding flux of charge is then (3.49) By comparison with Ohm's law,
6 = pV$,
the electrical conductivity, p, is (3.50)
The conductivity is therefore directly proportional to the diffusivity. 3.2.2
Electromigration in Metals
An applied electrical potential gradient can induce diffusion (electromigration) in metals due to a cross effect between the diffusing species and the flux of conduction electrons that will be present. When an electric field is applied to a dilute solution of interstitial atoms in a metal, there are two fluxes in the system: a flux of conduction electrons, J q , and a flux of the interstitials, 51.For a system maintained at constant + temperature with Fq =  0 4 = E , Eq. 2.21 gives
J;
= L11Vp1+ L1,Z
(3.51)
where the interstitial chemical potential is again given by Eq. 3.36. Evaluating the quantity L1, requires understanding the physical mechanism that couples the mass flux of the interstitials to the electron current. The electron current in a metal produces a force Fe on a diffusing particle, such as an interstitial atom, which is proportional to the local current density [17]. The force arises from the change in the selfconsistent electronic charge distribution surrounding the interstitial defect. The defect scatters the currentcarrying electrons and creates a dipole, which in turn creates a resistance and a voltage drop across the defect. This dipole, known as a L a n d a u e r resistivity dipole, exerts an electrostatic force on the nucleus of the interstitial. This currentinduced force is usually described phenomenologically by ascribing an effective charge to the defect, which couples to the applied electric field to create an effective force. When this force is averaged
56
CHAPTER 3: DRIVING FORCES AND FLUXES FOR DIFFUSION
over all jumps of a diffusing interstitial, an average force proportional to g, so that (+) = pE
(ge) is obtained which is (3.52)
where p is a constant. This force, in turn, induces a diffusional drift flux of interstitials given by +
+
DlClPZ Jf = ( G I ) c = ~ 1M1(Fe)cl= kT Therefore, upon comparison with Eq. 3.51,
(3.53)
DlClP L1, = (3.54) kT Consider now the interstitial flux in a material subjected to both an electrostatic driving force and a concentration gradient. Using Eqs. 3.36, 3.43, 3.51, and 3.54, for a dilute species obeying Henry's law, (3.55)
Data describing this type of electromigration of interstitial atoms in a number of systems are described by Shewmon [18]. p can be measured by passing a fixed current through an isothermal system until a quasisteady state is achieved where & in Eq. 3.55 approaches zero. In this case, uphill difusion (flux in the direction of the concentration gradient) takes place until the concentration gradient term (proportional to V c l ) cancels the electromigration term. All the quantities can be measured experimentally and p can be inferred from the measurements. Electromigration can also be used to purify a variety of metals by sweeping interstitials to one end of a specimen [18]. Electromigration is also important in the narrow metal conductors that form the currentcarrying vias in integratedcircuit devices. Here, the electric field induces a directed migration of substitutional atoms by a vacancy mechanism (Exercise 3.10 develops a relation analogous to Eq. 3.55 for this case). With increasing miniaturization, the current densities are pushed higher and higher. In certain cases, electromigration is so severe that mass can be transported away from thin regions of metallic conductors, causing open circuits and the destruction of the electronic device. Additional Joule heating, resulting from increased current density in the thin regions, can exacerbate the damage.
3.3
MASS DIFFUSION I N A THERMAL GRADIENT
Both thermal gradients and electricalpotential gradients can induce mass diffusion. In a system containing a thermal gradient where both heat flow and mass diffusion of a dilute interstitial component 1 can occur, Eq. 2.21 predicts the interstitial flux +
LIQ (3.56) J1 = L11V/L1 VT T The interstitial chemical potential is a function of both concentration and temperature, and therefore
(3.57)
3.4: CAPILLARITY AND DIFFUSION
57
The partial atomic entropy, 31, is
s1=(CkL)
(3.58) c1
and therefore (3.59) Finally, combining Eqs. 3.36, 3.43, 3.56, and 3.59 gives (3.60) where the parameter QYans,which is seen to have dimensions of energy, is termed the heat of transport and is given by (3.61) Equation 3.60 indicates that mass diffusion can be induced by gradients in either the composition, or the temperature, or both. The degree of coupling of mass diffusion t o the thermal gradient is determined by the heat of transport, QFans. The origin of QYansis in the asymmetry between the energy states before, during, and after a diffusing species jumps to a neighboring site. Methods of measuring QP,,, are similar to those for measuring /3 in an electromigration experiment. A temperature gradient is established, causing a quasisteady state to exist where 3 = 0. The concentration gradient in this state can be determined experimentally and the heat of transport can then be calculated using ,Fans = kT2Vcl/(clVT). In the case of interstitial carbon in b.c.c. aFe, the carbon atoms diffuse toward the hot end of a specimen, which indicates that the heat of transport in this system is negative. Various data for Q Y s are presented and discussed by Shewmon [18]. 3.4
MASS DIFFUSION MOTIVATED BY CAPILLARITY
Capillarity is another important motivation for diffusion in many materials systems containing interfaces. The diffusion potentials of the components in the direct vicinity of an interface depend upon the local interface curvature; when interfaces possessing regions of different curvatures are present, differences in diffusion potential will drive diffusional transport between these regions in a direction that reduces the amount of energy in the system. Figure 3.7 provides a simple example of a pure crystalline material with an undulating surface in which selfdiffusion takes place by the vacancy exchange mechanism. In this case, the diffusion potential of the atoms just below the convex surface is higher than in the region where the surface is concave. This tends to establish a diffusion current through the bulk from the convex region to the concave region, as indicated, smoothing the surface and reducing the total interfacial energy. Any creation or destruction of vacancies at dislocations within the bulk
58
CHAPTER 3: DRIVING FORCES AND FLUXES FOR DIFFUSION
Figure 3.7: An uiidulrtt,ing surface possessing rcgioiis of positive and riegat,ive curvature. The ci.irvature differences lead to diffiisioriI)oterit,ia.l gradients t.hat ~.esiilt in surface smoothing by diffusional transport,.
can be ignored, an approximation that is usually j ~ s t i f i a b l e .The ~ rate of surface smoothing can then be determined by finding expressions for the atom flux and the diffusion equation in the crystal, and then solving the diffusion equation subject to the boundary conditions at the surface. In the following section, the diffusion equation and boundary conditions are established. Exercise 14.1 provides the complete solution to the problem.
3.4.1
The Flux Equation and Diffusion Equation
The system contains two networkconstrained componentshost atoms and vacancies; the crystal is used as the frame for measuring the diffusional flux, and the vacancies are taken as the N,th component. Note that there is no mass flow within the crystal, so the crystal Cframe is also a Vframe. With constant temperature and no electric field, Eq. 2.21 then reduces to
4
Jv

=  JA
(3.62)
An expression for the coefficient L A Amay be obtained by considering diffusion in a very large crystal with flat surfaces. The free energy of the system, containing N A atoms and NV vacancies (in dilute solution), can be expressed
Here, p i is the free energy per atom in a vacancyfree crystal composed of only Aatoms with a flat (zero curvature) surface, GG = H ;  TS;(vib) is the free energy [exclusive of that due to the mixing entropy, Sb(vib) is the vibrational entropy] to form a vacancy, and the last term is the free energy of mixing due to the entropy 'Vacancy crcation and destruction is discussed in Sections 11.1 anti 1 1 . 4
3 4: CAPILLARITY AND DIFFUSION
59
associated with the random distribution of the vacancies. Therefore, P A =
89
+ kTln

~ N A
a9
PV =a N v = G;
NA
( N A + N v ) EP:
+ k T In (N A T N v ) = G; + k T l n X v
(3.64)
where X V is the atom fraction of vacancies.1° If p v = 0 when the vacancies are at their equilibrium fraction, XFq, Eq. 3.64 may be written x;q = e  G : / ( k T ) (3.65) and
Pv = kTln
(s) X?
= kTln
Putting these expressions into Eq. 3.62 yields
(z)
(3.66)
Using Eq. A.12, Eq. 3.67 can be written as a Fick'slaw expression for the vacancy
where DV is the vacancy diffusivity, the volume per site is assumed to be uniform, and the fact that C A >> cv has been incorporated. The diffusion equation for vacancies in the absence of significant dislocation sources or sinks within the crystal is then = V . Jv = DvV2cv (3.69)
* at

From Eq. 3.68, (3.70) and an expression for the atom flux can be obtained by substituting Eq. 3.70 into Eq. 3.62 to obtain (3.71) If the variations in X V throughout the crystal in Fig. 3.7 are sufficiently small, D v X v / ( ( R ) k Tcan ) be assumed to be constant, and the conservation equation (see Eq. 1.18) may be writtenll
'ONote that Eqs. 3.64 for the chemical potentials are of the form given by Eq. 2.2. "Equations 3.71 and 3.72 can be further developed in terms of the selfdiffusivity using the atomistic models for diffusion described in Chapters 7 and 8. The resulting formulation allows for simple kinetic models of processes such as dislocation climb, surface smoothing, and diffusional creep that include the operation of vacancy sources and sinks (see Eqs. 13.3, 14.48, and 16.31).
60
CHAPTER 3: DRIVING FORCES AND FLUXES FOR DIFFUSION
The smoothing of a rough isotropic surface such as illustrated in Fig. 3.7 due to vacancy flow follows from Eq. 3.69 and the boundary conditions imposed on the vacancy concentration at the surface.12 In general, the surface acts as an efficient source or sink for vacancies and the equilibrium vacancy concentration will be maintained in its vicinity. The boundary condition on cv at the surface will therefore correspond to the local equilibrium concentration. Alternatively, if cv , and therefore X V ,do not vary significantly throughout the crystal, smoothing can be modeled using the diffusion potential and Eq. 3.72 subject to the boundary conditions on @A at the surface and in the b ~ 1 k . l ~ During surface smoothing, differences in the local equilibrium values of X V maintained in the different regions and differences in vacancy concentration throughout the crystal will be relatively small. Assuming that the crystal has isotropic surface tension, the local equilibrium vacancy concentration at the surface is a function of the local curvature [i.e., c? = c ? ( K ) ] , and can be found by minimizing Eq. 3.63 with respect to NV after adding in the energy required to create the vacancies directly adjacent to the surface. When a vacancy is added to the crystal at a convex region, the crystal expands by the volume AV = Rv and the surface area is increased by AA. Work must therefore be done to create the additional area. Because AA = KAV = KRV,the work is A W = YKQV
(3.73)
where y is the isotropic surface tension.14 When this surface work is added to the free energy in Eq. 3.63 and the sum is minimized, (3.74) When typical values are inserted into Eq. 3.74, c ? ( ~ ) / c y ( O )does not vary from unity by more than a few percent. Because only relatively small variations in cv occur in typical specimens undergoing sintering and diffusional creep (Chapter 16), we prefer to carry out the analyses of surface smoothing, sintering, and diffusional creep in terms of atom diffusion and the diffusion potential using Eq. 3.72. In this approach, the boundary conditions on @ A can be expressed quite ~ i m p 1 y . l ~ To solve the surface smoothing problem in Fig. 3.7, Eq. 3.72 can be simplified further by setting &A/& equal to zero because the diffusion field is, to a good approximation, in a quasisteady state, which then reduces the problem to solving the Laplace equation v2@A =0 (3.75) within the crystal subject to the boundary conditions on
@A
described below
12Methods for solving diffusion problems by setting up and solving the diffusion equation under specified boundary conditions are discussed in Chapter 5 . 13The vacancy concentration far from the surface will generally be a function of the total surface curvature. In this case, the crystal can be assumed to be a large block possessing surfaces which on average have zero curvature. The vacancies in the deep interior can then be assumed t o be in equilibrium with a flat surface. 14See Exercise 3.11 for further explanation. 15However, during the annealing of small dislocation loops (treated in Section 11.4.3), larger variations of the vacancy concentration occur and Eq. 3.68 must be employed.
3.5: STRESS AND DIFFUSION
3.4.2
61
Boundary Conditions
The boundary conditions on the diffusion potential @ A = p~  pv are readily found using results from the preceding section. At the surface where the vacancies are maintained in equilibrium, pv = 0. The diffusion potential for the atoms is the surface work term of the form given by Eq. 3.73 plus the usual chemical term, p i :
@z
= pi
+ TKflA
(3.76)
= pi. The Deep within the crystal, p v = 0 and p~ = p > , and therefore diffusion potential at the convex region of the surface is greater than that at the concave region, and atoms therefore diffuse to smooth the surface as indicated in Fig. 3.7. We discuss surface smoothing in greater detail in Chapter 14. Exercise 14.1 uses Eq. 3.75 subject t o the boundary condition given by Eq. 3.76 to obtain a quantitative solution for the evolution of the surface profile in Fig. 3.7.
3.5
MASS DIFFUSION I N T H E PRESENCE OF STRESS
Because stress affects the mobility, the diffusion potential, and the boundary conditions for diffusion, it both induces and influences diffusion [19]. By examining selected effects of stress in isolation, we can study the main aspects of diffusion in stressed systems. 3.5.1
Effect of Stress on Mobilities
Consider again the diffusion of small interstitial atoms among the interstices between large host atoms in an isothermal unstressed crystal as in Section 3.1.4. According to Eqs. 3.35 and 3.42, the flux is given by +
J1
= L11Vp1 = M1c1Vp1
(3.77)
The diffusion is isotropic and the mobility, M I , is a scalar, as assumed previously. If a general uniform stress field is imposed on a material, no force will be exerted on a diffusing interstitial because its energy is independent of position.16 Assuming no other fields, the flux remains linearly related t o the gradient of the chemical = MlclVpl. However, M I will be a tensor because the potential so that stress will cause differences in the rates of atomic migration in different directions; this general effect occurs in all types of ~ r y s t a 1 s . l It ~ may be understood in the following way: there will be a distortion of the host lattice when the jumping atom squeezes its way from one interstitial site t o another, and work must be done during the jump against any elements of the stress field that resist this distortion. Jumps in different directions will cause different distortions in the fixed stress field, so different amounts of work, W , must be done against the stress field during these jumps. The rate of a particular jump in the absence of stress is proportional to the exponential factor exp[Gm/(lcT)], where G" is the freeenergy barrier to the 16When the stress is nonuniform and stress gradients exist, the stress will exert a force, as discussed in the following section. 17The tensor nature of the diffusivity (mobility) in anisotropic materials is discussed in Section 4.5.
62
CHAPTER 3: DRIVING FORCES AND FLUXES FOR DIFFUSION
jumping process (see Chapter 7). When stress is present, the work, W , must be added to this energy barrier, and the jump rate will therefore be proportional to the factor exp[(Gm W)/(kT)]. For almost all cases of practical importance, W / ( k T ) is sufficiently small so that exp[W/(kT)] E 1  W / ( k T )and , the factor can then be written as exp[G"/(kT)] [l W/(kT)]. The overall interstitia1,mobility will be the result of the interstitials making numbers of different types of jumps in different directions. As just shown, each type of jump depends linearly on W ,which, in turn, is a linear function of the elements of the stress tensor. The latter function depends on the direction of the jump, and it is therefore anticipated that the mobility should vary linearly with stress and be expressible as a tensor in the very general linear form (3.78)
+
kl
where the stressdependent terms in the sum are relatively small. Similar considerations hold for the migration of substitutional atoms in a stress field (see Fig. 8.3), and the form of Eq. 3.78 should apply in such cases as well. These and other features of Eq. 3.78 are discussed by Larch6 and Voorhees 1191. 3.5.2
Stress as a Driving Force for Diffusion: Formation of SoluteAtom Atmosphere around Dislocations
In a system containing a nonuniform stress field, a diffusing particle generally experiences a force in a direction that reduces its interaction energy with the stress field. Ignoring any effect of the stress on the mobility and focusing on the force stemming from the nonuniformity of the stress field, the stressinduced diffusion of interstitial solute atoms in the inhomogeneous stress field of an edge dislocation would look like Fig. 3.8. An interstitial in a host crystal is generally oversized for the space available and pushes outward, acting as a positive center of dilation and causing a volume expansion as illustrated in Fig. 3.9. To find the force exerted on an interstitial by a stress field, one must consider the entropy production in a
m s o D o t e n t i a l s
7tdislocation
 \ ,/Direction
of
ctrnccinrii irnri ",I "V" I, lUUYVU
force and flux
Figure 3.8: Edge dislocation in an isotropic elastic body. Solid lines indicate isopotcntial cylinders for the portion of the diffusion potential of any interstitial atom present in the hydrostatic stress field of the dislocation. Dashed cylinders and tangential arrows indicate the direction of the corresponding force exerted on the interstitial atom.
3 5 STRESS AND DIFFUSION
Figure 3.9: Dilation produced by an iiiterst,it,ial atoiii iii out,warti displacenients of the interstit,inl's nearest neighbors.
H
63
cryst,al. Arrows iiidicate
small cell embedded in the material as in Section 2.1. Suppose that the interstitial causes a pure dilation A01 and there are no deviatoric strains associated with the interstitial; then the supplemental work term which must be added to the right side of Eq. 2.4 is dw = PARIdcl (3.79) where P is the hydrostatic pressure. For the case of an edge dislocation in an isotropic elastic material
p =  ff1.7.
+ 0 6 6 + ffzz
  ffxx
+ ffyy + ffzz
3 3 p ( 1 + v)b sine p(1 v)b y 3 ~ ( 1 U ) T 3 ~ (l V ) x 2 + y2
+
(3.80)
where p and v are the elastic shear modulus and Poisson's ratio: respectively, and b is the magnitude of the Burgers vector [20]. When this work term is added to the chemical potential term, pldcl, and the procedure leading to Eq. 2.11 is followed: the force is $1
= V (p1
+ AR1P)
(3.81)
The diffusion potential is therefore an "elastochemical" type of potential corresponding to18 a1 = p 1 + A R l P (3.82) Therefore, using Eqs. 2.16, 3.37, 3.43, and 3.82,

J1
f
= L11F1 = L11V@1 = L11V (p1
+ A Q l P ) = D1
(VCl + clAR1 kT

(3.83) The flux has two components: t'he first results from the concentration gradient and the second from the gradient in hydrostatic stress.19 The solid circles (cylinders 18The general diffusion potential for stress and chemical effects is
Aczj is the local strain associated with the migrating species.
= 111
+ Ae,,oi,cl,
where
"Several typically negligible effects have been neglected in the derivation of Eq. 3.83: including (1) interactions between the interstitials, (2) effects of the interstitials on the local elastic constants, ( 3 ) quadratic terms in the elastic energy, and (4) nonlinear stressstrain behavior. A more complete treatment, applicable to the present problem, takes into account many of these effects and has been presented by Larch6 and Cahn 1211.
64
CHAPTER 3: DRIVING FORCES AND FLUXES FOR DIFFUSION
in three dimensions) in Fig. 3.8 are isopotential lines for the portion of the diffusion potential due to hydrostatic stress. They were obtained by setting P equal to constant values in Eq. 3.80. Tangents to the dashed circles indicate the directions of the corresponding diffusive force arising from the dislocation stress field (this is treated in Exercise 3.6). Because AR1 is generally positive, this force is directed away from the compressive region (y > 0) and toward the tensile region (y < 0) of the dislocation, as shown. In the case where an edge dislocation is suddenly introduced into a region of uniform interstitial concentration, solute atoms will immediately begin diffusing toward the tensile region of the dislocation due to the pressure gradient alone (treated in Exercise 3.7). However, opposing concentration gradients build up, and eventually a steadystate equilibrium solute atmosphere, known as a Cottrell atmosphere, is created where the compositiongradient term cancels the stressgradient term of Eq. 3.83 (this is demonstrated in Exercise 3.8). From these considerations, Cottrell demonstrated that the rate at which solute atoms diffuse to dislocations and subsequently pin them in place is proportional to time2/3 (this time dependence is derived by an approximate method in Exercise 3.9). This provided the first quantifiable theory for the strain aging caused by solute pinning of dislocations [22]. 3.5.3
Influence of Stress on the Boundary Conditions for Diffusion: Diffusional Creep
In a process termed dz~usionalcreep, the applied stress establishes different diffusion potentials at various sources and sinks for atoms in the material. Diffusion currents between these sources and sinks are then generated which transport atoms between them in a manner that changes the specimen shape in response to the applied stress. A particularly simple example of this type of stressinduced diffusional transport is illustrated in Fig. 3.10, where a polycrystalline wire specimen possessing a “bamboo” grain structure is subjected to an applied tensile force, $app. This force subjects the transverse grain boundaries to a normal tensile stress and therefore reduces the diffusion potential at these boundaries. On the other hand, the applied stress has no normal component acting on the cylindrical specimen surface and, to first order, the diffusion potential maintained there is unaffected by the applied is sufficiently large that the diffusion potential at the transverse stress. When gaPp boundaries becomes lower than that at the surface, atoms will diffuse from the surface (acting as an atom source) to the transverse boundaries (acting as sinks), thereby causing the specimen to lengthen in response to the applied stress.20 A similar phenomenon would occur in a singlecrystal wire containing dislocations possessing Burgers vectors inclined at various angles to the stress axis. The diffusion potential at dislocations (each acting as sources or sinks) varies with each dislocation’s inclination. Vacancy fluxes develop in response to gradients in diffusion potential and cause the edge dislocations to climb, and as a result, the wire lengthens in the applied tensile stress direction. The problem of determining the elongation rate in both cases is therefore reduced to a boundaryvalue diffusion problem where the boundary conditions at the sources 20Surface sources and grain boundary sinks for atoms are considered in Sections 12.2 and 13.2.
3.5: STRESS AND DIFFUSION
t EPP
65
t EPP
Figure 3.10: Polycrystalline wire specimen with bamb2o grain structure subjected to uniaxial tensile stress, u z z ,arising from the applied force, Fapp.The bulk crystaldiffusion fluxes shown in (a) and grainboundary and surfacediffusion fluxes shown in (b) cause diffusional elongation. ( c ) Enlarged view at the junction of the grain boundary with the surface.
and sinks are determined by the inclination of the sources and sinks relative to the applied stress and the magnitude of the applied stress. In the following we outline the procedure for obtaining the elongation rate of the polycrystalline wire shown in Fig. 3.10 for the case where the material is a pure cubic metal and the diffusion occurs through the grains as in Fig. 3.10a by a vacancy exchange mechanism. The diffusional creep rate of a single crystal containing various types of dislocations is treated in Chapter 16. Flux and diffusion equations. During diffusional creep, the stresses are relatively small, so variations in the vacancy concentration throughout the specimen will generally be small and can be ignored. The flux equation and diffusion equation in the grains are then given by Eqs. 3.71 and 3.75 (with @ A = p~  p v ) , which were derived for diffusion in a crystal during surface smoothing. In both cases, quasisteadystate diffusion may be assumed, and any creation or destruction of vacancies a t dislocations within the grains can be neglected.
Boundary conditions. The cylindrical wire surface is a source and sink for vacancies, and the condition pv = 0 is therefore maintained there. The diffusion potential at the curved surface, a;, is given by Eq. 3.76. At the grain boundaries, the condition pv = 0 should also hold. The boundaries will be under a traction, unn = fiT.cr.fi,and when an atom is inserted, the tractions will be displaced as the grain expands by the volume C I A . For the case in Fig. 3.10, the boundary is oriented so that its normal is parallel to the zaxis and therefore unn = u r z . This displacement contributes work, unnCI~= ~ , , Q A , and reduces the potential energy of the system by a corresponding amount. This term must be added to the chemical term, p;, and therefore the diffusion potential along the
66
CHAPTER 3: DRIVING FORCES AND FLUXES FOR DIFFUSION
grain boundary is2'
decreases as the stress increases; an increase in the applied force increases onn, and when onnis sufficiently large so that @: < @ ,: atoms will diffuse from the surface to the boundaries at a quasisteady rate. The bamboo wire behaves like a viscous material, due to the quasisteadystate diffusional transport.22 Complete solutions for the elongation rates due to the grain boundary and surface diffusion fluxes shown in Fig. 3.10a and b are presented in Sections 16.1.1 and 16.1.3. @:
3.5.4
Summary of Diffusion Potentials
The diffusion potential is the generalized thermodynamic driving force that produces fluxes of atomic or molecular species. The diffusion potential reflects the change in energy that results from the motion of a species; therefore, it includes energystorage mechanisms and any constraints on motion. @j
= p j : For chemical interactions and entropic effects with no other constraint
(e.g., interstitial diffusion). Section 3.1.4. @j
= pj  p v : Reflecting the additional network constraint when sites are con
@j
= pj
served (e.g., vacancy substitution). Section 3.1.1.
+
q j 4 : When the diffusing species has an associated charge q j in an electrostatic potential (e.g., interstitial Li ions in a separator between an anode and a cathode). Section 3.2.1. #J
@j
+
R j P : Accounting for the work against a hydrostatic pressure, P, to move a species with volume R j (e.g., interstitial diffusion in response to hydrostatic stress gradients). Section 3.5.2.
= pj
+
7 ~ R . j : Accounting for the work against capillary pressure T K to move a species with volume R j to an isotropic surface (e.g., surface diffusion in response to a curvature gradient). Section 3.4.2.
@ j = pj
@j
K
@j
+K
~ R Accounting ~ : for the anisotropic equivalent to capillary pressure. the , weighted mean curvature, is the rate of energy increase with volume addition (e.g., surface diffusion on a faceted surface). Section 14.2.2.
= pj
 a,,Rj: Accounting for the work against an applied normal traction onn= fiT (a f i ) as an atom with volume R j is added to an interface with normal f i ; f i T is the transpose of fi (e.g., diffusion along an incoherent grain boundary in response to gradients in applied stress). Section 3.5.3.
= pj
@j=
~

p j + R j { [ ( P . a ) x ~ ] . ( ( x ~ ) } / { [ ( ( xxi].;}: ~)
in energy as a dislocation with Burgers vector
b'
Accountingforthechange and unit tangent ( climbs
21Again, as in the derivation of Eq. 3.82, quadratic terms in the elastic energy, which are of lower order in importance, have been neglected (see Larch6 and Cahn [21]). 22For a n ideally viscous material, the strain rate is linearly related to the applied stress u by the relation = (l/a)o, where 17 is the viscosity.
3.5:STRESS AND DIFFUSION
67
with stress CT due to applied loads and other stress sources (i.e., other defects) for each added volume R j (e.g., diffusion to a climbing dislocation by the substitutional mechanism). Section 13.3.2.23 Cpj
= d2fhom/acj2 2K,V2cj: Accounting for the gradientenergy term in the dif
fuse interface model for conserved order parameters (e.g., “uphill” diffusion during spinodal decomposition). Section 18.3.1. Bibliography 1. J.S. Kirkaldy and D.J. Young. Diffusion in the Condensed State. Institute of Metals,
London, 1987.
2. J.G. Kirkwood, R.L. Baldwin, P.J. Dunlap, L.J. Gosting, and G. Kegeles. Flow equations and frames of reference for isothermal diffusion in liquids. J . Chem. Phys., 33(5):15051513, 1960. 3. J. Bardeen and C. Herring. Diffusion in alloys and the Kirkendall effect. In J.H. Hollomon, editor, A t o m Movements, pages 87111. American Society for Metals, Cleveland, OH, 1951. 4. A.D. Smigelskas and E.O. Kirkendall. Zinc diffusion in alpha brass. P a n s . AIME, 171:130142, 1947. 5. R.W. Balluffi and B.H. Alexander. Dimensional changes normal to the direction of diffusion. J . Appl. Phys., 23:953956, 1952. 6. L.S. Darken. Diffusion, mobility and their interrelation through free energy in binary metallic systems. P a n s . AIME, 175:184201, 1948. 7. J . Crank. The Mathematics of Diffusion. Oxford University Press, Oxford, 2nd edition, 1975. 8. R.W. Balluffi. The supersaturation and precipitation of vacancies during diffusion. Acta Metall., 2(2):194202, 1954.
9. R.F. Sekerka, C.L. Jeanfils, and R.W. Heckel. The moving boundary problem. In H.I. Aaronson, editor, Lectures on the Theory of Phase Transformations, pages 117169. AIME, New York, 1975. 10. R.W. Balluffi. On the determination of diffusion coefficients in chemical diffusion. Acta Metall., 8(12):871873, 1960. 11. R.W. Balluffi and B.H. Alexander. Development of porosity during diffusion in substitutional solid solutions. J. Appl. Phys., 23(11):12371244, 1952. 12. R.W. Balluffi. Polygonization during diffusion. J . Appl. Phys., 23(12):14071408, 1952. 13. V.Y. Doo and R.W. Balluffi. Structural changes in single crystal copperalphabrass diffusion couples. Acta Metall., 6(6):428438, 1959.
14. R.W. Cahn. Recovery and recrystallization. In R.W. Cahn and P. Haasen, editors, Physical Metallurgy, pages 15951671. NorthHolland, Amsterdam, 1983. 15. C. Robinson. Diffusion and swelling of high polymers. 11. The orientation of polymer molecules which accompanies unidirectional diffusion. P a n s . Faraday Soc., 42B: 1217, 1946. 16. D.R. Gaskell. Introduction to Metallurgical Thermodynamics. McGrawHill, New York, 2nd edition, 1981. 23The expression for this diffusion potential is derived in Exercise 13.3
68
CHAPTER 3: DRIVING FORCES AND FLUXES FOR DIFFUSION
17. J. Hoekstra, A.P. Sutton, T.N. Todorov, and A.P. Horsfield. Electromigration of vacancies in copper. Phys. Rev. B, 62(13):85688571, 2000. 18. P. Shewmon. Diffusion in Solids. The Minerals, Metals and Materials Society, Warrendale, PA, 1989. 19. F.C. Larch6 and P.W. Voorhees. Diffusion and stresses, basic thermodynamics. Defect and Diffusion Forum, 129130:3136, 1996. 20. J.P. Hirth and J. Lothe. Theory of Dislocations. John Wiley & Sons, New York, 2nd edition, 1982. 21. F. Larch6 and J.W. Cahn. The effect of selfstress on diffusion in solids. Acta Metall., 30 ( 10):18351845, 1982. 22. A.H. Cottrell. Dislocations and Plastic Flow. Oxford University Press, Oxford, 1953. 23. L.S. Darken. Diffusion of carbon in austenite with a discontinuity in composition. Trans. AIME, 180:430438, 1949. 24. U. Mehmut, D.K. Rehbein, and O.N. Carlson. Thermotransport of carbon in twophase VC and NbC alloys. Metall. Trans., 17A(11):19551966, 1986. 25. A.H. Cottrell and B.A. Bilby. Dislocation theory of yielding and strain ageing of iron. Proc. Phys. SOC.A , 49:4962, 1949.
EXERCISES 3.1 Component 1, which is unconstrained, is diffusing along a long bar while the temperature everywhere is maintained constant. Find an expression for the heat flow that would be expected to accompany this mass diffusion. What role does the heat of transport play in this phenomenon? Solution. The basic forceflux relations are

1 J1 =  L 1 1 V p i  L i g  V T T TQ=  L ~ 1 O p 1  LQQVT 1 T
(3.85)
Under isothermal conditions
J;
= L11Vp1
TQ=  L ~ l V p i
(3.86)
Therefore, using Eqs. 3.61 and 3.86,
(3.87) The heat flux consists o f t w o parts. The first is the heat flux due t o the flux of entropy, which is carried along by the mass flux in the form of the partial atomic entropy, S:. Beca_use 31 = +85'/8N1, a flux of atoms will transport a flux of heat given by JQ = T J s = T S 1 J 1 . The second part is a "cross effect" proportional t o the flux of mass, with the proportionality factor being the heat of transport.
3.2 As shown in Section 3.1.4, the diffusion of small interstitial atoms (component 1) among the interstices between large host' atoms (component 2) produces a interdiffusivity, 5, for the interstitial atoms and host atoms in a Vframe given by Eq. 3.46, that is D =c ~ O Z D ~ (3.88)
EXERCISES
69
and therefore a flux of host atoms given by
 dc:!
J 2v = D
(3.89)
dX
This result holds even though the intrinsic diffusivity of the host atoms is taken to be zero and the flux of host atoms across crystal planes in the local Cframe is therefore zero. Give a physical explanation of this behavior. Solution. When mobile interstitials diffuse across a plane in the Vframe, the material left behind shrinks, due t o the loss o f the dilational fields o f the interstitials. This establishes a bulk flow in the diffusion zone toward the side losing interstitials and causes a compensating flow (influx) o f the large host atoms toward that side even though they are not making any diffusional jumps in the crystal. The rate of loss of volume of the material (per unit area) on one side o f a fixed plane in the Vframe due t o a loss o f interstitials is
(3.90) In the Vframe this must be compensated for by a gain of volume due t o a gain o f host atoms so that dV1 +  = odV2 (3.91) dt dt where dVz/dt is the rate o f volume gain due t o the gain o f host atoms corresponding to
(3.92) Substituting Eqs. 3.90 and 3.92 into Eq. 3.91 and using Eq. A.lO,
(3.93)
3.3 In a classic diffusion experiment, Darken welded an FeC alloy and an FeCSi alloy together and annealed the resulting diffusion couple for 13 days at 1323 K, producing the concentration profile shown in Fig. 3.11 [23]. Initially, the C concentrations in the two alloys were uniform and essentially equal, whereas the Si concentration in the FeCSi alloy was uniform at about 3.8%. After a diffusion anneal, the C had diffused “uphill” (in the direction of its concentration gradient) out of the Sicontaining alloy. Si is a large substitutional atom, so the Fe and Si remained essentially immobile during the
6
0.6
0 C
0.5
ecu
+
a,
2
% 0.4
E0l .
0.3
20
10
0
I
l
10
l
Distance from weld (mm)
1
20
Figure 3.11: Nonuniform concentration of C produced by diffusion from an initially uniform distribution. Carbon migrated from the FeSiC (left) to the FeC alloy (right). From Darken [23].
70
CHAPTER 3: DRIVING FORCES AND FLUXES FOR DIFFUSION
diffusion, whereas the small interstitial C atoms were mobile. Si increases the activity of C in Fe. Explain these results in terms of the basic driving forces for diffusion. Solution. As the C interstitials are the only mobile species, Eq. 3.35 applies, and therefore
J;
= L11Vp1
(3.94)
Using the standard expression for the chemical potential, p1 = py
+ kTlna1
(3.95)
where a1 = 71x1 is the activity of the interstitial C,
(3.96) The coefficient L11 in Eq. 3.96 is positive and the equation therefore shows that the C flux will be in the direction of reduced C activity. Because the C activity is higher in the Sicontaining alloy than in the nonSicontaining alloy a t the same C concentration, the uphill diffusion into the nonSicontaining alloy occurs as observed. In essence, the C is pushed out of the ternary alloy by the presence of the essentially immobile Si.
3.4 Following Shewmon, consider the metallic couple specimen consisting of two different metals, A and B , shown in Fig. 3.12 [18]. The bonded end is at temperature TI and the open end is a t T2. A mobile interstitial solute is present at the same concentration in both metals for which QYans = 84 kJ/mol in one leg and QFans= 0 in the other. Assuming that the interstitial concentration remains the same at the bonded interface at T I , derive the equation for the steadystate interstitial concentration difference between the two metal legs at Tz. Assume that TI > T2. r1
Figure 3.12: Metallic couple specimen made up of metals A and B. Solution. In the steady state, Eq. 3.60 yields C i Q Y a n s VT VCl = ~ kT2
(3.97)
Reducing t o one dimension and integrating,
(3.98) Therefore,
(3.99)
EXERCISES
71
Therefore, for leg A,
(3.100) while for leg B , cf(T2) = c f ( T 1 ) . Finally, because cf(T1)= $ ( T i ) = cf(T2)
ci(Ti),
{ [
Ac1 = cl(T1) exp
1
84000 (Ti  T2) NokTiTz l>
(3.101)
3.5 Suppose that a twophase system consists of a fine dispersion of a carbide phase in a matrix. The carbide particles are in equilibrium with C dissolved interstitially in the matrix phase, with the equilibrium solubility given by c1 = c,eo  A H / ( k T )
(3.102)
If a barshaped specimen of this material is subjected to a steep thermal gradient along the bar, C atoms move against the thermal gradient (toward the cold end) and carbide particles shrink at the hot end and grow at the cold end, even though the heat of transport is negative! (For an example, see the paper by Mehmut et al. [24].) Explain how this can occur. 0
Assume that the concentration of C in the matrix is maintained in local equilibrium with the carbide particles, which act as good sources and sinks for the C atoms. Also, AH is positive and larger in magnitude than the heat of transport.
Solution. The local C concentration will be coupled t o the local temperature by Ea. 3.102. and therefore
dcl  dci dT  AH dT I
dx
dT dx kT2 dx Substitution of Eq. 3.103 into Eq. 3.60 then yields Jl
kT2
Because ( A H observed.
dz
= D1cl ( A H + Qtrans) dT
(3.103)
(3.104)
+ Qtrans)is positive, the C atoms will be swept toward the cold end, as
3.6 Show that the forces exerted on interstitial atoms by the stress field of an edge dislocation are tangent to the dashed circles in the directions of the arrows shown in Fig. 3.8. Solution. The hydrostatic stress on an interstitial in the stress field is given by Eq. 3.80 and the force is equal t o =  0 l V P . Therefore, (3.105) where A is a positive constant. Translating the origin of the (x’,y’) coord+inate system t o a new position corresponding t o (2’= R,y’ = 0 ) , the expression for Fl in the new ( x ,y) coordinate system is
72
CHAPTER 3: DRIVING FORCES AND FLUXES FOR DIFFUSION
Converting t o cylindrical coordinates, $1
1
r sin 8 = R1 A V [ r Z + R 2 + 2 r R c ~ ~ B
The gradient operator in cylindrical coordinates is
d V =fir+Cedr
Therefore, using Eq. 3.107 and $1
=
(3.107)
l d de
(3.108)
T
Eq. 3.108 yields
0 1A { f i r ( Rzr 2 ) s i n 8 + f i e [ ( R 2+ r 2 ) c o s e + 2 R r ] } [RZ + r2 + 2 R r cos el2
(3.109) The force on an interstitial lying on a cylinder of radius R centered on the origin where r = R is then
(3.110) The force anywhere on the cylinder therefore lies along 60, which is tangential t o the cylinder in the direction of decreasing 0.
3.7 Consider the diffusional flux in the vicinity of an edge dislocation after it is suddenly inserted into a material that has an initially uniform concentration of interstitial solute atoms. (a) Calculate the initial rate at which the solute increases in a cylinder that has an axis coincident with the dislocation and a radius R. Assume that the solute forms a Henrian solution. (b) Find an expression for the concentration gradient a t a long time when mass diffusion has ceased. Solution. (a) The diffusion flux is given by Eq. 3.83. Initially, the concentration gradient is zero and the flux is due entirely t o the stress gradient. Therefore,
h k T ( 1  v)
1
r2
'
Now, integrate the flux entering the cylinder, noting that the B component contributes nothing: 2x
Asin6
Rd9 =0
(3.112)
where A = constant. Note that this result can be inferred immediately, due t o the symmetry of the problem. (b) When mass flow has ceased, the flux in Eq. 3.83 is zero and therefore
7:;;;;t yVlb [+1 ] sine
vc1= 
Cr
cos0 T u e r ~
(3.113)
3.8 The diffusion of interstitial atoms in the stress field of a dislocation was considered in Section 3.5.2. Interstitials diffuse about and eventually form an
73
EXERCISES
equilibrium distribution around the dislocation (known as a Cottrell atmosphere), which is invariant with time. Assume that the system is very large and that the interstitial concentration is therefore maintained at a concentration cy far from the dislocation. Use Eq. 3.83 to show that in this equilibrium atmosphere, the interstitial concentration on a site where the hydrostatic pressure, P , due to the dislocation is cyl
= Cle 0 nlp/(W
(3.114)
Solution. According t o Eq. 3.83, (3.115) A t equilibrium,
= 0 and therefore lncyq
+
kT
= a1 = constant
Because cyq = c? a t large distances from the dislocation where P = 0,
(3.116) a1
C1 eq  C;e%P/(kT)
= In&,
(3.117)
3.9 In the Encyclopedia of Twentieth Century Physics, R.W. Cahn describes A.H. Cottrell and B.A. Bilby's result that strain aging in an interstitial solid solution increases with time as t213 as the coming of age of the science of quantitative metallurgy [ 2 5 ] . Strain aging is a phenomenon that occurs when interstitial atoms diffuse to dislocations in a material and adhere to their cores and cause them to be immobilized. Especially remarkable is that the t213 relation was derived even before dislocations had been observed. Derive this result f0r an edge dislocation in an isotropic material. 0
0
0
0
Assume that the degree of the strain aging is proportional to the number of interstitials that reach the dislocation. Assume that the interstitial species is initially uniformly distributed and that an edge dislocation is suddenly introduced into the crystal. Assume that the force,  R l V P , is the dominant driving force for interstitial diffusion. Neglect contributions due to V c . Find the time dependence of the number of interstitials that reach the dislocation. Take into account the rate a t which the interstitials travel along the circular paths in Fig. 3.8 and the number of these paths funneling interstitials into the dislocation core.
Solution. The tangential velocity, u , of an interstitial tkaveling along a circular path of radius R in Fig. 3.8 will be proportional t o the force F1 = fIlVP exerted by the dislocation. In cylindrical coordinates, P is proportional t o sinO/r, so (3.118)
74
CHAPTER 3: DRIVING FORCES AND FLUXES FOR DIFFUSION
Therefore, v K F1 LX l / r z . As shown in Fig. 3.8, v at equivalent points on each circle will scale as l/r*, and because r a t these points scales as R,
1
(3.119)
The averagewelocity, (v), around each circular path will therefore scale as l / R Z .Since the distance around a path is 2 n R , the time, t R , required t o travel completely around
(3.120) Therefore, at time, t , the circles with radii less than Rcrit K
t1/3
(3.121)
will be depleted o f solute. During an increment of time d t , the average distance a t which interstitials along the active flux circles approach the dislocation is equal (to a reasonable approximation) t o d s = ( v ) d t . The total volume (per unit length of dislocation) supplying atoms during this period is then
dV
LX
dt
Jm(v) d R L i t
0:
L d t %it
(3.122)
where the integral is taken over only the active flux circles. Because the concentration was initially uniform, the number of interstitials reaching the dislocation in time t , designated by N , is therefore proportional t o the volume swept out. Therefore, substituting Eq. 3.121 in Eq. 3.122 and integrating,
(3.123) More detailed treatments are given in the original paper by Cottrell and Bilby [25] and in the summary in Cottrell's text on dislocation theory [22].
3.10 Derive the expression
+ DVCVPZ J A = 
kT for the electromigration of substitutional atoms in a pure metal, where D v is the vacancy diffusivity and cv is the vacancy concentration. Assume that: There are two mobile components: atoms and vacancies. Diffusion occurs by the exchange of atoms and vacancies. There is a sufficient density of sources and sinks for vacancies so that the vacancies are maintained at their local equilibrium concentration everywhere. Solution. Vacancies are defects that scatter the conduction electrons and are therefore subject t o a force which in turn induces a vacancy current. The vacancy current results in an equal and opposite atom current. The components are network constrained so that Eq. 2.21 for the vacancies, which are taken as the N,th component, is
Because V ~ = A0 (see Eq. 3.64) and p v = 0,
EXERCISES
75
The vacancy current is therefore due solely t o the_cross term arising from the current o f conduction electrons (which is proportional t o E ) . The coupling coefFicient for the vacancies is the offdiagonal coefficient Lvq which can be evaluated using the same procedure as that which led t o Eq. 3.54 for the electromigration o f interstitial atoms in a metal. Therefore, if (CV) is the average drift velocity o f the vacancies induced by the current and Mv is the vacancy mobility,
3.11 (a) It is claimed in Section C.2.1 that the mean curvature, K , of a curved interface is the ratio of the increase in its area to the volume swept out when the interface is displaced toward its convex side. Demonstrate this by creating a small localized “bump” on the initially spherical interface illustrated in Fig. 3.13. I1
c
L Figure 3.13:
Circular cap (spherical zone)
011
a spherical interface.
(b) Show that Eq. 3.124 also holds when the volume swept out is in the form of a thin layer of thickness dw, as illustrated in Fig. 3.14.
Figure 3.14: with curvature
0
K
Layer of thickness diu swept out by additioii of material at = (1/R1) (1/&).
+
a11 interface
Construct the bump in the form of a small circular cap (spherical zone) by increasing h infinitesimally while holding r constant. Then show that
dA dV
/$=
(3.124)
where dA and dV are, respectively, the increases in interfacial area and volume swept out due to the construction of the bump.
76
CHAPTER 3: DRIVING FORCES AND FLUXES FOR DIFFUSION
Solution. (a) The area of the circular cap in Fig. 3.13 is
A = 7r (T’
+ h2)
Here T and h are related t o the radius o f curvature of the spherical surface, R , by the relation
R = ?2(hl + $ )
(3.125)
The volume under the circular cap is given by 7r
V = hr2 2
+ h3 6 7r
If the bump is now created by forming a new cap o f height h T
constant,
+ dh while keeping
dA = 27rhdh
(3.126) (3.127)
Therefore, using Eqs. 3.125, 3.126, and 3.127, and the fact that h2/r2<< 1,
dA  2 
dVRZK
(b) The increase in area is
dA = (R1
+ d w ) dB1 (Rz + d w )
dB2
+ Rz)dw
 R1 dB1 R2 dBz = ( R I
The volume swept out is
dV = Ri dB1 Rz dBz dw Therefore,
dA _  Ri1 dV
 +  = K
1
Rz
dB1 dB2
CHAPTER 4
T H E DIFFUSION EQUATION
The diffusion equation is the partialdifferential equation that governs the evolution of the concentration field produced by a given flux. With appropriate boundary and initial conditions, the solution to this equation gives the time and spatialdependence of the concentration. In this chapter we examine various forms assumed by the diffusion equation when Fick’s law is obeyed for the flux. Cases where the diffusivity is constant, a function of concentration, a function of time, or a function of direction are included. In Chapter 5 we discuss mathematical methods of obtaining solutions to the diffusion equation for various boundaryvalue problems. 4.1
FICK’S SECOND LAW
If the diffusive flux in a system is f,Section 1.3.5 and Eq. 1.18 are used to write the diffusion equation in the general form dC _  n  V * J
+
at
where n is an added source or sink term corresponding to the rate per unit volume a t which diffusing material is created locally, possibly by means of chemical reaction or fastparticle irradiation, and :is any flux referred to a Vframe. There frequently are no sources or sinks operating, and n = 0 in Eq. 4.1. When Fick’s law applies (see Section 3.1) and n = 0, Eq. 4.1 takes the general form Kinetics of Materials. By Robert W. Balluffi, Samuel M. Allen, and W. Craig Carter. Copyright @ 2005 John Wiley & Sons, Inc.
77
78
CHAPTER 4 THE DIFFUSION EQUATION
dC _ d t  V f = V .( D V c ) *
which is sometimes called Fick’s second law (note that Fick’s second law is simply a consequence of the conservation of the diffusing species). Accumulation within a volume depends only on the fluxes at its boundary. For example, in one dimension,
where N is the number of particles and A is the area through which the diffusion occurs. In three dimensions,
t ) is ? the timedependent , value of flux at the oriented where in the final integral, I( surface dV that bounds V. The geometrical interpretation in Fig. 4.1 shows how c ( z ,t ) changes locally; the equations above imply a conservation constraint for the entire concentration field. Because Eq. 4.2 has one time and two spatial derivatives, its solution requires three independent conditions: an initial condition and two independent boundary conditions. Boundary conditions typically may look like C ( T = TB) = f ( t )= c g ( t )
or
f ( ~T B=) .
=g(t) = J B ( ~ )
(4.5)
where RB is the normal to the boundary and the initial conditions have the form c(z, y, 2 , t = t o ) = c(T,t = t o ) = h ( z ,y, 2 ) = h(F) = C O ( 5 , y, 2 )
(4.6)
In Chapter 3, several different types of diffusivity were introduced for diffusion in a chemically homogeneous system or for interdiffusion in a solution. In each case, Fick’s law applies, but the appropriate diffusivity depends on the particular system. The development of the diffusion equation in this chapter depends only on the form of Fick’s law, f =  D V c . D is a placeholder for the appropriate diffusivity, just as f and c are placeholders for the type of component that diffuses. Equation 4.2 can take various forms, depending upon the behavior of D. The simplest case is when D is constant. However, as discussed below, D may be a function of concentration, particularly in highly concentrated solutions where the interactions between solute atoms are significant. Also, D may be a function of time: for example, when the temperature of the diffusing body changes with time. D may also depend upon the direction of the diffusion in anisotropic materials. 4.1.1
Linearization of the Diffusion Equation
Methods to solve the diffusion equation for specific boundary and initial conditions are presented in Chapter 5. Many analytic solutions exist forthe special case Lhat D is uniform. This is generally not the case for interdiffusivity D (Eq. 3.25). If D does not vary rapidly with composition, it can be replaced by successive approximations of a uniform diffusivity and results in a linearization of the diffusion equation. The
4.1:FICK'S SECOND LAW
79
linearized form permits approximate models from known solutions. The diffusivity is expanded about its average value, D O ,as follows
where A c = c  ( c ) , and
The diffusion equation becomes (4.9) The lowestorder approximation for small A c and small lVcl is (4.10) which is the diffusion equation for constant diffusivity. 4.1.2
Relation of Fick's Second Law to the Heat Equation
For evolution of a temperature field during heat flow, an equation with the same form as Eq. 4.2 arises:
(4.11)
where h is the enthalpy density and cp is the heat capacity per unit volume. The ratio K I c p is called the thermal daffusivaty, K . It is assumed that no enthalpy is stored by a phase change and that c p is constant. Therefore, any result that follows from considerations of the form of Fick's second law applies to evolution of heat as well as concentration. However, the thermal and mass diffusion equations differ physically. The mass diffusion equation, d c l d t = V . D V c , is a partialdifferential equation for the density of an extensive quantity, and in the thermal case, d T l d t = V . KVTis a partialdifferential equation for an intensive quantity. The difference arises because for mass diffusion, the driving force is converted from a gradient in a potential V p to a gradient in concentration Vc, which is easier to measure. For thermal diffusion, the timedependent temperature arises because the enthalpy density is inferred from a temperature measurement.
80
4.1.3
CHAPTER 4: THE DIFFUSION EQUATION
Variational Interpretation of the Diffusion Equation
The rate of entropy production, tr (Eq. 2.19), for onedimensional diffusion becomes
.
.=&) kD
dc
(4.12)
when the activity coefficient is independent of concentration. Localized changes in c ( x ,t ) affect the rate of total entropy production. How changes in the evolution of a field affect a functional (such as an integral quantity like total entropy production) is a topic in the calculus of variations [l]. For an adiabatic system, the rate of total entropy production Stotis a functional of the concentration field c ( x ) , (4.13) The functional gradient of Stotindicates the function pointing in the “direction” of fastest increase. Gradients depend on an inner product because it provides a measure of “distance” for functions [2]. One choice of an inner product for functions is the L2 inner product, defined by (4.14)
J
so the magnitude of a function is related t o the integral of its square: lp(x)l = ( p p ) l / ’ . Note that leastsquares data fits use this inner product. The functional gradient of F (or gradient of a vector function) can be defined by G F , and the inner product with a velocity field v: (4.15) That is, of all possible functions v ( x ) ,those that are parallel, subject to choice of norm or inner product, to G F give the fastest increase in F . For the entropy production with D = constant, dC dt
2kD
(4.16)
Integrating by parts, x2
d2c dc
dc dc
(4.17)
If the boundary conditions are zero flux or fixed composition, the last term vanishes. Comparison with the L2 inner product reveals that for evolution according to the diffusion equation, c ( x ,t ) changes so that Stot(total entropy “acceleration”) is its most negative. Thus, entropy production, which is always positive, decreases in time as rapidly as possible when dcldt cc Gs,,, cc d2c/dx2.
81
4.2 CONSTANT DlFFUSlVlTY
4.2
CONSTANT DlFFUSlVlTY
When D is constant, Eq. 4.2 takes the relatively simple form of the linear secondorder partial differential equation dC
 = DV'C at
(4.18)
Some of the major features of this equation are discussed below, and methods of solving it under a variety of boundary and initial conditions are described at length in Chapter 5 . 4.2.1
Geometrical Interpretation of the Diffusion Equation when Diffusivity is Constant
Figure 4.1 illustrates how a onedimensional concentration field, c(x,t ) ,evolves according t o Eq. 4.18. The righthand side of Eq. 4.18 is proportional t o the curvature of the concentration profile. Where the curvature is negative, as on the lefthand side, the concentration must decrease at a rate proportional to the magnitude of the curvature. Conversely, the concentration must increase on the righthand side, where the curvature is positive.
h z
%
v
X
Figure 4.1: Evolut,ion of concentration field according to Fick's law. proportional to the curvature of the concentration field.
4.2.2
&/at is
Scaling of the Diffusion Equation
Under certain conditions, boundaryvalue diffusion problems can be solved conveniently by scaling. First, introduce the dimensionless variable q, q=
2
rn
(4.19)
into the diffusion equation. Using Eq. 4.18 for onedimensional diffusion and
a = av a at at aq
a = aq a ax a x a q
(4.20)
the diffusion equation becomes (4.21)
82
CHAPTER 4: THE DIFFUSION EQUATION
Next, suppose that for the particular boundaryvalue problem under consideration, the initial and boundary conditions are unchanged by scale change:
z= Ax t = A2t
(4.22)
Then 77 is invariant under the scaling corresponding to Eq. 4.19 and c becomes a function of the single variable, v. The diffusion equation becomes an ordinary differential equation (i.e., d + d ) . If the boundaryvalue diffusion problem can be scaled according to Eq. 4.19, it is considerably easier to solve. Consider the onedimensional stepfunction diffusion problem shown in Fig. 4.2, where
c(x,t = 0 ) =
{ ::
m<x
(4.23)
c(co,t) = cL; C(co,t)= C R The initial and boundary conditions given by Eq. 4.23 are transformed by scaling into c(co) = c L and c ( m )= c R (4.24) and the diffusion equation has the form in Eq. 4.21. The entire boundaryvalue diffusion problem is now rescaled. Equation 4.21 can be integrated by letting 9'
Then
dc d7
dq 279 = dv
(4.25)
(4.26)
which can be integrated to produce (4.27) where a1 is a constant. Integrating again yields (4.28) Applying the stepfunction initial conditions in Eq. 4.24,
Figure 4.2:
Onedimensional stepfunction initial conditions.
l T h e diffusion equation itself can always be rescaled. However, to solve a boundaryvalue diffusion problem using the scaling method, the initial and boundary conditions must also be scalable.
4
where a2 is a constant. The integral with the limit x function, abbreviated "erf" :
/
z
CONSTANT DIFFUSIVITY
83
m is known as the error
(4.30) The error function has the properties erf(0) = 0, erf(m) = 1, and erf(z) = erf(z). So, after evaluating a2 by using the boundary conditions, the diffusion problem posed above has the solution
(4.31)
+
where C = (cR c L ) / 2 and A c = cR  cL. When c is assigned units of particles per unit length, Eq. 4.31 describes the onedimensional diffusion along r from an initial step function on a line in one dimension as in Fig. 4 . 3 ~ When . c has units of particles per unit area. it describes the onedimensional diffusion from a step function in a twodimensional plane as in Fig. 4.3b, and when the units are particles per unit volume, it describes the onedimensional diffusion from a step function in three dimensions. as in Fig. 4 . 3 ~ .
Figure 4.3:
diriierisioris.
Initial stepfunction distributions iri (a) one, (b) two, arid (c) three
Scaling as a Means to Compare Similar Systems. When the diffusion problem is invariant to the scaling parameter ri = x / m . equal values of can be used to determine relationships between length. time, and the value of the diffusivity. For example. consider two masses that differ only in their length dimension. Let the first block have length L and the second block have length NL. If at a time, 7 . a particular concentration appears at the center of the first block. the same concentration will appear in the second block at time o2r.
4.2.3
Superposition
Suppose that ~ ( xt ). is a solution to the onedimensional diffusion equation (4.32)
84
CHAPTER 4: THE DIFFUSION EQUATION
with boundary and initial conditions p (= ~ a, t ) = A p ( t ) p ( x = b, t ) = B,(t) p ( x ,t = 0 ) = I P ( x )
(4.33)
and that q ( x ,t ) is a solution to (4.34) with boundary and initial conditions
q ( x = a , t ) = A q ( t ) q ( x = b, t ) = B q ( t ) q ( x ,t = 0 ) = I q ( x )
(4.35)
Then, because the diffusion equation is a linear secondorder differential equation, = p ( x , t ) q ( x , t ) is a solution for the boundary conditions and the initial condition:
+
T ( X ,t )
T(X
+ = b, t ) = B p ( t )+ B q ( t ) t = 0 ) = I p ( x )+ I q ( x )
= a, t ) = Ap(t) Aq(t)
T(Z
T(X,
(4.36)
The superposition of two solutions therefore also solves the diffusion equation with superposed boundary and initial conditions. Superposition of two displaced stepfunction initial conditions permits solutions that describe diffusion from an initially localized source into an infinite domain. The two stepfunction initial conditions in Fig. 4.4 have errorfunction solutions (Eq. 4.31), and their superposition is a localized source of width A x . The two step functions are m<x
c ( x ,t = 0 ) =
{
W < x < AX Ax<x<m
"0
(4.38)

x = Ax
Figure 4.4: diffusion along
 co
Superposition method for coIistructing localized source for onedimensional 2.
'Although one initial condition is uiiphysical (i.e., a negative concentration), the superposition is physical and justifies its use. The negative concentration is similar to the use of a negative electrical image charge to solve the electrostatics problem of the potential field produced by a positive charge in a planar halfspace where the plane bounding the halfspace is held at zero potential. The negative image charge outside the halfspace allows superposition and satisfies the boiindary condition at the plane bounding the halfspace [3].
85
4 3 DIFFUSIVITY AS A FUNCTION OF CONCENTRATION
Each step function evolves according to an errorfunction solution of the type given by Eq. 4.31. and their superposition is
When
Ax
is small compared to the distance x, (4.40)
where the source strength,
nd,
is given by
When c is assigned units of particles per unit length, nd corresponds to the total number of particles in the source, and Eq. 4.40 describes the onedimensional diffusion from a point source as in Fig. 4 . 5 ~ .Also, when c has units of particles per unit area, nd has units of particles per unit length and Eq. 4.40 describes the onedimensional diffusion in a plane in two dimensions from a line source initially containing nd particles per unit length as in Fig. 4.5b. Finally, when c has units of particles per unit volume, nd has units of particles per unit area, and Eq. 4.40 describes the onedimensional diffusion from a planar source in t’hree dimensions initially containing nd particles per unit area as in Fig. 4 . 5 ~ . These results are summarized in Table 5.1.
Figure 4.5: Onedirrierisiorial diffusion into an infinite doriiaiii. (a) Point source diffusing into it liric. (b) Line soiircc diffusing into a plane. ( c ) Planar source diffusiiig into a volume.
4.3 DlFFUSlVlTY AS A FUNCTION OF CONCENTRATION When D is a function of concentration [i.e., D = D ( c ) ] ,Eq. 4.2 takes the form dC V .[ D ( c ) V C ] dt
(4.42)
This differential equation is generally nonlinear [depending upon the form of D ( c ) ] . and solutions therefore can be obtained analytically only in certain special cases which are not discussed here [4].
86
CHAPTER 4: THE DIFFUSION EQUATION
When Fick’s law applies, the concentration profile generally contains information about the concentration dependence of the diffusivity. For constant D , stepfunction initial conditions have the error function (Eq. 4.31) as a solution to dc/dt = Dd2c/dx2.When the diffusivity is a function of concentration,
dC d2c dD(c) (8c)2 = D(c)+dt
dx2
(4.43)
dc
For identical initial conditions, the difference between a measured profile and the errorfunction solution is related to the last (nonlinear) term in Eq. 4.43. When diffusivity is a function of local concentration, the concentration profile tends to be relatively flat at a concentration where D ( c ) is large and relatively steep where D ( c ) is small (this is demonstrated in Exercise 4.2). Asymmetry of the diffusion profile in a diffusion couple is an indicator of a concentrationdependent diffusivity. Matano developed a graphical method which, for certain classes of boundary value problems, relates the form of the diffusion profile with the concentration dependence of the interdiffusivity, E ( c ) , introduced in Section 3.1.3 [ 5 ] . This method can determine 6 ( c )from the diffusion profile in chemical concentrationgradient diffusion experiments where atomic volumes are sufficiently constant so that changes in overall specimen volume are insignificant and diffusion can be formulated in a Vframe. The method uses scaling, as discussed in Section 4.2.2. Consider a case where the initial and boundary conditions for a diffusion couple are
c(x,t= 0) =
{ :I
00<x
c (  m , t ) = c: Using the scaling parameter q = x/&,
C(00,t)
(4.44)
= c1R
the diffusion equation becomes (4.45)
and the initial and boundary conditions become
c1(q = 00)= c?
c1(q = 00) = c1L
(4.46)
Equation 4.45 can be integrated as (4.47) If c1 is a monotonically increasing function, variables can be changed so that (4.48)
If the profile is measured at some particular time t = 7, x = q&?,
so (4.49)
4.4: DIFFUSIVITY AS A FUNCTION OF TIME
87
because dcl/dx(cl = cF) = 0. Equation 4.49 is an equation for 6 in terms of integrals and derivatives of the function q ( x ) and its inverse x ( c ~ )which , can be determined from a measured profile. The boundary condition (4.50) determines the position of the original interface (commonly termed the Matano interface) where x = 0 (Exercise 4.1 demonstrates this). The expression for the interdiffusivity is (4.51) Equation 4.51 is an integral equation that can be used to determine E ( c 1 ) by a graphical construction or numerical solution. The derivative required in Eq. 4.51 is provided by the measured concentration profile at time r and the integration is performed on the inverse of q ( z ) [6]. However, this historically important method is only moderately accurate, and it would be preferable to obtain diffusion profiles for various assumed diffusivities as a function of concentration by computation. D(c) could be deduced by fitting calculated results for a parametric representation of 6 ( c ) to an experimentally determined diffusion profile. 4.4
DlFFUSlVlTY AS A FUNCTION OF TIME
When D is a function of time, but not position, Eq. 4.2 takes the form
dC
 = V . [D(t)Vc]= D ( t ) V 2 c at
(4.52)
This could be the case for a diffusion specimen that is slowly cooled while a uniform temperature is maintained. Problems of this type can be treated by making the change of variable TO
=
Jd
t
D(t’) dtl
(4.53)
Then d c / d t = (dc/dTD)(dTD/dt)= (dC/dTD)D(t)and Eq. 4.52 is transformed to dC drD
= v 2 c
(4.54)
) unit diffusivity. Equation 4.54, with the same with the solution c = c ( x , r ~ for form as Eq. 4.18, holds when D is uniform. If the boundary conditions for a timedependent diffusivity problem are invariant under this change of variable, solutions from known constantD problems can be applied to the timedependent D case. Consider, for example, the boundaryvalue problem in Fig. 4.2, which for the constantD case was solved by Eq. 4.31. Because TD = 0 when t = 0, the initial and boundary conditions are invariant under the change of variable, and the
88
CHAPTER 4: THE DIFFUSION EQUATION
solution is
(4.55)
4.5
DlFFUSlVlTY AS A FUNCTION OF DIRECTION
In the expressions for Fourier's law of heat conductivity and Fick's law for niass flux, it has been assumed that the flux vector is always parallel to the driving force vector. However, these vectors are not parallel for general materials. For instance, consider a bar. made of alternating layers of copper and silica glass, which is conducting heat from a reservoir at high temperature to one of lower temperature, as in Fig. 4.6. Because copper's heat conductivity is more t,han 60 times greater than silica's, the temperature along each inclined copper sheet will be nearly uniform. Furthermore, because the thermal gradient is always normal to lines of uniform temperature, it points in a direction approximately normal to the copper sheets. However, the heat flux is parallel to the bar because the only sources and sinks for heat are the reservoirs at the ends. This hypothetical example is similar to the case of a graphite single crystal. Graphite has a hexagonal Bravais lattice. Along the basal planes, the carbon bonding is covalent, so the thermal conductivity is K11 = 355 J m' s' K* , nearly that of carbondiamond. Between the graphite layers, where the bonding is very weak, the conductivity is much lower, K l = 89.3 J m  l s  l Kl . Figure 4.6 is therefore representative of singlecrystal graphite, where the basal plane is parallel to the layers shown. In general, the properties of crystals and other types of materials, such as composites, vary with direction (i.e., macroscopic materials properties such as mass diffusivity and electrical conductivity will generally be anisotropic). It is possible to generalize the isotropic relations between driving forces and fluxes to account for
High conductivity
Low conductivity Figure 4.6: Tlierrrial conduction in a laminar composite. The macroscopic value of the thermal conductivity depends on the individual values of conductivity for the materials as well as the inclination of the larriiriates.
4 5 DIFFUSIVITY AS A FUNCTION OF DIRECTION
89
a n i ~ o t r o p y .The ~ isotropic form for Fick’s law is
f = DVc
dC dXi
Ji = D
(4.56)
where the final expression represents three equations, one for each coordinate axis, written in component form. For the anisotropic case, there is a linear relation between the flux and gradient vectors. As discussed in Section 1.3.7, the matrix of the linear coefficients depends on the particular material and the orientation of the material with respect to the Vframe:
or in component form,
J~ =
dC ED^^8%
(4.58)
3
or simply,
f= D V c
(4.59)
D is called the diffusivity tensor and acts as an object that connects one vector to another (e.g., the flux vector with the gradient vector). This connection can be written in matrix form as in Eq. 4.57. The diffusivity tensor D is symmetric (i.e.> Dij = D j i ) for any underlying material symmetry. The anisotropic form of Fick’s law would seem to complicate the diffusion equation greatly. However, in many cases, a simple method for treating anisotropic diffusion allows the diffusion equation to keep its simple form corresponding to isotropic diffusion. Because Daj is symmetric, it is always possible to find a linear coordinate transformation that will make the Dij diagonal with real components (the eigenvalues of D ) . Let elements of such a transformed system be identified by a “hat.” Then B,, 0 0 (4.60)
.=[
i3]
;
The diagonal elements of b are the eigenvalues of D, and the coordinate system of b defines the principal axes 21,22, 23 (the eigensystem). In the principal axes coordinate system, the diffusion equation then has the relatively simple form
det
Dll D12 Dl3
Dl2 022 023
X
Dl3 023 033 
=0
(4.62)
90
CHAPTER 4: THE DIFFUSION EQUATION
If & is the matrix that rotates the original ( 2 1 , 2 2 , x 3 ) coordinate system into the principal ( 2 1 , 2 2 , 2 3 ) system, then according to Eq. 1.36, fi must be related to D by D = RDRl (4.63) To solve the diffusion equation in the principal coordinate system (i.e., Eq. 4.61), the Cartesian space can now be stretched or contracted along the principal axes by scaling:
(4.64) A1/2
This scaling conserves the volume. Using Eq. 4.64, the diffusion equation can now be written in terms of the &: (4.65) where V = ( 6 1 1 f i 2 2 f i 3 3 ) 1 / 3 . Equation 4.65 has the same form as Fick’s second law for a material with a constant isotropic diffusivity. Thus, known solutions to the diffusion equation for constant isotropic diffusivity can be used to find solutions for anisotropic constant diffusivities by a simple algorithm. A solution to Eq. 4.65 with ID and coordinates [1,<2,[3 is rescaled back to the the principal axis coordinates 2 1 , 2 2 , 2 3 using Eq. 4.64. If necessary, the system can be transformed back into the original, anisotropic laboratory coordinate system with D = &‘DB. The diffusivity tensor has special forms for particular choices of coordinate axes if the diffusing body itself has special symmetry (e.g., if it is crystalline). Neumann’s principle states: The symmetry elements of any physical property of a material must include the symmetry elements of the point group of the materiaL4
A consequence of Neumann’s symmetry principle is that direct tensor Onsager coefficients (such as in the diffusivity tensor) must be symmetric. This is equivalent to the addition of a center of symmetry (an inversion center) to a material’s point group. Thus, the direct tensor properties of crystalline materials must have one of the point symmetries of the 11 Laue groups. Neumann’s principle can impose additional relationships between the diffusivity tensor coefficients Dij in Eq. 4.57. For a hexagonal crystal, the diffusivity tensor in the principal coordinate system has the form D11 0 0 (4.66) 4This also applies t o the macroscopic properties of composite materials with underlying symmetrylike honeycomb, wood, and woven materialsfor which the crystal structure, if any, may play no direct role.
91
EXERCISES
when i g lies along the crystal's caxis arid il and i 2 lie anywhere in the basal plane. Exercise 4.6 demonstrates that the diffusivity tensor in a cubic crystal has the form
ro 0
01
(4.67)
and that the diffusion is therefore isotropic. Forms of the diffusivity tensor D for other crystal systems are tabulated in Nye's text [7]. Bibliography 1. I.M. Gelfand and S.V. Fomin. Calculus of Variations. PrenticeHall, Englewood Cliffs, NJ. 1963. 2. W.C. Carter, J.E. Taylor, and J.W. Cahn. Variational methods for microstructural evolution. J O M , 49(12):3036. 1997.
3. P.M. Morse and H. Feshbach. Methods of Theoretical Physics, Vols. 1 and 2. McGrawHill, New York, 1953. 4. J. Crank. The Mathematics of Diffusion. Oxford University Press, Oxford, 2nd edition. 1975.
5. C. hlatano. On relation between diffusion coefficients and concentrations of solid metals (the nickelcopper system). Jpn. J . Phys., 8(3):109113, 1933.
6. P. Shewmon. Diffusion in Solids. The Minerals, Metals and Materials Society, Warrendale, PA, 1989. 7 . J . F . Nye. Physical Properties of Crystals. Oxford University Press, Oxford, 1985. 8. L.C.C. Da Silva and R.F. hlehl. Interface and marker movements in diffusion in solid solutions of metals. Trans. AIME, 191(2):155173, 1951.
EXERCISES
4.1 Consider the BoltzmannhIatano analysis leading to Eq. 4.51. Explain why the condition imposed by Eq. 4.50 determines the location of the x = 0 plane (i.e.. the position of the original interface). Solution. The laboratory coordinate system is used and there is no change in the overall specimen volume. The integral in Eq. 4.50 is proportional t o the sum area 1 area 2 in Fig. 4.7. Area 1 is positive and area 2 is negative. When z = 0 is set at the position of the original interface, area 2 is proportional t o the amount o f diffusant that has left
+
0
Figure 4.7:
X
Composition profile arising from interdiffusiori
92
CHAPTER 4: THE DIFFUSION EQUATION
the original block o f composition c f , and area 1 is proportional t o the amount that has entered the original block of composition c p . Because these quantities must be equal, the condition imposed by Eq. 4.50 determines the z = 0 plane.
5,which measures the interdiffusion between Cu and Zn in the laboratory frame, is a strong function of the concentration of Zn. The curve describing 5 ( c z n ) is concave upward and roughly parabolic in shape, and 6 ( c z n ) increases by a factor of about 20 when the Zn content increases from 0 to 30 at. % [8]. Describe how the shape of the diffusionpenetration curve for a diffusion couple made of Cu/CuSO at. % Zn is expected to deviate from the symmetric form of the constant diffusivity errorfunction solution.
4.2 The interdiffusivity,
Solution. Base your argument on the BoltzmannMatano solution (Eq. 4.51), which links the interdiffusivity with the shape of the diffusion curve. T w o factors are present: the integral under the diffusion curve from cz", t o the concentration in question, c z n , and the reciprocal o f the slope a t czn. The integral varies from 0 a t z = 00 t o 0 at z = m and reaches a maximum a t z = 0 (see Exercise 4.1). The slope varies from 0 a t z = 03 t o 0 a t x = m and reaches a maximum somewhere in between. A little trial and error quickly shows t h a t the only way D can increase by a factor of 20 with increasing czn with a difFusion curve o f reasonable shape is t o have a curve with a small slope a t high CZ,, and a large slope at low czn. Such a curve is markedly nonsymmetric around its midpoint. Figure 4.8 shows an observed interdifFusion profile for this system.
30
0
0.6 0.4 0.2
0
0.2
Distance (cm) Figure 4.8:
Silva and Mehl [8].
Concentration profile observed in Cu30 at. % Zn diffusion couple.
From Da
4.3 The Kirkendall effect can be studied by embedding an inert marker in the original stepfunction interface (x = 0) of the diffusion couple illustrated in Fig. 3.4. Show that this marker will move in the Vframe or, equivalently, with respect to the nondiffused ends of the specimen, according to
x, where
cy
= at1I2
is a constant.
Solution. According t o Eq. 3.23, the instantaneous velocity of any marker is given by (4.68)
93
EXERCISES
Now, in general, c1 = C I ( ~ ) ,where q = x/&. Because ( D l  0 2 ) is a function of 7, we can represent it as [Dl  0 2 1 = h(q). Similarly, we can write d c l / d x = (dcl/dq)t’/’ = f ( 7 ) t’l2. Putting these results into Eq. 4.68 yields
A solution that satisfies this equation and also the initial condition that x m = 0 when t=Ois xm = at’/2 with the constant a given by a = 2 f l l h ( a ) f ( a ) .
4.4 A diffusion measurement at the temperature TOis made by annealing a dif
fusion couple comprised of two semiinfinite bars. However, there is a complication; after the completion of the isothermal anneal, carried out at TOfor the time to, the specimen must be cooled to room temperature a t a finite rate. During this cooling period, a small amount of additional nonisothermal diffusion occurs. If an expression can be found for the amount of time, At, re
quired to produce this same additional increment of diffusion at the constant
temperature TO,the specimen could be analyzed very simply at the end of the experiment by assuming that it was annealed at To for the time to At. Assume that D = Doexp[E/(kT)] and that the temperature during the cooling period is
+
(4.69)
+
where a is constant. When t = t o a, T = To12 and it may be assumed that beyond that time during the cooling, any further diffusion is negligible. Find an expression for At. Solution. During the cooling the diffusivity is time dependent and the solution is therefore obtained by utilizing the variable T O , which is described and defined in Section 4.4. The value o f T D a t the end o f the actual experiment is then (4.70) where D = DOexp[E/(ICTo)] and
D ( t ) = Do e  E / ( k T o )
(4.71)
Putting these expressions into Eq. 4.70 and integrating,
(4.72) On the other hand, the value of r achieved a t the end of an isothermal diffusion anneal o f duration t o A t is = D o e  E / ( k T o ) [+ t oAt] (4.73)
+
rzd’
The amounts o f diffusion achieved in these two anneals will be equal if Therefore, setting these two quantities equal,
.Ed
= rzd’
(4.74)
94
CHAPTER 4: THE DIFFUSION EQUATION
4.5 The transport relations for the thermoelectric effect in an isotropic material
are
+
JQ = UT LQQ T
LQ~U$
(4.75)
VT LqQ  LqqU$ (4.76) T (a) Write the corresponding relations that apply for an anisotropic material. Jq + =
(b) From Onsager's symmetry theorem, what can be said about the symmetry of the ranktwo tensors that are involved and any relations between them? (c) Are the crosscoupling tensors (which couple nonconjugate forces and
fluxes) positive definite? Solution.
For an anisotropic material, the coefficients must be ranktwo tensors.
Therefore,
(4.77) (4.78) or in a matrix representation involving rankone tensors (vectors) and ranktwo tensors,
(4.79) (a) When written in full, Eq. 4.79 becomes
 J?
JZQ
J?
51"
J,4
 539
.
ff11
ff12
ff13
p11
pl2
p13
ff2l
ff22
ff23
p2l
p22
p23
a31
a32
ff33
p31
p32
p33
711
712
713
711
v12
713
721
722
723
721
731
732
733
731
722 v32
v33
7723
(b) Onsager's relation applies t o the entire 6 x 6 matrix above, so
p2, = y3% or
P = Y~
at, = a j 2
or
a = aT
7 1 %= ~ ~
or
TI =
7,~
(4.81)
vT
2',
2
(c) If a flux, 2 , is coupled t o a force, by a tensor, <, so that = the tensor is positive definite if the projection of 2 on i b is always positive; that is,
p . p =( < l b ) . d b > O
(4.82)
The directeffect a and 77 must be positive definite because of Fourier's law of heat conduction (where the thermal conductivity is always positive, according t o
EXERCISES
95
Eq. 2.18) and Ohm's law for electrical conduction (where the electrical conductivity is also always positive, according t o Exercise 2.1's solution). However, this is not and y . For example, in mass necessarily the case for the crosseffect tensors diffusion in a thermal gradient, the heat o f transport can be either positive or negative; the direction of the atom flux in a temperature gradient can then be in either direction. The anisotropic equivalent t o the heat of transport relates the direction of the mass difFusion t o the direction o f the temperature gradient. There is no physical requirement that these quantities could not be in reversed directions, and indeed, sometimes they are.
4.6 Show by the use of symmetry arguments that the diffusivity in a cubic crystal
must be isotropic. Solution. Take the three cubic axes 2 1 , 2 2 , and 2 3 as the coordinate system and assume initially t h a t the diffusivity has the most general form possible, which, according t o Eq. 4.57, is
D=
I:
[
Dii
D12
D12
D22
023
013
023
033
I:
013
1
(4.83)
Now, establish a concentration gradient o f magnitude, g, successively along 21,2 2 , and The three corresponding flux vectors will then be, respectively,
23.
g[
9
013
[
9
023
[ I,I]
(4.84)
Because of the cubic crystal symmetry, the fluxes parallel t o the directions o f the gradients in the three cases (i.e.,  g D 1 1 ,  g D 2 2 , and  9 0 3 3 ) must be equal. Therefore, 0 1 1
(4.85)
= D22 = 0 3 3
Preservation o f fourfold symmetry along the 2 1 , 2 2 , and 2 3 axes requires that any flux components in directions perpendicular t o the gradients be zero. Therefore, 9012
and
D = [
i
D
:I=.[;
=9013 =gD23 = 0
O
0
1
(4.86)
0
:] 0
(4.87)
According t o Eq. 4.63, the diffusivity tensor in any other rotated system (indicated by a prime) will have the form
r l Because
D ' = D ,the
o 01
(4.88)
difFusivity is isotropic.
4.7 Consider twodimensional anisotropic diffusion in an infinite thin film where
the initial condition consists of a point source of atoms located at 2 1 = x2 = 0. The diffusivity tensor D , in arbitrary units, in the ( X I ,z2) coordinate system is
.=[
4
y] 4
(4.89)
96
CHAPTER 4: THE DIFFUSION EQUATION
Determine the fundamental solution, c = c ( q , 22,t ) ,of the diffusion equation for the point source in this coordinate system. Solve the problem in the principal axes coordinate system and then transform the solution back to the ( 2 1 , 22) system. Note that a rotation matrix, a, has the properties det = 1 and B' = RT,where BT is the transpose of a. Solution. First transform the problem t o the principal axes system. The eigenvalue equation for
D
is
Therefore, the diffusivity tensor in the principal axes system is
16 0 D=[ 0 11
(4.91)
The rotation, B, required t o rotate the original (x1,x2) coordinate system into the principal coordinate system must satisfy
D = BDR'
(4.92)
yielding a set o f linear equations which, in conjunction with the properties of rotation matrices given above produces the result
.=[? $1
(4.93)
which corresponds t o a rotation of x/6. Now solve the diffusion problem in the principal coordinate system where the difFusion equation is
(4.94) Changing variables in Eq. 4.94 using 21 = (&/@)
V
=
22 =
(&/a)&, and
d m , a new difFusion equation is obtained with the solution C(El,EZ,t)=
N a
 N 
e
(€?+€3/(4Dt)
= c(21,22,t)
el~t:/(4Dllt)+~:Hl(4D~~t)l
(4.95)
4nvt
The concentration therefore spreads t o an ellipse.

We can now find the final solution in the original coordinate system by using
f=&r'
(4.96)
where ?= ( 2 1 , i z )and r'= ( x l , x 2 )t o solve for 21 and $2 and by putting the results into Eq. 4.95. It is an ellipse of aspect ratio 4 with axes rotated x/6 with respect t o the axes of the original coordinate system.
4.8 To measure selfdiffusivities along different directions in a hexagonal crystal,
a flat surface is prepared perpendicular to the direction along which the dif
EXERCISES
97
fusivity is to be measured. A thin instantaneous plane source is deposited on this surface and the specimen is then annealed at a constant diffusion temperature. After the diffusion anneal, the diffusionpenetration profile normal to the surface is measured and D is determined. (The technique is described further in Section 5.2.1.) If the selected crystal direction makes an angle 8 with the caxis of the crystal, show that the measured D [i.e., D(O)] is given by (4.97) D ( 8 ) = DS3cos2 8 D l l sin2 8
+
0
Note that the concentration gradient will always be along the selected crystal direction (perpendicular to the planar source), regardless of the direction of the diffusion flux.
k
Solution. Adopting a principal axis system in which is parallel t o the caxis and .i and j lie in the basal plane, the diffusivity tensor will have the form given in Eq. 4.66 and the flux will be given by (4.98) Thenormal t o the isoconcentration surfaces will be A = V c / l V c l and the component of J along 4 [i.e., J ( e ) ] is
Therefore,
But
VC. k
1
(4.101)
(4.102) Therefore, Eq. 4.100 has the form
q e ) = D~~sin’ e + 0 3 3 cos’ e
(4.103)
CHAPTER 5
SOLUTIONS TO THE DIFFUSION EQ UAT I0N
In Chapter 4 we described many of the general features of the diffusion equation and several methods of solving it when D varies in different ways. We now address in more detail methods to solve the diffusion equation for a variety of initial and boundary conditions when D is constant and therefore has the relatively simple form of Eq. 4.18; that is,
dC
 = DV2c
at
This equation is a secondorder linear partialdifferential equation with a rich mathematical literature [l].For a large class of initial and boundary conditions, the solution has theorems of uniqueness and existence as well as theorems for its maximum and minimum values. Many texts, such as Crank’s treatise on diffusion [2], contain solutions in terms of simple functions for a variety of conditionsindeed, the number of worked problems is enormous. As demonstrated in Section 4.1, the differential equation for the “diffusion” of heat by thermal conduction has the same form as the mass diffusion equation, with the concentration replaced by the temperature and the mass diffusivity replaced by the thermal diffusivity, K . Solutions to many heatflow ‘If the diffusivity is imaginary, the diffusion equation has the same form as the timedependent Schrodinger’s equation at zero potential. Also, Eq. 4.18 implies that the velocity of the diffusant can be infinite. Schrodinger’s equation violates this relativistic principle. Kinetics of Materials. By Robert W. Balluffi, Samuel M. Allen, and W. Craig Carter. Copyright @ 2005 John Wiley & Sons, Inc.
99
100
CHAPTER 5: SOLUTIONS TO THE DIFFUSION EQUATION
boundaryvalue problems can therefore be adopted as solutions to corresponding mass diffusion problems.2 For problems with relatively simple boundary and initial conditions, solutions can probably be found in a library. However, it can be difficult to find a closedform solution for problems with highly specific and complicated boundary conditions. In such cases, numerical methods could be employed. For simple boundary conditions, solutions to the diffusion equation in the form of Eq. 4.18 have a few standard forms, which may be summarized briefly. For various instantaneous localized sources diffusing out into an infinite medium, the solution is a spreading Gaussian distribution:
C(F,t) =
er’?/(4Dt)
nd
2d (.rrDt)d/2
where d is the dimensionality of the space in which matter is diffusing and nd is the source strength introduced in Section 4.2.3. When the initial condition can be represented by a distribution of sources, one simply superposes the solutions for the individual sources by integration, as in Section 4.2.3. When the boundaries are planar orthonormal surfaces, solutions to the diffusion equation have the form of trigonometric series. For diffusion in a cylinder, the trigonometric series is replaced by a sum over Bessel functions. For diffusion with spherical symmetry, trigonometric functions apply. All such solutions can be obtained by the separationofvariables method, which is described below. A third methodsolution by Laplace transformscan be used to derive many of the results already mentioned. It is a powerful method, particularly for complicated problems or those with timedependent boundary conditions. The difficult part of using the Laplace transform is backtransforming to the desired solution, which usually involves integration on the complex domain. Fortunately, Laplace transform tables and tables of integrals can be used for many problems (Table 5.3). 5.1 STEADYSTATE SOLUTIONS A particularly simple case occurs when the diffusion is in a steady state and the composition profile is therefore not a function of time. Steadystate conditions are often achieved for constant boundary conditions in finite samples at very long times.3 Then dc/dt = 0, all local accumulation (divergence) vanishes, and the diffusion equation reduces to the Laplace equation,
v2c= 0
(5.2) Solutions to the Laplace equation are called harmonic functions. Some harmonic functions are given below for particular boundary conditions.
5.1.1
One Dimension
Consider diffusion through an infinite flat plate of thickness L , with 0 subject to boundary conditions c(0, t ) = co
c(L,t ) = CL
< x < L, (5.3)
2Carslaw and Jaeger’s treatise on heat flow is a primary source [3]. 3Estimates of times required for “nearly steadystate’’ conditions are addressed in Section 5.2.6.
5 1 STEADYSTATE SOLUTIONS
101
Integrating the onedimensional Laplacian, d2c/ d x 2 = 0 , twice yields ~ ( z= ) alz
+ a2
(5.4)
where al and a2 are integration constants. Solving for the integration constants using the boundary conditions, Eq. 5 . 3 , produces the onedimensional steadystate solution, c ( x ) = c0  (c0  c t) z (5.5)
L
i.e., the concentration varies linearly across the plate as illustrated in Fig. 5.1. The flux is constant and proportional t o the slope:
0
Figure 5.1:
X 
Concentration, C(Z). vs.
L
for steadystate diffusion through a plate
J
5.1.2 Cylindrical Shell Consider steadystate diffusion through a cylindrical shell with inner radius r'" and outer radius rollt as in Fig. 5.2. The boundary conditions are c ( T ' " , 8,z , t ) = c'"
c(rUUt. 8. z . t ) = c""~
(5.7)
The Laplacian operator operating on c(r, 8. z ) in cylindrical coordinates is
Figure 5.2: shell.
Concentration,
c(T),
vs.
T
for steadystate diffusion through a cylindrical
102
CHAPTER 5 SOLUTIONS TO THE DIFFUSION EQUATION
Because the boundary conditions are independent of 0 and z , the solution will also be independent of these variables. The solution must therefore satisfy
Integrating twice produces
c ( r ) = a1 l n r
+ a2
(5.10)
and applying the boundary conditions gives
c ( r ) = cln 
 Gout
(5.11)
In(r o u t / r i n )
The flux J = D(dc/dr) depends inversely on r : ,in
 ,out
1
(5.12)
Note that the total current of particles entering the inner surface per unit length of cylinder [ I = J ( r i " ) 2 m i n ] is the same as the total current leaving the outer surface, ,in  ,out
(5.13)
which is a requirement for the steady state. 5.1.3
Spherical Shell
The Laplacian operator operating on c(r, 8 , # ) in spherical coordinates is
The steadystate solution for diffusion through spherical shells with boundary conditions dependent only on r may be obtained by integrating twice and determining the two constants of integration by fitting the solution to the boundary conditions. 5.1.4
Variable Diffusivity
When steadystate conditions prevail and D varies with position (e.g., D = D ( f ) ) , the diffusion equation can readily be integrated. Equation 4.2 then takes the form
In one dimension] the solution can then be obtained by integration,
+
c ( z ) = c(z1) a1
I: &
(5.15)
103
5 2 . NONSTEADYSTATE DIFFUSION
N0N S T EA DY STAT E (TIME DEPENDENT) DIFFUSI0N
5.2
When the diffusion profile is timedependent, the solutions to Eq. 4.18 require considerably more effort and familiarity with applied mathematical methods for solving partialdifferential equations. We first discuss some fundamentalsource solutions that can be used to build up solutions to more complicated situations by means of superposition. 5.2.1
Instantaneous Localized Sources in Infinite Media
Equation 4.40 gives the solution for onedimensional diffusion from a point source on an infinite line, an infinite thin line source on an infinite plane, and a thin planar source in an infinite threedimensional body (summarized in Table 5.1). Corresponding solutions for two and threedimensional diffusion can easily be obtained by using products of the onedimensional solution. For example, a solution for threedimensional diffusion from a point source is obtained in the form
where
n d z , nd,,
and
nd,
are constants. This may be written simply c(r,t) =
nd
er2/(4Dt)
(5.17)
( 4 ~ D t ) ~ ~ ~
where n d E n d , x n d , x n d , This result has spherical symmetry and describes the spreading of a point source into an infinite domain. Integration verifies that n d is equal to the total amount of diffusant in the system. As t + 0, the solution approaches a delta function form, corresponding to the initial localized source [i.e., Table 5.1: Fundamental Solutions for Instantaneous, Localized Sources in One, Two, and ThreeDimensional Infinite Media
Solution Type
Symmetric Part of V2
Fundamental Solution
OneDimensional Diffusion Point source in 1D Line source in 2D Plane source in 3D
d2
2 2
c(z,t)=
(4n;:)1,2
ez2/(4Dt)
TwoDimensional Diffusion Point source in 2D Line source in 3D
I d_ d _ r d r r z
ThreeDimensional Diffusion Point source in 3D
1 d 2 d T z rdr
C(T,
t)=
(4n;:)3,2
er2/(4Dt)
104
CHAPTER 5 : SOLUTIONS TO THE DIFFUSION EQUATION
C(T,t = 0 ) = b ( ~ ) ]Corresponding .~ results for twodimensional diffusion are given in Table 5.1. The form of the solution for onedimensional diffusion is illustrated in Fig. 5.3. The solution c(x,t) is symmetric about x = 0 (i.e., c(x,t ) = c(x, t ) ) . Because the flux at this location always vanishes, no material passes from one side of the plane to the other and therefore the two sides of the solution are independent. Thus the general form of the solution for the infinite domain is also valid for the semiinfinite domain (0 < x < m) with an initial thin source of diffusant at x = 0. However, in the semiinfinite case, the initial thin source diffuses into one side rather than two and the concentration is therefore larger by a factor of two, so that
c(x,t)=
nd
(rD t )l I 2
e22/(4Dt)
(5.18)
Figure 5.3: Spreading of point, line, and planar diffusion sources with increasing time according to the onedimensional solution in Table 5.1. Curves were calculated from Eq. 5.18 for times shown and n d = 1, D = and 1 < 3: < 1 (all units arbitrary).
Equation 5.18 offers a convenient technique for measuring selfdiffusion coefficients. A thin layer of radioactive isotope deposited on the surface of a flat specimen serves as an instantaneous planar source. After the specimen is diffusion annealed, the isotope concentration profile is determined. With these data, Eq. 5.18 can be written X2
In *c = constant  
4 *Dt
(5.19)
and *Dcan be determined from the slope of a In *c vs. x2 plot, as shown in Fig. 5.4.5 4 A delta function, 6(F'),is a distribution that equals zero everywhere except where its argument is zero, where it has an infinite singularity. It has the property j(F')6(F Fo)dr'= f ( r ' 0 ) ; so it also follows that s 6 ( F  Fo)dr'= 1. The singularity of 6 ( F  TO)is located at Fo. 5This technique can be used to measure the diffusivity in anisotropic materials, as described in Section 4.5. Measurements of the concentration profile in the principal directions can be used to determine the entire diffusion tensor.
s
5 2 . NONSTEADYSTATE DIFFUSION
\ ,+Slope
= 1/(4
105
*Dt)
Figure 5.4: Plot of In *c vs. xz used to determine selfdiffusivity when an iiistaiitaneous planar source is used and Eq. 5.18 applies.
5.2.2
Solutions Involving the Error Function
The instantaneous localsource solutions in Table 5.1 can be used to build up solutions for general initial distributions of diffusant by using the method of superposition (see Section 4.2.3). Section 4.2.2 shows how to use the scaling method to obtain the error function solution for the onedimensional diffusion of a step function in an infinite medium given by Eq. 4.31. The same solution can be obtained by superposing the onedimensional diffusion from a distribution of instantaneous local sources arrayed to simulate the initial step function. The boundary and initial conditions are
c(x,O) = dc
(x dx
{0
cg
x>o x
(5.20)
= kx,t)= 0
The initial distribution is simulated by a uniform distribution of point, line, or planar sources placed along x > 0 as in Fig. 5.5. The strength, or the amount of diffusant contributed by each source, must be co dx. The superposition can be achieved by replacing n d in Table 5.1 with c(Z)dV [c(x)dxin one dimension] and integrating the sources from each point. Consider the contribution at a general position x from a source at some other position 5. The distance between the general point x and the source is 5  x, thus (5.21)
So the solution corresponding to the conditions given by Eq. 5.20 must be the integral over all sources, (5.22)

m
t
I
X
I
x=o
I
6
Figure 5 . 5 : Diagram used to determine the contribution at the general point z of a local souice of strength cg d< located at [.
106
CHAPTER 5 SOLUTIONS TO THE DIFFUSION EQUATION
or by transforming the integration variable by using u = (<  x ) / m and the properties of an even integrand, c ( x , t )= 
=co
2
eu2 du
+ erf co 2
()
(5.23) X
2
m
which is consistent with the solution given by Eq. 4.31. Summations over point, line, or planarsource solutions are useful examples of the general method of Green's functions. For instance, the boundary and initial conditions for a triangular source are x>a c(x,t = 0) =
(5.24) 0
dC ( x = f c q t )
=
dX
x < a
0
A solution to this boundaryvalue problem can be obtained by using Eq. 4.40 with a positiondependent pointsource density (this method is useful for solving Exercise 5.7). As a last example, the solution for twodimensional diffusion from a line source lying along z in three dimensions can be obtained by integrating over a distribution of point sources lying along the zaxis. If the point sources are distributed so that the source strength along the line is n d particles per unit length, the contribution of an effective point source of strength n d d< at (0, O,<) to the point ( x ,y, z ) is dc =
n d d< e[x2+y2+(Ez)2]/(40t) (4nD t )3/2
(5.25)
so that
In cylindrical coordinates, r2 = x 2 the entrv in Table 5.1.
+ y2 and, after integration, in agreement with (5.27)
where the source strength
nd
has dimensions length'.
6Green's functions arise in the general solution t o many partialdifferential equations. They are generally obtained from the fundamental solution for a point, line, or planar source. Subsequently, an integral equation for a general solution is obtained by integrating over all the source terms; the fundamental solution becomes the kernel t o the integral equation, which is the term that multiplies the source density in the integrand.
107
5.2: NONSTEADYSTATE DIFFUSION
5.2.3
Method of Superposition
In Section 4.2.3 we described application of the method of superposition to infinite and semiinfinite systems. The method can also be applied, in principle, to finite systems, but it often becomes unwieldy (see Crank’s discussion of the reflection method [2]). 5.2.4
Method of Separation of Variables: Diffusion on a Finite Domain
A standard method to solve many partialdifferential equations is to assume that the solution can be written as a product of functions, each a function of one of the independent variables. Table 5.2 provides several functional forms of such solutions. Product Solutions for the SeparationofVariables Method in Table 5.2: Cartesian and Cylindrical Coordinates System
Equation
One dimension, z
d ct  D d2c s
Three dimensions, (z, y , z ) Cylindrical,
(T,
Solution
= DV2c
c(a, t ) = X ( z ) T ( t )
c(a, y , z , t ) = X ( z ) Y ( y ) Z ( z ) T ( t )
dt  ~o~~ c ( r ,8 , z , t ) = R ( r ) @ ( e ) q z ) T ( t )
8, z )
dc
The following example illustrates the method. Consider a onedimensional diffusion problem with the initial and boundary conditions for the domain 0 < x < L:
c(z,O)= co
c ( 0 , t )= 0
c ( L , t )= 0
(5.28)
This situation may represent the diffusion of a highvaporpressure dopant out of a thin film (thickness L , initial dopant concentration cg) of silicon when placed in a c(x,t ) = X ( x ) T ( t and ) vacuum. Assume that the variables are ~ e p a r a b l e Letting .~ substituting into the diffusion equation gives 1 dT
1 d2X
  
DT dt
X dx2
(5.29)
Because the left side depends only on t and the right side depends only on x , each side must be equal to the same constant. This may be understood by considering Fig. 5.6, in which f is a function of y only and g is a function of x only. Each surface is a “ruled” surface; that is, the surface contains lines of constant value running in one direction. If the two functions are equal as in the separation equation (Eq. 5.29), the surface must be flat in both variables. Thus, if the two functions are equal, they are constant. Let that constant be A. Then dT dt
=
XDT
(5.30)
71f a solution is found for the initial and boundary conditions, there is a uniqueness theorem that justifies the assumption. Whether a solution can be found using separation of variables depends on whether the boundary conditions follow the symmetry of the separation variables.
108
CHAPTER 5 SOLUTIONS TO THE DIFFUSION EQUATION
X
X
Figure 5.6:
Represer1tat)ionin (z, y) space of g(z) and f ( y )
and
d2X AX dx2 Equation 5.31 has solutions of the form
(5.31)
=
x ( x )=
{
A sin(fix) + B cos( fix) AIeG”+BIeG” A / / x+ B / /
( A > 0) ( A 0)
(5.32)
( A = 0)
where A and B are constants that must satisfy t,he boundary conditions. For the particular boundary conditions specified in Eq. 5.28, nontrivial solutions to Eq. 5.31 exist only if A > 0 and B = 0. However, there is no nonzero A that can satisfy the boundary conditions for a general X > 0, so X must take on values appropriate to the boundary conditions. Therefore, A,, = n2 7r2 L2
(5.33)
because sin f i L = sin nr = 0, where n is an integer. The A, are the linear differential equation’s eigenvalues for the boundary conditions. Because use of any A,, satisfies the boundary conditions in Eq. 5.28, each of the functions X n ( z )= a, sin nr(5.34)
(
3
satisfies Eq. 5.31 for the boundary conditions in Eq. 5.28. The X,, are known as the eigenfunctions for the boundary conditions. The general solution to Eq. 5.30 is
T ( t )= To e  X D t
(5.35)
where T o is a constant. But A must take on the values given in Eq. 5.33, and t,herefore the timedependent eigenfunction solutions can be written
T T L (=t )T,” e n 2 n 2D t l L z
(5.36)
The general solution, satisfying the boundary conditions. is then (by superposit’ion) a sum of the products of the eigenfunction solutions and is of the form
109
5.2: NONSTEADYSTATE DIFFUSION
where A, = a,T,O. It is now necessary to satisfy the initial condition given in Eq. 5.28. This requires that 00 co =
c
A , sin (n7rz)
(5.38)
n=l
which, as seen in Eq. 5.42, is a Fourier sine series representation of Synopsis of Fourier Series
If a function u ( z ) exists on the interval  L
u(z)=
<+ b
m n=l
CO.
< z < L , u ( z ) can be represented as
[ansin (n.2)
+ bncos
(5.39)
where the coefficients are given by (5.40) (5.41)
I).(.
If u ( z ) is an odd function [ u ( z ) =
and the sine expansion is applied, (5.42)
(5.43)
Similarly, if u ( z ) is an even function [ u ( z ) = u (  z ) ] , all an will vanish and u ( z ) can be written as a cosine expansion only: (5.44)
(5.45)
Finally, any function can be written as a sum of an odd and an even function.
Using Eq. 5.43, the coefficients, A,, are then given by n7r
0
n even
(5.46)
Therefore, the final solution is given by (5.47) The coefficients of the higherorder (shorterwavelength) terms in Eq. 5.47 decrease as l / n . Not only do the shorterwavelength terms start out smaller but they
110
CHAPTER 5 : SOLUTIONS TO T H E DIFFUSION EQUATION
also decay exponentially at rates that scale inversely as the square of the wavelength. Thus, even at times as short as L2/(250), the first term of the series in Eq. 5.47 suffices to a good approximation, such that (5.48) with a maximum error of about 1%. The average composition C in this “longtime” regime can be obtained by integration of Eq. 5.48: 8cO  r 2 D t / L 2 c ( t )= 7 e
(5.49)
C therefore decays exponentially with the characteristic time r = L 2 / ( r 2 0 ) This . is reasonably consistent with estimates of diffusion depths and times in Section 5.2.6. The method of separation of variables can be applied in the same manner to other initial distributions of diffusant. The effort lies only in determining the Fourier coefficients, which, for many cases, can be looked up in tables. If the spatial dimension of the system is higher [e.g., c(z, y, z , t ) ] ,a separate Fourier series must be obtained for each of the three separate functions in the product X ( x ) Y ( y ) Z ( z ) .
Cylindrical Coordinates. The separationofvariables method also applies when the
boundary conditions and initial conditions have cylindrical symmetry (see Eqs. 5.7 , resulting ordinary differential equation for R ( r ) and 5.8). If c ( r ,t ) = R ( r ) T ( t )the is d2R 1dR (5.50)  a 2 R= 0 dr2 r dr
+
+
This equation has general solutions (5.51) where Jo and YOare Bessel functions of order zero of the first and second kind. The an are solved by matching boundary conditions, and the coefficients a, and bn are determined by matching the initial conditions in a Bessel function series expansion. See Carslaw and Jaeger for examples [3]. 5.2.5
Method of Laplace Transforms
The Laplace transform method is a powerful technique for solving a variety of partialdifferential equations, particularly timedependent boundary condition problems and problems on the semiinfinite domain. After a Laplace transform is performed on the original boundaryvalue problem, the transformed equation is often easily solved. The transformed solution is then backtransformed to obtain the desired solution. t ) is defined as The Laplace transform of a function f(z, (5.52)
111
5.2: NONSTEADYSTATE DIFFUSION
The Laplacetransformed f is represented by both the operational form L{f}and the shorthand f. The variable p is the transformation variables8 The key utility of the Laplace transform involves its operation on time derivatives: (5.53) Integrating the righthand side of Eq. 5.53 by parts, t=m
ePtf(x, t )
~
+ p~~
eptf(x, t ) dt = pelf}  f ( x ,t = 0)
t=O
Therefore,
c
{}:
=pC{f}  f ( x , t = O )

(5.54)
(5.55)
The Laplace transform of a spatial derivative of f is seen from Eq. 5.52 to be equal to the spatial derivative of f;that is, (5.56) The method can be demonstrated by considering diffusion into a semiinfinite body where the surface concentration c(x = 0, t ) is fixed:
c(x = 0 , t ) = co dC  ( x = 03, t ) = 0 dX c ( x , t = 0) = 0 for 0 5 x < co
(5.57)
Applying the Laplace transform to both sides of the diffusion equation yields
L: d2? ax2
{ $}
= DC
{ g}
c(x,t= 0) D
p
c=
D
=o
(5.58)
Thus, the Laplace transform removes the tdependence and turns the partialdifferential equation into an ordinarydifferential e q ~ a t i o n The . ~ solution to Eq. 5.58 is t ( x , p )= a l e m x a z e  m x (5.59)
+
The boundary conditions must also be transformed:
? ( x = 0 , p ) =CO
I"
d? (x dX
CO eCPt d t = 
P
(5.60)
= 03,p) = 0
*Technical requirements on p are that its real part must be positive and large enough that the integral converges. gNote that it also automatically incorporates the initial condition.
112
CHAPTER 5: SOLUTIONS TO THE DIFFUSION EQUATION
Solving for the coefficients in Eq. 5.59 leads to the solution (5.61) This solution is then inversely transformed by use of a table of Laplace transforms (see Table 5.3) to obtain the desired solution:
I)&(
[
c(x,t ) = co 1  erf 
= coerfc ( 7 3
(5.62)
where erfc(z) = 1  erf(z) is known as the complementary error function. Note that this solution could have been deduced directly from Eq. 5.23 (the solution for the stepfunction initial conditions for an infinite system) because in that solution, the plane 2 = 0 always maintains a constant composition. Table 5.3:
Selected Laplace Transform Pairs
1
P
pyil
v>1
w
w2
+w 2
1 t" r ( v 1)
+
sin w t
cos w t
Example with TimeDependent Boundary Conditions. Consider the case where a constant flux, J o , is imposed on the surface of a semiinfinite sample:
dC Jo = 0 , t ) =  =constant dX D c(x = 0 ,t ) = co c(x,t = 0 ) = co for 0 5 x < 00
(x
(5.63)
This boundary condition might apply for solute absorption with its rate moderated by some thin passive surface layer. Note that the surface concentration at x = 0 must be a function of time to maintain the constantflux condition (see Fig. 5.7).
5.2: NONSTEADYSTATE DIFFUSION
113
Diffusion profiles necessary to maintain constant flux into a semiinfinite Figure 5.7: body. Note the fixed value of dc/dz(,=o for t > 0.
Using the Laplace transform, (5.64) Equation 5.64 is an inhomogeneous ordinary differential equation and its solution is therefore the sum of the solution of its homogeneous form (i.e., Eq. 5.59) and a particular solution (i.e., E = c o / p ) . Therefore, (5.65) The transformed boundary conditions are
%(x = 0 , p ) = 5, ax PD CO E(x = C q p ) = P Solving for the coefficients a1 and
(5.66)
a2,
CO
e&Fa: E(X1P) =  + p 3 / Jo 2Dl/2 P
(5.67)
Inversely transforming this solution with the use of Table 5.3 yields
The surface concentration must therefore increase as (5.69) 5.2.6
Estimating the Diffusion Depth and Time to Approach Steady State
A rough estimate of the diffusion penetration distance from a point source is the location where the concentration has fallen off by = 0. This occurs when
x
5 M
2 f i
M
l / e of the concentration at
(5.70)
114
CHAPTER 5: SOLUTIONS TO THE DIFFUSION EQUATION
An estimate of the penetration distance for the errorfunction solution (Eq. 5.23) , equivalently, e r f [ x / ( 2 m ) ] = 3/4: which is the distance where c ( x ,t ) = ~ 0 / 8 or corresponds to x RZ 1 . 6 f i (5.71) A reasonable estimate for the penetration depth is therefore again 2m. To estimate the time at which steadystate conditions are expected, the required penetration distance is set equal to the largest characteristic length over which diffusion can take place in the system. If L is the characteristic linear dimension of a body, steady state may be expected to apply at times r >> L2/Dmin, where Dmin is the smallest value of the diffusivity in the body. Of course, there are many physical situations where steadystate conditions will never arise, such as when the boundary conditions are time dependent or the system is infinite or semiinfinite. Bibliography 1. P.M. Morse and H. Feshbach. Methods of Theoretical Physics, Vols. 1 and 2. McGrawHill, New York, 1953. 2. J. Crank. The Mathematics of Diffusion. Oxford University Press, Oxford, 2nd edition, 1975. 3. H.S. Carslaw and J.C. Jaeger. Conduction of Heat i n Solids. Oxford University Press, Oxford, 2nd edition, 1959.
EXERCISES
5.1 A flat bilayer slab is composed of layers of material A and B , each of thickness L . A component is diffusing through the bilayer in the steady state under conditions where its concentration is maintained at c = co = constant at one surface and at c = 0 at the other. Its diffusivity is equal to the constants D A and D B in the two layers, respectively. No other components in the system diffuse significantly. Does the flux through the bilayer depend on whether the concentration is maintained a t c = co at the surface of the A layer or the surface of the B layer? Assume that the concentration of the diffusing component is continuous at the A / B interface. Solution. Solve for the difFusion in each layer and match the solutions across the A / B interface. Assume that c = co a t the surface of the A layer and let c = c ~ be/the~ concentration a t the A / B interface. Using Eq. 5.5, the concentration in the A layer in the interval 0 < x < L is (5.72)
(5.73) For the B slab in the interval L
5 x 5 2L,
(5.75)
EXERCISES
Setting J A =
JB
115
and solving for c A I B , CAIB
= co
DA DA + DB
(5.76)
The steadystate flux through the bilayer is then J=
c0 D
~ D L DA+DB
~
(5.77)
J is invariant with respect t o switching the materials in the two slabs, and therefore it does not matter on which surface c = CO. 5.2 Find an expression for the steadystate concentration profile during the radial
diffusion of a diffusant through a cylindrical shell of thickness, AR,and inner radius, R'", in which the diffusivity is a function of radius D ( r ) . The boundary conditions are C(T = R'") = c'" and c(r = R'" A R )= coUt.
+
Solution. The gradient operator in cylindrical coordinates is
d V = Cr dr
1 6 d + go + Cz rd0 dz
(5.78)
The divergence of a flux J ' i n cylindrical coordinates is

1d ( r J r ) dr
V. J=r
1 dJ0 ++r d0
dJ, dz
(5.79)
Therefore, the steadystate radiallysymmetric difFusion equation becomes
(5.80) which can be integrated twice t o give
(5.81) The integration constant a1 is determined by the boundary condition a t R'"
+AR: (5.82)
5.3 Find the steadystate concentration profile during the radial diffusion of a
diffusant through a bilayer cylindrical shell of inner radius, R'", where each layer has thickness AR/2 and the constant diffusivities in the inner and outer layers are Din and DOut. The boundary conditions are c(r = R'") = c'" and C(T = R'" A R )= coUt.Will the total diffusion current through the cylinder be the same if the materials that make up the inner and outer shells are exchanged? Assume that the concentration of the diffusant is the same in the inner and outer layers at the bilayer interface.
+
Solution. The concentration profile a t the bilayer interface will not have continuous derivatives. Break the problem into separate difFusion problems in each layer and then impose the continuity of flux a t the interface. Let the concentration a t the bilayer interface be Inner region: R'"
5 r 5 Ri"
+
116
CHAPTER 5. SOLUTIONS TO THE DIFFUSION EQUATION
Using Eq. 5.82,
(5.83) The flux a t the bilayer interface is
(5.84)
Outer region: R'"
+ COUt(T)
5 r 5 Rin + AR C ~ ut ci/o
=
In
(
(Rin +rAR/2
R'"+AR In R1"+AR/2)
+ $0
(5.85)
The flux a t the bilayer interface is
(5.86)
Setting the fluxes a t the interfaces equal and solving for ci/o
=
C y ~ u out t
c
+
ci/O
yields
ainCin
+ Cyin
aout
(5.87)
where R'"
(5.88)
+A R /2
Putting Eq. 5.87 into Eqs. 5.83 and 5.85 yields the concentration profile of the entire cylinder . The total current diffusing through the cylinder (per unit length) is
(5.89) Using Eq. 5.87, ci/o


(Gout
aout
@out
If everything is kept constant except Din and that IK
 Gin)
+
DOut,
use of Eq. 5.90 in Eq. 5.89 shows
n i n nout u u
C Y DOut ~
+
Din
CY~
(5.90)
(5.91)
where a1 and a2 are constants. Clearly, I will be different if the materials making up the inner and outer shells are exchanged and the values o f DOut and Dinare therefore exchanged. This contrasts with the result for the two adjoining flat slabs in Exercise 5.1.
5.4 Suppose that a very thin planar layer of radioactive Au tracer atoms is placed
between two bars of Au to produce a thin source of diffusant as illustrated in Fig. 5.8. A diffusion anneal will cause the tracer atoms to spread by selfdiffusion as illustrated in Fig. 5.3. (A mathematical treatment of this spreading out is presented in Section 4.2.3.) Suppose that the diffusion ex
EXERCISES
117
Thin source
Figure 5.8:
Thin planar traceratom source between two long bars.
periment is now carried out with a constant electric current passing through the bars along x. (a) Using the statement of Exercise 3.10, describe the difference between the way in which the tracer atoms spread out when the current is present and when it is absent.
(b) Assuming that DVCVis known, how could you use this experiment to determine the electromigration parameter p for Au? Solution. (a) The electric current produces a flux of vacancies in one direction and an equal flux of atoms in the reverse direction, so that 4
+
JA =  J v
(5.92)
Using the statement of Exercise 3.10, this will result in an average drift velocity for each atom, given by (5.93) The tracer atoms will spread out as they would in the absence of current: however, they will also be translated bodily by the distance Ax = ( V A ) t relative t o an embedded inert marker as illustrated in Fig. 5.9.
(a)
t=O
I
1 1 4 I
Inert embedded marker
Figure 5.9: (a) The initially thin distribution of tracer atoms that, subsequently, will spread due to diffusion and drift due to electromigration. (b) The electromigration has caused the distribution to spread out and to be translated bodily by Ax = ( V A ) t relative to the fixed marker.
118
CHAPTER 5: SOLUTIONS TO THE DIFFUSION EQUATION
This may be shown by choosing an origin a t the initial position of the source in a coordinate system fixed with respect t o the marker. The diffusion equation is then
(5.94) where ( V A ) C is the flux due t o the drift. Defining a moving (primed) coordinate system with its origin a t x = (‘UA)t, 2’
[a(
(5.95)
= X  (WA)t
[a(
Using )/ax], = )/ad]t,the drift velocity does not appear in the resulting diffusion equation in the primed coordinate system, which is
d *c =
at
*Da2*c
(5.96)
ax‘2
The solution in this coordinate system can be obtained from Table 5.1; *c(x/, t ) =
nd ee’2/(4*Dt) 
d
m
(5.97)
The distribution therefore spreads independently of ( w A ) , but is translated with velocity ( V A ) with respect t o the marker. ( V ) A can be measured experimentally and then p can be obtained through use of Eq. 5.93 if DVCVis known. It will be seen in Chapter 8 that DVCV can be determined by use of Eq. 8.17 if *D is known. *D can be determined from the measured distribution illustrated in Fig. 5.96 using Eq. 5.97 and the method outlined in Section 5.2.1.
(b) The velocity
5.5 Obtain the instantaneous planesource solution in Table 5.1 by representing
the plane source as an array of instantaneous point sources in a plane and integrating the contributions of all the point sources.
Solution. Assume an infinite plane containing m point sources per unit area each of ) a t x = 0. All the point sources strength n d . The plane is located in the ( y ~ plane in the plane lying within a thin annular ring of radius r and thickness dr centered on the zaxis will contribute a concentration a t the point P located along the xaxis at a distance, x , given by dc = m27rr dr
nd
(47rDt)3I2
e(z2+r2)/(4Dt)
(5.98)
where the pointsource solution in Table 5.1 has been used. The total concentration is then obtained by integrating over all the point sources in the plane, so that
where M = mnd is the total strength of the planar source per unit area.
x. Starting at x = 0 plane. Show that the
5.6 Consider an infinite bar extending from cc to +cc along
t
= 0, heat is generated at a constant rate in the
temperature distribution along the bar is
(5.100)
119
EXERCISES
where P = power input at x = 0 (per unit area) and cp = specific heat per unit volume. Next, show that
Finally, verify that this solution satisfies the conservation condition x
T ( z ,t )cp dx = Pt
Solution. The amount o f heat added (per unit area) at z = 0 in time dt is P d t . Using the analogy between problems o f mass diffusion and heat flow (Section 4.1), each added amount of heat, P d t , spreads according t o the onedimensional solution for mass
diffusion from a planar source in Table 5.1:
d T =  1[ CP
]
Pdt 2(7rKt)1/2
(5.102)
ez2/(4nt)
Because the term in brackets represents an incremental energy input per unit volume, the factor (cp)’ must be included t o obtain an expression for the corresponding incremental temperature rise, dT. Let a1
Then
=
P
 a2=lG t = y 2CP J ...
T ( x , y ) = 2a1
X2
J:/”
exp (my2)
Y2
2
(5.103)
dY
(5.104)
Integrating by parts and converting back t o the variables (z, t ) yields
~ ( zt ), = 2a1 e  a z l t d 2 Substituting for a1 and
a2,
+4 a 1 6
eCCZd<
(5.105)
we finally obtain
(5.106) Note t h a t the solution given by Eq. 5.106 holds for z 2 0 because the positive root of The symmetric solution for z 5 0 is easily obtained by changing the sign of z. All the heat stored in the specimen at the time t is represented by the integral
& was used. Q =2
[w
T ( a ,t )c p dx
The first bracketed term in Eq. 5.107 has the value 2 P t . The second term can be integrated by parts and has the value Pt. Therefore,
Q = 2 P t  Pt = Pt and the stored heat is equal t o the heat generated during the time
t , given by Pt.
120
CHAPTER 5 SOLUTIONS TO THE DIFFUSION EQUATION
5.7 Consider the following boundaryvalue problem:
dC
= 4 m , t)= 0
ax
(z 0
0
Use the superposition method to find the timedependent solution. Show that when 2 6 >> a, the solution in (a) reduces to a standard instantaneous planarsource solution in which the initial distribution given by Eq. 5.108 serves as the source. Use the following expansions for small E : erf(z
+ E ) = erf(z) + e'2E
2
J;;
Solution.
+
*
*.
e' = 1 + E + . . . (5.109)
+
(a) The concentration of diffusant located between 6 and 5 d< in the initial distribution acts as a planar source of thickness, d<, and produces a concentration increment a t a distance, 2 , given by
(5.110) The total concentration produced a t distribution. Therefore,
x
is then obtained by integrating over the
Using the relations oeu2
du = J2;;[erf(P)  erf(cu)]
(5.112) (5.113)
The solution is
{ (x)+x a
2a erf c ( 2 ,t ) =%
xa
 erf
(T)
121
EXERCISES
(b) Expanding Eq. 5.114 for small values o f a/A = a
/
m produces the result
c ( x , t )= 
(5.115)
This is just the solution for a planar source of strength n d corresponding t o the content per unit area o f the original distribution given by Eq. 5.108.
5.8 (a) Find the solution c(z, y, z , t ) of the constantD diffusion problem where
the initial concentration is uniform at CO, inside a cube of volume u3 centered at the origin. The concentration is initially zero outside the cube. Therefore, c(z, y, z , t = 0) =
if 1x1 5 4 and Iy1 5 $ and otherwise
121
5
4
and c(z = fm, y = f m l z = A m ,t ) = 0
(b) Show that when 2 m >> a, the solution reduces to a standard instantaneous pointsource solution in which the contents of the cube serve as the point source. Use the erf(z E) expansion in Eq. 5.109.
+
Solution. (a) The method of superposition o f pointsource solutions can be applied t o this problem. Taking the number of particles in a volume dV = dXdqdC equal t o dN = co dXdqdC as a point source and integrating over all point sources in the cube using the pointsource solution in Table 5.1, the concentration a t x , y, z is
c ( x ,Y l 2 ,t )
co dX dqdC e  [ ( ~  ~ ) 2 + ( y  q ) 2 + ( z  C ) z ] / ( 4 D t ) (5.116)
(4~Dt)~l~ The integral can be factored
Ja/2
'
Ja/z
The integrals all have similar forms. Consider the first one. Let u then
=( x  x ) / a ;
122
CHAPTER 5: SOLUTIONS TO THE DIFFUSION EQUATION
Therefore, the solution can be written
x  a/2
(b) Expansion o f Eq. 5.119 using Eq. 5.109 produces the result C=
cga3 (47rDt)3/2
r2/(4Dt)
(5.119)
which is just the solution for a point source containing the contents of the cube corresponding t o cga3 particles.
5.9 Determine the temperature distribution T = T ( z y, , 2 ,t ) produced by an ini
tial point source of heat in an infinite graphite crystal. Plot isothermal curves for a fixed temperature as a function of time in:
(a) The basal plane containing the point source (b) A plane containing the point source with a normal that makes a 60" angle with the caxis (c) A plane containing the caxis and the point source The thermal diffusivity in the basal plane is isotropic and the diffusivity along the caxis is smaller than in the basal plane by a factor of 4. Solution. Using Eq. 4.61 and the analogy between mass diffusion and thermal diffusion, the basic differential equation for the temperature distribution in graphite can be written (5.120) where 21 and 22 are the two principal coordinate axes in the basal plane and principal coordinate along the caxis.
23
is the
In order t o make use of the pointsource solution for an isotropic medium as in Section 4.5, rescale the axes 53
=
(qh) 6 1/6
(5.121)
Then Eq. 5.120 becomes
dT
= (RiRL)
at
(5.122)
The solution of Eq. 5.122 for the point source in these coordinates then has the form (Table 5.1)
Twhere
cy
t3/2
e(€:+Eg+E~)/[4(kini)1/3tl
(5.123)
is a constant. Converting back t o the principal axis coordinates yields (5.124)
EXERCISES
123
(a) Isotherms in the basal plane: In the basal plane passing through the origin, 3% = 0
and
T
Q 2 2 ,%3 = 0 , t ) = ,(*?+*P)/(4kllt)
t3/2
(5.125)
Isotherms for a fixed temperature a t increasing times are shown in Fig. 5.10. They are circles, as expected, because the thermal conductivity is isotropic in the basal plane. Initially, the isotherms spread out and expand because of the heat conduction b u t they will eventually reverse themselves and contract toward the origin, due t o the finite nature of the initial point source of heat.
i h
Figure 5.10: Isotherms for a fixed temperature at increasing times in a basal plane that passes through the origin.
(b) Isotherms in a 60" inclined plane: The isotherms on a plane with a normal inclined 60" with respect t o the caxis can be determined by expressing the solution (Eq. 5.124) in a new coordinate system rotated 60" about the 21 axis. The new (primed) coordinates are
( ) ( =
0
;os60" sin60"
0 sin60' cos60"
)(i )
In the new coordinates, with zb = 0, the temperature profile in the inclined plane passing through the origin is
Figure 5.11 shows the isotherms as a function of time. Again the curves expand and contract with increasing time. However, the isotherms are elliptical because the thermal conductivity coefFicient is different along the caxis and in the basal plane.
124
CHAPTER 5: SOLUTIONS TO THE DIFFUSION EQUATION
Figure 5.11: Isotherms for a fixed temperature at increasing times in a plane with its normal inclined 60' from the caxis and passing through the origin. (c) Isotherms on a plane containing the caxis: Here we simply examine the plane containing 21 and &. The temperature profile on this plane is
T ( & , 6 2= 0 , 2 3 , t ) = t3/2exp cy
[I)&+(
(5.127)
The isotherms are shown in Fig. 5.12. Again they expand and contract with increasing time. The elliptical isotherms are slightly more eccentric than those in Fig. 5.11 because of the greater rotation away from the basal plane.
Figure 5.12: Isotherms for a fixed temperature at increasing times in a plane containing 23 (the caxis) and 21.
5.10 Consider onedimensional diffusion in an infinite medium with a periodic "square wave" initial condition given by c ( 2 , t = 0) =
+
if 0 5 2 n~ 5 otherwise
$
where n takes on all (positive and negative) integer values.
(5.128)
EXERCISES
125
(a) Obtain a solution involving an infinite sine series. (b) Investigate the accuracy of truncating the full series solution. How many sine terms must be retained in order for the concentration at x = X/4 to agree with the full solution to within 1%when Dt/X2 = 0.002? Solution. (a) Use the method o f separation o f variables. Let c ( x , t ) = Y ( x ) T ( t )Substituting . this into the diffusion equation yields
(5.129) where q is a constant. The solutions t o these two ordinary differential equations are
T = a1 exp(qDt)
Y ( x )= bl sin(&x)
+ bzcos(&x)
(5.130)
where a l , b l , and b2 are constants. The constant b2 must be zero because the initial concentration profile is an odd function if the origin is shifted upward by  c 0 / 2 . Further, the periodicity requires that
Y ( & ( x + 4) = Y ( & X )
(5.131)
This condition will be satisfied if & A = 27rm, where m is an integer. Therefore, solving for q and assigning i t an index,
&=
27rm
x
(5.132)
The general solution is then the sum of all the terms with different indices, plus a constant, Ao. Thus,
(5.133) The coefficients can be determined by using the initial condition given by Eq. 5.128. When t = 0, Eq. 5.37 is a standard Fourier series with coefFicients given by A0
=
x
c ( x ,0 ) dx
A,
Inserting Eq. 5.128 and integrating, and A , = 0 for m even. Therefore,
=
f
A0
1 x
c ( x ,0 ) sin
(x> 2m7rx
dx
(5.134)
= c 0 / 2 and A , = 2co/(m7r) for m odd
(b) Symbolic algebra software can efFiciently calculate the partial sums in Eq. 5.135 for the specified values of x and Dt/X2. Setting co = 1, partial sums for 1 t o 10 sine terms give the values: 1.08829, 0.984021, 1.00171, 0.999809, 0.999927, 0.999923, 0.999923, 0.999923, 0.999923, 0.999923, respectively. The series converges fairly rapidly t o a value of approximately 0.9999, From the partial sums calculated, three sine terms are required t o give a concentration value that is within 1%of that given by the complete series. Note that successive terms in the sum are of opposite sign, causing the partial sums t o oscillate about the exact value of the complete sum.
126
CHAPTER 5 : SOLUTIONS TO THE DIFFUSION EQUATION
5.11 Consider a plate of thickness L (0 < x < L ) with the following boundary and initial conditions:
T ( x= 0, t ) = 0
T ( z t, = 0) = Tosin
T ( x= L , t ) = 0
Assume that the thermal diffusivity, IE., is constant. (a) Find an exact expression for the temperature as a function of time.
(b) Find an exact relation for t l p , the time when the temperature at the center of the plate drops to T0/2(half its initial value). (c) If the heat flux at the surface of the plate is set to zero, would the time calculated in part (b) be longer, shorter, or the same? Solution. (a) Use the separationofvariables method as in Exercise 5.10. Assume a solution of . this into the thermal diffusion equation, the form T ( x , t )= Y ( x ) T ( t )Putting two ordinary difFerential equations are obtained whose solutions are
T ( t )= a1 exp(qnt) Y ( x )= bl sin ( f i x )
+ bz cos ( f i x )
(5.136)
where a l , b l , bz, and q are constants. The resulting product solution can be fitted t o the initial and boundary conditions by setting al = 1, bl = To,bz = 0 , and fi = r / L , so that
T = T, sin (n:)
er’fitl~~
(5.137)
Equation 5.137 is a sineseries solution t o the diffusion equation, but because of the sinusoidal initial condition, it consists of only a single term. (b) Setting T = T0/2,x = L / 2 , and t = tllz in Eq. 5.137, the time for the temperature in the center o f the plate t o drop t o half i t s initial value is L2
t l p = 
7r2n
ln(0.5)
(5.138)
(c) Much longer! In fact, if no heat is allowed t o leave the plate, the fixed amount o f heat in the plate will spread until the temperature everywhere is uniform a t the value T, given by
T, =
lL
2 Tosin (rz) dx = To r
(5.139)
The temperature in the center will therefore never drop t o the level T = T,/2!
5.12 It is desired to degas a thick plate of material containing a uniform concentration of dissolved gas by annealing it in a vacuum. The rate at which the gas leaves the plate surface is proportional to its concentration at the surface; that is, Jsurf = a csurf (5.140) where a = constant.
(a) Solve this diffusion problem during the early degassing period before the outward diffusion of gas has any significant effect a t the center of
EXERCISES
127
the plate. The initial and boundary conditions are therefore c(z,O)
= co
c(oo,~)= co J = D
=
a ~ ( 0t,)
(5.141)
Incorporate the parameter h = a / D into the solution. (b) Show that when the dimensionless parameter h a is large, c(0, t ) M 0, and that when h a is small, c ( 0 , t ) M co. You will need the following series expansions of erf(z): For small z , (5.142)
and for large z , 1 +1 x 31X3X5 1  
erfc(z) = 1 erf(z) =
2 3 9
+...) (5.143)
(c) Give a physical interpretation of the results in (b).
Solution. (a) Use the Laplace transform method. Transforming the diffusion equation along with the initial condition given by Eq. 5.141 yields the same result as Eq. 5.64: (5.144) The solution is therefore Eq. 5.65 with
~ ( x , p=) To determine
u2,
a1
= 0:
co + u2 e
P
(5.145)
 m m
transform the boundary condition given by Eq. 5.141 t o obtain
D
(g)
=
x=o
a E(0,p)
(5.146)
Therefore, putting Eq. 5.145 into Eq. 5.146 yields CY Cn
(5.147)
and (5.148) where h = a / D . Find the desired solution by taking the inverse transform using a table o f transforms t o obtain
c(x,t ) = co [erf
(m)+ X
eh=+h2gt
erfc
(&
+h m ) ]
(5.149)
(b) From Eq. 5.149 the concentration at the surface is
c(0,t ) = co eh2’(Dt)erfc ( h m )
(5.150)
128
CHAPTER 5: SOLUTIONS TO THE DIFFUSION EQUATION
For large h m , use the series expansion for a large argument, t o obtain c(0,
co t)= 
h
a
(5.151)
Therefore, c ( 0 , t ) approaches zero for large h m . For small h m , use the smallargument expansion t o obtain
~ ( 0t ), = co (1
+ h2Dt)
(5.152)
Therefore, c(0, t ) approaches co for small h m , (c) W e can rewrite h m as a m . Therefore, as cy becomes small, or at short times t , or as D increases, c(0, t ) approaches CO. For small a,surface desorption is compensated by diffusion from the bulk, so that c(0, t ) decreases slowly. However, a t short times, the concentration gradients near the surface will be large, so c(0, t ) will initially change rapidly. W i t h large D , bulk difFusion t o the surface compensates the surface desorption. The reverse applies for large values o f h f i .
5.13 Solve the following boundary value problem on the semiinfinite domain with discontinuous initial conditions,
c ( x ,t = 0 ) =
{ 0co
O<x
with zero flux conditions a t x = 0 and x = cm.
Suggestion: Use superposition of known solutions, or split the problem into two parts and use continuity to match Laplacetransformed solutions. Solution. Designate the region z < L as region I and the region x > L as region II. The Laplace transform method will be used t o solve the problem in each region and the solutions will then be matched across the interface a t z = L . In region I the diffusion equation and initial condition are the same as in the problem leading t o Eq. 5.64, and therefore the general solution after Laplace transforming corresponds t o Eq. 5.65. Similarly, in region 11, the initial condition is the same as in the problem leading t o Eq. 5.58 and the general solution therefore corresponds t o Eq. 5.59. The four constants of integration can be determined from the boundary conditions imposed a t z = 0, z = L , and z = co.After Laplace transforming, these become (5.153) (5.154) E'(L,p) = EJ'(L,p)
(5.155)
After determining the four constants o f integration and putting them into Eqs. 5.59 and 5.65, the solutions in regions I and II are I
E =
6''
co co   exp(ql)
+
[exp(qz) exp(qz)] 2P co =  exp(qz) [exp(qL)  e x p ( q ~ ) l 2P
P
(5.156)
129
EXERCISES
where q = @, Using standard tables of transforms t o transform back t o coordinates, the final solutions are
Because erf(z) = erf(z),
(s)I)%(
(2,
t)
the solutions are identical in the two regions and thus
c( x,t ) = 2 2 [erf
 erf
(5.158)
CHAPTER 6
DIFFUSION IN M U LTICOMPON ENT SYSTEMS
In earlier chapters we examined systems with one or two types of diffusing chemical species. For binary solutions, a single interdiffusivity, 5, suffices to describe composition evolution. In this chapter we treat diffusion in ternary and larger multicomponent systems that have two or more independent composition variables. Analysis of such diffusion is complex because multiple cross terms and particleparticle chemical interaction terms appear. The cross terms result in N 2 independent interdiffusivities for a solution with N independent components. The increased complexity of multicomponent diffusion produces a wide variety of diffusional phenomena. The general treatment for multicomponent diffusion results in linear systems of diffusion equations. A linear transformation of the concentrations produces a simplified system of uncoupled linear diffusion equations for which general solutions can be obtained by methods presented in Chapter 5 . 6.1
GENERAL FORMULATION
In Chapter 2 we considered diffusion in a closed system containing N components, exclusive of any mediating point defects.l If only chemical potential gradients are present and all other driving forcessuch as thermal gradients or electric fields'Such defects, if present, will be assumed to be in local thermal equilibrium a t very small concentrations. Kinetics of Materials. By Robert W. Balluffi, Samuel M. Allen, and W. Craig Carter. Copyright @ 2005 John Wiley & Sons, Inc.
131
132
CHAPTER 6 DIFFUSION IN MULTICOMPONENT SYSTEMS
are absent, the general formulation presented in Eq. 2.21 and developed further in Chapter 3 applies, and for onedimensional diffusion,’
Equation 2.15 for the rate of entropy production is then
Assuming that the atomic volumes of the components are constants and the fluxes are measured in a Vframe, as defined in Section 3.1.3, Eq. 3.22 holds for all N components, N
C Q i J i =0 i=l
The N t h flux can now be eliminated in Eq. 6.2 by using Eq. 6.3 and putting the result into Eq. 6.2, so that .(
N1
and
The force, Fi, conjugate to the flux, J i , is
and therefore the general linear relation between the independent fluxes and the N  1 independent driving forces is
The chemical potential gradients and Onsager coefficients in Eq. 6.7 can be converted to concentration gradients and interdiffusivities (Table 3.1). Each chemical potential in Eq. 6.7 is a function of the local concentration:
2This treatment is similar to that of Kirkaldy and Young [l].
6.1: GENERAL FORMULATION
133
There are N  1 independent concentrations because Eq. A.10 provides a single relation between concentrations and their atomic volumes. Under the assumption of local equilibrium, the GibbsDuhem relation applies, which places an additional constraint on chemical potential changes in Eq. 6.7 and implies that only N  1 of the p i can vary independently: (6.9)
(6.10) Interdiffusivities,
Eij, are defined by Eq. 6.10, (6.11)
(6.12) Dij
is the product of two matrices, (6.13)
where the L i k are Onsager coefficients and T k j are thermodynamic factors that couple chemical potentials to concentrations, (6.14) The analysis of the diffusion for N components requires N  1 independent concentrations and ( N  1)2 interdiffusivities. For the ternary case, (6.15) L
J
The eigenvalues, A h , of the interdiffusivity matrix (see Eq. 4.62) must be real and positive [l].For the ternary case,
where
134
CHAPTER 6 DIFFUSION IN MULTICOMPONENT SYSTEMS
The real and positive condition on the eigenvalues places physical limits on the interdiffusivities. For the ternary case,
(6.18) (511522 I
+
512521)
L
0
I
The sum (Dll D 2 2 ) must be positive, but a direct interdiffusivity, oii, could be negative and still satisfy the conditions in Eq. 6.18. The offdiagonal terms, Eij, need not be symmetric with respect to the exchange of i and j. In the steps leading to Eq. 6.5, the choice of the N t h component is arbitrary, and a different set of values for the four interdiffusivities will be obtained for each choice. However, each set leads to the same physical behavior predicted for the system: the diffusion profiles of the three components predicted by the equations are independent of the choice for N.3 For some choices, the interpretation of interdiffusivities in terms of kinetic and thermodynamic data may be more straightforward [l]. 6.2
SOLUTIONS O F M U L T I C O M P O N E N T DIFFUSION EQUATIONS
Generally, a set of coupled diffusion equations arises for multiplecomponent diffusion when N 2 3. The least complicated case is for ternary ( N = 3) systems that have two independent concentrations (or fluxes) and a 2 x 2 matrix of interdiffusivities. A matrix and vector notation simplifies the general case. Below, the equations are developed for the ternary case along with a parallel development using compact notation for the more extended general case. Many characteristic features of general multicomponent diffusion can be illustrated through specific solutions of the ternary case. The coupled ternary diffusion equations in one dimension are obtained from the accumulation fluxes in Eq. 6.11:
_ dCl V.J1= + ax a (Ell%) + at
_ ac2   V . J2 +=a at
or
dX
& (E12$)
(&%) + (5222)
(6.19)
(6.20) and generally,
ac' = a [5E] at ax ax
(6.21)
In general, the 5ij are functions of the concentrations, so these equations are nonlinear. Numerical methods must then be employed. However, solutions can be obtained for a variety of special cases, several of which are described below. 3This independence is similar to a constrained system's insensitivity to the choice of Nc in Section 2.2.2.
6.2: SOLVING THE DIFFUSION EQUATIONS
6.2.1
135
Constant Diffusivities
If the interdiffusivities are each constant and uniform, the coupled ternary diffusion equations, Eq. 6.20, are a linear system, (6.22) and in general,
dc' = 5,Vzc'
at
(6.23)

It is possible to uncouple the expressions for the fluxes by diagonalizing the diffusivity matrix through a coordinate transformation. The transformed interdiffusivity matrix will have eigenvalues X i as its diagonal entries. For the ternary system, the eigenvalues are the A& from Eq. 6.16. There will be N positive eigenvalues AN in the general case, where N is the number of indeKendent components. According to E% 1.36, the eigenvectors 2i of D form the columns of the matrix that diagonalizes 12 by the coordinate transformation. For the ternary system, let the eigenvector for the (fast) A+ eigenvalue be f a n d for the (slow) A be s':
The slow and fast eigendirections are related by an angle 8 ,
s'.f = case = =
Iqlfl


D2l  5 1 2
J ( D l l  zj22)2+ (zj12+ fj21)2
The transformation matrix, A, that diagonalizes eigenvectors f a n d 3. For the ternary case,
(6.25)
5 has columns formed by the
and for the general case,
and therefore (6.28) Transforming Eq. 6.43 yields (6.29) or
[;I=[
;+]v[
:,I
(6.30)
136
CHAPTER 6: DIFFUSION IN MULTICOMPONENT SYSTEMS
or
J , =  XVC, J p =  X+Vcp
(6.31)
and the fluxes are seen to be uncoupled in the diagonalized system. J , and J p are the two fluxes in the diagonalized system given by
[$I=”“
;I
(6.32)
and c, and cp are the two concentrations given by
[ ;;]
;; ]
=Al[
(6.33)
These quantities therefore have the forms
 D22 + A
J , = J i + A 2A D2 1 D l l  D22  A Jp = J1 A 2A 021
Dii
J2
(6.34)
52
and 021 c, = 
A
cp
D2 1 A
=c1
c1
+

Dll
D22
+A
c2
2A
Dll  D22  A 2A
(6.35) c2
The flux problem can now be easily solved in the diagonalized system using Eq. 6.31; the solution can then be transformed back to the original concentration coordinates by using the inverse relationships
[;:]=A[
[:;I=”[
and
:]
(6.36)
:;]
(6.37)
SteadyState Solutions. For the steadystate case, Eq. 6.22 becomes
(6.38) and in general,
If
has an inverse,
0’= kv2z I
D O=Q or
I
QV2Z
[ ; ] = v 2:;] [
(6.39) (6.40) (6.41)
6.2: SOLVING
THE DIFFUSION EQUATIONS
137
that is,
v2ci = 0
(6.42)
Therefore, Laplace's equation holds for each component separately. However, the steadystate fluxes are interdependent, as may be seen from Eq. 6.11 for the ternary case, (6.43) TimeDependent Solutions. In the timedependent case, the diffusion equations given by Eq. 6.23 are coupled. However, they can be uncoupled by again using the diagonalizat ion met hod. Using the transformation matrix A on Eq. 6.23 gives for the ternary case,
a
[at and for the general case,
I.'
= [ ;:+Iv2[
cg
A1
a
0

at
: 0
0.'' x
0 2
0
...
:;]
(6.44)
0 0
.*.
0
:
(6.45)
0 AN1
where the concentrations Ei are linear combinations given by the eigensystem transformation of the actual components ci. Each partialdifferential equation in the diagonal frame is independent:
at
Tr(@  A (6.46)
In general,
(6.47)
138
CHAPTER 6: DIFFUSION IN MULTICOMPONENT SYSTEMS
For onedimensional ternary diffusion, the boundary and initial conditionsc1(z = L , t ) ,c1(x = R , t ) ,cl(x,t = 0), c2(x = L , t ) ,C Z ( X = R , t ) ,and cz(x,t = 0)become
I
021
ca(s,t= 0) = C l ( X , t = 0) A
+

Dii  5 2 2 2A
+A
c 2 ( 2 ,t
= 0)
(6.48)
In general,
Z(x = L , t ) = Alc'(x = L , t )
Z(x = R,t ) = Alc'(x +
qx,t
= 0) = Alc'(z,
= R, t )
(6.49)
t = 0)
The system is reduced to a set of uncoupled diffusion equations with diffusivities constructed from the component interdiffusivities by a prescribed algorithm. Each equation can be solved by methods described in Chapter 5. The transient behavior at the interface of two ternary alloy compositions in a system with complete solid solubility will lead to a path in composition "space" as shown in Fig. 6.1. Evolution is initially parallel to the fast eigendirection S a n d , after its gradients become small, finally proceeds parallel to the slow direction S: c.
c
+ S
Figure 6.1: General evolution of a ternary diffusion couple with initial conditions specified by a concentration pair on the left (z = L ) and on the right (z = R ) .
6.2. SOLVING THE DIFFUSION EQUATIONS
139
The solution for a diffusion couple in which two semiinfinite ternary alloys are bonded initially at a planar interface is worked out in Exercise 6.1 by the same basic method. Because each component has stepfunction initial conditions, the solution is a sum of errorfunction solutions (see Section 4.2.2). Such diffusion couples are used widely in experimental studies of ternary diffusion. In Fig. 6.2 the diffusion profiles of Ni and Co are shown for a ternary diffusion couple fabricated by bonding together two FeNiCo alloys of differing compositions. The Ni, which was initially uniform throughout the couple, develops transient concentration gradients. This example of uphill diffusion results from interactions with the other components in the alloy. Coupling of the concentration profiles during diffusion in this ternary case illustrates the complexities that are present in multicomponent diffusion but absent from the binary case. 80
70 60 50
40
30 20 10 0
Distance (arbitrary scale)
Fi ure 6.2: Concentration profiles for Ni and Co in ternary diffusion couple fabricated w i f i FeNiCo alloys. From Kirkaldy and Young [l], and Vignes and Sabatier [2].
The results of ternary diffusion experiments are often presented in the form of daflusion paths, which are plots of the concentrations measured across the diffusion zone. The diffusion path corresponding to the measurements in Fig. 6.2 is shown in Fig. 6.3; note the characteristic Sshape, due to the inflections in the C N ~profile.
6.2.2
ConcentrationDependent Diffusivities
If the diffusivities are functions of concentration, the BoltzmannMatano method, described in Section 4.3 for the binary case, can be employed if the initial and boundary conditions are appropriate. The diffusion equations are (6.50) and when the scaling parameter 77 = x / d is employed, these equations become (6.51)
140
CHAPTER 6: DIFFUSION IN MULTICOMPONENT SYSTEMS
Ni
Fe " 0
20
40
xco Figure 6.3: Sabatier [ 2 ] .
60
80
100 c o
Diffusion path for ternary diffusion profiles shown in Fig. 6.2.
From Vignes and
Consider a ternary diffusion couple in which each component has an initial stepfunction profile and boundary conditions similar to those given by Eq. 4.44. Integrating and changing variables, as in the development leading up to Eqs. 4.48 and 4.49 for the binary case, (6.52)
and (6.53)
Because the diffusion profiles q ( x ) and c2(x) are known, the fluxes 51 and 5 2 can ) ~ ( xand ) evaluating the integrals be determined at any x by inverting c ~ ( xand in Eqs. 6.53 for i = 1 , 2 . Because dclldx and dcsldx are known at the selected x , two equations relating the four diffusivities are obtained. Therefore, if two ternary diffusion experiments are analyzed at a point of common concentration, four equations relating the four diffusivities at those common concentrations will be obtained and all four diffusivities can be determined. However, use of this method to derive diffusivities from experimental results is highly labor intensive and subject to significant error [3]. Alternatively, coupled diffusion equations with concentrationdependent diffusivities and comparison with experimental results can be solved with numerical methods (see Kirkaldy and Young [l]and Glicksman [4]). In many systems, complex particleparticle interactions can produce a plane inside the diffusion zone where the flux of one of the components is zero. Such planes can be found by evaluating the integral in Eq. 6.53 along the diffusion profile to find
141
6.3: MEASUREMENT OF DlFFUSlVlTlES
points where Ji = 0. This approach can be used to obtain information regarding diffusion in the system [5]. Exercise 6.3 provides an illustration.
6.3 MEASUREMENTS AND INTERPRETATIONS OF DlFFUSlVlTlES There are extensive reviews of the many measurements of the E i j , particularly in ternary systems [l].Numerous systems exhibit uphill diffusion, due to strong particleparticle interactions, and efforts have been made to interpret the diffusivity behavior in terms of thermodynamic activity data and particleparticle interaction models. In many cases the diffusion behavior has been explained, and more details and discussion are found in Kirkaldy and Young’s text [l]. Bibliography 1. J.S. Kirkaldy and D.J. Young. Diffusion in the Condensed State. Institute of Metals,
London, 1987.
2. A. Vignes and J.P. Sabatier. Ternary diffusion in FeCoNi 245:17951802, 1969.
alloys. Trans. TMSAIME,
3. C. Cserhati, U. Ugaste, M.J.H. van Dal, N.J.H.G.M. Lousberg, A.A. Kodentsov, and F.J.J. van Loo. On the relationship between interdiffusion and tracer diffusion coefficients in ternary solid solutions. Defect and Diffusion Forum, 194199:189194, 2001.
4. M.E. Glicksman. Diffusion an Solids. John Wiley & Sons, New York, 2000. 5. M.A. Dayananda. Zeroflux planes, flux reversals and diffusion paths in ternary and quaternary diffusion. In Diffusion in Solids: Recent Developments, pages 195230, Warrendale, PA, 1985. The Metallurgical Society.
EXERCISES
6.1 Find the diffusion profile solutions for ternary diffusion in a diffusion couple fabricated by bonding two semiinfinite alloy blocks face to face along a planar interface. Assume constant diffusivities. Solution. The method o f diagonalization described in Section 6.2.1 is employed. The initial conditions for all components are stepfunction concentration profiles and hence errorfunction profiles having the form
(6.54)
are tried as solutions t o the uncoupled diffusion equations given by Eq. 6.44. Using Eqs. 6.26 and 6.37, the relationships between the concentrations c1 and c2 and the concentrations ca and cp in the diagonalized system are
DII  0 2 2  A ‘Or 2021 cz = co. cg
+
c1 =
+
+
DII  DZZ A cp 2021
(6.55)
142
CHAPTER 6: DIFFUSION IN MULTICOMPONENT SYSTEMS
By combining the equations above, the solutions take the forms
(6.56)
The boundary conditions on c1 and
c2
are
R C l ( C o , t ) = Cl(X,O) = c1 c1(Co,t) = C1(Z,O) = cf
C2(Co,t)
c2(Co,t)
= C 2 ( Z , O ) = c2R = c2(x,O) = c2L
(6.57)
and therefore
R
c2
L
c2
= a1
+ + + a4
=a1
 a2
a2
a3
+ a3  a4
Solving the four equations above for the four coefficients,
(6.59)
a4
=
(022
 Dl1
+ A)(c,R  c;) + 2D21(~? c?) 4A
Substituting Eq. 6.59 into Eq. 6.56, the final solution for c2
cz"
c2
is
+ ck
= ___
2
+ +
(011
(D22
022  Dli
+ A)(c,R  c;)
 2 0 2 1 ( ~ p ~
+ A)($
+ 2 0 2 1 ( ~ ? c?) erf
4A
 ck)
4A
f )
A similar expression holds for c1.
6.2 Point sources of components 1 and 2, containing N1 and Nz atoms, respec
tively, are located at the origin r = 0 in a large piece of pure component 3. Solve for the resulting threedimensional diffusion field, assuming that the diffusivities D l l , 0 2 1 , and 0 2 2 , are independent of concentration.
EXERCISES
143
Solution. Assume solutions in the diagonalized system having the standard point
source form
=
C,
(w) r2
cp = (4.iixa+Rt)3/2 exp
(6.61)
Using Eqs. 6.26 and 6.37,
c1 = Dii  0 2 2  A 2021 c2 = c, cg
+
I
t
Dll  D~~+ A CP 2021
(6.62)
Conservation o f components 1 and 2 requires that W
47~
4n
r
c l r 2 d r =N1 = constant (6.63)
W
c272dr = N ~= constant
Jo
By substituting Eq. 6.61 into Eq. 6.62 and requiring that Eq. 6.63 be satisfied,
Dl1  0 2 2  A 2021
+
+
Dl1  0 2 2 A a g = N1 2021 a, a p = N2
+
(6.64)
By solving Eq. 6.64 for a, and a g and putting the results into Eq. 6.62 with the help of Eq. 6.61, the final solution for c2 is
+ + exp (+ (Dl1  + A)N2  2021N1
c2 = 2D21N1
( A 0 2 2  D11)Nz 16A(7 ~ X + t ) 3 / 2 022
16A(rX t)3/2
exp
&) (A)
(6.65)
A similar expression may be found for c1.
6.3 Show that the simple relation (6.66)
holds for a plane of zero flux of component 1 in the diffusion zone of a ternary system when component 3 is chosen as the N t h component, the approximation 01 = 0 2 = 0 23 is used, and the activity coefficients are constants. Solution. From Eq. 6.7, J1
= L11
d dX
d (111  p3)  L12 (p2  p3) = 0 OX
(6.67)
Therefore,
(6.68) Then, substitution o f Eq. 2.2 into Eq. 6.68 produces the desired result
6.4 Construct a diffusion path for the Cu/Zn binary diffusion zone in Fig. 4.8.
144
CHAPTER 6: DIFFUSION IN MULTICOMPONENT SYSTEMS
Solution. For the binary CuZn system,
+
(6.69)
xcu Xzn = 1 Therefore, the path appears as in Fig. 6.4.
0 Figure 6.4:
0.7
xcu
1
Diffusion path for the Cu/Zn binary diffusion zone in Fig. 4.8.
CHAPTER 7
ATOMIC MODELS FOR DIFFUSION
Macroscopic treatments of diffusion result in continuum equations for the fluxes of particles and the evolution of their concentration fields. The continuum models involve the diffusivity, D, which is a kinetic factor related to the diffusive motion of the particles. In this chapter, the microscopic physics of this motion is treated and atomistic models are developed. The displacement of a particular particle can be modeled as the result of a series of thermally activated discrete movements (or jumps) between neighboring positions of local minimum energy. The rate at which each jump occurs depends on the vibration rate of the particle in its minimumenergy position and the excitation energy required for the jump. The average of such displacements over many particles over a period of time is related to the macroscopic diffusivity. Analyses of random walks produce relationships between individual atomic displacements and macroscopic diffusivity. 7.1
THERMALLY ACTIVATED ATOMIC JUMPING
The fundamental process in atomistic diffusion models is the thermally activated jump between neighboring sites of local minimum energy. The duration of any jump is typically very short compared to the particle’s residence time in a minimumenergy site. Therefore, the average jump ratethe basis for any model of atomistic diffusive motionis essentially inversely proportional to the average residence time. The residence time depends upon the probability that the local potential energy will undergo a fluctuation large enough to enable the particle to surmount the Kinetics of Materials. By Robert W. Balluffi, Samuel M. Allen, and W. Craig Carter. Copyright @ 2005 John Wiley & Sons, Inc.
145
146
CHAPTER 7 ATOMIC MODELS FOR DIFFUSION
potentialenergy barrier that it will encounter while making a jump. This barrier can readily be visualized by considering, as an example. t,he diffusion of interstitial a t o m among the interstices of large substitutional host atoms as described in Section 3.1.4. In this case, a jumping interstitial atom must squeeze its way past the large intervening substitutional atjonis to make a successful jump between interstices. This squeezing increases the potential energy in the local region, and a potentialenergy barrier to the jump t,herefore exists. Similar barriers exist for t,he jumps of particles in other systems. The height of the barrier will depend upon the interaction between the jumping particle and its surroundings arid can vary depending upon the path of the jumping particle and the posit,ioiis of its neighbors. For example, neighboring atoms may cooperatively enlarge the gap through which the jumping particle passes. The complexit,y of any analysis is increased by this multiplicity of possible activated configurations. However, useful approximations of varying accuracy can be obtained. There are numerous approaches to modeling the jump rate.' Below, three progressively more realistic models are presented. All three approaches produce the same basic resultthe jump rate is a product of the vibration frequency in the initial stable site and a Boltzmann probability of a sufficient energy fluctuat,ion for the jump.
7.1.1 OneParticle Model with Square PotentialEnergy Wells The simplest model is composed of identical noniriteracting particles sitting in rectangular potentialenergy wells separated by flat potentialenergy barriers. The barriers have widths L A , as illustrated in Fig. 7.1. The rate at which the particle1 traverses a barrier is calculated as a oneparticle event that occurs in one dimension. The manybodied aspects are ignored and it is assumed that the migrating particle's surroundingsand therefore the potentialenergy landscapeis static. Furthermore. the system is assumed to be in thermal equilibrium, so that the local temperature provides a statistical probability of a particle's kinetic energy fluctuations. Under this condition, a given particle spends most of its time in the energy
t
I
I
Distance. x

Figure 7.1: Square poterit,ialeIiergy wells arid an eriergy barrier for a particle jurnpirig in one dinierisiori. The iiuniber of particles is proportioiial t,o t lie occupat,ioii probnhilit~yof well st,ates along L~~~~rid activateci states along L ~ . 'See Glasstone et al.. Wert and Zener. Vineyard, Rice, Flynn, Girifalco. Christian, and Franklin for examples [l81.
7.1: THERMALLY ACTIVATED ATOMIC JUMPING
147
wells that correspond to lowenergy (highprobability) well states. However, fluctuations produce brief intervals during which a particle is situated atop the energy barrier along L A in highenergy (lowprobability) activated states. The jump rate is the inverse of the average migration time, the average amount of time between an atom’s arrival at one site and its arrival at a neighboring site. The average migration time is the sum of two distinct terms: the time an atom waits to reach an activated state and the migration time in the activated state. It is assumed that the system behaves classically and that any contribution from quantummechanical tunneling between the energy wells is negligible. Quantum tunneling can become important for light particles at low temperatures and is discussed elsewhere [5, 81. The average time for a particle in an activated state to cross the activation barrier is
where (v) is the particle’s average velocity along L A and m is its mass. The expression for ( u ) is found by determining its average momentum (p) and then using (w)= (p)/m. In this classical system, the probability that the particle has momentum in the forward direction (i.e., with positive values of p) between p and p dp is proportional to exp[p2/(2mkT)]dp [l].Therefore,
+
In a system of N particles, the total rate at which particles cross the barrier, , is  number of particles in an activated state (7.3) Tcross
&cross
Consider a total time T activated state. Then.
>> r A ,where
r A is the time that a particle spends in an
N T is the average duration in a well state. Therefore, for one particle, where rwel1 the crossing frequency (i.e., the jump frequency, I?’), is
(7.5) or (7.6) The ratio of times spent in a well state and in an activated state is TA Twell
24
  
where Z A and
Zwel1
Zwell
CAeEA/(bT)
Cwell eEwe” /(kT)
(7.7)
are the partition functions for the activated and well states.2
2 T h e partition function plays a central role in statistical mechanics [9]. If the probability of finding a system in a state i with energy Ei is proportional to exp[Ei/(kT)], the partition
148
is
CHAPTER 7: ATOMIC MODELS FOR DIFFUSION
If d(z) is the potential energy function illustrated in Fig. 7.1, the classical limit
Therefore,
where Em = EA Ewe''(i.e., the height of the barrier) is termed the activation energy for migration of the particle. The bracketed term that multiplies the BoltzmannArrhenius term exp[Em/(kT)] has dimensions (time)' and represents the number of attempts a t the barrier per unit timethe average attempt frequency. The BoltzmannArrhenius exponential term is the activation success probability for each attempt. As demonstrated in less simple models below, this simple resultthat there is a characteristic attempt frequency multiplied by a BoltzmannArrhenius factor containing the activation energyis quite robust. 7.1.2
OneParticle Model with Parabolic PotentialEnergy Wells
An improved approximation to the potentialenergy landscape can be obtained by introducing parabolic wells and a smooth barrier as in Fig. 7.2.3 This model is more realistic, as particles that are displaced small distances from their average positions of minimum energy in a solid will generally experience restoring forces that increase linearly with the displacements. This leads to a potential energy that increases as the square of the particle displacement, which corresponds to a static (i.e., nonmanybodied) harmonic model for a solid [9]. The energies of the states of the particles are approximately
In Fig. 7 . 2 , the well states are located in the region denoted by Lwei' near the minima. The particles spend the remainder of their time at the approximately flat region denoted by L A ,where the changes in average particle velocity are small. Particles at other positions experience significant forces from V+(z) and therefore tend to accelerate, resulting in low occupation probabilities for those positions. The analysis method is the same as that for the rectangularwell model, and Eqs. 7.6 and 7.7 again hold. Using the harmonic potential, the ratio of partition functions function is related to the normalization factor for the probabilities 2 = Estates exp[E,/(kT)]  Eenergles 3 W E , )exp[J%/(kT)l = Cenergies 3 exp(%/k) exp[J%/(kT)I, where WE,) is the number of states of identical energy E3 . Because ZA is proportional to a sum of probabilities, it is proportional to the total probability of finding a particle in the activated state and therefore the average time in that state. 3By illustrating the potentialenergy landscape in one dimension in Fig. 7.2, it appears that the activated state is one of maximum energy. The single dimension represents the most likely trajectory between the minimum states which requires the least energy, so the activation energy is that of the trajectory's saddle pointthe minimum of all the maximum energies of the trajectories between two minima (see Fig. 7 . 3 ) .
7 1. THERMALLY ACTIVATED ATOMIC JUMPING
t
F
149
EA
C
a, m
.
E Emin a, 0
I
a
f)
I
Lwell
Lwell U
Distance. x
Figure 7.2: Parabolic potentialenergy well for onedimensional particle jumps. Unlike the square potential energy function in Fig. 7.1. the energy barrier is no longer perfectly flat.
(Eqs. 7.6 and 7.7) becomes
and because states far from the well minimum do not contribute significantly, the limits of integration can be approximated with
and integrated to give (7.13) where (7.14) is the characteristic attempt frequency. Again, the activation energy is the height of the energy barrier and the jump rate is given by an attempt frequency niultiplied by a BoltzmannArrhenius factor of the form exp[Em/(kT)]. The frequency. u. is that of a simple harmonic oscillator of mass, m, with a restoringforce constant given by /3 (demonstrated in Exercise 7.1).
7.1.3 ManyBody Model The two simple singlebody models can be improved by including manybody aspects and by allowing the jumping particle to differ from the remaining particles. A treatment similar to Vineyard's is developed [3]. The Nbody system consists of N  1 identical particles of mass m and a single migrating particle of mass m J . The state of such a system of N interacting particles can be defined by 3 N spatial coordinates, q L , and 3N momenta, p , , and can then be represented by a point in a 6Ndimensional phase space with coordinates (41,q2, . . . . q 3 N . P I . p 2 . . . . .p 3 ~ [9]. ) Furthermore, the total energy of such a system can be expressed as the sum of its
150
CHAPTER 7 ATOMIC MODELS FOR DIFFUSION
kinetic energy (a function of the 3 N momenta) and its potential energy (a function of the 3 N spatial coordinates). Assuming that there are numerous sites in the system that the jumping particle can occupy while maintaining a stable system structure, the rate at which this particle jumps from one stable site to another can be determined. Figure 7.3a depicts how the total potential energy of the system, o = + ( q ~q.2 as t'he jumping particle occupies positions throughout the syste sites of local minimum energy. Because it is impossible to make such a plot in three dimensions, the many displacements of particles in the system that acconipany the displacement of the jumping particle are suggested by the added multiple axes. Point P represents the situation of the jumping particle in a stable site while point Q represents the corresponding situation when the jumping particle is in a neighboring stable site. In both cases, the system is stable because it is at a local potentialenergy minimum, as indicated by the two minima in the hypersurface shown in the 3Ndimensional space of Fig. 7.3. In Fig. 7.3b, hypersurfaces of constant potential energy are a function of the 3 N coordinates indicated in Fig. 7.3a. [These hypersurfaces are of dimensionality 3 N  1 because they are defined by the level sets of 4 = + ( q l , q 2 , , q 3 ~ ) so , that 3 N  1 coordinates are independent.] There are many choices for a particle trajectory between P and Q, but the trajectories that cross the saddle point (located at the point P A ) require the smallest energy fluctuation and are the most probable. Therefore, the saddle point energies in the potentialenergy landscape determine the transition probabilities. The saddles are present because each minimum is surrounded by neighboring maxima. Neighboring niininia pairs have at least one connecting path that has an associated saddle energy; the path between P and Q in Fig. 7.3 passes through the saddle point P A . The force on a particle exactly at P A is zero, but the configuration is an unstable equilibrium. A unique hypersurface, S A , passes through P A and is
Figure 7.3: In a syst,eni with 3N spatial coordinates. t,he potentialenergy landscape consists of minima for each of the stable at,omic sites. such as P and Q. The pot,entialenergy landscape surface (a is the surface and b shows its isopot,entials) represents such a landscape. but only for t,wo spatial coordinates. The surface is impossible to illustrate as a funct,ion of all coordinates 41.q 2 : . . . , q 3 ~ The . migrating atom traverses t,he region between P and Q via the saddle point P A . During migration the landscape chaiiges in response to the geometrical coiifiguratiori of the activat,ed state.
7.1: THERMALLY ACTIVATED ATOMIC JUMPING
151
perpendicular to the contours of constant 4. S A constitutes an energy ridge and is analogous to a “continental divide” separating the region associated with P from the region associated with Q. In an equilibrium system, a migrating particle spends most of its time vibrating with small amplitude about lowenergy states such as P and Q. The crossing time is very short compared to the equilibrium duration, but as the migrating atom crosses, it slows near the saddle point. For the crossing interval depicted in Fig. 7 . 3 , most of the active migration time is spent near saddle points such as P A in a volume of the hyperspace centered on the saddle point of width L A . Considering the states in the activated volume and the states near the minima, Eqs. 7.6 and 7.7 can be applied to model the jump rate, I?, but the analysis must be modified if the system is a t constant pressure instead of constant volume. The jump rate for a system at constant temperature and pressure is
(7.15)
where Z p is the fixedpressure partition function, Z is the fixedvolume partition are the system volumes in the activated and well states. function, and V Aand Vwel1 Using Ui = p:/2mi &(x) in the classical limit [the number of energetically degenerate states = ( d p d q ) / h ] and integrating the momentum terms for Z yields
+
To find an expression for the potential energy of the vibrating system in the well state at P, the harmonic approximation is used and $(3is expanded about P, so the potentialenergy surface near P has the form
where i and j sum over the 3N displacements of the J atom and the N  1 other atoms, q; is the average coordinate of the ith vibrating atom, and $O is the potential energy per atom when all atoms are located in their average positions. The elements of the matrix of second derivatives are the linearized spring constants for each atom site pair and correspond to the quantity p in Eq. 7.10, which was employed in the static harmonic model. Typically, only the near neighbors have nonnegligible entries, the number of which depends on the interatomic potential
152
CHAPTER 7: ATOMIC MODELS FOR DIFFUSION
length scale. The matrix of second derivatives is real and symmetric and therefore has real eigenvalues, all of which are positive in the stable state. If the 6qi are transformed to its diagonalized coordinate eigensystem 6qi,
(7.18) where mi and wi are the effective masses and characteristic angular frequencies of the three vibrational modes of each harmonic mode and i now runs over the 3N modes of the J atom and the N  1 other atoms. The modes are decoupled in the eigensystem and this transformation exists for any interatomic potential. If the interactions are shortrange, the matrix will be sparse and the effective masses and characteristic frequencies will be nearly the same in the eigensystem (qi) and the lattice system ( q i ) . In Eq. 7.16,$ can be approximated using Eq. 7.18; the integral's value is dominated by 6qi x 0, and therefore its limits can be taken to be k m , even though the parabolic approximation is valid only near equilibrium,
=e
N$'/(kT)
/F/F. . /? mul
,
m2w2
~ ~ N W S N
( 2TkT)B(z) 3(N1)
 eN$o/(kT)
~ J W J
mw2
(7.19)
where w is the same for all masses except the migrating atom. If the masses and characteristic frequencies differ, a product would appear above for each unique effective mass and characteristic frequency. When the jumping atom is located along L A ,where the potentialenergy hypersurface has principal curvatures of opposite sign, there is one negative eigenvalue corresponding to the unstable direction along the path between P and Q and
where i iterates over all N atoms and j iterates over all but the J atom. It is reasonable to assume that only a relatively small number of atoms surrounding the jumping atom are affected when the system goes from the well state to the activated state. Let this number be N A . Also, approximate the potential
7.1: THERMALLY ACTIVATED ATOMIC JUMPING
153
energy of the jumping atom along L A at the saddle point by a parabola in a single variable, 77.~1. Let the approximating parabola have its maximum 4f at 6 7 5 1 = 0 and decrease by a factor 1  E at 6 7 ~ = 1 fLA/2:
(7.21)

3NA
3(NNA1)
where i iterates over all N A affected atoms, j iterates over the 3 N A modes of the affected atoms, and k iterates over all modes of the ( N  N A 1) nonaffected atoms. Equation 7.21 can be integrated with the same approximation employed to obtain Eq. 7.19. To lowest order in L A and E ,
(7.22)
where i iterates over all N A affected atoms and 1 iterates over the modes of the affected atoms and it is assumed that w f 2 = w f 3 . Therefore,
 Z=AL
Zwell
2rkT
A e [$$+C,": +f+(NNAl)+o]/(kT)eN+O/(kT) mJ(w?)2
(7.23)
and
r' = %e[+$+Ez{ 27r +f(NA+l)+a+P(VAVwe'' The final expression for the jump rate is then
r' = y e  G " / ( k T )
(2)'(n2) 3NA
e= 1
= y e S m / k e  H m / ( k T ) = uePVm/(kT)eS"/k,U'/(kT)
(7.24) (7.25)
where
3NA
I)$(
(7.26)
N
2 k ( wWf J ' " J )
+ 3kNA(Aw) W
154
CHAPTER 7: ATOMIC MODELS FOR DIFFUSION
and ( A w ) is the average difference between the activated and stable frequencies, wf
 w.
The interpretation of the jump rate for this multibody harmonic model is the same as for the simpler models. Equation 7.25 is the product of an attempt frequency and a BoltzmannArrhenius exponential factor containing a migration activation energy. This result will be used throughout the remainder of this book. If none of the migrating atom’s neighbors are affected in Eq. 7.25, the activation energy is simply the difference between the migrating atom’s energy in the activated and well states, and the entropy is proportional to the difference between the migrating atom’s frequencies in the activated and well states.
7.2
DIFFUSION AS A SERIES
OF DISCRETE JUMPS
In general, a particle migrates in a material by a series of thermally activated jumps between positions of local energy minima. Macroscopic diffusion is the result of all the migrations executed by a large ensemble of particles. The spread of the ensemble due to these migrations connects the macroscopic diffusivity to the microscopic particle jumping. If a particle jumps with average frequency r in a sequence of displacements r‘, (6gives the magnitude and direction of the ith jump), then after a period of time, 7 , the particle will execute N , = individual jumps.4 The position relative to its starting point is the sum of the individual displacements,
i=l
i=l
The random walk process can be characterized by the distribution of total displacements for either a large set of noninteracting walkers or for repeated trials of an isolated walker. The average displacement is a vector (Z(N,))and the meansquare displacement (Z(N,) . Z ( N , ) ) = ( R 2 ( N T is ) ) a scalar that characterizes the spread or difluseness of the distribution of total displacements about its average. The square displacement for a given sequence of random steps is
4r represents the average total jump rate during the sequence, which generally consists of jumps of different lengths and directions. This contrasts with r’,which represents the jump rate between
two specified sites.
7.2: DIFFUSION AS A SERIES OF DISCRETE JUMPS
This sum consists of N , x N , products that can be collected into diagonal and offdiagonal (6 Fj = Fj ..i) parts,
N,
N,1
N,j
i=l
j=1
i=l
155 *
Fi
(7.29)
The 6 . 6+jcan be expressed as products of the jump distances and the cosine of the angle between the jumpvector directions, O i , i + j (i.e.,i'? . Fi+j = l F i l \ f i + j \ cos &,i+j). The meansquare jump distance is (7.30) Averaging over a large number of independent walkers or trials for a single walker,
w2(w) =~ , ( r+ ~ 2)
(c C N,l
j=1
N,j
)
I F ~ I I F cosei,i+j ~+~I
i=l
(7.31)
Equation 7.31 is general. No assumptions have been made about the randomness of the displacements, the lengths of the various displacements, the allowed values of O i , i + j , or the number of dimensions in which the random walk is occurring. 7.2.1
Relation of Diffusivity t o the MeanSquare Particle Displacement
A relationship between the macroscopic diffusivity, D , of a component i and the , be obtained from the behavior of ci(z, t ) meansquare displacement, (R2( N T ) )can as it evolves from an initial point source at the origin. Using the solution for diffusion from an instantaneous point source in three dimensions in Table 5.1, the distribution of particles after a time T will be given by (7.32) The second moment of the distribution in Eq. 7.32,
Jrr2c(r,
47rr2dr c(r, T ) 47rr2 dr T)
(R2
=
(7.33)
gives the meansquare displacement away from the original point source. Using Eq. 7.32 and the relationship (7.34) in Eq. 7.33, the meansquare displacement for isotropic threedimensional diffusion is related to the diffusivity by
(R2( T ) ) = ~ D T
(7.35)
156
CHAPTER 7: ATOMIC MODELS FOR DIFFUSION
For diffusion in one and two dimensions, similar calculations show that (R2( r ) )= 2 D r and 4 D r , respectively. An analogous expression for ( R 2( r ) )when the diffusivity is anisotropic is explored in Exercise 7.4. Equation 7.35 is a fundamental relationship between the diffusivity and the meansquare displacement of a particle diffusing for a time 7. Because diffusion processes in condensed matter are comprised of a sequence of jumps, the meansquare displacement in Eq. 7.31 should be equivalent to Eq. 7.35. This equivalence, as demonstrated below, results in relations between macroscopic and microscopic diffusion parameters. 7.2.2
Diffusion and Random Walks
If a particle moves by a series of displacements, each of which is independent of the one preceding it, the particle moves by a random walk. Random walks can involve displacements of fixed or varying length and direction. The theory of random walks provides distributions of the positions assumed by particles; such distributions can be compared directly to those predicted to result from macroscopic diffusion. Furthermore, the results from random walks provide a basis for understanding nonrandom diffusive processes. The distribution of positions is easily formulated for a random walker on a onedimensional lattice and illustrates important aspects of all random walks. Such a distribution can be compared to the solution for macroscopic diffusion in Table 5.1. Extensions to two and three dimensions are not difficult. The particles are assumed t o migrate independently. A given particle starts at the origin and jumps either forward (along +z) with probability p~ or backward (along z) with probability p ~ where , 0 < p~ < 1 and p~ + p~ = 1. Suppose that each displacement is of length one, then after N , >> 1 displacements it is possible that the particle will 1, . . .  1, 0 , 1, . . . N ,  1, N,. It is highly unlikely that end up at N,, N, the particle will make all positive jumps to reach site N , or all negative jumps to reach N,. If p~ = p~ = 1 / 2 , then, on average, the particle will be located at the origin because the equally probable positive and negative displacements negate each other. To find the probability that a particle occupies a position n after N , jumps, let N R be the number of positive displacements and N L be the number of negative displacements, NR NL= n (7.36) (7.37) N R N L = N, The number, R(n, N,), of different ways (trajectories, sequences, etc.) the walker can get t o site n from the origin is given by the binomial coefficient N,! N,! (7.38) n ( n ,N,) = N R !N L ! [ ( N , n ) / 2 ] ![ ( N ,  n ) / 2 ] ! Therefore, the probability of getting to site n after N, jumps is
+
+
~
+
(7.39) If the probability of jumping right, p ~ is ,equal to the probability of jumping left, PL 1
(7.40)
7 2 . DIFFUSION AS A SERIES OF DISCRETE JUMPS
157
Using Stirling's formula, Q! = m Q Q e  &
and taking the limit n / N ,
(7.41)
<< 1 yields
Equation 7.42 shows that the distribution of a point source in one dimension spreads as a Gaussian. , probability distribution for the displacement R is Letting R = n ( r 2 ) l I 2the (7.43) The probability distribution must be normalized, so that 00
p(R,7 )dR = 1
(7.44)
Therefore, the probability distribution becomes (7.45) which is of the same form as the macroscopic solution for onedimensional diffusion from a point source in Table 5.1. The first and second moments of Eq. 7.45 are readily evaluated: (7.46) and
00
( R 2 )=
p ( R ,N,)R2 dR = N , ( r 2 )
(7.47)
J03
Equation 7.46 demonstrates that if each jump of a walk occurs randomly (i.e., is uncorrelated), the average displacement is zero and the center of mass of a large number of individual random jumpers is not displaced. Equation 7.47 gives the . Eqs. 7.46 and 7.47 meansquare displacement of a random walk, N T ( r 2 ) Although were derived here for onedimensional random walks, both are valid for two and threedimensional random walks. The probability distribution of a random walk shows that the meansquare displacement after N , jumps is ( R 2 )= N T ( r 2 )= I ' 7 ( r 2 ) (Eq. 7.47). Comparison of the probability distribution (Eq. 7.45) to the pointsource solution for onedimensional diffusion from a point source (Table 5.1) indicates that (7.48) Equation 7.48 relates the macroscopic diffusivity and microscopic jump parameters for uncorrelated diffusion in one dimension.
158
CHAPTER 7: ATOMIC MODELS FOR DIFFUSION
7.2.3
Diffusion with Correlated Jumps
The calculated rootmeansquare displacement for a general sequence of jumps has two terms in Eq. 7.31. The first term, N,(r2), corresponds to an ideal random walk (see Eq. 7.47) and the second term arises from possible correlation effects when successive jumps do not occur completely at random. For walks with correlation^,^ a correlation factor, f , can be defined (7.49) so that Eq. 7.31 becomes
(7.50)
(R2)= N,(r2)f
For a random walk, f = 1 because the double sum in Eq. 7.49 is zero and Eq. 7.50 reduces to the form of Eq. 7.47. In principle, f can have a wide range of values corresponding to physical processes relating to specific diffusion mechanisms. This is readily apparent in extreme cases of perfectly correlated onedimensional diffusion on a lattice via nearestneighbor jumps. When each jump is identical to its predecessor, Eq. 7.49 shows that the correlation factor f equals N7.6 Another extreme is the case off = 0, which occurs if each individual jump is exactly opposite the previous jump. However, there are many real diffusion processes that are nearly ideal random walks and have values of f x 1, which are described in more detail in Chapter 8. The relationship between the macroscopic isotropic diffusivity, D, and microscopic jump processes can be evaluated in three dimensions. The equivalence of Eqs. 7.31 and 7.35 means that
\
j=1
i=l
I
Substitution of Eq. 7.49 into Eq. 7.51 yields the relation between the macroscopic isotropic diffusivity and microscopic parameters (7.52) Equation 7.52 is of central importance for atomistic models for the macroscopic diffusivity in three dimensions (see Chapter 8). For isotropic diffusion in a system of dimensionality, d , the generalized form of Eq. 7.52 is (7.53) Equations 7.52 and 7.53 reduce to D for randomwalking particles (i.e., Eq. 7.48) where there are no correlations and f = 1. Values of f for several diffusion mechanisms are discussed in Section 8.2.1. 5Correlated jumps are discussed in Chapter 8. 6There are (N:  N T ) / 2cosine terms in the double sum and all are equal to unity.
159
EXERCISES
Bibliography
1. S. Glasstone, K.J. Laidler, and H. Eyring. The Theory of Rate Processes. McGrawHill, New York, 1941.
2. C.A. Wert and C. Zener. Interstitial atom diffusion coefficients. Phys. Rev., 76(8):11691175, 1949. 3. G.H. Vineyard. F’requency factors and isotope effects in solid state rate processes. J . Chem. Phys. Solids, 3(12):121127, 1957. 4. S.A. Rice. Dynamical theory of diffusion in crystals. Phys. Rev., 112(3):804811, 1958. 5. C.P. Flynn. Point Defects and Dzffusion. Oxford University Press, Oxford, 1972.
6. L A . Girifalco. Statistical Physics of Materials. John Wiley & Sons, New York, 1973. 7. J.W. Christian. The Theory of Transformations in Metals and Alloys. Pergamon Press, Oxford, 1975.
8. W.M. Franklin. Classical and quantum theory of diffusion in solids. In A.S. Nowick and J. J. Burton, editors, Diflusion in Solids, Recent Developments, pages 172. Academic Press, New York, 1975. 9. D.A. McQuarrie. Statistical Mechanics. HarperCollins, New York, 1976.
EXERCISES
7.1 Prove that the preexponential frequency factor given by Eq. 7.14 is indeed the frequency of a linear oscillator of mass, m, and force constant, p. Solution. The equation o f motion o f a linear oscillator is F ( x ) = px(t) =
d2x
mdt2
(7.54)
where z ( t ) is the displacement o f the mass from the position where the restoring force, F, is zero. The solution of Eq. 7.54 is of the form x(t) = Asin(wt) where A = constant. Substitution of z ( t )in Eq. 7.54 shows that
w = 27ru =
(7.55)
7.2 The quantity V”, given by Eq. 7 . 2 6 , is the difference between the volume of the system in an activated state and a well state. This volume difference is generally termed the activation volume for migration and is a positive quantity because of the atomic squeezing and resulting expansion of the system that occurs in the activated state. The activation volume can be measured experimentally by measuring the pressure dependence of the jump frequency, I”. Find an expression for the pressure dependence of I” and describe how it can be used to determine V m . Solution. Use Eq. 7.25 for I?’ and differentiate r’ with respect t o pressure, so that d In r’
dlnv
(7.56)
160
CHAPTER 7. ATOMIC MODELS FOR DIFFUSION
Using the standard thermodynamic relation [ ~ G / B P ] = T V and realizing that the pressure dependence o f l n v will be relatively very small, we may write t o a good approximation
(7.57) If a plot of l n r ' vs. P is now constructed using the experimental data, V" can be determined from its slope.
7.3 Consider small interstitial atoms jumping by the interstitial mechanism in b.c.c. Fe with the diffusivity D for a time T . (a) What is the most likely expected total displacement after a large number of diffusional jumps? (b) What is the standard deviation of the total displacement? Solution. (a) The expected total displacement will be zero because there is no correlation between successive jumpsafter a jump the interstitial loses its memory of its jump and makes its next jump randomly into any one o f its nearestneighbor sites. (b) The distribution of displacements will be Gaussian (Eq. 7.32) and the standard deviation will be the rootmeansquare displacement given by Eq. 7.35 as
m.
7.4 Suppose the random walking of a diffusant in a primitive orthorhombic crystal where the particle makes N1 jumps of length a1 along the X I axis, NZjumps
of length a2 along the xz axis, and N3 jumps of length a3 along the 2 3 axis. The three axes are orthogonal and aligned along the crystal axes of the orthorhombic unit cell and the diffusivity tensor in this axis system is
.=[ : Doz Dll
0
4 0
(7.58)
(a) Find an expression for the meansquare displacement in terms of the numbers of jumps and jump distances.
(b) Find another expression for the meansquare displacement in terms of the three diffusivities in the diffusivity tensor and the diffusion time. Your answer should be analogous to Eq. 7.35, which holds for the isotropic case. Solution. (a) Using Eqs. 7.30 and 7.31,
c N
(R2) =
i=l
r', . r', = Nla:
+ N2a; + N3ai
(7.59)
(b) The diffusion equation will have the form o f Eq. 4.61. By using the method of scaling described in Section 4.5 (based on the scaling relationships in Eq. 4.64), the solution can be written
A
c ( a , m , ~ ,= t )exp
d
EXERCISES
161
where A = constant. The meansquare displacement is then
(R2) = 
S;;OS,"S;;"c(zi,22,23,t)~~d5id~2d23 ~,oo~o~~o~c(zl,z2,z3,t)dzl~~2~~3
J," J," J,"
Le 2Le L (zf+ zg + z:)
e4Diit
4D22t
4D33t
dzl dz2dz3
SoooSoooS,"C(zl1z2,X3,t)dzldz2dz3
(7.61)
Equation 7.61 can be factored into standard definite integrals and the result is
(R2) = 2D11t + 2022t + 2D33t
(7.62)
Comparison of Eqs. 7.59 and 7.62 shows that the meansquare displacement consists of three terms, each of which is the meansquare displacement that would be achieved in one dimension along one of the three coordinate directions.
7.5 Suppose a random walk occurs on a primitive cubic lattice and successive jumps are uncorrelated. Show explicitly that f = 1 in Eq. 7.49. Base your
argument on a detailed consideration of the values that the cosOi,i+j terms assume. Solution. Because all jumps are o f the same length,
=1
+(cos 01,2 + cos 01,3 . . . + cos e2,3+ cos e2,4 + cos eN,l,NT) NT
(7.63)
2
' '
and thus,
2
f = I + [(cosel,2) NT
+ (cosel,3)+...+(cose2,3)...+(COSeN,1,NT)1 (7.64)
Any j u m p can be one of the six vectors: [aOO],[TiOO], [OaO],[OZO],[OOa],and [OOTi]. Each occurs with equal probability. For each pair o f j u m p vectors, i and i+j, the six possible values of cosQz,a+3are 1,  1 , O , O , O , and 0, and these occur with equal probability. For a large number o f trajectories, each mean value in Eq. 7.64 is zero and therefore f = 1.
7.6 For the diffusion of vacancies on a facecentered cubic (f.c.c.) lattice with
lattice constant a, let the probability of first and secondnearestneighbor jumps be p and 1  p , respectively. At what value of p will the contributions to diffusion of first and secondnearestneighbor jumps be the same? Solution. There is no correlation and, using Eq. 7.29, N
(7.65) The number of first nearestneighbor jumps is NTp and the number of second nearestneighbor jumps is N T ( l p ) . Therefore,
(R2) = N T p+~NT(1  p ) a 2 a2
They make equal contributions when NTpa2/2= N T ( l p ) a 2 or p = 2/3.
(7.66)
CHAPTER 8
DIFFUSION IN CRYSTALS
The driving forces necessary to induce macroscopic fluxes were introduced in Chapter 3 and their connection to microscopic random walks and activated processes was discussed in Chapter 7. However, for diffusion to occur, it is necessary that kinetic mechanisms be available to permit atomic transitions between adjacent locations. These mechanisms are materialdependent . In this chapter, diffusion mechanisms in metallic and ionic crystals are addressed. In crystals that are free of line and planar defects, diffusion mechanisms often involve a point defect, which may be charged in the case of ionic crystals and will interact with electric fields. Additional diffusion mechanisms that occur in crystals with dislocations, free surfaces, and grain boundaries are treated in Chapter 9.
8.1 A T O M I C M E C H A N I S M S Atom jumping in a crystal can occur by several basic mechanisms. The dominant mechanism depends on a number of factors, including the crystal structure, the nature of the bonding in the host crystal, relative differences of size and electrical charge between the host and the diffusing species, and the type of crystal site preferred by the diffusing species (e.g., anion or cation, substitutional or interstitial). Kinetics of Materials. By Robert W. Balluffi, Samuel M. Allen, and W. Craig Carter. Copyright @ 2005 John Wiley & Sons, Inc.
163
164
CHAPTER 8 DIFFUSION IN CRYSTALS
8.1.1
Ring Mechanism
A substitutional atom (indicated by shading in Fig. 8.1) may jump and replace an adjacent nearestneighbor substitutional atom. In the rang mechanasm. the substitutional atom exchanges places with a neighboring atom by a cooperative ringlike rotational movement.
00000 00000 00000 00000 OOOc90
OOO@O
00000 00000 Figure 8.1:
8.1.2
Riiig riiecliaiiisiri for diffusioii of substitutioiial atorris.
Vacancy Mechanism
A substitutional atoni can migrate to a neighboring substitutional site without cooperative motion and with a relatively small activation energy if the neighboring
substitutional site is unoccupied. This is equivalent to exchange with a neighboring vacancy.l In Fig. 8.2a, the vacancy is initially separated from a particular substitutional atom (again indicated by shading). In Fig. 8.2b, it has migrated by exchanging places with host atoms to a nearestneighbor substitutional site of the shaded atom. In Fig. 8 . 2 ~ the vacancy has exchanged sites with the substitutional atom: and in Fig. 8.2d the vacancy has migrated some distance away. As a result, the particular substitutional at,om is displaced by one nearestneighbor distance while the vacancy has undergone at least five individual displacements. The atomic environment during a vacancyexchange mechanism can be illustrated in a threedimensional cubic lattice. Figure 8.3 shows an atomvacancy exchange between two facecentered sites in an f.c.c. crystal. The migrating atom ( Ain Fig. 8.3) moves in a (110)direction through a rectangular “window” framed by two cube corner atoms and two opposing facecentered atoms. The f.c.c. crystal is closepacked and each site has 12 equivalent nearestneighbor sites [l]. In
00000 000000000000000 00000 000 0 000000000000000 0000000000 00000 00000 Figure 8.2:
Vacaiicy mecliaiiism for diffiisioii of substitutional atonis.
‘Vacancies will always exist in equilibrium in a crystal because their enthalpy of formation can always be compensated by a configurational entropy increase a t finite temperatures (see the derivation of Eq. 3.65). Therefore, vacancies function as a component that occupies substitutional sites.
8 1 ATOMIC MECHANISMS
165
X
4
Figure 8.3: Atomvacancy exchange in f.c.c. cryshl. Atom init,ially at A jumps into a nearestneighbor vacancy (dashed circle). The four nearest,neighbor atoms common to A and t,he vacant site (joined by the bold rectangle) form a "window" 1234 through which the A atom must, pass. The A atom is centered in unitcell face 2356. The vacancy is centered in unitcell face 2378.
a hardsphere model. in which nearestneighbor atoms are in contact, the atoni must "squeeze" through a window that is about 27% smaller than its diameter. The potentialenergy increases required for such distortions create the energetic migration barriers discussed in Section 7.1.3.
8.1.3 lnterstitialcy Mechanism A substitutional atom can migrate to a neighboring substitutional site by the twostep process illustrated in Fig. 8.4. The first step is an exchange with an interstitial defect in which the migrating substitutional atom becomes the interstitial atom.2 The second step is to exchange the migrating atom with a neighboring substitutional atom. This mechanism is only possible when substitutional atoms can occupy interstitial sites. This cooperative and serpentine motion constitutes the interstitialcy mechanism, and when large normally substitutional atoms are involved, can occur with a much lower migration energy than the interstitial mechanism (see below). Interstitialcy migration depends on the geometry of the interstitial defect. However, an a priori prediction of interstitial defect geometry is not straightforward in real materials. For an f.c.c. crystal, a variety of conceivable interstitial defect candidates are illustrated in Fig. 8.5. The lowestenergy defect will be stable and predominant. For example. in the f.c.c. metal Cu. the stable configuration is the (100) splitdumbbell configuration in Fig. 8.5d [ 3 ] . The (100) splitdumbbell defect in Fig. 8.5d, while having the lowest energy of all interstitial defects, still has a large formation energy (Ef= 2.2 eV) because of the large amount of distortion and ioncore repulsion required for its insertion into the closepacked Cu crystal. However, once the interstitial defect is present, it persists until it migrates to an interface or dislocation or annihilates with a vacancy. The 21nterstitial point defects involving normally substitutional atoms will always exist (although typically at very low concentration) a t equilibrium in a crystal a t finite temperatures because. as in the case of vacancies described above, their enthalpy of formation can always be compensated by a configurational entropy increase.
166
CHAPTER 8. DIFFUSION IN CRYSTALS
00000 0 0 0 0
00 00 00 00 00000 00000 00000
Figure 8.4: Substitutional diffusion by the iiiterst,itialcy mechanisrn. (a)The iiiterstit ial defect, corresponding to the interstitial atom ( 3 ) is separated from a part,iciilar siibst,itutional atom B (shaded). (b) The interstitial defect, moved adjacent t,o B when t>hepreviously interstitial atom (3) replaced the substit,utional atom (2). (2) then became the int,erstitial atom. ( c ) At.om (2) has replaced B. and B has become the interst,it,ial atom. (d) B has replaced atom (4): which has become the interstitial atom. (e) The int,erstitial defect has migrated away from B . As a result. B has completed one nearestneighbor jump and the interstitial defect has moved at, least four times.
Figure 8.5: Geonietric corifiguratioris for a selfinterst,itialdefect atom in an f.c.c. crystal: (a) oct,ahedral site, (b) tetrahedral site, ( c ) (110) crowdion, (d) (100) split, dumbbell. (e) (111) split,. ( f ) (110) split crowdioii [2].
activation energy for migration ( E m = 0.1 eV) is small compared to Ef because little additional distortion is required for its serpentine motion, which is illustrated in Fig. 8.6. It therefore migrates relatively rapidly.
8 1 ATOMIC MECHANISMS
167
X
A
Z
Diffusiorial niigratioii of a [loo] splitduiiibbell selfiiiterstitial iii ail f.c..c.. Figure 8.6: uystal. The durnbbell in (a)rail juirip int,o four iiearestiieighbor sites: c,rwtiiig [OOl] durnbbells [one of which is sliowii iii (b)]atrid into four others. creatirig [OlO]diirnbliells.
8.1.4
Interstitial Mechanism
An interstitial atom can simply migrate between interstitial sites as in Fig. 8.7. The interstitial atom must attain enough energy to distort the host crystal as it migrates between substitutional sites. This mechanism is expected for small solute atoms that normally occupy interstitial sites in a host crystal of larger atoms. Diffusion by the interstitial mechanism and by the interstitialcy mechanism are quite different processes and should not be confused. Diffusion by the vacancy and interstitialcy niechanisms requires the presence of point defects in the system. whereas diffusion by the ring and interstitial mechanisms does not.
00 00 .oo 00 00000 ~00000 Figure 8.7: Interstitial mechanism for diffusion of interstitial atoms. T h r snialler shaded interstitial atom niigrates through the openiiig betweeii host atoms (1) and ( 2 ) to a neighboring interstitial site.
8.1.5
Diffusion Mechanisms in Various Materials
Diffusion of relatively small atoms that normally occupy interstitial sites in the solvent crystal generally occurs by the interstitial mechanism. For example, hydrogen atoms are small and migrate interstitially through most crystalline materials. Carbon is small compared to Fe and occupies the interstitial sites in b.c.c. Fe illustrated in Fig. 8.8 and migrates between neighboring interstitial sites. Migration of atoms that occupy substitutional sites may occur through a range of mechanisms involving either vacancy or interstitialtype defects. In f.c.c., b.c.c., and hexagonal closepacked (h.c.p.) metals, selfdzffuszon occurs predominantly by the vacancy mechanism [4, 51. However, in some cases selfdiffusion by the
168
CHAPTER 8 DIFFUSION IN CRYSTALS
X
Figure 8.8: 1nterst)itial sites for C atjoins iii b.c..c.. Fe. (a) Tlie intrrstitial sites liwe pointgroup syriiirietry 4/mmm, and tlie orient,ations of tlie fourfold axes are indicxtrti by the shorter, grey spokes on tlie symbols. (b) Noiiicnclat,ure uscd in t,he model for diffusion of interstitial atonis in b.c.c. Fe discussed in Section 8.2.1 Three different types of sit,es are present: sites 1. 2. and 3 have nearestneighbor Fe atonis lying along 2 . y. and z . rcymtiwly.
interstitialcy mechanism contributes a small amount to the overall diffusion (see Section 8.2.1). In Ge, which has the less closely packed diamondcubic structure, selfdiffusion occurs by a vacancy mechanism. In Si (which like Ge has covalent bonding), selfdiffusion occurs by the vacancy mechanism at low temperatures and by an interstitialcy mechanism at elevated temperatures [681. In ionic materials, diffusion mechanisms become more complex and varied. Selfdiffusion of Ni in N i 0 occurs by a vacancy mechanism; in C u a 0 the diffusion of 0 involves interstit,ial defects [9]. In the alkali halides, vacancy defects predominate and the diffusion of both anions and cations occurs by a vacancy mechanism. However: the predominant defect is not easy to predict in ionic materials. For example, vacancyinterstit,ial pairs dominate in AgBr and the smaller Ag cations diffuse by an interstitialcy mechanism (see Section 8.2.2). Solutes that normally occupy substitutional positions can migrate by a variety of mechanisms. In many systems they migrate by the same mechanism as for selfdiffusion of the host atoms. However, the details of migration become more complex if there is an interaction or binding energy between the solute atoms and point defectsthis is described in Section 8.2.1 for vacancysoluteatom binding. Certain solute a t o m can migrate by more than one mechanism. For example. while Au solute atoms in Si are mainly substitutional, under equilibrium conditions: a relatively small number of Au atoms occupy interstitial sites. The rate of migration of the interstitial Au atoms is orders of magnitude faster than the ratmeof the substitutional Au atoms, and the small population of interstit,ial Au atoms therefore makes an important contribution to the overall soluteat,om diffusion rate [6. 81. The solute atoms transfer from substitutional sites to interstitial sites by either kickout or dissociative mechanisms (Fig. 8.9). In the kickout mechanism, an interstitial host atom, H I , pushes the substitutional solute atom, Ss. into an interstitial position and simultaneously takes up a substitutional position according to the reaction
169
8.2 ATOMIC MODELS FOR DlFFUSlVlTlES
0000 00 00 00 0 000 ( h ) O 0 0 O 0000 Figure 8.9: Transfer of a soliitr at,oni (filled at,orii) from a subst,it,utional site to interstitial site by (a) the kickout rriechanisni arid (b) t,lw dissoriative mechanism.
ail
In the dissociative mechanism, a substitutional solute atom enters an interstitial site. leaving a vacancy, V ,behind according to the reaction
ss = v, + SI
(8.2)
These reactions are reversible. This dualsit,e occupancy leads to complicated solute diffusion behavior and has been described for several solut,e species in Si [4, 6, 81. There is no compelling evidence that the ring mechanism in Fig. 8.1 contributes significantly to diffusion in any material.
8.2
ATOMIC MODELS FOR DlFFUSlVlTlES
Atomic models for the diffusivity can be constructed when the diffusion occurs by a specified mechanism in various crystalline materials. A number of cases are considered below. 8.2.1
Metals
Diffusion o f Solute Atoms by the Interstitial Mechanism in the B.C.C. Structure. The general expression that connects the jump rate. I?. the intersite jump distance, r , and the correlation factor, Eq. 7.52. then takes the form
(8.3) Because each interstitial site has four nearestneighbors, the jump rate. r. is given by 4 r ' , where I" has the form of Eq. 7.25.3 If a is the lattice constant for the b.c.c. unit cell in b.c.c. Fe, then r = a12 and Eq. 8.3 yields (8.4) ,'The quantity r', introduced in Section 7.1.1, is the jump rate of an atom from one specified site to a specified neighboring site. r is the total jump rate of the atom in the material. If the atom is diffusing among equivalent sites in a crystal where each site has z equivalent nearestneighbors, then r = zr'.
170
CHAPTER 8 DIFFUSION IN CRYSTALS
where the weakly temperaturedependent terms have been collected into D,”. Because D; is relatively temperature independent, the Arrhenius form of Eq. 8.4 indicates a thermally activated process. The enthalpy of migration, H m , is the activation energy, E , for the interstitial diffusion. For C in Fe, 0; = 0.004 cm2 sl and Hm= 80.1 kJ mol’ [lo]. This experimental value of D; is consistent with the value predicted by Eq. 8.4 for a = 2.9 x m, I/ = 1013 sl, and S” = lk/atom. The relationship between jump rate and diffusivity in Eq. 8.3 can be obtained by an alternate method that considers the local concentration gradient and the number of sitepairs that can contribute to flux across a crystal plane. A concentration gradient of C along the yaxis in Fig. 8.8b results in a flux of C atoms from three distinguishable types of interstitial sites in the cy plane (labeled 1, 2, and 3 in Fig. 8.8). The sites are assumed to be occupied at random with small relative populations of C atoms that can migrate between nearestneighbor interstitial sites. If c’ is the number of C atoms in the cy plane per unit area, the carbon concentration on each type of site is c’/3. Carbon atoms on the types 1 and 3 sites jump from plane Q to plane at the rate ( c 1 / 3 ) I ” .The jump rate from type2 sites in plane Q to plane p is zero. The contribution to the flux from all three site types is
If c is the number of C atoms per unit volume, c = 2c’/a, and therefore Ja+P
ar’c =3
The reverse flux can be obtained by using a firstorder expansion of the concentration in the p plane, so that
Therefore, the net flux is
Comparison of Eq. 8.8 with the Fick’s law expression, (8.9)
Droduces (8.10) The total jump frequency for a given C atom is
r = 4r’,and therefore
a 2 r r2r DI==24
6
(8.11)
which is identical to Eq. 8.3. The same result would have been obtained with the cy and /3 planes chosen at any arbitrary inclination in the Fe crystal because DI is isotropic in all cubic crystals (see Exercise 4.6).
8 . 2 : ATOMIC MODELS FOR DlFFUSlVlTlES
171
SelfDiffusion by the Vacancy Mechanism in the F.C.C. Structure. Each site on an f.c.c. lattice has 12 nearestneighbors, and if vacancies occupy sites randomly and have a jump frequency rv, rv = 1217; (8.12)
where
I'b
is given by Eq. 7.25, (8.13)
If the fraction of sites randomly occupied by the vacancies is X V ,the jump rate of the host atoms must be rA= xvrv (8.14) Using Eq. 7.52, the selfdiffusivity is (8.15) where r = a/&' is the nearestneighbor jump distance in an f.c.c. crystal. The diffusion of the vacancies is uncorrelated4 and the vacancy diffusivity is (8.16) which is related to the selfdiffusivity by
*D = X v D v f
(8.17)
If the vacancies are in thermal equilibrium, X V = XEq,where, according to Eq. 3.65, (8.18) where 5'6 and H b are the vacancy vibrational entropy and enthalpy of formation, re~pectively.~ Using Eqs. 8.13 and 8.15
*D = fa2v ,(SF+SC)/~,(HF+HG)/(~T)
 *DoeE/("T)
where
*DO
fa2v e ( S F + S $ ) / k
(8.19)
and the activation energy is given by
E=H;+H~
(8.20)
Equation 8.19 contains the correlation factor, f , which in this case is not unity since the selfdiffusion of tracer atoms by the vacancy mechanism involves correlation. Correlation is present because the jumping sequence of each tracer atom produced by atomvacancy exchanges is not a random walk. This may be seen by 4The diffusion of vacancies is uncorrelated for the same reasons given above for diffusion of the interstitial atoms. After each jump, a vacancy will have the possibility of jumping into any one of its 12 nearestneighbor sites with equal probability. 5Because Gfv is the free energy to form a vacancy exclusive of the configurational mixing entropy (see Section 3.4.1),the only entropy included in Sf in the relation Gfv = Hf TSf is the thermal vibrational entropy.
172
CHAPTER 8: DIFFUSION IN CRYSTALS
considering a tracer atom immediately after a jump. The vacancy with which it just exchanged will be one of its 12 nearestneighbors. For its next jump, the tracer atom can either jump back into the vacancy with which it has just exchanged, jump into another vacancy which happens to be present in another nearestneighbor site, or wait for another vacancy to arrive at a nearestneighbor site into which it jumps. Because the first possibility is most probable, the atom jumping is nonrandom. The second jump is correlated with respect to the first because the first jump creates a situation (i.e., the existence of a nearestneighbor vacancy) that biases the second jump . A rough estimate for f can be obtained based on the number of nearestneighbors and the probability that a tracer atom which has just jumped and vacated a site will return to the vacant site on the vacancy's next jump. A vacancy jumps randomly into its nearestneighbor sites, and the probability that the return will occur is l / z . This event will then occur on average once during every z jumps of an atom. For each return jump, two atom jumps are effectively eliminated by cancellation, and the overall number of traceratom jumps that contribute t o diffusion is reduced by the fraction 2/25. According to Eq. 8.3, *D is proportional to the product rf, and since the number of effective jumps is reduced by 2/2, f can be assigned the value f M 1  2/25 = 0.83 for f.c.c. crystals. More accurate calculations (see below) show that f = 0.78. To find a more accurate value of f , Eq. 7.49 is applied [4, 1113]. If all displacements are of equal length, (8.21)
The quantity (cosOi,i+j) can be evaluated with the aid of the law of cosines from spherical trigonometry: (cos 6'i,i+z) = (cos6'i,i+lcos 6'i+1,i+2)
+ (sin6'i,i+lsin 6'i+l,i+2
cos a )
(8.22)
where a is the angle between the two planes defined by the successive jump vectors r', and < + I and the successive jump vectors r',+1 and r'i+z. For cubic crystals, contributions from angle a will be canceled by those from angle (180'  a ) on the average. Therefore, the last term in Eq. 8.22 containing cosa will average to zero: (cos 6 ' i , i + z ) = (cos & , i + l cos Q i + l , i + Z )
(8.23)
The average cosine of the angle between successive jumps must be the same for all pairs of successive jumps.6 Therefore, ( c o s ~ ~ ,=~ (+C~O )S B ~ , ~ + ~ ) ( C ~ S ~=~ +( ~c. ~~ +s~ )~ ) ~
(8.24)
where cos 6' denotes the angle between successive jumps. By induction,
ei,i+3)= (COS ei,i+2)(COS ei+2,i+3)= (COS e)3 (COS ei,i+j)= (COS e ) j
(COS
(8.25)
6The immediate surroundings after each jump must be the same (excepting a change of orientation of the vacancyatom pair); consisting of the atom with a nearestneighbor vacancy next t o it. The average of what happens t o produce the next jump must be the same for all pairs of jumps (in their respective orientations).
8.2: ATOMIC MODELS FOR DlFFUSlVlTlES
173
Putting Eq. 8.25 into Eq. 8.21 yields
(8.26)
As N, becomes large, the term j/N, in Eq. 8.26 can be neglected and the finite sum becomes an infinite sum, (8.27) This infinite sum is known as (8.28) and therefore (8.29) Equation 8.29 is exact, and the accuracy of the determination of f then depends on the accuracy with which (cos8) can be determined. Equation 8.29 can be used t o obtain another approximation for f by employing an estimated value of (cos8). To estimate this quantity, consider an atom that has just exchanged with a vacancy; there is a probability l / z that the vacancy’s next exchange will be with the same atom and, therefore, the probability that cos8 = 1 is l / z or (cos8) = l/z. If the vacancy separates from the particular atom, that particular atom cannot migrate until it obtains another (or the same) vacancy as a neighbor; the contribution to (cos 8) from these displacements will be small compared to l/z, and therefore Eq. 8.29 can be written fx
1l/z  21 l+l/z z+1
(8.30)
and f = 0.85 for f.c.c. crystals, which is close to the previous estimate. An accurate determination of f can be obtained by considering all contributing vacancy trajectories to determine (cos8) by use of Eq. 8.29 [13]. For f.c.c., the accurate value o f f is found to be 0.78; thus, correlations affect the diffusivity value by about 22% in Eq. 7.52.7 Correlations can have a considerably larger effect on the diffusivity for substitutional solute atoms by the vacancy mechanism. For the vacancy selfdiffusion mechanism in many metals, experimental values of *Doare approximately 0.11.0 cm2 sl, which correspond to physically reasonable values of the quantities in *Do according to Eq. 8.19: f x 1, a x 3.5 x lo’’ m, v x 1013 sl, and (S& SF) x 2 k . In metals, as in many classes of materials, the
+
7 A calculation of f in a twodimensional lattice that takes into account multiple return vacancy trajectories appears in Exercise 8.8.
174
CHAPTER 8: DIFFUSION IN CRYSTALS
activation energy for vacancy selfdiffusion, E in Eq. 8.20, scales with the melting temperature because the crystal binding energy correlates with both melting temperature and vacancy formation energy. Activation energies are typically 0.56 eV (1 eV = 96.46 kJ moll) and *Do is often nearly the same for materials with the same crystal structure and bonding [4]. Vacancy formation and migration energies, such as H; and H F , have been obtained by independent experiments. For example, to obtain H,,f equilibrium vacancy concentrations can be measured from simultaneous thermal expansion and lattice expansion during quasiequilibrium heating [14] and by positron annihilation [15]. The vacancy migration rate can be determined by measuring the decay of a supersaturated population of quenchedin vacancies to their equilibrium population in order to measure H F [16]. The results of these independent determinations are generally consistent with the measured values of the substitutional diffusivity activation energies inferred from Eq. 8.19 [4]. In Section 3.1.1, selfdiffusion was analyzed by studying the diffusion of radioactive tracer atoms, which were isotopes of the inert host atoms, thereby eliminating any chemical differences. Possible effects of a small difference between the masses of the two species were not considered. However, this difference has been found to have a small effect, which is known as the isotope effect. Differences in atomic masses result in differences of atomic vibrational frequencies, and as a result, the heavier isotope generally diffuses more slowly than the lighter. This effect canif migration is approximated as a singleparticle processbe predicted from the mass differences and Eq. 7.14. If ml and m2 are the atomic masses of two isotopes of the same component, Eqs. 7.13 and 7.52 predict the jumprate ratio,
Jump rate and diffusivity scale inversely with the square root of atomic mass. However, if migration involves manybody effects and collective motion, the assumptions leading t o Eq. 8.31 are no longer valid and this model must be discarded. Diffusion of Solute Atoms by Vacancy Mechanism in ClosePacked Structure. Diffusion of substitutional solutes in dilute solution by the vacancy mechanism is more complex than selfdiffusion because the vacancies may interact with the solute atoms and no longer be randomly distributed. If the vacancies are attracted to the solute atoms, any resulting association will strongly affect the soluteatom diffusivity. The effect is demonstrated in a simple manner in two dimensions in Fig. 8.10, which shows an isolated solute atom with a vacancy occupying a nearestneighbor site [4]. Three jump frequencies are considered: the intrinsic hostvacancy jump rate, the solutevacancy jump rate, and the jump rate for a vacancy and a host atom that also has a neighboring solute, When there is an attractive interaction between a solute atom and the vacancy ( a negative binding energy), is decreased because of the increase in activation energy of the jump due t o the binding energy between the vacancy and the solute atom. The activation energies for the remaining two types of exchange are not influenced by the binding energy, and two extremes can be considered:
a2
ATOMIC MODELS FOR DIFFUSIVITIES
175
Figure 8.10: A solute atoiri (darker shading) with a nearestneighbor vacancy iii a closepacked at,oniic plnric. 'I'hc vacancy itlid its three different nearestneighbor types exchange places with differiiig j i u r i p freqiiencies.
Case A is an example of strong correlation. Since the jump rate rlfsSvis relatively small, the vacancy remains bound to the solute atom for relatively long periods and the solute atom and bound vacancy exchange positions repeatedly at the rate rkSv,which is relatively high in comparison to rhos. However, eventually the vacancy will exchange with a host atom that is a nearestneighbor of the solute atom (at the rate and a new mode of oscillation of the solute atom is established with the bound vacancy in a new nearestneighbor site. This allows the solute atom to occupy a new site outside the first oscillating mode. If this occurs repeatedly, the solute atom can occupy new sites and execute longrange migration by a sort of tumbling motion of the oscillating mode's axis. The effective jump frequency of the solute atom during the period when the vacancy is bound to the solute atom is then and the selfdiffusivity of the solute atom during the time that the vacancy is bound to it can be written as
*Di= CYArLos
(8.32)
where C Y Ais a constant that includes various geometrical factors. An approximate expression for the diffusivity over a much longer period, including many H S V jumps, may now be obtained by using a simple nearestneighbor model for the binding of a vacancy to a solute atom. According to Boltzmann statistics, the probability of finding a bound vacancy in a nearestneighbor site to a solute atom at equilibrium is (8.33) $(bound) = e  G G / ( k T ) XVe q(free) where Gb, is the binding energy (negative when attractive) of the vacancy to the solute atom and Xbq(free) is the fraction of free vacancies in the bulk crystal. The number of bound vacancies (per unit volume) in a system where the solute concentration is c s is therefore 12csp7(bound), and since 12p7(bound) << 1, the probability of finding more than one vacancy bound to a solute atom at any time is very small. The fraction of solute atoms with a bound vacancy is then approximately 12p"vqbound). Over a long period of time, the fraction of time that any solute atom has a vacancy bound to it is then also given by 12p7(bound). The effective jump rate of the solute during this long time period is therefore lower than
176
CHAPTER 8: DIFFUSION IN CRYSTALS
the jump rate when a bound vacancy is present by the factor 12py(bound), and putting this result into Eq. 8.32 and using Eqs. 3.63 and 8.33, the solute diffusivity over a long period of time, including many H f V jumps, is (8.34) The selfdiffusivity of solute atoms is then proportional to the rate at which bound vacancies circulate around them rather than the rate at which they exchange with vacancies. In Case B, vacancies are again bound to solute atoms for relatively long periods of time. However, a bound vacancy will spend most of its time circling around a stationary solute atom by making a large number of V O S jumps, although it will occasionally make an S S V jump, allowing the solute atom to occupy a new site. Repetition of this process leads to longrange migration of the solute atom. Using an analysis similar to the above, the solute selfdiffusivity is then (8.35) In contrast to Case A, the solute selfdiffusivity is now proportional to the rate at which solute atoms exchange with vacancies. If the binding energy was negligible and all the frequencies in Fig. 8.10 were equal, the solute atom selfdiffusivity would be the same as that of the host atoms. Additional features of soluteatom diffusion can be studied using this threefrequency model. These, as well as models in three dimensions, are described by Shewmon [4]. DifFusion of SelfInterstitial Imperfections by the lnterstitialcy Mechanism in the F. C.C. Structure. For f.c.c. copper, selfinterstitials have the (100) splitdumbbell configu
ration shown in Fig. 8.5d and migrate by the interstitialcy mechanism illustrated in Fig. 8.6. The jumping is uncorrelated,8 (f = l),and a / f i is the nearestneighbor distance, so
These defects will always be present at thermal equilibrium, but their concentrations will be very small because of their high energy of formation. They can also be created by nonequilibrium processes such as irradiation [3]. SelfDiffusion by the lnterstitialcy Mechanism. If their formation energy is not too large, the equilibrium population of selfinterstitials may be large enough to contribute t o the selfdiffusivity. In this case, the selfdiffusivity is similar to that for selfdiffusion via the vacancy mechanism (Eq. 8.19) with the vacancy formation and migration energies replaced by corresponding selfinterstitial quantities. The 8After each jump the (100) dumbbell has an equal probability of making any of eight different jumps. Its next jump is therefore made at random.
8 2 ATOMIC MODELS FOR DIFFUSIVITIES
177
correlation factor fsimilar to selfdiffusion by the vacancy mechanismis less than unity because the atom jumps produced by the interstitialcy mechanism are correlated. For example, the (100) splitdumbbell configuration of the selfinterstitial defect in Cu has a formation energy that is considerably larger than the vacancy formation energy [3]. However, the relatively small population of equilibrium selfinterstitials may contribute significantly to the selfdiffusivity because the activation energy for interstitial migration is considerably lower than that for vacancy migration (as described in Section 8.1.3).
8.2.2
Ionic Solids
Diffusion in ionically bonded solids is more complicated than in metals because site defects are generally electrically charged. Electric neutrality requires that point defects form as neutral complexes of charged site defects. Therefore, diffusion always involves more than one charged speciesg The pointdefect population depends sensitively on stoichiometry; for example, the hightemperature oxide semiconductors have diffusivities and conductivities that are strongly regulated by the stoichiometry. The introduction of extrinsic aliovalent solute atoms can be used to fix the lowtemperature population of point defects. Intrinsic Crystal Self DifFusion. A simple example of intrinsic selfdiffusion in an ionic material is pure stoichiometric KC1, illustrated in Fig. 8 . 1 1 ~ As . in many alkali halides, the predominant point defects are cation and anion vacancy complexes (Schottky defects), and therefore selfdiffusion takes place by a vacancy mechanism. For stoichiometric KC1, the anion and cation vacancies are created in equal numbers because of the electroneutrality condition. These vacancies can be created
Figure 8.11: (a) Rocksalt st,riictiire of KCI and AgHr with (100) planes delineated. (b) Schottky defect on t~ (100) plaiie in KC1 coriiposed of anion vacancy arid cittion va.caricy ( c ) Freiikel defect on a. (100) plaiie in AgHr composed of cation selfiriterstitirtl and cation vacancy. 'For general discussions, see Kingery et al. [17] or Chiang et, al. [ls].
178
CHAPTER 8: DIFFUSION IN CRYSTALS
by removing K+ and C1 ions from the bulk and placing them at an interface or dislocation, or on a surface ledge as illustrated in Fig. 8.12. A vacancy on a K+ cation site will have an effective negative electronic charge and a vacancy on a C1site will have a corresponding effective positive charge. This defect creation is a reaction written in KrogerVink notation as KG
+ Cl& = V& + Vb1 + KZ + Cl& or > null = Vl, V&
+
(8.37)
In the KrogerVink notation used here, the subscript indicates the type of site the species occupies and the superscript indicates the excess effective charge associated with the species in that site [17]. A positive unit of charge (equal in magnitude to the electron charge) is indicated by a dot ( 0 ) superscript, a corresponding negative charge by a prime (') superscript, and zero charge (a neutral situation) by a times ( x ) superscript. The equilibrium constant, Keq, for Eq. 8.37 is related to the free energy of formation, G$, of the Schottky pair G i = kTlnKeq
(8.38)
or (8.39) where the a's are the activities of the anion and cation vacancies. For dilute concentrations of the vacancies, activities are equal to their site fractions by Raoult's law, [VL] [v:,] = Keq = e  G f s / ( k T ) (8.40) where the square brackets indicate a site fraction. Equation 8.40 is a general massaction law for the combined anion and cation vacancy site fractions. Furthermore, electrical neutrality requires that (8.41) Combining Eqs. 8.40 and 8.41, (8.42) The vacancy populations enter the expressions for the selfdiffusivity of the K+ cations and C1 anions. Starting with Eq. 7.52 and using the method that led to Eq. 8.19 for vacancy selfdiffusion in a metal, (8.43)
Figure 8.12: Creation of Schottky defect by transfer of anion and cation from regular crystal sites to ledges a t the surface.
8 2. ATOMIC MODELS FOR DlFFUSlVlTlES
179
where g is a geometrical factor and the correlation factor, f , has a value slightly less than unity. The activation energy for the selfdiffusion is therefore
E = HFV
+ Hi12
(8.44)
A similar expression applies to C1 selfdiffusion on the anion sublattice. Selfdiffusion of Ag cations in the silver halides involves Frenkel defects (equal numbers of vacancies and interstitials as seen in Fig. 8.11b). In a manner similar t o the Schottky defects, their equilibrium population density appears in the diffusivity. Both types of sites in the Frenkel complexvacancy and interstitialmay contribute to the diffusion. However, for AgBr, experimental data indicate that cation diffusion by the interstitialcy mechanism is dominant [4]. The cation Frenkel pair formation reaction is (8.45) The activity of Ag;,
is unity and, therefore, (8.46)
The electrical neutrality condition constrains the two site fractions: (8.47) The activation energy for selfdiffusivity of the Ag cations by the interstitialcy mechanisms is the sum of onehalf the Frenkel defect formation enthalpy and the activation enthalpy for migration,
E=HF+ H i 2
(8.48)
Extrinsic Crystal SelfDiffusion. Charged point defects can be induced to form in an ionic solid by the addition of substitutional cations or anions with charges that differ from those in the host crystal. Electrical neutrality demands that each addition results in the formation of defects of opposite charge that can contribute to the diffusivity or electronic conductivity. The addition of aliovalent solute (impurity) atoms to an initially pure ionic solid therefore creates extrinsic defects.'O For example, the selfdiffusivity of K in KC1 depends on the population of both extrinsic and intrinsic cationsite vacancies. Extrinsic cationsite vacancies can be created by incorporation of Ca++ by doping KC1 with CaCl2 and can be considered a twostep process. First, two cation vacancies and two anion vacancies form as illustrated in Fig. 8.12.'' Second, the single Ca++ cation and two C1 anions from CaC12 are inserted into the cation and anion vacancies, respectively; electric neutrality requires that each substitutional divalent cation impurity in KC1 be balanced 10Eztrinsic has the same meaning as in doped semiconductors. llThis process involves creation of additional sites in the crystal. Cation and anion sites must be created in the same proportion as the ratio of cation to anion sites in the host crystalin this case, 1:l. These defects can also be formed at pointdefect sources such as dislocations and grain boundaries (see Sections 11.4 and 13.4).
180
CHAPTER 8: DIFFUSION IN CRYSTALS
by the formation of a cation vacancy. The cationic and anionic vacancy populations are related to the site fraction of the extrinsic Ca++ impurity, [Cakl+ [Vt,l =
[v’,]
(8.49)
The massaction relationship in Eq. 8.40 for the product of the cation and anion vacancy site fractions combined with Eq. 8.49 yields (8.50) The last term on the righthand side of Eq. 8.50 is the square of the cation vacancy site fraction in pure (intrinsic) KC1. Solving the quadratic equation for the cation vacancy site fraction yields (8.51) There are two limiting cases for the behavior of [V’,] according to Eq. 8.51: Intrinsic: [V’,]pure >> [Cak],then [V’,] = [V’,]pure
Extrinsic: [V’,]pure
<< [Cak],then
[V’,] = [Cak]
The intrinsic case applies at small doping levels or at high temperatures where the thermal equilibrium site fraction of the intrinsic cation vacancy population exceeds that due t o the aliovalent solute atoms. In this case, the effect of the added solute atoms is negligible. The activation energy for cation selfdiffusion is therefore the same as in the pure material and is given by Eq. 8.44. The extrinsic case applies at low temperatures or large doping levels. The site fraction of cation vacancies is equal to the soluteatom sitefraction and is therefore temperature independent. In the extrinsic regime, no thermal defect formation is necessary for cation selfdiffusion and the activation energy consists only of the activation energy for cation vacancy migration. The expected Arrhenius plot for cation selfdiffusion in KC1 doped with Ca++ is shown in Fig. 8.13. The twopart curve reflects the intrinsic behavior at high temperatures and extrinsic behavior at low temperatures.
range 1IT
Arrhenius plot for selfdiffusivity on the cation sublattice, *DK,in KC1 Figure 8.13: doped with Ca++. The intrinsic and extrinsic ranges have different activation energies.
8 2 ATOMIC MODELS FOR DIFFUSIVITIES
181
Crystal Self D i f h i o n in Nonstoichiometric Materials. Nonstoichiometry of semiconductor oxides can be induced by the material's environment. For example, materials such as FeO (illustrated in Fig. 8.14), N O , and COO can be made metaldeficient (or 0rich) in oxidizing environments and Ti02 and ZrOz can be made 0deficient under reducing conditions. These induced stoichiometric variations cause large changes in pointdefect concentrations and therefore affect diffusivities and electrical conductivities. In pure FeO, the point defects are primarily Schottky defects that satisfy massaction and equilibrium relationships similar to those given in Eqs. 8.39 and 8.42. When FeO is oxidized through the reaction
FeO
+ X20 2
= FeOl+,
(8.52)
each 0 atom takes two electrons from two Fe++ ions, as illustrated in Fig. 8 . 1 4 ~ ~ according t o the reactions
(8.53)
corresponding to the combined reaction, 2Fe++
+ 210 2
+ 0
= 2Fe"'
(8.54)
Electrical neutrality requires that a cation vacancy be created for every 0 atom added, as in Fig. 8.14b; this, combined with site conservation, becomes 2Fege
+ 21
02
= 2Febe
+ 0; + V:e
(8.55)
te
I
o=
y
o=
1
o=
)
Fe+++
Figure 8.14: Addition of R ncwtral 0 atom to FeO to produce 0rich (metaldeficient) oxide. (a) An 0 atom receives two electrons from Fe" ions in the hulk material. (b) The final structure contains defects in the forni of t,wo Fc+++ ions and a cation (Fe++)vacancy.
182
CHAPTER 8 DIFFUSION IN CRYSTALS
which can be written in terms of holes, h , in the valence band created by the loss of an electron from an Fe++ ion producing an Fe+ft ion, 1
20 2 = 0;
+ Vge + 2h;e
hFe = FeFe  Fege
(8.56)
Equation 8.56 predicts a relationship between the cation vacancy site fraction and the oxygen gas pressure. The equilibrium constant for this reaction is important for oxygensensing materials: (8.57) For the regime in which the dominant charged defects are the oxidationinduced cation vacancies and their associated holes, the electrical neutrality condition is [Gel
=2 [Gel
(8.58)
Therefore, inserting Eq. 8.58 into Eq. 8.57 and solving for [Vke] yields (8.59) The cation selfdiffusivity due to the vacancy mechanism varies as the onesixth power of the oxygen pressure at constant temperature and the activation energy is (8.60) The dominance of oxidationinduced vacancies creates an additional behavior regime. The effect of this additional regime on diffusivity behavior is illustrated in Fig. 8.15. Other types of environmental effects create defects through other mechanisms and may lead to other behavior regimes.
\
Slope a Hcv+ Hfi2
1IT
Figure 8.15: Arrhenius plot for selfdiffusivity on the cation sublattice, *DFc,in FeO made Orich by exposure to oxygen gas at a pressure Poz or doped with an aliovalent impurity. Three regimes of behavior are possible. each with a different activation energy.
8.3: DIFFUSIONAL ANELASTICITY (INTERNAL FRICTION)
8.3
DIFFUSIONAL ANELASTICITY (INTERNAL FRICTION)
183
‘
In this section, pedagogical models for the time dependence of mechanical response are developed. Elastic stress and strain are ranktwo tensors, and the compliance (or stiffness) are rankfour material property tensors that connect them. In this section, a simple spring and dashpot analog is used t o model the mechanical response of anelastic materials. Scalar forces in the spring and dashpot model become analogs for a more complex stress tensor in materials. To enforce this analogy, we use the terms stress and strain below, but we do not treat them as tensors. For an ideally elastic material, the stress is linearly related to the strain by u = C&
(8.61)
(where the constant C represents the elastic stiffness), and conversely, the strain is linearly related to the stress by & = Su (8.62) (where the constant S = 1/C represents the compliance). For each level of stress, such a material responds immediately with a unique value of the strain. However, in many real materials, stressinduced diffusional processes cause additional timedependent anelastic strains and nonlinear behavior. This anelastic behavior degrades the mechanical work performed by the stresses into heat so that the material exhibits internal friction, which can damp out mechanical oscillations in a material. Anelasticity therefore affects the mechanical properties of materials. As seen below, its study yields unique information about a number of kinetic processes in materials, such as diffusion coefficients, especially at relatively low temperatures. 8.3.1
Anelasticity due to Reorientation of Anisotropic Point Defects
Anelastic behavior can be produced by the stressinduced diffusional jumping of anisotropic point defects. An example of such a process is described in Exercise 8.5, in which an f.c.c. metal contains a concentration of selfinterstitial point defects having the (100) splitdumbbell configuration (see Fig. 8.5d). Each defect produces a tetragonal distortion of the crystal, elongating it preferentially along its dumbbell axis. The three types of sites in the crystal in which the interstitials can lie with their axes along [loo], [ O l O ] , or [OOl] exist in equal numbers and will be occupied equally in the absence of any stress. However, if the crystal is suddenly stressed uniaxially along [loo], an excess of dumbbells will jump to sites where they are aligned along [loo],because the crystal is elongated along the direction of the applied stress and the applied stress performs work. This principle applies to loading along the other cube directions as well. (Note that this is a good example of LeChatelier’s principle.) When the stress is released suddenly, the defects repopulate the sites in equal numbers and the crystal regains its original shape. The relaxation time for this repopulation is 2 r=(8.63) 317 where r is the total jump frequency of a dumbbell (see Exercise 8.5). This process therefore causes the crystal to elongate or to contract in response to the applied
184
CHAPTER 8. DIFFUSION IN CRYSTALS
stress at a rate dependent upon the rate at which the dumbbells jump between the different types of sites. The overall response of the crystal to such a stress cycle is shown in Fig. 8.16. When the stress uo is applied suddenly, the crystal instantaneously undergoes an ideally elastic strain following Eq. 8.62. As the stress is maintained, the crystal undergoes further timedependent strain due to the repopulation of the interstitials. When the stress is released, the ideally elastic strain is recovered instantaneously and the remaining anelastic strain will be recovered in a timedependent fashion as the interstitials regain their random distribution.
t
Stress applied
Stress oo removed
Time, t Figure 8.16: Strain vs. time for an anelastic solid during a stress cycle in which stress is applied suddenly at t = 0, held constant for a period of time, and then suddenly removed.
General Formulation of Anelastic Behavior. Anelastic behavior where the strain is a function of both stress and time may be described by generalizing Eq. 8.62 and expressing the compliance in the more general form
(8.64)
The initial value of the compliance, corresponding to
S(0) = su
(8.65)
is the unrelaxed compliance, which corresponds to ideal elastic behavior because there is no time for pointdefect repopulation. The value of S ( t ) at long times, corresponding to s(m) = SR (8.66)
is the relaxed compliance, since it includes the maximum possible additional strain due to the stressinduced repopulation of the defects. Clearly, SR > Su. Suppose now that the crystal is subjected to a periodic applied stress of amplitude uo corresponding to g = uoeiWt (8.67) The resulting strain is also periodic with the same angular frequency but generally lags behind the stress because time is required for the growth (or decay) of the anelastic strain contributed by the pointdefect repopulation during each cycle. The strain may therefore be written &
= &oei(wt4)
(8.68)
8 3. DIFFUSIONAL ANELASTICITY (INTERNAL FRICTION)
185
where q5 is the phase angle by which the strain lags behind the stress. Note that 4 = 0 at both very high and very low frequencies. At very high frequencies, the cycling is so rapid that the point defects have insufficient time to repopulate and therefore make no contribution to the strain. At very low frequencies, there is sufficient time for the defects to repopulate (relax) at every value of the stress, and the stress and strain are therefore again in phase. To proceed with the more general intermediate case, it is convenient to write the expression for the strain, E
(8.69)
= Ele'wt  i E 2 e i W t
In this formulation, the first term on the righthand side is the component of E that is in phase with the stress, and the second term is the component that lags behind the stress by 90". Also, E2 = t a n 4 (8.70) El
The compliance (again the ratio of strain over stress) is then S(W) =
( ~1 2 ~ 2 eiWt )
uoeiWt
El _ uo
.E2
 1
g o
(8.71)
Because the strain lags behind the stress, the stressstrain curve for each cycle consists of a hysteresis loop, as in Fig. 8.17, and an amount of mechanical work, given by the area enclosed by the hysteresis loop,
AW=
f
ode
(8.72)
will be dissipated (converted to heat) during each cycle. To determine AW, only the part of the strain that is out of phase with the stress must be considered. The stress and strain in Eq. 8.72 can then be represented by u = uocoswt
and
AW =
O,E~L
and
E
= ~2 cos(wt  7r/2)
(8.73)
2W/T
(8.74)
Hysteresis loop shown by the stressstrain curve of an anelastic solid Figure 8.17: subjected to an oscillating stress.
186
CHAPTER 8 DIFFUSION IN CRYSTALS
The energy dissipated can be compared with the maximum elastic strain energy, W ,which is stored in the material during the stress cycle. Because the elastic strain is proportional t o the applied stress, W is equal to just half of the product of the and therefore maximum stress and strain (i.e., W = oo&1/2),
AW
E2
(8.75)
 = 27rW El
AW/W can be measured with a torsion pendulum, in which a specimen in the form of a wire containing the point defects is made the active element and strained periodically in torsion as in Fig. 8.18. If the pendulum is put into free torsional oscillation, its amplitude will slowly decay (damp out), due to the dissipation of energy. As shown in Exercise 8.20, the maximum potential energy (the elastic energy, W )stored in the pendulum is proportional to the square of the amplitude of its oscillation, A. The amplitude of the oscillations therefore decreases according to
where N is the number of the oscillation and it is realistically assumed that AW << W .The logarithmic decay of the amplitude is the logarithmic decrement,designated by 6. Therefore, (8.77) Measurements of 6 yield direct information about the magnitude of the energy dissipation and the phase angle. $ measures the fractional energy loss per cycle due to the anelasticity and is often termed the internal friction. According to the discussion above, 6 will be a function of the frequency, w ;should approach zero at both low and high frequencies; and will have a maximum at some intermediate frequency. The maximum occurs at a frequency that is the reciprocal of the relaxation time for the repopulation of the point defects.
k
Specimen
Figure 8.18:
Torsion pendulum in which the specimen is in the form of a wire subjected
to an oscillating stress.
Analog Model for Standard Anelastic Solid. To find the dependence of 6 on frequency, a model that relates the stress and strain and their time derivatives must
8.3: DIFFUSIONAL ANELASTICITY (INTERNAL FRICTION)
187
be constructed. Figure 8.19’s analog model for a standard anelastic solid serves this purpose; it consists of two linear springs, S1 and S2, and a dashpot, D , which is a plunger immersed in a viscous fluid. The dashpot changes length at a rate proportional to the force exerted on it. This model gives a good account of the anelastic behavior illustrated in Fig. 8.16. When a force, F , is first applied, S2 elongates instantaneously. At the same time, in the upper section of the model, F is fully supported by D and the force on S1 is zero. However, with increasing time, D extends and the force is gradually transferred to S1,which extends under its influence. Eventually, the force is fully transferred, as both S1 and S2 experience the full force while D experiences nothing. At this point, the model reaches its fullest extension. The extension remains constant until F is suddenly removed. S2 then contracts instantaneously and S1 gradually relaxes by forcing D back to its original extension and the model recovers its original state. S2 therefore accounts for the ideal elasticity of the solid, and the combination of S1 and D accounts for the anelasticity. The linear spring element S1 will undergo an extension Axsl according to
Axsl = aslFs1
(8.78)
where Fsl is the force on S1 and as1 is a constant. Similarly for S2,
Also, for the dashpot,
(8.80) where A X D is the extension of D, FD is the force on D , and addit ion,
aD
is a constant. In
A X S= ~ AXD F = F.92
(8.81) (8.82)
(8.83) F
t
F Figure 8.19:
Analog model for a standard anelastic solid.
188
CHAPTER 8: DIFFUSION IN CRYSTALS
Finally, the stress, 0 , and strain, E , may be expressed
and
1 F (8.85) a, where a, and a, are constants. By combining Eqs. 8.788.85, the following equation, which contains three independent constants (bracketed) corresponding to the three elements in the model, can be obtained: o=
Equation 8.86 may be solved for the time period in Fig. 8.16 during which the stress is held constant at uo. Under this condition, it reduces to (8.87) Equation 8.87’s general solution can be written
The constant of integration, A, can be evaluated by recalling that at t = 0 only S2 is extended. The strain is then
~ ( 0=) U ~ A X =S aEas2Fs2 ~ = u , u ~ ~=F~ , ~ s 2 ~ , u , and therefore from Eq. 8.88, A = a,a,asl
E(t)
= a,auas2a,
(8.89)
and
+ a,a,as10,
(1  eaDt’a=
)
(8.90)
Examining the forms of ~ ( 0and ) ~ ( mand ) comparing the results with Eqs. 8.648.66 shows that a,a,asz = Su and a,a,asl = SR  Su. Also, the anelastic relaxation occurs exponentially, in agreement with the results in Exercise 8.5, and the relaxation time corresponds to r = U S ~ / U D . Equation 8.90 then takes the simpler form E ( t ) = suuo (SR SrJ)ao(le+) (8.91)
+
and Eq. 8.86 takes the form
(8.92) Frequency Dependence of the Logarithmic Decrement. The frequency dependence of S can now be found. Putting Eqs. 8.67 and 8.69 into Eq. 8.92 and equating the real and imaginary parts yields two equations which can be solved for ~1 and ~2 in the forms El
= ffo
(su+ 1sR +w2r2
(8.93)
8.3: DIFFUSIONAL ANELASTICITY (INTERNAL FRICTION)
189
(8.94) Therefore, (8.95) Because ( S R Su)<< Su in the majority of cases, (8.96) The decrement 6(w) forms a Debye peak, as shown in Fig. 8.20. The maximum damping (anelasticity) occurs when the applied angular frequency is tuned t o the relaxation time of the anelastic process so that w r = 1. Also, S(w) approaches zero at both high and low frequencies, as anticipated.
0
In cot
Figure 8.20: Curve of the decrement, 6 ( w ) , according to Eq. 8.96, vs. l n u r . The curve exhibits a Debye peak at l n w = 0 (or w = l / ~ ) .
8.3.2
Determination of Diffusivities
The preceding analysis provides a powerful method for determining the diffusivities of species that produce an anelastic relaxation, such as the splitdumbbell interstitial point defects. A torsional pendulum can be used to find the frequency, wp, corresponding to the Debye peak. The relaxation time is then calculated using the relation r = l / w p , and the diffusivity is obtained from the known relationships among the relaxation time, the jump frequency, and the diffusivity. For the splitdumbbell interstitials, the relaxation time is related to the jump frequency by Eq. 8.63, and the expression for the diffusivity (i.e., D = l?a2/12), is derived in Exercise 8.6. Therefore, D = a2/18r. This method has been used to determine the diffusivities of a wide variety of interstitial species, particularly at low temperatures, where the jump frequency is low but still measurable through use of a torsion pendulum. A particularly important example is the determination of the diffusivity of C in b.c.c. Fe, which is taken up in Exercise 8.22. Bibliography 1. S.M. Allen and E.L. Thomas. The Structure of Materials. John Wiley & Sons, New York, 1999. 2. R.A. Johnson. Empirical potentials and their use in calculation of energies of pointdefects in metals. J . Phys. F , 3(2):295321, 1973.
190
CHAPTER 8: DIFFUSION IN CRYSTALS
3. W. Schilling. Selfinterstitial atoms in metals. J . Nucl. Mats., 6970( 12):465489, 1978. 4. P. Shewmon. Diffusion in Solids. The Minerals, Metals and Materials Society, Warrendale, PA, 1989. 5 . G. Neumann. Diffusion mechanisms in metals. In G.E. Murch and D.J. Fischer, editors, Defect and Diffusion Forum, volume 6669, pages 4364, Brookfield, VT, 1990. SciTech Publications.
6. W. Frank, U. Gosele, H. Mehrer, and A. Seeger. Diffusion in silicon and germanium. In G.E. Murch and A.S. Nowick, editors, Diffusion in Crystalline Solids, pages 63142, Orlando, Florida, 1984. Academic Press. 7. T.Y. Tan and U. Gosele. Pointdefects, diffusion processes, and swirl defect formation in silicon. Appl. Phys. A , 37(1):117, 1985.
8. W. Frank. The interplay of solute and selfdiffusionA key for revealing diffusion mechanisms in silicon and germanium. In D. Gupta, H. Jain, and R.W. Siegel, editors, Defect and Diffusion Forum, volume 75, pages 121148, Brookfield, VT, 1991. SciTech Publications. 9. A. Atkinson. Interfacial diffusion. Mat. Res. SOC.Symp., 122:183192, 1988. 10. D. Beshers. Diffusion of interstitial impurities. In Diffusion, pages 209240, Metals Park, OH, 1973. American Society for Metals. 11. L.A. Girifalco. Statistical Physics of Materials. John Wiley & Sons, New York, 1973.
12. A.D. LeClaire and A.B. Lidiard. Correlation effects in diffusion in crystals. Phil. Mag., 1(6):518527, 1956. 13. K. Compaan and Y. Haven. Correlation factors for diffusion in solids. Trans. Faraday SOC.,52:786801, 1956. 14. R.O. Simmons and R.W. Balluffi. Measurements of equilibrium vacancy concentrations in aluminum. Phys. Rev., 117:5261, 1960.
15. A. Seeger. The study of point defects in metals in thermal equilibrium. I. The equilibrium concentration of point defects. Cryst. Lattice Defects, 4:221253, 1973. 16. R.W. Balluffi. Vacancy defect mobilities and binding energies obtained from annealing studies. J . Nucl. Mats., 6970:240263, 1978. 17. W.D. Kingery, H.K. Bowen, and D.R. Uhlmann. Introduction to Ceramics. John Wiley & Sons, New York, 1976. 18. Y.M. Chiang, D. Birnie, and W.D. Kingery. Physical Ceramics. John Wiley & Sons, New York, 1996.
19. D. Halliday and R. Resnick. Fundamentals of Physics. John Wiley & Sons, New York, 1974.
EXERCISES 8.1 It has sometimes been claimed that the observation of a Kirkendall effect implies that the diffusion occurred by a vacancy mechanism. However, a Kirkendall effect can be produced just as well by the interstitialcy mechanism. Explain why this is so. Solution. Substitutional atoms o f type 1 may diffuse more rapidly than atoms of type 2 if they diffuse independently by the interstitialcy mechanism in Fig. 8.4. To sustain the unequal fluxes, interstitialatom defects can be created a t climbing dislocations acting
EXERCISES
191
as interstitial sources in the region richer in 1 and destroyed a t dislocations acting as interstitial sinks in the region poorer in 1. This will cause the region richer in 1 t o contract and the other region t o expand, thereby producing a Kirkendall efFect.
8.2 For copper selfdiffusion by the vacancy mechanism, demonstrate that Eq. 7.14
predicts that the preexponential “attempt” frequency factor is on the order of 1013 s s l . Use a harmonic oneparticle model for the configuration illustrated in Fig. 8.3. For Cu, Young’s modulus is E = 12 x lo1’ MPa, the lattice constant is a = 0.36 nm, the atomic weight is 63.5 g, and the structure is f.c.c. (12 nearestneighbors). 0
Assume a simple ballandspring model in which the atoms are replaced by balls of mass m, which are coupled by nearestneighbor bonds represented by linear springs having a restoring force spring constant, Make reasonable approximations to estimate the restoring force experienced by the atom as it vibrates along its jump path. Remember that in the oneparticle model the environment of the jumping particle remains fixed.
s.
Solution. A value of the spring constant, S, can be obtained by applying a tensile stress, 0 ,t o the ball and spring model along [loo],finding the elastic strain, E , resulting from the stretching o f the springs, and then using the relation u = EE
(8.97)
Each atom in a (200) plane has four nearestneighbors lying in an adjacent (200) plane. The springs connecting it t o these nearestneighbors lie a t 45” with respect t o [loo]. Because there are 2 / a 2 atoms per unit area in a (200) plane, the force stretching each spring along the spring axis due t o the applied stress is a2u
FS = 
(8.98)
Fs ALs = S
(8.99)
4 4
The extension o f each spring is then
and the strain along
[loo]is & =
2fiALs a
(8.100)
Therefore, using Eqs. 8.97,8.98,8.100,and 8.99,
E =  =   2 Fs E
aALs
= al s
(8.101)
and S = a E / 2 = 2.2 x lo3 MPa. The restoring force experienced by an atom vibrating in the direction o f a nearestneighbor vacancy (e.g., atom A in Fig. 8.3)in the oneparticle model can be estimated. Atom A is in a cage o f 11 nearestneighbors. These include atoms 1, 2 , 3, and 4 in the window in the ( l i 0 ) plane on one side, and four atoms (including atoms 5 and 6) in a similar window configuration in the (1TO) plane on the back side o f atom A , atom 9 in the same ( 1 i O ) plane as atom A along with another atom symmetrically disposed on the other side o f A in the direction [ O l l ] , and a final atom behind A along [ O l i ] . Making the oneparticle assumption that the environment of the jumping particle is fixed, simple geometry shows that if the A atom moves toward
192
CHAPTER 8. DIFFUSION IN CRYSTALS
the vacancy by the distance AL, eight springs will change their lengths by AL/2 t o first order when 6L << a, and one spring will stretch by AL. When the forces induced by these changes in spring length are resolved along [ O i l ] , the total restoring force on A is found t o be 3 s AL: the total effective linear restoringforce constant is then p = 3 s . Putting this value into Eq. 7.14 yields v M 0.4 x 1013 s'.
8.3 The selfdiffusivity in an f.c.c. crystal for diffusion by a vacancy mechanism can be written *D = g f a 2 v ,(s~+s:)/k,(H~+H:)/(kT) where g = 1. Find the value of g for selfdiffusion in a b.c.c. crystal. Solution. The diffusion of the atoms will be correlated because o f the vacancy exchange mechanism and, therefore, using Eq. 7.52,
rr2
D=f But
6
r = x;qr
(8.102) (8.103)
where X;q and Tv are the equilibrium atom fraction of vacancies and the vacancy jump rate, respectively. Also, r 2 = (3/4)a2 and r v = 8r;, so that
*D = X;.Pr;a2f
(8.104)
Using Eqs. 8.13 and 8.18,
*D = f a Z v
,(sg+s:)/ke(Hg+H:)/(kT)
(8.105)
and therefore g = 1.
8.4 An interstitial C atom will generally diffuse in b.c.c. Fe by jumping almost
exclusively between nearestneighbor interstitial sites such as sites 1 and 2 in Fig. 8.8b. However, very occasionally it may jump between nextnearestneighbor sites such as 1 and 3. Find an expression for the overall diffusivity of the C atoms, 4 , as a result of both nearestneighbor and nextnearestneighbor jumps. Solution. The diffusion is uncorrelated and therefore
r&
Let and be the frequencies for type 1 + 2 (Atype) and type 1 + 3 (Btype) jumps, respectively, in Fig. 8.8b. Then, because there are four nearestneighbors for Atype jumps and eight nextnearestneighbors for Btype jumps, the frequencies for Atype and Btype jumps are = 4 r a and FB = 8FL, respectively. The meansquare displacement during time 7 is then
(8.107) and Therefore,
(8.109)
EXERCISES
193
The quantities u 2 r ~ / 2 4and U 2 r B / 1 2 may be regarded as the hypothetical difFusivities o f the C atoms if they are allowed t o make only A type and Btype jumps, respectively, and therefore Eq. 8.109 may be written
01= DIA
+ DIB
(8.110)
where DIA and DIB are the two hypothetical diffusivities. In general, DIB
<< DIA.
8.5 As discussed in Section 8.3.1, the (100) splitdumbbell selfinterstitial in the f.c.c. structure can exist with its axis along [loo], [ O l O ] , or [OOl]. Under stress,
certain of these orientation states are preferentially populated due to the tetragonality of the defect as a center of dilation. When the stress is suddenly released, the defects repopulate the available states until the populations in the three states become equal. Show that the relaxation time for this repopulation is r)
'T=
where
r
L
(8.111)
3r is the total jump frequency of a dumbbell.
Derive the differential equation that describes the rate at which [loo] dumbbells convert to [ O l O ] and [OOl] dumbbells, and then solve the equation. Solution. According t o Fig. 8.6, a [loo] dumbbell can j u m p into a neighboring site in eight different ways, four with [OlO] orientations and four with [OOl] orientations. Therefore, dc[100]  ~r/cllOOl + 4r/c[0101+ 4r/cioo11 dt

(8.112)
where I?' is the jump rate into a specific adjacent site, and the are the concentrations in the three orientations. However, the total concentration, ctot, is constant, and therefore Ctot = c[lool + c[olol + c[ooll (8.113) CIS
Combining Eqs. 8.112 and 8.113 yields
(8.114) Integrating and applying the condition t h a t c[lool(t = m) = ctot/3,
(8.115) Because the total j u m p rate is
r = 8r', the relaxation time is 1
2
'T=12r'=F
(8.116)
8.6 It is possible to express the diffusivity of the splitdumbbell selfinterstitial in an f.c.c. crystal (illustrated in Fig. 8.6) in terms of its total jump frequency, I?, and the lattice constant of the crystal, a. Show that the following approaches lead to the same result.
Approach 1: Start with Eq. 8.3.
194
CHAPTER 8 DIFFUSION IN CRYSTALS
Approach 2: Start by determining the net flux between two adjacent (002) planes when the gradient of the interstitial concentration is normal to these planes. Solution. Approach 1: As seen in Fig. 8.6, the j u m p distance for the dumbbell is equal t o the displacement o f its center of mass, a / d . Every neighboring site t o the dumbbell is equally probable for the next jump, so f = 1. Thus,
Approach 2: Alternatively, we can analyze diffusion arising from a gradient of interstitial concentration along [002] in Fig. 8.6. Consider the jumping of interstitials between two adjacent (002) planes. If there are c’ interstitials per unit area with centers of mass on plane A , onethird will have their axes along [loo], onethird along [OlO], and onethird along [OOl]. Each [ O O l ] interstitial on plane A has four sites on an adjacent (002) plane (i.e., plane B ) in which t o jump. Each [loo] interstitial and [OlO] interstitial has two sites in which t o jump. The total concentration o f interstitials per unit volume associated with plane A is c = c’/(a/2) = 2c’/a and the flux from plane A t o plane B is
Expanding c t o first order, the flux from plane B t o plane A is
and the net flux is
2 a 3
2
ac r/dz
Therefore, 01= ( 2 / 3 ) a 2 r ’ . However, the total j u m p rate is
r = 8r’ and
in agreement with the results of Approach 1
8.7 Consider the diffusion of particles along x in a dilute system where no fields are present and there is only a concentration gradient. Under these conditions, the potential energy of the system will vary as shown in Fig. 8.21a when a diffusing particle jumps from a site in a plane at x = xo into an equivalent site in an adjacent plane at x = xo + a. Suppose now that a conservative field is imposed that interacts with the diffusing particles so that the potential energy varies with the position of the jumping particle as shown in Fig. 8.21 b. AU is the increase in the potential energy when a particle advances by one planar spacing and is given by AU = ad$
ds
(8.117)
EXERCISES
195
Figure 8.21: Barrier to atom jumping. (a) No field present. (b) After imposition of a field that interacts with jumping particles.
where 1c, is the potential associated with the imposed field. Obtain an expression for the net flux of particles between planes and show that it will have the form of Eq. 3.48 with the electrical potential, 4, replaced by $. Assume that the barrier to jumping is modified by the field as indicated by Fig. 8.21b and that the quantity AU/2 << kT. Solution. The net forward flux along z between planes can be written as
where A is a constant. Expanding exponentials which involve the powers *AU/(ZkT) t o first order and neglecting higherorder terms yields
(8.119) Finally, identifying aAexp[Uo/(kT)] with D and using Eq. 8.117, J =
Ddc
dx
_ _ kT dx
 DcdlC,
(8.120)
8.8 Calculate the correlation factor for tracer selfdiffusion by the vacancy mech
anism in the twodimensional closepacked lattice illustrated in Fig. 8.22. The tracer atom at site 7 has just exchanged with the vacancy, which is now at let p k be the probability that the tracer will site 6. Following Shewmon [4], make its next jump to its kth nearestneighbor (i.e., a 7 3 k jump). tlk is the angle between the initial 6 + 7 jump and the 7 + k jump. The average of the cosines of the angles between successive tracer jumps is then z
(cos 6 ) =
k= 1
p k COS e k
(8.121)
and f is given by Eq. 8.29. The quantity p k can be expressed in the form (8.122)
196
CHAPTER 8: DIFFUSION IN CRYSTALS
where Pi = ( l / ~is)the ~ probability that the vacancy on its ith jump will make a k + 7 jump (thereby producing a 7 + k tracer jump) for the first time. n i k is the number of different paths that will allow the vacancy to accomplish this, and z = 6 is the number of nearestneighbors. Calculate p k , (cos e), and f if all vacancy trajectories longer than four jumps are neglected.
Figure 8.22: Twodimensional closepacked lattice. The tracer atom at 7 has just exchanged with the vacancy at 6. Solution. First evaluate the n , k in Eq. 8.122. Consider k = 6 first. For i = 1, the only possibility is a direct 6 + 7 jump. Therefore, 7216 = 1. For i = 2, no possible paths exist, so 7226 = 0. For i = 3, there are five paths, so 7236 = 5. For i = 4, there are eight paths, so 7246 = 8. Similar inspections produce the results shown in Table 8.1 for k = 5 , 4 , and 3. Note that by symmetry the results will be the same for k = 1 and k = 5 and for k = 2 and k = 4, respectively. Putting these results into Eq. 8.122,
(8.123)
Table 8.1: Values of n i k in Eq. 8.122
6 5 4 3
1 0 0 0
0
1 0 0
5 1 1 0
8 11 2 2
197
EXERCISES
Substituting these values into Eq. 8.121 yields
(cosej = 0.1960 (1)
+ 0.0409
= 0.2293
Finally,
(8.124) When all relevant trajectories including those beyond i = 4 are taken into account, the true value of f is 0.560 [13]. The truncation at i = 4 therefore causes f t o be overestimated by about 12%.
8.9 Consider the diffusion of a randomly walking diffusant in the h.c.p. structure, which is composed of closepacked basal planes stacked in the sequence A B A B A . . . The lattice constants are a and c. The probability of a firstnearestneighbor jump within a basal plane (jump distance = a ) is p , and the probability of a jump between basal planes (jump distance = is 1  p . If axes 5 1 and x2 are located in a basal plane, derive the following expressions for the diffusivities Dll and 0 3 3 :
d
m
)
(8.125) (8.126) where N , is the total number of jumps in time, 7 . Note that we have employed a principal coordinate system in which the diffusivity tensor is given by Eq. 4.66. Solution. W e will determine the Di, by the general method used t o obtain Eq. 8.11. According t o Eq. 4.66, the diffusion is isotropic in directions perpendicular t o 2 3 . We parallel t o 21 across the C D plane illustrated shall therefore determine the net flux, Pet, in Fig. 8.23.
Here, ni is the concentration on plane i, I?; is the j u m p frequency from one site t o a is the jump frequency from a site in single neighboring site in the basal plane, and
Figure 8.23: View of h.c.p. structure looking along 23. Open circles lie in the A plane; X's lie in the B plane.
198
CHAPTER 8. DIFFUSION IN CRYSTALS
a basal plane t o a single neighboring site in an adjacent basal plane. Therefore,
pet= J ( + )

J(t) =
3 a' o ( 2
~ 2
+
n 3 ) &(nz
+ r;(nl 2
T Z ~ )
0 .
7
~
(8.129) )
~
Making the usual Taylor expansions for the concentration differences yields
Now
(8.131) where rois the total j u m p frequency for jumping in the basal plane and I?, is the total j u m p frequency for jumping between basal planes. Using Eqs. 8.130 and 8.131,
(8.132) The difFusivity 0 3 3 is obtained by analyzing the net flux parallel t o two adjacent basal planes, A and B . In this case, Jnet
= J(*)
 J ( C ) = TZACr, 3 /
2
Using a Taylor expansion t o evaluate
3 2
 TZBCrL
( T Z A T Z B and )
=
'Crk(TZA
2
2 3
passing between
nB)
(8.133)
employing Eq. 8.131,
(8.134)
8.10 Show that the results obtained in Exercise 8.9 (i.e., Eqs. 8.125 and 8.126), can be obtained in a simpler way by using Eq. 7.53 in one dimension if ( R 2 )is taken as the mean value of the squares of the jump vector components along the chosen direction. Solution. For difFusion along axis
21
in Fig. 8.23, Eq. 7.53 is written
(8.135) where ( r f )is the mean square of the jump vector components along axis 1:
(8.136) Putting Eq. 8.136 into Eq. 8.135 and using the relation
r = NT/r, (8.137)
Using the same method for diffusion along 2 3 yields
(8.138) and
(8.139)
199
EXERCISES
8.11 Exercise 7.4 demonstrated that the meansquare displacement during random threedimensional diffusion in a primitive orthorhombic crystal is equal to the sum of the meansquare displacements achieved during onedimensional diffusion along each of the three coordinate axes.
Demonstrate this result for the diffusion of a randomly walking diffusant in an h.c.p. crystal using the information and results in Exercises 8.9 and 8.10. Solution. Using the same procedure as in Exercise 7.4,
and the meansquare displacement is then
= 20117
+ 2Dll.r + 2 0 3 3 7
B u t according t o Eq. 7.31, Because ( r ' ) = a 2 p
(R')= N(T')
(8.142)
+ (1  p)(a2/3) + (1  p)c2/4,
Substituting Eqs. 8.125 and 8.126 into Eq. 8.143 yields the relation
( R 2 )= 20117
+ 20117 + 20337
(8.144)
which is consistent with Eq. 8.141.
8.12 Exercise 7.5 shows explicitly for a random walker on a primitivecubic lattice that the mean values of the cosOi,i+j terms in Eq. 7.49 sum to zero and, therefore, that f = 1. Use Eq. 8.29 to demonstrate the same result. Solution. First evaluate (cosQ). Possible values of cosQ are 1, 1,O,O,O, of which occur with equal probability. Therefore, ( C O S Q ) = 0 and
f =
1  (COSQ) =1 1 (cos 0)
and 0, all
(8.145)
+
8.13 Using Eq. 7.52, calculate an expression for selfdiffusivity by the vacancy mechanism in a primitive cubic lattice. Suppose that the backjump probabili t y (i.e., an atom returns to the site from which it jumped previously) is p . Consider firstneighbor jumps only.
Evaluate the case p = 0 and compare it to an uncorrelated random walk. Solution. There are six firstneighbor sites in the primitive cubic lattice, and the firstneighbor j u m p distance, T , is equal t o the lattice constant, a. Once an atom has jumped into a given site, the probability that it will next jump into any o f i t s nearestneighbor sites (with the exception of the site from which it just jumped) is (1 p)/5. Therefore,
U
"
"
200
CHAPTER 8 DIFFUSION IN CRYSTALS
and using Eq. 8.29,
+
The selfdiffusivity is then
f = 1 (case)  3(i  p ) 1  (case) 2 3p
(8.147)
* D =  r(2)f =  ra2 1  p 2 2+3p
(8.148)
+
In the random case when p = 1/6,f = 1. In the most correlated case when p = 1, f = 0. When p = 0 and the atom cannot j u m p backward t o erase i t s previous jump, f = 3/2 and diffusion is enhanced relative t o the random, uncorrelated case.
8.14 A computer simulation of diffusion via the vacancy mechanism is performed on a square lattice of screen pixels with a spacing of a = 0.5 mm. The computer performs the calculations so that the vacancy jumps at a constant rate of r = ~ O O O S  ~ .The simulation cell is a square of edge length 5 cm containing 10,000 pixels. There is just one vacancy in the simulation cell: and as it moves by nearestneighbor jumps, it remains within the cell (by using periodic boundary conditions or reflection at the borders). (a) Estimate the vacancy diffusion coeficient in this simulation if the vacancy moves by a random walk.
(b) One tracer atom, represented by a specially marked pixel, is initially located at the center of the simulation cell. The vacancy is introduced in the cell at a random location and then moves by a random walk. Estimate the value of the tracer diffusion coeficient in this simulation. ( c ) Estimate the average time for the tracer atom to move from the center of the cell t o the cell border. Solution. (a) Diffusion o f a vacancy in a lattice is uncorrelated, so f = 1. The vacancy diffusivity DV for this twodimensional diffusion is
rr' D v = f 4
rr2 1000 s' 0.5' mm2 = = = 6.25 x 4 4
m2 s'
(b) Selfdiffusion of a tracer by vacancy exchange is correlated, so in this square lattice we have f E ( 2  l ) / ( z 1) % 0.6.The tracer selfdiffusivity *D is
+
= 6.25 x
rn's'
x
x 0.6 = 3.8 x lo'
m's'
(c) A very simple estimate can be made by using the relation (R') = 4 *Dt and taking R E 2.5 cm. This gives
tE
(R') = 4*D
(2.5cm)' = 4.1 x 104 4 x 3.8 x lo' rn2sl
which is probably an overestimate. The time required is the average time for the tracer atom t o first hit the wall. Also, depending on where along the wall the tracer first hits, the path will be somewhat longer because o f the square shape of
EXERCISES
201
the simulation cell. Nevertheless, this method gives an estimate. A more accurate value could be determined most easily by doing a computer simulation and keeping statistics on the times for the tracer t o "hit the wall."
8.15 Schottky defects form at equilibrium in stoichiometric ZrO2. Show that the equilibrium site fraction of anion vacancies is given by
Solution. First write the Schottky reaction: I,,,
null = V,,
+ 2Vg0
(8.149)
The corresponding massaction equilibrium equation for this reaction is
(8.150) where Gfs is the free energy of formation o f a Schottky defect, which in this case consists o f a cation vacancy and two anion vacancies. Then, charge neutrality requires that
2[v;:'] = [VO"]
(8.151)
Substituting Eq. 8.151 into Eq. 8.150 yields
8.16 Schottky defects are the predominant equilibrium point defects in stoichiometric zirconia ZrO2 (see Exercise 8.15). Suppose that the soluble oxide Ta2O5 is added to ZrO2. Assume that cation vacancies form without the formation of any interstitial defects.
(a) Find an expression for the equilibrium cation vacancy site fraction that will form. (b) Discuss how the selfdiffusion of the cations will be affected by the addition of Ta2O5. Solution. (a) When two units of Tan05 are added t o ZrOz, four Ta ions will be put into four existing Zr sites. The four displaced Zr ions will be put into four new normal Zr cation sites. The ten incoming 0 ions will be put into new normal 0 sites, and one Zr ion will be removed from its existing site and placed in a new normal Zr site, thereby creating a cation vacancy. This process preserves electrical neutrality and may be expressed
2Ta205
' 3 100; + 4Ta;, + VLy
(8.153)
In addition t o this reaction, V&"and VG*defects will be produced by the Schottky reaction (Eq. 8.149), and the massaction equilibrium in Eq. 8.150 will hold. The condition for electrical neutrality may be obtained by realizing that the introduction o f 1 unit of Ta;, produces 1 / 4 unit of VLy'. Also, for every unit o f VGoformed,
202
CHAPTER 8: DIFFUSION IN CRYSTALS
1/2 unit of VLf’ is produced. Therefore, the chargebalanced site fraction of V i r must be 1 1
+ 5 [Vi?]
[Vd:”] = 4 [Ta&]
(8.154)
Combining Eq. 8.154 and Eq. 8.150 yields
(8.155) (b) The selfdiffusivity on the cation sublattice will be proportional to the cation vacancy site fraction, [VA:’]. At high temperatures, the numbers of anion and cation vacancies produced by the Schottkypair reaction will be much larger than the number of Tai, defects, so that
[VL;’] =
1 [VG’] >> [Tai,] 2
Therefore, from Eq. 8.155,
(8.156) At low temperatures, the site fraction of cation vacancies due t o Schottkypair formation will be negligible and their site fraction will therefore be fixed a t the level 1
[V&”] = 4 [Tal,]
An Arrhenius plot of the cation selfdiffusivity will then possess two linear regions. H ” ) / k ; in In the hightemperature intrinsic regime, the slope will be (Hsf/3 the lowtemperature extrinsic regime, the slope will be simply H ” / k , where H“ is the migration enthalpy of a cation vacancy.
+
8.17 ZrOn can be made 0 deficient in a sufficiently reducing atmosphere. Show that the oxygen anion vacancy site fraction increases with a decrease in the oxygen pressure in the atmosphere according to
Show that the selfdiffusivity on the anion (oxygen) sublattice, *Do, increases with decreasing oxygen pressure (at constant temperature) according to 1 
PA;,
varies with temperature (at constant oxygen pressure) according to e(AG13+Gr)I(w
where AG is the freeenergy change due to the reduction reaction and GP is the free energy of migration of an oxygen anion vacancy.
EXERCISES
203
Solution. (a) The reduction reaction involves removing an 02 anion from the structure and transferring two electrons from it t o two Zr4+ cations. This makes two Zr3+ cations, a neutral 0 atom, and a cation vacancy Vt;. Therefore, the reaction can be written 1 2Zr,Xr 0; = 2Zrkr V r  0 2 2 and for this reaction,
+
The neutrality condition is
+
+
[Zrk,] = 2 [Vy]
Therefore, combining these equations,
(b) Because *Do is proportional t o Vt;, *DO
o: ,  A G / ( a k T )
a t constant T. Because *Do is proportional t o Vt; and also t o the Boltzmann factor exp[GT /(kT)],
8.18 Consider an oxygendeficient oxide M02z containing a low concentration of solute A;, due to the addition of the soluble oxide AO. Oxygen diffusion occurs by a vacancy mechanism. Assume that all oxygen vacancies are doubly ionized. (a) Write the reduction reaction for reducing MOzPz and a corresponding equation for its equilibrium constant, Keq.
(b) Write a defect reaction for the incorporation of the solute A into MOa. ( c ) Write the charge neutrality condition for the impure, nonstoichiometric oxide. (d) How would Po, qualitatively affect the selfdiffusivity of oxygen on the anion sublattice, *Dol in the intrinsic and extrinsic regimes? Solution. (a) The reduction occurs by removing one 0 ion and transferring two electrons from it t o two M ions, creating two [ M h ] defects and one [V$*] defect and one free 0 atom. This reaction may be written 2MG A t equilibrium,
+ 0; = 2Mh + VG* + 210 2
[ M ~ I ~ [ V $ * ] P=; K ~ e~q = e  A G / ( k T )
(8.157) (8.158)
204
CHAPTER 8 DIFFUSION IN CRYSTALS
(b) When A 0 is added, A is added a t a new M site and 0 goes t o a new 0 site. This creates one A& defect. To maintain electrical neutrality, an 0 ion is removed from an 0 site and placed in a new 0 site, thereby creating a V$* defect. The reaction may be written as
+ V*: + 0:
A 0 = A;
(8.159)
(c) Overall charge neutrality requires that
1
[VG*] = 5 [ M L ]
+ [A:]
(8.160)
(d) The massaction law given by Eq. 8.158 will hold and, therefore, putting the neutrality condition given by Eq. 8.160 into Eq. 8.158,
(8.161) A t high temperatures, [V;"] is entirely due t o the reduction process and [V,"] [A&]. Therefore, in this intrinsic regime,
>>
(8.162) Because *Do is proportional t o [VG*],*Do cx contribution of the reduction process t o [V,"] becomes constant a t the value
PO,^/^.
A t low temperatures, the is essentially negligible and [Vz*]
[VG*] = [A;] which is determined by the amount of solute A 0 that has been added. In this extrinsic regime, *Do is therefore independent of P o z .
8.19 The relationship between the intrinsic diffusivity, D1 , of charged interstitial ions in an ionic solid and the ionic electrical conductivity, p, due to the motion of these ions in the absence of a significant concentration gradient is given by Eq. 3.50; that is,
Suppose that an ionic solid contains charged cation vacancies such as NaCl containing Na' vacancies. Find a relationship, comparable to Eq. 3.50, beand the electrical tween the cation tracer selfdiffusion coefficient, *Dcation, conductivity, p, due to voltageinduced motion of the cations. Solution. In this case, the charged cation vacancies, possessing a diffusivity DVtion, will respond t o the voltage just as the charged interstitials did in Section 3.2.1. The relationship between DVtionand p will then be given by the same type of relation as Eq. 3.50; that is, DVtion cv q$ (8.163)
'= kT where cv is the cation vacancy concentration and qv the charge carried by the vacancy. , will be related t o the O n the other hand, the cation tracer selfdiffusivity, *Dcation cation vacancy concentration by a relationship similar t o Eq. 8.17:
*Dcation = ~
~ ~ c $ t i o n f
(8.164)
EXERCISES
205
where X V is the fraction o f cation sites occupied by the vacancies and f is the correlation factor for the operative vacancy exchange mechanism. Combining Eqs. 8.163 and 8.164 and setting ccationequal t o the number o f cation sites per unit volume,
(8.165) Note that independent measurements of p and *Pation will yield information about f , because the other factors in Eq. 8.165 are known.
8.20 Show that the maximum potential energy stored in a torsion pendulum is
proportional to the square of the amplitude of its oscillation. Solution. The restoring torque for a torsion pendulum is k0, where 0 is the angle o f rotation (see Fig. 8.18) and k is the torsion constant. The equation of motion [19] is then where
I
rc d20 _  0 I dt2
(8.166)
is the moment o f inertia. Equation 8.166’s solution is
0 = Omax cos(wt
+ @)
(8.167)
The stored energy is a maximum when 0 = Omax and is therefore
(8.168)
8.21 Figure 8.17 shows a hysteresis loop for an anelastic solid subjected to an
oscillating stress. If the amplitude of the stress is hysteresis loop: (a) When w r
go,
find the shape of the
<< 1
(b) When W I T>> 1 ( c ) When W T = 1 Specify the direction in which the loop is traversed with increasing time, the width of the loop at r~ = 0, and the slope of the dashed line in Fig. 8.17. Express your answer in terms of o o ,S R , and S U . Solution. B y using Eqs. 8.678.69 and constructing the diagram for plane,
E2 tan4 = 
sin@= E2
El
C O S = ~
€0
El €0
E
in the complex
(8.169)
Also, using the real parts of u and E yields
u = u o coswt E
= E~ cos(wt  4) = E~ (cos wt cos @
+ sin w t sin 4)
(8.170)
When u = u o ,coswt = 1 and sinwt = 0. Therefore, E = E~ cos@= E I and the slope of the dashed line is u o / ~ When l. u = 0, coswt = 0, and sinwt = 1, E = E~ sin@= ~ 2 Also, when u = 0, coswt = 0, and sinwt = 1, E =  E ~sin4 =  4 2 .
(a) When w t
<< 1, use o f
Eqs. 8.93 and 8.94 shows that €1
=S
R and ~ ~€2 = 0
(8.171)
.
206
CHAPTER 8. DIFFUSION IN CRYSTALS
The hysteresis loop will therefore appear as a line o f negligible width and slope 1/SR as in Fig. 8.24a. Negligible internal friction therefore occurs. U
Figure 8.24: ( c )W T = 1.
U
U
Frequency dependence of anelastic behavior. (a)w~ << 1. (b)W T >> 1.
(b) When w t >> 1,
EI
= Suu0 and
€2
=O
(8.172)
The hysteresis loop will therefore appear again as a line of negligible width but with a larger slope, as in Fig. 8.246. Negligible internal friction occurs.
( c ) When w t = 1,
+
SR SU SR  SU and E Z = ~ u , (8.173) = 2uo The hysteresis loop will therefore appear as in Fig. 8 . 2 4 ~ .The slope of the dashed line is 1 u o (8.174)
_El
(SRfSU)/2
and the width of the loop a t u = 0 is 2EZ
= ( S R s U ) U o
(8.175)
Also, because the strain lags behind the stress, the direction of traversal of the loop must be as indicated. In this situation, maximum internal friction occurs.
8.22 Describe in detail how to determine the diffusivity of C in b.c.c. Fe using a torsion pendulum. Include all of the necessary equations.
See Section 8.3.1 and Fig. 8.8, where C atoms in sites 1, 2, and 3 expand the crystal preferentially along z, y, and z , respectively. Solution. Using a torsion pendulum, find the anelastic relaxation time, T , by measuring T 1. Having T , the the frequency o f the Debye peak, u p ,and applying the relation W ~ = relationship between T and the C atom jump frequency is found by using the procedure t o find this relationship for the splitdumbbell interstitial point defects in Exercise 8.5. Assume the stress cycle shown in Fig. 8.16 and consider the anelastic relaxation that occurs just after the stress is removed. A C atom in a type 1 site can jump into two possible nearestneighbor type 2 sites or two possible type 3 sites. Therefore,
r
dcl = 4r/cl
dt
Because c1
+ 2r’c2 + 2 r / c 3
(8.176)
+ c2 + c3 = ctot = constant, (8.177)
EXERCISES
which may be integrated t o obtain
[
[
c;] c;] c i ( t )   = ~ ( 0 ) = e
6r’t
207
(8.178)
The relaxation time is then T = 1/(6l?), and because the total jump frequency is According t o Eq. 7.52, D Z= r r 2 / 6 because f = 1, and because r = a / 2 , D I = ra2/24. Substituting for
r = 4l?, T = 2/(3r).
r,
(8.179) Finally, insert the experimentally determined value o f T into Eq. 8.179 t o obtain D I
8.23 Under equilibrium conditions in a stressed b.c.c. Fe crystal, interstitial C
atoms are generally unequally distributed among the three types of sites identified in Fig. 8.8b. This occurs because the C atoms in sites 1, 2, and 3 in Fig. 8.8b expand the crystal preferentially along the 2, y, and z directions, respectively. These directions are oriented differently in the stress field, and the C atoms in the various types of sites therefore have different interaction energies with the stress field. In the absence of applied stress, this effect does not exist and all sites are populated equally. In Exercise 8.22 it was shown that when the stress on an equilibrated specimen is suddenly released, the relaxation time for the nonuniformly distributed C atoms to achieve a random distribution, T , is T = 2/(3r), where r is the total jump frequency of a C atom in the unstressed crystal. Show that when stress is suddenly applied to an unstressed crystal, the relaxation time for the randomly distributed C atoms to assume the nonrandom distribution characteristic of the stressed state is again T = 2/(3r). Assume the energylevel system for the specimen shown in Fig. 8.25. Write the kinetic equations for the rates of change of the concentrations of the interstitials in the various types of sites and solve them subject to the appropriate initial and final conditions. Assume that the barriers to the jumping interstitials shown in Fig. 8.25 are distorted by the differences in the site energies (indicated in Fig. 8.21).
Figure 8.25: Energylevel diagram for a stressed b.c.c. specimen containing an interstitial atom in sites 1, 2, or 3 illustrated in Fig. 8.8.
Solution. Let c1, c2, and c3 be the concentrations of interstitials occupying sites of types 1, 2, and 3, respectively. Also, c1 +c2 +c3 = ctot = constant. Since an interstitial
208
CHAPTER 8: DIFFUSION IN CRYSTALS
in a given type of site can jump into two sites of each other type,
dci =  2 ( r L + rL3+ r L ) c1 + 2 (rL1 r L )c2 + 2r’3+1~t0t dt dc2 =  2 (rL1 + rL3+ rL2)c2 + 2 ( r L  r;,2) dt
c1
+ 2r$2~tot
(8.180)
If the barrier t o the j u m p o f an interstitial between two sites of differing energy is deformed as indicated in Fig. 8.21, the information given in Fig. 8.25 may be used t o derive expressions for the various j u m p rates that appear in the coefficients of Eq. 8.180. Neglecting small differences in the entropies o f activation in the presence and absence of stress, and expanding Boltzmann factors of the form exp[U,,,/(kT)] t o first order so t h a t exp[U,,/(kT)] = 1 U t  J / ( k T ) ,
+
r;,3
w) + w)
r;2 = r’ (1 = r’ (1  h = r’ (1 2kT ) = r/ (1 
2kT

h) r;,, 2kT
r;+l = r’ (1 + WJ = r’ (1 + *) r L l = r’ (1 +
w)
(8.181)
where I?’ is the j u m p rate between any two adjacent sites in the absence of stress. Equation 8.180 is a pair o f simultaneous linear firstorder equations with constant coefFicients. The initial and final conditions are Cl(0) = c2(0) =
Ctot 
c1 (m) = ci‘
3
c2(m)
= qc;
(8.182)
where el(..) and c2(m) are the final equilibrium concentrations reached a t long times in the presence of the applied stress. In view of the symmetry of Eqs. 8.180, we try Cl(t)
=
(f ‘p> 
ek‘t
+
.;‘
c2(t) =
(f
 c;~) e“lt
+ c‘lq
(8.183)
which satisfy the conditions in Eq. 8.182. Direct substitution shows that Eqs. 8.183 indeed satisfy Eqs. 8.180 when higherorder terms involving products of the small quantities U t  j / ( k T ) are neglected and
k‘ = 6r’ c‘lq =
 I++)Ul2 3
(
1
3kT
2u1+2 3kT
u 1 3
3kT
+
(8.184)
3kT
This shows that relaxation t o the equilibrium distribution occurs exponentially with a relaxation time T = 1/(6r’). Since = 4r’,where r is the total jump frequency in the unstressed crystal, 7 = 2 / ( 3 r ) . Finally, the equilibrium concentrations obtained in Eqs. 8.184 from the kinetic equations agree with those obtained using equilibrium statistical mechanics. In the threelevel system in Fig. 8.25, the occupation probability for level 1 is
Since c1 = ctotpl, the result for CI is the same as that given by Eq. 8.184. Similar agreement is obtained for c2.
CHAPTER 9
DIFFUSION ALONG CRYSTAL IMPERFECTIONS
Experiments demonstrate that along crystal imperfections such as dislocations, internal interfaces, and free surfaces, diffusion rates can be orders of magnitude faster than in crystals containing only point defects. These line and planar defects provide shortcircuit diffusionpaths, analogous to highconductivity paths in electrical systems. Shortcircuit diffusion paths can provide the dominant contribution to diffusion in a crystalline material under conditions described in this chapter.
9.1 T H E DIFFUSION SPECTRUM IN IMPERFECT CRYSTALS Rapid diffusion along line and planar crystal imperfections occurs in a thin region centered on the defect core. For a dislocation, the region is cylindrical, roughly two interatomic distances in diameter, and includes the “bad material” in the dislocation core.’ For a grain boundary, the region is a thin slab, roughly two interatomic distances thick, including the bad material in the grain boundary core. For a free surface, this region is the first few atomic layers of the material at the surface. These regions are very thin in comparison to the usual diffusional transport distances. To model the diffusion due to these imperfections, we replace them by thin slabs or cylinders of effective thickness, 6,possessing effective diffusivities which are much larger than the diffusivity in the adjoining crystalline material. Table 9.1 lists the Bad material is disordered material in which the regular atomic structure characteristic of the crystalline state no longer exists. Good bulk material is free of line or planar imperfections. Kinetics of Materials. By Robert W . Balluffi, Samuel M. Allen, and W . Craig Carter. Copyright @ 2005 John Wiley & Sons, Inc.
209
210
CHAPTER 9 DIFFUSION ALONG CRYSTAL IMPERFECTIONS
Table 9.1:
Notation for Shortcircuit Diffusivities
D D(undissoc)
diffusivity along an undissociated dislocation core (i.e., a cylinder, or a “pipe” of diameter, 6)
D D(dissoc)
diffusivity along a dissociated dislocation core (i.e., a cylinder, or a “pipe” of diameter, 6)
DB
diffusivity along a grain boundary (i.e., a slab of thickness, 6)
DS
diffusivity along a free surface (i.e., a slab of thickness, 6)
DXL DL
diffusivity in a bulk crystal free of line or planar imperfections diffusivity in a liquid
notation to be used to describe the diffusivities in various regions of crystalline materials containing line and planar imperfections. Figure 9.1 presents selfdiffusivity data for *DD(dissoc), *DD(undissoc), *DB, *Ds, * D x L , and *DL,for f.c.c. metals on a single Arrhenius plot. With the exception of the surface diffusion data, the data are represented by ideal straightline Arrhenius plots, which would be realistic if the various activation energies were constants (independent of temperature). However, the data are not sufficiently accurate or extensive to rule out some possible curvature, at least for the grain boundary and dislocation curves, as discussed in Section 9.2.3. Dislocations, grain boundaries, and surfaces can possess widely differing structures, and these structural variations affect their diffusivities to significant degrees. If the defective core region is less dense or “looser” than defectfree material, or if a defect possesses structurally “open” channels in its core structure, transport will generally be more rapid along the defect, particularly in the open directions. Some grain boundary structures can be represented by dislocation arrays, and their boundary diffusivity can be modeled in terms of transport along the grainboundary
0.6 0.8 1.0 1.2 1.4 1.6 1.8 2.0
Reduced temperature, T,,, lT Figure 9.1: Master Arrhenius plot of *DxL, *DD(dissoc),*D”(undissoc), *DB, *Ds, and *DL characteristic of f.c.c. metals. Data for various f.c.c. metals have been normalized by using a reduced reciprocal temperature scale, (l/T)/(l/Tm) = T,/T. All diffusivities were derived from experimental data by assuming that all 6 = 0.5 nm. From Gjostein [I].
9.1: THE DIFFUSION SPECTRUM
211
dislocation cores. General grain boundary structures cannot support discrete localized dislocations but, nevertheless, still act as shortcircuit diffusion paths. Shortcircuit diffusion along grain boundaries has been studied extensively via experiments and modeling. Because diffusion along dislocations and crystal surfaces is comparatively less well characterized, particular attention is paid to grainboundary transport in this chapter. However, briefer discussions of diffusion along dislocations and free surfaces are also presented. To describe the effects of grainboundary structure on boundary diffusion, it is necessary to review briefly some important aspects of boundary structure. Additional details appear in Appendix B. It takes a minimum of five geometric parameters to define a crystalline interface. Three describe the crystal/crystal misorientation: e.g., two to specify the axis about which one crystal is rotated with respect to the other, and one for the rotation angle. The remaining two parameters define the inclination of the plane along which the crystals abut at the interface.2 If the interface is a free surface, just two parameters are required to specify the surface's inclination (unit normal). Crystal symmetries determine special values of the parameters at which the interfacial energies take on extreme values. Depending on the specific nature of a system with interfaces, some of the parameters may be constrained and others free to vary as the system seeks a lowerenergy state. Smallangle grain boundaries have crystal misorientations less than about 15" and consist of regular arrays of discrete dislocations (Le., where the cores are separated by regions of defectfree material). As the crystal misorientation across the boundary increases beyond about 15", the dislocation spacing becomes so small that the cores overlap and the boundary becomes a continuous slab of bad material; these are called largeangle boundaries. Largeangle boundaries can be further classified into singular boundaries, vicinal boundaries, and general b ~ u n d a r i e s . ~ An interface is regarded as singular with respect to a degree of freedom if it is at a local minimum in energy with respect to changes in that degree of freedom. It is therefore stable against changes in that degree of freedom. A vicinal interface is an interface that deviates from being singular by a relatively small variation of one or more of its geometric parameters from their singularinterface values. A vicinal interface can therefore minimize its energy by adopting a fitmisfit structure consisting of patches of the nearby minimumenergy singular interface delineated by arrays of discrete interfacial dislocations or steps as illustrated in Figs. B.4 and B.9. These line defects serve to accommodate the relatively small deviations of the vicinal interfaces from the singular interfaces. A general interface is not energyminimized with respect to any of its degrees of freedom, and is far from any singularinterface values of the parameters that set its degrees of freedom. Such an interface cannot reduce its energy by adopting a fitmisfit structure (as in the vicinal case) and therefore cannot support localized dislocations or steps. Two examples serve to clarify these distinctions: Example 1 The tilt grain boundary in Fig. B.4a is singular with respect to its tilt angle.4 The boundary in Fig. B.4c is vicinal to the singular boundary 2Additional variables may be required, such as three that specify a relative translation of one crystal with respect to the other. 3Similar terminology is used for classification of freesurface structure. 4See Appendix B for descriptions of tilt, twist, and mixed grain boundaries.
212
CHAPTER 9: DIFFUSION ALONG CRYSTAL IMPERFECTIONS
with respect to its tilt angle. It consists of patches of the singular boundary delineated by dislocations that accommodate the change in tilt angle.
Example 2 A surface corresponding to the patch of lightcolored atoms in Fig. B.l is singular with respect to its inclination about an axis parallel to the surface steps in the figure. The stepped surface in Fig. B.l is vicinal to such a flat surface and consists of patches of the flat surface delineated by steps that accommodate the change in surface inclination. Because the structure of general largeangle grain boundaries is usually less regular and rigid than that of singular or vicinal boundaries, its activation energies for diffusion are typically lower and the diffusivities correspondingly higher. The diffusion rate along smallangle grain boundaries is generally lower than along largeangle grain boundaries and, indeed, approaches D x L as the crystal misorientation approaches zero. This is due t o two factors: first, the diffusion rate along the bad material in dislocation cores is about the same as, or lower than, that along largeangle grain boundary cores (see Fig. 9.1); second, because smallangle grain boundaries consist of periodic arrays of lattice dislocations at discrete spacings that approach infinity as the crystal misorientation approaches zero, the density of fastdiffusion paths is smaller in smallangle boundaries than in largeangle boundaries. Figure 9.2 presents diffusivity data for a series of tilt boundaries as a function of the misorientation tilt angle. The structures of these boundaries vary considerably as the misorientation changes. In the central part of the plot, the minima occur at crystal misorientations (values of Q) corresponding to singular and vicinal boundaries. The ends of the plot (where the crystal misorientation approaches zero) correspond to smallangle boundaries, and the diffusivities are correspondingly low. The regions centered around the maxima in Fig. 9.2 correspond to general grain boundaries. Polycrystalline materials not subjected to special processing conditions possess mainly general boundaries; the grainboundary data in Fig. 9.1 are for general boundaries that have fairly similar diffusivities and can therefore be described reasonably well by average normalized values.
s 4 / ;; I \

N 0
0
I
\
I
X
I
11
I
4
60
120
6 (degrees)
180
Figure 9.2: Grainboundary diffusivity of Zn along the tilt axes of (1101 symmetric tilt grain boundaries in A1 as a function of tilt angle, 8. From Interfaces in Cvystalline Materials by A.P. Sutton and R.W. Balluffi (1995). Reprinted by permission o f Oxford University Press. Data from I. Herbeuval and M. Biscondi [2].
9.1:THE DIFFUSION SPECTRUM
213
The wide range of diffusivity magnitudes evident in the diffusivity spectrum in Fig. 9.1 may be expected intuitively; as the atomic environment for jumping becomes progressively less free, the jump rates, r, decrease accordingly in the sequence rS > rB x rD(undissoc) > rD(dissoc) > rXL.The activation energies for these diffusion processes consistently follow the reverse behavior,
E S < E B FZ ED(undissoc) < ED(dissoc) < E x L
(9.1)
The diffusivity in free surfaces is larger than that in general grain boundaries, which is about the same as that in undissociated dislocations. Furthermore, the diffusivity in undissociated dislocations is greater than that in dissociated dislocations, which is greater than that in the c r y ~ t a l : ~
*Ds > *DB M *DD(undissoc) > *DD(dissoc) > *DxL
(94
Freesurface and grainboundary diffusivities in metals at 0.5Tm are seven to eight orders of magnitude larger than crystal diffusivities. Provided that defects are present at sufficiently high densities, significant amounts of mass transport can occur in crystals at 0.5Tmvia surface and grainboundary diffusion even though the crosssectional area through which the diffusional flux occurs is relatively very small. As the temperature is lowered further, the ratio of diffusivities becomes larger and shortcircuit diffusion assumes even greater importance. Generally, similar behavior is found in ionically bonded crystals, as shown in Fig. 9.3. 1 2 N
E
1 4
M
1 6
v
8 0
1 8
20
22 6
8
10 1 0 4 1 (~~  1 )
12
Figure 9.3: Selfdiffusivities of 0 and Ni on their respective sublattices in a NiO sin le crystal free of significant line imperfections and along grain boundaries in a polycrystal. &e grainboundary diffusivities of both Ni and 0 in the oxide semiconductor NiO are very much greater than corresponding crystal diffusivities. From Atkinson [3].
There are many situations, particularly at low temperatures, where shortcircuit diffusion along grain boundaries and free surfaces is the dominant mode of diffusional transport and therefore controls important kinetic phenomena in materials; 5We discuss diffusion along dislocations and free surfaces in Sections 9.3 and 9.4.
214
CHAPTER 9: DIFFUSION ALONG CRYSTAL IMPERFECTIONS
several examples are discussed in Sections 9.2 and 9.4. Similar conclusions hold for dislocation diffusional shortcircuiting, although to a lesser degree because of the relatively small cross sections of the highdiffusivity pipes. 9.2 9.2.1
DIFFUSION ALONG GRAIN BOUNDARIES Regimes of GrainBoundary Shortcircuit Diffusion in a Polycrystal
In a polycrystal containing a network of grain boundaries, atoms may migrate in both the grain interiors and the grain boundary slabs [4]. They may jump into or out of boundaries during the time available, and spend various lengths of time jumping in the grains and along the boundaries. Widely different situations may occur, depending upon such variables as the grain size, the temperature, the diffusion time, and whether the boundary network is stationary or moving. For example, as the grain size is reduced and more boundaries become available, the overall diffusion will be enhanced due to the relatively fast diffusion along the boundaries. At elevated temperatures where the ratio of the boundary diffusivity to the crystal diffusivity is lower than at low temperatures (Fig. 9.1), the importance of the boundary diffusion will be diminished. At very long diffusion times, the distance each atom diffuses will be relatively large, and each atom will be able to sample a number of grains and grain boundaries. If the boundaries are moving, an atom in a grain may be overrun by a moving boundary and be able to diffuse rapidly in the boundary before being deposited back into crystalline material behind the moving boundary. Consider first the relatively simple case where the boundaries are stationary and each diffusing atom is able to diffuse both in the grains and along at least several grain boundaries during the diffusion time available. This will occur whenever the diffusion distance in the grains during the diffusion time t is significantly larger than the grain size [i.e., approximately when the condition *DXLt> s2 (where s is the grain size) is satisfied]. For each atom, the fraction of time spent diffusing in grain boundaries is then equal to the ratio of the number of atomic sites that exist in the grain boundaries over the total number of atomic sites in the specimen [5]. This fraction is q x 36/s: for each atom, the meansquare displacement due to diffusion along grain boundaries is then *DBqt,and the meansquare displacement in the grains is * D x L ( l q)t. The total meansquare displacement is then the sum of these quantities, which can be written
(*D)t=* D x L ( l  q)t +*DBqt
(9.3)
+ (36/s)*DB
(9.4)
and because q << 1,
(*D)= *DxL
*DLt > s2
The quantity (*D)is the average effective diffusivity, which describes the overall diffusion in the system. The diffusion in the system therefore behaves macroscopically as if bulk diffusion were occurring in a homogeneous material possessing a uniform diffusivity given by Eq. 9.4. The situation is illustrated schematically in Fig. 9.4a, and experimental data for diffusion of this type are shown in Fig. 9.5. This diffusion regime is called the multipleboundary daffusion regime since the diffusion field
9 2 GRAIN BOUNDARIES
215
B regime
( b )boundary region
C regime (c) core only
Figure 9.4: The A. B, and C regimes for selfdiffusion in polycrystal with stationary grain boundaries according to Harrison [6]. The tracer atoms are diffusing into the semiinfinite specimen from the surface located along the top of each figure. Regions of relatively high tracer concentration are shaded. (a) Regime A: the diffusion length in the grains is considerably longer than the average grain size. (b) Regime B: the diffusion length in the grains is significant but smaller than the grain size. ( c ) Regime C: the diffusion length in the grains is negligible, but significant diffusion occurs along the grain boundaries. In all figures, preferential penetration within the grain boundaries is too narrow to be depicted.
overlaps multiple boundaries. Note that in Fig. 9.4a, fast grainboundary diffusion will cause preferential diffusion to occur along the narrow grainboundary cores beyond the main diffusion front, but the number of atoms will be relatively small and this effect cannot be depicted.
12
I
900°C 700°C I
I
1.o
I
500°C
I
1.2
I
I
1.4
350°C
I
1.6
lOOO/T (KI)
Figure 9.5: Values of the average selfdiffusivity. (*D).in single and polycrystalline silver. At lower temperatures. painboundary diffusion makes significant contributions to the overall measured average di usivity in the polycrystal. From Turnbull [7].
216
CHAPTER 9 DIFFUSION ALONG CRYSTAL IMPERFECTIONS
At the opposite extreme when essentially no diffusion occurs in the grains but significant diffusion still occurs along the boundaries, the overall diffusion will consist of only diffusion penetration along the boundaries, as illustrated in Fig. 9 . 4 ~ . This will tend t o occur at low temperatures or short times under the conditions *DXLt< X2 and *DBt > X2, where X is the interatomic distance. Many intermediate cases may also occur in which diffusion takes place in both the boundaries and in the grains but where the diffusion length in the grains is smaller than the grain size, as in Fig. 9.4b. The conditions for this type of diffusion are X2 <* D X L t < s2 and *DBt > X2. The latter two regimes are called isolatedboundary diffusion regimes, since in both cases there is no overlap of the diffusion fields associated with the individual boundary segments, as in the multipleboundary regime. The three types of regimes just described are often termed the A, B, and C regimes, as indicated in Fig. 9.4, corresponding to Harrison’s original designation [6]. When the boundaries move during the diffusion, as they might during grain growth or recrystallization, the situation is considerably altered. If w is the average boundary velocity, the boundaries will be essentially stationary when w t < A, and the regimes described above will again pertain. However, when the condiwt] > s is satisfied, the multipleboundary diffusion regime will tion [ v ‘ m hold, and Eq. 9.4 will apply even if is negligible, since in such a case the boundaries visit the atoms rather than vice versa. Conversely, when the condition wt] < s is satisfied, the isolatedboundary diffusion regime will exist. The various regimes of possible diffusion behavior can be represented graphically in an approximate manner, as shown in Fig. 9.6 [8]. The axes are taken to be log(*DXLt)and log(wt): logarithmic scales have been used to show the details near the origin because s/X is typically lo3 or more. The stationaryboundary regimes
+
[m +
Crystal diffusion ahead of grain
4 ’diffusion ahead of
grain boundaries
log V t + Figure 9.6: The regimes of diffusion behavior in a pol cr stal in which diffusion may occur both in the rains and along the grain boundaries and txe ioundaries may be stationary or moving. X is t f e interatomic spacin and s is the grain size. On the left side. where th. boundaries are essentially stationary. garrison’s A. B, and C regimes are shown. S.I.XL = Stationary boundaries, Isolated boundary diffusion, and crystal ( X L ) diffusion penetration into adjacent grains. S . I .N X L E Stationary boundaries, Isolated boundary diffusion. and N o crystal (XL) diffusion penetration into adjacent grains. M .I X L G Moving boundaries, Isolated boundary diffusion. CIystal ( X L ) diffusion ahead of boundaries. M.1. NXL E Moving boundaries. Isolated boundary diffusion, N o crystal ( X L ) diffusion ahead of boundaries. S 0 M . M = Stationary O r Moving boundaries, Multiple boundary diffusion. +
From
Cahn
and Balluffi [8]
9.2: GRAIN BOUNDARIES
217
(vt < A) are shown on the left and include Harrison's A, B, and C regimes. The isolatedboundary regimes are enclosed in a region that includes the origin and extends out along the vertical and horizontal axes to distances where * D X L t= s2 and vt = s , respectively. Beyond the isolatedboundary regimes the multipleboundary regime holds sway in all locations. The isolatedboundary regime for moving boundaries in Fig. 9.6 is subdivided into two regimes, depending on whether the crystal diffusion is fast enough so that the atoms are able to diffuse out into the grains ahead of the advancing boundaries. To analyze this, consider a boundary segment between two grains moving with velocity u as in Fig. 9 . 7 ~ . Atoms are diffusing into the boundary laterally from its edges and can diffuse out through its front face into the forward grain. At the same time, atoms will be deposited in the backward grain in the wake of the boundary. In the quasisteady state in a coordinate system fixed to the moving boundary, the diffusion flux in the forward grain is J = *DXL(dc/dx) wc and the diffusion equation is
with the solution
dc * D ~ ~+ wc  =A dx where A is a constant. At a large distance in front of the boundary, dcldx + 0 and c + 0 and therefore A = 0. Finally, upon integration, = c~ e  v x / * D x L
(9.7)
where cG is the concentration maintained at the boundary. The resulting concentration profile is shown in Fig. 9.7b. According to Eq. 9.7, the concentration in front of the boundary will be negligible when * D x L / v < A. Therefore, the curve separating the regimes indicated by M.I.XL and M.I.NXL in Fig. 9.6 should t Xvt, as indicated. follow the straightline relationship * D X L = The diagram in Fig. 9.6 is highly approximate, but it is useful for visualizing the various regimes that might be expected during diffusion in a polycrystal. With increasing time, the point representing the system will start at the origin and move
X
*DxLIv 0
X
Figure 9.7: (a) Grain boundary moving with constant velocity w. Tracer atoms are diffusing rapidly transversely into the boundary slab from its edges, are also diffusing normally out of the boundary into the grain ahead of the boundary. and are being deposited in the grain behind the boundary. Diffusion is in a steady state in a coordinate system moving with the boundary. (b) Tracer concentration in the vicinity of the boundary according to Eq. 9.7.
218
CHAPTER 9 DIFFUSION ALONG CRYSTAL IMPERFECTIONS
progressively away from it. If diffused long enough it will inevitably reach the multipleboundary regime, regardless of whether the boundaries are stationary or moving. 9.2.2
Analysis of Diffusion in the A, B, and C Regimes
A Regime: Since diffusion in this regime is macroscopically similar to diffusion in a homogeneous material possessing an effective bulk diffusivity (Eq. 9.4). it may be analyzed by the methods described in Chapters 4 and 5. B Regime: In this regime, the diffusant diffuses along a boundary while simultaneously leaking out by diffusing into the adjoining grains. Analysis of this type of diffusion is therefore considerably more complex than for diffusion in the A and C regimes since it involves solving for the coupled diffusion fields in the grain boundary and in the adjoining grains. This problem has been solved to different degrees of accuracy for several boundary conditions [9]. Solutions are generally obtained that contain the lumped grainboundary diffusion parameter p = 6*DB and the crystal diffusivity * D x L. The analyses can then be applied to experimental results to obtain values of p when *DxL is known. Fisher has produced a relatively simple solution for a specimen geometry that is convenient for experimentalists and which has been widely used in the study of boundary selfdiffusion by making several approximations which are justified over a range of conditions [9, lo]. The geometry is shown in Fig. 9.8; it is assumed that the specimen is semiinfinite in the y direction and that the boundary is stationary. The boundary condition at the surface corresponds to constant unit tracer concentration, and the initial condition specifies zero tracer concentration within the specimen. Rapid diffusion then occurs down the boundary slab along y. while tracer atoms simultaneously leak into the grains transversely along z by means of crystal diffusion. The diffusion equation in the boundary slab then has the form
Free surface at y = 0, where cB(0.A = 1
c4
Figure 9.8: Isolatedboundary (TypeB) selfdiffusion associated with a stationary grain boundary. (a) Grain boundary of width 6 extending downward from the free surface at y = 0. The surface feeds tracer atoms into the grain boundary and maintains the diffusant concentration a t the grain boundary's intersection with the surface a t the value cB(y = 0, t ) = 1. Diffusant penetrates the boundary along y and simultaneously diffuses transversely into the grain interiors along 2. (b) Diffusant distribution as a function of scaled transverse distance. 1c1, from the boundary at scaled depth, y l , from the surface. Penetration distance in grains is assumed large relative t o 6.
9 z GRAIN BOUNDARIES
219
where 5 1 , y1, and t l are reduced dimensionless variables defined by x1 = 216, y1 = ( y / 6 ) J w , and t l = t*DXL/d2. In the process of solving this equation, Fisher found that the combination of relatively fast diffusion along the grain boundary and slower leakage into the grains causes the concentration in the boundary slab to quickly “saturate” so that the concentration in the adjoining grains at the time t l is essentially the same as the concentration that would have been there if the concentration distribution which existed in the boundary at t l had been maintained constant there since the start of the diffusion at t l = 0. Also, since the diffusion along the boundary is rapid compared to the transverse diffusion in the grains, gradients along y in the grains are much smaller than gradients along x in the grains and can therefore be neglected. The transverse concentration profile along X I in the grains at constant y1 is therefore, to a good approximation, an errorfunction type of solution (Eq. 5.23) of the form
Also, the rapid saturation found in the boundary slab produces a quasisteadystate condition along the boundary: dcB/dtl in Eq. 9.8 can then be set equal to zero so that d2CB(Yl,t l ) (9.10) O=
aY:
x1=0
The solution to Eq. 9.10 must satisfy the boundary condition cB(O, t l ) = 1 and is therefore (9.11) Putting this result into Eq. 9.9 in order to find cxL(xl, y1, t l ) ,
The results above and the approximations made to obtain them have been shown to be valid when the dimensionless parameter p = d*DB(*DXL)3/2t1/2 2 20 [9]. When this condition is not satisfied, more rigorous but complex analysis is required. Experimentalists have frequently used Eq. 9.12 to determine values of the lumped grain boundary diffusion parameter p = 6*DB. The specimen is diffused for the time t and is sectioned by removing thin slices parallel to the surface of thickness Ay. The tracer content of each slice, A N , is then measured and plotted logarithmically against y. From Eq. 9.12 the resulting curve should have the slope
d In A N dY
[
~*DXL
____
~
=
Tt
]
1/4
1
112
[MI
(9.13)
and p = 6*DB can then be determined when *DxL is known. Further analyses of Bregime diffusion, including diffusion under different boundary conditions, are described by Kaur and Gust [9]. When solute atoms rather than tracer isotope atoms diffuse in the B regime, further analysis is necessary. Solute atoms may be expected to segregate in the
220
CHAPTER 9: DIFFUSION ALONG CRYSTAL IMPERFECTIONS
grain boundary, and the concentration in the boundary slab cf(y1,tl) will then differ from the concentration in the grains in the direct vicinity of the boundary slab cFL(0, y1, t l ) . Assuming local equilibrium between these concentrations and that a simple McLeantype segregation isotherm typical of a dilute solution applies [4], the two concentrations will be related by
(9.14)
where k is a constant equilibrium segregation ratio. When Eq. 9.14 is substituted into Eq. 9.9,
(9.15)
When Eq. 9.15 is used instead of Eq. 9.9 and the same procedure is used that produced Eq. 9.13 for selfdiffusion, it is found (see Exercise 9.3) that
(9.16)
holds for the solute diffusion, where D2XL and DF are the solute diffusivities in the crystal and the boundary, respectively. The lumped grainboundary diffusion parameter kSDf can be determined experimentally as before from a plot of In A N vs. yl but it now contains the segregation ratio Ic. Values of SDf can therefore be obtained only when independent information about k is available. Further analysis is required if the simple McLean isotherm does not apply and k is concentrationdependent. C Regime: In this regime, diffusion occurs only in the thin grainboundary slabs. Since the number of diffusing atoms within the slabs is exceedingly small, the experimental measurement of boundary concentration profiles is difficult. Recourse has therefore been made to accumulation methods where the number of atoms which have diffused along a grain boundary are collected in a form that can readily be measured. For example, solute atoms have been deposited on one surface of a thinfilm specimen possessing a columnar grain structure and then diffused through the film along the grain boundaries so that they accumulated on the reverse surface [ll, 121. The diffusion was carried out at low temperatures where no crystal diffusion occurred, and where, according to Fig. 9.1, the diffusion along the surfaces was much more rapid than the diffusion along the grain boundaries. Diffusion through the film specimen was therefore controlled by the rate of grainboundary diffusion. Measurement of the rate of accumulation of the solute on the reverse surface then allowed the measurement of the lumped parameter SO? as detailed in Exercise 9.4.
9.2: GRAIN BOUNDARIES
9.2.3
221
Mechanism of Fast GrainBoundary Diffusion
The mechanisms by which fast grainboundary diffusion occurs are not well established at present. There is extensive evidence that a net diffusional transport of atoms can be induced along grain boundaries, ruling out the ring mechanism and implicating defectmediated mechanisms as responsible for grainboundary diffusion [13]. Due to the small amount of material present in the grain boundary, it has not been possible, so far, to gain critical information about defectmediated processes using experimental techniques. Recourse has been made to computer simulations which indicate that vacancy and interstitial point defects can exist in the boundary core as localized bona fide point defects (see the review by Sutton and Balluffi [4]). Calculations also show that their formation and migration energies are often lower than in the bulk crystal. Figure 9.9 shows the calculated trajectory of a vacancy in the core of a largeangle tilt grain boundary in b.c.c. Fe. Calculations showed that vacancies were more numerous and jump faster in the grain boundary than in the crystal, indicating a vacancy mechanism for diffusion in this particular boundary. However, there is an infinite number of different types of boundaries, and computer simulations for other types of boundaries indicate that the dominant mechanism in some cases may involve interstitial defects [4, 121. During defectmediated grainboundary diffusion, an atom diffusing in the core will move between the various types of sites in the core. Because various types of jumps have different activation energies, the overall diffusion rate is not controlled by a single activation energy. Arrhenius plots for grainboundary diffusion therefore should exhibit at least some curvature. However, when the available data are of only moderate accuracy and exist over only limited temperature ranges, such curvature may be difficult to detect. This has been the case so far with grainboundary diffusion data, and the straightline representation of the data in the Arrhenius
Boundary midplane
[ooi]
Figure 9.9: Calculated atom jumps in the core of a C5 symmetric (001) tilt boundary in model was employed. For purposes of clarity. b.c.c. Fe. A pairpotentialmoleculardynamics the scales used in the figure are [I301 : [310] : [OOT] = 1 : 1 : 5 . All jumps occurred in the fastdiffusing core region. Along the bottom, a vacancy was inserted at B.and subse uently executed the series of jumps shown. The tra'ectory was essentially parallel to the t j t axis. Near the center of the figure, an atom in a site jumped into an interstitial site at I . At the top an atom jumped between B , I and B' sites. From Balluffi et al. [14].
b
222
CHAPTER 9 DIFFUSION ALONG CRYSTAL IMPERFECTIONS
plot in Fig. 9.3 must be regarded as an approximation that yields an effective activation energy, E B , for the temperature range of the data. Some evidence for curvature of Arrhenius plots for grainboundary diffusion has been reviewed [4].
9.3
DIFFUSION ALONG DISLOCATIONS
As with grain boundaries, dislocationdiffusion rates vary with dislocation structure, and there is some evidence that the rate is larger along a dislocation in the edge orientation than in the screw orientation [15]. In general, dislocations in closepacked metals relax by dissociating into partial dislocations connected by ribbons of stacking fault as in Fig. 9.10 [16]. The degree of dissociation is controlled by the stacking fault energy. Dislocations in A1 are essentially nondissociated because of its high stacking fault energy, whereas dislocations in Ag are highly dissociated because of its low stacking fault energy. The data in Fig. 9.1 (averaged over the available dislocation orientations) indicate that the diffusion rate along dislocations in f.c.c. metals decreases as the degree of dislocation dissociation into partial dislocations increases. This effect of dissociation on the diffusion rate may be expected because the core material in the more relaxed partial dislocations is not as strongly perturbed and “loosened up’’ for fast diffusion, as in perfect dislocations. In Fig. 9.1, *DD for nondissociated dislocations is practically equal to *DB,which indicates that the diffusion processes in nondissociated dislocation cores and largeangle grain boundaries are probably quite similar. Evidence for this conclusion also comes from the observation that dislocations can support a net diffusional transport of atoms due to selfdiffusion [15]. As with grain boundaries, this supports a defectmediated mechanism. The overall selfdiffusion in a dislocated crystal containing dislocations throughout its volume can be classified into the same general types of regimes as for a polycrystal containing grain boundaries (see Section 9.2.1). Again, the diffusion may be multiple or isolated, with or without diffusion in the lattice, and the dislocations may be stationary or moving. However, the critical parameters include *DDrather than *DB and the dislocation density rather than the grain size. The multiplediffusion regime for a dislocated crystal is analyzed in Exercise 9.1. Figure 9.11 shows a typical diffusion penetration curve for tracer selfdiffusion into a dislocated single crystal from an instantaneous plane source at the surface [17]. In the region near the surface, diffusion through the crystal directly from the surface source is dominant. However, at depths beyond the range at ,Stacking fault ribbon
Partial f dislocation 1
2 Partial dislocation 2
Dissociated lattice dislocation in f.c.c. metal. The structure consists of two Figure 9.10: partial dislocations separated by a ribbon of stacking fault.
9.4 FREE SURFACES
C e
223
Dislocation pipe diffusion
Penetration depth w Figure 9.11: Typical penetration curve for tracer selfdiffusion from a free surface at tracer concentration csurfinto a single crystal containing dislocations. Transport near the surface is dominated by diffusion in the bulk; at greater depths, dislocation pipe diffusion is the major transport path.
which atoms can be delivered by crystal diffusion alone, long penetrating “tails” are present, due to fast diffusion down dislocations with some concurrent spreading into the adjacent lattice and no overlap of the diffusion fields of adjacent dislocations. This behavior corresponds to the dislocation version of the B regime in Fig. 9.4. 9.4
DIFFUSION ALONG FREE SURFACES
The general macroscopic features of fast diffusion along free surfaces have many of the same features as diffusion along grain boundaries because the fastdiffusion path is again a thin slab of high diffusivity, and a diffusing species can diffuse in both the surface slab and the crystal and enter or leave either region. For example, if a given species is diffusing rapidly along the surface, it may leak into the adjoining crystal just as during typeB kinetics for diffusion along grain boundaries. In fact, the mathematical treatments of this phenomenon in the two cases are similar. The structure of crystalline surfaces is described briefly in Sections 9.1 and 12.2.1 and in Appendix B. All surfaces have a tendency to undergo a “roughening” transition at elevated temperatures and so become general. Even though a considerable effort has been made, many aspects of the atomistic details of surface diffusion are still unknowns6 For singular and vicinal surfaces at relatively low temperatures, surfacedefectmediated mechanisms involving single jumps of adatoms and surface vacancies are p r e d ~ m i n a n t .Calculations ~ indicate that the formation energies of these defects are of roughly comparable magnitude and depend upon the surface inclination [i.e., ( h k l ) ] . Energies of migration on the surface have also been calculated, and in most cases, the adatom moves with more difficulty. Also, as might be expected, the diffusion on most surfaces is anisotropic because of their low twodimensional symmetry. When the surface structure consists of parallel rows of closely spaced atoms, separated by somewhat larger interrow distances, diffusion is usually easier parallel to the dense rows than across them. In some cases, it appears that the 6 0 u r discussion follows reviews by of Shewmon [18] and Bocquet et al. [19]. 7Adatoms, surface vacancies, and other features of surface structure are depicted in Fig. 12.1
224
CHAPTER 9: DIFFUSION ALONG CRYSTAL IMPERFECTIONS
transverse diffusion occurs by a replacement mechanism in which an atom lying between dense rows diffuses across a row by replacing an atom in the row and pushing the displaced atom into the next valley between dense rows. Repetition of this process results in a mechanism that resembles the bulk interstitialcy mechanism described in Section 8.1.3. In addition, for vicinal surfaces, diffusion rates along and over ledges differs from those in the nearby singular regions. At more elevated temperatures, the diffusion mechanisms become more complex and jumps to more distant sites occur, as do collective jumps via multiple defects. At still higher temperatures, adatoms apparently become delocalized and spend significant fractions of their time in “flight” rather than in normal localized states. In many cases, the Arrhenius plot becomes curved at these temperatures (as in Fig. 9.1), due to the onset of these new mechanisms. Also, the diffusion becomes more isotropic and less dependent on the surface orientation. The mechanisms above allow rapid diffusional transport of atoms along the surface. We discuss the role of surface diffusion in the morphological evolution of surfaces and pores during sintering in Chapters 14 and 16, respectively. Bibliography 1. N.A. Gjostein. Short circuit diffusion. In Diffusion, pages 241274. American Society
for Metals, Metals Park, OH, 1973.
2. I. Herbeuval and M. Biscondi. Diffusion of zinc in grains of symmetric flexion of aluminum. Can. Metall. Quart., 13(1):171175, 1974.
3. A. Atkinson. Diffusion in ceramics. In R.W. Cahn, P. Haasen, and E. Kramer, editors, Materials Science and TechnologyA Comprehensive Treatment, volume 11, pages 295337, Wienheim, Germany, 1994. VCH Publishers. 4. A.P. Sutton and R.W. Balluffi. Interfaces in Crystalline Materials. Oxford University Press, Oxford, 1996. 5. E.W. Hart. On the role of dislocations in bulk diffusion. Acta Metall., 5(10):597, 1957. 6 . L.G. Harrison. Influence of dislocations on diffusion kinetics in solids with particular reference t o the alkali halides. Trans. Faraday Soc., 57(7):11911199, 1961.
7. D. Turnbull. Grain boundary and surface diffusion. In J.H. Holloman, editor, A t o m Movements, pages 129151, Cleveland, OH, 1951. American Society for Metals. Special Volume of ASM. 8. J.W. Cahn and R.W. Balluffi. Diffusional masstransport in polycrystals containing stationary or migrating grain boundaries. Scripta Metall. Mater., 13(6):499502, 1979. 9. I. Kaur and W. Gust. Fundamentals of Grain and Interphase Boundary Diffusion. Ziegler Press, Stuttgart, 1989. 10. J.C. Fisher. Calculation of diffusion penetration curves for surface and grain boundary diffusion. J . Appl. Phys., 22(1):7477, 1951. 11. J.C.M. Hwang and R.W. Balluffi. Measurement of grainboundary diffusion at lowtemperatures by the surface accumulation method 1. Method and analysis. J . A p p l . Phys., 50(3):13391348, 1979.
12. Q. Ma and R.W. Balluffi. Diffusion along [OOl]tilt boundaries in the Au/Ag system 1. Experimental results. Acta Metall., 41(1):133141, 1993.
13. R.W. Balluffi. Grain boundary diffusion mechanisms in metals. In G.E. Murch and A S . Nowick, editors, Diffusion in Crystalline Solids, pages 319377, Orlando, FL, 1984. Academic Press.
EXERCISES
225
14. R.W. Balluffi, T. Kwok, P.D. Bristowe, A. Brokman, P.S. Ho, and S. Yip. Deter
mination of the vacancy mechanism for grainboundary selfdiffusion by computer simulation. Scripta Metall. Mater., 15(8):951956, 1981. 15. R.W. Balluffi. On measurements of self diffusion rates along dislocations in f.c.c. metals. Phys. Status Solidi, 42(1):1134, 1970. 16. R.E. ReedHill and R. Abbaschian. Boston, 1992.
Physical Metallurgy Principles.
PWSKent,
17. Y.K. Ho and P.L. Pratt. Dislocation pipe diffusion in sodium chloride crystals. Radiat. Eff., 75~183192, 1983. 18. P. Shewmon. Diffusion in Solids. The Minerals, Metals and Materials Society, Warrendale, PA, 1989. 19. J.L. Bocquet, G. Brebec, and Y. Limoge. Diffusion in metals and alloys. In R.W. Cahn and P. Haasen, editors, Physical Metallurgy, pages 535668. NorthHolland, Amsterdam, 2nd edition, 1996.
EXERCISES 9.1 In a TypeA regime, shortcircuit grainboundary selfdiffusion can enhance the effective bulk selfdiffusivity according to Eq. 9.4. A density of lattice dislocations distributed throughout a bulk single crystal can have a similar effect if the crystal diffusion distance for the diffusing atoms is large compared with the dislocation spacing.
Derive an equation similar to Eq. 9.4 for the effective bulk selfdiffusivity, (*D), in the presence of fast dislocation diffusion. Assume that the dislocations are present at a density, p, corresponding to the dislocation line length in a unit volume of material. Solution. During selfdiffusion, the fraction of the time that a diffusing atom spends in dislocation cores is equal t o the fraction o f all available sites that are located in the dislocation cores. This fraction will be 7 = p7d2/4. The meansquare displacement due t o selfdiffusion along the dislocations is then *DDqt,while the corresponding displacement in the crystal is *DxL(l 7 ) t . Therefore,
(*D)t = * D X L ( l 7 ) t and because 7
<< 1,
+ *DD7t
p7rP (*D)= * D x L+ *DD
4
(9.17)
(9.18)
9.2 Exercise 9.1 yielded an expression, Eq. 9.18, for the enhancement of the effective bulk selfdiffusivity due to fast selfdiffusion along dislocations present in the material at the density, p. Find a corresponding expression for the enhancement of the effective bulk selfdiffusivity of solute atoms due to fast solute selfdiffusion along dislocations. Assume that the solute atoms segregate to the dislocations according to simple McLeantype segregation where cf/cf" = k = constant, where cf is the solute concentration in the dislocation cores and cfL is the solute concentration in the crystal. Solution. Because the fraction of solute sites in the dislocations is small, the number of occupied soluteatom sites (per unit volume) in the crystal is c g L , and the number of
226
CHAPTER 9: DIFFUSION ALONG CRYSTAL IMPERFECTIONS
occupied sites in the dislocations is pd2kc?XL/4. The fraction of time that a diffusing solute atom spends in dislocation cores is then 17 = p7d2k/4. Therefore, following the same argument as in Exercise 9.1,
(*Dz)t = *D,””(l  v)t and thus
(*D2) = * D f L+
+ *Dpqt
(9.19)
@ *Df 4
(9.20)
9.3 For TypeB diffusion along a grain boundary, Eq. 9.9, which holds for self
diffusion, takes the form of Eq. 9.15 for solute diffusion when simple McLeantype segregation occurs with c f / c g L = k. Show that this causes Eq. 9.13, which holds for selfdiffusion, to take the form (9.21) for solute diffusion. Solution. As indicated in the text, Eq. 9.9 must have the form of Eq. 9.15 in order t o satisfy the segregation condition k = cf/c?” a t the boundary slab. Equation 9.10 then becomes
Equation 9.11 becomes B
c2
( y i , t i ) = exp
Equation 9.12 becomes
czX L ( z l , y l , t l ) = exp 1 k and, finally, Eq. 9.13 becomes
[ (A) 
[ (A)”* YI]
Yl]
[1  e r f
I)$
(9.23)
(9.24)
(9.25)
9.4 As described in Section 9.2.2, grainboundary diffusion rates in the TypeC
diffusion regime can be measured by the surfaceaccumulation method illustrated in Fig. 9.12. Assume that the surface diffusion is much faster than the grainboundary diffusion and that the rate at which atoms diffuse from the %ource” surface to the “accumulation” surface is controlled by the diffusion rate along the transverse boundaries. If the diffusant, designated component 2, is initially present on the source surface and absent on the accumulation surface and the specimen is isothermally diffused, a quasisteady rate of accumulation of the diffusant is observed on the accumulation surface after a short initial transient. Derive a relationship between the rate of accumulation
EXERCISES
227
and the parameter SDF that can be used to determine SDf experimentally. Assume that each grain is a square of side d in the plane of the surface.
c
Source
Fil thi
surface
Accumulation surface Figure 9.12: diffusion.
Transport of diffusant through a thin polycrystalline film by grainboundary
Solution. Because of the fast surface diffusion, the concentrations of the diffusant on both surfaces are essentially uniform over their areas. After the initial transient, the quasisteady rate (per unit area of surface) a t which the diffusant diffuses along the transverse boundaries between the two surfaces is
Here, d is the average grain size of the columnar grains, JB is the diffusional flux along the grain boundaries, dcB/dx = [cB(0)  c B ( I ) ]/ I , where cB(0) and cB(I) are the diffusant concentrations in the boundaries a t the source surface and accumulation surface, respectively, and I is the specimen thickness. In the early stages, c B ( I ) 0 and, therefore, t o a good approximation,
=
dN B Id 6D2 = 2cB(0) d t
(9.27)
All quantities on the righthand side of Eq. 9.27 are measurable, which allows the determination of bDf [12].
9.5 Using the result of Exercise 9.1 and data in Fig. 9.1, estimate the density of
dissociated dislocations necessary to enhance the average bulk selfdiffusivity by a factor of 2 at Tm/2,where T, is the absolute melting temperature of the material. Note: typical dislocation densities in annealed f.c.c. metal crystals are in the range 106108 cm2. Solution. Equation 9.18may be solved for p in the form (9.28) It is estimated from Fig. 9.1that *DD(dissoc)/*DXL= 3 x lo6 at Tm/T = 2.0. Also, 6 % 6 x lo* cm*. Using these values and (*D)/*DxL = 2 in Eq. 9.28, p
E
10' cmP2
Therefore, it appears that the dislocations could make a significant contribution t o diffusion under many common conditions.
228
CHAPTER 9: DIFFUSION ALONG CRYSTAL IMPERFECTIONS
9.6 The asymmetric smallangle tilt boundary in Fig. B.5a consists of an array of parallel edge dislocations running parallel to the tilt axis. During diffusion they will act as fast diffusion “pipes.” Show that fast selfdiffusion along this boundary parallel to the tilt axis can be described by an overall boundary diffusivity, sin 4 cos 4 lr e (9.29) *DB(para) =  *DD6 4 b where b is the magnitude of the Burgers vector and 6’ is the tilt angle.
+
Use
*DD>> *DL
(9.30)
Solution. As usual, take the boundary as a slab that is 6 thick. In considering diffusion along the t i l t axis, any contribution of the crystal regions in the slab can be neglected and only the contributions of the dislocation pipes are included because *DD >> *DxL. The flux through a unit crosssectional area of the boundary slab is then (9.31) where the first bracketed term is the flux along a single pipe and the second is the number o f pipes per unit area of the boundary slab. The desired expression is obtained by equating this result with J =  *DB(para)&/ax and solving for *DB.
9.7 Selfdiffusion along the boundary in Exercise 9.6 is highly anisotropic because diffusion along the tilt axis (parallel to the dislocations) is much greater than diffusion transverse to it (i.e., perpendicular to the dislocations but still in the boundary plane). Find an expression for the anisotropy factor,
*D (para) *D (transv)
(9.32)
where *DB(transv) is the boundary diffusivity in the transverse direction. Solution. The transverse diffusion rate is controlled by the relatively slow crystal diffusion rate because the diffusing atoms must traverse the patches of perfect crystal between the dislocation pipes. Therefore, when the dislocations are discretely spaced, a good approximation is the simple result
*DB(para) *DB(para) *DB(transv) *DxL
(9.33)
CHAPTER 10
DIFFUSION IN NONCRYSTALLINE MAT ER IA LS
Noncrystalline materials exist in many different forms. A huge variety of atomic and molecular structures, ranging from liquids to simple monatomic amorphous structures to network glasses to dense longchain polymers, are often complex and difficult to describe. Diffusion in such materials occurs by a correspondingly wide variety of mechanisms, and is, in general, considerably more difficult to analyze quantitatively than is diffusion in crystals. The understanding of diffusion in many noncrystalline materials has lagged behind the understanding of diffusion in crystalline material, and a unified treatment of diffusion in noncrystalline materials is impossible because of its wide range of mechanisms and phenomena. In many cases: basic mechanisms are still controversial or even unknown. We therefore focus on selected cases, although some of the models discussed are still under development and not yet firmly established.
10.1 FREEVOLUME MODEL FOR SELFDIFFUSION IN LIQUIDS Selfdiffusion in simple monatomic liquids at temperatures well above their glasstransition temperatures may be interpreted in a simple manner.' Within such liquids, regions with free volume appear due to displacement fluctuations. Occasionally, the fluctuations are large enough to permit diffusive displacements. 'This section closely follows Cohen and Turnbull's original derivation [l]. The original paper should be consulted for further details.
Kinetics of Materials. By Robert W. Balluffi, Samuel M. Allen, and W. Craig Carter. Copyright @ 2005 John Wiley & Sons, Inc.
229
230
’
CHAPTER 10: DIFFUSION IN NONCRYSTALLINE MATERIALS
The hardsphere model for the liquid serves as a reasonably good approximation for the atomic interactions [2]. Here, the potential energy between any pair of approaching particles is assumed to be constant until they touch, at which point it becomes infinite. On average, the particles in the liquid maintain a volume larger than that which they would have if they all touched; the resulting volume difference is the free volume. Each particle effectively traverses a small confined volume within which the interatomic potentials are essentially flat [3]. The average velocity of a particle in the region of flat potential inside the confining volume is the same as the velocity of a gas particle. Most .of the time a particular particle is confined to a particular region. However, there will occasionally be a fluctuation in local density that opens a space large enough to permit a considerable displacement of the particle. If another particle jumps into that space before the displaced first particle returns, a diffusivetype jump will have occurred. Diffusion therefore occurs as a result of the redistribution of the free volume that occurs at essentially constant energy because of the flatness of the interatomic potentials. According to the kinetic theory of gases, the selfdiffusivity of a hardsphere gas is given by *DG = (2/5)(u)L, where (u)is the average velocity and L is the mean free path [4]. Because the mean free path of a confined particle in the liquid is about equal to the diameter of its confining volume, the contribution of the confined particle t o the selfdiffusivity of the liquid may be written
*D(V)= Cgeom a ( V )(u)
(10.1)
where u ( V ) is the diameter of the confining volume, V is the free volume associis a ated with the particle, (u)is the average velocity of the particle, and C,,,, geometrical constant.It is reasonable to assume that the diffusivity is very small, *D(V)= 0, unless the local free volume V exceeds a critical volume, Vcrit.Therefore, the overall diffusivity may be expressed (10.2)
+
where p ( V )dV is the free volume’s probability that it lies between V and V dV. To determine this probability distribution, consider a system containing n/ particles and divide the total range of possible free volumes for a particle into bins indexed by i. Let Ni(V,)be the number of particles with free volume V,. If Vfreeis the total free volume, the condition Vfree = NiV, (10.3) i
must hold. The factor y accounts for all freevolume overlap between adjacent particles. y lies between zero and one because of the physical limits of complete and no overlap; its value is probably closer to one. The total number of particles, N . is (10.4) i
The entropy associated with the number of ways that the free volume can be distributed at constant energy is (10.5)
10 1. FREEVOLUME MODEL FOR LIQUIDS
231
for bin populations given by Ni. The equilibrium probability distribution in Eq. 10.2 is the continuum limit of the bin populations Ni that maximize Sconf subject to constraints, Eqs. 10.3 and 10.4. Introducing Lagrange multipliers p and X for the total free volume and fixednumber constraints, the extremal conditions are
which, using Stirling's formula Ni! x Ni In Ni and the limit of Ni
>> 1, reduces to
Ni= eX/kefi7V%/k
(10.7)
The constraints Eqs. 10.3 and 10.4 determine the Lagrange multipliers. With Eq. 10.7,
(10.8)
and
The average free volume per particle is (afree) = Vfree/N = k / p . Therefore, comparison of the average free volume to its definition from a probability distribution,
shows that the probability distribution p(V) must be proportional to y exp[ypV/k] = y exp[yV/(Rfree)]. The proportionality factor can be determined by setting the sum of probabilities equal to one, and (10.11) The probability distribution, Eq. 10.11, can be used in Eq. 10.2 as an estimate for evaluating *DL. Above the critical free volume Vcrit,*D(V) is probably nearly constant; therefore,
*D(vcrit)e  y ~ C P ' t / ( ~ f r e = e)
cgeom U(vcrit)(u) e
/(afree)
(10.12)
y~crit
Equation 10.12 matches diffusivities measured in simple liquids if the characteristic "cage" diameter, u(Vcrit),is approximately the particle diameter and yVcritis approximated by the particle volume [l].*DL is not thermally activatedit does not exhibit Arrhenius behavior as does, for example, the diffusivity in crystals, increases approximately linearly with T [4]. Less because (u)0; T1/*and (afree) approximate models for diffusion in liquids have been reviewed by Frohberg [ 5 ] .
232
CHAPTER 10 DIFFUSION IN NONCRYSTALLINE MATERIALS
10.2
DIFFUSION IN AMORPHOUS METALS
Amorphous metallic alloys (metallic glasses) can be produced by rapid cooling (quenching) from the liquid phase. If the initially stable liquid avoids solidification by crystallization by being quenched rapidly below its ordinary melting temperature, T,, it first becomes a supercooled liquid, and then, a t a still lower temperature, it undergoes a glass transition to an amorphous glassy state as in Fig. 10.1. Occurring over a range of temperatures that is dependent upon the cooling rate, the glass transition is characterized by an abrupt change in the rate at which the volume and other physical properties change with decreasing temperature. The glass transition temperature, T,, which occurs a t a given cooling rate, is obtained from the intersection of the extrapolated cooling curves from well above and well below the transition. Because the glass transition occurs at a higher temperature during rapid cooling than during slow cooling, less free volume remains in glasses formed at low temperatures. Below the glass transition temperature, the combined effects of the low temperature and the loss of free volume cause the initially liquid material to lose its characteristic fluidity and become relatively rigid and unable to reorganize itself quickly as the temperature is decreased further (i.e., it becomes a frozenin glass).
Temperature Figure 10.1: Volume of metallic glass during fast and relatively slow cooling from the liquid phase. T,, is the melting teinperature; Tq is the glasstransition temperature (shown for both fast and relatively slow cooling).
10.2.1
SelfDiffusion
If a rapidly cooled metallic glass is reheated and annealed isothermally at a temperature below T,, the excess free volume that is frozenin will anneal out as the
system attempts t o relax and equilibrate without crystallizing. The free volume is mobile and is presumably annihilated when it encounters regions of higher than average atomic density [6, 71. The selfdiffusivity that is measured during such annealing decreases initially. However, it eventually reaches an asymptotic value and becomes time independent, as in Fig. 10.2. The asymptotic value of the diffusivity is then that of the relaxed glassy state in which the supersaturated excess volume has annealed out. This dense structure is,randomly packed, and the atoms are arranged with the highest density compatible with their hardsphere radii and
10.2: DIFFUSION IN AMORPHOUS METALS

h
h
233
613 K 4
Figure 10.2: Selfdiffusion coefficient of 5gFe in amorphous Fe40Ni40B20 during isothermal annealing below T, after rapid quenching from liquid state as in Fig. 10.1. Arrows indicate different time scales used at each temperature. Reprinted from "Tracer Diffusion of Fe59 in Amorphous F e m N i m B m , " J. Horvath and H. Mehrer, 1986, C r y s t a l Lattice D e f e c t s and Amorphous
M a t e r i a l s , Taylor and Francis, http://www.tandf.co.uk/journals/ [8].
lack of translational symmetry. Locally, the atoms form various polyhedral units in definite ratios with neither microcrystallites nor large holes present. Even though relaxed, this structure is still metastable with respect to the crystalline state. Extensive measurements show that selfdiffusivities in the relaxed glassy state are time independent and closely exhibit Arrhenius behavior (i.e., ln*D, vs. 1/T plots appear as essentially straight lines) [8111. The diffusion therefore is thermally activated (in contrast to selfdiffusion in the liquid above Tg as described in Section 10.1). The mechanism by which the selfdiffusion in the relaxed state occurs is not firmly established at present. However, there are reasons to believe that for certain atoms in glassy systems, selfdiffusion occurs by a direct collective mechanism and is not aided by point defects in thermal equilibrium as in the vacancy mechanism for selfdiffusion in crystals (Section 8.2.1). 2 These reasons include: 0
0
0
Sudden changes in temperature during diffusion cause instantaneous changes in the diffusivity [9, 121. This result is unexpected if diffusion occurs by a pointdefect mechanism because significant time is required to obtain the new equilibrium defect concentrations corresponding to the temperature changes. The activation volume for diffusion, as measured by the pressure dependence of the diffusivity, is zero to within experimental accuracy [13, 141. This is unexpected for defectmediated diffusion, as in such cases, the activation volume for diffusion should consist of the sum of the volume of formation of the defect and the activation volume for the defect migration, and this is usually measurable. Computer simulations of the diffusion process in relaxed F e Z r glasses reveal diffusion which takes place directly via thermally activated displacement
2The ring mechanism in Section 8.1.1 is an example of a direct mechanism.
CHAPTER 10 DIFFUSION IN NONCRYSTALLINE MATERIALS
234
chains like that in Fig. 10.3 [7, 9, 151. These chains do not start at localized
hlechanism of diffusion in amorphous glasses by thermally activated Figure 10.3: displacement chains.
point defects but in regions where the initial density deviations are small. Furthermore, when the displacement sequences are completed, any largedensity deviations disperse gradually and do not leave behind localized point defects. The entire displacement process, from beginning to end, involves a relatively large number of atoms and, therefore, is of a collective nature. Such a direct collective diffusion process, which is spread over a considerable volume and involves relatively little ioncore overlap and repulsion, presumably occurs with relatively little volume change, in agreement with the small activation volume cited above. 0
0
The observation that the selfdiffusion exhibits Arrhenius behavior is consistent with a direct collective mechanism because the thermally activated displacement chains are spread over a considerable number of atomic distances. Irregularities in the disordered glassy structure are therefore averaged in the activated state, and all activation energies for displacements are then closely the same.
No isotope effect is observed (see Eq. 8.31) during selfdiffusion in relaxed glasses [16, 171. In tracer selfdiffusion studies of crystalline materials, where the atomic displacements that lead to vacancy migration and diffusion are highly localized, the harmonic model for the isotope effect is justified. However, if the migration process involves a relatively large number of atoms and is highly collective, this estimate of the effective attempt frequency is no longer valid. Instead, it is expected that two isotopes diffuse at close to the same rates because the mass difference of the two isotopes hardly affects their jump frequencies when relatively large numbers of atoms are strongly involved in the activated state.
Further discussion of selfdiffusion in relaxed metallic glasses and other disordered systems may be found in key articles [7, 10, 14, 18, 191. 10.2.2
Diffusion of Small Interstitial Solute Atoms
Small solute atoms in the interstices between the larger host atoms in a relaxed metallic glass diffuse by the direct interstitial mechanism (see Section 8.1.4). The host atoms can be regarded as immobile. A classic example is the diffusion of H solute atoms in glassy Pd80Si20. For this system, a simplified model that retains the essential physics of a thermally activated diffusion process in disordered systems is used to interpret experimental measurements [20221.
10.2: DIFFUSION IN AMORPHOUS METALS
235
Because many different types of interstitial sites exist in the disordered glassy structure, the energy of the system varies as an interstitial atom jumps between the sites. The trace of the energy during successive jumps has the general form illustrated in Fig. 10.4a, where, for simplicity, the energy at each saddle point is assumed to be the same [20, 22, 231. This approximation has the realistic feature that a diffusing interstitial encounters sites of varying energy and jump barriers of various heights. The following quantities will be of use in describing the interstitial selfdiffusion and intrinsic chemical diffusion: N = total number of interstitial sites p = fraction of all interstitial sites that are occupied *p = fraction of all sites that are tracerinterstitial occupied p i = fraction of all sites that are type k sites (Fig. 10.4a) p ( k ) = fraction of type k sites that are occupied pk = fraction of all sites that are occupied type k sites *pk = fraction of all sites that are traceroccupied type k sites
The occupation probability at the various sites should follow FermiDirac statistics because each site can accommodate only one interstitial. Therefore, (10.13) where Gk is the energy corresponding to occupation of the type k site and p is the chemical potential of the interstitials [24]. The fraction of all interstitial sites that are occupied is then (10.14)
W
W
E"
Figure 10.4: (a) The energy variation of an amorphous glass with the displacement of a diffusing interstitial atom as it jumps between successive interstitial sites. (b) A plot similar to (a) for interstitial jumping in a hypothetical material containing only sites of the reference state and having activation energies corresponding to E " .
236
CHAPTER 10: DIFFUSION IN NONCRYSTALLINE MATERIALS
and the partial concentration,
pk,
can be written
( 10.15) Also, c P k = P
( 10.16)
k
A model for the tracer selfdiffusivity of the interstitials is now developed for a system in which the total concentration of inert interstitials and chemically similar radioactivetracer interstitials is constant throughout the specimen but there is a gradient in both concentrations. Since the inert and tracer interstitials are randomly intermixed in each local region, *Pk *P
Pk
P
(10.17)
Therefore, with the use of Eq. 10.15, (10.18) In a typical tracer selfdiffusion experiment, the tracer concentration probability, *p, depends upon position, whereas the total interstitial concentration probability, p , does not. An expression for the tracer selfdiffusivity, of the interstitials, *D, can be derived by employing the same basic method applied to a crystalline material to obtain the selfdiffusivity given by Eq. 8.19. This involves finding the net flux of tracer interstitials jumping through a unit crosssectional area in the diffusion zone perpendicular to the concentration gradient. For a crystalline material, this flux is found by considering the jumping of atoms between welldefined adjacent atomic planes lying parallel to the unit cross section. This approach, however, cannot be applied to a glassy material because of the disorder that is present, and therefore the flux must be determined by a slightly modified method. Consider two thin slabs in the material, each of thickness Ax and having unit area, lying perpendicular to the concentration gradient along x. Slab 1 extends from zo Ax to 20,and slab 2 extends from xo to zo Ax.Let I?;, be the jump rate of a tracer interstitial from ~ ~ activation energy an i site to an adjacent empty i site. According to Fig. 1 0 . 4 the for such a jump will be Go E o  Gk, so
+
+
r/kz  v e  ( G o + E o  G k ) / ( k T )
(10.19)
The rate of ktoi site jumping originating in slab 1is proportional to the quantity (P/(Q))Ax *pk(pp  p z ) q Z . In this expression, (a) is the average atomic volume in the glass, p is the ratio of interstitial sites to atoms, and @/(a)) is the number of interstitial sites per unit volume. (p,"  p z ) is the probability that a site is an empty i site. Making the approximation that all jump distances in the disordered material are of the same magnitude and equal to Ax,the net number of jumps of all types crossing the x = zo plane per unit time in the x direction is
(10.20)
10.2.DIFFUSION IN AMORPHOUS METALS
237
where g is a purely geometrical constant and the double summation ensures that all types of different jumps between the various sites are included. The first term represents the jumps that originate in slab 1 and cross x = xo in the x direction, while the second term represents the jumps that originate in slab 2 and cross x = xo in the x direction. During tracer selfdiffusion, the total concentration of inert and tracer interstitial atoms is constant, so both p and (pg  pi) are independent of 2 . Making the usual Taylor expansion to evaluate the small difference between the terms and using Eqs. 10.18 and 10.19,
Using Eq. 10.16 and the fact that z i p ; = 1, c i ( p g  p i) = 1  p. Also, using this result and Eq. 10.15,
Putting these results into Eq. 10.21 then yields
Equation 10.23 can be put into the simpler form (10.24) where *D; = g (Az)' vexp[E"/(kT)] is the selfdiffusivity in a hypothetical material that contains only sites of the reference state with the energy Go, and in which jumps may occur between them with the activation energy E", as illustrated in Fig. 10.4b. Equation 10.24 is a Fick'slaw equation with a tracer interstitial selfdiffusivity corresponding to (10.25) Having this result, an expression can be obtained for the "intrinsic" chemical diffusivity, D I , which describes the diffusion arising from an inertinterstitial concentration gradient. According to Eqs. 3.35 and 3.42, the flux in such a system is (10.26) Also, p = yo
+ IcTlnyp
(10.27)
where the activity coefficient yis generally a function of concentration and therefore of position. Putting Eq. 10.27 into Eq. 10.26 leads to the Fick'slawtype expression
( 10.28)
238
CHAPTER 10: DIFFUSION IN NONCRYSTALLINE MATERIALS
and, therefore, (10.29) For tracer selfdiffusion, a similar initial equation for the flux is (10.30) However, in this system, the ideal free energy of mixing of the inert and tracer interstitials is the only component that varies with x. By taking the derivative of the free energy to obtain the chemical potential, the xdependent component of the chemical potential of the tracer interstitials is simply kT ln(*p/p), and therefore, because p is constant, (a*p/dx) = (kT/*p)(d*p/dx). Putting this result into Eq. 10.30, (10.31) which is a Fick’slawtype expression with an interstitial tracer selfdiffusivity given bY *DI =* MkT (10.32) Neglecting any small isotope effect, M I =*MI, and comparing Eqs. 10.29 and 10.32, (10.33) which is of the same form as Eq. 3.13. The model above has been compared to experimental results for the diffusion of H in glassy PdsoSizo by Kirchheim and coworkers [21, 221. D I increases strongly with increasing H concentration as seen in Fig. 10<5.By assuming that the energies of the interstitial sites follow a Gaussian distribution around a mean value, good agreement was obtained between the model and experiment. The increase of DI 1 1
1 3
5
4
3
2
1
log P Figure 10.5: Logarithm of the diffusivity of H in amorphous PdsoSizo as a function of the H concentration probability at different temperatures. Points are experimental data. The curves are the predictions of the model leading to Eq. 10.25. From Kirchheim [22].
10 3. SMALL ATOMS (MOLECULES) IN GLASSY POLYMERS
239
with p arises from the successive saturation of the lowerenergy sites as the concentration is increased. This causes a progressive decrease of the activation energy and a corresponding increase in the diffusivity. For example, at very low concentrations, essentially all of the interstitials become trapped at the lowestenergy sites and they engage in longrange diffusion only with difficulty. Further aspects are discussed elsewhere [22]. Figure 10.6 plots the tracer diffusivity data for a number of solute species in glassy Ni80Zr50 as a function of their metallic radius. The diffusivity increases rapidly as the metallic radius decreases. The relatively rapid diffusion of the small atoms in this case may result from the fact that they diffuse by the interstitial mechanism [lo, 181. 19
 20
Ti
h
N
E
v
P21 g 22 I
2 3
Metallic radius (nm) Figure 10.6: Tracer diffusivities in glassy Ni80Zr50 of various solute atoms as a function of their size (as measured by their metallic radii) [25]. Reprinted, by permission, from H. Hahn and R.S. Averback. "Dependence of tracer diffusion on atomic size in amorphous NiZr,"
p. 6534. Copyright 01988 by the American Physical Society.
Phys. Rev. B, Vol. 37,
10.3 SMALL ATOMS (OR MOLECULES) IN GLASSY POLYMERS Some small atoms and molecules, such as He, Ar, COz, and Nz, dissolve in glassy polymers from the gas phase. These particles then diffuse in the bulk polymer presumably by occupying interstices in the glassy structure and jumping between them by the direct interstitial mechanism. The solubilities increase with increasing partial pressure, and the behavior observed can be well explained on the basis of a model in which the dissolved species occupy interstitial sites, the site occupancy obeys FermiDirac statistics, and the site energies are distributed about a mean value in the form of a Gaussian distribution [26, 271. The corresponding diffusivities of these species increase with increasing concentration, in a manner similar to the diffusion of small solute atoms in amorphous metals. This behavior can be explained by the same interstitial diffusion model. Here, the diffusing particles must again occupy progressively higherenergy sites as their concentration increases, causing the average activation energy for diffusion to decrease and the diffusivity to increase. The diffusion of small particles in glassy polymers therefore appears to be quite similar to that in glassy metals.
240
CHAPTER 10. DIFFUSION IN NONCRYSTALLINE MATERIALS
10.4
DIFFUSION OF ALKALI IONS I N NETWORK OXIDE GLASSES
The structure of a pure oxide network glass having stoichiometry G203, free of any alkali ions, is illustrated in Fig. 10.7a [28]. In this structure, cations are threecoordinated and the oxygen anions are twocoordinated. In threedimensional silica glass, each glassforming Si4+ cation is enclosed in a polyhedron of oxygen anions, and these polyhedra are arranged in a network lacking special symmetry and periodicity. The oxygen polyhedra share corners, not edges or faces, and each oxygen ion is covalently bonded to no more than two cations. The oxide glass structure changes significantly when modzfyzng alkali ions are added, as in Fig. 10.7b. where the G203 glass has been altered by adding a significant amount of the network modifier M 2 0 . The structure accommodates the network modifier M+ ions by substitution of three onecoordinated modifier cations for one threecoordinated glassforming ion. In threedimensional silica glass, the addition of Na ions (e.g., via Na2O) causes oxygen ions. previously covalently bonded to two of the glassforming Si4+ cations between which it formed a brzdge. to reduce this bonding so that they become bonded to only one glassforming cation. These oxygen ions, called nonbrzdgzng oxygens, possess an effective negative charge. The corresponding positively charged Na’ ions are then ionically bonded to the nonbridging oxygens, resulting in a partly covalent and partly ionic overall structure. Studies show that in silica glasses with low concentrations of NazO, the ionically bound material exists in the form of small isolated patches or lakes. As the concentration increases, these patches link and eventually form a network of continuous channels [29321. Continuous percolation networks are present at and above a percolation threshold of about 16 vol. % of modifier. Na’ ions are highly mobile compared to the glassforming components and possess a diffusivity which follows Arrhenius behavior [21, 26, 29, 31, 331. Furthermore, the activation energy for diffusion decreases markedly (and the diffusivity increases correspondingly) as the modifier concentration is increased, as in Fig. 10.8. The
Figure 10.7: (a) Twodimensional schematic of pure, oxide network glass of composition G z 0 3 . Small open circles are glassforming cations G 3 + . Large open circles represent oxygen anions. From Kingery et a1 [28] (b) Schematic of glass as modified by the addition of alkali hl+ cations (filled small circles). At high modifierion content, the modifier ions aggregate and form highdiffusivity “lakes” or channels in the glass. Adapted from Greaves [29]
10.5: DIFFUSION OF POLYMER CHAINS
241
4
0.51
,
,
0.1
0.2
, 0.3
.
Figure 10.8: Activation energy for diffusion of Na+ ions in sodium silicate glass of composition (Na20),(Si02)1, as a function of Na+ ion concentration as measured by the fraction of NazO,
2 . From Frischat [33].
mechanism for the diffusion of the Na’ ions is not thoroughly understood, but the results above can be explained with a model in which the Na’ ions diffuse in the modified randomnetwork structure by a direct interstitial mechanism. To engage in longrange diffusion at low concentrations, the Na’ ions must dissociate themselves from their ionic bonding with the nonbridging oxygens and diffuse through the interstices in the covalently bonded network glass regions. This generally requires a relatively large activation energy. At higher concentrations above the percolation threshold, the Na’ ions diffuse relatively easily along the interstices in the ionically bonded percolation channels with a low activation energy. As the modifier concentration increases, the activation energy decreases progressively. Also, the correlation coefficient decreases as the modifier concentration increases, due to the increased degree of correlation arising from the restriction of the diffusion to the narrow channels [31]. 10.5
DIFFUSION OF POLYMER CHAINS
Polymer structure is characterized by long chains of molecules arranged in a wide variety of ways. Diffusion of these long chains occurs in two important and characteristic situations3 In the first, each chain is essentially isolated and embedded in a solvent melt made up of much smaller molecules, and the long chains diffuse by a type of Brownian motion. In the second situation, the long chains are in a dense entangled arrangement, much like cooked spaghetti, and a given chain can then only diffuse in the entangled structure by a snakelike process called reptation. 10.5.1 Structure of Polymer Chains A polymer chain is typically composed of a large number of units (i.e., monomers) arranged in a chainlike configuration held together by covalent bonds. When the monomers are identical, it is termed a homopolymer chain. The chain possesses considerable flexibility since the covalently bonded monomers can change their bonding angles with one another, allowing the chain to act as if were almost “freely jointed.” This flexibility allows a chain to adopt a huge number of possible configurations. An important parameter for describing the chain configuration is the meansquare 3For detailed treatments of this topic, see de Gennes [34, 351 and Lodge et al. [36]
242
CHAPTER 10 DIFFUSION IN NONCRYSTALLINE MATERIALS
distance between the two ends of the chain ( h 2 ) .This can be approximated using the freely jointed chain model, in which it is assumed that the direction of each bond between monomers is random. This model ignores the fact that covalent bonds tend to assume specific angles and also that it is physically impossible for the chain to bend sharply backward and overlap on itself (i.e.. it ignores the existence of an excluded volume that the flexible chain cannot enter). Nevertheless, the model is a reasonable first approximation under many conditions and retains much of the essential physics of the problem. If each monomer is of length b, a chain consisting of N monomers can be constructed by joining them together sequentially end to end. If the angles at which they are added are at random, the problem of determining the distance between the ends, ( h 2 ) ,is identical to that of finding the meansquare displacement resulting from a random walk given by Eq. 7.47. Therefore,
( h 2 )= Nb2
(10.34)
A typical freely jointed chain will therefore be quite compact since the root= f i b , will be small compared meansquare value of its endtoend length, with its length if it were stretched out (i.e., N b , when N is large). Figure 10.9 shows a simulated molecule of polyethylene, (CH2CH2 )N,which approximates a freely jointed configuration. 0: N1/’ derived on the basis of the freely jointed model is The relationship often quite satisfactory despite the approximate nature of the model. Even though the excluded volume clearly exists, its effect can essentially be canceled out under many circumstances. When the chains are in dilute solution in a theta solvent. interactions between the solvent and the chain monomers favor compression of the chain so that the relation x N112is nearly obeyed. On the other hand, in a “good solvent” where monomermonomer and monomersolvent interactions are closely the same, any interactions favoring compression are absent and the excluded volume then acts to reduce the degree of compactness of the chain and produce K N3 I 5 holds to a good approximation. swelling. In these cases, the relation In the case of homopolar polymer melts where the polymer chains are densely entangled, the excluded volume does not play an important role in determining the degree of swelling since each monomer is surrounded by similar monomers, and is unable to distinguish whether they belong to its own chain or another nearby x N 1 / 2will hold closely for a given chain. Even though the relationship
m
m
m
Figure 10.9: N = 50.
Conformation of polyethylene. (CHzCHz )N. Degree of polymerization
10.5:DIFFUSION OF POLYMER CHAINS
243
type of chain of fixed N in different theta solvents and in its melt, the magnitudes of for the chain will differ. 10.5.2
Diffusion of Isolated Polymer Chains in Dilute Solutions
From a hydrodynamical standpoint, a single isolated chain immersed in a liquid solvent consisting of relatively small molecules may be regarded as a porous sponge having a uniform density [35]. Vorticity cannot penetrate this sponge except over a certain screening length which is negligible for a long chain. As far as global properties (such as viscosity and sedimentation) are concerned, the coil possesses Using previous results, Rh an effective radius, Rh, which is proportional to is therefore Rh 0; N 3 / 5 b (10.35)
m.
for a chain in a good solvent, and for a chain in a theta solvent is
Rh 0; N 1 / 2 b
(10.36)
Using this approximation, the diffusivity of the chain is the diffusivity of the effective sponge of radius, Rh, due to its classical Brownian motion in the solvent. The Brownian motion of the sponge is its irregular motion due to random collisions with surrounding solvent molecules that induce the sponge to follow a random walk. The diffusivity of a small particle due to Brownian motion was determined in the early part of the twentieth century by Einstein, Smoluchowski, and Langevin. We follow here a more recent description which imagines that the particle (i.e., the sponge) is embedded in an effectively uniform medium having a viscosity 77 [37]. At the same time, the particle is subjected to random collisions with molecules in the surrounding medium. The model therefore has a continuummolecular duality. The Newtonian force equation for all forces in the 2 direction is
dX md2X = 3F, (10.37) dt2 dt where X is the instantaneous xcoordinate of the sponge’s position. The first term in Eq. 10.37 is the usual inertial term (rn is the effective mass of the chain). The second term is the frictional force exerted on the sponge by the viscous medium and is proportional to the velocity via the friction factor, F,as would be expected on the basis of Stokes’s law. The third term includes all forces associated with collisions with the surrounding molecules. Multiplying Eq. 10.37 by X yields
+
d2 X dX r n x  dt2 =  3 X  d t
But
d2X 1 d x=dt2
and
2 dt
[
+XF,
] (x)
d(X2) dt 
___
xd X
dX
1d ( X 2 ) = dt 2 dt Putting these expressions into Eq. 10.38 then yields
[
m_ d d (X2) _ 2 dt
~
dt
dX
.Fd(X2)
=  2 d t+ X F ,
(10.38)
(10.39) (10.40)
(10.41)
244
CHAPTER 10: DIFFUSION IN NONCRYSTALLINEMATERIALS
Next, the mean values of these terms over a long period are introduced so that (10.42) Now, according to equipartition, (10.43) Also. (10.44) and
(XF,) = 0
(10.45)
because the F, forces are exerted randomly. Therefore,
mdu 3 + U2 = kT 2 dt
__ where
(10.46)
.=(V)
(10.47)
Equation 10.47 has the solution (10.48) where A is constant. The exponential term in Eq. 10.48 is negligible for all times of interest, and therefore
dt
3
(10.49)
By integrating Eq. 10.49,
2kT (10.50) 3 Results for the meansquare displacement along y and z will be the same and, therefore, 6kT (R2) = ( X 2 ) ( Y 2 ) ( Z 2 ) = t (10.51) 3 Comparing this result with Eq. 7.52, the diffusivity of the isolated chain is (x2)=t
+
+
*D1=7 kT
( 10.52)
An expression for the friction factor, 3,can be obtained from Stokes's law, which gives the force, F, exerted by a viscous medium on a sphere of radius, R, moving through it with a velocity, v, in the form [38]
F = 6.irqRv
(10.53)
10.5:DIFFUSION OF POLYMER CHAINS
245
where 7 is the viscosity. Therefore,
r
3= =6 ~ 7 R V
(10.54)
Putting this result into Eq. 10.52 and setting R = Rh for the chain (sponge), (10.55) where Rh is given by Eq. 10.35 or 10.36. Therefore, *D1 for the chain varies inversely with the viscosity and decreases as the chain length increases since it scales approximately as N  1 / 2 or N  3 / 5 . Because the viscosity, 7 , is generally thermally activated, the diffusivity is similarly thermally activated. The determination of the proportionality constant implicit in Eq. 10.55 requires more detailed calculations. 10.5.3
Diffusion of Densely Entangled Polymer Chains by Reptation
In a polymer melt or a concentrated polymer solution, chains are densely packed and highly entangled. An unattached chain in such an entangled structure is able to diffuse through a process called reptation, first proposed by de Gennes [39].* In the densely packed and entangled environment of a polymer melt, a given chain will be unable to move bodily in directions perpendicular to itself because of the resistance provided by its closely packed environment. On the other hand, it will be able to move in directions tangential to itself by a sliding type of motion much like the movement of a snakehence, the term reptation. The freely jointed “head” at the leading end of the chain can always find an optimum region of low density in the material in front of it to advance into, and the remainder of the chain can then follow along by an appropriate sliding motion. This type of motion is similar in many respects to the motion of a train along a curved track. The chain can move equally well in the reverse direction in the same manner since its “head” and “tail” are interchangeable. For conceptual purposes, the highly constricting and anisotropic environment just described can be represented by a fictitious rigid tube within which the chain can slide backward and forward. The sliding can be accomplished by the propagation along the chain length of localized dispiration defects [41], as in Fig. 10.10. The motion of the chain is then visualized essentially as a quasi onedimensional Brownian motion in which the chain randomly walks forward and backward along its tube. As a result of this motion, the tube that initially surrounds the chain (i.e., the initial primitive tube), will be replaced progressively by a new tube, as in Fig. 10.10. By executing excursions in random directions, the ends of the chain iteratively change their surroundings. After a large number of excursions, the chain’s conformation eventually loses contact with its original primitive tube. At this loss of contact, the chain’s trailing end ceases to touch the original primitive tube (Fig. 10.10d) and a new primitive tube is defined. Thus, each successive primitive tube is connected t o its predecessor as in Fig. 10.11. An approximate expression for the chain’s selfdiffusivity can be obtained using the theory of random walks. Let rrepbe the average time required for the chain to move from one primitive tube t o its successor. During an interval T , , ~ , the chain’s 4This discussion of reptation is a simplified version of other rigorous treatments [36, 401.
246
CHAPTER 10: DIFFUSION I N NONCRYSTALLINE MATERIALS
Figure 10.10: Stages in the elimination of the initial primitive tube associated with a reptating polymer chain. (a) Configuration of the initial chain (thin line) and its associated primitive tube (cylinder). The chain can diffuse along the tube by the propagation along its length of the small defects shown. (b) The chain has diffused toward the right by emerging from the end of the primitive tube on the right and creating a newly configured segment outside the primitive tube. ( c ) The chain has diffused toward the left by emerging from the end of the portion of the primitive tube that it occupied in (b) and creating a newly configured segment outside the primitive tube. The portion of the initial primitive tube that it now occupies is indicated by the heavy lines. (d) The chain has diffused toward the right by emerging from the portion of the primitive tube that it occupied in (c) and creating a newly configured segment outside the primitive tube. The chain has almost completely escaped from the initial primitive tube and is almost completely enclosed in a new successor primitive tube (not shown). From Lodge et al [36]
center of mass will undergo a displacement that is approximately the mean length of a primitive tube, ( h 2 )= Nb2 (Eq. 10.34). The relationship between rrepand the meansquare displacement for random walks (Eq. 7.53) provides a model for the chain’s selfdiffusivity: (10.56) An estimate for rKep may be found by considering the Brownian motion of the chain. At the transition from one isolated primitive tube to its successor, the chain must have executed enough excursions to travel the chain length Nb. If the distance associated with each excursion is u and the number of excursions is n, Eq. 7.47 also establishes the estimate b f i M Nb. Therefore, the number of excursions, n, is approximately n = N2b2/u2.If u is the “excursion” frequency,
n
N2b2
r,,, x  x v uu2
(10.57)
Fi ure 10.11: Successive configurations of noncorrelated primitive tubes for a reptating pobmer chain, formed in the sequence 1 + 5 . One end of each tube configuration must be in contact with its predecessor at points indicated by dots. From Lodge et a1 (361
10 5. DIFFUSION OF POLYMER CHAINS
247
It is reasonable that u will be smaller for long chains. Therefore, as an approximation, let u = v o / N ,where uo = constant. Therefore, Trep %
N2b2 N3b2 =vu2 u, u2
~
(10.58)
and, putting Eq. 10.58 into Eq. 10.56, u0u2
*D% 6N2
(10.59)
The diffusivity scales as 1/N2, decreasing rapidly with increasing chain length. A comparison of Eqs. 10.55 and 10.59 shows that the diffusivity of an isolated chain due to Brownian motion falls off more slowly with increasing chain size than the diffusivity of an entangled chain diffusing by the reptation mechanism. Bibliography 1. M.H. Cohen and D. Turnbull. Molecular transport in liquids and glasses. J . Chem. Phys., 31(5):11641 169, 1959.
2. G.H. Vineyard. The theory and structure of liquids. In Liquid Metals and Solidification, pages 148, Cleveland, OH, 1958. American Society for M'etals. 3. D. Turnbull and M.H. Cohen. Freevolume model of the amorphous phase glass transition. J . Chem. Phys., 34(1):120125, 1961. 4. E.H. Kennard. Kinetic Theory of Gases. McGrawHill, New York, 1938.
5. G. Frohberg. Diffusion in liquid metals between the glass transition and the evaporation temperature. Defect and Diffusion Forum, 143147:869874, 1997. 6. M.H. Cohen and G.S. Grest. The nature of the glass transition. J. NonCryst. Solids, 6162: 749759, 1984. 7. W. Frank, U. Hamlescher, H. Kronmuller, P. Scharwaechter, and T. Schuler. Diffusion in amorphous metallic alloysExperiments, moleculardynamics simulations, interpretation. Phys. Scripta, T66:201206, 1996. 8. J. Horvath and H. Mehrer. Tracer diffusion of Fe59 in amorphous Fe40Ni4oB20. Lattice Defects Amorphous Mater., 13(1):114, 1986. 9. W. Frank, J. Horvath, and H. Kronmuller. Diffusion mechanisms in amorphous alloys. Mater. Sci. Eng., 97:415418, 1988. 10. H. Mehrer and W. Dorner. Diffusion in amorphous alloys. Defect and Diffusion Forum, 6669~189206, 1989. 11. W. Frank, A. Horner, P. Scharwaechter, and H. Kronmuller. Diffusion in amorphous
metallic alloys. Muter. Sci. Eng. A , 179:3640, 1994.
12. C.J. Rank. Evaluation of diffusion and relaxation in metallic glasses after shortterm annealing in a mirror furnace. PhD thesis, Stuttgart University, 1992. In German. 13. K. Ratzke and F. Faupel. Pressure dependence of cobalt diffusion in amorphous Fe39Ni40B21. J . NonCryst. Solids, 181(3):261265, 1995. 14. H. Mehrer and G. Rummel. Amorphous metallic alloysdiffusional aspects. In H. Jain and D. Gupta, editors, Diffusion i n Amorphous Materials, pages 163176, Warrendale, PA, 1994. The Minerals, Metals and Materials Society. 15. A. Horner. Selfdiffusion in metallic glasses: Approximation of the eflectiwe medium and molecular simulation. PhD thesis, Stuttgart University, 1993. In German.
248
CHAPTER 10: DIFFUSION IN NONCRYSTALLINE MATERIALS
16. K. Ratzke, P.W. Huppe, and F. Faupel. Transition from singlejump type to highly cooperative diffusion during structural relaxation of a metallicglass. Phys. Rev. Lett., 68(15):23472349, 1992. 17. K. Ratzke, A. Heesemann, and F. Faupel. The vanishing isotope effect of cobalt diffusion in Fe39Ni40B21 glass. J . Phys. Condens. Matter, 7(39):76637668, 1995. 18. R.S. Averback. Defects and diffusion in amorphous alloys. Muter. Res. SOC.Bull., 16(11):4752, 1991.
19. F. Faupel. Diffusion in noncrystalline metallic and organic media. Phys. Status Solidi. A , 134(1):959, 1992. 20. U. Stolz, R. Kirchheim, J.E. Sadoc, and M. Laridjani. Hydrogen in liquidquenched and vaporquenched amorphous PdgoSizo. J . LessCommon Muter., 103(1):8190, 1984. 21. R. Kirchheim and U. Stolz. Modeling tracer diffusion and mobility of interstitials in disordered materials. J . NonCryst. Solids, 70(3):323341, 1985. 22. R. Kirchheim. Hydrogen solubility and diffusivity in defective and amorphous metals. Prog. Muter. Sci., 32(4):261325, 1988. 23. R. Kirchheim. Solubility, diffusivity, and the trapping of hydrogen in dilute alloys, deformed and amorphous metals. 2. Acta Metall., 30(6):10691078, 1982. 24. D.A. McQuarrie. Statistical Mechanics. HarperCollins, New York, 1976. 25. H. Hahn and R.S. Averback. Dependence of tracer diffusion on atomic size in amorphous NiZr. Phys. Rev. B, 37(11):65336535, 1988. 26. R. Kirchheim. Interstitial diffusion in glass. Defect and Diffusion Forum, 9598:11591164, 1993. 27. R. Kirchheim. Interstitial diffusion in glasses and the mixed alkali effect. In H. Jain and D. Gupta, editors, Diffusion in Amorphous Materials, pages 4354, Warrendale, PA, 1994. The Minerals, Metals and Materials Society. 28. W.D. Kingery, H.K. Bowen, and D.R. Uhlmann. Introduction to Ceramics. John Wiley & Sons, New York, 1976. 29. G.N. Greaves. EXAFS and the structure of glass. J . NonCryst. Solids, 71(13):203217, 1985. 30. C. Huang and A.N. Cormack. The structure of sodium silicate glass. J . Chem. Phys., 93(11):81808186, 1990. 31. G.N. Greaves, S.J. Gurman, C.R.A. Catlow, A.V. Chadwick, S. Houdewalter, C.M.B. Henderson, and B.R. Dobson. A structural basis for ionic diffusion in oxide glasses. Phil. Mag. A , 64(5):10591072, 1991. 32. Y. Cao and A.N. Cormack. A structural model for interpretation of an anomaly in alkali aluminosilicate glasses at Al/alkali = 0.20.4. In H. Jain and D. Gupta, editors, Diffusion in Amorphous Materials, pages 137151, Warrendale, PA, 1994. The Minerals, Metals and Materials Society. 33. G.H. Frischat. Ionic Diffusion in Oxide Glasses. Trans Tech Publications, Bay Village, OH, 1975. 34. P.G. de Gennes. Scaling Concepts in Polymer Physics. Cornell University Press, Ithaca, NY, 1979. 35. P.G. de Gennes. Introduction to Polymer Dynamics. Cambridge University Press, Cambridge, 1990.
105 DIFFUSION OF POLYMER CHAINS
249
36. T.P. Lodge, N.A. Rotstein, and S. Prager. Dynamics of entagled polymer liquids: Do linear chains reptate? In I. Prigogine and S.A. Rice, editors, Advances in Chemical Physics, volume 79, pages 1132, New York, 1990. John Wiley & Sons. 37. J.F. Lee, F.W. Sears, and D.L. Turcotte. Statistical Themodynamics. AddisonWesley, Reading, MA, 1963. 38. K. Huang. Statistical Mechanics. John Wiley & Sons, New York, 1963. 39. P.G. de Gennes. Reptation of a polymer chain in the presence of fixed obstacles. J . Chem. Phys., 55(2):572579, 1971. 40. M. Doi and S.F. Edwards. Press, Oxford, 1986.
The Theory of Polymer Dynamics. Oxford University
41. S.M. Allen and E.L. Thomas. The Structure of Materials. John Wiley & Sons, New York, 1999.
PART II
MOTION OF DISLOCATIONS AND INTERFACES
A host of important kinetic processes in materials depends upon the motion of dislocations and various types of interfaces, and we now describe the basic features of the different types of motion that can occur. Different atomic mechanisms are involvedincluding jumping processes of the diffusive type described in Chapter 7, longrange diffusion of components in the system, and atomic shuffles (shortrange displacements that produce local structural changes as the dislocation, or interface, moves). The situation is compounded further by the fact that dislocations and interfaces are themselves generally complex entities that can have a variety of structures, and therefore varying responses, t o the forces that drive their motion. We start with dislocations and describe both glissile (conservative) and climb (nonconservative) motion in Chapter 11. The motion of vapor/crystal interfaces and liquid/crystal interfaces is taken up in Chapter 12. Finally, the complex subject of the motion of crystal/crystal interfaces is treated in Chapter 13, including both glissile and nonconservative motion.
CHAPTER 11
MOTION OF DISLOCATIONS
The motion of dislocations by glide and climb is fundamental to many important kinetic processes in materials. Gliding dislocations are responsible for plastic deformation of crystalline materials at relatively low temperatures, where any dislocation climb is negligible. They also play important roles in the motion of glissile interfaces during twinning and diffusionless martensitic phase transformations. Both gliding and climbing dislocations cause much of the deformation that occurs at higher temperatures where selfdiffusion rates become significant, and significant climb is then possible. Climbing dislocations act as sources and sinks for point defects. This chapter establishes some of the basic kinetic features of both dislocation glide and climb. 11.1 GLIDE A N D CLIMB The general motion of a dislocation can always be broken down into two components: glide motion and climb motion. Glide is movement of the dislocation along its glide (slip) plane, which is defined as the plane that contains the dislocation line and its Burgers vector. Climb is motion normal to the glide plane. Glide motion is a conservative process in the sense that there is no need to deliver or remove atoms at the dislocation core during its motion. In contrast, the delivery or removal of atoms at the core is necessary for climb. This is illustrated for the simple case of the glide and climb of an edge dislocation in Fig. 11.1, The glide along IC in Fig. 11.1a and b is accomplished by the local conservative shuffling of atoms at the dislocaKinetics of Materials. By Robert W. Balluffi, Samuel M. Allen, and W. Craig Carter. Copyright @ 2005 John Wiley & Sons, Inc.
253
254
......... ......... ......... ......... ..................... .................. ..................
CHAPTER 11: MOTION OF DISLOCATIONS
.&.
0
0
@
(b)
Y
t
Figure 11.1:
Glide and climb of edge dislocation in primitive cubic crystal
(g = [boo].
( = [OOl]) [l]. (a) and (b) Glide from left to right. (c)(f) Downward climb along
y.
In (d), the lightershaded substitutional atom shown adjacent to the dislocation core in (c) has joined the extra half plane and created a vacancy. In (e), the vacancy has migrated away from the dislocation core by diffusion. In ( f ) , the vacancy has been annihilated at the surface step. This overall process is equivalent to removing an atom from the surface and transporting it to the dislocation at its core. A new site was created at the dislocation, which acted as a vacancy source. This site was subsequently annihilated at the surface. which acted as an atom source.
tion core as it moves. The climb along y, however, requires that the extra plane associated with the edge dislocation be extended in the y direction. This requires a diffusive flux of atoms to the dislocation core, and when selfdiffusion occurs by a vacancy mechanism, the corresponding creation of an equivalent number of new lattice sites in the form of vacancies. In this case, the dislocation acts as a sink for atoms and, equivalently, as a source for vacancies. Glide can therefore occur at any temperature, whereas significant climb is possible only at elevated temperatures where the required diffusion can 0ccur.l Defects such as dislocations can be sources or sinks for atoms or for vacancies. Whether such point entities are created or destroyed depends on the type of defect, its orientation, and the stresses acting on it. It is convenient to adopt a single term source, which describes a defect’s capability for creation and destruction of crystal sites and vacancies in the crystal. “Source” will generically indicate creation of point entities (i.e., “positive” source action) as well as destruction of point entities (i.e., “negative” source action). Thus, a climbing edge dislocation that destroys vacancies will be, equivalently, both a (positive) source of atoms and a (negative) source of vacancies. If the sense of climb is reversed, the dislocation would be a (negative) source of atoms. lProvided that the Peierls force is not too large (see Section 11.3.1).
11 2 . DRIVING FORCES ON DISLOCATIONS
11.2
255
DRIVING FORCES ON DISLOCATIONS
Dislocations in crystals tend to move in response to forces exerted on them. In general, an effective driving force is exerted on a dislocation whenever a displacement of the dislocation causes a reduction in the energy of the system. Forces may arise in a variety of ways. 11.2.1
Mechanical Force
In general, a segment of dislocation in a crystal in which there is a stress field is subjected t o an effective force because the stress does an increment of work (per unit length), bW, when the dislocation is moved in a direction perpendicular to itself by the vector, 67.In this process, the material on one side of the area swept out by the dislocation during its motion is displaced relative to the material on the opposite side by the Burgers vector, b', of the dislocation. Work bW is generally done by the stress during this displacement. This results in a corresponding reduction in the potential energy of the system. The magnitude of the effective force on the dislocation (often termed the "mechanical" force) is then just f = bW/br. A detailed analysis of this force yields the PeachKoehler equation: (11.1)
L
where is the mechanical force exerted on the dislocation (per unit length), u the stress tensor in the material at the dislocation, and ( the unit vector tangent to the dislocation along its positive direction [2]. Equation 11.1 is consistent with the convention that the Burgers vector of the dislocation is the closure failure (from start to finish) of a Burgers circuit taken in a crystal in a clockwise direction around the dislocation while looking along the dislocation in the positive direction.2 When written in full, Eq. 11.1 has the form (11.2) where (11.3) With this result, the mechanical force exerted on any straight dislocation by any stress field can be calculated. For example, if the edge dislocation (b' = [boo], ( = [OOl]) in Figure 11.1 is subjected to a shearing stress uxy,it experiences a force urging it to glide on its slip plane in the 2 direction. However, if the dislocation is subjected to the tensile stress, g x x ,Eq. 11.1 shows that it will experience the force .+ f,, =  j b a x x (i.e., a force urging it to climb in the 9 direction). In a more general stress field, the force (which is always perpendicular to the dislocation line) can have a component in the glide plane of the dislocation as well as a compor!ent normal to the glide plane. In such a case, the overall force will tend t o produce both glide and climb. However, if the temperature is low enough that no significant diffusion is possible, only glide will occur. 2The Burgers circuit is constructed so that it will close if mapped step by step into a perfect reference crystal. See Hirth and Lothe [2].
256
CHAPTER 11 MOTION OF DISLOCATIONS
11.2.2 Osmotic Force A dislocation is generally subjected to another type of force if nonequilibrium point defects are present (see Fig. 11.2). If the point defects are supersaturated vacancies, they can diffuse to the dislocation and be destroyed there by dislocation climb. A diffusion flux of excess vacancies to the dislocation is equivalent to an opposite flux of atoms taken from the extra plane associated with the edge dislocation. This causes the extra plane to shrink, the dislocation to climb in the f y direction, and the dislocation to act as a vacancy sink. In this situation, an effective “osmotic” force is exerted on the dislocation in the f y direction, since the destruction of the excess vacancies which occurs when the dislocation climbs a distance by causes the free energy of the system to decrease by 66. The osmotic force is then given by f;. =  j 66lSy. By evaluating 66 and b y when SNv vacancies are destroyed, an expression for f;. can be obtained. The quantity 66 is just pvGNv, where the chemical potential of the vacancies, p v , is given by Eq. 3.66. If a climbing edge dislocation destroys SNv vacancies per unit length, the climb distance will be by = ( R / b ) b N v . The osmotic force is therefore (11.4)
This result is easily generalized for mixed dislocations which are partly screwtype and partly edgetype, and also for cases having subsaturated vacancies. For a mixed dislocation, b must be replaced by the edge component of its Burgers vector
Figure 11.2: Oblique view of edge dislocation climb due to destruction of excess vacancies. The extra plane associated with the edge dislocation is shaded. At A , a vacancy from the crystal is destroyed directly at a jog. At B , a vacancy from the crystal jumps into the core. At C, an attached vacancy is destroyed at a jog. At D , an attached vacancy diffuses along the core.
11 2 DRIVING FORCES ON DISLOCATIONS
257
and the result (see Exercise 11.1) is (11.5)

where
kT
B = b In R
($)
(11.6)
If the vacancies are subsaturated, the dislocation tends to produce vacancies and therefore acts as a vacancy source. In that case, Eq. 11.5 will still hold, but pv will be negative and the climb force and climb direction will be reversed. Equation 11.5 will be reversed. also holds for interstitial point defects, but the sign of
6
11.2.3
Curvature Force
Still another force will be present if a dislocation is curved. In such cases, the dislocation can reduce the energy of the system by moving to decrease its length. An effective force therefore tends to induce this type of motion. Consider, for example, the simple case of a circular prismatic dislocation loop of radius, R. The energy of such a loop is
W = R 2 ( 1pb2  u ) [In(:)
 11
(11.7)
where R, is the usual cutoff radius (introduced to avoid any elastic singularity at the origin) [ 2 ] . The energy of such a loop can be reduced by reducing its radius and therefore its length. Thus, a climb force, exists which is radial and in the direction to shrink the loop. A calculation of the reduction in the loop energy achieved when its radius shrinks by 6R shows that (dW/dR)6R = 27rRf K 6R. The force is therefore
fl;,
(11.8) This result may be generalized. Any segment of an arbitrarily curved dislocation line will be subjected to a curvature force of similar magnitude because the stress fields of other segments of the dislocation line at some distance from the segment under consideration exert only minimal forces on it. For most curved dislocation geometries, the magnitude of the righthand side of Eq. 11.8 is approximately equal to pb2 ( l / R ) .Therefore, for a general dislocation with radius of curvature, R, (11.9) The quantity pb2 has the dimensions of a force (or, equivalently, energy per unit length) and is known as the line tension of the dislocation. Equation 11.9 can also be obtained by taking the line tension to be a force acting along the dislocation in a manner tending to decrease its length.3 This approximation is supported by detailed calculations for other forms of curved dislocations [2]. 3This is explored further in Exercise 11.2.
258
CHAPTER 11: MOTION OF DISLOCATIONS
The vector form of Eq. 11.9 is readily obtained. If r'is the position vector tracing out the dislocation line in space and ds is the increment of arc length traversed along the dislocation when r' increased by dr',4 (11.10) where at the point r' on the line, f i is the principal normal, which is a unit vector perpendicular to ( and directed toward the concave side of the curved line, K is the curvature, and R is the radius of curvature. Therefore, (11.11)
11.2.4 Total Driving Force on a Dislocation The total driving force on a dislocation, considered and, therefore,
$=flr+$+.L 11.3
=
( I X
t) + ('
>' +
x B
f: is the df = pb2 ds
sum of the forces previously
x
4 (2 4+ pb2 ds
(11.12)
DISLOCATION GLIDE
Of central interest is the rate at which a dislocation is able to glide through a crystal under a given driving force. Many factors play potential roles in determining this rate. In perfect crystals, relativistic effects can come into play as dislocation velocities approach the speed of sound in the medium. At elevated temperatures, dissipative phonon effects can produce frictional drag forces opposing the motion. Also, the atom shuffling at the core, which is necessary for the motion, may be difficult in certain types of crystals and thus inhibit glide. In imperfect crystals, any point, line, and planar defects and inclusions can serve as additional obstacles hindering dislocation glide. We begin by discussing glide in a perfect single crystal, which for the present is taken to be a linear elastic continuum.
11.3.1 Glide in Perfect Single Crystals Relativistic Effects. Consider the relatively simple case of a screw dislocation moving along 5 at the constant velocity v' (see Fig. 11.3). The elastic displacements, u l , u2, and 213, around such a dislocation may be determined by solving the Navier equations of isotropic linear elasticity [3].5 For this screw dislocation, the only nonzero displacements are along z , and for the moving dislocation the Navier equations therefore reduce to
(11.13) where p is the density of the medium, p is the shear modulus, and on the left is the inertial term due to the acceleration of mass caused by the moving dislocation. 4See Appendix C for a brief survey of mathematical relations for curves and surfaces. 5See standard references on dislocation mechanics [2, 4, 51.
113 DISLOCATION GLIDE
Y
259
Y‘
i
AI
Figure 11.3: Screw dislocation with b’ = [OOb], = [OOl] moving in the +z direction at a constant velocity v’. The origin of the primed (d, y’, z ’ ) coordinate system is fixed to the niovi ng dislocation.

Equation 11.13 is readily solved after making the changes of variable
7
rvt xI 
yL E
Y’ = Y 2‘ I
=z
(11.14)
 tvx
where c = is the velocity of a transverse shear sound wave in the elastic medium. The origin of the ( X I , y‘, z’) coordinate system is fixed on the moving dislocation as in Fig. 11.3. These changes of variable transform Eq. 11.13 into d2u3 32213 ++,=o dXl2 dy
(11.15)
because u g is a not a function of tl in the moving coordinate system and du3/dt’ = 0. Equation 11.15 has the form of the Navier equation for a static screw dislocation and its solution6 has the form 2.n
(11.16)
Transforming this solution back to x ,y , t space,
b uz(x,y , t) =  tan2i7
(11.17)
The shear stress of the dislocation in cylindrical coordinates, g o z , may now be found by using the standard relations orz = p(au,/dx), uyz = p(du,/dy), and Ooz = oyzcose  ozzsine. The result is goz =
p b YL (x; + yg)’” 2.n
x;+r;y;
6Further discussion of this can be found in Hirth and Lothe [2].
(11.18)
260
CHAPTER 11: MOTION OF DISLOCATIONS
where the distances 20 and yo (measured from the moving dislocation) have been introduced. Equation 11.18indicates that the stress field is progressively contracted along the 20 axis and extended along the yo axis as the velocity of the dislocation is increased. This distortion is analogous to the Lorentz contraction and expansion of the electric field around a moving electron, and the quantity y~ plays a role similar to the LorentzEinstein term (1 w2/c2)lI2 in the relativistic theory of the electron, where c is the velocity of light rather than of a transverse shear wave. In the limit when w + c and y~ + 0, the stress around the dislocation vanishes everywhere except along the y'axis, where it becomes infinite. Another quantity of interest is the velocity dependence of the energy of the dislocation. The energy density in the material around the dislocation, w, is the sum of the elastic strainenergy density and the kineticenergy density,
w = 2w,,2
+ 2pLEyz+ z p
(;;)2=;[(EE)2+(L!%)2+;( 
(11.19) where the first two terms in each expression make up the elastic strainenergy density and the third term is the kineticenergy density [3]. The total energy may then be found by integrating the energy density over the volume surrounding the
(11.20) where W" is the elastic energy of the dislocation per unit length at rest [2, 4, 51, (11.21)
Here, R, is again the usual cutoff radius a t the core and R is the dimension of the crystal containing the dislocation. According to Eq. 11.20, the energy of the moving dislocation will approach infinity as its velocity approaches the speed of sound. Again, the relationship for the moving dislocation is similar to that for a relativistic particle as it approaches the speed of light. These results indicate that in the present linear elastic model, the limiting velocity for the screw dislocation will be the speed of sound as propagated by a shear wave. Even though the linear model will break down as the speed of sound is approached, it is customary to consider c as the limiting velocity and to take the relativistic behavior as a useful indication of the behavior of the dislocation as w + c. It is noted that according to Eq. 11.20, relativistic effects become important only when w approaches c rather closely. The behavior of an edge dislocation is more complicated since its displacement field produces both shear and normal stresses. The solution consists of the superposition of two terms, each of which behave relativistically with limiting velocities corresponding to the speed of transverse shear waves and longitudinal waves, respectively [a, 4, 51. The relative magnitudes of these terms depend upon w. Drag Effects. Dislocations gliding in real crystals encounter dissipative frictional forces which oppose their motion. These frictional forces generally limit the dislocation velocity to values well below the relativistic range. Such drag forces originate from a variety of sources and are difficult t o analyze quantitatively.
11.3: DISLOCATION GLIDE
261
Drag by Emission of Sound Waves. When a straight dislocation segment glides in a crystal, its core structure varies periodically with the periodicity of the crystal along the glide direction. The potential energy of the system, a function of the core structure, will therefore vary with this same periodicity as the dislocation glides. Because of this position dependence, there is a spatially periodic Peierls force that must be overcome to move a dislocation. Therefore, the force required to displace a dislocation continuously must exceed the Peierls force, indicated by the positions where the derivative of potential energy in Fig. 11.4 is maximal [2].’As the dislocb tion traverses the potentialenergy maxima and minima, it alternately decelerates and accelerates and changes its structure periodically in a “pulsing” manner. These structural changes radiate energy in the form of sound waves (phonons). The energy required to produce this radiation must come from the work done by the applied force driving the dislocation. The net effect is the conversion of work into heat, and a frictional drag force is therefore exerted on the dislocation.
I
I
X
b
Position of dislocation Figure 11.4: Variation of potential energy of crystal plus dislocation w a function of dislocation position. Periodicity of potential energy corresponds to periodicity of crystal structure.
In a crystal, sound waves of a given polarization and direction of propagation are dispersivetheir velocity is a decreasing function of their wavenumber, which produces a further drag force on a dislocation. The dispersion relation is (11.22)
where w is the angular frequency, d is the distance between successive atomic planes in the direction of propagation, k = 27r/X is the wavenumber, and X is the wavelength.8 In the longwavelength limit (A >> d) corresponding to an elastic wave in a homogeneous continuum, the phase velocity is c (as expected). However, at the shortest wavelength that the crystal can transmit (A = 2 4 , the phase velocity is lower and, according to Eq. 11.22, is given by 2c/7r. The displacement field of the dislocation can now be broken down into Fourier components of different wavelengths. If the dislocation as a whole is forced to travel at a velocity lower than c but higher than 2c/7r, the shortwavelength components will be compelled to travel faster than their phase velocity and will behave as components of a su‘However, dislocations will still move by thermally activated processes below the Peierls force. *For more about the dispersion relation, see a reference on solidstate physics, such as Kittel [6].
262
CHAPTER 11: MOTION OF DISLOCATIONS
personic dislocation. These components will radiate energy and therefore impose a viscous drag force on the dislocation (see Section 11.3.4). Drag by Scattering of Phonons and Electrons. A dislocation scatters phonons by two basic mechanisms. First, there are density changes in its displacement field which produce scattering. Second, the dislocation moves under the influence of an impinging sound wave and, as it oscillates, reradiates a cylindrical wave. If the dislocation undergoes no net motion and is exposed to an isotropic flux of phonons it will experience no net force. However, if it is moving, the asymmetric phonon scattering will exert a net retarding force, since, in general, any entity that scatters plane waves experiences a force in the direction of propagation of the waves. If, in addition, free electrons are present, they will be scattered by an effective scattering potential produced by the displacement field of the dislocation. This produces a further retarding force on a moving dislocation. Peierls Force: Continuous vs. Discontinuous Motion. In some crystals (e.g., covalent crystals) the Peierls force may be so large that the driving force due to the applied stress will not be able to drive the dislocation forward. In such a case the dislocation will be rendered immobile. However, at elevated temperatures, the dislocation may be able to surmount the Peierls energy barrier by means of stressaided thermal activation, as in Fig. 11.5. I
<
I I I I I I I
I I I I I I I
I I I I I I I
I I I I I I I
I I I I I I I
I I
I I
I I
I I
I I
I I I I I I I I
I I I
I I I I I I I I
I I I
,
I I I I I I I I
I I I
,
I I I I I I I I
I I I
,
I I I I I I I I
I I I
:: ,
I
,
,
,
I
I
I
I
I
I
I
I
I
I
I
I
I
I
I I I I I 1 I I I
I I I l I 1 I I I
I I I I I I l 1 I I 1 I I I I I I I
I I I 1 I l I I I
I I I I I
l l 1 I I I / I 1 / 1 I
1 I 1 I 1
I
I
I
I
I
I
Figure 11.5: Movement of dislocation across a Peierls energy barrier by thermally activated generation of double kinks. Dashed lines represent positions of energy minima shown in Fig. 11.4.
In Fig. 11.5a, the dislocation is forced up against the side of a Peierls “hill” by an applied stress as in Fig. 11.4. With the aid of thermal activation, it then generates a double kink in which a short length of the dislocation moves over the Peierls hill into the next valley (Fig. 11.5b).9 The two kinks then glide apart transversely under the influence of the driving force (Fig. 1 1 . 5 ~ and ) ~ eventually, the entire dislocation advances one periodic spacing. By repeating this process, the dislocation will advance in a discontinuous manner with a waiting period between each advance, and the overall forward rate will be thermally activated. This is an 9 A kink is an offset of the dislocation in its glide plane; it differs fundamentally from a jog, an offset normal t o the glide plane.
11 3 DISLOCATION GLIDE
263
example of discontinuous motion, which results when the driving force is not large enough to drive the dislocations forward continuously in purely mechanical fashion. Figure 11.6 illustrates the energy that must be supplied by thermal activation. The curve of ab vs. A shows the force that must be applied to the dislocation (per unit length) if it were forced to surmount the Peierls barrier in the manner just described in the absence of thermal activation. The quantity A is the area swept out by the double kink as it surmounts the barrier and is a measure of the forward motion of the double kink. A = 0 corresponds to the dislocation lying along an energy trough (minimum) as in Fig. 1 1 . 5 ~ .A2 is the area swept out when maximum force must be supplied to drive the double kink. A4 is the area swept out when the saddle point has been reached and the barrier has been effectively surmounted. The area under the curve is then the total work that must be done by the applied stress to surmount the barrier in the absence of thermal activation. When the applied stress is a~ (and too small to force the barrier), the sweptout area is A l , and the energy that must be supplied by thermal activation is then the shaded area shown in Fig. 11.6. The activation energy is then
E = bh:(a

0A)dA
(11.23)
and the overall dislocation velocity will be of the form
where vo is proportional to an attempt frequency. The area A3  A1 swept out during the activation event, is termed the activation area. Of particular interest from a kinetics standpoint is the result (Eq. 11.23) that the activation energy decreases as the applied stress increases: hence, the term stressaided thermal activation.
Ob
t
Figure 11.6: Curve of applied force, ab, vs. area swept out, A , when dislocation surmounts an obstacle to glide.
11.3.2 Glide in Imperfect Crystals Containing Various Obstacles Real crystals can contain a large variety of different types of point, line, and planar crystal defects and other entities, such as embedded particles, which interact with dislocations and can act as obstacles to glide. Solute atoms are good examples of point defects that hinder dislocation glide by acting as centers of dilation
264
CHAPTER 11: MOTION OF DISLOCATIONS
(see Fig. 3.9) and therefore possess stress fields that interact with dislocation stress fields, causing localized dislocationsoluteatom attraction or repulsion. If a dispersion of solute atoms is present in solution, a dislocation will not move through it as a rigid line but will consist of segments that bulge in and out as the dislocation experiences close encounters with nearby solute atoms. The overall dislocation motion therefore consists of a uniform motion with superimposed rapid forward or backward localized bulging. This type of rapid bulging motion dissipates extra energy by a number of the mechanisms already discussed and therefore exerts a drag force. At sufficiently high temperatures, solute atoms may migrate in the stress field of dislocations (Section 3.5.2), and such induced diffusion can dissipate energy and produce a drag force, particularly for slowly moving dislocations. In addition, solute atoms with anisotropic displacement fields can change orientations under the influence of the stress field of a moving dislocation, thereby producing an increment of macroscopic strain (see Section 8.3.1). This can also lead to a dissipative drag force. Solute atoms can also segregate to the cores of dislocations and form atmospheres around dislocations and thus hinder, or even pin, their motion. Dislocations attract and repel other dislocations. Perhaps the most important example is the work hardening that occurs during the plastic deformation of crystals. Here, large numbers of dislocations are generated during the deformation; many remain in the crystal, where they act as obstacles to the passage of further dislocations, causing the material to strengthen and harden. At elevated temperatures during creep, gliding dislocations, which are held up at obstacles in their slip planes, can climb around them with the help of thermal activation (see the following section) and thus continue their glide. Grain boundaries act as barriers to slip, since, in general, a gliding dislocation will encounter a discontinuity in its slip plane and Burgers vector when it impinges on a boundary and attempts to pass through it into the adjoining grain. The host of interesting kinetic processes associated with the movement of dislocations through materials containing various obstacles to their motion is far too large to be described in this book. The reader is therefore referred to specialized texts [2, 791. 11.3.3
Some Experimental Observations
Figure 11.7 shows measurements of the velocity of edge and screw dislocation segments in LiF single crystals as a function of applied force (stress) [lo]. Stresses above a yield threshold stress were required for any motion. The velocity then increased rapidly with increasing stress but eventually began to level off as the velocity of sound was approached. Results within the significantly relativistic range were not achieved in these experiments, since for all measurements y~ x 1. It is likely that at the lower stresses (where the results are impurity sensitive), the velocities were limited by impediments arising from dislocationdislocation and dislocationdefect interactions [2]. This regime holds for the plastic deformation of essentially all crystalline materials deformed at normal strain rates. At the higher stresses in Fig. 11.7 (where the smaller slope is impurity insensitive and decreases with increasing temperature), the higher velocities were limited by phononviscosity drag. High dislocation velocities may be achieved at the start of even lowstrainrate deformation if the initial concentration of mobile dislocations is unusually low [ll]. In such cases, a small number of dislocations must move very rapidly to accom
ii 3: DISLOCATION GLIDE
265
107
105
103 I0 101
103 105
107 0.1
1
10
100
Applied shear stress (kg mm2)
Figure 11.7: crystals.
Velocity vs. resolved shear stress for dislocation motion in LiF single
From Johnston and Gilman [lo].
plish the strain required. Further experimental evidence has been presented for the strong frictional drag forces that come into play at high velocities approaching the relativistic range [ l l ] . Finally, it is noted that the viscous damping of dislocation motion converts mechanical energy to heat. This produces internal friction when a crystal containing a dislocation network is subjected to an oscillating applied stress (see Section 11.3.5). 11.3.4
Supersonic Glide Motion
If a dislocation is injected into a crystal at a speed greater than the speed of sound in the crystal, it will radiate energy in the form of sound waves similar to the way that a charged particle emits electromagnetic Cherenkov radiation when it is injected into a material at a velocity greater than the speed of light in that medium [5]. This causes rapid deceleration of the dislocation. However, steadystate supersonic motion of dislocations is possible in special cases where the motion of the dislocation in its glide plane causes a sufficiently large reduction in the energy of the system [2, 51. In such a case, this reduction of energy provides the energy that must be radiated during the supersonic motion. Conceivable examples include motion of a partial dislocation that removes its associated fault (see Fig. 9.10) or dislocation motion in a glissile martensitic interface (Section 24.3) , which converts the higher freeenergy parent phase to the lowerenergy martensitic phase. Models for the motion of such dislocations are entirely different from those discussed in Section 11.3.1 and are described by Nabarro [5] and Hirth and Lothe [2]. So far, there is no clear evidence for the supersonic motion of martensitic interfaces, probably due to the influence of frictional drag forces. However, there is some evidence that supersonic dislocations are present in shockwave fronts, as in Fig. 11.8 [12]. Models for the motion of such fronts have been described [ l l , 131, and some evidence for the existence of dislocations in them has been obtained by computer simulation [14].
266
CHAPTER 11 MOTION OF DISLOCATIONS
Figure 11.8: Possible interface between normal (lower) and compressed (upper) lattice in a shockwave front.
11.3.5
Contributions of Dislocation Motion to Anelastic Behavior
The stressinduced glide motion of dislocation segments in the dislocation networks usually present in materials can produce anelastic strains. (See the general discussion of anelasticity in Section 8.3.1.) If a segment that is pinned at its ends is subjected to an oscillating stress, it will periodically bow in and out in a manner similar to a vibrating string, as illustrated in Fig. 11.9. This will produce a small oscillating strain in the material. Because dissipative drag forces will be in play and the dislocation velocity is not infinite, this strain will lag the stress, causing internal friction [15]. Further aspects are considered in Exercise 11.12.
Figure 11.9: Dislocation segment pinned at A and B bowing out in the slip plane due to the applied shear stress, o.
11.4
DISLOCATION CLIMB
Figure 11.2 presents a simplified threedimensional representation of the climb of an edge dislocation arising from the destruction of excess vacancies in the crystal. The jogs (steps in the edge of the extra plane) in the dislocation core are the sites where vacancies are created or permanently destroyed. Vacancies can reach a jog by either jumping directly into it or else by first jumping into the dislocation core and then diffusing along it to a jog, where they are destroyed. The elementary processes involved include: 0
0
The jumping of a vacancy directly into a jog and its simultaneous destruction, as at A The jumping of a vacancy into the core, where it becomes attached as at B
11 4 DISLOCATION CLIMB
267
The destruction of an attached vacancy at a jog, as at C The diffusion of an attached vacancy along the core, as at D In many cases, vacancies are bound to the dislocation core by an attractive binding energy and diffuse along the dislocation more rapidly than in the crystal. Many more vacancies may therefore reach jogs by fast diffusion along the dislocation core than by diffusion directly to them through the crystal. The jogs required for the climb process can be generated by the nucleation and growth of strings of attached excess vacancies along the core. When a string becomes long enough, it will collapse to produce a fully formed jog pair, as, for example, in the region along the core bounded by A and C in Fig. 11.2. The spacing of the jog pair then increases due to the continued destruction of excess vacancies at the jogs until a complete row of atoms has been stripped from the edge of the extra plane. During steadystate climb, this process then repeats itself.
11.4.1 DiffusionLimited vs. SourceLimited Climb Kinetics A detailed kinetic model for the overall climb rate based on the above mechanisms has been developed [2, 1620]. In this model it is assumed that because the vacancies are easily destroyed at jogs, they are maintained at their equilibrium concentration in the immediate vicinity of the jogs. If the vacancies experience an attractive binding energy to the core and also diffuse relatively rapidly along it, a typical attached vacancy will diffuse a significantly large mean distance, ( Z ) ,along the core before it jumps back off into the crystal. The magnitude of ( 2 )increases with the binding energy of the vacancy to the dislocation and the relative rate of diffusion of the vacancy along the dislocation core. Each jog is therefore capable of maintaining the vacancy concentration essentially at equilibrium over a distance along the dislocation on either side of it equal approximately to the distance ( 2 ) . Each jog, with the assistance of the two adjoining segments of highdiffusivity core, therefore acts effectively as an ellipsoidal sink of semiaxes b and ( 2 )having a surface on which the vacancy concentration is maintained in local equilibrium with the jog. The overall effectiveness of the dislocation as a sink then depends upon the magnitude of ( 2 )and the mean spacing of the jogs along the dislocation, (S). When the vacancy supersaturation is small and the system is near equilibrium, the jog spacing will be given approximately by the usual Boltzmann equilibrium expression ( S )Z b exp[Ej/(kT)], where Ej is the energy of formation of a jog. However, at high supersaturations when excess vacancies can aggregate quickly along the dislocation and nucleate jogpairs rapidly, the number of jogs will be increased above the equilibrium value and their spacing will be reduced correspondingly [17, 181. A wide range of dislocation sink efficiencies is then possible. When 2 ( 2 ) / ( S )2 1, the effective jog sinks overlap along the dislocation line, which then acts as a highly efficient line sink capable of maintaining local vacancy equilibrium everywhere along its length. The rate of vacancy destruction is limited only by the rate at which the vacancies can diffuse to the dislocation, and the rate of destruction will then be the maximum possible. The kinetics are therefore daflusionlimited, and the dislocation is considered an “ideal” sink. Conditions that promote this situation are a high binding energy for attached vacancies, a relatively fast diffusion rate along the core, a small jog formation energy, and a large vacancy supersaturation.
268
CHAPTER 11 MOTION OF DISLOCATIONS
On the other hand, when the fast diffusion of attached vacancies to the jogs is impeded and (2)is therefore small (i.e., (2)2 b ) , each jog acts as a small isolated spherical sink of radius b. If, at the same time, (S) is large, the jog sinks are far apart and the overall dislocation sink efficiency is relatively small. Under these conditions the rate of vacancy destruction will be limited by the rate at which the vacancies can be destroyed along the dislocation line, and the overall rate of vacancy destruction will be reduced. In the limit where the rate of destruction is slow enough so that it becomes essentially independent of the rate at which vacancies can be transported to the dislocation line over relatively long distances by diffusion, the kinetics are sinklimited. When the dislocation acts as a sink for a flux of diffusing vacancies (or alternatively, as a source of atoms) or as a source for a flux of vacancies, it is useful to introduce a source or sink efficiency, 17, defined by flux of atoms created at actual source 17 = flux of atoms created at corresponding “ideal” source
(11.25)
A dislocation source that climbs rapidly enough so that ideal diffusionlimited conditions are achieved therefore operates with an efficiency of unity. On the other hand, slowly acting sources can have efficiencies approaching zero. Applications of these concepts to the source action of interfaces are discussed in Section 13.4.2. The climb of mixed dislocations possessing some screw character can proceed by basically the same jogdiffusion mechanism as that for the pure edge dislocation.1° On the other hand, a pure screw dislocation can climb if the excess vacancies convert it into a helix, as in Fig. 11.10. Here the turns of the helical dislocation possess
Figure 11.10: Formation of a helical segment on an initially straight screw dislocation lying along [loo] in a primitivecubic crystal by progressive addition of vacancies to the core. For graphic purposes, each vacancy is represented by a vacancytype prismatic loop of atomic size. (a) Vacancy in a crystal with an initial straight screw dislocation nearby. (b) Configuration after a vacancy has joined the dislocation. ( c )  (e ) Configurations after two, three, and four vacancies have been added. ‘ODetails are discussed by Balluffi and Granato [19].
11 4 DISLOCATION CLIMB
269
strong edge components and, once formed, continue to climb as mixed dislocation segments. Additional factors may play a role during dislocation climb in many systems. These include the possibility that jogs may be able to nucleate heterogeneously at nodes or regions of sharp curvature. Also, in low stackingfaultenergy materials, the dislocation may be dissociated into two partial dislocations bounding a ribbon of stacking fault as shown in Fig. 9.10. In such cases, the jogs may also be dissociated and possess a relatively high formation energy, causing the climb to be more difficult [2, 191. 11.4.2
Experimental Observations
Reviews of experimental observations of the efficiency with which dislocations climb under different driving forces have been published [18221. A wide range of semiquantitative results is available only for metals, including: Vacancy quenching experiments where the destruction rate at climbing dislocations of supersaturated vacancies obtained by quenching the metal from an elevated temperature is measured (see the analysis of this phenomenon in the following section) Dislocation loop annealing where the rate at which dislocation loops shrink by means of climb is measured (see analysis in following section) Sintering experiments where the rate at which vacancies leave voids and are then destroyed at climbing dislocations is measured Of main interest is the efficiency of climb and its dependence on the magnitude of the force driving the climb process. In general, the efficiency of climbing dislocations as sources increases as the driving force increases, since more energy is then available to drive the climb. A convenient measure of the relative magnitude of this force is the energy change, gsl which is achieved per crystal site created as a result of the climb. All dislocations, including dissociated dislocations in lowerstackingfaultenergy metals and relatively nondissociated dislocations in highstackingfaultenergy metals, operate as highly efficient sources when lgsj is large, as in rapidly quenched metals [20]. However, when lgsl is reduced, lower efficiencies, which may become very small, are found for the lowerstackingfaultenergy metals. The efficiencies for the higherstackingfaultenergy metals appear to fall off less rapidly with Jgs1. This may be understood on the basis of the tendency of the dislocations to contain more jogs as lgsl increases and the greater difficulty in forming jogs on dissociated dislocations than on undissociated dislocations because of the larger jog energies of the former. 11.4.3
Analyses of Two Climb Problems
Climbing Dislocations as Sinks for Excess Quenchedin Vacancies. Dislocations are generally the most important vacancy sources that act t o maintain the vacancy concentration in thermal equilibrium as the temperature of a crystal changes. In the following, we analyze the rate at which the usual dislocation network in a
270
CHAPTER 11: MOTION
OF DISLOCATIONS
crystal destroys excess supersaturated vacancies produced by rapid quenching from an elevated temperature during isothermal annealing at a lower temperature. If the dislocations in the network are present at a density Pd (dislocation line length per unit volume), a reasonable approximation is that each dislocation segment acts as the dominant vacancy sink in a cylindrical volume centered on it and of radius R = ( r p d )  l l 2 . The problem is then reduced to the determination of the rate at which excess vacancies in the cylinder diffuse to the dislocation line as illustrated in Fig. 11.11. The diffusion system is assumed to contain two components (Atype atoms and vacancies) and is network constrained. Equation 3.68 for the diffusion of vacancies is applicable in this case, and therefore +
J v = DVVCV
(11.26)
According to the results in Section 11.4.2, the dislocations should act as highly effective sinks for the highly supersaturated vacancies. We therefore assume diffusionlimited kinetics in which each dislocation segment is capable of maintaining the vacancies in local thermal equilibrium at its core, represented as a cylinder of effective radius R,, where R, is of atomic dimensions. Also, in this type of problem, the effect of the dislocation climb motion on the diffusion of the vacancies to the dislocation can be neglected to a good approximation [2, 231. Using the separationofvariables method (Section 5.2.4), the diffusion equation corresponding to Eq. 3.69, (11.27) may be solved subject to the conditions
c v = c? cv = c b dCV  0 dr
for r = R, and t 2 0 for R, < r 5 R and t = 0
(11.28)
forr=RandtLO
where c b is the quenchedin vacancy concentration and c? is the equilibrium vacancy concentration maintained at the “surface” of the dislocation core at the an
Figure 11.11: Vacancy diffusion fields in cylindrical cells (of radius R ) around dislocations acting as line sinks (of radius Ro).
11.4: DISLOCATION CLIMB
271
nealing temperature. The solution shows that the fraction of the excess vacancies remaining in the system decays with time according to (11.29) where the an are the roots of
Yo(Roan)Jl(Ran)  Jo(Roan)Yl(Ran) =0
(11.30)
and Jn and Yn are Bessel functions of the first and second kind of order n [24]. For typical values of Ro and R, the first term in Eq. 11.29 will be dominant except at very early times when the fraction decayed is small [24]. The major portion of the excess vacancy decay will therefore be essentially exponential [i.e., f ( t ) exp(a:Dvt)]. Finally, it is noted that the above treatment does not take account of the effect of the dislocation stress field on the diffusivity of the vacancies, as discussed in Section 3.5.2. In general, this stress field is of importance only within a relatively small distance from the dislocation. Under these circumstances, its effect during the major portion of the decay can be approximated in a simple manner by making a relatively small change in the value of the effective dislocation core radius, R, [25]. Since the roots of Eq. 11.30 are fairly insensitive to the value of Ro,the decay rate is also rather insensitive to this choice of R,. The effect of the stress field will therefore be relatively small. Shrinkage of Dislocation Loops by Climb. Prismatic dislocation loops are often
formed in crystals by the precipitation of excess vacancies produced by quenching or by fastparticle irradiation (see Exercise 11.7). Once formed, these loops tend to shrink and be eliminated by means of climb during subsequent thermal annealing. A number of measurements of loop shrinkage rates have been made, and analysis of this phenomenon is therefore of interest [2]. In this section we calculate the isothermal annealing rate of such a loop located near the center of a thin film in a highstackingfaultenergy material (such as Al) where the climb efficiency will be high, and the shrinkage rate is therefore diffusionlimited. The situation is illustrated in Fig. 11.12a. The loop is taken as an effective torus of large radius, R L ,with much smaller core radius, Ro,and the film thickness is 2d with d >> R L . The vacancy concentration maintained in equilibrium with the loop
Figure 11.12: (a) Vacancy diffusion fluxes around a dislocation loop (of radius R L ) shrinking by climb in a thin film of thickness 2d. (b) Spherical approximation of a diffusion field in (a).
272
CHAPTER 11: MOTION OF DISLOCATIONS
at the surface of the torus, c?(loop), is larger than the equilibrium concentration, c"vqco), maintained at the flat film surfaces. These concentrations can differ considerably for small loops, and the approximation leading to Eq. 3.72, which ignored variations in cv throughout the system, cannot be employed. Equation 3.69 can be used to describe the vacancy diffusion. Vacancies therefore diffuse away from the "surface" of the loop to the relatively distant film surfaces, and the loop shrinks as it generates vacancies by means of climb. The concentration, cT(loop), can be found by realizing that the formation energy of a vacancy at the climbing loop is lower than at the flat surface because the loop shrinks when a vacancy is formed, and this allows the force shrinking the loop (see Section 11.2.3) to perform work. In general, N;q = exp[Gf/(kT)] according to Eq. 3.65, and therefore (11.31) where Gf(m)  Gf(1oop) is the work performed by the force on the shrinking loop during the formation of a vacancy. The number of vacancies stored in the loop is NV = .irRib/R. The reduction in the radius of the loop due to formation of a vacancy by climb is then 6RL/6Nv =  R / ( 2 r b R ~ ) . Therefore,
R G;(CO)  Gv(loop) f =2.irbR~2 . i r ~ L 1 . 1 2
(11.32)

where the force has been evaluated with Eq. 11.8. The vacancy diffusion field around the toroidal loop will be quite complex, but at distances from it greater than about ~ R Lit ,will appear approximately as shown in Fig. 11.12a. A reasonably accurate solution to this complex diffusion problem may be obtained by noting that the total flux to the two flat surfaces in Fig. 1 1 . 1 2 ~ will not differ greatly from the total flux that would diffuse to a spherical surface of radius d centered on the loop as illustrated in Fig. 11.12b. Furthermore, when d >> R L ,the diffusion field around such a source will quickly reach a quasisteady state [20, 261, and therefore (11.33) v2cv = 0
(A justification of this conclusion will be obtained from the analysis of the growth of spherical precipitates carried out in Section 13.4.2.) In the steady state, the vacancy current leaving the loop can be written as
where C is the electrostatic capacitance of a conducting body with the same toroidal geometry as the loop placed at the center of a conducting sphere so that the geometry resembles Fig. 11.12b. This result is a consequence of the similarity of the concentration fields, c(z, y, z ) , and electrostaticpotential fields, $(z, y, z ) , which are obtained by solving Laplace's equation in steadystate diffusion (V2c = 0) and electrostatic potential (V2$ = 0) problems, respectively [20, 261. The shrinking
11.4: DISLOCATION CLIMB
273
rate of the loop is then
R bNv  RI 6t 2.irbR~ bt 2rbR~ _ 2r *D e p b C 2 / [ 4 x ( l  v ) k T R ~l ]n ( 4 R ~ / R , ) 1 f b In(8RL/Ro)
6RL 
(11.35)
This final result is obtained by using Eqs. 8.17, 11.31, 11.32, 11.34, and the relation C = nRL/ ln(8RL/Ro) for the capacitance of a torus in a large space when RL >> R, [27]. Analyses of the climbing rates of many other dislocation configurations are of interest, and Hirth and Lothe point out that these problems can often be solved by using the method of superposition (Section 4.2.3) [2]. In such cases the dislocation line source or sink is replaced by a linear array of point sources for which the diffusion solutions are known, and the final solution is then found by integrating over the array. This method can be used to find the same solution of the loopannealing problem as obtained above. As in Fig. 11.13, the loop can be represented by an array of point sources each of length R,. Using again the sphericalsink approximation of Fig. 11.12b and recalling that d >> RL >> R,, the quasisteadystate solution of the diffusion equation in spherical coordinates for a point source at the origin shows that the vacancy diffusion field around each point source must be of the form a1 (11.36) c:(r I )  cveq (m) = r’ where a1 is a constant to be determined. The value of a1 is found by requiring that the concentration everywhere along the loop be equal to c?(loop). This concentration is due to the contributions of the diffusion fields of all the point sources around the loop, and therefore, from Fig. 11.13 and using R, << R L ,
ceVq(1oop)  ceVq(m) = 2a1 =In 2al Ro
Figure 11.13: point sources.
(x) ~ R L
(11.37)
Annealing prismatic dislocation loop taken as a circular array of vacancy
274
CHAPTER 11: MOTION OF DISLOCATIONS
Note that the integral is terminated at the cutoff distance R0/2 in order to avoid a singularity. The vacancy concentration at a distance from the loop appreciably greater than RL can now be found by treating the loop itself as an effective point source made up of all the point sources on its circumference. The number of these R , ,therefore sources is ~ T R L ~ and
The vacancy current leaving the loop is then
d ~ R L [c7(lOOp)  c ~ ( c o ) ] I = 4 r r 2 D v  [cv(r)]= 47rDv dr In(~ R/ R Lo )
(11.39)
in agreement with the results of the previous analysis. Applications of Eq. 11.35 and closely related equations to the observed annealing rate of loops have been described [19, 281. Bibliography 1. S.M. Allen and E.L. Thomas. The Structure of Materials. John Wiley & Sons, New York, 1999.
2. J.P. Hirth and J. Lothe. Theory of Dislocations. John Wiley & Sons, New York, 2nd edition, 1982. 3. I.S. Sokolnikoff. Mathematical Theory of Elasticity. McGrawHill, New York, 1956. 4. J. Weertman. High velocity dislocations. In P.G. Shewmon and V.F. Zackay, editors, Response of Metals to High Velocity Deformation, pages 205247, New York, 1961. Interscience. 5. F.R.N. Nabarro. Theory of Crystal Dislocations. Clarendon Press, Oxford, 1967. 6. C. Kittel. Introduction to Solid State Physics. John Wiley & Sons, New York, 3rd edition, 1967. 7. F.R.N. Nabarro, editor. Dislocations in Solids (Series), volume 112. Elsevier NorthHolland, New York, 19792004.
8. J. Friedel. Dislocations. Pergamon Press, Oxford, 1964. 9. U.F. Kocks, A.S. Argon, and M.F. Ashby. Thermodynamics and kinetics of slip. Prog. Muter. Sci., 19:l288, 1975. 10. W.G. Johnston and J.J. Gilman. Dislocation velocities, dislocation densitites, and plastic flow in lithium fluoride crystals. J. Appl. Phys., 30(2):129144, 1959. 11. J. Weertman. Dislocation mechanics at high strain rates. In R.W. Rohde, B.M. Butcher, J.R. Holland, and C.H. Kames, editors, Metallurgical Eflects at High Strain Rates, pages 319332, New York, 1973. Plenum Press. 12. C.S. Smith. Metallographic studies of metals after explosive shock. Trans. A I M E , 212( 10):574589, 1958. 13. J. Weertman. Plastic deformation behind strong shock waves. Mech. Muter., 5(1):1328, 1986.
14. B.L. Holian. Modeling shockwave deformation via moleculardynamics. Phys. Rev. A , 37(7):25622568, 1988. 15. A S . Nowick and B.S. Berry. Anelastic Relaxation in Crystalline Solids. Academic Press, New York, 1972.
EXERCISES
275
16. J. Lothe. Theory of dislocation climb in metals. J. Appl. Phys., 31(6):10771087, 1960. 17. R.M. Thomson and R.W. Balluffi. Kinetic theory of dislocation climb I. General models for edge and screw dislocations. J . Appl. Phys., 33(3):803817, 1962. 18. R.W. Balluffi. Mechanisms of dislocation climb. Phys. Status Solidi, 31(2):443463, 1969. 19. R.W. Balluffi and A. V. Granato. Dislocations, vacancies and interstitials. In F.R.N. Nabarro, editor, Dislocations in Solids, volume 4, pages 1133, Amsterdam, 1979. NorthHolland. 20. A.P. Sutton and R.W. Balluffi. Interfaces in Crystalline Materials. Oxford University Press, Oxford, 1996. 21. D.N. Seidman and R.W. Balluffi. Dislocation as sources and sinks for point defects in metals. In R.R. Hasiguti, editor, Lattice Defects and Their Interactions, pages 911960, New York, 1967. Gordon and Breach.
22. R.W. Balluffi. Voids, dislocation loops and grain boundaries as sinks for point defects. In M. T. Robinson and F.W. Young, editors, Proceedings of the Conference on Fundamental Aspects of Radiation Damage in Metals, volume 2, pages 852874, Springfield, VA, 1975. National Technical Information Service, US.Department of Commerce. 23. R.W. Balluffi and D.N. Seidman. Diffusionlimited climb rate of a dislocation: Effect of climb motion on climb rate. J . Appl. Phys., 36(7):27082711, 1965.
24. D.N. Seidman and R.W. Balluffi. Sources of thermally generated vacancies in single crystal and polycrystalline gold. Phys. Rev., 139(6A):18241840, 1965. 25. F.S. Ham. Stress assisted precipitation on dislocations. J . Appl. Phys., 30(6):915926, 1959. 26. C.P. Flynn. Monodefect annealing kinetics. Phys. Rev., 133(2A):A587,1964. 27. H. Buchholz. Electrische und Magnetische Potentialfelder. SpringerVerlag, Berlin, 1957. 28. D.N. Seidman and R.W. Balluffi. On the annealing of dislocation loops by climb. Phil. Mag., 13:649654, 1966. 29. J. Bardeen and C. Herring. Diffusion in alloys and the Kirkendall effect. In J.H. Hollomon, editor, Atom Movements, pages 87111. American Society for Metals, Cleveland, OH, 1951. 30. W.T. Read. Dislocations in Crystals. McGrawHill, New York, 1953.
EXERCISES 11.1 Show that Eq. 11.4 for the osmotic force on an edge dislocation may be generalized for a mixed dislocation in the form
where

kT B = b In R
(s)
(11.40)
(11.41)
276
CHAPTER 11: MOTION OF DISLOCATIONS
Solution. The climb force is normal t o the glide plane, which contains both the Burgers vector and the tangent vector. The unit normal vector t o the glide plane is therefore
so
(11.42) Since the climb distance t h a t results from the destruction of 6Nv vacancies is now ) ~ N vusing , Eqs. 3.64 and 3.66,
11.2 Interpret the line tension, p b 2 , of a dislocation to be a force that acts along its length in a direction to decrease its length (see Eq. 11.9). Using a simple geometrical argument, show that the curvature force per unit length of dislocation acting locally on a curved segment of dislocation is then just = pb2/R, where R is the radius of curvature.
/f;cl
Solution. The linetension forces acting on a curved differential segment of dislocation having a radius o f curvature R due t o its line tension will be as shown in Fig. 11.14. The net force exerted on the segment toward the concave side is then
df = 2pb2 sin
pb2 ds (f) pb2 dB = R M
(11.44)
and therefore
(11.45)
ds
Figure 11.14: Line tension forces on a curved dislocation segment.
11.3 Use Eq. 11.12 to show that a dislocation in a crystal possessing a uniform nonequilibrium concentration of point defects and a uniform stress field will
EXERCISES
277
tend to adopt a helical form. Note that both a circle and a straight line are special forms of a helix. Solution. The dislocation will tend t o adopt a form for which the net force on i t given by Eq. 11.12 is everywhere zero. We therefore want t o show that a helical dislocation will possess a tangent vector f that satisfies p b2 d+t [ x ( d  d ) = O
( 11.46)
ds
To evaluate
t , we recall that the equation for a helix with i t s axis along z is F = iacose + j a s i n e
+ Lpe
(11.47)
where 6 is the polar angle in the zyplane, a is the radius of the circular projection on the zyplane, and 27rp is the distance between successive turns along z . Therefore,
dr' < =  = [  ' ;a sine A
ds
and
dt
d2r'
+ j a cos e + Lp]
1
Jm
(11.48)
a
(11.49)    = [icose+jsine]ds ds2 a2 + p 2 Comparing the last result with Eq. 11.10, we see that the curvature given by IC = ./(a2 + p 2 ) is constant everywhere and that the principal normal vector at any point :0 the hzlix is pointed toward the helix axis and is perpendicular t o it. Also, the vectors B and d are constant vectors independent o f (. If we now take the axis of the helix t o be along
A
(2d', so t h a t (d  d', = L (B 
we find that it is satisfied if
4
and put the results above into Eq. 11.46, (11.50)
Note t h a t the solution has the form o f a circle when p = 0 and a straight line along the axis when p + m.
11.4 When a metal crystal free of applied stress and containing screw dislocation segments is quenched so that supersaturated vacancies are produced, the screw segments are converted into helices by climb. Show that the converted helices can be a t equilibrium with a certain concentration of supersaturated vacancies and find an expression for this critical concentration in terms of appropriate parameters of the system. Use the simple linetension approximation leading to Eq. 11.12. We note that the helix will grow by climb if the vacancy concentration in the crystal exceeds this critical concentration and will contract if it falls below it. S o h t i o n . In this case, c i = 0, and therefore we must have (11.51) The axis of the helix is parallel t o g, which, in turn, is parallel t o Eq. 11.50 of Exercise 11.3 applies in the form
g,
and therefore
(11.52)
278
CHAPTER 11: MOTION OF DISLOCATIONS
The concentration is therefore
(11.53)
11.5 Show that regardless of the orientation of a straight dislocation line and its Burgers vector, there will exist a stress system that will convert the dislocation line into a helix whose axis is along the position of the original dislocation when the pointdefect concentration is at the equilibrium value characteristic of the stressfree crystal. Use the simple linetension approximation leading to Eq. 11.12. Solution. In this case, the equation
= 0 and the equilibrium shape o f the dislocation must satisfy 2d(

f=pb <xd=O +
ds
(11.54)
The vector Z i s given by Eq. 11.3, and because the six stre_sses are independent of each other, a value o f the stress tensor may be found so that d is parallel t o the dislocation line. As shownin Exercise 11.3, a solution of Eq. 11.54 corresponding t o a helix with its axis along d can then be found.
11.6 Show that the effective mass per unit length of a moving screw dislocation is m* = Wo/c2when its velocity is relatively small compared with c. 0
Expand Eq. 11.20 to first order in ( u / c ) and ~ examine the form of the result.
Solution. Expanding Eq. 11.20 t o first order in ( w / c )produces ~ the result
( 11.55) which is seen t o have the form o f a rest potential energy plus a kinetic energy involving an effective mass given by W o / c 2 Therefore, . a t relatively small velocities, the inertia of the regions that must be displaced as the dislocation moves produces the same effects as if the dislocation possessed the mass m*.
11.7 (a) Describe how excess supersaturated vacancies in a crystal can precipitate and collapse to form a prismatic dislocation loop. (A prismatic dislocation loop is a loop whose Burgers vector possesses a component normal to the plane of the loop. It therefore can glide out of the loop plane.)
(b) Find an expression for the number of vacancies required to form a circular loop of radius R. Solution. (a) The vacancies can precipitate in the form of a planar layer as shown in Fig. 11.156. If the vacancy precipitate then collapses as shown in Fig. 11.15c, a prismatic dislocation loop will be produced. In essence, this process removes a circular patch o f one o f the ( h k l ) planes as shown. The Burgers vector of the loop will have a component normal t o the loop plane equal t o the interplanar spacing d h k l . If there is a shear displacement, S, parallel t o the loop plane during the collapse,
EXERCISES
279
the Burgers vector will also have a component in the loop plane equal t o S. The free energy o f the supersaturated vacancies is generally greater than the free energy of the resulting loop and therefore there is an excess o f free energy available t o drive the loop formation.
Figure 11.15: Formation of prismatic dislocation by vacancy precipitation and collapse. (a) Excess vacancies dispersed in crystal. (b) Precipitation of excess vacancies. ( c ) Collapse of vacancy precipitate to form dislocation loop. (b) The loop may be constructed formally by making a cut parallel t o the loop plane and removing a circular disc o f material of area xRT and thickness d h k l and then displacing the two circular faces of the cut by b so that they are joined together. The volume o f material that must be removed in this operation is then V = iiR2dt,k, = .irR2G.6 ,where fi is a unit vector normal t o the loop plane. The number of vacancies required t o remove this volume of material is then (11.56)
11.8 Find the number of supersaturated vacancies that must diffuse to a unit length of climbing screw dislocation to convert it into a helix of radius a. turn spacing 2 ~ p and . Burgers vector length b. Solution. The helical dislocation may be regarded as equivalent t o a stack o f circular prismatic edge dislocation loops of radius a as illustrated in Fig. 11.16. This may be confirmed by realizing that the stack o f loops can be converted into a helix in a conservative fashion by cutting each loop a t its intersection with A B and then sliding
Figure 11.16: (a) A stack of four prismatic edge dislocation loops perpendicular to A B arid also tangent to A B at the points indicated. ( b ) Helix formed from loops in (a).
280
CHAPTER 11 MOTION OF DISLOCATIONS
various segments of each loop along the cylindrical glide surface in an appropriate way t o form a continuous helix after joining the free ends. Each prismatic loop contains N = na2b/R collapsed vacancies. The total number of vacancies, Ntot,required per unit length of helix is then
N  a2b N tot = 2np 2pR
(11.57)
11.9 Bardeen and Herring first pointed out that if the pinned dislocation segment in Fig. 11.17 has its Burgers vector normal to the plane of the paper, it can act as an infinite source or sink for vacancies (and also as a source for dislocation loops) [29]. As the segment climbs by creating (destroying) vacancies, it bulges as shown in Fig. 11.17b. Upon further climb it creates a surrounding closed loop as seen in Fig. 1 1 . 1 7 ~and d. This process can then repeat itself, producing further loops.
Suppose now that such a source is present in a crystal that is rapidly quenched from a temperature Tqto a temperature T, to produce supersaturated vacancies. Find an expression for the critical value of the quenching temperature, Tq,which must be used to produce sufficient supersaturation to activate the source so that it will be able to create dislocations loops capable of destroying the supersaturated vacancies by climb. The vacancy formation energy is E& and the segment length is L.
Figure 11.17: Generation of a dislocation loop by expansion of a dislocation segment with ends pinned at A and B . Solution. The source will be able t o become active if the driving osmotic climb force is large enough t o overcome the restraining curvature force that reaches a maximum when the dislocation segment has bowed out t o the minimum radius of curvature corresponding t o R = L/2. Setting f, = f n , we then have the critical condition
(11.58) Since form
XV = A exp[E{/(kT,)]
and X;q = Aexp[Ef/(kT,)], we obtain T, in the
Tq =
T, 1  2pbR/(LEf)
( 11.59)
11.10 Imagine that the Burgers vector of the dislocation segment in Fig. 11.17a lies in the plane of the figure rather than normal to it as in Exercise 11.9. Frank
EXERCISES
281
and Read first pointed out that the configuration in Fig. 1 1 . 1 7 ~could then act as a source for a large number of dislocation loops which would expand by glide rather than climb (as in Exercise 11.9) in the presence of a sufficiently large shear stress, CT,parallel to the plane of the paper [30]. Find an expression for the critical stress, o,., required to activate such a source. Solution. The source will become active when the forward driving force due t o the stress is large enough t o overcome the maximum restoring force due t o curvature which occurs when the dislocation segment has bowed out t o the minimum radius o f curvature corresponding t o R = L / 2 . Setting fo = fn, we then have the critical condition pb2 gb==
“
2pb2
R
L
(11.60)
so that ffc
=2Pb
L
(11.61)
11.11 Two parallel edge dislocations of opposite sign, spaced a distance 1 apart, lie along the center of a cylindrical body of radius, R, as shown in Fig. 11.18, with R >> 1 >> R,, where R, is the dislocation core diameter. The two dislocations attract one another with a force (per unit length) given by Pb2
= 2 4 1  v)1
(11.62)
At an elevated temperature, they will therefore climb toward one another and eventually anneal out. Obtain an expression for the rate at which they approach each other. Assume diffusionlimited climb, that the diffusion is by a vacancy mechanism, and that no other sources or sinks are present except for the surface. 0
Use the method of superposition described at the end of Section 11.4.3.
Figure 11.18: Two closely spaced edge dislocations of opposite sign at the center of a large cylindrical body.
Solution. Because o f the interaction between the two dislocations, the work required t o produce a vacancy a t either dislocation and cause it t o climb in the direction o f the attractive force is reduced by the force by the amount f f l / b . The equilibrium vacancy
282
CHAPTER 11: MOTION OF DISLOCATIONS
concentration a t each dislocation, cy(disl), is therefore higher than the concentration in equilibrium with the surface of the cylinder, cy(m). Vacancies will therefore diffuse from each climbing dislocation t o the surface of the cylinder and the dislocations will climb toward one another. Using the same procedures used t o treat the problem of the shrinkage o f dislocation loops in Section 11.4.3, and described for this particular problem by Hirth and Lothe [2], we therefore have
c"vqdis1)  cy(co) = cy(m) [e
fR'(bkT)
 11
(11.63)
The solution o f the diffusion equation for the quasisteady state in cylindrical coordinates shows that each dislocation line source will have a vacancy concentration difFusion field around i t o f the form
cv(r')  c","m) = a1 In
($) + a z
(11.64)
where a1 and a2 are constants. The constants can be obtained from the conditions that the concentration a t each dislocation produced by the superimposed diffusion fields of the two dislocations must correspond t o the equilibrium concentration, cy(disl), and that the concentration a t the surface must be c y ( m ) . Taking an origin a t one dislocation, these conditions are therefore
(&) +
a1 In a1 \fro/
a1 In
(4)+ (11
2a2 = cy(dis1) a2 = C X m )
(11.65)
2
A t a distance from the two closely spaced dislocations appreciably greater than 1, the concentration due t o their superimposed difFusion fields will then be
c v ( r )  c"v"m) =
cy(dis1)  c y ( m ) ln(R/a)
(11.66)
The vacancy current diffusing away from the two dislocations is then
I = 27rrDv
dcv 27rDv [cy(disl)  c y ( m ) ] = dr ln(R/a)
(11.67)
Finally, making use of Eqs. 8.17 and 11.63, the velocity o f approach is
2,
= 1 s1 =
27r*D
b
[
efn/(kTb)

fbI n ( R / a )
( 11.68)
11.12 Consider a segment of dislocation in the dislocation network of a crystal pinned at its ends and lying in its slip plane as in Fig. 11.9. Suppose that an oscillating shear stress of the form g
= g,eiwt
(11.69)
is imposed along the slip plane, causing it to bow out.
(a) Describe qualitatively the stressinduced motion of the segment. (b) Write the equation of motion of the segment taking into account all of the forces acting on it, including the influence of its effective mass (Ex
EXERCISES
283
ercise 11.6), the frictional drag force (Section 11.3.1),and the curvature force (Section 11.2.3). 0 0
Assume that the stress is relatively small. Any lateral displacement of the segment will be small compared to its length; and the drag force can be taken as viscous (i.e., proportional to the dislocation velocity).
Solution.
(a) The applied stress exerts a force on each element of the segment, bowing i t out laterally in the slip plane. As the stress oscillates, the segment is forced t o bow backward and forward much in the manner o f a vibrating string.
(b) The equation o f motion will be of the form (11.70) where u(y, t ) is the displacement in the 2 direction. The first term is the inertial term proportional t o the acceleration d 2 u /d t2 and the effective mass per unit length m*. The second is the viscous damping term that is proportional t o the velocity au/dt ( B is a damping constant). The third term is the restoring force proportional t o the curvature d 2 u / d y 2 ,and the fourth term is the oscillating driving force ba. Solutions t o Eq. 11.70 have been found, and further development of the model is given by Nowick and Berry [15].
CHAPTER 12
MOTION OF CRYSTAL/VAPOR AND CRYSTAL/LIQUID INTERFACES
A vast number of engineering materials are used in solid form, but during processing may be found in vapor or liquid phases. The vaporhsolid (condensation) and liquidjsolid (solidification) transformations take place at a distinct interface whose motion determines the rate of formation of the solid. In this chapter we consider some of the factors that influence the kinetics of vapor/solid and liquid/solid interface motion. Because vapor and liquid phases lack longrange structural order, the primary structural features that may influence the motion of these interfaces are those at the solid surface.
12.1 T H E R M O D Y N A M I C SOURCES OF INTERFACE M O T I O N An interface has an effective driving pressure if its displacement decreases the total system’s free energy. This effective pressure can derive from any mechanism by which a material stores energy, but for many cases it arises from only two sources: the volumetric freeenergy differences between the interface’s adjacent phases, and mechanical pressure differences due to reduction of the interfacial energy. The conditions and kinetic equations for phase transformations are treated in Chapters 17 and 20 and involve local changes in freeenergy density. The quantification of thermodynamic sources for kinetically active interface motion is approximate for at least two reasons. First, the system is out of equilibrium (the transformations are not reversible). Second, because differences in normal component of mechanical stresses (pressures, in the hydrostatic case) can exist and because the thermal conKinetics of Materials. By Robert W . Balluffi, Samuel M. Allen, and W . Craig Carter. Copyright @ 2005 John Wiley & Sons, Inc.
285
286
CHAPTER 12: MOTION OF CRYSTALLINE SURFACES
ditions of interfacial motion are systemspecific (i.e., interfacial motion can involve the generation of heat), identification of the appropriate minimizing system free energy is troublesome. However, if the interface’s adjacent phases are treated as nearequilibrium and if the total free energy, 6, can be used as a placeholder for the appropriate free energy, the effective driving pressure due to phase transformations can be modeled roughly with (12.1)
where 66 is the change in total free energy when interface with area A moves normal to itself by a distance Sx, AG is the difference in free energy per atom, and R is related t o the atomic volumes, which may differ, in each phase. For a liquid/crystal interface that moves as the undercooled liquid crystallizes a t temperature T , a model for Phase trans can be developed. Using AG(T) = A H ( T ) T A S ( T )and treating the volumetric heat capacities as temperature leads to the approximation independent, AS(Tm)= AH(Tm)/Tm,
where the undercooling is A T = Tm T . The approximation from Eq. 12.1 shows that (12.3) is proportional to the undercooling. The surface energy per area, y, has the same units as a force per length and for some interfacial geometries can lead to an interfacial net force that is balanced by a difference in pressure between the two adjacent phases. If y is isotropic, this pressure difference is directly proportional to the interfacial curvature through the the GibbsThomson equation (see Sections C.2.1 and C.4.1), (12.4) where the Ri are the principal radii of curvature and K is the mean curvature. The pressure is higher on the side that contains the center of curvature (e.g., the pressure inside a soap bubble is larger than the ambient pressure). A P = y ~is.the thermodynamic potential to move a small volume R across an isotropic interface, absent any chemical or other effects. 12.2
M O T I O N O F CRYSTAL/VAPOR INTERFACES
Crystals grow from their supersaturated vapor by the addition of vapor atoms at their free surfaces. In this process, the surface is subjected to an effective pressure due t o the difference in free energy between the solid and vapor. The interface moves outward toward the vapor as it acts as a sink for the incoming flux of atoms. The mechanism by which atoms leave the vapor phase and eventually become permanently incorporated in the crystal is often relatively complex, and the kinetics of the process depends upon the type of surface involved (i.e., singular, vicinal,
12 2 MOTION OF CRYSTAL/VAPOR INTERFACES
287
or general). Also, crystal growth from the vapor is generally anisotropic because surfaces of different inclination (indices) usually possess different structures. Another type of motion of crystal/vapor interfaces occurs when a supersaturation of vacancies anneals out by diffusing to the surface where they are destroyed. In this process, the surface acts as a sink for the incoming vacancy flux and the surface moves inward toward the crystal as the vacancies are destroyed. This may be regarded as a form of crystal dissolution, and the kinetics again depend upon the type of surface that is involved. 12.2.1
Structure of Crystal/Vapor Surfaces
Just as for grain boundaries, crystal surfaces at equilibrium with their vapor can be singular, vicinal, or genera1.l As explained in Section 9.1 and Appendix B, an interface is regarded as singular with respect to a degree of freedom if it is at a local minimum of energy with respect to changes in that degree of freedom. Such surfaces correspond to the bases of cusps on the surface of the Wulff plot. These surfaces are generally of low index and high atomic density and exist at low temperatures relative t o their melting points. Surfaces with inclinations close to those of singular surfaces and having energies lying on the sides of cusps are composed of discrete steps and terraces corresponding t o the structures of their nearby singular surfaces and are classified as vicinal (see Fig. B.l and Exercise 12.9). Surfaces far from singular and vicinal inclinations have highly stepped and irregular structures of higher energies and are therefore general. As the temperature is raised, singular and vicinal surfaces tend t o undergo a roughening transition in which they develop highly stepped and irregular structures. During this transition, the ledges roughen as a result of the thermal generation of surface and ledge vacancies, adatoms, and vacancy and adatom clusters (Fig. 12.1). Ledge vacancy clusters and adatom clusters (which form in strings along the ledge) are topologically equivalent to pairs of kinks on the ledges. The roughening occurs because of the configurational entropy that is contributed by the structural disorder (see Exercise 12.7). This process is therefore thermodynamically similar to the thermal generation of equilibrium vacancies in the bulk. In general, the more singular a surface, the higher the temperature at which it will roughen. The roughening Surface vacancy
Figure 12.1:
Ledge
atom
Various point arid line defects on a vicinal crystal/vapor surface.
'See Appendix B for further discussion of t h e structure of surfaces.
288
CHAPTER 12: MOTION OF CRYSTALLINE SURFACES
of a (40 0 1) vicinal surface during heating, as determined by computer simulation, is shown in Fig. 12.2. Surfaces that have become roughened in this manner must now be classified as general.
T , = 0.025
T, = 0.0375
T, = 0.05
T, = 0.075
Figure 12.2: A MonteCarlo simulation of roughening of a [40 0 11 vicinal surface in a primitive cubic crystal with first and secondneighbor pair interactions. El and E2. The binding enthalpy Affblnd = 6E1+12Ez and the calculations were performed at the indicated values of the reduced temperature defined by T, = kT/AHblnd, with Ez = 0.66E1.
12.2.2 Crystal Growth from a Supersaturated Vapor Singular and Vicinal Crystal Surfaces. Kinks on ledges are the only places on a vicinal surface where an incoming atom from the vapor can become fully incorporated in the crystal with its full binding energy. These kinks therefore play the same role during crystal growth as jogs on dislocations during dislocation climb.2 If ledges with kinks are present, the incoming atoms can be incorporated at the kinks by several mechanisms. The mechanisms are illustrated in Fig. 12.3 and include: 0
Direct impingement on the surface of an atom from the vapor, as at A
0
Direct impingement on a ledge of an atom from the vapor. as at B
0
0
0
0
Direct impingement on a kink of an atom from the vapor and its incorporation into the crystal, as at C Jumping of an adatom into a kink from the surface by surface diffusion and its incorporation into the crystal, as at D Jumping of an adatom onto a ledge by surface diffusion, as at E Jumping of an adatom attached to a ledge into a kink and its incorporation into the crystal, as at F
'This is demonstrated in Exercise 12.1.
12.2: MOTION OF CRYSTAL~VAPORINTERFACES
A
C
? ! ?
289
B
e I
Figure 12.3: Elementary processes at vicinal surface during crystal growth from a supersaturated vapor.
Because the adatoms diffuse relatively rapidly along the surface and the ledges to the kinks, many more atoms reach the kinks by these routes than by direct impingement from the vapor. Note the close similarity between this crystal growth process on a vicinal surface and the climb of dislocations depicted in Fig. 11.2. When the surface is initially vicinal, it contains a population of ledges, and growth can then occur by the incorporation of adatoms at the ledges. The efficiency of the surface as a sink for the incoming atoms varies widely depending upon a number of factors. It is usually assumed that sufficient kinks are present at normal growth temperatures so that the ledges act as highly efficient line sinks for the incorporation of adatoms (see Exercise 12.1). If most adatoms jump back into the vapor phase before reaching a ledge, the sink efficiency will be low. This is a result of a small energy of adatom adsorption, a low rate of diffusion on the surface, and a large spacing between ledges. On the other hand, a high surface sink efficiency, corresponding to 17 = 1 (see Eq. 11.25); can be achieved if the relative magnitudes of the above parameters are reversed and essentially all adatoms that arrive from the vapor become incorporated at ledges before rejoining the vapor. These variables have been considered in analytical treatments of crystal growth [l] and in Exercise 12.1. In Exercise 12.2 it is shown that the growth velocity can be expressed in the form
u = K ( P  P"")
(12.5)
where P is the pressure of the vapor in the system, Peq is the vapor pressure that would be in equilibrium with the surface, and K is a rate constant that is proportional to the efficiency, 7, of the surface as a sink for the impinging vapor atoms. If the surface acts as an ideal sink, 17 = 1 and u will be proportional to ( P  Peq) as indicated by the ideal sink curve in Fig. 12.4. Otherwise, the curve of ZI vs. ( P  P"") will fall below the ideal sink curve. An initially singular and atomically flat surface advances only if ledges, possessing kinks, are nucleated and formed on the surface. This can occur if adatoms cluster together on the surface and nucleate new ledges at small pillboxshaped clusters of adatoms as indicated in Fig. 12.1. The free energy to form such a cluster
290
CHAPTER 12. MOTION OF CRYSTALLINE SURFACES
Figure 12.4: Crystal growth velocity 71 as a fuiiction of excess vapor pressure ( P  P""). Ideal sink curve pertains when all impinging adatoms are incorporated. Screw dislocation ledges curve pertains when ledges associated with screw dislocations limit the kinetics. Twodimensional nucleation curve pertains when twodimensional nucleation of ledges is ratelimiting.
is
AGClUSt 
nR2h
 2rcRgL  R
(12.6)
where R is the cluster radius, gL is the ledge energy per unit ledge length, h is the ledge height, P is the actual vapor pressure, and Peq is the equilibrium vapor pressure of the bulk crystal. The radius of the critical cluster for nucleation (see Section 19.1) obtained from the condition 6'AGc1Ust/dR= 0 is R 

gLR hkTln(P/Peq)
(12.7)
The role of ledge nucleation on the kinetics of crystal growth can now be explored.
If the surface is initially singular, no growth occurs a t very low supersaturations
where, according to Eq. 12.7, R, is relatively large. There are no ledges under these conditions because the critical free energy for nucleation is so large that the nucleation rate is negligible.3 However, as the supersaturation is increased and R, is decreased, the nucleation rate of ledges will at some point increase rapidly, and a significant density of ledges and kinks will appear on the surface. For the initially singular surface, the curve of v vs. P  Peq as a function of increasing P  P"q (Fig. 12.4) therefore exhibits a negligible growth rate a t small values of P Peq but increases extremely rapidly when the supersaturation reaches a value where copious ledge nucleation occurs, and from there it follows closely the ideal sink curve. In this situation, the initially singular surface has become effectively roughened in the presence of the large driving force for its motion. Ledge nucleation for crystal growth can be bypassed in many cases if the crystal contains dislocations. If a dislocation impinges on a singular surface and has a component of its Burgers vector normal to the surface, it is topologically necessary that a ledge be present on the surface as illustrated in Fig. 1 2 . 5 ~ .Adatoms can then become incorporated in the crystal at the ledge, causing it to move normal to itself in the directions of the arrows in Fig. 12.5. The ledge therefore wraps itself up into a spiral configuration centered on the dislocation and the total length 3See Chapter 19 for a treatment of thc kinetics of nucleation.
12.2:MOTION OF CRYSTAL~VAPORINTERFACES
291
Figure 12.5: Formation of a spiral ledge on the surface of a crystal growing from the vapor phase at the intersection of a screw dislocation with the surface at the point S.
of ledge available t o support crystal growth increases continuously. Dislocations of this type provide readymade sources of ledges and crystal growth occurs in the absence of any ledge nucleation. When such sources of ledges are present, significant crystal growth occurs at lower vapor supersaturations than those required for ledge nucleation and analysis of the growth kinetics shows that the v vs. P  Peq curve appears as in Fig. 12.4 [l]. General Crystal Surfaces. General surfaces possess a high density of sites where atoms from the vapor can be incorporated in the crystal and are therefore expected to operate as essentially ideal sinks. Crystal growth from the vapor is often anisotropic, with singular and vicinal surfaces having lower mobilities than general surfaces. In such cases, any fastmoving surface inclinations bounding a growing crystal grow out of existence, leaving behind only slowgrowing inclinations. The result is a faceted crystal bounded by slowmoving inclinations. Anisotropic growth when the growth velocity is a known function of surface inclination is analyzed in Section 14.2.2. There is a body of experimental evidence generally supporting the models above for growth at the different types of surfaces [l].
12.2.3 Surfaces as Sinks for Supersaturated Lattice Vacancies When a crystal surface acts as a sink for supersaturated vacancies, atoms are supplied from the surface to replace the incoming flux of vacancies. The process of crystal dissolution that occurs is, in many respects, the opposite of the crystal growth process described above. Vacancies diffusing to the surface become surface vacancies and may then either leave the surface by jumping back into the crystal bulk or, in vicinal surfaces, diffuse in the surface to ledges, where they become ledge vacancies, which are eventually destroyed at kinks by being replaced by lattice atoms. The sink efficiency of the surface is high if most of the surface vacancies are destroyed at the kinks before reentering the lattice. The analysis of the sink efficiency is then analogous to the preceding analysis of crystal growth at vicinal surfaces. When the surface is initially singular, the required ledges can be nucleated by the clustering of supersaturated surface vacancies in monolayer surface cavities or
292
CHAPTER 12. MOTION OF CRYSTALLINE SURFACES
they can be supplied by impinged dislocations having Burgers vector components normal to the surface. The driving pressure for the nucleation of the ledges is the vacancy supersaturation rather than the vapor supersaturation as in the previous crystal growth situation. Otherwise, the general features of the surface as a sink for vacancies are similar to those of the surface as a sink for atoms during growth from the vapor. General surfaces possess a high density of kinks at which vacancies are easily destroyed, and they thus have a high sink efficiency. Gold (100) surfaces are highly efficient sinks for supersaturated vacancies produced by quenching [2]. In this case, the process is undoubtedly aided by the high degree of supersaturation of the quenchedin vacancies. 12.3 12.3.1
M O T I O N OF INTERFACES DURING SOLIDIFICATION Structure of Crystal/Liquid Interfaces
Because experimental study of the structure of crystal/liquid interfaces has been difficult due to the buried nature of the interface and rapid structural fluctuations in the liquid, it has been investigated by computer simulation and theory. Figure B.3 provides several views of crystal/liquid (or amorphous phase) interfaces, which must be classified as diffuse interfaces because the phases adjoining the interface are perturbed significantly over distances of several atomic layers. A critical question has been whether crystal/liquid interfaces are usually rough (and therefore general) or singular or vicinal. Jackson developed a simple statistical mechanical model in which adatoms were added to a crystal/liquid interface possessing an initially smooth crystal face [3]. The model shows that the interface remains smooth, and hence singular, whenever the dimensionless parameter Q = (AS,/k) ( T ] / z )is of magnitude Q > 2 and is rough (general) otherwise. Here, AS, is the entropy of melting, is the number of nearestneighbor adatom sites around an adatom on the crystal face, and z is the number of nearestneighbors in the bulk. The model therefore predicts that the equilibrium interface is smooth when the entropy of melting is large and the interface is lowindex (closepacked). This result is reasonable because a smooth interface (one without any intermixing of the solid and liquid due to the presence of adatoms or adatom clusters) is expected when the liquid and solid are strongly dissimilar with respect to their vibrational and configurational character and when the interface plane is relatively closepacked and therefore strongly bonded. In other work it has been argued that crystal/liquid interfaces roughen under the nonequilibrium conditions that exist during solidification when the driving pressure becomes sufficiently high [4,51. Under such conditions, the barrier to the nucleation of new growth layers is effectively eliminated and the interface becomes rough. This behavior is similar to a dislocation becoming highly jogged in the presence of a large vacancy supersaturation (Section 11.4.2) and of a crystal/vapor interface developing a high ledge density at a large vapor supersaturation. 12.3.2
Crystal Growth from an Undercooled Liquid
Singular and Vicinal Interfaces. The crystal/liquid interface during crystal growth from an undercooled liquid can be singular, vicinal, or general, depending upon the type of material and the driving force [l]. Many types of crystals require
12 3 INTERFACE MOTION DURING SOLIDIFICATION
293
a relatively large amount of undercooling (corresponding to 1' to 2") to obtain significant growth rates and solidify in faceted forms. This behavior is expected when singular (or vicinal) interfaces are dominant and the growth occurs by the movement of discrete ledges across the interface.* Crystals exhibiting this behavior have highly directional bonding or strongly bonded complex structures and possess values of the Jackson a parameter greater than two. On the other hand, most metals and some organic materials, possessing a values less than two, solidify with nonfaceted interfaces at exceedingly small undercoolings. This behavior is expected when the interface is rough (general) and there is a high density of sites everywhere in the interface where atoms can easily be incorporated into the solid. The manner in which a singular (or vicinal) crystal/liquid interface moves during solidification into an undercooled liquid by the lateral movement of ledges is similar t o the way a singular (or vicinal) crystal/vapor interface advances in a supersaturated vapor. Data showing the velocity of (001) and (111) interfaces in Ga as a function of the degree of undercooling resulting from the twodimensional nucleation and growth of atomic layers are in Fig. 12.6. The velocity increases rapidly with increased undercooling in a manner similar to the rapid increase of growth rate predicted schematically by the twodimensional nucleation and growth curve in Fig. 12.4 for the crystal/vapor case. 2 h
'i,
1.5
g
0.5
t % v '
0
0
1
2
3
4
5
Figure 12.6: Velocity v of singular (or vicinal) (001) and (111) surfaces as a function of undercooling durin solidificntion. The growth rate is limited by the twodimensional nucleation of ledges. h e dashed hies are niodel predictions. From Howe [I] Original figure from Peteves and Abbaschian [6]
General Interfaces. When the crystal/liquid interface is rough (general) , atoms from the liquid can easily be incorporated into the solid at a high density of sites in the interface. A primitive expression for the rate of solidification is easily obtained by using Fig. 12.7, which shows the change in energy when an atom is transferred across the crystal/liquid interface. For an atom to leave the liquid, it must surmount the energy barrier AGLIxL, and to leave the crystal, it must surmount the barrier ( A G + A G L I xL), where AG is given by Eq. 12.2. If N is the number of atoms (per unit area) in a position to jump from liquid to solid (or vice versa), the liquidtocrystal flux is
J ( L + X L ) = Nve  A G L ' X L / ( k T ) 4This is demonstrated in Exercise 12.1.
(12.8)
294
CHAPTER 12. MOTION OF CRYSTALLINE SURFACES
Distance,x Figure 12.7: Changes i n energy during solidification of an undercooled liquid when an atom is transferred across a crystal/liquid interface.
where v is a vibrational frequency. The reverse flux is
J ( X L + L ) = Nve ( A G ~ ’ ~ ~ + A G ) / ( I C T )
(12.9)
and the rate of growth is ZI
= [ J ( L+ X L )  J ( X L $
L ) ]R
(12.10)
When AG << IcT, the exponential in Eq. 12.10 can be expanded to first order and, using Eq. 12.2,
Under these conditions, the growth velocity is simply proportional to the undercooling, and the situation resembles crystal growth a t a rough crystal/vapor interface where the growth rate is proportional to the excess vapor pressure (Fig. 12.4).5 Bibliography 1. J.M. Howe. Interfaces in Materials. John Wiley & Sons, New York, 1997.
2. K.C. Jain and R.W. Siegel. Temperature dependence of the vacancy sink efficiency of stackingfault tetrahedra in quenched gold. Phil. Mag., 25( 1):105115, 1972.
3. K.A. Jackson. Mechanism of growth. In Liquid Metals and Solidification, pages 174186, Cleveland Park, OH, 1958. American Society for Metals. 4. J.W. Cahn. Theory of crystal interface motion in crystalline materials. Acta Metall., 8 ( 8 ):554562, 1960. 5. J.W. Cahn, W.B. Hillig, and G.W. Sears. The molecular mechanism of solidification. A c t a Metall., 12(12):14211439, 1964.
6. S.D. Peteves and R. Abbaschian. Growthkinetics of solidliquid Ga interfaces. 1. Experimental. Metall. Trans. A , 22(6):12591270, 1991. 5Note that this primitive singlejump model neglects t h e diffuse nature of the crystal/liquid in
t er face.
EXERCISES
295
EXERCISES
12.1 Construct a simple steadystate model for the growth from the vapor of a crystal with a vicinal surface and investigate the efficiency of the surface as a sink for the incoming vapor atoms. For simplicity assume that (i) the surface contains an array of evenly spaced straight, parallel ledges at the spacing A, and (ii) the ledges contain enough kinks to act as ideal line sinks for adatoms. Consider first the surface free of any ledges (i.e., the ledge spacing is infinite). Atoms from the vapor then land on the surface as adatoms and spend a mean time, T , on the surface before jumping back into the vapor. During the time T they are able to migrate in the surface layer, which is of thickness 6, a mean distance (x2)1/2 = 2 @ 5 where DZ is their diffusivity in the surface layer. The steadystate concentra, q5i tion of adsorbed atoms in the surface layer is then cm = ~ 4 =i T $ ~ where and & are, respectively, the rates of impingement and evaporation (per unit volume of surface slab), which in this case are equal. Consider now the vicinal surface where the impingement rate is the same as above. Adsorbed atoms will now either evaporate or diffuse to a ledge and become incorporated into the growing crystal. Show that the diffusion equation for the adsorbed atoms in the surface layer can be written as (12.12) where x is the distance coordinate running perpendicular to the ledges. Show that the solution to the diffusion equation above, subject to the applicable boundary conditions, is (12.13) where ceq is the equilibrium concentration maintained at the perfect ledge sinks. Ignore any effects of the motion of the ledges (see Exercise 12.3). Use the results to show that the efficiency (see Eq. 11.25) of the surface as a sink for the incoming atoms from the vapor is 1 7 7 =X / J q
m,
tanh
(L)
rn
(12.14)
q x m / X << 1 and the efficiency Therefore, when X >> is very low. This is the case where the ledge spacing is much greater than the adatom diffusion distance on the surface and very few adatoms reach the ledge sinks before jumping back into the vapor phase. On the
296
CHAPTER 12: MOTION OF CRYSTALLINE SURFACES
m,
other hand, when X << 77 cz 1. This is the case where the ledge spacing is relatively small and essentially all adatoms reach the ledge sinks before they jump back into the vapor. The surface therefore acts essentially as a perfect sink. Solution. (a) The rate o f accumulation o f adatoms in unit volume of the surface slab is
(12.15) where +i = c m / r and +e = c / r (because the evaporation rate will be proportional t o the concentration c). Because the diffusion is in the steady state,
d2c  c  c m _ dx2
Dir

4(ccm) (x2)
(12.16)
(b) The general solution of Eq. 12.16 is
where
a1
and
a2
are constants. Fitting Eq. 12.17 t o the boundary conditions
c(x = 0) = ceq
(12.18)
then yields the desired result (c) The rate a t which adatoms reach a unit length of ledge on the vicinal surface is
(12.19) The corresponding rate at which adatoms would reach the ledge if the surface acted as a perfect sink would be
(12.20) Therefore,
12.2 In Fig. 12.4 the velocity of crystal growth from the vapor is plotted as a function of the excess vapor pressure ( P  P""). When the surface acts as an ideal sink for incoming vapor atoms, the plot indicates that the velocity of growth should vary linearly with ( P  P""). When the sink efficiency is lower, the curve of v vs. ( P  Peq) falls below the ideal curve. Use the results of Exercise 12.1 to demonstrate that the velocity of growth for the model employed there can be expressed in the form
v = RJne, zz K ( P  P"")
(12.22)
EXERCISES
297
where K is a rate constant that is proportional to the sink efficiency, q , given by Eq. 12.14. The behavior predicted by this expression is seen to be consistent with the curves in Fig. 12.4. Solution. The rate a t which adatoms diffuse into a unit length of ledge is q5 = 2 6 0 2
(g)
(12.23)
x=o
Using Eq. 12.13 yields
q5=
4bD2(c"  C"") tanh
m
L)
m
(12.24)
The rate of impingement o f atoms from the vapor (per unit area) is Ji = Sq5i = b c " / r , while the rate of evaporation from the surfaceif the surface were in equilibrium (i.e,, in detailed balance) with the vaporwould be J,"" = 64:" = b c e q / r . Since, according t o the kinetic theory o f gases, the rate o f impingement from the vapor phase is proportional
(12.25) In detailed balance, the rate of evaporation is equal t o the rate of impingement from the vapor a t its equilibrium pressure, Peq,and therefore
(12.26) Solving these equations for C" and ceq and using Eq. 12.24, the net flux of atoms incorporated into the crystal from the vapor is
Jnet
=!
=
1
tanh
&)
K ' ( P  P'") (12.27)
= q K ' ( P  P"") = K ( P  P"")
2.3 One aspect of crystal growth from the vapor is the diffusive transport of adatoms to ledges (see Exercise 12.1). A suggestion is that the motion of ledges can be ignored in the analysis of crystal growth if
(12.28) where (x2)'/' is the rootmeansquare distance that an adatom diffuses in the surface during a time 7 while the ledge moves with a maximum velocity v,, corresponding to a large separation between ledges. Explain and derive this criterion. Solution. The effect of the ledge motion on the diffusion of adatoms t o i t will be small if the mean distance that adatoms can diffuse in the surface during a time T is large compared t o the distance that the ledge moves in the time T . Under these circumstances, the surface adatoms diffuse quickly enough in the surface so that their concentration in the vicinity of a moving ledge is only negligibly affected by the ledge motion. The mean diffusion distance is (z2)1/2= ~ ( D : T ) ' / ~ and the distance traveled The criterion is therefore (z2)1/2>> w m a x ~ . Substituting for r , by the ledge is w,,,r. we then obtain (x2)1/2 wmax/(4D5)<< 1.
298
CHAPTER 12: MOTION OF CRYSTALLINE SURFACES
12.4 During the evaporation of crystals with vicinal (or singular) faces, surface ledges of height, h; nucleate preferentially at the edges of the crystals where the faces meet. Develop a model for this type of heterogeneous nucleation and show that the critical free energy for the nucleation is much smaller than the critical free energy for the corresponding homogeneous nucleation of ledges by the formation of pillboxshaped cavities in the crystal surfaces. An overview of heterogeneous nucleation is provided in Section 19.2. Solution. The homogeneous nucleation geometry is shown in Fig. 12.8a. Using the approach that developed Eqs. 12.6 and 12.7 for homogeneous ledge nucleation during crystal growth, the free energy of the corresponding evaporation nucleus is A G = 27rRgL  a k T l n
n
(F)
(12.29)
R, is found by setting d A G / d R = 0. Putting the result into Eq. 12.29 then yields the critical free energy o f nucleation AGc(homo) =
7rn ( S L y hkTln ( P e q / P )
(12.30)
A model for the heterogeneous nucleation of a ledge a t a crystal edge is shown in Fig. 12.8b. The free energy for i t s formation is
A G = r R g L  2RhyS  a
k 2R
T In
(7)
(12.31)
Using the same procedure as above,
AG,(edge) =
7rR[gL  (2hyS/7r)I2 2hkT In(Peq/ P )
(12.32)
Therefore,
(12.33) Because gL = hyS, the critical free energy for heterogeneous edge nucleation is indeed considerably smaller than the energy for homogeneous nucleation.
Figure 12.8: (a) Homogeneous nucleus for surface evaporation. (b) Corresponding heterogeneous nucleus at crystal edge. Cavity depth and radius of curvature are h and R, respectively.
EXERCISES
299
12.5 A crystal growing from the vapor phase possesses a singular surface with two screw dislocations intersecting it. The dislocations are very close to one another (relative to the dimensions of the surface) and have opposite Burgers vectors. Describe the form of the step structure that is produced because of the presence of the two dislocations. Solution. Before any growth, the two dislocations are associated with steps that may be as indicated in Fig. 1 2 . 9 ~ .During growth, each dislocation rotates about its point of intersection t o produce a spiral step, as in Fig. 12.5. However, the spirals will rotate in opposite directions, and sections will annihilate one another when they meet as in (a) and (b). The process will then continue as in (c)(f) generating a potentially unlimited series o f concentric steps.
I
I
Figure 12.9: Step structure generated on growing crystal surface at the intersections of two screw dislocations with opposite Burgers vectors.
12.6 Suppose that the Burgers vectors of the two screw dislocations in Exercise 12.5 are now the same. Describe the ledge structure that is produced. Solution. Start with the ledge structure in Fig. 12.10~.The growth spirals of the two dislocations now rotate in the same direction as indicated. This will generate an interleaved double growth spiral of potentially unlimited extent as illustrated in Fig. 12.10bd.
Figure 12.10: Step structures generated on growing crystal surface at the intersections of two screw dislocations with the same Burgers vectors.
12.7 Consider a ledge on a surface which, on average, lies parallel to a closely spaced row of atoms. The ledge contains N sites, with spacing a , where either a positive or a negative kink can exist. (When traveling along a ledge, positive and negative kinks displace the ledge in opposite directions.) Show that the total number of kinks present in thermal equilibrium, NEq,is
(12.34)
300
CHAPTER 12 MOTION OF CRYSTALLINE SURFACES
where GL is the kink free energy of formation (excluding any configurational entropy). Solution. The increment of free energy due t o the presence of NZ positive kinks and N i kinks is A g = NZGL N i G L  k T l n P (12.35)
+
where the last term is the configurational entropy. P is the number of distinguishable ways of arranging the positive and negative kinks on the N sites and is given by
P=
N! (NZ)! ( N F ) ! ( N  Nk+  N L ) !
(12.36)
Using Eqs. 12.35 and 12.36 and the approximation l n z ! = z l n z  z,
d Ag = G{ dN$
+ G[ d N i
NZ + k T l n (N  N? ) d N z + k T I n (N  ~i

N'
N,$ 
) dNF NF
(12.37)
Numbers of positive and negative kinks are equal and therefore dN$ = d N i . The condition for equilibrium is then
(12.38) Therefore, because N
>> NZ + N;, (12.39)
and
N,'q N

[$1
eq +
[g] eq
= 2 eG{/(lcT)
(12.40)
12.8 Exercise 12.7 showed that the total equilibrium concentration of positive and negative kinks on a ledge running, on average, along a relatively closepacked direction is given by Eq. 12.34. Find the concentrations of positive and negative kinks on a ledge lying at an angle 0 with respect to the closepacked direction. Assume that the direction of 8 requires the buildingin of positive kinks. Solution. The population of kinks consists of BaNld builtin positive kinks, where d is the kink height, along with equal numbers of thermally generated positive and negative kinks, represented by N$ and N i , respectively. Following the same procedure as in Exercise 12.7, the derivative o f the total kink free energy, AG, is d AG = GidN$
+ G,fdNi
+ kTln [N + kTln
1

+
(BaNld) N,' (BaN/d) NZ  N i
N  (OaN/d)  NZ  N i
EXERCISES
301
The numbers of thermally generated positive and negative kinks are equal and therefore dN,f = d N L and the condition of equilibrium is
d ng  0 = 2 G L + k T l n
dN,'
[ N  ( e a N / d )  N,'  N i l 2
Assuming that 0 is small enough so that N
>> (OaN/d)+ N,'
}
(12.41)
+ NF, (12.42)
12.9 Consider the energy of a vicinal surface a t a low temperature that consists of an array of straight parallel ledges separated by patches of singular terraces as in Fig. B.l. Express the form of the energy cusp in which the surface lies (i.e., express the surface energy as a function of 0, the angle by which the inclination of the vicinal surface deviates from that of the singular terraces). Note that this model will break down at higher temperatures where the system's entropy increases and free energy decreases as the ledges wander and become nonparallel and other roughening processes occur. Solution. The structure of the vicinal surface is shown in Fig. 12.11. The energy of unit area of surface can be expressed as the sum of two parts: the first is that of the singular terraces, which is ys cose , where ys is the energy per unit area of the terraces; the second is that of the ledges, which is (gL sinB)/h, where h is the ledge height and g L is the energy per unit length o f a ledge. Therefore, = ys
h 
i t
gLsine +h
e
b
t
'
I
Figure 12.11: Structure of vicinal surface.
(12.43)
CHAPTER 13
MOTION OF CRYSTAL/CRYSTAL INT ER FACES
Crystal/crystal interfaces possess more degrees of freedom than vapor/crystal or liquid/crystal interfaces. They may also contain line defects in the form of interfacial dislocations, dislocationledges, and pure ledges. Therefore, the structures and motions of crystal/crystal interfaces are potentially more complex than those of vapor/crystal and liquid/crystal interfaces. Crystal/crystal interfaces experience many different types of pressures and move by a wide variety of atomic mechanisms, ranging from rapid glissile motion to slower thermally activated motion. An overview of crystal/crystal interface structure is given in Appendix B.
13.1 T H E R M O D Y N A M I C S O F CRYSTALLINE INTERFACE M O T I O N In Section 12.1, common sources of driving pressures for the motion of vapor/crystal and liquid/crystal interfaces were described. These and additional sources of pressure exist for crystal/crystal interfaces. For example, during recrystallization, the interfaces between the growing recrystallized grains and the deformed matrix are subjected to a pressure that is due to the bulk freeenergy difference (per atom) AG between the free energy of the deformed matrix and that of the recrystallized grains.' Also, compatibility stresses are often generated in stressed polycrystals so Recrystallization occurs when a crystalline material is plastically deformed a t a relatively low temperature and then heated [l]. The asdeformed material possesses excess bulk free energy resulting from a high density of dislocations and pointdefect debris produced by the plastic Kinetics of Materials. By Robert W. Balluffi, Samuel M. Allen, and W. Craig Carter. Copyright @ 2005 John Wiley & Sons, Inc.
303
304
CHAPTER 13. MOTION OF CRYSTALLINE INTERFACES
that two crystals adjacent to a grain boundary possess markedly different stresses. Equation 12.1 then holds, with AF equal to the difference between the elastic strain energy per atom in the two adjoining crystals. Pressures on crystal/crystal interfaces can also arise when the motion of the interface causes a change in the shape of the body in which it moves. Figure 13.1 shows the motion of a smallangle symmetric tilt grain boundary under applied shear stress. The motion occurs by the forward glide motion of the edge dislocations which comprise the boundary along x, causing the specimen to shear in the y direction. When this occurs, the applied stresses perform work, and the potential energy of the system is reduced. A displacement of the interface by Sx allows the applied stress, crzy, t o perform the work, oxyO62. The pressure on the interface is
p=
oxyo6s SX
= oxyo
(13.1)
There is a close similarity between this type of pressure and the mechanical force exerted on a dislocation by a stress (see Section 11.2.1 and Exercise 13.2). Estimated values of the magnitudes of the pressures commonly applied to crystal/crystal interfaces extend over a wide range of values, spanning about six orders of magnitude [2]. Generally, the pressures generated by phase transformations are the highest (107109 Pa), whereas those generated by interface curvature are relatively small (i03io5 Pa).
Figure 13.1: Motion of smallangle symmetric tilt boundary by means of glissile motion of its edge dislocations. Dislocation spacing, d , is equal to b/B, where b is the magnitude of the Burgers vector and B is the misorientation between the two grains.
13.2 CONSERVATIVE A N D NONCONSERVATIVE INTERFACE M O T I O N The motion of a crystal/crystal interface is either conservative or nonconservative. As in the case of conservative dislocation glide, conservative interface motion occurs in the absence of a diffusion flux of any component of the system to or from the deformation. Upon heating, nuclei of relatively perfect recrystallized material form and then grow into the deformed material, eliminating most of the crystal defects a t the moving interfaces between the recrystallized and deformed material.
13.3: CONSERVATIVE MOTION
305
interface. On the other hand, nonconservative motion occurs when the motion of the interface is coupled to longrange diffusional fluxes of one or more of the components of the system. Conservative motion can be achieved under steadystate conditions only when the atomic fraction of each component is the same in the adjoining crystals (see Exercise 13.1). For sharp interfaces, atoms are simply transferred locally across the interface from one adjoining crystal to the other and there is no need for the longrange diffusion of any species to the boundary. This local transfer can occur by the simple shuffling of atoms across the interface and/or by the creation of crystal defects (vacancies or interstitials) in one grain which then diffuse across the boundary and are destroyed in the adjoining grain, thus transferring atoms across the interface.* Examples of conservative motion are the glissile motion of martensitic interfaces (see Chapter 24) and the thermally activated motion of grain boundaries during grain growth in a polycrystalline material. During nonconservative interface motion, the boundary must act as a source for the fluxes. To accomplish this for sharp interfaces, atoms must be added to, or removed from, one or both of the the crystals adjoining the interface. This generally causes crystal growth or shrinkage of one or both of the adjoining crystals and hence interface motion with respect to one or both of the crystals. This can occur by the creation at the interface of the point defects necessary to support the longrange diffusional fluxes of substitutional atoms or by atom shuffling to accommodate the addition or removal of interstitial atoms. Nonconservative interface motion and the role of interfaces as sources or sinks for diffusional fluxes are of central importance in a wide range of phenomena in materials. For example, during diffusional creep and sintering of polycrystalline materials (Chapter 16), and the thermal equilibration of point defects, atoms diffuse to grain boundaries acting as pointdefect sources. In these cases, the fluxes require the creation or destruction of lattice sites at the boundaries. In multicomponentmultiphase materials, the growth or shrinkage of the phases adjoining heterophase interfaces often occurs via the longrange diffusion of components in the system. In such cases, heterophase interfaces again act as sources for the diffusing components. Further aspects of the conservative and nonconservative motion of sharp interfaces are presented below. The mechanism for the motion of a diffuse interface is discussed in Section 13.3.4. 13.3
CONSERVATIVE MOTION
13.3.1 Glissile Motion of Sharp Interfaces by Interfacial Dislocation Glide
Sharp boundaries of several different types can move conservatively by the glide of interfacial dislocations. In many cases, this type of motion occurs over wide ranges of temperature, including low temperatures where little thermal activation is available. SmallAngle Grain Boundaries. As described in Appendix B, these semicoherent boundaries are composed of arrays of discretely spaced lattice dislocations. For 2Shuffles are small displacements of atoms (usually smaller than an atomic spacing) in a local region, such as the displacements that occur in the core of a gliding dislocation.
306
CHAPTER 13: MOTION OF CRYSTALLINE INTERFACES
certain smallangle boundaries, these dislocations can glide forward simultaneously, allowing the boundary to move without changing its structure. The simplest example is the motion of a symmetric tilt boundary by the simultaneous glide of its edge dislocations as in Fig. 13.1. An important aspect of this type of motion is the change in the macroscopic shape of the bicrystal specimen which occurs because the transfer of atoms across the boundary from grain 2 to grain 1 by shuffling is a highly correlated process. Each atom in the shrinking grain is moved to a predetermined position in the growing grain as it is overrun by the displacement field of the moving dislocation array and shuffled across the boundary. The positions of all the atoms in the bicrystal are therefore correlated with the position of the interface and there is a change in the corresponding macroscopic shape of the specimen as the boundary moves. This type of interface motion has been termed military to distinguish it from the disorganized civilian type of interface motion that occurs when an incoherent general interface moves as described in Section 13.3.3 [3]. In the latter case, there is no change in specimen shape. Numerous experimental observations of the glissile motion of smallangle boundaries have been made [2]. Most general smallangle boundaries possess more than one family of dislocations having different Burgers vectors. Glissile motion of such boundaries without change of structure is possible only when the glide planes of all the dislocation segments in the array lie on a common zone with its axis out of the boundary plane. When this is not the case, the boundary can move conservatively only by the combined glide and climb of the dislocations as described in Section 13.3.2. LargeAngle Grain Boundaries. Semicoherent largeangle grain boundaries containing localized line defects with both dislocation and ledge character can often move forward by means of the lateral glissile motion of their line defects. A classic example is the motion of the interface bounding a (111) mechanical twin in the f.c.c. structure illustrated in Fig. 13.2. This boundary can be regarded alternatively as a largeangle grain boundary having a misorientation corresponding to a 60" rotation around a [lll]axis. The twin plane is parallel to the (111) matrix plane, and the twin (i.e., island grain) adopts a lenticular shape in order to reduce its elastic energy (discussed in Section 19.1.3). The macroscopically curved upper and lower sections of the interface contain arrays of line defects that have both dislocation and ledge character, as seen in the enlarged view in Fig. 13.2b. Note that the interface is semicoherent with respect to a reference structure (see Section B.6) taken to be a bicrystal containing a flat twin boundary parallel to (111). The line defects are glissile in the (111) plane and their lateral glissile motion across the interface in the directions of the arrows causes the upper and lower sections of the interface to move normal to themselves in directions that expand the thickness of the lenticular twin. In essence, the gliding line defects provide special sites where atoms can be transferred locally across the interface relatively easily by a military shuffling process, making the entire boundary glissile. This type of glissile interface motion produces a macroscopic shape change of the specimen for the same geometric reasons that led to the shape changes illustrated in Fig. 13.1. When a line defect with Burgers vector b' passes a point on the interface, the material is sheared parallel to the interface by the amount b. At the same time, the interface advances by h, the height of the ledge associated with the line defect. These effects, in combination, produce the shape change. A pressure urging the interface sections to move to
13.3 CONSERVATIVE MOTION
fY I
X
307
Matrix
/
Twin Matrix
/
Figure 13.2: (a) A lenticular twin in an f.c.c. structure bounded by glissile interfaces containing dislocations possessing ledge character viewed along [TlO]. (b) An enlarged view of the dislocationstep region. The interface is semicoherent with respect to a reference structure. corresponding to the bicrystal formed by a 60” rotation around [lll].The Burgers vector of the dislocation is a translation vector of the DSClattice of the reference bicrystal. which is the fine grid shown in the figure (see Section B.6). ( c ) The same atomic structure as in ( b ) . The interface now is considered to be coherent with respect to a reference structure. corresponding to the f.c.c. matrix crystal. In this framework. the dislocation is regarded as a coherency dislocation (see Section B.6). (d) The shape change produced by formation of a twin across the entire specimen cross section.
expand the twin and produce this shape change can be generated by applying the shear stress, oxy,shown in Fig. 1 3 . 2 ~ .The magnitude of this pressure is readily found through use of Eq. 12.1. The force (per unit length) tending t o glide the line defects laterally is given by Eq. 11.1, f = baxy. The work done by the applied force in moving a unit area of the boundary a distance 6s is then (bxlh)boxy,and the pressure is therefore (13.2) This type of glissile boundary motion occurs during mechanical twinning when twins form in matrix grains under the influence of applied shear stresses [4]. The glissile lateral motion of the line defects can be very rapid, approaching the speed of sound (see Section 11.3.1), and the large number of line defects that must be generated on successive (111) planes can be obtained in a number of ways, including a dislocation “pole” mechanism. Glissile motion of other types of largeangle grain boundaries by the same basic mechanism have been observed [2]. Heterophase Interfaces. In certain cases, sharp heterophase interfaces are able to move in military fashion by the glissile motion of line defects possessing dislocation character. Interfaces of this type occur in martensitic displacive transformations, which are described in Chapter 24. The interface between the parent phase and the newly formed martensitic phase is a semicoherent interface that has no longrange stress field. The array of interfacial dislocations can move in glissile fashion and shuffle atoms across the interface. This advancing interface will transform
308
CHAPTER 13: MOTION OF CRYSTALLINE INTERFACES
the parent phase to the martensite phase in military fashion and so produce a macroscopic shape change.
13.3.2 Thermally Activated Motion of Sharp Interfaces by Glide and Climb of Interfacial Dislocations
The motion of many interfaces requires the combined glide and climb of interfacial dislocations. However, this can take place only at elevated temperatures where sufficient thermal activation for climb is available. SmallAngle Grain Boundaries. As mentioned, a smallangle grain boundary can move in purely glissile fashion if the glide planes of all the segments in its dislocation structure lie on a zone that has its axis out of the boundary plane. However, this will not usually be the case, and the boundary motion then requires both dislocation glide and climb. Figure 13.3 illustrates such an interface, consisting of an array of two types of edge dislocations with their Burgers vectors lying at 45" to the boundary plane, subjected to the shear stress oZy. Equation 11.1 shows that the shear stress exerts a pure climb force f = bnZyon each dislocation, which therefore tends to climb in response to this force. However, mutual forces between the dislocations in the array will tend to keep them at the regular spacing corresponding to the boundary structure of minimum energy. All dislocations will then move steadily along +z by means of combined glide and climb. The boundary as a whole will therefore move without changing its structure, and its motion will produce a specimen shape change, the same as that produced by the glissile motion of the boundary in Fig. 13.1. Successive dislocations in the array must execute alternating positive and negative climb, which can be accomplished by establishing the diffusion currents of atoms between them as shown in Fig. 13.3. Each current may be regarded as crossing the boundary from the shrinking crystal to the growing crystal. An approximate model for the rate of boundary motion can be developed if it is assumed that the rate of dislocation climb is diffusion limited [2]. Neglecting any effects of the dislocation motion and the local stress fields of the dislocations on
Figure 13.3: Thermally activated conservative motion of a smallangle symmetric tilt boundary containing two arrays of edge dislocations with orthogonal Burgers vectors. f is the force exerted on each dislocation, by the applied stress. Arrows indicate atom fluxes between dislocations.
13.3.CONSERVATIVE MOTION
309
the diffusion] a flux equation for the atoms can be obtained by combining Eqs. 3.71 (13.3)
Under diffusionlimited conditions, the vacancies can be assumed to be maintained at equilibrium at the dislocations. The dislocations act as ideal sources (Section 11.4.1) and, therefore] at the dislocations pv = 0. When an atom is inserted at a dislocation of type 2 acting as a sink (Fig. 13.3), the dislocation will move forward along x by the distance f i R/b. The force on it acting in that direction is a x y b / f i , and the work performed by the stress is therefore ( f iR / b ) ( o x y b / f i= ) oxyR. The boundary value for the diffusion potential @ A at the cores of these dislocations is, therefore, (13.4) +:(sink) = p i  oxyR where p i is the chemical potential of atoms in stressfree material. Similarly, at dislocations of type 1, acting as sources, @(source) = p i gzyR. The average potential gradient in the region between adjacent dislocations is , d is the dislocation spacing. The approximate area then (V@A)= 2R o z y / dwhere per unit length, A, through which the diffusion flux passes is of order A E d . Using these quantities and Eq. 13.3, and assuming that the variations in *D due to local variations in the vacancy concentration are small enough to be neglected, the total atom current per unit length entering a dislocation of type 2 is given by
+
(13.5)
where *D is the selfdiffusivity as measured under equilibrium conditions. The volume of atoms causing climb (per unit length per unit time) is then IAR,and the corresponding climb rate is therefore vc = IAR/b. Each dislocation moves along z by combined climb and glide at a rate that exceeds its climb rate by f i ,and the boundary velocity is then v = five, or V =
4 f i R*D
bfkT
gxy
(13.6)
Since d = b / ( O f i ) [7] and the pressure on the boundary is P = tbzylEq. 13.6 may be expressed (13.7)
Equation 13.7 shows that the velocity is proportional to the pressure through a boundary mobility, MBl itself proportional to the selfdiffusivity, *D. The activation energy for boundary motion will therefore be that for crystal selfdiffusion as expected for a crystal diffusionlimited process. LargeAngle Grain Boundaries. Semicoherent largeangle boundaries may move conservatively through the lateral motion of their dislocations (which also generally possess ledge character) by means of combined glide and climb. In these boundaries, the coherent patches of the boundary between the dislocations are relatively 3Equation 13.3 was first obtained by Herring and is useful in modeling the kinetics of diffusional creep [5] and sintering [6] in pure metals.
310
CHAPTER 13: MOTION OF CRYSTALLINE INTERFACES
stable and therefore resistant to any type of motion. The dislocations, however, are special places in the boundary that support the transfer of atoms across the interface from the shrinking to the growing crystal relatively easily as the dislocations glide and climb. The example in Fig. 13.4 is an extension of the model for the motion of a smallangle boundary by the glide and climb of interfacial dislocations (Fig. 13.3). Figure 13.4 presents an expanded view of the internal “surfaces” of the two crystals that face each other across a largeangle grain boundary. Crystal dislocations have
I
V
Figure 13.4: Expanded view of the “internal surfaces” of two crystals facing each other across a grain boundary. Lattice dislocations AB and D E have impinged upon the boundary, creating line defects with both ledge and dislocation character which may glide and climb in the boundary in the directions of the arrows creating growth or dissolution spirals.
impinged upon the boundary from crystals 1 and 2, causing the formation of extrinThese sic dislocation segments in the boundary along CB and EF, re~pectively.~ extrinsic segments have Burgers vector components perpendicular to the boundary plane and possess ledge character. Crystal 1 can grow and crystal 2 can shrink if the segments CB and EF climb and glide in the directions of the arrows under the influence of the pressure driving the boundary. This can be achieved by the diffusion of atoms across the boundary from segment EF to segment CB, thus allowing the boundary to move conservatively. The continued motion of the segments in these directions will cause them to wrap themselves up into spirals around their pole dislocations in the grains (i.e., AB and E D ) . The dislocations will therefore form crystal growth or dissolution spirals in the boundary similar to the growth spirals that form on crystal free surfaces at points where lattice dislocations impinge on the surface (see Fig. 12.5). There is therefore a close similarity between this mode of dislocationinduced boundary motion and the motion of free surfaces due t o the action of growth or dissolution ledge spirals as discussed in Section 12.2.2. Probable observed examples of such dislocation growth or dissolution spirals on grain boundaries are shown in Fig. 13.5. The rates of boundary motion will depend strongly upon the available densities of boundary dislocations with ledge character. The formation of such dislocations by 4See Section B.7 for a discussion of extrinsic vs. intrinsic interfacial dislocations.
13 3 CONSERVATIVE MOTION
311
Figure 13.5: Observed examples of apparent dislocation growth or dissolution spirals on grain boundaries. From Gleiter 181 and Dingley and Pond 191.
the homogeneous nucleation of dislocation loops in the boundary is highly unlikely at the pressures that are usually exerted on boundaries [2]. An important source may then be impinged lattice dislocations, as described above. However, under many conditions, the rate of this type of boundary motion may be very slow.
13.3.3 Thermally Activated Motion o f Sharp Interfaces by Atom Shuffling Shuffling a t Pure Ledges. Interfaces capable of supporting pure ledges (see Section B.7) may migrate by the transverse motion of the ledges across their faces much like the motion of free surfaces described in Section 12.2.2. However, the ledges in interfaces can move conservatively by the shuffling of single atoms or small groups of atoms from the shrinking crystal to the growing crystal at kinks in the interface ledges. This type of motion does not produce a specimen shape change. Its conservative nature is in contrast to the nonconservative nature of freesurface motion via surfaceledge migration. The shuffles will be thermally activated, and a simple analysis shows that the interface velocity can then be written
(13.8) where NI, is the number of kink sites per unit interface area, N, is the average number of atoms transferred per shuffle, vo is a frequency. and Ss and E S are the activation entropy and energy for the shuffling. As in Eq. 13.7, the velocity is proportional to the driving pressure, P , through a boundary mobility, M B . This mobility is critically dependent upon the density of kink sites, which may vary widely for different interfaces. Ledges will be present initially in vicinal interfaces,
312
CHAPTER 13: MOTION OF CRYSTALLINE INTERFACES
but these will tend to be grown off during the interface motion and can therefore support only a limited amount of motion. Ledges cannot be nucleated homogeneously in the form of small pillboxes at significant rates at the driving pressures usually encountered. However, heterogeneous nucleation could be of assistance in certain cases. In general, widely different boundary mobilities may be expected under different circumstances [ 2 ] . Uncorrelated Shuffling at General Interfaces. Interfaces that are general with respect to all degrees of freedom possess irregular structures and cannot support localized line defects of any significant strength. However, in many places along an irregular general interface, the structure can be perturbed relatively easily to allow atoms to be shuffled from the shrinking crystal to the growing crystal by means of thermal activation. In this case, a simple analysis of the interface velocity leads again to a relationship of the form of Eq. 13.8 [ 2 ] . However, the quantity Nk appearing in the mobility M B is now the density of sites in the interface at which successful shuffles can occur. Under most circumstances, the intrinsic density of these sites will be considerably larger than the density of kink sites on vicinal stepped boundaries, and the mobility of general interfaces will be correspondingly larger.
13.3.4 Thermally Activated Motion of Diffuse Interfaces by SelfDiffusion Diffuse interfaces of certain types can move by means of selfdiffusion. One example is the motion of diffuse antiphase boundaries which separate two ordered regions arranged on different sublattices (see Fig. 18.7). Selfdiffusion in ordered alloys allows the different types of atoms in the system to jump from one sublattice to the other in order to change the degree of local order as the interface advances. This mechanism is presented in Chapter 18.
13.3.5 Impediments t o Conservative Interface Motion The conservative motion of interfaces can be severely impeded by a variety of mechanisms, including soluteatom drag, pinning by embedded particles, and pinning at grooves that form at the intersections of the interfaces with free surfaces. We take up the first two of these mechanisms below and defer discussion of surface grooving and pinning at surface grooves to Section 14.1.2 and Exercise 14.3. SoluteAtom Drag. Solute atoms, which are present either by design or as unwanted impurities, often segregate to interfaces where they build up “atmospheres” or segregates. This effect is similar in many respects to the buildup of soluteatom atmospheres at dislocations (discussed in Section 3.5.2). For the interface to move, it must either drag the solute atmosphere along with it or tear itself away. The dragging process requires that the solute atoms diffuse along with the moving interface under the influence of the attractive interaction forces exerted on them by the interface. In many cases, the forced diffusive motion of the solute atmosphere will be slow compared to the rate at which the interface would move in the absence of the solute atoms. The solute atoms then exert a soluteatom drag force on the moving interface and impede its motion. In cases where the applied pressure moving the interface is sufficiently large, the interface will be torn away from the solute atmosphere. A number of models for soluteatom drag, involving various simpli
13 3 CONSERVATIVE MOTION
313
fications, have been developed [2]. Figure 13.6 shows some of the main behavior predicted by Cahn's model [lo]. When the driving pressure, P , is zero, the steadystate interface velocity, w, is also zero and the distribution of solute atoms around the interface, shown in Fig. 13.6a, is symmetric. No net drag force is therefore exerted on the interface by the solute atoms in the atmosphere. However, as w increases, the atmosphere becomes increasingly asymmetric and increasing numbers of atoms cannot keep up the pace and are lost from the atmosphere. Figure 13.6b shows the steadystate velocity as a function of P . For the pure material ( c x L = 0), the velocity is simply proportional t o the pressure. This is known as intrinsic behavior. When solute atoms are added to the system, the velocity is reduced by the drag effect and the system now exhibits extrinsic behavior. At low pressures, the extrinsic velocity increases monotonically with increasing pressure, but a t high pressures the interface eventually leaves behind its atmosphere and the velocity approaches the intrinsic velocity. When the solute concentration is sufficiently high, a region of instability appears in which the interface suddenly breaks free of its atmosphere as the pressure is increased. Figure 1 3 . 6 ~shows that essentially intrinsic behavior is obtained at elevated temperatures at all solute concentrations because of thermal desorption of the atmospheres. However, extrinsic behavior appears a t the lawer temperatures in a manner that is stronger the higher the solute concentration. Finally, Fig. 13.6d shows that essentially intrinsic behavior can be obtained over a range of solute concentrations as long as the driving pressure is sufficiently high. To summarize, the drag effect becomes more important as the solute concentration increases and the driving pressure and temperature decrease.
Constant T
xc
P,
Constant P
Constant T
x=o
,
IIT +
log (.XI.

Figure 13.6: Grainboundary solutedrag phenoinena predicted by Cahn's model. (a) Segregated solute concentration profile c(z) across boundary as a function of increasing boundary velocity v (the z axis is perpendicular to the boundary). c x L is the solute concentration in the adjoining crystals. (b) Bouiidary velocity vs. pressure, P , on boundary as u, function of increasing c x L . ( c ) In v VS. 1/T as a function of increasing cxL. (d) In v vs. hi cayLas a function of increasing P. From Cahn [lo]
314
CHAPTER 13 MOTION OF CRYSTALLINE INTERFACES
Pinning Due t o Embedded Second Phase Particles. A single embedded secondphase particle can pin a patch of interface as illustrated in Fig. 13.7. Here, an interface between matrix grains 1 and 2, in contact with a spherical particle, is subjected to a driving pressure tending to move the interface forward along y past the particle. Interfacial energy considerations cause the interface to be held up at the particle. as analyzed below, and therefore to bulge around it. Inspection of the figure shows that static equilibrium of the tangential capillary forces exerted by the particle/grain 1 interface, the particle/grain 2 interface, and the grain l/grain 2 interface requires that the angle Q satisfy the relation
(13.9) The net restraining force along y exerted on the interface by the particle (i.e., the negative of the force exerted by the interface on the particle) is
F = ~ T R C OQ S7''
COS(Q
 4)
( 13.10)
The maximum force, F,,, occurs when d F / d Q = 0, corresponding to Q = a/2. Applying this condition to Eq. 13.10, the maximum force is
F,, For the simple case where ypl
+ COSQ)
(13.11)
= .irRy12(1
0 and Q
E y p 2 , COSQ
F,,
Er
7r/4 and thus
R y 12
(13.12)
depends only on R and and F,, Consider now the pressuredriven movement of an interface through a dispersion of randomly distributed particles. At any instant, the interface will be in contact with a certain number of these particles (per unit area). each acting as a pinning point and restraining the interface motion as in Fig. 13.7. Additionally, the particles themselves may be mobile due to diffusional transport of matter from the particle's leading edge to its trailing edge [a,121. Each particle's mobility depends upon its size and the relevant diffusion rates. A wide range of behavior is then possible depending upon temperature, particle sizes, and other factors. If the particles are Matrix grain 1 Interface \
~
f
Y12
Figure 13.7: Spherical particle inning an interface between grains 1 and 2. The interface is subjected to a driving pressure tRat tends to move it in the y direction. From Nes e t a1 [Ill.
13.3: CONSERVATIVE MOTION
315
immobile and the driving pressure is low, the particles may be able to pin the interface and hold it stationary. At higher pressures, the interface may be able to break free of any stationary pinning particles and thereby move freely through the distribution. The breakingfree process may also be aided by thermal activation (thermally activated unpinning, as analyzed in Exercise 13.5) if the temperature is sufficiently high or the particles sufficiently small. Also, if the particles are mobile, the interface and its attached particles may move forward t ~ g e t h e r . ~ 13.3.6
Observations of Thermally Activated GrainBoundary Motion
The motion of largeangle grain boundaries has been studied more thoroughly than that of any other type of interface. Many measurements of thermally activated motion have been made as a function of temperature, the geometric degrees of freedom, driving pressure, specimen purity, etc. The results have been reviewed [2, 131. According to the models described earlier, intrinsic motion is expected in materials of extremely high purity at elevated temperatures under large driving pressures.6 In addition, intrinsic mobilities of general boundaries should commonly be higher than those of singular or vicinal boundaries because of insufficient densities of kinks at dislocationledges on boundaries of the latter types. However, in almost all cases, observed interface motion has been influenced to at least some extent by soluteatom drag effects, so that the motion has been extrinsic and not intrinsic. For example, general grain boundaries moved as much as three orders of magnitude faster in A1 that had been zonerefined (see Section 22.1.2) using twelve rather than four passes [14]. Also, as in Fig. 13.8, activation energies for the motion of a number of [loo] tilt grain boundaries in 99.99995% pure A1 were about half as large as the energies for corresponding boundaries in 99.9992% pure Al. Such results show that grain boundary mobilities are extremely sensitive to soluteatom drag effects, and can be strongly affected by them even at exceedingly small soluteatom concentrations.
Purity
99.9992 4 1
0 " " " " " ' 0 10 20
I
30
40
50
Misorientation 8 (degrees) Figure 13.8: Activation energy, E B , for the motion of (100) tilt boundaries in A1 as a function of tilt angle. The arrows at the top indicate misorientations of singular boundaries. Data for A1 of 99.99995%, 99.9992%, and 99.98% purity. From Fridman et al. [15]. 5Detailed analyses of these processes are given by Sutton and Balluffi [2]. 61f motion is unaffected by drag effects due to impurity atoms, it is called intrinsic.
316
CHAPTER 13: MOTION OF CRYSTALLINE INTERFACES
The degree of solute segregation and drag is a function of the intrinsic grainboundary structure as well as the type and concentration of the solute atoms. When solute drag is rate controlling, the intrinsic boundary structure is only one of several factors that influences the drag and therefore the boundary mobility. The interpretation of boundarymotion experiments solely in terms of the nature of the intrinsic boundary structure then becomes rather indirect and exceedingly treacherous. For general boundaries, essentially all measurements are consistent with the linear relationship between velocity and pressure given by Eq. 13.7 (i.e., 'u = M B P ) ,as might be expected on the basis of the preceding shuffling model. Available mobility data have been collected for the motion of general grain boundaries in exceptionally highpurity A1 and the activation energy of 55 kJ mol' is significantly lower than that of boundary selfdiffusion, which is expected to be about 69 kJ molI [2]. Also, the data can be fit to the uncorrelated atomshuffling model for intrinsic motion in Section 13.3.3 using reasonable values of the parameters. These results are at least consistent with the shuffling mechanism. Regarding the motion of singular or vicinal grain boundaries, Fig. 13.5 shows direct electron microscopy images of dislocationledge spirals on such boundaries. The importance of line defects with ledgedislocation character to the mobility of singular boundaries has been demonstrated in a particularly clear manner for highly singular (111) twin boundaries in Cu [16]. These boundaries were essentially immobile in the annealed state but became mobile after picking up dislocation line defects which impinged upon them during plastic deformation. In other work, electronmicroscope observations of the motion of vicinal boundaries by atom shuffling at pure ledges have been made [17191. The motion of boundaries by shuffling at pure ledges has also been studied by computer simulation [20]. Evidence from measurements of the generally faster intrinsic motion of general boundaries relative to that of singular or vicinal boundaries has been collected [2]. The situation is complicated because the degree of solute segregation at singular or vicinal boundaries is often expected to be lower than that at general boundaries. The extrinsic mobilities of general boundaries may therefore be smaller than those of singular or vicinal boundaries (because of increased soluteatom drag), while their intrinsic mobilities may be larger. This supposition is at least partially supported by the data in Fig. 13.8. Here, the relatively large activation energies for the motion of general tilt boundaries in the 99.9992% material (having misorientations between those of the singular boundaries indicated by the arrows) most probably arose from strong drag effects associated with relatively strong impurity segregation at these boundaries. This effect disappears in the higherpurity, 99.99995%, material. At even higher purity, the situation could reverse and the activation energies for the general boundaries could become lower than for the singular boundaries [13]. Observations of further soluteatom drag effects have been reviewed [2, 131. A number of effects measured as a function of driving pressure, temperature, and solute concentration appear to follow the general trends indicated in Fig. 13.6. The approximate nature of the model makes some discrepancies unsurprising. In Fig. 13.9, the discontinuous increases in boundary mobility as the temperature is increased are presumably caused by successive detachments of portions of a soluteatom atmosphere that exerted a drag on the boundaries.
.v)
13 4. NONCONSERVATIVE MOTION
317
2
.I
c
3
;
2 8
1.1
1.2
1.3
1.4
1.5
1000/T (KI) Figure 13.9: Experimentally determined plot of l n M B vs. 1/T for a (111)tilt boundary with a 46.5' tilt angle in A1 containing Fe solute atoms. M B = boundary mobility. From Molodov et a l . 1211.
13.4 NONCONSERVATIVE M O T I O N : INTERFACES AS SOURCES A N D SINKS FOR ATOMIC FLUXES
The basic mechanisms by which various types of interfaces are able to move nonconservatively are now considered, followed by discussion of whether an interface that is moving nonconservatively is able to operate rapidly enough as a source to maintain all species essentially in local equilibrium at the interface. When local equilibrium is achieved, the kinetics of the interface motion is determined by the rate at which the atoms diffuse to or from the interface and not by the rate at which the flux is accommodated a t the interface. The kinetics is then digusionlimited. When the rate is limited by the rate of interface accommodation, it is sourcelimited. Note that the same concepts were applied in Section 11.4.1 to the ability of dislocations to act as sources during climb.
13.4.1 Source Action of Sharp Interfaces By the Climb o f Dislocations in Vicinal Interfaces. The climb of the discrete lattice dislocations that comprise smallangle grain boundaries allows them to act as sources for fluxes of point defects (e.g., vacancies). In such cases, the various dislocation segments in the array making up the boundary will attempt to climb in the manner described for individual dislocations in Section 11.4. However, they will be constrained by the tendency to maintain the basic equilibrium structure of the boundary array. In the simplest case of the symmetric tilt boundary illustrated in Fig. 13.1, the edge dislocations will all be able to climb in unison relatively e a ~ i l y . ~ However, a pure twist boundary will act as a source only if the screw dislocations are able to climb into helices as illustrated in Fig. 11.10. This climb process will seriously perturb the structure of the boundary and will be possible only at large driving forces (i.e., large super or subsaturations of the point defects). Figure 13.10 shows evidence for smallangle boundaries in Au acting as efficient sinks for supersaturated vacancies under a large driving force. Here, the supersaturated vacancies have collapsed in the form of vacancy precipitates in the region of 7Note that this process will cause the boundary to move relative t o inert markers embedded in either crystal adjoining the boundary.
318
CHAPTER 13 M O T I O N OF CRYSTALLINE INTERFACES
Figure 13.10: Denudation of vacancy precipitation i n ~1 zone lying alongside a sniallangle grain boundary in quenched and subsequently anneitled Ail. The boundary (lower right) acted as a sink for the supersaturated vacancies. Vacancy precipitates are sniall dislocation configurations resulting from the collapse of vacancy aggregates (as illustrated sclieniatically in Fig. 11.15). From Siege1 et a1 (221
the bulk away from the boundary. However, a precipitatedenuded zone is present adjacent t o the boundary due to the annihilation of supersaturated vacancies in that region by the sink action of the boundary. Largeangle singular or vicinal grain boundaries containing localized line defects with dislocationledge character can also act as sources for point defects by means of the climb (and possibly accompanying glide) of these defects across their faces. The patches of coherent interface between the line defects remain inactive since they are relatively stable and difficult to perturb. The source efficiency then depends upon the ability of the climbing dislocations to collect or disperse the point defects by diffusion along their lengths as well as in the grainboundary core. (Note the similarity of this situation to the growth of a crystal at a vicinal surface in a supersaturated vapor as in Fig. 12.3.) A vicinal grain boundary acting as a sink for supersaturated selfinterstitial defects is shown in Fig. 13.11. The interfacial line defects needed t o support the source action may often be produced by impinged lattice dislocations as in Fig. 13.4. However, a t sufficiently high driving forces, the necessary line defects with dislocation character may be nucleated homogeneously in the boundary in the form of small loops possessing ledge character.8 In the case of supersaturated point defects, the free energy to nucleate such a loop may be written approximately as pb2 R A F = 2(1 ~ n( v) ~)l]+2nRfL
nR2('*
R
1'
Edefect
(13.13)
where R is the loop radius, f is the energy per unit length of ledge, and Edefect is the energy supplied per precipitated defect. The first term is the elastic energy of the loop, the second the coreledge energy, and the third the energy supplied by the precipitated point defects. For a material with a high vacancy supersaturation, such as one subjected to hightemperature annealing and rapid quenching, Eq. 13.13 may be used t o evaluate A F , and it may then be shown that loops may be nucleated at significant rates. During highenergy irradiation, boundaries can act as sinks for highly supersaturated selfinterstitials by the nucleation (and subsequent growth) 8NNucleatiori theory is presented in Chapter 19.
13 4 NONCONSERVATIVE MOTION
319
Figure 13.11: Experimentally observed climb of extrinsic grainboundary dislocations A. B. and C in vicinal (001) twist grain boundary in Au. Static array of screw dislocations in background accommodates the twist deviation of the vicinal boundary shown from the crystal misorientation of the nearby singular twist boundary to which it is vicinal. Excess selfinterstitial defects were roduced in the specimen by fastion irradiation and were destroyed at the grainboundary &locations by climb, causing the boundary to act as a defect sink. (a) Prior to irradiation. (b) Same area as in (a) after irradiation. ( c ) Diagram showing the extent of the climb. From Komen et al [24]
of boundary dislocation loops [23]. Triangular dislocation loops formed on twin boundaries in irradiated Cu are shown in Fig. 13.12. Experimental evidence shows generally that vicinal grain boundaries can act as efficient sinks for point defects under high driving forces where grain boundary dislocation climb is possible [a]. In the case of largeangle boundaries, line defects with dislocation character may be generated as the boundary absorbs vacancies from the bulk. However, at low driving forces the efficiency is often relatively low. Vicinal heterophase interfaces can act as overall sources (or sinks) for fluxes of solute atoms by the motion across their faces of line defects possessing both dislocation and ledge character of the general type illustrated in Fig. B.6. The line defects act as line sources; during their lateral motion, lattice sites are shuffled from one adjoining crystal to the other, and the interface moves with respect to both phases. If the two phases adjoining the interface have different compositions, solute atoms must be either supplied or removed at the ledge by longrange diffusion. The motion of the ledge is therefore essentially a shuffling process coupled to the longrange diffusional transport of solute atoms. Figure 13.13 illustrates how platelet precipitates grow and thicken by the movement of line defects of the type just described. The efficiency of the growing precipitate platelet as a sink for the flux of incoming solute atoms then depends upon the density of ledges and their ability to move while incorporating the solute atoms.
320
CHAPTER 13: MOTION OF CRYSTALLINE INTERFACES
Figure 13.12: (111) twin boundary in Cu acting as a sink for excess selfinterstitial defects produced by 1 MeV electron irradiation. Defects are destroyed by aggregating in the boundary and then collapsing into triangular grainboundary dislocation loops as illustrated schematically in Fig. 11.15. Once formed, the loops destroy further defects by climbing (and expanding). Micrograph provided by A H King
Figure 13.13: (a) Ag,A1 precipitates in the form of thin platelets in AlAg alloy. The broad faces of the platelets are parallel to (111) planes of the matrix, which lie at different angles to the viewer. (b) Precipitate platelets in CuA1 alloy. Line defects that possess both dislocation and ledge character are present on the broad faces. Platelets grow in thickness by climb of these line defects across their faces. From Rajab and Doherty 1251 and Weatherly [26]
Available experimental information about the source (or sink) efficiency of heterophase interfaces for fluxes of solute atoms indicates that low efficiencies are often associated with a lack of appropriate ledge defects [2]. By the Uncorrelated Shuffling of Atoms in General Interfaces. Homophase and heterophase interfaces that are general with respect to all degrees of freedom are incoherent interfaces unable to sustain localized line defects. However, in many cases, such interfaces are able to act as highly efficient sources for fluxes of point defects or solute atoms by means of atom shuffling in the interface core. The process may be modeled by assuming that the core is a slab of bad material containing a density of favorable sites where point defects can be created and destroyed, or where atomic sites containing solute atoms can be transferred across the interface, by the uncorrelated local shuffling of atoms. It has been shown that high source efficiencies can be obtained in many cases for reasonably low densities of the favorable sites [ 2 ] . From experimental results, this appears to be the case for homophase (grain) bound
13 4 NONCONSERVATIVE MOTION
321
aries as sources for point defects. However, it may not be the case for heterophase boundaries when one of the adjoining phases has a relatively high binding energy and a correspondingly high melting temperature and thermodynamic stability. 13.4.2
DiffusionLimited Vs. SourceLimited Kinetics
The efficiency of an interface as a source or sink can be specified by using the same parameter, q , which defined the source or sink efficiency of climbing dislocations (see Eq. 11.25).’ To illustrate this explicitly under diffusion and sourcelimited conditions, consider the rate at which a dilute concentration of supersaturated B atoms, which are interstitially dissolved in an Arich a solution, diffuse to a distribution of growing spherical Brich @phaseprecipitate particles during a precipitation process. The rate depends upon the efficiency of the a / @interfaces as sinks for the incoming B atoms. Consider first the case where the interfaces perform as ideal sinks and the solute concentration at each a / @interface is therefore maintained at the equilibrium solubility limit of the B atoms in the a phase, c$. If the particles are initially randomly distributed, an approximately spherically symmetric diffusion field will be established around each particle in a spherical cell as in Fig. 13.14. The problem of determining the rate at which the B atoms precipitate is then reduced to solving the appropriate boundaryvalue diffusion problem within a given cell. The particle radius is R and the cell radius is given, to a good approximation, ~, n is the density of precipitate particles. We assume by R, = [ 3 / ( 4 ~ n ) ] l /where that the particle radius is always considerably smaller than the cell radius and first find a solution for the case where the particle radius is assumed (artificially) to be constant during the precipitation. The more realistic case where it increases due to the incoming flux of B atoms is then considered. The diffusion equation is &/at = D g V 2 c ,where D B and c are, respectively, the diffusivity and concentration of the B atoms in the a phase. The initial condition
Figure 13.14:
Spherical diffusion cells surrounding particles during precipitation.
gMuch of this section closely follows Interfaces in Crystalline Materials, by A.P. Sutton and R.W. Balluffi [2].
322
CHAPTER 13: MOTION OF CRYSTALLINE INTERFACES
in the cell is
(13.14)
c(r,O) = co
and the boundary conditions are
[TI.=,. c(R, t ) = ce"4p
(13.15)
=0
The separationofvariables method (Section 5.2.4) then gives the series solution [27] c ( r , t ) = ce"9p
where the eigenvalues,
Xi,
+
OL?
i=O
5 e'TDBt r
sin [&(r  R)]
(13.16)
are the roots of tan[Xi(R,  R)] = XiR,
( 13.17)
and the coefficients, ai, are given by
ai =
+
2(c0  c , * , ~ ) R ( x ~ R 1)~ Xi[XiR?(R,  R)  R]
(13.18)
The diffusion current into the particle carried by the ith term in the series given in Eq. 13.16 is
Ii = 4.rrR2D~ [d~/dr],=~
The total diffusion current into the particle is therefore a sum of the terms given by Eq. 13.19. Each term decays exponentially with a characteristic relaxation time corresponding to Ti = 1/X;DB. When R << R,, all of the shortwavelength terms decay very rapidly compared to the lowestorder i = 0 term, which, with acceptable accuracy, is
I, = 47rD~(c,
 cz!)
R etlTo
( 13.20)
where ro = R ~ / ~ D B[27]. R Letting (c) be the average concentration in the spherical cell,
(13.21) Integrating Eq. 13.21 and combining the result with Eq. 13.20 leads to the remarkably simple expression for the total diffusion current entering the particle:
I = 4.irD~R((c)  c$)
(13.22)
The analysis shows that the diffusion current quickly settles down to the value given by Eq. 13.22 during all but very early times and that the transients which occur at the early times due to the higherorder eigenfunctions can be neglected whenever the degree of precipitation is significant. Because the effects of any transients are
13 4 NONCONSERVATIVE MOTION
323
small, Eq. 13.22 also describes, with acceptable accuracy, the instantaneous quasisteady current of atoms to the particle when it is growing due to the incoming diffusion. Section 20.2.1 (see Eq. 20.47) shows that Eq. 13.22 also holds with acceptable accuracy for an isolated sphere which is growing in an infinite matrix. It also holds for an isolated sphere of constant radius in an infinite matrix (see Exercise 13.6). The result given by Eq. 13.22 is therefore insensitive to the effects due to sphere growth or to the volume in which it is growing as long as R << R,. In Exercise 13.8 this result is used to determine the growth of the precipitates in Fig. 13.14 as a function of time. The situation becomes quite different when the a l p interface is no longer capable of maintaining the Concentration of B atoms in its vicinity at the equilibrium If the concentration there rises to the value cap, the instantaneous value quasisteadystate current of atoms delivered to the particle by the diffusion field (obtained from Eq. 13.22) will be given by
czt.
I = 4 . i r D ~ R( ( c ) P a )
(13.23)
This must be equal to the rate at which these atoms are incorporated into the particle locally at the interface. The rate at which B atoms in the matrix transfer to the particle across the a l p interface will be proportional to the local matrix concentration. The reverse rate of transfer from the particle to the matrix will be the same as the rate of transfer from the matrix to the particle that would occur under equilibrium conditions when detailed balance prevails. The net rate of transfer will then be (13.24) I' = 4.irR2K ( c " ~ c$) where K is a rate constant. This rateconstant model should apply over a range of situations and has been widely used in the literature. The rate at which incoming B atoms are permanently incorporated in the particle depends upon the product of the impingement rate of B atoms on the particle (which is proportional to the B atom concentration in the matrix at the interface) and the fraction of the impinging B atoms that is permanently incorporated (this fraction depends upon the efficiency with which the particle collects and incorporates these atoms). This efficiency depends upon sink characteristics of the interface, such as the density of incorporation sites, the binding energy of a B atom to the interface, and its rate of diffusion along the interface. These factors can be lumped together in the form of a rate constant, K , so that the rate of permanent incorporation (per unit area of interface) is expressed as the product Kc"0. The rate at which B atoms are permanently removed from the particle at the interface can be determined by a stratagem in which the particle (with the identical interfacial sink structure) is imagined to be in detailed balance with the equilibrium concentration of B atoms in the matrix. The rate of permanent removal is then equal to the rate of permanent incorporation. However, the rate of incorporation depends upon the same rate constant as in the nonequilibrium case and is therefore given by Kc$. This must also be equal to the rate of permanent removal because of the detailed balance. However, it will also be equal to the rate of removal under nonequilibrium conditions since the sink structure is assumed to be unchanged. The net rate of incorporation (per unit area) in the nonequilibrium situation is then K(c"@ c::). The magnitude of the rate constant. K . can vary widely depending upon the sink efficiency of the particle and it can evolve with time if the structure of the interface
324
CHAPTER 13: MOTION OF CRYSTALLINE INTERFACES
(sink) changes. A detailed analysis of the analogous problem of crystal growth due to the impingement of atoms from the vapor phase in Exercises 12.1 and 12.2 shows that the growth rate can be represented by a rateconstant expression of similar form. Setting I = I ' , solving for cap, and putting the result into Eq. 13.23 yields the rate of precipitation (13.25) which is smaller than the rate of precipitation under diffusionlimited conditions (Eq. 13.22) by the factor 1 D B / ( K R ) .In fact, the efficiency of the particle as a sink is just
+
1
rl = 1
1
+DB/(KR)
(13.26)
if the previous definition of the efficiency given by Eq. 11.25 is employed. When the transfer rate is very high (or the diffusivity is very small) so that D B / ( K R )<< 1, 2 1, caO E c$, and the kinetics is diffusionlimited. At the other extreme, when D B / ( K R )>> 1, q E 0, cap E (c), and the kinetics is sourcelimited. When the kinetics is between these limits, it is regarded as rnixed.l0 Bibliography 1. R.W. Cahn. Recovery and recrystallization. In R.W. Cahn and P. Haasen, editors, Physical Metallurgy, pages 15951671. NorthHolland, Amsterdam, 1983.
2. A.P. Sutton and R.W. Balluffi. Interfaces in Crystalline Materials. Oxford University Press, Oxford, 1996. 3. J.W. Christian. T h e Theory of 'Pransformations in Metals and Alloys. Pergamon Press, Oxford, 1975. 4. J.P. Hirth and J. Lothe. Theory of Dislocations. John Wiley & Sons, New York, 2nd edition, 1982. 5. C. Herring. Diffusional viscosity of a polycrystalline solid. J. Appl. Phys., 21:437445, 1950. 6. C. Herring. Surface tension as a motivation for sintering. In W.E. Kingston, editor, The Physics of Powder Metallurgy, pages 143179, New York, 1951. McGrawHill. 7. W.T. Read. Dislocations in Crystals. McGrawHill, New York, 1953. 8. H. Gleiter. The mechanism of grain boundary migration. Acta Metall., 17(5):565573, 1969. 9. D.J. Dingley and R.C. Pond. On the interaction of crystal dislocations with grain boundaries. Acta Metal l., 27(4) :667682, 1979. 10. J.W. Cahn. The impuritydrag effect in grain boundary motion. 10(9) :789798, 1962.
Acta Metall.,
11. E. Nes, N. Ryum, and 0. Hunderi. On the Zener drag. Acta Metall., 33:ll22, 1985.
12. M.F. Ashby. The influence of particles on boundary mobility. In N. Hansen, A.R. Jones, and T. Leffers, editors, Recrystallization and Grain Growth of MultiPhase and Particle Containing Materials, pages 325336, Roskilde, Denmark, 1980. Riso National Laboratory. 13. G. Gottstein and L.S. Shvindlerman. Grain Boundary Migration in Metals: Thermodynamics, Kinetics, Applications. CRC Press, London, 1999. "See
Exercise 13.7 for further results.
EXERCISES
325
14. K.T. Aust and J.W. Rutter. Effect of grain boundary mobility and energy on preferred orientation in annealed high purity lead. Trans. AIME, 224:lll115, 1962. 15. E.M. Fridman, C.V. Kopezky, and L.S.Shvindlerman. Effects of orientation and concentration factors on migration of individual grainboundaries in aluminum. Z. Metallkd., 66(9):533539, 1975. 16. P.R. Howell, J.O. Nilsson, and G.L. Dunlap. The effect of creep deformation on the structure of twin boundaries. Phil. Mag. A , 38(1):3947, 1978. 17. D.A. Smith, C.M.F. Rae, and C.R.M. Grovenor. Grain boundary migration. In R.W. Balluffi, editor, Grain Boundary Structure and Kinetics, pages 337571, Metals Park, OH, 1980. American Society for Metals. 18. H. Ichinose and Y. Ishida. In situ observation of grain boundary migration of silicon C3 boundary and its structural transformation at 1000 K. J . Phys. Colloq. (Paris), 5l(suppl. no. l):C1:185190, 1990. 19. T. Kizuka, M. Iijima, and N. Tanaka. Grain boundary migration at atomic scale in MgO. Muter. Sci. Forum, 233234:405412, 1997. 20. R.J. Jahn and P.D. Bristowe. A molecular dynamic study of grain boundary migration without the participation of secondary grain boundary dislocations. Scripta Metall., 24(7):13131318, 1990. 21. D.A. Molodov, C.V. Kopetskii, and L.S. Shvindlerman. Detachment of a special ( C = 19, (111))tilt boundary from an impurity in irondoped aluminum bicrystals. Sow. Phys. Solid State, 23(10):17181721, 1981. 22. R.W. Siegel, S.M. Chang, and R.W. Balluffi. Vacancy loss at grainboundaries in quenched polycrystalline gold. Acta Metall. Muter., 28(3):249257, 1980. 23. A.H. King and D.A. Smith. On the mechanisms of pointdefect absorption by grain and twin boundaries. Phil. Mag. A , 42(4):495512, 1980. 24. Y. Komem, P. Petroff, and R.W. Balluffi. Direct observation of grain boundary dislocation climb in ionirradiated gold bicrystals. Phil. Mag., 26:239252, 1972. 25. K.E. Rajab and R.D. Doherty. Kinetics of growth and coarsening of faceted hexagonal precipitates in an fcc matrix. 1. Experimentalobservations. Acta Metall. Muter., 37( 10):27092722, 1989. 26. G.C. Weatherly. The structure of ledges at plateshaped precipitates. Acta Metall., 19(3):181192, 1971. 27. F.S. Ham. Theory of diffusion limited precipitation. J . Phys. Chem. Solids, 6(4):335351, 1958.
EXERCISES 13.1 Consider the conservative motion of a heterophase a l p interface in an AB binary system. cs, cg, ,c: and c$ are the concentrations of A and B in the two phases facing each other across the interface. Show that the conservative motion requires that Xz = X$ and that it is generally expected that c 2 # Ct.
SoZution. If the interface moves conservatively into the LY phase, it will convert a slab of the cy phase of thickness be into a slab of ,8 phase of thickness b P . Each slab must contain the same number of A and B atoms ( i t , NZ = N$ = N A and NE = N$ = N B ) . Each slab will then have the same mass, but because the slab
326
CHAPTER 13: MOTION OF CRYSTALLINE INTERFACES
densities will generally differ, the slab thicknesses will generally differ. The condition X : = X $ must then be satisfied since
x; = NANA = x$ t N B
(13.27)
However, since (for unit area of boundary)
NA
NA
c z =  and c p  A 60 6"
the concentrations will be expected t o differ since in general 6"
(13.28)
# bP.
13.2 Equation 13.1 for the pressure exerted on the smallangle tilt boundary by a shear stress was derived by considering the work done by the shear stress during the change in macroscopic shape of the bicrystal which occurred when the boundary moved (see Fig. 13.1). Obtain the same result by considering the force exerted on each moving edge dislocation by the applied stress and summing the forces on all dislocations. Solution. Using Eq. 11.2, the force per unit length on each dislocation is fo = uxyb. The spacing, d , o f the dislocations in a symmetric t i l t boundary is d = b / 0 [7].The pressure on the boundary due t o all dislocations is then 1 0 P = a x y b  = uz,b  = 0 Z y 0 b
d
(13.29)
Note that this result is expected since the force exerted on an individual dislocation by a stress is the result of the change in crystal shape that occurs when the dislocation moves. Since the change in shape of the bicrystal due t o the boundary motion is just the sum of the changes due t o the motion of each of its individual dislocations, the total force on the boundary must be just the sum of the forces on the individual dislocations.
13.3 An expression for the diffusion potential at an edge dislocation in a smallangle tilt boundary subjected to a pure shear stress has been derived in Section 13.3.2. Derive a general expression for the diffusion potential at an isolated general (mixed) straight dislocation acted on by a general stress field. Express your answer in terms of the stress tensor, u ,the Burgers vector, b, and the unit tangent vector, (. Remember that the potential is related to the work performed by the stress field when an atom is inserted at the dislocation (per unit dislocation length) during the dislocation climb. The force exerted on the dislocation is given by the PeachKoehler equation (Eq. 11.1). Also, only the edge component of the dislocation plays a role in the climb. #
Solution. The dislocation will climb in a direction perpendicular t o its glide plane (i.e., the plane containing both b'and The unit normal, A,t o the glide plane is
0.
(13.30) The force per unit length, f , exerted on the dislocation by the stress field in the climb direction normal t o the glide plane is then +
f = f,.A
(13.31)
EXERCISES
327
The climb distance per unit length, d c , due t o the insertion o f an atom is
d c    R =be
R ( A x r^)
'b'
(13.32)
t)
where be = ( h x . 6 is the magnitude o f the edge component of the Burgers vector. The potential relative t o the reference potential, p i , is then the negative o f the work done by the stress during the climb and is therefore given by
Note that the sign of the final expression in Eq. 13.33 must be consistent with the convention for determining the Burgers vector (see the text following Eq. 11.1).
13.4 A singlephase bicrystal sheet of thickness, h, is produced in a laboratory and cut into a symmetrical wedge as in Fig. 13.15. Upon heating, the boundary
Figure 13.15: Bicrystal specimen with a planar grain boundary initially located a distance L ( 0 ) froin the apex.
is found to migrate toward the apex and data for L ( t ) as a function of time, t , are shown in Fig. 13.16.
t (min)
Figure 13.16: Migration data for boundary in Fig. 13.15
Develop a plausible model for the observed data in Fig. 13.16. State two assumptions of the model. Give a plausible explanation for the observed initial transient behavior in Fig. 13.16. Using only the information in Fig. 13.16, estimate the activation energy for boundary motion.
328
CHAPTER 13
MOTION OF CRYSTALLINE INTERFACES
(d) Closer examination of the data in Fig. 13.16 shows that growth is not uniform but oscillates between slow and fast growth, as shown in Fig. 13.17. Give a plausible explanation for this behavior. L2(0 )b
L2(t) (mm2)
9 10 20 30 40 SO
0 Figure 13.17:
t (min)
Magnified view of data. from Fig. 13.16 a t 1000°C.
( e ) The same experiment is repeated, but the material is obtained from a
different supplier. Give a plausible explanation for the kinetic transition which is now observed after about 30 minutes a t T = 8OO0C, as in Fig. 13.18.
0
Figure 13.18: supplier.
10
20 30 t (rnin)
LK)
50
Same experiment as for Fig. 13.16, but with material from a different
Solution. Assuming that the surface energies o f grains 1 and 2 are the same and that the grainboundary energy is isotropic, the boundary will quickly adopt a circulararc shape which is perpendicular t o the wedge edges in order t o balance surfacetension forces. The driving pressure on the boundary will then be P = y / R , where the radius of curvature is R = L / c o s ( a / 2 ) . Therefore,
P
=
Y cos a L
(13.34)
2
Assuming a constant boundary mobility, M B ,
or
a!
L dL =  M B Y cos ~  dt 2
(13.35)
EXERCISES
329
Integrating Eq. 13.35 yields
L 2 ( 0 ) L 2 ( t )= 2 M ~ cos y cy~ t 2
(13.36)
(b) The data indicate t h a t the boundary motion corresponding t o Eq. 13.36 does not begin immediately. This could be the result o f grain boundary pinning by solute atoms or small precipitates or by the existence of a grainboundary groove in the initial position o f the boundary from which the boundary must break away. It could also be the result of time taken for the boundary t o adopt the curved shapea process that would presumably begin from the specimen edge. (c) Equation 13.35 indicates that the slope of the linear regions of the two curves in Fig. 13.16 is proportional t o the boundary mobility, M B . Assuming that the boundary energy, y B , is independent of temperature and that M B follows an Arrhenius law, M B = M g exp[EB/(kT)], the activation energy for migration can be calculated. Letting TI = 1073 K and T2 = 1273 K, the corresponding mobilities are proportional t o the slopes of the curves in Fig. 13.16: M B ( T 1 ) 0:
= 0.082
and
4 M B ( T ~0:) = 0.23 19  2
(13.37)
From the Arrhenius law,
(13.38) and hence
 1.054 x 1.38 x lo'' 
1.46 x 104 KI
J K'
(13.39) = 1.0 x 1 0  l ~ J
(d) The most likely explanation for jerky motion of the boundary is localized pinning by precipitates or small inclusions from which the boundary must repeatedly escape. (e) Figure 13.18 indicates that the boundary initially moves steadily at a relatively slow rate, then undergoes a transition t o steady motion at a higher rate. Such behavior is consistent with an impuritydrag breakaway effect, which could be due t o certain impurities in the material from the different supplier. Note that according t o Eq. 13.34, the driving pressure increases as the boundary migrates and L decreases. The initial slow migration regime takes place when the boundary is less highly curved and is moving under a relatively small capillary driving force. Under these conditions, the boundaries in the impure material could have an impurity atmosphere that would have t o move along with the boundary as it migrates with a relatively low mobility (extrinsic migration). As the boundary moves toward the apex o f the wedgeshaped bicrystal specimen, it becomes more highly curved and the capillary driving force rises (ultimately becoming infinite). When the driving force becomes sufFiciently high, the moving boundary can break free of the impurity atoms and move with a higher intrinsic mobility.
13.5 Consider the pinned secondphase particle illustrated in Fig. 13.7 and described by Eqs. 13.913.12. Assume that ypl = yp2, so that a = 90". (a) Show that t,he force exerted by the interface on the particle (or alternately, the force exerted by the particle on the interface) when the interface is a t a position where it meets the particle at the distance along
330
CHAPTER 13 MOTION OF CRYSTALLINE INTERFACES
y denoted by y = 77 is given (as a function of q) by
(13.40)
which is plotted in Fig. 13.19.
Figure 13.19: F ( q ) vs. 7 . F ( q ) is the pinning force exerted on an interface by a spherical particle embedded in the interface in the configuration illustrated in Fig. 13.7. q is the displacement of the interface in the y direction, corresponding to q = Rsiri 4 in Fig. 13.7.
(b) Consider the possible thermally activated unpinning of the particle when the interface is initially held a t the position 71; by a force F'. The activation energy E for the unpinning will be the work required to move the interface off the particle in the direction of y in the presence of the initial force F'. The force resisting this motion will correspond to F ( q ) . Show that E is given by
(
E =  F2 m a x R 1 F 3
V
2
(13.41)
The thermally activated unpinning is therefore favored by a small particle size and a large applied force, as might be expected intuitively. Solution. (a) When
QC
= go", Eqs. 13.10 and 13.12 yield
F = 2Fmaxcos 4 cos(90  4) = 2Fma, cos q5 sin 4
(13.42)
From Fig. 13.7, C O S = ~ J m / R , and cos(90  4) = s i n 4 = q / R . Substitution of these quantities into Eq. 13.42 then yields the desired relationship. (b) The energy that must be supplied by thermal activation in the presence of the initial force F' is the shaded area in the figure, and therefore
E
=
S,f""'
Using q = R s i n 4 , Aq = R(sin42
Aq(F) d F
 sin41). From
F(q1) = 2Fmp.x cos 41 CoS(90  41)
(13.43)
Eq. 13.42,
F(q2) = 2Fmax cos 4 2 cOs(90  4 2 ) (13.44)
EXERCISES
F ( q 1 ) = F ( q 2 ) requires that
$2
Aq = R(sin $ 2
= 90 
 $1.
Therefore,
sin $1) = R(cos 41  sin $1)
= R J ~ 2sin41 C
331
O S = ~ R ~
(13.45)
J
~
Putting Eq. 13.45 into Eq. 13.43 and integrating then produces the desired result.
13.6 Equation 13.22 holds for the quasisteady rate at which B atoms diffuse to a spherical precipitate in a distribution of similar precipitates in a dilute supersaturated solution. Show that an equation of the same form holds for the quasisteady rate of diffusion to a single spherical precipitate of constant radius R embedded in an infinite volume of a similar solution. [Note that a similar result is also obtained in Section 20.2.1 (Eq. 20.47) for the more realistic case where the particle is allowed to grow as the diffusion occurs.] 0
Use spherical coordinates and solve the resulting boundaryvalue problem by making the change of variable u = (c  c0)r, where co is the concentration when r + 03.
Solution. The basic differential equation is (13.46) and the boundary and initial conditions are c ( r = R,t
> 0) = ce*,"
c(r
2 R, t = 0) = co
c(r
t > 0 ) = co
+ co,
Making the change o f variable u = ( c  c o ) r , Eq. 13.46 becomes
(13.47)
(13.48) A standard solution of Eq. 13.48 (see Chapter 4) is
(13.49) where
a1
and
a2
are constants. Therefore,
(13.50)
r
and applying the boundary and initial conditions, final solution is then
a2
= 0 and
a1
= R(c:{
 c o ) . The
(13.51) The total difFusion current entering the particle is then
The second term inside the brackets is seen t o be an initial transient that falls off as t  1 / 2 . It is associated with the establishment a t early times o f a steep concentration gradient in the difFusion field over a distance from the particle equal t o about R.
332
CHAPTER 13: MOTION OF CRYSTALLINE INTERFACES
Once the diffusion distance, 2 ( D ~ t ) ’ / ’substantially , exceeds R , the transient becomes unimportant, and Eq. 13.52 then has the same form as Eq. 13.22.
13.7 Consider the analysis leading to Eqs. 13.23 and 13.24 for a spherical precipi
tate particle acting as an ideal or nonideal sink.
(a) Show that when E/(rcR) << 1 and the particle is acting almost as a perfect sink, the concentration maintained at the particle/matrix interface, c a p , must inevitably be slightly larger than the equilibrium concentration, c$, and that, in fact, (13.53) (b) Next, show that when E/(rcR)>> 1 and the particle is acting as a very poor sink, the concentration at the interface will inevitably be slightly lower than the average concentration in the bulk, (c), and that, in fact,
(13.54) 0
Neglect higherorder terms in any expansions that are employed.
Solution. First, solve for caP by equating Eqs. 13.23 and 13.24 t o obtain (13.55) (a) When D / ( K R < )< 1, let D / ( K R = ) E . Then
(b) When D / ( K R >> ) 1, let K R / D= E . Then
cap = ( c )
+
Ecg = (c) I+&
+ EC:!
 (C)E

= (c)
C,aq41KR D I
(13.57)
13.8 Using the model and results in Section 13.4.2, find a relationship showing
how the particle radius grows with increasing time during the precipitation of the finite number of supersaturated interstitial atoms with diffusivity D B available. Assume that the particles are of fixed composition throughout and act as perfect sinks and that R << R,. Solution. Starting with Eq. 13.22, the instantaneous rate a t which the particle volume increases is
dV dt
2
dR dt

 = 47rR  = 47rDR[(c) c:!]
R’
(13.58)
where R’ is the increase in particle volume per added interstitial. A t any time, the volume of the precipitate is given by 4 3 4 3 V = 7rR = 7rR,[co  ( c ) ]R’ 3 3
(13.59)
EXERCISES
333
Solving Eq. 13.59 for ( c ) and putting the result into Eq. 13.58 yields the differential equation
(co  c:!)
R dR = 50’ dt  R3/R2f l t
(13.60)
The final size o f the particle when the precipitation is complete is given by
R,3 = R:(co  c:[)Rt
(13.61)
and therefore Eq. 13.60 may be put into the more convenient form

D RdR = dt RL R3 RZ
(13.62)
The solution of Eq. 13.62, subject t o the initial condition R = 0 when t = 0, is
ln(’
R 2 + R w R + R &)  & t a n  ’ ( R,R
2R+ R, & R,
) +rr G3R,5 =T t (13.63)
A few calculations show t h a t R increases with time at an everdecreasing rate and approaches R, asymptotically as t + m.
13.9 Consider a smallangle tilt boundary of the type shown in Fig. 13.1, which is acting as a sink for highly supersaturated vacancies at initial concentration given by i?. Assume that each edge dislocation acts as a perfect line sink and that the vacancies are diffusing t o the boundary from a distance, L , larger than the spacing of the dislocations in the boundary, d. Show that the boundary will act as a perfect sink for all practical purposes whenever L >> d. 0
Neglect any effects due to the climb motion of the dislocations and assume quasisteadystate diffusion. The vacancy isoconcentration contours around the dislocations in the boundary will then appear approximately as illustrated in Fig. 13.20.
At distances from the boundary along 2 greater than about half the dislocation spacing (i.e., d / 2 ) , the contours will be unaffected by the fine structure of the boundary and will essentially be planes running parallel to the boundary. Nearer t o the dislocation cores, the contours will be concentric cylinders. A reasonable approximation is then to represent the diffusion field as shown in
Figure 13.20: Approximate flux lines around edge dislocations in a smallangle tilt boundary acting as a sink for supersaturated vacancies.
334
CHAPTER 13: MOTION OF CRYSTALLINE INTERFACES
Fig. 13.20. Here, at distances from each core less than d / 2 , the diffusion into each core is taken to be cylindrical. Beyond this distance, the diffusion into the boundary as a whole along 2 is taken to be planar (onedimensional). At the “surface” of the core (i.e., the core radius of the dislocation, r = R o ) , the equilibrium vacancy concentration is negligible compared with the high concentration, C, at the large distance, L . Therefore, c ( r = R,) = 0. Assume a quasisteady state in the boundary region. The concentration at x = d / 2 will then take on an intermediate value, c’, which can be determined. The total diffusion current into the boundary can then be determined. Solution. Using Eq. 5.13, the quasisteadystate current entering each dislocation by cylindrical diffusion is (13.64) while the current diffusing toward each dislocation from the distance L by planar diffusion is 2 d D v ( E  c’) (13.65) Ip = L d/2 Equating these currents then yields
’
c =
‘
d In [d/ (2 R 0 ) ] T ( L d / 2 ) d In [ d / ( 2 R o ) ]
+
(13.66)
Substituting this into the expression for Ic,
Ic =
21rDvd
T(L d / 2 ) + d In [ d / ( 2 R o ) ]
(13.67)
The current that would diffuse into the boundary if it were a perfect sink would be Iideal
2dDvE L
=
(13.68)
The sink efficiency (see Eq. 11.25) is then (13.69) Therefore, 7 x 1 when L >> d . Note: a more exact treatment using the analogy between steadystate diffusion fields and electrostatic fields leads t o a very similar result [22].
PART 111
MORPHOLOGICAL EVOLUTION DUE T O CAPILLARY AND APPLIED MECHANICAL FORCES
A material can change its morphologyits external macroscopic shape and its internal microstructurewhen suitable driving forces exist. As always, these driving forces result from differential decreases in total free energy. Morphology depends to a major extent upon the shapes and positions of interfaces. Every real material has at least one interfacethe exterior interface which separates it from its environment. If an interface separates a material from its vapor or a vacuum, it is typically called a free surface. Interfaces that exist in materials within a condensed phase (or between condensed phases) are termed internal interfaces. Chapters 14 and 15 are concerned with the contributions made to morphological change by the motion of free surfaces and internal interfaces. Interfaces contribute an excess free energy to a material which depends on their areas and their crystallographic degrees of freedom, and they can also respond to mechanical forces. As a result, interfaces are commonly subjected t o two independent forces which tend to drive their motion and produce morphological change. If the interface motion decreases the total excess free energy associated with the interface itself (i.e., through the product of its area and energy per unit area), the resulting force for motion is conventionally called a capillary force. For a curved isotropic interface, the capillary force is present due to the pressure difference across the interface caused by its
336 local mean curvature. Such capillary forces are especially influential in finescale microstructures containing interfaces with large curvatures where pressure differences can become correspondingly large. In addition t o a capillary force, a force for interface motion is produced whenever motion of the interface allows an applied force to perform work: such a force is an applied force. The three chapters that comprise Part I11 are limited t o cases where chemical driving forces are absent, and phase transformations therefore do not occur. Morphological change due to the evolution of free surfaces under the influence of capillary forces is treated in Chapter 14. Topics include surface smoothing and faceting, surface grooving at intersections with grain boundaries, and the incipient evolution of a cylinder into a row of spheres. Transport mechanisms considered include surface and volume diffusion and vapor transport. Morphological change due t o the capillaritydriven motion of internal interfaces is treated in Chapter 15, which includes grain growth in polycrystals and the coarsening of a fine distribution of secondphase particles. In Chapter 16 we address cases of morphological change that involve free surfaces and internal interfaces and include capillary and applied mechanical forces. Attention is focused on two technologically important kinetic processes: the surface smoothing and removal of porosity which occurs during sintering of porous bodies and the change in body shape produced by diffusional creep.
CHAPTER 14
SURFACE EVOLUTION DUE T O CAPILLARY FORCES
The total interfacial contribution to the free energy of a system corresponds to the integral of the interfacial free energy per unit area, y,over all interfaces. y is a material property that is a function of the geometric degrees of freedom of an interface. Therefore, driving forces for interfacial motion in a particular material derive from two sourcesreductions in interfacial area and reductions in interfacial energy per unit area due to changes in the geometrical/crystallographic attributes of the interfaces. Analysis is simplified if y is isotropici.e., independent of geometrical attributes such as interfacial inclination f i and, for internal interfaces in crystalline materials, the crystallographic misorientation across the interface. All interfacial energy reduction then results from a reduction of interfacial area through interface motion. The rate of interfacial area reduction per volume transferred across the interface is the local geometric mean curvature. Thus, local driving forces derived from variations in mean curvature allow tractable models for the capillarityinduced morphological evolution of isotropic interfaces. This chapter treats the morphological evolution of free surfaces under capillary driving forces, including phenomena associated with both isotropic and anisotropic surfaces. The kinetics of surface smoothing, the formation of surface grooves on free surfaces at intersections with grain boundaries, and the incipient evolution of a cylinder into a row of isolated spheres are considered for bodies with isotropic surfaces. Transport mechanisms include surface and volume diffusion and vapor transport. General methods of analyzing the evolution of anisotropic surfaces are Kinetics of Materials. By Robert W. Balluffi, Samuel M. Allen, and W. Craig Carter. Copyright @ 2005 John Wiley & Sons, Inc.
337
338
CHAPTER 14: SURFACE EVOLUTION DUE TO CAPILLARY FORCES
discussed; particular attention is given to the phenomenon of faceting and crystal growth when the surface velocity is a function of the surface inclination. In a twophase composite material of isolated spherical particles embedded in a matrix, there is a driving force to transport material from particles enclosed by isotropic surfaces of larger constant mean curvature to particles of smaller constant mean curvature. This coarsening process and the motion of internal interfaces due to curvature are treated in Chapter 15. 14.1
ISOTROPIC SURFACES
An isotropic surface with undulations will generally evolve toward constant mean curvature as a result of the driving force arising from differences in curvature. As indicated by Eq. 3.76, material below a bump of large mean curvature has a larger diffusion potential than material below a bump of smaller mean curvature.’ Considering only capillary driving forces, it can be shown that irregularities on a uniform flat surface flatten due to capillarityinduced evolution, as illustrated in Fig. 3.7. However, a cylinder with surface irregularities can either evolve back to a uniform cylinder or toward a row of isolated spheres. The rate and characteristics of surface evolution depend on the particular transport mechanisms that accomplish the necessary surface motion. These can include surface diffusion, diffusion through the bulk, or vapor transport. Kinetic models of capillarityinduced interface evolution were developed primarily by W.W. Mullins [l41. The models involving surface diffusion, which relate interface velocity t o fourthorder spatial derivatives of the interface, and vapor transport, which relate velocity to secondorder spatial derivatives, derive from Mullins’s pioneering theoretical work. 14.1.1
Flattening of Free Surfaces by Surface Diffusion
Consider a system composed of only one type of atom along with its equilibrium point defects, having an initial surface profile y  yo = h ( z )
or
F ( z ,y) = y  h ( z )= constant
(14.1)
where h ( z )represents deviations from a flat (y = constant) surface as in Fig. 14.1.2 The diffusion potential of an atom at the surface is proportional to local surface curvature as demonstrated in Section 3.4. The curvature can be determined from Eq. 14.1 and is a function of z. The local diffusion potential produces boundary conditions for diffusion through the bulk or transport via the vapor phase. For surface diffusion, gradients in the diffusion potential produce fluxes along the surface. For surface diffusion, migration is constrained to a thin surface slab of thickness 6, as described in Section 9.1. Because the surface is an efficient pointdefect source, point defects may be assumed to be at their local equilibrium populations. l T h e following convention is employed: when a center of curvature is on the same side as the material in question, the curvature is positive. A ball has positive curvature; a spherical hole has negative curvature. ’Additional material regarding the mathematical descriptions of interfaces is given in Appendix C, particularly Eq. C.9.
14 1 ISOTROPIC SURFACES
339
Figure 14.1: Flattening of a ruled surface h(s)by surface diffusion. The normal velocity is proportional t o the accumulation of flux. The rate of vertical motion dhldt is related to the normal velocity u, by the local geometry of the surface.
Therefore, combining the forceflux equation (Eq. 2.21) and the diffusion potential at a curved interface (Eq. 3.76),
where c = 1/R is the concentration of atoms in a surface layer of thickness 6, and the surface mobility M s is related to the surface diffusivity *Ds by Eq. 3.43. Vsurf in Eq. 14.2 is the surface gradient operator, which has derivatives within the interface (i.e., it is a twodimensional gradient operator in the interface tangent plane). For a twodimensional interface embedded in three dimensions {z(u, w),y(u, w), z(u,w)}, with interfacial coordinates (u, w) and curvature K , the surface gradient of K , (14.3) is a vector perpendicular to the surface normal which points in the direction of fastest increase in K . For the ruled surface described by Eq. 14.1,
Js
=
ys*Ds dr; k T ds
(14.4)
where s is the arc length along the surface curve y  h ( z )= constant, as illustrated in Fig. 14.1. The rate of particle accumulation at a particular surface site is the integral of the flux over the surface enclosing each surface site. Representing each surface site as a box with a square base of area l/cs (where cs is the number of surface sites per area) and height 6, the particle accumulation rate is
ii/s
=
J
boxwalls
 . dA
JS
=
J
boxvolume
+
V . J s dV
RZ
 6
V . J s 
CS
(14.5)
The atom addition rate per unit area is N s c s =  6 V . 3 , and therefore the normal velocity of the surface is
340
CHAPTER 14: SURFACE EVOLUTION DUE T O CAPILLARY FORCES
where BS collects the kinetic and material coefficients that multiply the surface Laplacian, VZurfE V7,,,f~Vsurf, the twodimensional Laplacian operator with derivatives with respect to coordinates in the interface as in Eq. 14.3. The figure indicates a relation between the rate of change of the surface height, h, and v,: (14.7) Figure 14.1 indicates that the derivatives with respect to arclength, s, can be converted to derivatives with respect to x using ds2 = dh2 dx2. From the expression for .K in Eq. C.5,
+
dh
BS
r
d
1
In the limit of small slopes, Idh/dxl << 1,
dh =
at
sd4h B +3BS 8x4
(14.9)
The second term on the righthand side is negligible unless there are regions where the (small) slopes change rapidly. Any such regions disappear rapidly, due to the first term. Therefore, the linearized surface diffusion equation is
dh _ B
dt
d4h =
6x4
RySG*DS d4h kT ax4
(14.10)
The dependence of h on the length scales of the surface roughness can be analyzed with independent Fourier components having the form
(2Y)
h ( x ,t ) = A ( t )sin Substitution of Eq. 14.11 into Eq. 14.10 gives dA(t)  
A(t)
RySG*DS
kT
(27r)4 dt
(14.11)
(14.12)
so that the time dependence of the Fourier amplitude, A @ )is ,
A ( t )= A(0)eBS(2"/w4t
(14.13)
The amplitude decay exponent is proportional to l / X 4 ; finescale roughness therefore disappears much more rapidly than longerwavelength surface roughness. General roughness can be decomposed into a sum of Fourier terms, and since Eq. 14.10 is linear, each term decays independently. Physically, the shortwavelength modes disappear rapidly and the flattening rate of an isotropic surface by surface diffusion is limited by the longest wavelength. Equation 14.13 is an approximation
14.1:ISOTROPIC SURFACES
341
for the limit of small slopes. However, numerical solutions of the nonlinear evolution equation, Eq. 14.8, for largeslope conditions indicate that the smallslope approximation can be applied in the general case without significant error [5]. The wavelength dependence in Eq. 14.13 can be used for experimental measurements of the surface and kinetic coefficients that constitute B S . If an array of evenly spaced parallel grooves is introduced on a surface, the spacing dependence of the grooves' amplitudedecay factor can be measured [6]. An analysis for flattening of an isotropic surface by bulk diffusion as in Fig. 3.7 is presented in Exercise 14.1. 14.1.2
Surface Evolution by Vapor Transport
Solid/vapor interface motion can be produced by evaporationthe atoms that compose the solid phase are removed from the surface via the vapor phase; reverse motion can be produced by condensation where a vaporphase flux is directed onto the solid phase. Figure 14.2 illustrates how simultaneous evaporation and condensation can result in surface smoothing. Vapor transport differs from surface diffusional transport, where the flux is always in the surface plane. For both surface diffusion and vapor transport. the diffusion potential at the surface is proportional to the local value of y s if~ the surface free energy is isotropic. For surface diffusion, the interface normal velocity is related to a derivative (Le., the divergence of the flux). Also, the total volume is conserved during surface diffusion. For vapor transport, the interface normal velocity is directly proportional to the vapor flux, and the total number of atoms is not necessarily conserved. Crystal growth from the vapor phase has been treated in Chapter 12. An expression for the net atom flux, Jv,gained at a macroscopically flat crystal surface during growth from the vapor has been obtained in Exercise 12.2 in the form of Eq. 12.27. To treat surfaces possessing nonuniform curvature, this relationship can be generalized in the form
J" = K[P""b  P""K)]
(14.14)
where Pamb is the ambient vapor pressure in the system, P " ~ ( K is )the vapor pressure in equilibrium with a local region of the surface with curvature K , and K is a ) be derived by equating the atom diffusion rate constant. The function P " ~ ( Kmay potential in the surface and in the equilibrium vapor. For the vapor, dG = kT In P , and therefore p ' ( ~ ) p " ( ~= 0) = a"(.)  Q
~ ( K= 0)
= kT1n
Peq ( K = 0 )
J"
Figure 14.2: Flattening of surface h ( z )by vapor transport involving evaporation from regions of larger curvature and condensation at regions of lower curvature. The velocity along the surface normal is proportional to the normal flux a t the solid/vapor interface.
342
CHAPTER 14: SURFACE EVOLUTION DUE T O CAPILLARY FORCES
while at the surface, according to Eq. 3.76, these expressions results in
as(&) @ ( K
= 0) = RySr;. Equating
(14.15) The firstorder expansion employed will be valid under all usual conditions. The normal growth velocity of a local region of the surface with curvature then be found by using Eqs. 14.14 and 14.15:
u, = R J V = OK
[pamb
Peq(tc= 0) 
P e q(r;
= 0) RyS
kT
K
can
(14.16)
In the common situation where the surface contains undulations but is macroscopwill be well approximated by Peq(n = 0), so that ically flat, Pamb 21, = 
K@ySPeq(r; = 0) tc=B kT
VK
(14.17)
where the coefficient BV collects the vaportransport kinetic and material parameters (and has the same units as a diffusivity). Surface Grooving a t Surface/GrainBoundary Intersections by Vapor Transport. When a grain boundary with isotropic surface energy y B intersects a free surface with isotropic surface energy ysl a grainboundary groove forms in order to achieve a capillaryforce balance, as illustrated in Fig. 14.3. The dihedral angle II, is determined by Young's equation,
YB cos1c, = 2 27s
(14.18)
Grainboundary grooves can develop during thermal annealing by mass transport arising from vapor transport, surface diffusion, or surfacetosurface transport by means of volume diffusion. Equation 14.17 can be used to model grainboundary grooving kinetics when vapor transport is the dominant mechanism. The normal velocity ah/& is related
boundary
I
I yB
Figure 14.3: (a) Initial intersection of grain boundary with flat surface and (b) subsequent formation of surface groove with dihedral angle, $. Because a grain boundary migrates toward its center of curvature (discussed in Section 15.2), stationary grain boundaries intersect the surface at right angles.
14.1:ISOTROPIC SURFACES
343
to the vertical velocity as in Fig. 14.1 and Eq. 14.7:
BV
dh
(14.19)
In the limit of small slopes
lgl << 1, (14.20)
This surface evolution equation has the same form as the bulk mass diffusion equation; the concentration is replaced by the height of the surface, h,and the diffusivity is replaced by BV. For the grainboundary grooving problem, the initial and boundary conditions derive from the initial shape of the surface and Young’s equation at the groove notch:
h(x,t= 0)= 0
dh (x dX
= 0 , t ) =tan(
T  $
2
)
dh
(x dX
=~
, t=)0
(14.21)
Only x > 0 is considered, since the solution will have mirror symmetry about the grain boundary plane x = 0. These boundary conditions correspond to the constant surfaceflux diffusion problem in Section 5.2.5, in which the surface concentration increased proportionally to t112. Therefore, adapting the solution given by Eq. 5.69 to the grainboundary grooving model, h(0,t ) = 2 tan
(Ti$)
(14.22)
and the groove therefore deepens proportionally with t112 as well. Stability of a Cylinder. A cylinder of radius R, with isotropic ys can reduce its total surface energy if it evolves into a row of spheres with radii greater than 3R,/2 (Le., if each cylinder section with a length of at least 9R,/2 evolves into a sphere). Therefore, microstructures with cylindrical features can be morphologically unstable. However. kinetics requires that the total surface energy (or, surface area for the isotropic case) must decrease continuously if a cylinder evolves into a row of isolated particles. Continuous surfaceenergy reduction sets a fundamental or critical length scale for the wavelength, X c r i t , of an infinitesimal axial undulation on a uniform cylinder, which produces instability. Rayleigh derived an expression for Xcrit using perturbation analysis as follows [7]. Consider a radially symmetric perturbation (or an infinitesimal Fourier mode) on a uniform cylinder of initial radius R,:
R ( z , t ) = Rcyl(t)
2TZ + c ( t ) cos x
(14.23)
where ~ ( tis)the timedependent perturbation amplitude (see Fig. 14.4). The cylin
344
CHAPTER 14 SURFACE EVOLUTION DUE TO CAPILLARY FORCES
Figure 14.4: Perturbation of cylindrical body by a sinusoid. Longwavelength perturbations reduce the surface area of the Lody and ultimately result in breakup of the body into a linear array of spheres.
der is isolated so that its volume per wavelength, ITRZA,is constant. Therefore,
TRZX=
Jd JdA
= IT
x
r R 2 ( z ,t ) d z 27rz + f 2 ( t )COS' [ R b l+ 2 R c y l ( t )~ ( cos t)
x
"1'
x
dz
( 14.24)
+ I T X 2E 2 ( t )
= ITXR:,~ 
The average cylinder radius, Rcyl,must shrink when c(t)/Rois small according t o (14.25) The total surface energy per wavelength for the surface of revolution, Eq. 14.23, is x x ES = y S d A = ys 2~Rd.s
Jd
Jd
x
RJ;lz2fdRZ
= 27rys
LA R
( 14.26)
J
W
d
z
*
Expanding in powers of ~ ( t ) ,
( 14.27) = E,"
+ 7 r2yXVR(, t ) [(27rRo)2 x2] t
14.1:ISOTROPIC SURFACES
345
Therefore, the energy decreases continuously with time if the Rayleigh instability condition is satisfied, (14.28) X > Xcrit = 2nR0 Any perturbation with a wavelength less than the circumference of the cylinder will not grow. The particular characteristics of morphological evolution are determined by the dominant transport mechanism; their analyses derive from the diffusion potential, which depends on the local curvature. For a surface of revolution about the zaxis, the curvature is given by Eq. (2.16; that is,
a2R
1
(14.29)
Substituting Eq. 14.23 into Eq. 14.29 and expanding for small E/R, yields (14.30) 14.1.3
Evolution of Perturbed Cylinder by Vapor Transport
Suppose that a perturbed cylinder with radius given by Eq. 14.23 evolves by vapor transport in an environment with an ambient vapor pressure in equilibrium with = P e q ( , = l/R,). Then, using Eqs. 14.15, 14.16, the unperturbed cylinder, Pamb and 14.17, u, = BV
($
(14.31)
 K )
According to Eq. 14.25, Rcyl N R,, so Eq. 14.23 shows that v, a t z = 0 is approximately d E ( t ) / d t . Therefore, using Eq. 14.30, 1
(14.32)
dt Small perturbations therefore evolve according to
E ( t ) = E(0)et/Tv(’)
( 14.33)
where the amplification factor l / r v = (Bv/Rz)[l  ( ~ T R , / X ) ~ This ]. firstorder kinetic result is consistent with the previous Rayleigh result: only perturbations with wavelengths longer than Xcrit will grow. 14.1.4
Evolution of Perturbed Cylinder by Surface Diffusion
Suppose that the perturbed cylinder considered above evolves by surface diffusion. A firstorder differential equation for the amplitude E ( t ) follows from inserting Eq. 14.30 into the surface diffusion relation, Eq. 14.6, and again setting u, = d c ( t ) / d t at z = 0:
39=47r2BS [ l dt
RZ X2
(i)2] 27rR,
E(t)
=
1
(14.34)
346
CHAPTER 14. SURFACE EVOLUTION DUE T O CAPILLARY FORCES
In addition to the Rayleigh result, Eq. 14.34 predicts that a particular perturbagrows the fastest and hence dominates the morphology of tion wavelength, A,, the evolving cylinder. This kinetic wavelength maximizes the righthand side of Eq. 14.34, giving the result ,,A = fiAcrit. 14.1.5
Thermodynamic and Kinetic Morphological Wavelengths
Comparison of surfacediffusion and vaportransport kinetics in Fig. 14.5 shows a difference in longwavelength behavior. The amplification factor ~ / T ( A )in the ) p[t/~ ( X)]is monotonically increasing for perturbation growth rate E ( t ) = ~ ( 0ex vapor transport and approaches BV/R: asymptotically for long wavelengths. For surface diffusion, ~ / T ( A )goes to zero for long wavelengths and has a maximum at A = fi (27rR,). For a cylinder with an initial small random roughness, evolution by . , , ,A For vapor surface diffusion results in a morphological scale associated with diffusion, no characteristic morphological scale is predicted. &d
dt
Figure 14.5: Behavior of the perturbationamplitude growth coefficients 1 / ~ " and l / r s for cylinderpertiirbatiori growth by vapor transport arid surface diffusioii, respectively. For surface diffusion, a fastestgrowing wavelength A,, determines a morphological scale for the initial instability. Except for the Rayleigh critical wavelength, &,.it, no characteristic length scale appears for vapor transport.
14.2 14.2.1
ANISOTROPIC SURFACES Some Geometrical Aspects of Anisotropic Surfaces
An anisotropic surface's energy per unit area, y(A), depends on its inclination, A. For isotropic surfaces, the surface energy is simply proportional to the area, but two additional degrees of freedom emerge for the anisotropic case. These correspond t o the two parameters required to specify the surface i n ~ l i n a t i o n .An ~ anisotropic surface can often decrease its energy at constant area by tilting (i.e., changing its normal). The variation of the interfacial energy with inclination can be represented conveniently in the form of a polar plot (or yplot), as shown in two dimensions in Fig. 14.6. Here, the energy of each inclination is represented by a vector, r ( A ) A 3Geometrical constructions for describing anisotropic surfaces are reviewed in Section C.3.1.
14.2: ANISOTROPIC SURFACES
C
347
D
Figure 14.6:
Construction for testing whether an interface of inclination A will prefer to be faceted into inclinations corresponding to points B and C. yplot same as in Fig. C.4a. (i.e., a vector normal to that inclination and of magnitude equal to the interfacial energy a t that inclination). If all of these vectors are referred to a single origin, the yplot is the surface passing through the tips of these vectors. Inclinations of particularly low energies will therefore appear as cusps or depressions in the plot. Conceptually, treatment of the morphological evolution for an anisotropic surface is no different than for an isotropic surfacekinetics requires that y(A) dA (compared to y J dA for an isotropic surface) must decrease monotonically. However, because the evolving surface's geometry is linked to the local surfaceenergy density through f i , the analysis is considerably more complicated. Furthermore, when a surface is sufficiently anisotropic, inclinations fi associated with large energies become unstable and cannot be in local equilibriumthe surface must develop corners or edges. The missing inclinations create points or curves on a surface where surface derivatives will be discontinuous. When the yplot has cusp singularities, planar facets may appear; such a surface can have portions that are smoothly curved or portions that are flat and these portions are separated by edges or corners where derivatives are discontinuous. For surfaces with the twodimensional yplot shown in Fig. 14.6, certain inclinations will be unstable and will be replaced by other inclinations (facets), even though this increases the total surface area. Whether a certain inclination is unstable and prone to facet into other inclinations can be determined by a simple geometrical construction using the yplot [8]. The surface will consist of two different types of facets, as in Fig. 14.7a. The energy of such a structure per unit area projected on the macroscopically flat surface, "ifac,is
s
where yi is the surface energy of the ithtype facet and f i is the fraction of the projected area contributed by facets of type i. If fi is the unit normal to the flat , and f i 3 are unit vectors normal to type1 facets, type2 facets, surface and f i ~ &, and along the facet intersections, respectively, as in Fig. 14.7a, fi = f i f i I +
f2h2
(14.36)
348
CHAPTER 14 SURFACE EVOLUTION DUE TO CAPILLARY FORCES
Figure 14.7: Morphology of an initially smooth surface that has reduced its energy by faceting. (a) Morphology if two facet inclinations are stable. (b) Morphology if three facet inclinations are stable.
If a set of vectors, St,reciprocal to the vectors hi, is introduced so that
6;=
a,
x
fi3
a1. (a, x a,)
'*
n2 =
a, x a1 (a, x a,)
6;=
??I x
a1. (752
a, x
fi3)
(14.37)
so that 6;. f i j = dij, Eq. 14.35 can be rewritten
where
Z= yl6p + 726; has the properties
Whether faceting will occur can now be settled by a simple geometrical construction using the yplot shown in Fig. 14.6. If the surface to be tested has the inclination fi and the inclinations corresponding to points B and C are chosen as the inclinations for the i = 1 and i = 2 facets, Zmust appear as shown in Fig. 14.6 in order to be consistent with Eq. 14.39. The energy of the surface of average inclination fi that is faceted into inclinations corresponding to points B and C is then, according to Eq. 14.38, the projection of Zon a. This energy is smaller than the energy of the nonfaceted interface (indicated by the outer envelope of the yplot) and the surface will prefer to be faceted. It may also be seen that the energies of all other surfaces with inclinations varying between those at B and C will fall on the dashed circle. All of these surfaces will therefore be faceted. On the other hand, a similar construction shows that all surfaces with inclinations between those at C and D will be stable against faceting into the inclinations at C and D . Points such as those at B and C where the dashed circle is tangent to the yplot therefore delineate the ranges of inclination between which the surface is either faceted or nonfaceted. The construction indicated in Fig. 14.6 is readily generalized to three dimensions: three facet planes could then be present, as in Fig. 14.7b, and c'then terminates at the point of intersection of three planes rather than two lines. Figure 14.8 shows a threedimensional yplot comprised of eight equivalent spherical surface regions. The shape of this yplot is consistent with all surfaces represented by the plot being composed of various mixtures of the three types of facets,
14 2 ANISOTROPIC SURFACES
349
The yplot for a material with a Wulff shape corresponding to a cube Figure 14.8: when y[100] = y[010] = y[001]. It consists of portions of eight identical spheres, shown here in cutaway view. These spheres share a common point at the origin. but each has a diametrically opposed point directed toward the eight (111) directions.
corresponding to the y[lOO],y[OlO],and y[OOl]vectors shown.4 Any interface corresponding to a vector lying on a groove at the intersection of two spheres, such as y h v l will consist of t w o types of facets. corresponding to a pair of the vectors y[100], y[OlO],or y[OOl].Any interface corresponding to a vector going to a spherical region of the plot. such as ypyrlwill consist of three types of facets. corresponding to y[lOO],y[OlO],and y[OOl]. Figure 14.9 shows a threegrain junction on the surface of polycrystalline A1203 after hightemperature annealing. Each grain surface has a different inclination
Fi ure 14.9: Surface morphology of three faceted grains in an annealed alumina pofjfcrystal. From J M Dynys [9]. 41n Fig. 14.6. which holds in two dimensions, the energies of all faceted surfaces with inclinations between B and C fall on the dashed tangent circle shown. In three dimensions, a comparable construction would show t h a t faceting would occur on three facet planes, such as in Fig. 14.7b, and t h a t the counterpart to the tangent circle would be a tangent sphere.
350
CHAPTER 14: SURFACE EVOLUTION DUE TO CAPILLARY FORCES
and exhibits a different facet morphology. Grain 1 remains flat, grain 2 shows two facet inclinations, and grain 3 exhibits three facet inclinations. Other constructions employing the yplot are reviewed in Section (2.3.1. These include the reciprocal yplot, which is also useful in treating the faceting problem above, and the Wulff construction, which is used to find the shape (Wulff shape) of a body of fixed volume that possesses minimum total surface energy. 14.2.2
Rate of Morphological Interface Evolution
The kinetics of the morphological evolution of anisotropic interfaces can be developed as an extension of the isotropic case. Isotropic interface evolution originates from a diffusion potential proportional to the local geometric curvature (mean curvature) multiplied by the surface energy per unit area. The local geometric curvature is the change of interface area, 6A,with the addition of volume 6V,K = 6A/6V (see Section C.2.1). Therefore, the local energy increase due to the addition of an atom of volume R is Ryn. The anisotropic analog to the isotropic energy increase is the weighted mean curvature K, = 6(yA)/6V,developed by J. Taylor [lo]. In the anisotropic case, the diffusion potential is increased by, RK,, the local energy increase per adatom. It can be shown that K,
= VJsurf
f(fi)
(14.40)
where f i s the capillarity vector and Vsurfis the surface divergence operator, similar to the surface gradient introduced in Eq. 14.2.5 Two different types of derivatives are involved in this expression for &,the first produces {from a derivative in yspace as seen in Eq. C.20; the second derivative used to obtain the divergence is taken along the evolving interface. Evolution by Surface Diffusion and by Vapor Transpott. Although calculation of the morphological evolution for particular cases can become tedious, the kinetic equations are straightforward extensions of the isotropic case [ l l ] . For the movement of an anisotropic surface by surface diffusion, the normal interface velocity is an extension of Eq. 14.6 which holds for the isotropic case; for the anisotropic case,
(14.41) If the surface diffusivity is anisotropic, its surface derivatives must appear as well. For movement by vapor transport of an anisotropic interface that is exposed to a vapor in equilibrium with a very large particle6, the normal interface velocity is an extension of Eq. 14.17:
vn = 
K R ~ P ~ =~ 0) ( K kT
6l
(14.42)
The expression for weighted mean curvature for any surface in local equilibrium is simplified when the Wulff shape is completely faceted [lo, 121. In this case, 5The capillarity vector $ and the weighted mean curvature ny are discussed in more detail in Section C.3.2. 6Weighted mean curvature, which is uniform on a Wulff shape, goes to zero in the limit of large body volumes.
14.2: ANISOTROPIC SURFACES
351
tractable expressions and simulations can be produced for morphological evolution by surface diffusion and vapor transport [13].However, these models do not include edge and corner energies because they are inadmissible in the Wulff constructionnor do they include nucleation barriers for ledge and step creation, ledgeledge interactions, and elastic effects associated with edges and corners. Growth Rate for InclinationDependent Interface Velocity For a crystalline particle growing from a supersaturated solution, the surface velocity often depends on atomic attachment kinetics. Attachment kinetics depends on local surface structure, which in turn depends on the surface inclination, A,with respect to the crystal frame. In limiting cases, surface velocity is a function only of inclination; the interfacial speed in the direction of A is given by w(A). The main aspects of a method for calculating the growth shapes for such cases when .(A) is known is described briefly in this section. Given an initial surface, F(t = 0), the surface morphology at some later time, t , can be computed from the growth law w(A) with a simple construction [14,151. Let r(fl be the time that the growing interface reaches a position r'; therefore, the The surface level set tconst= r(fl could be inverted to give the surface F(tcOnst). normal must be in the direction of the gradient of 7 ; A = Vr/lVrl,where IVrI must be proportional to [w(A)]'. Solving for the constant of proportionality, a , as a function of V r ,
(14.43)
wext(p3 is the homogeneous extension of the surface velocity w(A) from A on the unit sphere t o gradients of arbitrary magnitude p" V r [16]. The extended normal velocity, wext (p3, can be used to construct characteristics that specify the surface completely at some time t [14].The characteristics are rays that emanate from each position on the initial surface ?(t = 0), given by ?(t) = r'(t = 0) + t V&=t(p3
(14.44)
The surface normal A is constant along the characteristics, and therefore the surface velocity u(A) is constant as well (see Exercise 14.5).The characteristics, defined as
(14.45) do not depend on the magnitude lVd. Therefore, the timedependent morphology can be calculated directly from any initial surface r'(t = 0) and a normal velocity .(A) by the following procedure. First calculate ((A) for every point on the initial surface ?(t = 0), then construct rays equal to tf from each point. Using Eqs. 14.44 and 14.45,the surface positions at an arbitrary time t are
?(t) = ?(t = 0) + tf((a)
(14.46)
The method is illustrated with a simple example in two dimensions. Suppose that the surface has the symmetry of a square and w(k) = w(n1,n2) = w(cos8, sine)
352
CHAPTER 14: SURFACE EVOLUTION DUE T O CAPILLARY FORCES
is given by
w(h)= 1 + p(n; + cun;n; + n;) (14.47)
where a: and ,B are constants. The velocity w(h) and its associated [ ( h ) are illustrated in Fig. 14.10 for particular values of Q and p.'
Figure 14.10: Exaniples of ~ ( A ) iand i <(ii) from Eq. 14.47 for ,B = 1/2 and LY = 4. (a) A polar plot of ~ ( i i ) i The i . magnitude of the plot in each direction, ii = (cos 8, sin O ) , is the velocity in that direction. (b) <(ii) is plotted parametrically as a function of 8. The vector
<(A) = f ( 8 ) is generally not in the direction of ii(8). However, t,he surface of the <(O)plot at any point is always normal to f i ( 8 ) , as shown in Eq. C.19, which although written for Gii) and y(A), also holds for <(?i) and ~(6).
Figure 14.11 shows the shape evolution due to w(h) and its characteristics f i n Eq. 14.47 for an initially circular particle. After very long times, the only remaining orientations on the growth shape are those that lie on the interior portion of the fsurface; therefore, the portion of the <surface with the spinodes (the swallowtailshaped region) is removed. For morphological evolution during dissolution of a crystal (or disappearance of voids in a crystalline matrix), the same characteristic construction applies, but the sense of the surface normal is switched compared to Fig. 14.11. An example of dissolution is illustrated in Fig. 14.12. The asymptotic growth shapes (Fig. 14.11) are composed of inclinations associated with the slowest growth velocities, and the fastest inclinations grow out of existence by forming corners. On the contrary, for dissolution shapes (Fig. 14.12), the inclinations associated with the fastest dissolution remain and the slowspeed inclinations disappear into the corners. The asymptotic growth shape is the in7((i?L) is related to v(7i) in the same way that the capillarity vector, (, is related to y(6) and is constructed in the sanie way. The Wulff construction applied to v(A) produces the asymptotic growth shape. This and other relations between the Wulff construction and the commontangent constriiction for phase equilibria are discussed by Cahn and Carter [16].
14 2 ANISOTROPIC SURFACES
Shape at t = 0
Shape at t = t ,
Shape at t = 0
353
Shape,at t 2 > t ,
Figure 14.11: Development of growth shape for a n initially circular particle for the v ( f i ) illustrated in Fig. 14.10. Rays t f ( f i ) are drawn from each associated inclination on the initial surface. Fastestgrowing inclinations accumulate at 45" and its equivalents and form corners.
Figure 14.12: Development of di_ssolution shape for initially circular particle for the w(h)illustrated in Fig. 14.10. Rays tC(h) are drawn from each associated inclination on the initial surface. The slowestgrowing inclinations accumulate at 90" and its equivalents and form corners.
terior of the fsurface and the asymptotic dissolution shape is composed of those inclinations between the cusps on the swallowtailshaped region on the fsurface. Bibliography 1. W.W. Mullins. Solid surface morphologies governed by capillarity. In N.A. Gjostein, editor, Metal Surfaces: Structure, Energetics and Kinetics, pages 1766, Metals Park, OH, 1962. American Society for Metals. 2. W.W. Mullins. Theory of thermal grooving. J . App2. Phys., 28(3):333339, 1957.
354
CHAPTER 14 SURFACE EVOLUTION DUE TO CAPILLARY FORCES
3. F.A. Nichols and W.W. Mullins. Surface (interface) and volumediffusion contributions to morphological changes driven by capillarity. Trans. AIME, 233( 10):18401847, 1965. 4. W . W . Mullins. Grain boundary grooving by volume diffusion. 2 18(4) :35436 1, 1960.
Truns. AIME,
5. W.M. Robertson. Grainboundary grooving by surface diffusion for finite surface slopes. J . Appl. Phys., 42(1):463467, 1971. 6. M.E. Keeffe, C.C. Umbach, and J.M. Blakely. Surface selfdiffusion on Si from the evolution of periodic atomic step arrays. J . Phys. Chem. Solids, 55:965973, 1994. 7. J.W.S. Rayleigh. On the instability of jets. Proc. London Math. SOC.,1:413, 1878. Also in Rayleigh’s Collected Scientific Papers and Theory of Sound, Vol. I, Dover, New York. 8. C. Herring. Some theorems on the free energies of crystal surfaces. Phys. Rev., 82 ( 1):8793, 1951.
9. J.M. Dynys. Sintering Mechanisms and Surface Diffusion for Aluminum Oxide. PhD thesis, Department of Materials Science and Engineering, Massachusetts Institute of Technology, 1982. 10. J.E. Taylor. Overview No. 98. 11Mean Acta Metall., 40(7):14751485, 1992.
curvature and weighted mean curvature.
11. J . E . Taylor, C.A. Handwerker, and J.W. Cahn. Geometric models of crystal growth. Acta Metall., 40(5):14431474, 1992.
12. A. Roosen and J . E . Taylor. Modeling crystal growth in a diffusion field using fullyfaceted interfaces. J . Computational Phys., 114(1):113128, 1994. 13. W.C. Carter, A.R. Roosen, J.W. Cahn, and J . E . Taylor. Shape evolution by surface diffusion and surface attachment limited kinetics on completely facetted surfaces. Acta Metall., 43(12):43094323, 1995. 14. J.E. Taylor, J . W . Cahn, and C.A. Handwerker. Overview No. 98. IGeometric of crystal growth. Acta Metall., 40(7):14431474, 1992.
models
15. W.C. Carter and C.A. Handwerker. Morphology of grain growth in response to diffusion induced elastic stresses: Cubic systems. Acta Metall., 41(5):16331642, 1993.
16. J.W. Cahn and W.C. Carter. Crystal shapes and phase equilibria: A common mathematical basis. Metall. Trans., 27A(6):14311440, 1996.
17. J.W. Cahn, J.E. Taylor, and C.A. Handwerker. Evolving crystal forms: Frank’s characteristics revisited. In R.G. Chambers, J.E. Enderby, A. Keller, A.R. Lang, and J.W. Steeds, editors, Sir Charles Frank, OBE, FRS, A n Eightieth Birthday Tribute, pages 88118, New York, 1991. Adam Hilger.
EXERCISES
14.1 Section 14.1.1 treated the smoothing of a sinusoidally roughened surface by means of surface diffusion to obtain Eq. 14.13. Show that the corresponding expression for smoothing by means of crystal bulk diffusion, as in Fig. 3.7, is (14.48) where w 0
= 27r/X.
Use the same smallslope approximations as in Section 14.1.1.
EXERCISES
355
Assume that selfdiffusion occurs by a vacancy mechanism and take Eq. 13.3 as the volume diffusion equation. Assume that the diffusion field is in a quasisteady state and that local equilibrium is maintained at the surface and in the volume at a long distance from the surface, where pv = 0 and p~ has the value characteristic of a flat surface. Note that one of the solutions to Laplace’s equation is @A =
p~  pv = a1
+ a2 sin(wz) ewy
(14.49)
Solution. The height of the surface is given by h = Asin(wx) and the flux equation is given by Eq. 13.3. Therefore, (14.50) To evaluate Eq. 14.50 we must obtain an expression for diffusion equation,
@A
by solving the steadystate
(14.51) in the volume, subject t o appropriate boundary conditions. A t the surface (i,e., at y = 0), p v = 0, and from Eq. 3.76, = pz ySRtcF.In the deep interior, pv = 0 and p~ = p i , so that @ A = p > . Because
+
.d 2 h
6x2
= Aw2 sinwx
(14.52)
the boundary conditions above and the diffusion equation are satisfied by a solution of the form of Eq. 14.49 with a1 = p i and a2 = ySCLAw2. Therefore, using Eqs. 14.49 and 14.50,
*DXLySRAw3 sinwx =  * D X L y S hRW 3 (14.53) kTf kTf Finally, because ( l / h ) ( d h / d t )= ( l / A ) ( d A / d t ) , Eq. 14.53 may be integrated t o prodh 
at
duce Eq. 14.48.
14.2 Figure 14.13 illustrates a portion of an infinite thin plate of thickness h containing a circular hole of radius R. The plate is held at a high temperature where diffusional transport processes become active. (a) At which specific location(s) will the shape of the plate first begin to change? Explain your reasoning in terms of driving forces for diffusion.
Figure 14.13:
Portion of infinite plate of thickness h containing a hole of radius R.
356
CHAPTER 14: SURFACE EVOLUTION DUE TO CAPILLARY FORCES
(b) What role do you expect the initial value of the ratio h l R t o have in determining whether the hole in the plate will either shrink and disappear spontaneously or grow spontaneously? Explain your reasoning. Solution. (a) Equation 3.76 demonstrates t h a t the diffusion potential of an atom a t a surface depends on the local surface curvature. Consistent with the convention that a convex spherical surface has a curvature +2/R (see Section 14.1),the curvature of the surface of the flat plate is zero and the initial curvature of the cylindrical surface inside the hole is K I = 1/m  1 / R = 1/R. The highest curvature is a t the "rim" o f the hole where the hole intersects the flat surface; the curvature here is K' = 1 / ~ 1 / R + +m. Therefore, there is a large diffusionpotential gradient for atoms at the rim of the hole. The first shape change would therefore be rounding o f the sharp edges of the hole. The driving force for diffusion would be reduction of the total surface area, and this would commence by movement of atoms away from the rim o f the hole toward both the flat plate surface and the cylindrical surface of the hole. The interior surface of the hole will continue t o evolve a t a slower rate, as described in part (6). (b) Recall t h a t curved interfaces can reduce their area by migration toward the center o f curvature o f the higher principal curvature. Consider t w o limiting cases, depicted in Fig. 14.14. Case 1, R >> h: assuming complete rounding of the sharp hole edges, as in Fig. 14.14a, the curvature o f the rounded hole will be K I l / ( h / 2 )1 / R x 2/h, and the surface tension force will cause the hole t o increase in diameter. Case 2 , h >> R : as in Fig. 14.146, the hole interior has curvature K' l / ( h / 2 ) 1 / R %  l / R , and the surfacetension force acts t o reduce the diameter o f the hole. One can make a simple calculation t o investigate this problem further. Assume that the hole o f diameter 2R lies somewhere in a fixed area A o f the plate. Then the initial total surface area o f the plate and hole (with sharp corners) will be Atot = 2A x2Rh  2xR2
=
=
+
Now the rate o f change o f Atot with hole diameter R is
dAtot = 2xh  4nR = 2 ~ ( h dR
~
and the limiting condition for hole expansion or contraction is simply h = 2R
Figure 14.14: Limiting cases of the evolving shape of a plate with a cylindrical hole. depicted in cross section. In Case 1, the hole expands; in Case 2, it will fill in.
14.3 Consider a pillboxshaped grain ernheddecl in a n otherwiw singlecrystal sheet (not shown) of thickness h. as in Fig. 14.15. Such a grain will shrink and
357
EXERCISES
r
Figure 14.15: Pillboxshaped grain in a singlecrystal sheet of thickness h.
eventually disappear. However, if grain boundary grooves develop on the two sheet surfaces and pin the boundary so that it is essentially stationary, the boundary can equilibrate locally and develop a minimumenergy form similar to that of a soap film held between two rigid circular wires. Show that such an equilibrated boundary would have the form T(Z)
= R, cosh
( 14.54)
Rul
Here, the cylindrical coordinate system in Fig. 14.15 has been employed and R, is the radius at the "waist" of the boundary. Calculate the force per unit length exerted on each groove by the pinned boundary when R, = h. Note: p = cosh(P/2) has two solutions, p = 1.1787 and p = 4.2536. What happens to the grain when R, decreases to 3/4h? Note: cosh(P/2) has no solutions when a < 0.75.
ap
=
Solution. (a) One way t o solve this exercise is t o show that the mean curvature of the boundary is zero when Eq. 14.54 is satisfied by inserting ~ ( zinto ) Eq. 14.29. There is then no pressure anywhere on the pinned boundary urging i t t o change its shape, and it possesses the shape of minimum energy. However, direct consideration of the two curvatures is instructive. Figure 14.16 shows a convenient choice for the two orthogonal planes which will be used t o find the mean curvature by the method illustrated in Fig. C.2. Consider the curvature a t a general point on the boundary such as P in Figs. 14.15 and 14.16. The first plane, Plane 1, selected is the constant4 plane in Fig. 14.15, which lies in the plane of the paper in Fig. 14.16. The second plane, Plane 2 (which must be orthogonal t o the first and intersect i t along fi) is indicated by its trace, A B , in Fig. 14.16. Using Eq. C.5, the curvature of the boundary intersection with Plane 1 is
(14.55) 
 cosh(z/Rw)
R,[1

1
+ ~ i n h ~ ( z / R , ) ] ~ R, / ~ coshz(z/Rw)
358
CHAPTER 14: SURFACE EVOLUTION DUE TO CAPILLARY FORCES
L
f
Figure 14.16: plane.
Intersection of the pillboxshaped grain in Fig. 14.15 with a constant4
Plane 2 is tilted with respect t o the Therefore,
z = 0 plane by the angle q5 = tan'(dr/dz).
cosq5 =
1
4
(14.56)
The curvature o f the line of intersection of the boundary with a plane parallel t o the sheet surface is ns = l / r ( z ) . The curvature of the line of intersection of the boundary with Plane 2 is then 1
(14.57) This follows from the fact that the curvature is the rate of change of the tangent vector as the curve is traversed (see Fig. C . l ) . Using Eq. 14.57, IC2
=
1
R, cosh(z/R,)Jl

+ sinh2(z/RW)
1 RWcosh2(z/Rw)
(14.58)
+
The mean curvature of the boundary a t P is therefore IC = ICI I C ~= 0. Alternatively, Eq. C.18 can be used t o demonstrate that the mean curvature is zero on the bou ndary. (b) If f is the force per unit length, the work required t o expand the boundary radially by dR, is dW = dB = f 2.rrRgdR,, where d 0 is the change in the energy of the boundary region lying between z = 0 and z = h/2. So
f= 1 dB 2xR, dR,
(14.59)
Integrating over this boundary region yields h/2
rJ1+ (dr/dz)2 dz =
2
hR,
+ RL sinh ) RW
(14.60)
Using Eq. 14.54,
(14.61) Because
B = B(Rw) and R,
= Rg(Rw),Eq. 14.59 can be written
f=
1 dB/dRw 2.rrR9 dRg/dR,
(14.62)
EXERCISES
Using Eqs. 14.60 and 14.61 and defining p
359
= h/R,,
+
f =  ~~h 1  coshp (2/p) sinhp 4Rg cosh(2lp)  (2//3) sinh(2/P)
(14.63)
When R, = h , Eq. 14.61 becomes
P
= cosh(2/p)
(14.64)
and Eq. 14.63 becomes
(14.65) The value of P in Eq. 14.65 must satisfy Eq. 14.64. The smaller solution of Eq. 14.64 for P gives the smaller boundary energy 9 , and therefore putting p = 1.1787 into Eq. 14.65 gives the force per unit length acting on the groove as
f =0.5296~~
(14.66)
The total force, Ftot,acting on the groove is
Ftot= 2?rRgF= 2.irRg(0.5296yB)= 3.3273RgyB
(14.67)
(c) When the groove shrinks below a critical size, no minimal solutions can be obtained for the grain boundary. Note that this happens well before the "waist" pinches down t o zero. The boundary then becomes unstable. Assuming that the boundary mobility is large compared t o the groove mobility, beyond the stability point, the boundary will pinch down and form two caps, which will subsequently "pop" through the top and bottom surfaces of the sheet. A circular "ghost" groove of the critical radius will be left on the surface.
14.4 Consider two faces of a faceted crystal advancing at different velocities during crystal growth as in Fig. 14.17. The growth rates of facets 1 and 2 are GI and (a) Find the condition on the velocities under which facet 2 will grow at the expense of facet 1. (b) Find the corresponding condition under which facet 1 will grow at the expense of facet 2 .
Figure 14.17: Two facets on a crystal growing at different velocities.
360
CHAPTER 14: SURFACE EVOLUTION DUE TO CAPILLARY FORCES
Solution.
In general, during unit time the faceted interface advances as shown in Fig. 14.17. In the situation shown, facets 1 and 2 will both grow with time. However, a few simple constructions show that if w2 < w1 cos8, facet 1 will shrink and facet 2 will grow. On the other hand, if w1 < w ~ c o s 8facet , 2 will shrink and facet 1 will grow.
14.5 Consider the growth from the vapor of a crystal possessing vicinal faces. The shape that the crystal assumes depends upon the number and rate at which ledges move across its surfaces. When one of the surfaces consists of a series of straight parallel ledges of height, h, running parallel to the z axis, the ledges move parallel to z, causing crystal growth along y. Let k = k(z,t)be the local ledge density at the point z. Also, let q = q(x!t ) be the ledge flux equal to the number of ledges passing the point z per unit time. The local slope of the surface is then (ay/ax), = hk and the rate of crystal growth along y is ( d y l d t ) , = qh. Assume that q = q ( k ) , which is often the case because the flux depends upon both the ledge density and the ledge velocity, which is, itself, dependent upon the ledge density. The rate of growth will then be a function of the inclination of the surface [i.e., 'u = w(fi)], as in Section 14.2.2. (a) Show that the moving ledges obey the equation of continuity,
(E),
=

(:It
(14.68)
(b) Using q = q ( k ) and the equation of continuity, show that (14.69) (c) Now consider a point on the evolving surface where the slope is constant.
Use the results above to show that this point moves along a trajectory which projects on the zyplane as a straight line. This trajectory, called a characteristic, is shown in Fig. 14.18.
Figure 14.18: (a) Various polar plots of w(A) for interfaces whose growth velocities, v(A),are functions of their inclinations, n. (b) Shapes at increasing times of a body that was initially spherical and whose w(A)plot is indicated by A in (a). Growth characteristics (outward rays) are shown which delineate the paths taken by points on the interface where the inclination remains constant. The tangent constructions along the characteristic indicated by B illustrate this constancy of inclination. From Cahn et al. (171.
EXERCISES
361
Solution. (a) In the usual way, the continuity relationship is (14.70) (b) Because k = k(x, t ) , (14.71) Because q = q(k), dq = (dq/dk)dk, and using Eq. 14.70,
(2)t dlc (z), ($Ix dk
dq
=
=
(14.72)

Therefore, combining Eqs. 14.71 and 14.72 yields (14.73) (c) The evolution of the surface shape as a function of x and t is shown in Fig. 14.19. A t a point where the slope is constant, k is constant and, since q = q(lc), q is also constant. Because dq/dk = f(k), dq/dk must also be constant. Therefore, according t o Eq. 14.73, dx/dt = dq/dk = constant. The point of constant slope must therefore project as a straight line in the ztplane. Now, d y = ($)tdx+ and
2
=
(
$)t
($)
g)x2
+(
(14.74)
dt
X
= hk
+ qhdt
dx
(14.75)
Because all the terms on the right side of Eq. 14.75 are constant, i t s projection in the xyplane must therefore be a straight line.
Y
tl
Figure 14.19: Steppedsurface evolution during crystal growth.
14.6 Prove that all of the results obtained in Exercise 14.5 for crystal growth (including the basic differential equation, its solution, and the expression for the sink efficiency) also hold for crystal evaporation.
362
CHAPTER 14: SURFACE EVOLUTION DUE TO CAPILLARY FORCES
Solution. The basic differential equation is in a form that holds for both growth and evaporation. The diffusion boundary conditions are the same for the two cases, and therefore the solution is equally applicable. Finally, the same expression for the efficiency of the surface is obtained. (Note that the two changes o f sign encountered in its derivation cancel.)
CHAPTER 15
COARSENING OF MICROSTRUCTURES DUE T O CAPILLARY FORCES
In Chapter 14 we focused on capillaritydriven processes that primarily alter the shape of a body. Two types of changes were considered: those driven by reduction of surface area, and those driven by altering the inclination of surfaces. In this chapter, changes in the length scales that characterize the microstructure are treated. Coarsening is an increase in characteristic length scale during microstructural evolution. Total interfacial energy reduction provides the driving force for coarsening of a particle distribution. Coarsening plays an important role in microstructural evolution in two principal ways. When a particulate phase is embedded in a matrix of a second phase, flux from smaller to larger particles causes the average particle size to increase as the total heterophase interfacial energy decreases. The particles compete for solute and the larger particles have the advantage. This process degrades many material properties, depending on the presence of fine precipitates. In singlephase polycrystalline materials, larger grains tend to grow at the expense of the smaller grains as the the total grainboundary free energy decreases. This process is also competitive and often produces unwanted coarsegrained structures. 15.1
COARSENING OF A DISTRIBUTION OF PARTICLES
15.1.1 Classical MeanField Theory of Coarsening In 1961, the classical theory of particle coarsening was developed at about the same time, but independently, by Lifshitz and Slyozov [l]and Wagner [2]. Most of the
*
Kinetics of Materials. By Robert W. Balluffi, Samuel M. Allen, and W. Craig Carter. Copyright @ 2005 John Wiley & Sons, Inc.
363
364
CHAPTER 15: COARSENING DUE TO CAPILLARY FORCES
theory’s essential elements were worked out earlier by Greenwood [3]. This theory is often referred to as the L S W theory of particle coarsening and sometimes as the GLSW theory. Consider a binary system at an elevated temperature composed of A and B atoms containing a distribution of spherical @phaseparticles of pure B embedded in an Arich matrix phase, a. The concentration of B atoms in the vicinity of each @phase particle has an equilibrium value that increases with decreasing particle radius, as demonstrated in Fig. 15.1. Because of concentration differences, a flux of B atoms from smaller to larger particles develops in the matrix. This flux causes the smaller particles to shrink and the larger particles to grow.
t
(4
G
t
T T
Distance, r

Figure 15.1: Effect of Pphase particle size on the concentration, Xeq,of component B in the cy phase in equilibrium with a Pphase particle in a binary system at the temperature T * . assuming that P is pure B. (a) Schematic freeenergy curves for cy phase and three Pphase particles of different radii, R1 > R2 > R3. The free energies (per mole) of the particles increase with decreasing radius due to the contributions of the interfacial energy. which increase as the ratio of interfacial area to volume increases. (b) Corresponding phase diagram. The concentration of B in the a phase in equilibrium with the &phase particles. as determined by the commontangent construction in ( a ) ; increases as R decreases, as shown in an exaggerated fashion for clarity. ( c ) Schematic concentration profiles in the cy matrix between the three Pphase particles.
365
15.1: COARSENING OF PARTICLE DISTRIBUTIONS
In the following, this model is used to analyze the kinetics for the two cases where the particle growth is either diffusion or sourcelimited. Each of the two cases yields a different growth law for the particles in the distribution. At any time t , a distribution of particle sizes will exist which can be quantified by defining a particlesize distribution function, f ( R ,t ) [units, (length)4], such that the number of particles per unit volume with radii between R and R dR, n ( R ,R dR;t ) , is given by
+
+
n ( R ,R + dR;t ) = f ( R t, )dR
(15.1)
It is assumed that the total number of B atoms in solution remains constant during coarsening, and that a particle increases its volume by R as it absorbs a B atom from solution. Therefore, the total volume of the particles is constant,' and (15.2) part Thus,
C R 2xdR= O
(15.3)
part where the sums are over all particles in the distribution. Diffusion Limited Coarsening. During diffusionlimited coarsening, the heterophase interfaces surrounding the particles act as highly effective pointdefect sources and sinks and maintain the concentrations of B in the Q phase in their direct vicinities at the equilibrium values. The rate of coarsening is then controlled by the rate at which diffusion can take place between the particles. An approximate expression for this equilibrium concentration as a function of particle radius can be obtained by assuming that: a and ,B are fluid phases; p is pure component B and is an incompressible spherical particle of radius, R; and Q is a dilute solution (see Section C.4.2). Using Eqs. A.4 and (3.37, the concentration of B atoms in Q at the a l p interface is
(15.4) where ceq(m) is the solubility of B in Q for a system with a planar a/,B interface. Because particles of different sizes are distributed throughout the bulk randomly, developing an exact model that couples diffusion to particle size evolution is daunting. However, a meanfield approximation is reasonable because diffusion near a spherical sink (see Section 13.4.2) has a short transient and a steady state characterized by steep concentration gradients near the surface. The particles act as independent sinks in contact with a meanfield as in Fig. 15.2. In the meanfield approximation, each particle develops a spherically symmetric diffusion field with the same farfield boundary condition fixed by the mean concentration, ( c ) . This mean concentration is lower than the smallest particles' 'This may not always be the case. For example, if the particles are formed by precipitation, coarsening may begin before complete precipitation has occurred [4].
366
CHAPTER 15 COARSENING DUE T O CAPILLARY FORCES
Figure 15.2: The meanfield approximation for diffusionlimited coarsening. Each particle is surrounded by a spherically symmetric diffusion field (fluxes are indicated by arrows). The concentration in the matrix at the interface of each particle is fixed by Eq. 15.4 and the concentration farremoved from particles is fixed at ( c ) . The flux is zero near particles of average size, ( R ).
equilibrium concentration and higher than the largest particles' equilibrium concentration. Therefore, the large particles tend to grow and the small particles to shrink, as shown in Fig. 15.2. Using Eq. 13.22, the growth rate of a particle with radius R is dR c"'(R)  ( c ) ,  = D (15.5) dt R Combining Eqs. 15.3 and 15.5 gives

C R(ceq(R) ( c ) )= 0
(15.6)
part
Substituting the expression for ceq(R)into Eq. 15.6,
c
R [ ( c ) c e q ( m )
(15.7)
part
Rearranging this equation gives (15.8) part
part
On further rearrangement, Eq. 15.8 becomes (15.9) where ( R )is the average particle size (radius), given by (15.10)
15 1 COARSENING OF PARTICLE DISTRIBUTIONS
367
where Ntot = Cpart 1 is the total number of particles. By comparison with Eq. 15.4, Eq. 15.9 shows that (c) is the matrix concentration in equilibrium with particles of size ( R ) : (4 = ceq((R)) (15.11) Subtracting Eq. 15.4 from Eq. 15.9 yields (c)  ceq(R)=
kT
( 15.12)
Equation 15.5 can be combined with Eq. 15.12 to obtain (15.13) Therefore, when R < ( R ) ,dR/dt is negative, and when R > ( R ) ,dR/dt is positive. Equation 15.13 is an example of the results of a meanfield theorythe behavior of any particular particle depends only on its size compared to the mean particle size ( R ) . Figure 15.3 presents a schematic plot of this equation for two different particlesize distributions, f l and f 2 , such that (R)z= 1.5(R)l. The particle size for which the rate of particiesize growth will be a maximum must satisfy the condition (15.14) Thus, the maximum rate of particle size increase occurs at R,,, = 2(R). Several qualitative observations may be made about the time dependence of the particlesize distribution. As predicted by Eq. 15.14, the growth of the largest particles will be slow and particles with smaller radii (but greater than ( R ) )will grow more quickly, shifting the distribution of particles toward 2 ( R ) . However, the average radius, ( R ) ,is an increasing function of time. Ultimately, the tail of the distribution at large R is expected to diminish with time and particles with R >> ( R )will be rarely observed. Figure 15.4 depicts this expected shift of the distribution.
t
Figure 15.3: Particle growth rate vs. particle size in Eq. 15.13. f l and f 2 represent the growth rate for two different particlesize distributions, such that (R)2= 1.5(R)l.
368
CHAPTER 15: COARSENING D U E T O CAPILLARY FORCES
Figure 15.4: Initial distribution, f l ( R ) ,changing with time according to the growth law, Eq. 15.13. The smallest particles disappear with relatively large shrinkage rates, so the lower end of the distribution collapses to zero.
The time dependence of the particlesize distribution can be studied analytically by developing a differential equation based on the flux of particles that occurs in particlesize space as the distribution evolves. The flux of particle density passing (15.15) The accumulation equation is then (15.16) Equation 15.16 is the rate of change o f f in the interval ( R ,R+ dR),and is related to the difference between the rates of particles entering from below and exiting the interval a t R dR. Combining Eqs. 15.13 and 15.16 gives
+
d f ( R ,t ) dt
dR[
25yR2ceq(m) d
kT(R)
]
( R ( R ) f) ( R t, ) R2
(15.17)
If an initial form of f ( R , t = 0) is assumed (e.g., a Gaussian distribution), it is possible to compute the form of f ( r ,t ) at later times using Eq. 15.17. Solutions of this type yield the following results [l,21:
A steadystate (normalized) distribution function is approached asymptotically as t + m. This steadystate distribution, illustrated in Fig. 15.5, is
approached by all initial distributions. The most frequent particle size in the steadystate distribution is 1.13(R)and there will be no particles larger than 1.5(R), the cutofl size.
During annealing, the mean particle size increases with time, and the number of particles, Ntot, decreases because the smallest particles disappear as the larger ones grow. The growth law (Eq. 15.13) and the continuity equation €or the particlesize distribution (Eq. 15.17) lead to the equation for the evolution of the mean particle size: (15.18)
where K D is the rate constant for diffusionlimited coarsening. See Exercise 15.2.
15 1. COARSENING OF PARTICLE DISTRIBUTIONS
0 Figure 15.5: coarsening.
0.5
369
I .o
Final steadystate normalized particlesize distribution for diffusionlimited
Experimental Observations. Generally, two quantities are measured in experimental studies of particle coarsening [5]. First, the mean particle size is studied as a function of time. For volumediffusionlimited coarsening, the t1I3law corresponding to Eq. 15.18 is generally observed, in agreement with theoretical predictions. The second measured characteristic is the particlesize distribution, including its time dependence. The experimental timedependent evolution of particlesize distributions does not always match predictions from classical coarsening theory [5, 61; the distributions observed are generally broader than the classical theory predicts and particles are often larger than the predicted cutoff size, 1.5(R). A study of coarsening in semisolid PbSn alloys verified the t1I3law kinetics predicted by the meanfield theory (see Fig. 15.6). However, some aspects of the classical theory are not observed in Fig. 15.6. Limitations of the classical meanfield theory are discussed in Section 15.1.2.
To same scale
Different scales
Figure 15.6: Particle distributions observed in coarsening experiments on semisolid PbSn alloys. The volume fraction of particles is 0.64. The upper row shows a steady increase in mean particle size with aging time. The lower row is scaled so that the apparent mean particle size is invariantdemonstrating that the particle distribution remains essentially constant during coarsening. From Hardy and Voorhees [7].
370
CHAPTER 15: COARSENING DUE TO CAPILLARY FORCES
Source Limited Coarsening. During sourcelimited coarsening, the interfaces surrounding the particles behave as poor sources and sinks, and the coarsening rate then depends upon the rate at which the diffusion fluxes between the particles can be created or destroyed (accommodated) at the particle interfaces. In a simple model, the same assumptions can be made about the source action at the particles as those that led to Eq. 13.24. The rate of particle growth can then be written
dR (15.19) [c(R) c""(R)]R dt where K is the same type of rate constant as in Eq. 13.24. If diffusion in the matrix between the particles is so rapid, or K is so small, that all gradients in composition are essentially eliminated on a short time scale compared to the growth time of the particle, c(R)= ( c ) and the ratelimiting process is the source action. An expression for the average composition ( c ) can be obtained by first combining the growth law, Eq. 15.19, with Eq. 15.3 and assuming that the concentration field is uniform ( ( c )= c(R);see Fig. 15.7): =K
C R ~ ( c " ~ ( R( c)) )= o
(15.20)
part
(15.21) Equations 15.19 and 15.21 lead to an expression for the growth rate of any particle in a particular size distribution: dR 
2Kce9(w)yR2 ( ( R ) dt kT ( R 2 ) €21 ) This leads to the integral equation,
R 2 ( t ) R2(0)= 4 K c yIcT m)yR2
(I'
g d t
(15.22)

t)
(15.23)
Figure 15.7: Solute concentration field for sourcelimited kinetics. The matrix concentration field is essentially uniform and c = (c) everywhere, including the regions adjacent to the particles where c ( R )= (c).
15.1: COARSENING OF PARTICLE DISTRIBUTIONS
371
Equation 15.23 can be averaged and Wagner derives the solution, (15.24) where KS is the rate constant for sourcelimited coarsening [2].
15.1.2 Beyond the Classical MeanField Theory of Coarsening The meanfield theory has a number of shortcomings, including the approximations of a mean concentration around all particles and the establishment of spherically symmetric diffusion fields around every particle, similar to those that would exist around a single particle in a large medium. The larger the particles’ total volume fraction and the more closely they are crowded, the less realistic these approximations are. No account is taken in the classical model of such volumefraction effects. Ratke and Voorhees provide a review of this topic and discuss extensions to the classical coarsening theory [8]. Work by Voorhees and Glicksman concludes that the classical theory is correct in the limit of zero volume fraction of the coarsening phase and that both the kinetics and the size distributions are significantly dependent on the precipitate volume fraction, 4 [9121. The temporal law for diffusionlimited coarsening, given by Eq. 15.18, remains valid for all volume fractions, but the rate constant K D is a monotonically increasing function of q3, as in Fig. 15.8. Volumefraction effects on particle coarsening rates have been observed experimentally. For comparisons between theory and experiment , data from liquid+solid systems are far superior to those from solid+solid systems, as the latter are potentially strongly influenced by coherency stresses. Hardy and Voorhees studied Snrich and Pbrich solid phases in PbSn eutectic liquid over the range 4 = 0.60.9 and presented data in support of the volumefraction effect, as shown in Fig. 15.9 [7]. Voorhees’s experimental study of lowvolumefractionsolid liquid+solid PbSn mixtures carried out under microgravity conditions during a space shuttle flight enabled a wider range of solidphase volume fractions to be studied without significant influence of buoyancy (flotation and sedimentation) effects [13]. The rate of approach to the steadystate particlesize distribution in 0.10.2 volumefraction
2
4 
G A a v

o Snrich particles a Pbrich particles Theory

a
a o
Figure 15.8: Rate constant KD(C$) for particle coarsening vs. volume fraction of particles, ) volume fraction C$ to that at q5 = 0.6. expressed as a ratio of the rate constant K ~ ( q 5at From Hardy and Voorhees [7].
372
CHAPTER 15: COARSENING DUE TO CAPILLARY FORCES
1.o
0.2 n
Figure 15.9: Coarsening data from experiments on semisolid PbSn alloys, showing the effect of volume fraction 4 on the rate constant for coarsening, which is proportional to the slope of the curves. ( L ) is the mean linear intercept of the coarsening particles, measured on a random twodimensional section of the microstructure. From Hardy and Voorhees [7].
solid specimens was very slow. The initial stages of coarsening involved significant solidparticle clustering that accelerated the coarsening kinetics compared to a system with a random spatial arrangement of particles. Another complication is that the particles interact elastically, causing shape changes and other effects. Ardell and Nicholson were first to realize that elastic energy could influence particle distributions during coarsening [14]. Their study reported the formation of modulated (aligned) precipitate structures in NiA1 alloys after prolonged aging, thereby demonstrating that alignment of coherent misfitting precipitates along the cube axes of a material could lower its elastic energy. Another effect of elastic energy, described as stress coarsening, is seen in systems with coherent misfitting precipitates aged under an applied load, as studied originally by Tien and Copley [15]. In a nickelbased superalloy, single crystals coarsen when subjected to an applied uniaxial load, and precipitates form either platelets or rods, depending on whether the load is tensile or compressive. In the absence of load, the particles are cuboidal. This phenomenon, known as rafting, may allow the production of structural alloys with improved creep resistance. Even for a single coherent particle in a matrix, elastic anisotropy, elastic inhomogeneity, the applied stress state, and the stressfree transformation strain of the precipitates all influence the equilibrium precipitate shapes [16]. Numerical simulations of the coarsening of several particles are now possible, allowing the particles to change shape due to diffusional interparticle transport in a manner consistent with the local interphase boundary curvatures [17]. These studies display interparticle translational motions that are a significant phenomenon at high volume fractions of the coarsening phase. Examples which show that elastic interactions between particles can stabilize distributions of fine particles against coarsening include the observation by Miyazaki et al. that large particles in aged NiSi and NiA1 alloys split into pairs and even octets of smaller particles as aging proceeds [18]. In such cases, the reduction in
1 5 2 GRAIN GROWTH
373
elastic energy achieved by the splitting outweighs the attendant increase in interphase boundary area. Johnson has given a theoretical treatment of the coarsening in a twoprecipitate system under applied load [19].
15.2
GRAIN G R O W T H
Grain growth is a kinetic process by which the average grain size of a polycrystalline material increases during annealing at an elevated temperature. In this process (illustrated in Fig. 15.10), the larger grains tend to increase in size while the smaller grains shrink and eventually disappear, causing the total number of grains to decrease and the average grain size to increase. The driving force is the decrease in the total interfacial energy of the system that accompanies the growth. The construction of realistic models for this process, which include detailed information about the distribution of the evolving grains’ sizes and shapes, has proven to be elusive and has been reviewed [20, 211. Grain growth in twodimensional polycrystals (e.g., polycrystalline sheets with columnar grain structures) is taken up first because it is considerably simpler than growth in three dimensions. For twodimensional growth, there are powerful topological rules, and considerable progress has been made in developing detailed models for the process. Following this, grain growth in three dimensions is considered. Here, relatively little success has been met in developing physical models. and progress has been achieved mainly by using computer simulation. Grain growth in polycrystalline materials is similar in many respects to the growth of bubbles in froths or foams, to magnetic domain coarsening, and to the growth of cells in many types of cellular materials. Concepts and results developed for grain growth therefore also apply to these phenomena.
Figure 15.10: Simulation of isotropic arid uniform grain growth in two dimensions. The ( N  6) rule is obeyed for all grains except those intersecting the edge of the domain. Calculation using Surface Evolver [22]. Courtesy of Ellen J Siem.
15.2.1
Grain Growth in Two Dimensions
Topology of TwoDimensional Polycrystals. In two dimensions, three (and only three) grains meet at every grain boundary vertex, as in Fig. 15.10. Vertices where
374
CHAPTER 15: COARSENING DUE TO CAPILLARY FORCES
larger numbers of boundaries come together are unstable: for example, a conceivable fourgrain vertex would immediately decompose into two threegrain vertices connected by a new boundary segment. It is expected that the three boundaries at each vertex will be locally equilibrated with respect to one another; when all boundary energies are isotropic and equal, this equilibration requires that the net capillary force exerted by the three boundaries on the vertex be zero. This is accomplished when the boundaries meet at equal 120" angles. An important geometrical growth parameter is the average number of sides per grain, ( N ) ,in the ensemble, which can be determined with Euler's theorem, which states that N~  N~ + N~ = 1 (15.25) where N G is the number of grains, N B is the number of boundary segments, and N V is the number of vertices in the system. If there are NV vertices, the number of boundary segments must be 3 N B = NV 2
(15.26)
Each boundary segment provides a side for two grains, therefore ( N )= 2 N B / N G . Since N G , N B , and NV in Eq. 15.25 are all much greater than unity, N G N V = N B to a good approximation, and, using Eq. 15.26, N B = 3NG. Therefore,
+
(15.27) Model for TwoDimensional Grain Growth. During growth, the distribution of the sizes and shapes of grains evolves with time. The changes in the overall structure can then be described adequately by a distribution function F ( A ,N , t ) ,which represents the number of grains in the system that have area A and N sides at time t. This distribution evolves when grains grow or shrink without changing the number of their sides or discontinuously change the number of their sides by means of switching events, as illustrated in Fig. 15.11. In Fig. 15.11a, two vertices meet, two grains each lose a side, and two grains each gain a side. In Fig. 15.11b, a threesided grain shrinks to disappearance and all three grains lose one side apiece. In Fig. 1 5 . 1 1 a~ foursided ~ grain disappears, two grains each lose one side, and the other two grains retain their sides. In Fig. 15.11d1a fivesided grain disappears, one grain gains one side, two grains lose one side apiece, and two grains retain their sides. As shown below, it is unlikely that grains with N 2 6 will shrink to disappearance, so all significant switching events are included in Fig. 15.11. The rate of change of the distribution, F ( A ,N , t ) , is then the sum of two terms: the first is the rate at which grains possessing area A and N sides accumulate due to the growth or shrinkage of grains in the absence of switching, and the second is the
.. Figure 15.11:
Switching events during twodimensional grain growth.
From Thompson [21].
375
15 2 GRAIN GROWTH
rate at which they accumulate due to the switching of grain sides. To determine the first term, an expression is needed for the rate of growth or shrinkage of a single grain in the absence of switching. Growth or Shrinkage of a Single Grain in the Absence of Switching. A simple expression can be obtained if it is assumed that all boundaries are isotropic and of the same energy, y. Consider first the single isolated interior grain shown in Fig. 1 5 . 1 2 ~ . According t o Eq. C.17, any portion of its boundary will be subjected to a normal pressure directed toward its concave side and given by P = Y K (see the arrows in Fig. 15.12a). Following Eq. 13.7, we assume that the resulting boundary velocity will vary linearly with the pressure according t o = MBP = MBYK
(15.28)
where MB is a mobility linking velocity with pressure. If the local velocities of the boundaries are integrated along the perimeter of a grain, an expression for the rate of change of area of the interior grain is obtained:
dA dt
= 
lB
u ds = 
(15.29)
Assuming that MB and y and do not depend on orientation and curvature,
(15.30) = 2.irM~y
In the relationships above, 0 is the angle that the boundary normal makes with a fixed direction in the plane of the specimen. Because the curvature is the rate of change of the boundary normal as the line integral is carried out, K = d 0 / d s . Also, 0 varies between 0 and 27r in the integration, because the normal rotates by 27r as the boundary is traversed. Therefore, independent of the shape of the grain, Eq. 15.30 becomes dA  = constant (15.31) dt
Figure 15.12: (a) Twodimensional isolated grain. Arrows indicate loc,al pressures acting on the boundary. (b) Fivesided grain in polycrystalline material with isotropic grainboundary energies.
376
CHAPTER 15: COARSENING DUE TO CAPILLARY FORCES
This result holds even if mass is leaving the grain along some segments of the boundary and entering the grain along other segments, as in Fig. 15.12a. Now consider that the grain is one of many in a twodimensional polycrystal, as in Fig. 15.12b. The rate of area change is again given by Eq. 15.29, but now the change in boundary orientation has discontinuities in d 0 / d s at the vertices. If the grain has N sides, and there are therefore N vertices, the integral can be written as a sum of contributions from each boundary segment: dA")
dt

MBy
d0
+
dB+'.'+/
seg N
d0)
(15.32)
where A0 is the change in the exterior angle at each vertex:
A0 = Obegin(segmenti
+ 1) Oend(segmenti)
Assuming that the boundaries are locally equilibrated at each vertex, the angles between boundaries at each vertex are 2 ~ 1 3so , A0 = 4x13  T . Therefore,
x
d A ( N )= M g y 3 ( N  6) dt
( 15.33)
and grains with more than six sides will grow and those with fewer than six will shrink. This remarkable result of Mullins [23] generalizes an earlier result for the ( N  6)rule by Smith and von Neumann [24]. The growth rate depends only on grain topology and not on grain size. Grains with more than six sides grow as shown in Fig. 15.13, because the fixed angles at each vertex force the boundary segments to be concave away from the grain center. The pressure due to this curvature therefore induces growth. Grains with fewer than six sides show the opposite behavior, whereas grains with six sides possess flat sides and are static.
Figure 15.13: Shapes of Nsided grains in twodimensional polycrystals.
Completion of Model and Description of Its Behavior. Having the result given by Eq. 15.33, the rate of change of the distribution, F ( A ,N , t ) ,can now be expressed in the form [25, 261:
(15.34) The first term in brackets is the rate at which grains of area A and sides N accumulate in area space due to the growth or shrinkage of grains as described by Eq. 15.33. The second is the corresponding rate of accumulation of such grains due
15.2: GRAIN GROWTH
377
t o switching. In this nomenclature, I s p l , for example, is the rate at which grains of area A with N  1 sides gain a side by switching to become grains of area A with N sides. The development of exact expressions for the switching terms in Eq. 15.34 is difficult and has not been achieved. Marder obtained approximate expressions by applying some simple rules that ignored spatial correlations [25]. For example, when a foursided grain disappears, four grains are picked at random from the distribution and a side is removed from the two having the smallest areas. When a fivesided grain disappears, the grain that gains a side is the one that has the largest area. Using several additional approximations to obtain expressions for the switching terms and the rule that ( N ) = 6, Marder solved Eq. 15.34 numerically t o obtain the results shown in Fig. 15.14. The figure also contains experimental measurements of bubble growth in twodimensional soap froths for purposes of comparison.
v)
.C
0.4
m
& 0.3
c
0
'0
Experiment
.c u
0.2.
2 0.1
LL
0.01
1
0.1
n
"2 4
10
Time
6 8 10 12 14 16 Number of sides
(b)
(a)
Figure 15.14: (a) Average area of grains vs. time. (b) Fraction of grains possessing N sides. Figures compare Marder's theoretical results with experimental measurements of bubble growth in soap froths made by Glazier et al. From Marder [25]and Glazier et al. (271.
The agreement between theory and experiment is reasonably good, indicating that the model captures the essential physics of the phenomena. An important result, apparent in Fig. 15.14a, is that, after an initial transient, the model predicts a linear increase in the average grain area with time:
(A)
t
( 15.35)
As discussed below, this is expected if Eq. 15.33 applies and if statistical selfsimilarity holds during the growth process2 This work is reviewed by Thompson [21]. Computer Simulation of TwoDimensional Grain Growth. Because of the great difficulties in developing rigorous models for grain growth, computer simulation has been used to obtain more information about the details of twodimensional grain growth [21]. A wide variety of techniques is employed, including, among others, *Statistical selfsimilarity holds when the normalized grainsize distribution and the numberofsides distribution remain constant during growth. A grain structure at a later time then looks statistically similar t o itself at an earlier time, except for a uniform magnification, and the structures are therefore scaled with respect t o each other.
378
CHAPTER 15: COARSENING DUE TO CAPILLARY FORCES
Monte Carlo methods, direct tracking methods, and vertex models, where the evolution of the twodimensional grain structure is described in terms of the motion of the vertices. After initial transients, all of these simulations exhibit statistical selfsimilarity during growth and an average grain area that increases linearly with time according to Eq. 15.35. Further Aspects. The constant growth rate of the average grain area found above (Eq. 15.35) is to be expected when statistical selfsimilarity holds and individual grains grow or shrink according to Eq. 15.33 [28]. Consider a large area, A, containing G grains. Then (A) = A/G and (A') = (1/G) a:, where ai is the area of the ith grain, and the sum is over all grains. The latter expression can also be written
xzl
(15.36) Differentiating Eq. 15.36, with (A2)/(A)' = constant because of selfsimilarity, and using Eq. 15.33,
where Ni is the number of sides of the ith grain. However, G
33
ai(Ni  6) =
( A N N AN)
(15.38)
N=2
n=l
where AN is the total area occupied by Nsided grains. Note that the second sum begins with N = 2, because onesided grains do not exist. Therefore, using Eq. 15.38 in Eq. 15.37 yields (15.39) Here, A N / A ,the fraction of the total area occupied by Nsided grains, is constant because of selfsimilarity. It is often convenient to express the growth law given by Eq. 15.39 in terms of a linear grainsize dimension. If R,,, is the effective rootmeansquare radius of the roughly equiaxed grains, (15.40) and, therefore, upon integrating, R;ms
C ( t ) R;ms (0) = t ./r
(15.41)
The growth laws expressed by Eqs. 15.35 and 15.41 are consistent with the behavior of a wide variety of experimental systems and models as well as computer simulation [21].
15 2 GRAIN GROWTH
379
Finally, it should be noted that during grain growth in thin polycrystalline films, twodimensional grain growth may be seriously impeded if surface grooves form at the intersections of the boundaries and the specimen surface(s) as described in Section 14.1.2 [21, 291. The boundaries can then become trapped at these grooves leading to growth stagnation (see Exercise 14.3). 15.2.2
Grain Growth in Three Dimensions
Topological Aspects. The geometry of grain growth in three dimensions is more difficult to visualize and to analyze than in two dimensions, and only limited success has been achieved. Figure 15.15 shows the relatively simple structure of an idealized polycrystal in which all the grains are identical. Each grain is a tetrakaidecahedron (possessing 14 faces) arranged on a b.c.c. lattice. The threedimensional grain structure can be described in terms of grains, boundaries, edges, and vertices. Boundaries are the interfaces where two grains meet, edges are the lines along which three grains meet, and vertices are the points where four edges (and also four grains) meet.
Figure 15.15: Threedimensional polycrystal with all grains identical. Each grain is a tetrakaidecahedron with 6 square and 8 hexagonal faces.
When the boundaries are equilibrated with respect to one another locally at all edges and vertices, the net capillary force exerted on each junction will be zero. When Y~ is isotropic and the same for all boundaries, this condition is satisfied when there is trihedral symmetry along each edge and tetrahedral symmetry a t each vertex [i.e., at threeboundary junctions, two faces have a dihedral angle cosl(1/2) = 120", and at fouredge junctions, each pair of edges makes an angle cos'(1/3) = 109'28'1. It is expected that these local equilibrium symmetry conditions, known as Plateau's laws, will be closely satisfied during grain g r ~ w t h . ~ However, Plateau's laws are not obeyed by the grain boundary structure in the special polycrystal in Fig. 15.15. To achieve local equilibrium at all grain junctions. so that Plateau's laws are obeyed, the faces of each grain must be curved [31]. A boundary structure in which all junctions obey Plateau's laws is presented in Fig. 15.16, which shows a polycrystal consisting of six grains that meet at four vertices. Each grain fully occupies one face of the polycrystal. As in Fig. 15.15, 3These conditions are Young's equation, ~ l / s i n c # q = y ~ sin42 / = y3/sin@3, which requires all grainboundary angles to be 2 ~ / 3for the uniform boundaryenergy cme and the requirement that quad and higherorder junctions are unstable in two dimensions [30].
380
CHAPTER 15: COARSENING DUE TO CAPILLARY FORCES
Figure 15.16: An ort,horhombicshaped polycrystal composed of six grains that meet at four vertices. Each grain occupies one face of the polycrystal. Each vertex is shared by four grains. Three grains meet at each edge (triple line). Four edges meet at each vertex. All edges and vertices are in local equilibrium and t.he system obeys Plateau’s laws. All boundary energies are isotropic and equal. Figure was computed with Surface Evolver [22].
three grains meet at each edge, four grains meet at each vertex, and four edges meet at each vertex. The grain structure during growth will generally consist of a distribution of grains possessing a range of sizes (volumes) and various numbers of faces and edges. Plateau’s laws will be obeyed at all junctions. To characterize the distribution of grain shapes and sizes in a large threedimensional polycrystalline system, we take w, e, and f as the volume, number of edges, and number of faces, respectively, possessed by any particular grain. If E is the number of grain edges in the system, Euler’s theorem states that BE+V=G (15.42) Each boundary in the system provides two faces for grains. Therefore, the average number of faces per grain, ( f ) s y s t , is
(f),,,t
=
2B
(15.43)
G
where the symbol (0)syst indicates an average over the system. Because three grains meet at each edge, each edge in the system provides three edges for grains. Therefore, the average number of edges per grain, (e)syst,is 3E (e)syst= G
(15.44)
Also, because four edges emanate from each vertex and every edge connects two vertices, 4v E =  =22 V (15.45) By combining Eqs. 15.4215.45, 6
(15.46)
Because each edge on a grain provides two edges for faces on that grain, the average number of edges per face on grains is (ef)syst = 2(e)syst/(f)syst. Combining this
15.2:GRAIN GROWTH
381
result with Eq. 15.46 yields ,n
(15.47) It is readily verified by inspection that Eqs. 15.46 and 15.47 are obeyed for the grain structure in Fig. 15.15. Rate of Grain G r ~ w t h . The ~ ( N  6)rule for twodimensional grain growth in a system with isotropic and uniform boundary energies (Eq. 15.33) is an exact example of a principle which states that equivalent grains grow at identical rates. Equivalent grains are grains that belong to an equivalence class (i.e., grains having at least one topological feature in common). In the twodimensional case, the equivalence class consists of grains with the same number of sides, N , and grains with the same number of sides grow at the same rate. The (N6)rule's derivation is simple because there are no outofplane contributions to the boundary c ~ r v a t u r e . ~ No known simple equivalence class describes grain growth in three dimensions. Although no exact growth law for an equivalence class exists, approximate laws can be found that are obeyed on average for grains of the same equivalence class. Any particular grain will obey a growth law that depends on the curvature of its boundaries, subject to Plateau's laws, as well as a statistical growth law applicable for all members of its equivalence class. In twodimensional growth, the particular growth law is identical to the statistical law when the topological feature defining the class is chosen to be the number of grain sides, N . For threedimensional growth, a statistical growth law can be justified if v and e are chosen as the characteristic topological features that define the equivalence class. The choice of e is favored because all edges terminate at vertices and have similar topologies. For symmetric grains of volume v and number of faces f, the average growth rate, ( d v / d t ) r , , f } ,varies as 8as f becomes large [32]. Here, the symbol {v, f} indicates an average over all grains in the equivalence class possessing volume v and number of faces f. Equation 15.46, where (e)systis approximately proportional to (f),,,, for large f and e, indicates possibly similar behavior on average if e is chosen rather than f, and this suggests the expansion
(2){e,w} o):( (aE1l2+ b + c E  ' / ~+ . . . ) =
(15.48)
where (dv/dt)(,,,) is the average volumetric growth rate of grains belonging to the equivalence class {e, w} and the quantity ( d v / d t ) o is the shrinkage rate of a sphere of the same volume embedded in a matrix grain. The undetermined coefficients, a , b, c, . . ., have no explicit dependence on e. To obtain the behavior for e >> 1, the third and higherorder terms are neglected, and in analogy with soap froths in two dimensions, b is set equal to 1. This represents an offset from the mean pressure of the froth. By enforcing conservation of total volume by summing over all classes, (15.49) 4We are grateful to David T. Wu for content and sharing his recent results in this section. 5The GaussBonnet theorem, which relates integrals of Gaussian curvature ( l I ( R l R 2 )in three dimensions) over a surface to integrals of mean curvature (1/R1 1/Rz in three dimensions) over boundaries of the surface, is particularly simple in two dimensions. In two dimensions, the ( N  6)rule is equivalent t o the GaussBonnet theorem.
+
382
CHAPTER 15: COARSENING DUE TO CAPILLARY FORCES
A statistical growth law follows for grains with large edge number, e, given by (15.50) where the critical edge number, ecrit, is given by (15.51) Comparisons to direct simulations of grain growth by Wu et al. show that Eq. 15.50 is correct for small as well as large e [33, 341. Unlike twodimensional growth, the critical topological feature controlling the growth rate (in this case e rather than N ) is not constant but depends upon the state of the grainboundary structure. Little progress has been made in analyzing the complicated problem of grain switching in three dimensions. In view of this, extensive recourse has been made to computer simulation. This work requires extensive computer power, and the results have not been as definitive as for twodimensional grain growth. Evidence for statistical selfsimilarity has been obtained, and reasonable agreement with experiment has been found in certain cases. In experiments and in simulations, agreement with Eq. 15.41 has been found (see Thompson’s review [21]). Bibliography 1. I.M. Lifshitz and V.V. Slyozov. The kinetics of precipitation from supersaturated solid solution. J. Phys. Chem. Solids, 19(12):3550, 1961. 2. C . Wagner. Theorie der Alterung von Niederschlagen durch Umlosen (Ostwaldreifung). 2. Elektrochem. , 65(78):581591, 1961. 3. G.W. Greenwood. The growth of dispersed precipitates in solutions. Acta Metall., 4(3):243248, 1956. 4. J.S. Langer and A.J. Schwartz. Kinetics of nucleation in nearcritical fluids. Phys. Rev. A , 21(3):948958, 1980. 5. A.J. Ardell. Experimental Confirmation of the Lifshitz Wagner Theory of Particle Coarsening, pages 111116. Institute of Metals, London, 1969. 6. A.J. Ardell. Precipitate coarsening in solids: Modern theories, chronic disagreement with experiment. In G.W. Lorimer, editor, Phase Transformations 87, pages 485490, London, 1988. Institute of Metals. 7. S.C. Hardy and P.W. Voorhees. Ostwald ripening in a system with a high volume fraction of coarsening phase. Metall. Trans., 19A(11):27132721, 1988. 8. L. Ratke and P.W. Voorhees. Growth and Coarsening. SpringerVerlag, Berlin, 2002.
9. A.D. Brailsford and P. Wynblatt. The dependence of Ostwald ripening kinetics on particle volume fraction. Acta Metall., 27(3):489497, 1979.
10. P.W. Voorhees and M.E. Glicksman. Solution to the multiparticle diffusion problem with application to Ostwald ripeningI. Theory. Acta Metall., 32( 11):20012011, 1984. 11. P.W. Voorhees and M.E. Glicksman. Solution t o the multiparticle diffusion problem with application to Ostwald ripening11. Computer simulations. Acta Metall., 32(11):20132030, 1984.
15.2: GRAIN GROWTH
383
12. P.W. Voorhees. The theory of Ostwald ripening. J . Stat. Phys., 38(12):231254, 1985. 13. V.A. Snyder, J. Alkemper, and P.W. Voorhees. The development of spatial correlations during Ostwald ripening: A test of theory. Acta Muterialia, 48( 10):26892701, 2000. 14. A.J. Ardell and R.B. Nicholson. On the modulated structure of aged NiAl. Acta Metall., 14(10):12951310, 1966. 15. J.K. Tien and S.M. Copley. The effect of uniaxial stress on the periodic morphology of coherent gamma prime precipitates in nickelbase superalloy crystals. Metall. Trans., 2(1):215219, 1971. 16. S.M. Allen and J.C. Chang. Elastic energy changes accompanying the gammaprime rafting in nickelbase superalloys. J . Mater. Res., 6(9):18431855, 1991. 17. P.W. Voorhees, G.B. McFadden, R.F. Boisvert, and D.I. Meiron. Numerical simulation of morphological development during Ostwald ripening. Acta Metall., 36( 1):207222, 1988. 18. T. Miyazaki, H. Imamura, and T. Kozakai. The formation of y precipitate doublets in NiA1 alloys and their energetic stability. Mat. Sci. Eng., 54(1):915, 1982. 19. W.C. Johnson. On the elastic stabilization of precipitates against coarsening under applied load. Acta Metall., 32(3):465475, 1984. 20. J. Stavans. The evolution of cellular structures. Rep. Prog. Phys., 56:733789, 1993. 21. C.V. Thompson. Grain growth and evolution of other cellular structures. Solid State Phys., 55:269314, 2001. 22. K. A. Brakke. The Surface Evolver. Exp. Math., 1(2):141165, 1992. Publicly available software. 23. W.W. Mullins. Twodimensional motion of idealized grain boundaries. J . Appl. Phys., 27 (8):900904, 1956. 24. C.S. Smith. Grain shapes and other metallurgical applications of topology. In Metal Interfaces, pages 65108, Metals Park, OH, 1952. American Society for Metals. Also, see discussion by von Neumann following article, pages 108110. 25. M. Marder. Soapbubble growth. Phys. Rev. A , 36(1):438440, 1987. 26. F.E. Fradkov. A theoretical investigation of twodimensional grain growth in the “gas” approximation. Phil. Mag. Lett., 58(6):271275, 1988. 27. J.A. Glazier, S.P. Gross, and J. Stavans. Dynamics of twodimensional soap froths. Phys. Rev. A , 36(1):306312, 1987. 28. W.W. Mullins. On idealized 2 dimensional graingrowth. Scripta Metall., 22(9):14411444, 1988. 29. W.W. Mullins. The effect of thermal grooving on grain boundary motion. Acta Metall., 6(6):414426, 1958. 30. J. A. F. Plateau. Statique exppe‘rimentale et thpe‘orique des liquides soumis aux seules forces mole‘culaires. GauthierVillars, Paris, 1873. 31. C.S. Smith. Grain shapes and other metallurgical applications of topology. In A Search for Stmcture, pages 1725, Cambridge, MA, 1981. MIT Press. 32. S. Hilgenfeldt, A.M. Kraynik, S.A. Koehler, and H.A. Stone. An accurate von Neumann’s law for threedimensional foams. Phys. Rev. Lett., 86:26852688, 2001. 33. D.T. Wu and C.E. Krill 111. Unknown title (work in progress). To be submitted, 2005 (expected). 34. D.T. Wu and F. Wakai. Unknown title (work in progress). To be submitted, 2005 (expected).
384
CHAPTER 15: COARSENING DUE T O CAPILLARY FORCES
EXERCISES
15.1 Consider how the particlesize distribution changes with time for sourcelimited kinetics. Suppose that at t = t o ,the particlesize distribution is given is the maximum radius of any by f ( R , t = to) = AR(R,,,  R), where R,, particle. Calculate the rate at which f ( R , t = to) is increasing at R = Rmax. At what particle size is the value of f ( ~t = , to) constant? Solution. First calculate expressions for (R) and (R') for the growth rate:
and
Putting these results into Eq. 15.22,
where
A4 = constant. Using Eq. 15.16, we can now find how f changes in time: af 
dt
Therefore, a t R = R,,,,
4Rmax /5.
a
dR
[
E]
f(R,t)
3Rmax
= 2AM (5R  4Rma,)
af/& = (2/3)AM, and the distribution is constant a t R =
15.2 In Section 15.1.1 we pointed out that during diffusionlimited coarsening a final steadystate particle distribution corresponding to Fig. 15.5 is expected to develop after initial transients die away. Derive the particle growth law given by Eq. 15.18 using only Eq. 15.13 and the fact that no particles larger than 1.5(R) appear in the steadystate particle distribution, as is evident in Fig. 15.5. Solution. In the distribution, the size of the largest particles in the distribution, Rcutoff,always corresponds t o 1.5(R). The rate of growth of the largest particles is therefore given by Eq. 15.13: dRcutoff  2&aceq(w) dt kTRcutoff
(1
(R)
1
&off
)
(15.52)
Substituting (R) = (2/3)RcutPoffinto Eq. 15.52 and integrating yields
R L  o s ( t )  RX,t,ff(O) =
3E,ynceq(m) t kT
(15.53)
or, again using (R) = (2/3)R,utos,
(R(tN3  (R(0N3 =
85,yRP(W) t 9kT
(15.54)
15.3 The ( N  6)rule was derived for twodimensional grain growth in a thin film. However, only the interior grains were treated. What is the rule for the growth
EXERCISES
385
of the edge and corner grains? Under the same assumptions that apply for the (N  6)rule, find how the growth of a side grain and a corner grain in a square specimen such as shown in Fig. 15.17 depends on the number of neighboring grains, N. It is reasonable to assume that the grain boundaries are maintained perpendicular to the edges of the sample at the locations of their intersections, as shown. Local interfacetension equilibration obtains and Young’s equation is satisfied.
Corner grain
Side grain
Figure 15.17: Twodimensional grain growth on a square domain. Solution. As shown in Fig. 15.17, for side grains and corner grains the number of triple junctions is one less than the number of neighboring grains, N . For the side grains, the inclination o f the boundary normal changes by 7r from one end t o the other:   (7rN  4 ) 13
(15.55)
Side grains with more than four neighboring grains therefore grow. For the corner grains, the change is 7r/2: (15.56) Since there is no integer number of neighbors that can produce constant area for a corner grain, it is impossible t o stabilize grain growth on a rectangular domain.
15.4 (a) A cylindrical grain of circular cross section embedded in a large singlecrystalline sheet is shrinking under the influence of its grainboundary energy. Find an expression for the grain radius as a function of time. Assume isotropic boundary energy, y, and a constant grainboundary mobility, M B .
(b) Derive a corresponding expression for a shrinking spherical grain embedded in a large single crystal in three dimensions. Solution. (a) The grain area, A , is related t o its radius, Eq. 15.30,
dA
= 27ThfB’)’ dt
R,by A
=
dR
= 2rR
dt
7rR2. Therefore, using (15.57)
Integration o f Eq. 15.57 then yields
R 2 ( t ) R2(0)=  2 M ~ y t
(15.58)
386
CHAPTER 15: COARSENING DUE TO CAPILLARY FORCES
(b) Here, the velocity o f the spherical interface normal t o itself is given by Eq. 15.28 and, therefore,
2 v = M B ~= KMBY =
Integration of Eq. 15.59 then yields
R
dR x
(15.59)
(15.60) and the spherical grain shrinks twice as fast as the cylindrical grain because of i t s larger curvature.
CHAPTER 16
MORPHOLOGICAL EVOLUTION DUE T O CAPILLARY AND APPLIED FORCES: DIFFUSIONAL CREEP AND SlNTERlNG
Capillary forces induce morphological evolution of an interface toward uniform diffusion potentialwhich is also a condition for constant mean curvature for isotropic free surfaces (Chapter 14). If a microstructure has many internal interfaces, such as one with fine precipitates or a fine grain size, capillary forces drive mass between or across interfaces and cause coarsening (Chapter 15). Capillarydriven processes can occur simultaneously in systems containing both free surfaces and internal interfaces, such as a porous polycrystal. Applied forces can also induce mass flow between interfaces. When tensile forces are applied, atoms from an unloaded free surface will tend to diffuse toward internal interfaces that are normal to the loading direction; this redistribution of mass causes the system to expand in the tensile direction. Applied compressive forces can superpose with capillary forces to cause shrinkage. In this chapter, we introduce a framework to treat the combined effects of capillary and applied mechanical forces on mass redistribution between surfaces and internal interfaces. Applications of this framework include diffusional creep in dense polycrystals and sintering of porous polycrystals. Diffusional creep and sintering derive from similar kinetic driving forces. Diffusional creep is associated with macroscopic shape change when mass is transported between interfaces due to capillary and mechanical driving forces. Sintering occurs in response to the same driving forces, but is identified with porous bodies. Sintering changes the shape and size of pores; if pores shrink, sintering also produces macroscopic shrinkage (densification). Kinetics of Materials. By Robert W. Balluffi, Samuel M. Allen, and W. Craig Carter. Copyright @ 2005 John Wiley & Sons, Inc.
387
388
CHAPTER 16 MORPHOLOGICAL EVOLUTION DIFFUSIONAL CREEP, AND SlNTERlNG
Microstructures are generally too complex for exact models. In a polycrystalline microstructure, grainboundary tractions will be distributed with respect to an applied load. Microstructures of porous bodies include isolated pores as well as pores attached to grain boundaries and triple junctions. Nevertheless, there are several simple representative geometries that illustrate general coupled phenomena and serve as good models for subsets of more complex structures.
16.1 MORPHOLOGICAL EVOLUTION FOR SIMPLE GEOMETRIES Both capillarity and stresses contribute to the diffusion potential (Sections 2.2.3 and 3.5.4). When diffusion potential differences exist between interfaces or between internal interfaces and surfaces, an atom flux (and its associated volume flux) will arise. These driving forces were introduced in Chapter 3 and illustrated in Fig. 3.7 (for the case of capillarityinduced surface evolution) and in Fig. 3.10 (for the case of shape changes due to capillary and applied forces). For pores within an unstressed body, the diffusion potential at a pore surface will be lower than a t nearby grain boundaries if the surface curvature is negative.' In this case, the material densifies as atoms flow from grain boundaries to the pore surfaces. Conversely, macroscopic expansion occurs if the pore surface has average positive curvature. An applied stress, as in Fig. 16.1, can reverse the situation by modifying the diffusion potential on interfaces if their inclinations are not perpendicular to the loading direction. With applied stress and capillary forces, the flux equations for crystal diffusion and surface diffusion are given by Eqs. 13.3 and 14.2. For grainboundary
L
A
t
Figure 16.1: A bundle of parallel wires bonded with grainboundary segments. An applied force per unit length of wire fapp is applied to each wire in the bundle. The system shrinks if mass is transported from the boundaries of width 2w into the pores. 'The sign of the average poresurface curvature will generally be negative if the dihedral angles are large and the number of neighboring grains is small. In two dimensionsif the poresurface average poresurface curvature will tension is equal to the grainboundary surface tensionthe be positive if there are more than six neighbors, and the pore can grow by absorbing vacancies from its abutting grain boundaries. This is equivalent to the ( N 6)rule (Eq. 15.33). If the grain boundaries have variable tensions, pore growth or shrinkage will depend on the particular abutting grain boundary energies. However, twodimensional pores with more than Ncrit = ~ T / ( T ($)) abutting grains (where ($) is the average dihedral angle (2cos' r B / ( 2 r S ) ) ) will grow on the average.
16.1: MORPHOLOGICAL EVOLUTION FOR SIMPLE GEOMETRIES
389
diffusion, the flux along a boundary under normal stress, u,,, is determined from Eqs. 2.21, 3.43, and 3.84,
As in surface diffusion (Eq. 14.6), flux accumulation during grainboundary diffusion leads to atom deposition adjacent to the grain boundary. The resulting accumulation causes the adjacent crystals to move apart at the rate’ (16.2) Three conditions are required for a complete solution to the problems illustrated in Figs. 3.10 and 16.1. If the grain boundary remains planar, d L / d t in Eq. 16.2 must be spatially uniformthe Laplacian of the normal surface stress under quasisteadystate conditions must then be constant:
V2unn= constant = A
(16.3)
Continuity of the diffusion potential at the intersection of the grain boundary and the adjoining surface requires that lbndy int
= 7 S
lbndy int
(16.4)
Finally, the total force across the boundary plane must be zero: ~ a p p =
/lndy +1 0nndA
yScos8ds
(16.5)
bndy int
The physical basis for the three terms in Eq. 16.5 is illustrated by Fig. 16.2 for the geometry indicated by Fig. 3.10.3
16.1.1 Evolution of Bamboo Wire via GrainBoundary Diffusion For this case of an isotropic polycrystalline wire loaded parallel to its axis as illustrated in Fig. 3.10b1Eqs. 16.3 and 16.4 become4
V’a,,
=
d2ann
dr2
lda,, + r dr
= A = constant
(16.6)
Solving Eqs. 16.6 subject to the symmetry condition (dann/drJr,o = 0), rT,,(T)
A
= (r2  RE)  7%
4
(16.7)
’This could be measured by observing the separation of inert markers buried in each crystal opposite one another across the boundary. 3The justification for the projected interface contribution is presented elsewhere [l41.The total force Fappis that measured by a wetting balance [5]. 4By symmetry, there is no angular dependence of unR.
390
CHAPTER 16 MORPHOLOGICAL EVOLUTION: DIFFUSIONAL CREEP, AND SlNTERlNG
Figure 16.2: Forcebalance diagram for a body with capillary forces and applied load Fapp.The plane cuts the body normal.to the applied force. There are two contributions from the body itself. One is the projection of the surface capillary force per unit length (rS)onto the normal direction and integrated over the bounding curve. The second is the normal stress onn integrated over the crosssectional areain the case of fluids bounded by a surface of uniform curvature K’, onn = ySnS [4].
The constant A is determined from the force balance in Eq. 16.5, (16.8) Using Young‘s forcebalance equation (Eq. 14.18), (16.9) at the grain boundary/surface intersection and the elongation rate (Eq. 16.2) becomes
( 16.10)
When the grain boundaries are not spaced too closely, the quantity T b a m b o o is generally negative because Rbn % 1 is less than 2J1  [yB/(2rS)I2and yB/(2yS) M 1/6 for metals. T, the capillary shrinkage force, arises from a balance between reductions of surface and grainboundary area. If Fappis adjusted so that the elongation rate goes t o zero, Fapp=  r b a m b o o , and this provides an experimental method t o determine yB/yS, and thus y” if is measured. This is known as the UdinSchalerWulff zerocreep method [6]. Scaling arguments can be used to estimate elongation behavior. Because K and 1/Rb will scale with and the grain volume, V, is constant, Eq. 16.10 implies that dL (16.11) d t cc L2 Fapp ) @ s y
+
Jm
(
16.1. MORPHOLOGICAL EVOLUTION FOR SIMPLE GEOMETRIES
391
where ?“bamboo M .irySRb is replaced by a term that depends on L alone. Elongation proceeds according to5
16.1.2
Evolution of a Bundle of Parallel Wires via GrainBoundary Diffusion
For the boundary of width 2w in Fig. 16.1, Eq. 16.4 becomes ann(Z= * W ) = 7 S K
(16.13)
where K is evaluated at the pore surface/grain boundary intersection. Solving Eq. 16.3 subject to Eq. 16.13 and the symmetry condition (da,,/dz)l,=o = 0,
a,,(x) = (x A 2 2
 w2)  7%
(16.14)
where the grainboundary center is located at x = 0. The constant A can be determined from Eq. 16.5,
 27 S KW  fapp
(16.15)
The shrinkage rate, Eq. 16.2, becomes
dL RAG* D~ A _  3R.46*DB (fapp + r w i r e s ) dt kT 2w3kT
$ rwires = 2y’(~w  sin ) 2
(16.16)
If surface diffusion or vapor transport is rapid enough, the pores will maintain their quasistatic equilibrium shape, illustrated in Fig. 16.1 in the form of four cylindrical sections of radius R.6 The dihedral angle at the four intersections with grain boundaries, $, will obey Young’s equation. $ is related to 8 by sin($/2) = cos 8. An exact expression can be calculated for the quasistatic capillary force, Ywires, as a function of the timedependent length L ( t ) . Young’s equation places a geometric constraint among L ( t ) ,the cylinder’s radius of curvature R(t),and boundary width w ( t ) ; conservation of material volume provides the second necessary equation. With Twire(L)and w ( L ) ,Eq. 16.16 can be integrated. This model could be extended to general twodimensional loads by applying different forces onto the horizontal and vertical grain boundaries in Fig. 16.1. The threedimensional case, with sections of spheres and a triaxial load, could also be derived exactly. 5An exact quasistatic [e.g., surfaces of uniform curvature (Eq. 14.29)] derivation exists for this model [4]. 6The Rayleigh instability (Section 14.1.2) of the pore channel is neglected. Pores attached to grain boundaries have increased critical Rayleigh instability wavelengths [7].
392
16.1.3
CHAPTER 16: MORPHOLOGICAL EVOLUTION: DIFFUSIONAL CREEP, AND SlNTERlNG
Evolution of Bamboo Wire by Bulk Diffusion
Morphological evolution and elongation can also occur by mass flux (and its associated volume) from the grain boundary through the bulk to the surface as illustrated in Fig. 3 . 1 0 ~ For . elongation of a crystalline material, vacancies could be created at the grain boundary and diffuse through the grain to the surface, where they would be removed. The quasisteadystate rate of elongation can be determined by solving the boundaryvalue problem described in Section 3.5.3 involving the solution to Laplace’s equation V 2 @=~0 within each grain of the idealized bamboo structure. For isotropic surfaces and grain boundaries, @ A is given by Eqs. 3.76 and 3.84. The expression for bulk mass flux is given by Eq. 13.3, and using the coordinate system shown in Fig. 3.10, symmetry requires that (16.17) If the grain boundary remains planar, the flux into the boundary must be uniform,
(%)
z=o
= C = constant
(16.18)
Laplace’s equation in cylindrical coordinates is (16.19) Assuming that the solution to Eq. 16.19 is the product of functions of z and r and using the separationofvariables method (Section 5.2.4), @A =
[c1sinh(kz)
+ cz cosh(kz)][c~J0(kr) + c4Yo(kr)]
(16.20)
where clrc2,c3,c4, and k are constants to be determined, and Jo and Yoare the zerothorder Bessel functions of the first and second kinds. Because @A(? = 0) must be bounded, c4 = 0. Introducing a new variable p ( r ,z ) that will necessarily vanish on the free surface, (16.21) The general solution to Eq. 16.19 is the superposition of the homogeneous solutions,
Jo(k,r) [b, sinh(k,z)
p ( r ,z ) =
+ c,
cosh(k,z)]
(16.22)
n
The bamboo segment can be approximated as a cylinder of average radius Re, where
nRZL =
1
L
nR2(z)d z
(16.23)
The boundary condition (Eq. 3.76) is then approximated by @A=po+
Re
or, equivalently,
p ( r = R,, z ) = o
(16.24)
16.1: MORPHOLOGICAL EVOLUTION FOR SIMPLE GEOMETRIES
393
The knR, quantities are the roots of the zerothorder Bessel function of the first kind, Jo ( k R c ) = 0 (16.25) The symmetry condition Eq. 16.17 is satisfied if b, cosh(k,l/2) 0, and therefore,
~ ( r2 ), =
C bnJo(knr)
sinh(k,z)  coth
n
+ c,
sinh(knl/2) =
(y )cosh(k,r)]
(16.26)
The planar grainboundary condition given by Eq. 16.18 is satisfied if
The coefficients, b,kn, of Jo in this Bessel function series can be determined [8]: (16.28) The constant C can be determined by substituting Eqs. 16.26 and 16.28 into the forcebalance condition (Eq. 16.5), (16.29) where
The total atom current into the boundary is I A = 27rRz J A ; therefore,
(16.31)
B z
[T
coth(k,l/2) k2R2
B M 12 for L/Rc M 2 [9]. The elongationrate expressions for grainboundary diffusion (Eq. 16.10) and bulk diffusion (Eq. 16.31) for a bamboo wire are similar except for a length scale. The approximate capillary shrinkage force 'Yapprox c y ~reduces to the exact force r b a m b o o as the segment shapes become cylindrical, Rb % R, % l/&. However, because the grainboundary diffusion elongation rate is proportional to *DB/R;f, while the bulk diffusion rate is proportional to *DXL/R2,grainboundary transport will dominate at low temperatures and small wire radii.
394
16.1.4
CHAPTER 16 MORPHOLOGICAL EVOLUTION DIFFUSIONAL CREEP, AND SlNTERlNG
Neck Growth between Two Spherical Particles via Surface Diffusion
Figure 16.3 illustrates neck growth between two particles by surface diffusion. Surface flux is driven toward the neck region by gradients in curvature. Neck growth (and particle bonding) occurs as a result of mass deposition in that region of smallest curvature. Because no mass is transported from the region between the particle centers, the two spheres maintain their spacing at 2R as the neck grows through rearrangement of surface atoms. This is surface evolution toward a uniform potential for which governing equations were derived in Section 14.1.1. However, the smallslope approximation that was used to obtain Eq. 14.10 does not apply for the spheresphere geometry. Approximate models, such as those used in the following treatment of Coblenz et al., can be used and verified experimentally [lo].
/
I
Overcut volume
Figure 16.3: (a) Model for formation of a neck between two spherical particles due to surface diffusion. (b) Approxiniation in which the surface diffusion zone within the saddleshaped neck regioii of (a) is mapped onto a riglit circular cylinder of radius 2. t is the distance parameter in the diffusion direction. Arrows parallel to the surface indicate surfacediffusion directions in hoth (a) and (11). From Coblenz et al. [lo]. Because of the proximity effect of surface diffusion, the flux from the regions adjacent to the neck leaves an undercut region in the neck ~ i c i n i t y . Diffusion ~ along the uniformly curved spherical surfaces is small because curvature gradients are small and therefore the undercut neck region fills in slowly. This undercutting . mass is conserved, the undercut volume is equal is illustrated in Fig. 1 6 . 3 ~ Because to the overcut volume. Conservation of volume provides an approximate relation between the radius of curvature, p, and the neck radius, x:
(G)
p =0.26~
1/3
(16.32)
This surfacediffusion problem can be mapped to a onedimensional problem by approximating the neck region as a cylinder of radius x as shown in Fig. 16.3b. The fluxes along the surface in the actual specimen (indicated by the arrows in ) mapped to a corresponding cylindrical surface (indicated by the Fig. 1 6 . 3 ~ are 3 . flux equation arrows in Fig. 16.3b). The zone extends between z = 1 2 ~ ~ 1 The has the same form as Eq. 14.4, so that' JS
x
*Dsys dr;
kT
dz
(16.33)
7The proxiniity effect is reflected in the strong wavelength dependence of surface smoothing (i.e., l / X 4 in Eq. 14.12). sEquation 16.33 ignores the relatively small effect of the increase in energy due to the growing grain boundary.
16 2 : DIFFUSIONAL CREEP
395
The curvature has the value 2/R at z = f2rrp/3 and approximately  l / p at z = 0 (neglecting terms of order p / R ) . The average curvature gradient 3/(2.irp2) can be inserted into Eq. 16.33 for an approximation to the total accumulation at the neck (per neck circumference),
Is
26Js
M
M
3 6 *Dsys .irkTp2
(16.34)
The corresponding neck surface area is approximately p (per neck circumference), and therefore the neck growth rate is approximately
dx dt
_
N N
36*DSySR~ .irkTp3
(16.35)
Putting Eq. 16.32 into Eq. 16.35 and integrating yields the neck growth law, (16.36) Equation 16.36 predicts that x ( t ) K t1I5 and that the neck growth rate will therefore fall off rapidly with time. The time to produce a neck size that is a given particlesize fraction is a strong function of initial particle sizeit increases as R4. Equation 16.36 agrees with the results of a numerical treatment by Nichols and Mullins [ 111
.’
16.2
DIFFUSIONAL CREEP
Mass diffusion between grain boundaries in a polycrystal can be driven by an applied shear stress. The result of the mass transfer is a hightemperature permanent (plastic) deformation called diffusional creep. If the mass flux between grain boundaries occurs via the crystalline matrix (as in Section 16.1.3), the process is called NabarroHerring creep. If the mass flux is along the grain boundaries themselves via triple and quadjunctions (as in Sections 16.1.1 and 16.1.2),the process is called Coble creep. Grain boundaries serve as both sources and sinks in polycrystalline materialsthose grain boundaries with larger normal tensile loads are sinks for atoms transported from grain boundaries under lower tensile loads and from those under compressive loads. The diffusional creep in polycrystalline microstructure is geometrically complex and difficult to analyze. Again, simple representative models are amenable to rigorous treatment and lead to an approximate treatment of creep in general.
16.2.1
Diffusional Creep of TwoDimensional Polycrystals
A representative model is a twodimensional polycrystal composed of equiaxed hexagonal grains. In a dense polycrystal, diffusion is complicated by the necessity gDifferent growthlaw exponents are obtained for other dominant transport mechanisms. Coblenz et al. present corresponding neckgrowth laws for the vapor transport, grainboundary diffusion, and crystaldiffusion mechanisms [lo].
396
CHAPTER 16 MORPHOLOGICAL EVOLUTION DIFFUSIONAL CREEP, AND SlNTERlNG
of simultaneous grainboundary slidinga thermally activated shearing process by which abutting grains slide past one anotherto maintain compatibility between the grains. In the absence of sliding, gaps or pores will develop. Sliding is confined to the grainboundary region and occurs by complex mechanisms that are not yet completely understood [12]. The need for such sliding can be demonstrated by analyzing the diffusional creep of the idealized polycrystal illustrated in Fig. 16.4[12151. The specimen is subjected to the applied tensile stress, u ,which motivates diffusion currents between the boundaries at differing inclinations and causes the specimen to elongate along the applied stress axis. Figure 16.4shows the currents associated with NabarroHerring creep. Currents along the boundaries can occur simultaneously, and if these dominate the dimensional changes, produce Coble creep. For the equiaxed microstructure in Fig. 16.4,there are only three different boundary inclinations with respect to a general loading direction; these are exhibited by the boundaries between grains A , B , and C indicated in Fig. 16.4.Mass transport between these boundaries will cause displacement of the centers of their adjoining grains. The normal displacements are indicated by L A ,L B , and Lc in Fig. 16.4and the shear displacements by S A , S B , and Sc. These combined graincenter displacements produce an equivalent net shape change of the polycrystal. Compatibility relationships between the displacements must exist if the grain boundaries remain intact. Along the 1 axis, the displacement of grain C relative to grain B must be consistent with the difference between the displacement of grain C with respect to grain A and with that of grain B with respect to grain A . This requirement is met if
LA
+ LB

2LC = v5sA d
3sB
(16.37)
Similarly, along the 2 axis,
( 16.38) Also, the volume must remain constant. Therefore, El1
+
E22
=0
(16.39)
2
t
Figure 16.4: Twodimensional polycrystal consisting of identical hexagonal grains subjected to uniaxial applied stress, g ,giving rise to an axial strain rate t . From Beer6 [14].
16.2:DIFFUSIONAL CREEP
397
where ~ 1 and 1 ~ 2 2 are the normal strains of the overall network connecting the centers of the grains in the (1,2) coordinate system in Fig. 16.4. These strains are related to the displacements through ~ 1 = 1 dul/dzl,~ 2 = 2 duz/dzz, and ~ 1 = 2 (1/2)(dul/dz2 $duz/dzl), where the ui are the displacements produced throughout the network of grain centers. For the representative unit cell PQRS in Fig. 16.4, El1
=
AC1 AB1 d (16.40)
where d is the width of a hexagonal grain, and ABi and ACi are the components of the displacements of the centers of the grains B and C relative to A and are given bY 2AB1=  LB 2AB2 =  S B & L B (16.41) 2ac1= &sA L~ 2AC2 = S A & L A
asB + + +
Therefore. El1
=
8(SB  SA) 2d
LA + LB k
2d
(16.42)
Substituting Eqs. 16.42 into Eq. 16.39 yields (16.43) Combining Eqs. 16.38, 16.37, and 16.43,
(16.44)
and
L~ + L~
+ L~ = o
(16.45)
which is equivalent to the constantvolume condition. To show that boundary sliding must participate in the diffusional creep to maintain compatibility, suppose that all of the S A ,S B ,and Scsliding displacements are zero. Equations 16.44 require that the L A ,L B , and Lc must also vanish. Therefore, nonzero Si 's (sliding) are required to produce nonzero graincenter normal displacements.
398
CHAPTER 16 MORPHOLOGICAL EVOLUTION DIFFUSIONAL CREEP AND SlNTERlNG
This result can be demonstrated similarly by solving for the strain, E , along the applied tensile stress axis shown in Fig. 16.4 in terms of only the Lz’s or only the 9’s: E = cos2 e E l l sin2 e~~~ 2 sin e cos e~~~ (16.46)
+
+
or, using Eq. 16.4016.44, d
( L +~L ~ ) (I2cos2e) +
1 SASB
LA  LB
v5
1
2 sin 8 cos 0
(16.47)
 SB 2 sin 0 cos 0] e) + 2sc  SA 3
(16.48) d v 5 Equation 16.47 indicates that the creep strain may be regarded as diffusional transport accommodated by boundary sliding, and Eq. 16.48 indicates that it may equally well be regarded as boundary sliding accommodated by diffusional transport.l0 The creep rate, t , can be obtained by taking time derivatives of E in Eqs. 16.47 and 16.48. The applied tensile stress, 0,shown in Fig. 16.4 will generate stresses throughout the polycrystal, and each boundary segment will, in general, be subjected to a shear stress (parallel to the boundary) and a normal stress (perpendicular to the boundary). The shear stresses will promote the grainboundary sliding displacements, S A , S B , and Sc, while the normal stresses will promote the diffusion currents responsible for the L A , L B , and Lc displacements. A detailed analysis of the shear and normal stresses at the various boundary segments is available (see also Exercise 16.2) [12141. & =  [
16.2.2
(1  2 C O S ~
Diffusional Creep of ThreeDimensional Polycrystals
The analysis can be extended to a threedimensional polycrystal with an equiaxed grain microstructure. As in twodimensional creep, grainboundary sliding must accompany the diffusional creep, and because these processes are interdependent, either sliding or diffusion may be rate limiting. In most observed cases, the rate is controlled by the diffusional transport [14, 15, 18, 191. Exact solutions for corresponding tensile strain rates are unknown, but approximate expressions for the Coble and NabarroHerring creep rates under diffusioncontrolled conditions where the boundaries act as perfect sources may be obtained from the solutions for the bamboostructured wire in Section 16.1.1. The equiaxed polycrystal can be approximated as an array of bonded bamboostructured wires with their lengths running parallel to the stress axis and with the lengths of their grains (designated by L in Fig. 3.10) equal to the wire diameter, 2R. This produces a polycrystal with an approximate equiaxed grain size d = L = 2R. The Coble and NabarroHerring creep rates of this structure can be approximated by those given for the creep rates of the bamboostructured wire by Eqs. 16.10 and 16.31 with L = 2R = d and the sintering potential set to zero. In this approximation, the effects of internal normal stresses generated along the vertical boundaries (between the bonded wires) may be neglected because these stresses are zero on average. Using this approximation, for diffusioncontrolled Coble creep, (16.49) ‘OThis duality has been recognized (e.g., Landau and Lifshitz [16] and Raj and Ashby [17]).
16.2:DIFFUSIONAL CREEP
399
with A1 = 32, and for diffusioncontrolled NabarroHerring creep,
(16.50) with A2 = 12." Because the Coble creep rate is proportional to *DB/d3and the , creep will be favored as the temperature NabarroHerring rate to * D X L / d 2Coble and grain size are reduced. Figure 16.5 shows a deformation map for polycrystalline Ag possessing a grain size of 32 pm strained at a rate of 108s1 [20]. Each region delineated on the map indicates a region of applied stress and temperature where a particular kinetic mechanism dominates. Experimental data and approximate models are used t o produce such deformation maps. The mechanisms include elastic deformation a t low temperatures and low stresses, dislocation glide a t relatively high stresses, dislocation creep at somewhat lower stresses and high temperatures, and NabarroHerring and Coble diffusional creep at high temperatures and low stresses. Coble creep supplants NabarroHerring creep as the temperature is reduced. An analysis of diffusional creep when the boundaries do not act as perfect sources and sinks has been given by Arzt et al. [19] and is explored in Exercise 16.1. The creep rate when boundary sliding is ratelimiting has been treated and discussed by Beer6 [13, 141. If a viscous constitutive relation is used for grainboundary sliding (i.e., the sliding rate is proportional to the shear stress across the boundary), the macroscopic creep rate is proportional to the applied stress, and the bulk polycrystalline specimen behaves as a viscous material. An analysis of the slidingcontrolled creep rate of the idealized model in Fig. 16.4 is taken up in Exercise 16.2. Variable boundary behavior complicates the results derived from the uniform equiaxed model presented above. Nonuniform boundary sliding rates may cause
*9
5
3
0.0
2.0.
Theoretical shear stress Dislocationglide Dislocationcreep .
4.0Elastic
6.08.0
cases by factors a s la r g e as three. See Ashby [20], Burton [18],Arzt et al. [19], and Pilling and Ridley [15].
400
CHAPTER 16: MORPHOLOGICAL EVOLUTION: DIFFUSIONAL CREEP, A N D SlNTERlNG
individual grains to rotate. Also, grainboundary migration and the formation of new grains by recrystallization will affect both microstructure and creep rate.12 Finally, mechanisms besides diffusional transport of mass between internal interfaces can contribute to diffusional creep. For instance, single crystals containing dislocations exhibit limited creep if the dislocations act as sources and sinks, depending on their orientation with respect to an applied stress (see Exercise 16.3). 16.3
SlNTERlNG
Sintering is a kinetic process that converts a compacted particle mass (or powder) or fragile porous body into one with more structural integrity. Increased mechanical integrity stems from both neck growth (due to mass transport that increases the particle/particle “necks”) and densification (due to mass transport that reduces porosity). The fundamental sintering driving forcecapillarityderives from reduction of total surface energy and is often augmented by applied pressure. The kinetic transport mechanisms that permit sintering are solidstate processes, and therefore sintering is an important forming process that does not require melting. Materials with high melting temperatures, such as ceramics, can be molded into a complex shape from a powder and subsequently sintered into a solid body.I3 16.3.1
Sintering Mechanisms
Neck growth can occur by any mass transport mechanism. However, processes that permit shrinkage by pore removal must transport mass from the interior of the particles to the pore surfacesthese mechanisms include grainboundary diffusion, volume diffusion, and viscous flow. Other mechanisms simply rearrange volume at the pore surfaces and contribute to particle/particle neck growth without reduction in porosity and shrinkaget hese mechanisms include surface diffusion and vapor transport. Particle compacts and porous bodies have complex geometries, but models for sintering and shrinkage can be developed for simpler geometries such as the one captured in Fig. 16.6.14 These models can be used to infer behaviors of
TimeFigure 16.6: h’Iodel sint,rririg cxpcriiricrit drrrioristratirig neck growth during sint,ering by viscous flow of iiiitially splierical 3 imri diameter glass beads at 1000°C over 30 iriiiiutes. Courtesy of HansEckart Exner.
I2These phenomena, and their effects on the creep rate, are described in more detail by Sutton and Balluffi [12], Beer6 [13, 141; and Pilling and Ridley [15]. 13General reviews of sintering appear in introductory ceramics texts [21, 221, and a more complete exposition is given in German’s book on sintering [23]. 14Further details about such models can be found in Reviews in Powder Metallurgy and Physical Ceramics or in Physical Metallurgy [24, 251.
163 SlNTERlNG
401
complex systems of which these simpler geometries are component parts. Figure 16.7 summarizes the atomtransport paths that can contribute to neck growth and also, in some cases, densification. If the particles are crystalline, a grain boundary will generally form at the contact region (the neck). A dihedral angle y will form at the neck/surface junction, and for the isotropic case, conform to Young’s equation, y B = 27’ cos($/2). The seven different transport paths in Fig. 16.7 are listed in Table 16.1 with their kinetic mechanisms. Atoms generally flow to the neck region, where the surface has a large negative principal curvature and therefore a low diffusion potential compared to neighboring regions. Densification will accompany neck growth if the centers of the abutting spheres move toward one another. For example. with mechanism BS.B, atoms are removed from the boundary region causing such motion. The dominant mechanism and transport pathor combinations thereofdepend upon material properties such as the diffusivity spectrum, surface tension, temperature, chemistry, and atmosphere. The dominant mechanism may also change as the microstructure evolves from one sintering stage to another. Sintering maps that indicate dominant kinetic mechanisms for different microstructural scales and environmental conditions are discussed in Section 16.3.5.
Figure 16.7: (a) Sintering of two abutting singlecrystal spherical particles of differing crystal orientations. A grain boundary has formed across the neck region. (b) Detail of neck perimeter. Seven possible sintering mechanisms for the growth of the neck are illustrated (see the text and Table 16.1).
16.3.2
Sintering Microstructures
Powder compressed into a desired shape at room temperature provides an initial microstructure for a typical sintering process. Such a microstructure may be composed of equiaxed particles or the particles may vary in size and shape. Particle packing may be regular and nearly ‘krystalline,” highly irregular, or mixtures of both. Sintering microstructures are generally complex, but some aspects of their microstructural evolution can be understood by investigating primary process models such as those described in Section 16.1 and the simple neckgrowth models presented in Section 16.1.4. However, some microstructural evolution processes are not easily captured by simple models. Additional modeling difficulties arise for irregular packings, variability in particle size and shape, and inhomogeneous chemistry.
402
CHAPTER 16. MORPHOLOGICAL EVOLUTION. DIFFUSIONAL CREEP, AND SlNTERlNG
Mass Transport Mechanisms for Sintering
Table 16.1:
Mechanism
Source
Sink
Transport Mechanism
Densifying or Nondensifying
SS.XL Surface Surface Crystal diffusion Nondensifying Atoms diffuse through the crystal from largercurvature surface regions to lowercurvature regions. BS.XL Boundary Surface Crystal diffusion Densifying Atoms diffuse through the crystal from the grain boundary to lowcurvature surface regions. ~~
~
BS.B Boundary Surface Boundary diffusion Densifying Atoms diffuse along the boundary to the surface; subsequently, they are transported along the surface by one or more of the SS.XL, SS.S, or SS.V paths. DS.XL Dislocation Surface Crystal diffusion Either Atoms diffuse through the crystal from climbing dislocations. Equivalently, vacancies diffuse from the surface.
ss.s
~~~~~
~~
Surface Surface Surface diffusion Nondensifying Atoms diffuse along the surface from largercurvature surface regions to lowercurvature surface regions.
ss.v
Surface Surface Vapor transport Nondensifying Atoms are transported through the vapor phase from largercurvature surface regions to lowercurvature surface regions.
VF Viscous flow Either Atoms are transported by viscous flow by differences in the capillary pressure at nonuniformly curved surfaces.
Nevertheless, there are parallel stages in any powder sintering process that can be used to catalog behavior. Each powder sintering process begins with particle/particle neck formation and a porous phase between the weakly attached particles. As these necks grow, the particle/pore interface becomes more uniformly curved but remains interconnected throughout the compact. Before the porous phase is removed, it becomes disconnected and isolated at pockets where four grain boundaries intersect. Initial, Intermediate, and Final Stages of Powder Sintering. Following Coble’s pioneering work, the microstructural evolution of a densifying compact is separated into an initial stage, an intermediate stage, and a final stage of sintering [26]. Figure 16.8 illustrates some of the microstructural features of each stage. The initial stage comprises neck growth along the grain boundary between abutting particles. The intermediate stage occurs during the period when the necks between the particles are no longer small compared to the particle radii and the porosity is mainly in the form of tubular pores along the threegrain junctions in the compact. The geometries of both the initial and intermediate stages therefore have intergranular porosity percolating through the compact.
16.3 SlNTERlNG
Initial powder compact
Initial stage of sintering
Intermediate stage of sintering
Final stage of sintering
403
Dense polycrystalline compact
Figure 16.8: Stages of powder sinterin . Initial stage involves neck growth. Intermediate state is marked by continuous porosity j o n g threegrain junctions. Final stage involves removal of isolated pores at fourgrain junctions. Figure calculated using SurfaceEvolver [27]; figure concept by Coble [26]. Courtesy of Ellen J. Siem.
The transition from the intermediate to the final stage occurs when the interconnected tubular porosity along the grain junctions (edges) breaks up because of the Rayleigh instability (see Section 14.1.2) and leaves isolated pores of equiaxed shape at the grain corners [7]. The final stage occurs when the porosity is isolated and located at multiplegrain junctions. Final pore elimination occurs by mass transfer from the grain boundaries to the pores attached to the grain boundaries. similar to the transport in the wirebundle model treated in Section 16.1.2. If grain growth occurs during any stage, the pores may break away from the grain boundaries. In such cases, the pores will be isolated from the grain boundaries in the final stage. and further densification will be limited by the rate of crystal diffusion of atoms from dislocation sources by the mechanism DS.XL illustrated in Fig. 16.7. Failure to reach full density is often caused by such pore breakaway. 16.3.3
Model Sintering Experiments
Experiments have been designed to reveal details of the sintering mechanisms indicated by Fig. 16.7 and the sintering stages illustrated by Fig. 16.8. Such sintering experiments include spheresphere model experiments similar to that depicted in Fig. 16.6 [28],sintering of rows of spheres [29],sintering of spheres and wires to flat plates [30],and sintering of bundles of wires such as that depicted in Fig. 16.9 [31]. With their simple geometry, these model experiments reveal fundamental processes during the various stages of sintering. Initialstage processes are illuminated by the spheresphere experiments, and transitions between the intermediate and final stages are captured in the wirebundle experiments. Figure 16.9d, in particular, demonstrates the important role of grainboundary attachment for pore removalessentially all of the grainboundary segments trapped between the pores have broken free and left the specimen. However, one boundary remains and continues to feed atoms to the pores to which it is connected. 16.3.4
Scaling Laws for Sintering
Because the surface energy per volume is larger for small particles and because the fundamental driving force for sintering is surfaceenergy reduction, compacts composed of smaller powders will typically sinter more rapidly. Smaller powders are more difficult to produce and handle; therefore, predictions of sintering rate dependence on size are used to make choices of initial particle size. Herring’s
404
CHAPTER 16 MORPHOLOGICAL EVOLUTION DIFFUSIONAL CREEP, AND SINTERING
(c)
Figure 16.9: Cross section of bundle of parallel 128 p n diameter Cu wires after sintering at 900°C: (a) 50 11. (b) 100 h, (c) 300 h; and at 1075°C: (d) 408 h. From Alexander and Balluffi [31]
scaling laws provide a straightforward method to predict sintering rate dependence on length scale [32]. Suppose that two sintering systems, S and B . are identical in all aspects except their size.15 Each length dimension of system B is X times as large as the corresponding dimension of system S . Under identical conditions and provided that the same sintering mechanism is operative. the ratio of sintering rates can be determined from the relative sizes of the specimens. In general, a sintering rate is proportional t o the masstransport current, I , due t o sintering driving forces and is inversely proportional t o the transported material volume, AV. required t o produce a given shape change (e.g., the volume associated with neck growth). The current I is the vector product of the atoniic flux :and the area through which the current flows during sintering. Therefore, the rates at which bodies S and B undergo geometrically similar changes will be in the ratio
A’
rateB =rates
I B AVs AVB I S
(16.51)
The current, I , is proportional t o the diffusion potential gradient, V@*and to the crosssectional area. through which this flux flows. Therefore,
A,
(16.52)
A’
Suppose that the plane is the bisector between the source of atoms and their sink (i.e.. the sources and sinks listed in Table 16.1). The component of diffusion I5The systems may be similar powder compacts of the same powder material but differing particle sizes, or they may be model systems such as those illustrated in Figs. 16.6 arid 16.9 but with all corresponding length dimensions scaled similarly.
163 SlNTERlNG
405
potential gradient normal to the plane A’ (the component projected onto the normal A of is proportional to the difference in diffusion potential between the source and the sink, A@, divided by the distance A1 between the source and sink. Therefore,
A)
(16.53)
Combining these relationships with Eq. 16.51, rate’ rates

A@’ Als AB AVs A@s A ~ B As AV’
(16.54)
For free sintering, the diffusion potential is proportional to curvature; A@’/A@s will scale as 1/X. The ratio Als/AlB also scales as 1/X. For surface diffusion, one of the crosssectional area’s dimensions is 6, the thickness of the highdiffusivity surface layer, independent of system size. The remaining crosssectional area length scales as A, and therefore A B / A s must scale as A. AVSIAVB scales as l / X 3 . Therefore, substituting into Eq. 16.54, rateB 1 1 1   x  x X x = X X A3 rates

(surface diffusion)
(16.55)
If sintering occurs by diffusion through the bulk crystal (mechanism BS.XL), all the ratios will be the same as for surface diffusion except for the crosssectional which , will scale as X2. Therefore, area A B / A ~ rateB 1 1 1   x  x X2 x  = rates X X X3

(crystal diffusion)
(16.56)
If sintering occurs by grainboundary diffusion, the ratio of rates will be the same as for the surfacediffusion case, A X’ scaling law can be derived for viscous flow and a law applies for vapor transport [32]. To show that the rate of twoparticle neck growth by surface diffusion in Section 16.1.4 is consistent with the XP4 scaling law, Eq. 16.36 can be written in terms of its fundamental length scales and differentiated: 1 dx x dt
R x5
0;
(16.57)
Therefore,
A similar result may be obtained (Exercise 16.6) using the result derived in Eq. 16.16 for the neck growth for a bundle of parallel wires by grainboundary diffusion. 16.3.5
Sintering Mechanisms Maps
Any of the various mechanisms for sintering identified in Table 16.1 may contribute to the sintering rate. Which of the mechanisms contributes most to sintering depends on, among other things, particle size and temperature. Sometimes certain
406
CHAPTER 16: MORPHOLOGICAL EVOLUTION: DIFFUSIONAL CREEP, AND SlNTERlNG
mechanisms can be ruled out immediately. For example, viscous flow (VF) cannot contribute for crystalline materials, and the nondensifying mechanisms (e.g., SS.S and SS.V) cannot contribute to pore removal in the final stages of sintering. Processing decisions depend on the particular mechanism, or combination of mechanisms, that contribute to sintering. Sintering maps such as Fig. 16.10 provide information for such decisions. These plots can be created by employing approximate models for the sintering rates for specific systems by the various mechanisms. These models, combined with experimental data, can be used to plot regimes for which a particular mechanism makes the largest contribution to the sintering rate [33]. Sintering maps for different systems vary considerablyeven for the same material, but having different initial particle sizes. For example, a map corresponding to Fig. 16.10 for silver particles of a smaller radius (i.e., 10 pm) shows a considerably reduced field for the BSsXL mechanism. On the other hand, a map for 10 pm UOZ particles shows a vaportransport (SSsV) regime [33]. Scaling laws are limited to regions of the sintering map where the dominant mechanism is unchanged (Section 16.3.4). Although sintering mechanism maps are no better than the models and data used to construct them, they provide useful insights. Temperature (“C) 400
500 600 700 800
900
Full density reached
0.50
0.60
0.70
0.80
0.90
1.0
Homologous temperature, T/T, Fi ure 16.10: Sintering mechanism map for silver powder of radius 100 p,m plotted w i k coordinates of reduced temperature and neck radius. The assumed conditions are that grain boundaries remain between abutting particles and that no trapped gases are to impede isolated pore shrinkage. Each region represents the regime where the ni%%: mechanism is dominant (see Table 16.1). The dashed line indicates transitions between initialstage and intermediate and finalstage sinterine. Although all possible mechanisms were considered, the three shown were dominant in their respective regimes. From Ashby [33].
Bibliography R.B. Heady and J.W. Cahn. An analysis of capillary force in liquidphase sintering of spherical particles. Metall. Trans., 1(1):185189, 1970. J.W. Cahn and R.B. Heady. Analysis of capillary force in liquidphase sintering of jagged particles. J. Am. Cerum. SOC.,53(7):406409, 1970.
W.C. Carter. The forces and behavior of fluids constrained by solids. Actu Metall., 36(8):22832292, 1988.
16.3:SlNTERlNG
407
4. R.M. Cannon and W.C. Carter. Interplay of sintering microstructures, driving forces, and mass transport mechanisms. J . Am. Ceram. SOC.,72(8):15501555, 1989. 5. F. M. Orr, L. W. Scrivin, and T. Y. Chu. Mensici around plates and pins dipped in liquidinterpretation of Wilhemy plate and solderability measurements. J . Colloid Interf. Sci., 60:402405, 1977. 6. H. Udin, A. J. Shaler, and.J. Wulff. The surface tension of copper. Trans. AIME, 186:186190, 1949. 7. W.C. Carter and A.M. Glaeser. The morphological stability of continuous intergranular phasesthermodynamics considerations. Am. Ceram. SOC.Bull., 63(8):993993, 1984.
8. F.B. Hildebrand. Advanced Calculus for Engineers. PrenticeHall, Englewood Cliffs, NJ, 2nd edition, 1976. 9. C. Herring. Diffusional viscosity of a polycrystalline solid. J. Appl. Phys., 21:437445, 1950. 10. W.S. Coblenz, J.M. Dynys, R.M. Cannon, and R.L. Coble. Initial stage solidstate sintering models: A critical analysis and assessment. In G. C. Kuczynski, editor, Proceedings of the Fijlh International Conference on Sintering and Related Phenomena, pages 141157, New York, 1980. Plenum Press. 11. F.A. Nichols and W.W. Mullins. Surface (interface) and volumediffusion contributions to morphological changes driven by capillarity. Trans. AIME,233( 10):18401847, 1965.
12. A.P. Sutton and R.W. Balluffi. Interfaces in Crystalline Materials. Oxford University Press, Oxford, 1996. 13. W. Beer& Stress redistribution during NabarroHerring and superplastic creep. Metal Sci., 10(4):133139, 1976. 14. W. Beer& Stresses and deformation at grain boundaries. Phil. Trans. Roy. SOC. London A , 288(1350):177196, 1978. 15. 3. Pilling and N. Ridley. Superplasticity in Crystalline Solids. Institute of Metals, London, 1989. 16. L.D. Landau and E.M. Lifshitz. Statistical Physics. Pergamon Press, New York, 1963. 17. R. Raj and M.F. Ashby. On grain boundary sliding and diffusional creep. Metall. Trans., 2: 11131 127, 1971. 18. B. Burton. Diffusional Creep of Polycrystalline Materials. Diffusion and Defect Monograph Series, No. 5. Trans Tech Publications, Bay Village, OH, 1977. 19. E. Arzt, M.F. Ashby, and R.A. Verrall. Interface controlled diffusional creep. Acta Metall., 31(12):19771989, 1983. 20. M.F. Ashby. A first report on deformation mechanism maps. Acta Metall., 20(7):887897, 1972. 21. Y.M. Chiang, D. Birnie, and W.D. Kingery. Physical Ceramics. John Wjley & Sons, New York, 1996. 22. W.D. Kingery, H.K. Bowen, and D.R. Uhlmann. Introduction to Ceramics. John Wiley & Sons, New York, 1976. 23. R.M. German. Sintering Theory and Practice. John Wiley & Sons, New York, 1996. 24. H.E. Exner. Principles of single phase sintering. Reviews on Powder Metallurgy and Physical Ceramics, 1:l237, 1979. 25. R.W. Cahn. Recovery and recrystallization. In R.W. Cahn and P. Haasen, editors, Physical Metallurgy, pages 15951671. NorthHolland, Amsterdam, 1983.
408
CHAPTER 16: MORPHOLOGICAL EVOLUTION: DIFFUSIONAL CREEP, AND SlNTERlNG
26. R.L. Coble. Sintering crystalline solids I. Intermediate and final state diffusion models. J . Appl. Phys., 32(5):787, 1961. 27. K. A. Brakke. The Surface Evolver. Exp.Math., 1(2):141165, 1992. Publicly available software. 28. W. Zhang, P. Sachenko, J.H. Schneibel, and I. Gladwell. Coalescence of two particles with different sizes by surface diffusion. Phil. Mag. A , 82(16):29953011, 2002. 29. W.D. Kingery and M. Berg. Study of the initial stages of sintering solids by viscouus flow, evaporationcondensation, and selfdiffusion. J . Appl. Phys., 26( 10):12051212, 1955. 30. G.C. Kuczynski. Theory of solid state sintering. In W. Leszynski, editor, Powder Metallurgy, pages 1130, New York, 1961. Interscience Publishers. 31. B.H. Alexander and R.W. Balluffi. Mechanism of sintering of copper. Acta Metall., 5(11):666677, 1957. 32. C. Herring. Effect of change of scale on sintering phenomena. J . A p p l . Phys., 21:301303, 1950. 33. M.F. Ashby. A first report on sintering diagrams. Acta Metall., 22(3):275289, 1974.
EXERCISES 16.1 An analysis of the rate of elongation of a wire possessing a bambootype grain structure is given in Section 16.1.3. An essential aspect of the analysis is the assumption that the stressinduced atomic transport producing the elongation is diffusionlimited. Now, construct the main framework of a model for the same system in which the atomic transport is sourcelimited, as indicated below, and explain how the model works. 0
0
0
Assume that the grain boundaries are much poorer sources than the wire surface and that it is the poor source action of the boundaries that causes the process to be sourcelimited. Use the simple rateconstant type of formulation employed in Sections 13.4.2 and 15.1.1 to analyze sourcelimited precipitate growth and particle coarsening, respectively. Assume, as in Section 16.1.1, that the diffusion occurs via vacancies and that the ratelimiting process is the rate of creation and destruction of vacancies at the grain boundaries.
Solution. When the process is diffusionlimited and the rateconstant formalism is used, the net rate a t which vacancies are destroyed a t a boundary (i.e,, the rate of destruction minus the rate of creation) is
IB
=2
lR lL
K B [c;(r) 
C E . ~ ~ (27rr ~ ) dr]
(16.59)
The corresponding rate at the free surface o f the cell, which is of length L , is
Is =
K S [c;  c $ ~ 27rRd.z ~ ]
(16.60)
EXERCISES
409
cF,~~
I B is negative, since > c; and vacancies are being created, whereas I s is positive, since c$ > c $ and ~ ~vacancies are being destroyed. The crystal diffusive current at each interface is equal t o the net destruction rate, and therefore
,I& = I B and Iiff= I s
(16.61)
In addition, in the quasisteady state, B I B = Idiff = I
and the elongation rate,
S
S = Idiff
(16.62)
1,is given by (16.63)
The diffusion within the grains is relatively slow, so that I& = IB and I& = I s are small compared t o the vacancy creation and destruction rates in the equations above. Therefore, c; 2 and c$ E cZeq and the rate is diffusionlimited,
~ t ' ~ ~
When the rate is sourcelimited, the vacancy diffusion rate within the grains is relatively large. K B << K S and the relatively slow source action a t the boundary has a negligible efFect on the vacancy gradients within the grains. The vacancy concentration is then maintained everywhere at an essentially constant level corresponding t o cZeq as a result of the relatively f a s t source action a t the wire surface. I B is then given by Eq. 16.59 with c; E cZeq. Because the stress and the concentration cFSeqare uniform over the boundary, the elongation rate is
(16.64) The equilibrium vacancy concentration is given, in general, by Eq. 3.65, which for present purposes may be written in the form
(16.65) where Gfv(m) is the work required t o form a vacancy a t a flat stressfree surface and AGf, is any additional work. The wire volume is increased when a vacancy is formed, and in the present model AGG is negative when a vacancy is formed a t the grain boundary because of the work done by the applied tensile stress during i t s formation. O n the other hand, AGf, is positive a t the wire surface because of the work that must be done t o increase the surface area. Therefore, > c ? and ~ ~ d L / d t is positive.
cF'~~
16.2 Consider the diffusional creep of the idealized twodimensional polycrystal illustrated in Fig. 16.4 and discussed in Section 16.2. Each boundary will be subjected to a normal stress, on,and a shear stress, us, as illustrated in Fig. 16.11. Suppose that all boundaries shear relatively slowly at a rate corresponding to dS_  K a , (16.66) dt where K is a boundary shear rate constant, whereas diffusional transport between the different boundary segments is extremely rapid. The creep will then proceed at a rate controlled by the rate of the grainboundary sliding and not by diffusional transport through the grains or along the grain boundaries. Using the results in Section 16.2, find an expression for the slidinglimited creep rate of the specimen illustrated in Figs. 16.4 and 16.11.
410
CHAPTER 16 MORPHOLOGICAL EVOLUTION DIFFUSIONAL CREEP, AND SlNTERlNG
Figure 16.11: Normal stresses and shear stresses present in twodimensional polycrystal subjected to uniaxial applied stress, 0 . The geometry is the same as in Fig. 16.4.
Determine the shear stresses acting on the three types of boundary segments present. When diffusion is extremely rapid, all differences in the diffusion potential will be eliminated, and all three normal stresses at the three different types of boundary segments will be uniform along each segment and equal to one another. Therefore, onA
= f‘n B =
onC
= cn
(16.67)
=0
(16.68)
Also, if each grain is not to rotate, 0,”
+ u,” +a:
Since the stresses in each grain are the same, the normal and shear stresses along planes PQ and RS can be found from the forces exerted on them by the applied stress, u , with the results uf = s i n e c o s e a
” e
u,” = sin2 cr
4
cos2 e +  sinecose 21
c r t = [Icos2e+ 3 sinecose+ fl
2
“ I 1
+sin2 e 4 sin20 1 4
u
( 16.69)
u
Next, each triangular shaded region in Fig. 16.11 must be in mechanical equilibrium (i.e., the sum of the forces on it parallel and normal to PQ, or R S , must be zero). This leads to the conditions 0 =  2&u,”  u,B +2&u,
+u,”
0 =2u,D +u,B +a,”
o=
(16.70)
2u,E+u,”+a~
0 = 2&,”
+ u,”  2&an
c  us
These linear equations are sufficient to allow the determination of the shear stress acting on each boundary segment.
EXERCISES
411
Solution. Expressions for the shear stresses at the three types o f boundary segments may be obtained by the simultaneous solution of the equations given above for the boundary stresses. The results are
a: =
[ Acos20 sinOcose
UF = 2 s i n e c o s ~ a

“I
2
u
(16.71)
The expression for the creep rate due t o boundary sliding is obtained by differentiating Eq. 16.48,
Substituting Eqs. 16.66 and 16.71 into Eq. 16.72 then produces the surprisingly simple result
.
K
E=u
d
(16.73)
The creep rate is therefore proportional t o the applied stress, and the polycrystal acts effectively as an ideally viscous material.
16.3 Diffusional creep can also occur by means of the stressmotivated transport of atoms between climbing dislocations in a material. This is illustrated in a highly idealized manner in Fig. 16.12, where a regular array of edge dislocations possessing four different Burgers vectors is present in a stressed material. The net Burgers vector content is zero. The stress exerts climb forces on the dislocations so that dislocations with Burgers vectors lying along &x and &g directions act alternately as sources and sinks. The arrows indicate the atomic fluxes associated with the climb. Each source dislocation is surrounded by four nearestneighbor sink dislocations, and vice versa for the sink disloca
Y
t
f
U
Figure 16.12: Idealized array of edge dislocations subjected to applied stress, u . Arrows show stressinduced diffusion current around each climbing dislocation.
412
CHAPTER 16: MORPHOLOGICAL EVOLUTION: DIFFUSIONAL CREEP, AND SlNTERlNG
tions. The climb of the dislocations in this arrangement adds atomic planes lying perpendicular to x and removes an equal number of planes lying perpendicular to y , causing the specimen to lengthen and shorten in the direction of the applied stresses. Find an expression for the instantaneous quasisteadystate creep rate of this idealized structure, assuming that the dislocations act as perfect sources or sinks. Surround each dislocation by a cylindrical cell in which the diffusion to/from the dislocation is assumed to be cylindrical (see Fig. 16.12), and use a meanfield approximation similar to the one used in the analysis of particle coarsening. Solution. The flux equation is given by Eq. 13.3, and the diffusion equation in the quasisteady state is V 2 @= ~ 0. The derivation o f Eq. 13.4 shows that the climb force exerted on the sink dislocations will cause the value o f @ A at their core radii, R,,t o have the value (16.74) @:(sinks) = p i  u i2 while at the source dislocations, @:(sources)
=p i
+uR
(16.75)
A t the surface of the cell at r = L/2, we use the meanfield boundary value @A
(g)
=b i
(16.76)
The general solution of the diffusion equation in cylindrical coordinates is @ A = a1 l n r + a z , and using the boundary conditions above t o determine the constants a1 and a2, (16.77) Using the flux equation, the diffusion current into a dislocation (per unit length) is
I = kt27rrJ~= =k
27r *Du f k T ln[L/(2Ro)]
(16.78)
and after taking account o f the density of dislocations, the creep rate along z is
.
IR 2LZ
E==
7r *DR f k T L zln[L/(2Ro)]
(16.79)
The creep rate is therefore proportional t o the stress and also closely proportional t o the dislocation density (i.e., L  2 ) .
16.4 A thinwalled puremetal pipe of inner radius R'" and outer radius Rout is
heated.
(a) Find an expression for the quasisteadystate rate at which it will shrink. Assume that the surfaces act as perfect sources for atoms and that the interior is free of internal sources. (b) An inert insoluble gas is introduced in the pipe at a pressure P . Find the value of P that will stop the pipe from shrinking. The external pressure is small enough so that it may be ignored.
EXERCISES
413
Solution. (a) In the quasisteadystate Laplace equation, V 2 @ ( r = ) 0 holds for the diffusion potential and Eq. 13.3 holds for the diffusion flux. The boundary conditions on @ a t the surfaces are
(16.80)
Using the solution o f the Laplace equation for diffusion in cylindrical coordinates given by Eq. 5.10, fitting it t o the boundary conditions given by Eq. 16.80, and employing Eq. 13.3 for the flux, the total diffusion current of atoms (per unit pipe length) passing radially from R'" t o Routis
I=
27r*D(@'"R k T f In(Rout/Rin) @Out)
(16.81)
which may be compared with Eq. 5.13. Now,
dRout  dt
RI 27rRoUt

(16.82)
+
and for the thinwalled pipe, 1n(Rout/Rin) = ln(1 AR/Rin)x AR/(R), where AR = Rout  Rin and Rout Rin x (R). Using these results and Eq. 16.81,
(16.83) (b) The internal pressure causes the diffusion potential at R'" t o be RyS/Rin R P . Equation 16.81 then becomes
+
I=
27r*D(P  2ys/(R)) 27r*D(ain @Out) R k T f ln(Rout/Rin) kTf ln(Rout/Rin)
@"
= po 
(16.84)
and shrinkage will stop when P = 2yS/(R).
16.5 Suppose that a body made up of fine particles can sinter by either the crystal diffusion mechanism BS . XL or the grainboundary diffusion mechanism BS . B as illustrated in Fig. 16.7. How will the relative sintering rates due to these two mechanisms vary as: (a) The particle size is decreased?
(b) The temperature is decreased? Solution. (a) Let Ratio =
sintering rate due t o grainboundary diffusion sintering rate due t o crystal diffusion
The sintering rate due t o boundary diffusion and crystal diffusion will be proportional t o *DB and *DxL, respectively. The scaling laws show that the sintering rate due t o boundary diffusion will decrease by the factor A4 when the particle size is increased by the factor A. The corresponding factor for sintering by crystal
414
CHAPTER 16 MORPHOLOGICAL EVOLUTION DIFFUSIONAL CREEP, AND SlNTERlNG
difFusion is X3.Therefore,
(16.85) Sintering by boundary diffusion will become more important as the particle size decreases. (b) Because *DB increases relative t o *DxL as the temperature decreases, sintering by boundary diffusion will become more important as the temperature decreases.
16.6 Show that a scaling law holds for the sintering of a bundle of parallel wires by means of grainboundary diffusion, which was analyzed in Section 16.1.2. Solution. The rate of sintering is given by Eq. 16.16. Using the formalism o f Section 16.3.4, where all dimensions in the B system are X times larger than in the S system,
+ %
rateB  ( ~ / L B )
rates
 [~/(XLSX~W;)]
+ +
2yS(nBwi3  sin [ ~ / ( L s w ; ) [japp ] 2 y s ( n s w s  sin
c( [ ~ / ( L B w ~ [)j aIp p
(1,'~s)
{japp
91
f)]
+ 2 y S [ ( n s / ~xws )  sin f]} = + 2yS(nsws  sin f)]
(16.86)
A4
[ ~ / ( L S W ; ) []j a p p
16.7 Consider a grain boundary containing a uniform distribution of small pores (as shown in Fig. 16.13) that is subjected to a normal tensile stress 0% at a large distance from the boundary.
The pores will either grow or shrink by transferring atoms via grainboundary diffusion to or from the grain boundary acting as a sink or source, respectively, depending upon the magnitude of the applied stress. Find an expression for the rate of growth of the pore volume in a form proportional to the quantity (Fapp T), where F a p p is the force applied to each pore cell (shown dashed in Fig. 16.13) and T is the corresponding capillary force given by
+
T=27rySR2
( 16.87)
R
0
Construct a cylindrical cell of radius R, centered on a single pore as illustrated in Fig. 16.13 and solve the diffusion problem within it using cylindrical coordinates and the same basic method employed to obtain : 0
tttfttttttttttt I
I I
Grain boundary W r\
w
I , I I I I
I
?I
l w l l l
R, I l
, l l l I
u
wircciwiicc :0
Figure 16.13:
Distribution of pores in grain boundary subjected to tensile stress
CT,"~.
EXERCISES
415
the sintering rate of a bundle of parallel wires in Section 16.1.2. Assume that the pore maintains the equilibrium shape illustrated in Fig. 16.14. The upper and lower surfaces are spherical with curvature 2/R.
Figure 16.14: Cross section of equilibrium shape of pore on grain boundary as in Fig. 16.13, assuming that yB/ys = 1/3, so that 6' = 9.6". R is the radius of curvature of the top and bottom surfaces. The cross section in the grainboundary plane is a circle of radius R cos 6'.
Solution. Equation 16.3 applies and therefore 1 d V2unn = constant = A =  r dr
(r
da,, dr
)

(16.88)
Integrating twice and applying the boundary conditions corresponding t o
I%[
and Eq. 16.4
r=R,
u n n = 4A [ ( r 2  R 2 c o s 2 8 ) + 2 R ~ l n
(16.89)
(16.90)
A is now obtained by applying the integral force condition given by Eq. 16.5 and using the curvature relation n = 2/R. Therefore, A=
T
{ R:
[41n (&)

8(Faw + 31 R 2 cos2 8(4R,"  R2 cos2 O)}
+
(16.91)
with T given by
(16.92) and Fapp = ~Rza:. The rate a t which volume is transferred t o the pore by grainboundary diffusion is then
_dV _ dt
02GDB~(Rz R2 cos2 6') A kT
(16.93)
416
CHAPTER 16: MORPHOLOGICAL EVOLUTION: DIFFUSIONAL CREEP, AND SINTERING
+
and dV/dt is seen t o be proportional t o (FappT).
16.8 Since pore shrinkage is driven by a decrease in interfacial energy, it may be expected on general principles that the capillary force, T,must correspond to T=dGI (16.94)
dL where dGI is the change in the total interfacial energy of the system and dL is the corresponding change in its length produced by the pore shrinkage. Now demonstrate that Eq. 16.94 is indeed obeyed for the shrinkage of the pores on the grain boundary considered in Exercise 16.7, where T was found to equal  27rySR,2/ R. 0
The volume and area of the pore (shown in detail in Fig. 16.14) are given by 3 V = 2 n ~ (2  3cose + sin3 e) 3 A =4.rrR2(1 sine)
(16.95)
Solution. Focus on one cell as illustrated in Fig. 16.13 and take the cell height t o be L. Using Eq. 16.95, the total interfacial energy of the cell is given by Gr = 4.rrR2(1 sinB)yS
+ .x(RZ  R2 cos2B ) y B
(16.96)
dR  4( 1  sin e)] 
(16.97)
Then, since sine = yB/(2yS), dGr = 27rySR[2sin 0 cos2 0
dL
dL
However, the volume in the cell must remain constant, so
.rrR~L*(23cosB+sin30) 3 and
dR dL
1
=O
R: 2R2(2  3cosQ sin3 0)
+
(16.98)
(16.99)
Substituting Eq. 16.99 into Eq. 16.97 and employing Eq. 16.94,
dGI dL
f==
2nySR:[sin8cos28  2 ( 1 sine)] 27rySR,2  _R(2  3 cos 0 sin3 0) R
in agreement with Eq. 16.92.
+
(16,100)
PART IV
PHASE TRANS FORMATI0 NS
Phase transformations are of central importance in materials science and engineering. An understanding of the thermodynamics of phase equilibria is the foundation for understanding their kinetics. Necessary conditions for equilibrium include: uniformity and equality of the diffusion potential for each chemical species that can be exchanged between the phases; equality of temperature; and equality of pressure if the two phases can freely exchange volume.16 Deviations from these equilibrium conditions set the stage for kinetic processes. Parts I1 and I11 chiefly treated kinetic processes that derived from nonuniformity of a potential, such as chemical potential or temperature, within a single phase. Phase transformations occur when a region of the material can reduce the total free energy by changing its symmetry, equilibrium composition, equilibrium density, or any other quantity that defines a phase. The transforming material portion may be adjacent to its prospective phase, which is the case for growth of a new phase; or the portion may be isolated, which is the case for nucleation of a new phase. In any case, the spatial variation of '%rict equality of pressure is required absent capillarity effects: if a deforming heterophase interface stores energy during volume transfer, the two phases will have an equilibrium pressure difference.
the phasedefining quantitiesorder parameterspermit a convenient means to identify heterophase interfaces. The definition of what constitutes a phase is troublesome. Gibbs required 40 pages of preamble before introducing phase with ‘‘such bodies as differ in composition or state, different phases of the matter considered, regarding all bodies which differ only in quantity and form as different examples of the same phase’’ [l]. This clearly eliminates two bodies that are identical except for their morphology and sizeand perhaps one may credit Gibbs with the foresight to exclude crystallographic misorientation and symmetry operations from distinguishing phases. However, special cases, such as the distinction of a nearly cubic tetragonal variant from a strained cubic phase, must be handled carefully. Contiguous phases must be separated by an interface, and therefore considerations of interface and morphological evolution play a role in phase transformation kinetics. However, every interface need not separate two phasesgrain and antiphase boundaries separate crystallographic or symmetric variants of a single phase. Nevertheless, it is instructive to treat such interface motionwhere a single phase alters its orientationanalogously with phase transformations. Such a treatment naturally introduces two different kinds of order parameters. Regions of material defined by one kind of order parametersuch as spin density, symmetry, and orientationmay alter without a corresponding flux. Such fluxless order parameters are called nonconserved variables. Conserved variables, such as composition, require flux for a material to change locally. The thermodynamics of phase equilibria is reviewed in Chapter 17 and the fundamental thermodynamic differences between conserved and nonconserved order parameters are reinforced with a geometrical construction. These order parameters are used in the kinetic analyses of continuous and discontinuous phase transformat ions. Continuous transformations are treated in detail in Chapter 18. Spinodal decomposition and certain types of orderdisorder transformations follow from similar principles but differ only in the kinetics of conserved and nonconserved variables. The remainder of the book treats discontinuous transformations. Nucleation, which is necessary for the production of a new phase, is treated in Chapter 19. The growth of new phases under diffusion and interfacelimited conditions is treated in Chapter 20. Concurrent nucleation and growth is treated in Chapter 21. Specific examples of discontinuous transformations are discussed in detail; these include solidification (Chapter 22), precipitation from solid solution (Chapter 23), and martensite formation (Chapter 24). Bibliography 1. J.W. Gibbs. On the equilibrium of heterogeneous substances (1876). In Collected Works,volume 1. Longmans, Green, and Co., New York, 1928.
CHAPTER 17
GENERAL FEATURES OF PHASE TRANS FORMAT10 NS
The conditions under which a portion of a material system will undergo a phase transformation are determined by the system’s current and equilibrium thermodynamic states. The equilibrium state is distinguished by the minimum of an energy function that is particular to physical constraints imposed on the system. For instance, under conditions of constant temperature, T, and applied pressure, P, if the total energy quantity
Q
U  TS + PV
F + PV
31  TS
(17.1)
can be decreased via any internal change in the system, the system is thermodynamically unstable with respect to that change, however large. If Q cannot be decreased by any possible small variation, the system is in local equilibrium; if Q achieves its global minimum, the system will remain in complete equilibrium as long as it is constrained to the same constant P and T. Under different constraints, other minimizing energy functionals can be derived through Legendre transformations. The necessary conditions for a spontaneous phase transformation relate directly to the system’s energy differences upon transformation. In addition to the transformed volume’s chemicalenergy change, its interfacial energy and the elastic energy to accommodate interfacial misfit contribute to the total freeenergy change. Calculations of energy differences are simplified when the host material can be a p proximated as a reservoir with constant properties, so that the transformed volume and its interface need to be considered. Kinetics of Materials. By Robert W. Balluffi, Samuel M. Allen, and W. Craig Carter. Copyright @ 2005 John Wiley & Sons, Inc.
419
420
CHAPTER 17: GENERAL FEATURES OF PHASE TRANSFORMATIONS
If in addition to a thermodynamic driving force, a system has kinetic mechanisms available to produce a phase transformation (e.g., diffusion or atomic structural relaxation), the rate and characteristics of phase transformations can be modeled through combinations of their cause (thermodynamic driving forces) and their kinetic mechanisms. Analysis begins with identification of parameters (i.e., order parameters) that characterize the internal variations in state that accompany the transformation. For example, site fraction and magnetization can serve as order parameters for a ferromagnetic crystalline phase. Analysis proceeds by considering the temporal evolution of small variations in order parameter fields. However, a variation may be “small” in different ways. J. Willard Gibbs distinguished between a variation that “initially is small in degree, but may be great in its extent in space” and one that is “initially small in extent but great in degree” [l]. In the context of phase transformations, degree applies to the magnitude of an order parameter that characterizes a phasespecifically, whether it may vary continuously or not. Extent refers to the spatial region over which such variation occursspecifically, whether the change is confined to a (typically small) finite material portion or throughout the entire material system. Gibbs’s classification serves as the fundamental basis for division of phase transformation processes into two broad categories: continuous phase transformations and discontinuous phase transformations. During a continuous transformation, order parameter fields evolve smoothly in time and evolution is not confined to a small region. Discontinuous transformations initiate with an abrupt variation in an order parameter field and are localized events (i.e., they involve nucleation). Subsequent to initiation, phase transformations can continue by growth, which occurs as host material adjacent to the interface transforms into the new phase. Growth is treated in Chapter 21. After driving forces for growth have been exhausted, the system can continue to evolve by coarsening through reducing the energetic contribution from interfaces at constant phase fraction (Chapter 15). Model energy functionals will be obtained through consideration of the energetic contribution of order parameter fields, and this is preceded by a survey of order parameters . 17.1 ORDER PARAMETERS 17.1.1
OneComponent or Fixed Stoichiometry Systems
Figure 17.1 shows the molar free energy, F , as a function of temperature for a pure, or stoichiometric, material at fixed volume. The material has a firstorder phase transformation at the temperature where the molar free energies cross. The equilibrium free energy is a function of temperature only. The corresponding order parameter, E , which is also a function of T as illustrated in Fig. 17.lb, is a subsidiary parameter introduced by the series expansion (17.2) commonly known as a Landau expansion [ 2 , 3 ] . The physical quantity corresponding to E might be a molar heat capacity, enthalpy density, or any derivative of the molar free energy and its metastable extensions. F is taken as a function of both T and E. At any temperature, the equilibrium value of 5, Eeq(T),is determined from the
17 1 ORDER PARAMETERS
421
(a) Molar free energy as a function of temperature for a melting transition. (b) Temperature dependence of an order parameter 5 for the transition in (a).
Figure 17.1:
condition (17.3) and using Eq. 17.2, the equilibrium free energy, Feq, can be expressed as a function of T alone, in the form Feq [T,Ceq(T)], and [(Z)  pq becomes a measure of the local departure from equilibrium. The function F ( T ,[) defined in Eq. 17.2 can be used t o model the free energies of systems that are in the process of moving toward equilibriumi.e., undergoing a phase transformation represented by particular values of [. Introduced in this manner, the order parameter, E , is a “hidden” thermodyare not independent but are fixed namic variable: its equilibrium values, cq(T), by Eq. 17.3. Therefore, an order parameter is characteristic of the transformation process because it cannot be fixed by an experimental condition. Whether the phase transition is first or secondorder depends on the relative magnitudes of the coefficients in the Landau expansion, Eq. 17.2. For a firstorder transition, the free energy has a discontinuity in its first derivative, as at the temperature T, in Fig. 17.la, and higherorder derivative quantities, such as heat capacity, are unbounded. In secondorder transitions, the discontinuity occurs in the secondorder derivatives of the free energy, while first derivatives such as entropy and volume are continuous at the transition. The order of a transition can be illustrated for a fixedstoichiometry system with the familiar PT diagram for solid, liquid, and vapor phases in Fig. 17.2. The curves in Fig. 17.2 are sets of P and T at which the molar volume, V , has two distinct equilibrium valuesthe discontinuous change in molar volume as the system’s equilibrium environment crosses a curve indicates that the phase transition is first order. Critical points where the change in the order parameter goes to zero (e.g., at the end of the vaporliquid coexistence curve) are secondorder transitions. Connections to other types of phase diagrams can be obtained if order parameters are exchanged for intensive variables. Figure 17.2 is replotted with the order parameter V as the ordinate in Fig. 17.3b. The diagram predicts the phases that would exist for a molar volume fixed by a rigid container at different temperatures. The tielines connect equilibrium molar volumes at the same temperature
422
CHAPTER 17: GENERAL FEATURES OF PHASE TRANSFORMATIONS
(4 fn I n
9?
Gas (vapor)
n
Temperature, T
Temperature, T
Figure 17.2: (a) Singlecomponent phase diagram. (b) Shading represents the equilibrium value of a molar extensive quantity such as molar volume V (i.e.. light gray represents a large value and dark gray a small value) that apply to each phase at that particular P and T . For phase transitions. the grayscale (or V )could be used as an order parameter indicating phase.
and pressure. An analog to a ternary diagram could be obtained by substituting molar entropy for the Taxis in Fig. 17.3. Order parameters may also refer to underlying atomic structure or symmetry. For example, a piezoelectric material cannot have a symmetry that includes an inversion center. To model piezoelectric phase transitions, an order parameter. 7, could be associated with the displacement of an atom in a fixed direction away from a crystalline inversion center. Below the transition temperature T,, the molar Gibbs free energy of a crystal can be modeled as a Landau expansion in even powers of 11 (because negative and positive displacements, 7 , must have the same contribution to molar energy) with coefficients that are functions of fixed temperature and pressure,
G(T,P, 77) = G,(T, P ) + a ( P ) ( T  TC)q2 + B(P)v4
(17.4)
The equilibrium state is entirely determined by the minima of G as a function of pressure and temperature. The equilibrium order parameter qeq is determined by the minima of G and the equilibrium molar free energy can be calculated explicitly. (17.5)
a
4
Temperature, T
Temperature, T
Figure 17.3: (a) Singlecomponent PT phase diagram. (b) Phase diagram obtained from ( a ) by plotting the molar volume, V ,as an order parameter in place of pressure. The grayscale could indicate variations in an order parameter such as S.
17.1: ORDER PARAMETERS
423
where Eq. 17.6 is the freeenergy change when a mole undergoes a phase transformation from the nonpiezoelectric phase ( r ] = 0) to a piezoelectric phase (q2 2 0). Atomic displacements of opposite sign, &r], correspond to different polarizations of the same piezoelectric phase. Naturally, the fixed composition phase transformations treated in this section can be accompanied by local fluctuations in the composition field. Because of the similarity of Fig. 17.3 to a binary eutectic phase diagram, it is apparent that composition plays a similar role to other order parameters, such as molar volume. Before treating the composition order parameter explicitly for a binary alloy, a preliminary distinction between types of order parameters can be obtained. Order parameters such as composition and molar volume are derived from extensive variables; any kinetic equations that apply for them must account for any conservation principles that apply t o the extensive variable. Order parameters such as the atomic displacement r] in a piezoelectric transition, or spin in a magnetic transition, are not subject to any conservation principles. Fundamental differences between conserved and nonconserved order parameters are treated in Sections 17.2 and 18.3.
17.1.2 TwoComponent Systems For a binary AB alloy, another independent parameter, X B (or X A = 1  X B ) must be added to the fixedstoichiometry order parameters in the preceding section. The phenomenological form of the Landau expansion, Eq. 17.2, can be extended t o include X B and has been used to catalog the conditions for many transitions in twocomponent systems [3]. The methods of constructing homogeneous molar free energies for phase diagrams can also be used to construct firstorder approximations of freeenergy densities when a composition order parameter field is heterogeneous. Multicomponent phase diagrams can be accurately predicted from empirical, computed, or theoretical models of the composition dependence of molar enthalpies and entropies of formation and mixing. Macroscopic models for molar free energies of mixing can be obtained from combinations of atomistic bond energies, crystal structure, and configurational and vibrational entropy. A simple example of ordering or clustering of an AB alloy on a b.c.c. lattice illustrates how composition and structural order parameters arise naturally in the construction of the homogeneous molar free energy. Decomposition and OrderDisorder Transformations on a B.C.C. Lattice. Suppose that two species, A and B , occupy a b.c.c. lattice. If unlike bonds have lower molar enthalpies than like bonds [i.e., HAB < ~ ( H A A H B B ) ] ,then at low temperatures, ordered structures result in which the nearestneighbors of A atoms are
+
'In this section, the terms ordered structures, order parameters, and ordering transformations appear and may present some confusion. Unfortunately, these historic terms are in common use. An ordered structure typically indicates a regular site occupation pattern at the microscopic scale. Ordering transformations are those associated with such regular microscopic patterns. Order parameters are coarsegrained measures that collectively indicate phase plus additional information indicating geometric configurations of the same phasefor example, at antiphase boundaries.
424
CHAPTER 17. GENERAL FEATURES OF PHASE TRANSFORMATIONS
predominately B atoms.2 At high temperatures, disordered structures should appear because of the significant entropic contributions of the numerous disordered configurations but at the expense of slightly increased molar enthalpies. In this case, the hightemperature phase is b.c.c. (A2, in Structurbericht notation) and, on cooling, there is a phase transition to the B2 structure (primitivecubic ionic CsCl is the prototype of the B2 structure shown in Fig. 17.4). At this phase transition, there is a decrease of symmetry on the transformation to the ordered phasethe a/2(111) translational symmetry of the A2 phase is lost. An order parameter that indicates this symmetry loss would be a candidate to characterize an orderdisorder transition on the b.c.c. lattice. An example of a structure that undergoes such an ordering transformation is Pbrass (a CuZn alloy).
Figure 17.4: B2 ordering on a b.c.c. lattice where grayscale is associated with the composition at each site. B2 is a particular type of microscupic urcleriiig (of which CsCl is the prototype); the compositions are the same on all aplanes but differ from the composition on all the &planes.
Considering Fig. 17.4, the development of the B2 structure creates two sublattices from the original A2 structure. One of the B2 sublattices consists of the b.c.c. unitcell centers (indicated by ,B in Fig. 17.4) are displaced from the b.c.c. corners ( a in Fig. 17.4) by u/2(111). An ordering transformation produces sublattices, (Y and p, with differing site fractions, x$ and Their difference becomes a structural order parameter:
&.
q=
4
XSXP 2l (
(17.7)
7 evolves from zero toward equilibrium finite values *qeq. Symmetric stable values
exist because the b.c.c. corner sites are equivalent to the b.c.c. center sitesany result must be invariant to exchange of Q with p sublattices. Compositions on the two sublattices must be coupled to the local average composition, (17.8) 2 T h e molar enthalpy and the molar internal energy of bonding, H A B and U A B ,are related to the bond energies E A B at constant pressure and a t constant volume, respectively.
17.1: ORDER PARAMETERS
425
which is unchanged from the system’s average composition upon ordering. The order parameters 7) and X B are derivable from microscopic values of X g and X i , However, if unlike bonds have higher molar enthalpies, lowtemperature equilibrium configurations will consist of twophase A and Brich A 2 regions. At higher temperatures, entropic contributions will favor complete mixing. Therefore, systems that favor like bonds will tend to have a decomposition transformation upon cooling. As a result of a decomposition transformation, composition (i.e., X B in a binary alloy, Eq. 17.8) plays the role of an order parameter and evolves into stable values indicated by tielines on a phase diagram. However, 7) in Eq. 17.7 remains zero during a decomposition reaction. A model for the homogeneous free energy of mixing and B2 ordering can be obtained with site occupation probabilities. In a homogeneous system, the probability, p g , of finding a Bspecies occupying an asite is X g ; similarly, from Eqs. 17.7 and 17.8,
xg = x, + 7 p i = xi = X B  q
pg =
p; = 1  xg = 1  X B  q ppA = 1  xg = 1  X B
(17.9)
+ 7)
These probabilities must all lie between zero and one; this sets bounds on physical values for the structural order parameter 1 xg
A S = Nk (pg lnpg + p i l n p i
+ pg lnpg + pg lnpg)
(17.11)
If it can be assumed that mixing, decomposition, and ordering transformations occur at constant volume, an estimate of the internal energy, U , can be used to obtain the appropriate minimizing molar free energy F = U ; T S . A model for the total internal energy can be obtained from the nearestneighbor bond energies of the three possible bond types EAA,E B B ,and E A B ,and their populations calculated from site probabilities. Because each atom contributes four bonds,
NAA= W ~ A=A 4p;ppA
= 4 [ ( I  X B ) 2 17’1
(17.12)
3The reference state is the compositionweighted linear combination of pure A and B components. This approximation neglects vibrational entropy. Higherorder meanfield approximat,ions t o configurational entropy, known as the clustervariation method, are known [5, 61.
426
CHAPTER 17: GENERAL FEATURES OF PHASE TRANSFORMATIONS
The last two terms in U can be used as a reference energythe total internal energy of a system of composition XB that is divided into pure A and pure B portions. The change in internal energy due to mixing and ordering relative to this reference state is
+ ( 17.13) = w { [ E A A + E B B  2EAB][XB(XB  1)b q2]} The nearestneighbor interaction coefficient, W = EAA+ EBB ~ E A B and , the (~ XB) EBBXB U AU = E A A 
temperature together characterize the molar free energy of mixing:
+
A F =  4W [XB(XB  1) q2]
+kT
[
+
=  4 w [q2  XBXA]
+kT
[
+ +
(XB 7 )ln(XB 77) (XB  77) ln(XB  q ) +(1  XB + q ) l n ( l  XB q ) (1 XB  q ) l n ( l  XB  q )
+
+ +
+ + +
(XB q ) 1n(XB 17) (XB  77) ln(XB  7) f(XA + q ) 1n(XA + 7 ) ( X A  17) In(XA  17)
1
1
(17.14)
The equilibrium order parameters Xgq and qeq minimize A F subject to any system constraints. Supposing that the system’s composition is fixed, the method of Lagrange multipliers leads to a commontangent construction for A F with respect t o XBor equivalently, equality of chemical potentials of both A and B . Two : and will coexist at equilibrium for average compositions compositions, X XB in the composition range < XB < X;+ if they satisfy
X2+, X2
X2
The condition expressed by Eq. 17.15 pertains only if # X 2 + ; it is automatically satisfied for fixed uniform compositions with variable order parameter (this situation appears below for B2 ordering). Because q is not constrained, (17.16)
The symmetry of the particular model, Eq. 17.14, simplifies the equilibrium condition, Eu. 17.15: (17.17)
X2*
= fAXiq. For this nearestneighbor b.c.c. model, equilibrium order where parameters can be reduced to solutions of
(17.18) and (17.19)
17 1. ORDER PARAMETERS
427
For the disordered ( A 2 ) phases, qeq = 0, Eq. 17.19 is satisfied automatically, and equilibrium tielines are present if W < 0 and T < Tcrit= IW/kl, as illustrated in Fig. 17.5. In the nearestneighbor model, ordered B2 solutions can appear at any uniform composition X B . Nonzero equilibrium structural order parameters appear only if W > 0 at temperatures T satisfying (17.20) as illustrated in Fig. 17.5. The development of the miscibility gap for W < 0 and the antiphases (kqeq) for W > 0 have entirely different kinetic implications. For decomposition, mass flux is necessary for the evolution of two phases with differing compositions. Furthermore, interfaces between these two phases necessarily develop. The evolution of ordered phases from disordered phases (i.e., the onset of nonzero structural order parameters) can occur with no mass flux; macroscopic diffusion is not necessary. Because the q:qphase is thermodynamically equivalent to the vegphase, the development of 77phase in one material location is simultaneous with the evolution of 72phase at another location. The impingement of these two phases creates an antiphase domain boundary. These interfaces are regions of local heterogeneity and increase the free energy above the homogeneous value given by Eq. 17.14. The kinetic implications of macroscopic diffusion and of the development of interfaces are treated in Chapter 18.
1 T
Tcrit
0
Figure 17.5: Phase diagrams for the nearestneighbor bondenergy model for the b.c.c. lattice. (a) The temperature dependence of the decomposition reaction for W = E A A EBB~EAB < 0. A miscibility gap appears at temperatures below Tcrit= W / k but qeq = 0 at all compositions and temperatures. (b) B2 ordering transformations occur if W > 0 and T/TCrit< 4XAXB and are indicated by the onset of nonzero values of qeq. The qeq are symmetric about 77 = 0. The two values &qeq indicate equivalent ordered states where the a and Pplanes in Fig. 17.4 are exchanged.
+
428
CHAPTER 17. GENERAL FEATURES OF PHASE TRANSFORMATIONS
The composition order parameter X B is an example of a conserved order parameter; it cannot increase or decrease locally without an opposite change elsewhere. The structural order parameter is an example of a nonconserved order parameterno spatial correlations in their variations are necessary. Energetic changes associated with the two different types of order parameters have already been distinguished by the difference between the commontangent condition (Eq. 17.18) and the global’minimum condition expressed by Eq. 17.19. The changes in molar free energies for the two different types of order parameters are treated in the next section.
17.2
MOLAR FREEENERGY CHANGES FOR CONSERVED A N D NONCONSERVED ORDER PARAMETERS
The composition or the number fraction of component B , X B , is an example of an order parameter that is conserved in a closed system. Figure 17.6 shows a molar free energy versus composition curve for a binary solution. The molar free energy for a solution at any composition X B can be written in terms of its partial molar quantities, F A ( X B )and FB(XB)z4 (17.21)
xi
xg
0 1 Number fraction of component B, XH Figure 17.6:
Molar free energy. F ( X g ) , as n function of X g for a binary solution. ) Fg(Xg)] Partial molar free energies for A and B a t the composition X g [i.e.. F A ( X ~and are given by the intercepts at X B = 0 and X g = 1 of the line tangent t o the curve F ( X B ) at X g = X g . AF,, is the change in free energy that occurs for a very large system of initial composition X i if one mole of the original system is transformed to one mole of a new solution of composition X h and the system is open and unconstrained so that matter can be transferred in or out. A F , is the corresponding change that occurs if the system is closed so that its total composition is fixed. 4The Helniholtz free energy. used here as an example of a molar free energy, is the appropriate minimizing functional for a system at fixed volume in equilibrium with a reservoir at fixed temperature. For different types of system constraints, F would be replaced with another appropriate molar free energy.
17 2: MOLAR FREEENERGY CHANGES
429
Consider a general system at composition X g . If any of its subsystems (i.e., material portions) could transform to a new composition X b without affecting the rest of the system, the change in the system’s total free energy .F would be simply
A F = F ( X L ) F ( X g )
(17.22)
for each transformed mole as indicated by A F , in Fig. 17.6. Such a change would be possible in a system that can exchange B with its environmentan open system for which no conservation principle applies. In a closed system, the total number of B, NB, is effectively conserved and such a change is not possible. Therefore, for any nonconserved parameter [, the change in molar free energy is
A F = F(J’)  F([o)
( 17.23)
In a closed system, where the numbers of A and B atoms are conserved, a change in any subsystem must affect the rest of the systematoms must be exchanged internally to accomplish the transformation. For each mole transformed, the change L , a similar in F for the X L moles of the B component is [ F ~ ( x b )  F ~ ( x g ) ] xwith term for the (1  X L ) moles of the A component,
which can be rewritten
or
A F = F ( X L ) F ( X g )  ( X b  X g )
(17.26)
which is numerically equal to the distance indicated in Fig. 17.6 by AF,. Note that A F , is negative if at X B = XL,the curve for F ( X B )lies below the tangent; A F , is positive otherwise. Equation 17.26 holds for any composition Xb when the composition X g is fixed. Consider a small fluctuation of composition (or any other order parameter that B is conserved for a system), ~ X =BX b  X g . Expanding F ( X B )in ~ X yields
Substitution of Eq. 17.27 into Eq. 17.26 gives (17.28) for the change in the molar free energy. Equation 17.28 indicates that when X B is )~. conserved, the variation in molar free energy is proportional to ( ~ X B Therefore, a barrier to the growth of small variations exists whenever the second derivative in Eq. 17.28 is positive.
430
CHAPTER 17: GENERAL FEATURES OF PHASE TRANSFORMATIONS
On the other hand, if [ is nonconserved, using Eq. 17.23 and expanding F(t"+b<) shows that the lowestorder term foi. the change in the molar free energy is (17.29)
A decrease in the free energy can always be achieved by picking a variation d t with
<
a sign that makes the product in Eq. 17.29 negative. Therefore, if is nonconserved, there is no barrier to evolution to a local minimum in the appropriate freeenergy functional, and the system will evolve if there are kinetic mechanisms that enable such variations.
17.3 CLASSIFICATION OF PHASE TRANSFORMATIONS: CONTINUOUS VERSUS DISCONTINUOUS TRANSFORMATIONS
Figure 17.7a shows a typical molar free energy versus composition curve for a binary system exhibiting a miscibility gap. The corresponding equilibrium diagram is shown in Fig. 17.7b. If a homogeneous alloy in Region I of Fig. 17.7b is rapidly cooled into the miscibility gap and held there at To, it decomposes into soluterich and solutelean phases at the ends of the tieline shown. If the alloy composition is only slightly higher than Xg' so that it is in the range where d 2 F / d X i > 0, Eq. 17.28 shows that a freeenergy barrier exists for any local region in the system to enrich itself progressively in soluteatom concentration. In addition, Fig. 17.6 shows that if such a region could undergo a fluctuation corresponding to a large increase in local solute concentration, the free energy would decrease. In contrast, if the alloy composition is higher and in the range where d 2 F / d X $ < 0, a region of the specimen can progressively enrich itself and eventually form the equilibrium soluterich phase as the free energy decreases continuously. The dividing line between these two types of behavior is set by the condition d 2 F / d X i = 0 and is known as the chemical spinodal. This line is mapped in Fig. 17.7b. Phase transformations proceed only when there is an ultimate decrease in the free energy, and the considerations above show that two quite different types of T
TO
Xi'
XB
x;"
XB
Figure 17.7: (a) Molar free energy, F ( X B )vs. cornpositmioncurve for a binary system exhibiting a miscibility gap. The corresponding equilibrium diagrani is shown in (b). The compositions of the a' and a" phases in equilibrium across the miscibility gap in (b) are obtained from commontangent constructions at each temperature such as the one shown in (a). The points on the chemical spinodal in (b) correspond to points on the curve in (a) where a 2 F l a X i = 0.
17 3 CONTINUOUS AND DISCONTINUOUS TRANSFORMATIONS
431
phase transformation can take place depending upon whether the composition is inside or outside the spinodal line in Fig. 17.7b. If the composition is outside the chemical spinodal (but still within the miscibility gap) there is a bulk freeenergy barrier to the formation of the soluterich phase in any local region, and the soluterich phase can form only if such a region somehow becomes sufficiently enriched in solute atoms so that the freeenergy barrier is overcome. Once the barrier is surmounted, the region can continue to develop into the equilibrium phase with a continuous decrease in the free energy. The only way that this can occur at a sensible rate is by means of a fluctuation that produces a relatively large enrichment of composition in a small region, i.e., nucleation of the soluterich phase must take place in a region of atomic dimensions (see Chapter 19). On the other hand, if the composition is within the chemical spinodal, there is no bulk freeenergy barrier to the progressive formation of soluterich regions, and the transformation takes place over large regions of the system with a continuous decrease in the free energy. This leads t o the general classification of continuous and discontinuous transformations. Continuous transformations: In this type of transformation, the system is initially unstable, and an infinitesimal variation will initiate the transformation and the decrease of bulk free energy. The transformation can begin over large regions, and all volumes of a system can transform simultaneously. The beginning of the transformation involves a change that is small in degree but large in extent. Primary examples include spinodal decomposition and some orderdisorder transformations in alloys that exhibit longrange order. Discontinuous transformations: In this type of transformation, there is a freeenergy barrier to infinitesimal variations and the system is initially metastable. However, a sufficiently large variation can cause the free energy to decrease. The transformation therefore can be initiated at a finite rate only by a variation that is large in degree but small in extent (i.e., nucleation is required). Examples include the formation of Brich precipitates from a supersaturated AB solution. Bibliography 1. J.W. Gibbs. On the equilibrium of heterogeneous substances (1876). In Collected Works, volume 1. Longmans, Green, and Co., New York, 1928.
2. L.D. Landau and E.M. Lifshitz. Statistical Physics. Pergamon Press, New York, 1963. 3. S.M. Allen and J.W. Cahn. Phase diagram features associated with multicritical points in alloy systems. Bull. Alloy Phase Diagrams, 3(3):287295, 1982. 4. G. Inden. Ordering and segregation reactions in BCC binary alloys. Acta Metall., 22(8):945951, 1974. 5. R. Kikuchi. A theory of cooperative phenomena. Phys. Rev. B,81(6):9881003, 1951. 6. D. de Fontaine. Studies of the thermodynamics of ordering by the cluster variation method. In H.I. Aaronson, D.E. Laughlin, R.F. Sekerka, and C.M. Wayman, editors, Proceedings of an International Conference on Solid+Solid Phase Transformations, pages 2547, Warrendale, PA, 1981. The Metallurgical Society of AIME.
CHAPTER 18
SPINODAL DECOMPOSITION AND 0R D ERD IS0R DER T RANS FOR M AT I0NS
Spinodal decomposition and certain orderdisorder transformations are the two categories of continuous phase transformations. Both arise from an order parameter instability: in the case of spinodal decomposition, it is a conserved order parameter; for continuous ordering, it is a nonconserved order parameter. As spinodal and ordering transformations progress, order parameter gradients arise and the extra energy associated with these gradients must be reflected in a modified diffusion potential for the transformations. The evolution of spinodal decomposition and continuous ordering transformations is described by the CahnHilliard equation and the AllenCahn equation, respectively. Both incorporate gradientenergy terms via the modified diffusion potential. Finescale, spatially periodic microstructures are characteristic of spinodal decomposition. In elastically anisotropic crystalline solutions, spinodal microstructures are aligned along elastically soft directions to minimize elastic energy. Microstructures resulting from continuous ordering contain interfaces called antiphase boundaries which coarsen slowly in comparison to the rate of the ordering transformat ion.
18.1 THE INTERDIFFUSIVITY AT UNSTABLE COMPOSITIONS Because composition is a locallyconserved order parameter, it cannot change in one location without affecting its neighborhoodfluxes are required to change a composition field. For example, in a binary alloy, the concentration field CB is reKinetics of Materials. By Robert W. Balluffi, Samuel M. Allen, and W. Craig Carter. Copyright @ 2005 John Wiley & Sons, Inc.
433
434
CHAPTER 18 SPINODAL AND ORDERDISORDER TRANSFORMATIONS
lated to the composition field ( C B = X B / ( R ) )and the flux of B is linearly related to its chemical potential gradient by Eq. 3.7.l The fluxes that produce a concentration change at some point necessarily affect concentrations in the neighborhood of that point. This coupling between the space and time behavior of concentration is encoded in Fick's first and second laws for a binary alloy by

JB= DVCB where the flux,
&,
(18.1)
is relative to the Vframe described in Section 3.1.3, and (18.2)
which is linearized by expanding the interdiffusivity 2, about an average composition. The exact form is given by Eq. 3.25:
E % ( R ) ( c A D B+ C B D A= ) X A D B+ X B D A =
+
( X A*DB X B *DA)
(18.3)
d In X A
If 5 > 0, Eq. 18.2 implies that a system with a uniform composition X g ( Z ) = < 0, small composition fluctuations (Cl)cgnst would not evolve. However, if would grow without bound: a system described by Eq. 18.2 would develop into many unphysical and finely spaced large fluctuations in composition. The stability conditions for a conserved order parameter are developed in Section 17.2, and Eq. 17.28 relates this condition to the sign of d 2 F / d X z . If a system is at a nearly uniform composition X B where the second derivative is negative, the system is unstable and should evolve. As shown below, the sign of D , determined by the sign of d 2 F / d X i ,predicts the decomposition of a uniform unstable composition. However, Eqs. 18.1 and 18.2 do not account for interfacial energies between the developing phases. The correction to Eqs. 18.1 and 18.2 due to interfacial energies is accomplished through the addition of a gradientenergy term and is addressed in Section 18.2. To show how the sign of 6 is related to the sign of d 2 F / a X $ , consider chemical diffusion in a substitutional AB crystalline material, as described in Section 3.1.3. in the Cframe are given by Eq. 3.7 and can be written in The fluxes fz and the forms 1 : = LAV/LA J Z = LBV/LB (18.4)
Jg
where L A = L A A ( C A / C B ) L Aand B L B = L B B (CB/CA)LBA.Using Eq. 3.15, the corresponding fluxes in the Vframe are related to the fluxes in the Cframe by (18.5) For simplicity, we assume in this chapter that the atomic volumes of A and B are equal and constant (i.e., C ~ A RB z R = constant).2 Then, using Eqs. 3.21, 18.4, and 18.5, solving for J Z , and simplifying the result using Eq. 3.9 yields
JZ = ~ ~ ( C A L B V PC B L A V P A )
(18.6)
See Section A.2 for this and similar conversions between composition and concentration. 2These approximations were eliminated by Hilliard [l],and a corresponding derivation that utilizes methods developed in Section 3.1.3 appears in Exercise 18.1.
435
18.2: DIFFUSE INTERFACE THEORY
Equation 18.6 can be simplified using the identity
+
C A L B V P B C B L A V ~=AR[(c%LB c ~ L A ) ( v ~ Bv ~ A ) (CALB CBLA)(cAvpA + C B V P B ) ]
+
In addition, because of the GibbsDuhem relation, chemical potential gradients are interdependent: CAV
+
C A ~ ~ cA
~ IA C B V ~ =BO
(18.7)
~ d = p 0,~ the (18.8)
With the aid of Eqs. 18.7 and 18.8, the flux of B in the volumefixed frame is then 7
JB
 R2
+
( ~ L B &A)
v(pB  P A )
MV(PB  P A ) (18.9)
+
where M = R2 ( ~ L Bc ~ L A must ) be positive to satisfy the basic postulate of irreversible thermodynamics, ir 2 0 (Eq. 2.16). Comparison of Eqs. 18.2 and 18.9 shows that 6 is negative when the system is unstable to small concentration fluctuations, a 2 F / 8 X ; < 0. This condition occurs during spinodal decomposition, and the negative interdiffisivity gives rise to uphill d i f l ~ s i o n . ~ However, a negative interdiffusivity makes the diffusion equation illposed. With a positive diffusion coefficient, the amplitude of a composition wave decays at a rate proportional to the square of the inverse wavelength (see Section 5.2.4). Conversely, if the diffusion coefficient is negative, the smallest wavelengths will grow the most rapidly. Consider two concentration profiles that are nearly the same except for small differences in their highestorder Fourier coefficients; after a short time, the profiles will be very different if the diffusion coefficient is negative. Therefore, when 6 < 0, the behavior of the concentration profile is not robust with respect to small variations in the initial data and the problem is illposed. However, as shown in the following section, interfacial energy terms can be included by associating additional energy with the concentration gradients, and their inclusion regularizes the diffusion equation when D < 0 (i.e., the resulting equation is not illposed). 18.2
FREE ENERGY OF INHOMOGENEOUS SYSTEMS: DIFFUSE INTERFACES AND THE POTENTIAL FOR TRANSFORMATION
The conditions for continuous phase transformations (described in Chapter 17) derive from considerations of the molar free energy of a homogeneous, spatially uniform system with no interfaces. For phase transformations involving nonconserved 3Spinodals occur at points where second derivatives vanish and for molar free energy and compositions give rise to the sharp “cusps” in Fig. 17.1 [a]. Spinodal derives from the Latin spina, for thorn (the plural, spinae, meant difficulties or perplexities).
436
CHAPTER 18: SPINODAL AND ORDERDISORDER TRANSFORMATIONS
order parameters, such as for A2 + B2* ((qeq = 0) + ( q = kqeq)), there is no bias t o form one ordered B2 variant over another (the two equivalent variants are indicated by B2*; see Fig. 17.4). The two equivalent variants emerge at random locations, and interfaces develop as one impinges upon the other. For conserved order parameters, such as composition, interfaces between phases on phasediagram tielines necessarily appear. In the absence of interfaces, a linear kinetic theory could be developed where the transformation driving force derives from decreases in homogeneous molar free energy as derived in Eqs. 17.28 and 17.29 for the conserved and nonconserved cases. However, at the onset of a continuous phase transition, the system is virtually all interface between new phases or variants. For example, when equivalent variants emerge in adjacent regions during ordering, gradients in the order parameter are generated; these constitute emerging diffuse antiphase boundaries. Neglecting the contribution of these interfaces leads to illposed linearized kinetics, as indicated by the negative interdiffusivity in Eq. 18.9. The theory for the free energy of inhomogeneous systems incorporates contributions from interfacial free energy through the diffuse interface method [3].Interfaces are defined by the locations where order parameters change and can be located by the regions with significant orderparameter gradients. Interfacial energy appears in the diffuseinterface methods because orderparameter gradients contribute extra energy.
18.2.1 Free Energy of an inhomogeneous System Let J(F) represent either a conserved or a nonconserved order parameter, such as C B ( F ) or q(F). Also, let the field f(F) = f(J(F),VJ(F)) be the freeenergy density = (energy/volume) at position F. The homogeneous freeenergy density, f f (J, VJ = 0), is the freeenergy density in the absence of gradients and is related to molar free energies, F(J)= N,(R) f h o m ( J ) , used to construct phase diagrams such as Figs. 17.5 and 17.7. Expanding the freeenergy density about its homogeneous value in powers of gradient^,^
f where
(e,VC) = f(J,0 ) + 2 VJ + VJ . K VJ + . . . *
(18.10) (18.11)
is a vector evaluated at zero gradient, and K is a tensor property known as the gradientenergy coefficient with components (18.12) The freeenergy density should not depend on the choice of coordinate system [i.e., f (J, 05) should not depend on the gradient's direction] and therefore 2 = 0 and K will be a symmetric t e n ~ o r Furthermore, .~ if the homogeneous material is isotropic 4There are expansions that contain higherorder spatial derivatives, but the resulting free energy is the same as that derived here [I, 41. 51f the homogeneous material has an inversion center (center of symmetry), 2 is automatically zero.
18.2: DIFFUSE INTERFACE THEORY
437
or cubic, K will be a diagonal tensor with equal components K . The freeenergy density will be, to second order,
f ( E , VE) = fhO"(E)+ KVE ' VE = fhO"(E)+ KIVEI2
(18.13)
The freeenergy density is thus approximated as the first two terms in a series expansion in orderparameter gradients: the first term is related to homogeneous molar free energy and the second is proportional to the gradient squared. In the expansion that leads to Eq. 18.13, it is assumed that the free energy varies smoothly from its homogeneous value as the magnitude of the orderparameter gradient increases from zero. This assumption is usually correct, but there may be cases that include a lowerorder term proportional to lVSl if the freeenergy density has a cusp at zero gradient. Such cusps appear in the interfacial free energy a t a faceting orientation; they are also present a t small tiltmisorientation grainboundary energies [5], Models with crystallographic orientation as an order parameter incorporate gradient magnitudes, lV(l, into the inhomogeneous freeenergy density [6]. 18.2.2
Structure and Energy of Diffuse Interfaces
There are two energetic contributions to interfaces in systems that undergo decomposition and ordering transformations such as illustrated in Figs. 17.5 and 17.7. One is due t o the gradientenergy term in Eq. 18.13; this contribution tends to spread the interface region and thereby reduce the gradient as the order parameter changes between its stable values in adjacent phases. A second contribution derives from the increased homogeneous freeenergy density associated with the "hump" in Fig. 18.1, and this term tends to narrow the interface region. Thus, systems modeled with Eq. 18.13 contain diffuse interfaces where the order parameter varies smoothly as in Fig. 18.2. Equilibrium orderparameter profiles and energies can be determined by minimizing F ,the volume integral of Eq. 18.13 [l,41. Figure 18.2a shows a planar interface between two equilibrium phases possessing different conserved order parameters corresponding to local freeenergy density minima in their order parameters as in Fig. 17.7a. Figure 18.2b shows a corresponding profile of the distribution of order between two identical ordered domains possessing different nonconserved order parameters corresponding to local freeenergy density
I
i
I
Figure 18.1: Properties of diffuse interfaces expressed in ternis of the function Afho"(<), which has the maximum value A f,!,;:.
438
CHAPTER 18 SPINODAL AND ORDERDISORDER TRANSFORMATIONS
Figure 18.2: (a) Composition and (b) order variations across diffuse. planar interfaces. The profiles c(z) and q(z)are continuous. In (a). the grayscale image represents the spatial variation of a conserved variable, and the quantities ca' and ca" are the equilibrium values in the bulk phases at large distances from the interface (see Fig. 17.7). In (b). the drawing below the profile illustrates the spatial variation of a nonconserved variable such as local magnetization in the region around a domain wall.
minima. Both kinds of interfaces can coexist, so that the variations of C B and 77 are coupled as in Fig. 18.3. In all cases, the distribution of the order parameter (or order parameters) minimizes the total free energy of the system. F. The coupledparameter case can be treated as an extension to the theory so that the free energy is a function of both C E and 17.
t
'I
or c
X
C
Figure 18.3: Coupled system of order and concentration parameters representing mi antiphase boundary with segregation.
18.2:DIFFUSE INTERFACE THEORY
439
Minimizing 3 = f (<, V E ) d V produces equilibrium interface profiles [(q. An equilibrated planar interface is characterized by its excess energy per unit area, y,
,=2l:
,/,d[=
,/=A[
(18.14)
and a characteristic width 6, (18.15) where A fhom is the increase in freeenergy density relative to a homogeneous system at its equilibrium values of E (i.e., relative to the commontangent line) and A f g T is the maximum value of Afhom (indicated in Fig. 18.1). y and 6 can be measured and their values uniquely determine the model parameters, A f z T and K . 18.2.3
Diffusion Potential for Transformation
The local diffusion potential for a transformation, @(q, at a time t = t o , can be determined from the rate of change of total free energy, 3, with respect to its current orderparameter field, [(F, t o ) .At time t = t o ,the total free energy is
3 ( t o )=
s,
+
[fhom(C(F, t o ) ) KV5 .V5] d V
(18.16)
which defines 3 as a functional of [(F‘, t o ) . sIf the order parameter is changing with t o ) t ] the , rate of change local “velocity” [i.e., such that [ ( F , t ) = c(F, t o ) ((7, of F can be summed from all the contributions to f([, V [ )due to changes in the orderparameter field and its gradient,
+
( 18.17) Using the relation (18.18) Eq. 18.17 can be written
itO s, (
1,
Applying the divergence theorem to the second integral in Eq. 18.19,
d 3
=
)‘(;:
4 d V + 2K
 2KV2[)
iV[ d 2
(18.20)
where aV is the oriented surface bounding the volume V . The boundary integral on the righthand side of Eq. 18.20 is negligible. It vanishes identically if i ( 8 V )= 0, ‘Some readers will recognize this development as the calculus of variations [7]. A functional is a function of a function; in this case, F takes the function [ ( F , t o ) and maps it to a scalar value that is numerically equal to the total free energy of the system.
440
CHAPTER 18 SPINODAL AND ORDERDISORDER TRANSFORMATIONS
which is the case if [ ( d V ) has fixed boundary values (Dirichlet boundary conditions), or if the projections of the gradients onto the boundary vanish (Neumann boundary conditions), If neither Dirichlet or Neumann conditions apply, the boundary integral will usually be insignificant compared to the volume integral for large systems (e.g., if the volumetosurface ratio is greater than any intrinsic length scale). Therefore, if the order parameter changes by a small amount 6[ = ( d t , the change in total free energy is the sum of local changes: (18.21) The quantity (18.22) is the localized density of freeenergy change due to a variation in the orderparameter field, 6[, and is therefore the potential to change [. Equation 18.22 is the starting point for the development of kinetic equations for conserved and nonconserved orderparameter fields. 18.3
18.3.1
EVOLUTION EQUATIONS FOR CONSERVED A N D NONCONSERVED ORDER PARAMETERS CahnHilliard Equation
The CahnHilliard equation applies to conserved orderparameter kinetics. For the binary AB alloy treated in Section 18.1, the quantity in Eq. 18.22 is the change in homogeneous and gradient energy due to a change of the local concentration C B and is related to flux by
(18.23)
where the subscript is affixed to the gradient energy coefficient as a reminder that the homogeneous system is expanded in composition and its gradient. t) Therefore, the accumulation gives a kinetic equation for the concentration C B(T, in an AB alloy: 2KCV2c~]}
(18.24)
18.3: EVOLUTION EQUATIONS FOR ORDER PARAMETERS
441
which is the CahnHilliard equation [3]. The CahnHilliard equation is often linearized for concentration around the average value of the inherently positive kinetic coefficient M , = ( M ) = ( 5 / [ 0 ( a 2 P o m defined in Eq. 18.9: dCB = Ado
~
at
[
)/(ax;)]),
horn ~2 V '
1
C B2 K , V 4 c ~
(18.25)
The first term on the righthand side in Eq. 18.25 is diffusive. The second term accounts for interfacialenergy penalties from concentration gradients. 18.3.2
AllenCahn Equation
The AllenCahn equation applies to the kinetics of a diffuseinterface model for a t ), nonconserved order parameterfor example, the orderdisorder parameter ~ ( 7 that characterizes the A2 t B2' phase transformation treated in Section 17.1.2. The increase in local freeenergy density, @(F) from Eq. 18.22, does not require any macroscopic flux.7 In a linear model, the local rate of change is proportional to its energydensity decrease,
(18.26)
where Mq is a positive kinetic coefficient related to the microscopic rearrangement kinetics. According to the AllenCahn equation, Eq. 18.26, 77 will be attracted to the local minima of f h o r n . Depending on initial variations in 77, a system may seek out multiple minima at a rate controlled by Mq. The second term on the righthand side in Eq. 18.26 will govern the profile of 77 at the antiphase boundary and will cause interfaces to move toward their centers of curvature [8]. 18.3.3
Numerical Simulation and the PhaseField Method
Numerical models of conserved orderparameter evolution and of nonconserved orderparameter evolution produce simulations that capture many aspects of observed microstructural evolution. These equations, as derived from variational principles, constitute the phasefield method [9]. The phasefield method depends on models for the homogeneous freeenergy density for one or more order parameters, kinetic assumptions for each orderparameter field (i.e., conserved order parameters leading t o a CahnHilliard kinetic equation), model parameters for the gradientenergy coefficients, subsidiary equations for any other fields such as heat flow, and trustworthy numerical implementation. The phasefield simulations reproduce a wide range of microstructural phenomena such as dendrite formation in supercooled fixedstoichiometry systems [lo], dendrite formation and segregation patterns in constitutionally supercooled alloy systems [ll],elastic interactions between precipitates [12], and polycrystalline solidification, impingement, and grain growth [6]. 'This ordering transition occurs at constant composition and is accomplished by microscopic rearrangement of atoms into two sublattices.
442
CHAPTER 18: SPINODAL AND ORDERDISORDER TRANSFORMATIONS
The simple twodimensional phasefield simulations in Figs. 18.4 and 18.5 were obtained by numerically solving the CahnHilliard (Eq. 18.25) and the AllenCahn equations (Eq. 18.26). Each simulation’s initial conditions consisted of unstable orderparameter values from the “top of the hump” in Fig. 18.1 with a small spatial
Figure 18.4: Example of numerical solution for the CahnHilliard equation, Eq. 18.25. demonstrating the kinetics of spinodal decomposition. The system is initially near an unstable concentration, (a), and initially decomposes into two distinct phases with compositions ca (black) and cB (white) with a characteristic length scale, ( c ) and (d). Subsequent evolution coarsens the length scale while maintaining fixed phase fractions. The effective time interval between images increases from (a)(f).
Figure 18.5: Example of numerical solution for the AllenCahn equation, Eq. 18.26, for an orderdisorder transition such as A2 + B 2 * . Initial data are near the disordered state. 7 = 0 (gray) in (a). The system evolves into two types of domains (shown in black and white) with antiphase boundaries (APBs) separating them. The phase fractions are not fixed. The local rate of antiphase boundary migration is proportional to interface curvature [8. 131. The effective time interval between images increases from (a)(f).
443
18.4: DECOMPOSITION AND ORDERDISORDER: INITIAL STAGES
variation. In each simulation, the magnitude of the order parameter is indicated by grayscale. Initial medium gray values correspond to the unstable initial conditions. The characteristics of the initial evolution during spinodal decomposition or orderdisorder transformations can be predicted by the perturbation analyses presented in the following section. 18.4
INITIAL STAGES OF DECOMPOSITION A N D ORDERDISORDER TRANSFORMATIONS
18.4.1 CahnHilliard: Critical and Kinetic Wavelengths
A homogeneous freeenergy density function fhom(cg)that has a phase diagram similar to Fig. 17.7b has the form fhoycg) =
l6f%F (CP 
ca)4
[(cg  C")(Cg
 CP)] 2
(18.27)
with stable (commontangent) concentrations located at its minima C" and cP and a maximum of height fkaTat cg = co E (c" cp)/2. Suppose that an initially uniform solution at CB = co is perturbed with a small onedimensional concentration wave, c g ( z , t ) = co e(t)sinPz, where /3 = 2n/X. Substituting cg(T;t) into Eq. 18.25 and keeping the lowestorder terms in e(t) yields
+
+
de(t) dt
MOP2 [lSf&:
(cP  c " ) ~
 2KcP2(cP
e(t)
(18.28)
so that
(18.29) where the sign of the amplification factor R(P) indicates whether a fluctuation will grow or not [i.e., only composition fluctuations wit.h wavelengths that satisfy R(P) > 01, or rr x > Xcrit = (cP  c") (18.30) 2 f2Kc kY
d
I
will have dcldt > 0 and will grow. Taking the derivative of the amplification factor in Eq. 18.28 with respect to p and setting it equal to zero, the fastestgrowing (18.31) The characteristic length scale in the early stage of spinodal decomposition will correspond approximately to this wavelength.8 sReaders may recognize an analogy t o the critical and fastestgrowing wavelengths derived for surface diffusion and illustrated in Fig. 14.5. Both the surface diffusion equation and the CahnHilliard equation are fourthorder partialdifferential equations. The AllenCahn equation has analogies t o the vapor transport equation. These analogies can be formalized with variational methods [14].
444
18.4.2
CHAPTER 18: SPINODAL AND ORDERDISORDER TRANSFORMATIONS
AllenCahn: Critical Wavelength
A homogeneous freeenergy density function f ho"(r]) that has an orderdisorder transition similar to Fig. 18.6b has the form (18.32)
with local minima at r] = f 1 and a local maximum at r] = 0. Suppose that the system is initially uniform with an unstable disordered structure (i.e., r] = 0). For instance, the system may have been quenched from a hightemperature, disordered state. r] = f l represents the two equivalent equilibrium ordered variants. If the system is perturbed a small amount by a onedimensional perturbation in the zdirection, r](q= b ( t )sin(pz). Substituting this ordering perturbation into Eq. 18.26 and keeping the lowestorder terms in the amplification factor, b ( t ) , (18.33)
(18.35)
which is about four times larger than the interface width given by Eq. 18.15. Note that the amplification factor is a weakly increasing function of wavelength (asymptotically approaching 4M, fk; at long wavelengths). This predicts that the longest wavelengths should dominate the morphology. However, the probability of finding a longwavelength perturbation is a decreasing function of wavelength, and this also has an effect on the kinetics and morphology.
Figure 18.6: (a) Free energy vs. nonconserved order parameter, q, at point TO,^) where the ordered phttse is stable. (b) Corresponding phase diagram. The ciirve is the locus of orderdisorder transition temperatures above which q c q becomes zero. The equilibrium are the values that would be achieved at equilibrium in values of the order parameters, A$q, two equivalent variants lying on different sublattices and separated by an antiphase boundary as in Fig. 1 8 . 7 ~ .
18 5: COHERENCYSTRAIN EFFECTS
445
It is instructive to contrast the nature of the evolving earlystage morphologies predicted by Eq. 18.25 (for spinodal decomposition) and Eq. 18.26 (for ordering) and illustrated by the simulations in Figs. 18.4 and 18.5. In spinodal decomposition, the solution to the diffusion equation gives rise to a composition wave of wavelength A,, given by Eq. 18.31. The decomposed microstructure is a mixture of two phases with different compositions separated by diffuse interphase boundaries (see Fig. 18.7b). In continuous ordering, the solution to the diffusion equation gives rise to a wave of constant composition in which the order parameter varies. The theory does not predict that the order wave will have a “fastestgrowing” wavelengthrather, it indicates that the longer the wavelength, the faster the wave should develop. The evolving structure will consist of coexisting antiphase domains, one with positive 71 and one with negative q, separated by diffuse antiphase boundaries (see Fig. 1 8 . 7 ~ ) . The crystal symmetry changes that accompany orderdisorder transitions, discussed in Section 17.1.2, give rise to diffraction phenomena that allow the transitions to be studied quantitatively. In particular, the loss of symmetry is accompanied by the appearance of additional Bragg peaks, called superlattice reflections, and their intensities can be used to measure the evolution of order parameters. Random
(a)
Spinodal
L)(
Figure 18.7: Interfaces resulting from two types of continnous transformatioii. (a)Initial structure consisting of ratidoirily mixed alloy. (b) After spinodal decomposition. Regions of Rrich and Blean pliaves separated by diffuse interfaces formed as a result of longrange diffusion. ( c ) After an ordering transforniatiori. Equivalent ordering variants (domains) separated by two antiphase boundaries (APBs). The APBs result from A and B atomic rearrangement onto different sublattices in each domain.
18.5
COHERENCYSTRAIN EFFECTS
The driving force for transformation, @ in Eq. 18.22, was derived from the total Helmholtz free energy, and it was assumed that molar volume is independent
446
CHAPTER 18 SPINODAL AND ORDERDISORDER TRANSFORMATIONS
of concentration or structural order parameter. However, if an orderparameter fluctuation produces internal volume fluctuations, the differential expansions or contractions will produce internal strains, and additional strainenergy terms must be considered in the energetics leading to Eq. 18.21. In crystalline solutions, the developing interfaces are initially coherentstrains are continuous across interfaces. Unless defects such as anticoherency dislocations intervene, the interfaces will remain coherent until a critical stress is attained and the dislocations are nucleated. For smallstrain fluctuations, the system can be assumed to remain coherent and the resulting elastic coherency energy can be derivedeg For example, consider a binary alloy in which the stressfree molar volume is . linear expansion due to the composition a function of concentration, V ( C B )The change can be inferred from diffraction experiments under stressfree conditions ( Vegard's efect) and is characterized by Vegard's parameter, Q, [e.g., in cubic or isotropic crystals egFo = eU=O = E Z ~ O= Q,(C  CO)]. The assumption of coherency yy. implies that the total strain in the interfacial planes is zero. If a planar composition fluctuation perturbation of the form CB(Z) = co
+ sccospz
(18.36)
is postulated and the material is elastically isotropic, the total strain, ciYt, will correspond to the sum of the strain due to the composition change, E;=O, and the elastic strain due to the coherency stresses, (i.e., €tot = EU=O + E??). Then, 23 23 using the equations of linear isotropic elasticity, l o
ezp
€tot zZ 
1v
cospz
The elastic strains, e:?,
and
€tot  tot
xx  eyy
tot  exy
 tot  eyr
 E tot ,,
0
(18.37)
required to satisfy Eq. 18.37 are 2v cos p z 1u   Q c 6c cos p z
€elas
 cy,sc
€elas
 elas
€elas xy
 elas  €elas  Eyz  Z X
zZ
xx  fyy
(18.38)
=o
where u is Poisson's ratio. The corresponding elastic stresses are given by u = C E e l a s where C is the fourthrank stiffness tensor:
.
uzz= 0
E cos pz 1u uzy = uyz = uzz= 0
uxz= uyy = Cy,sc
(18.39)
9J.W. Cahn's early contributions to elastic coherency theory were motivated by his work on spinodal decomposition. His subsequent work with F. Larch6 created a rigorous thermodynamic foundation for coherency theory and stressed solids in general. A single volume, The Selected Works of John W. Cahn [15],contains papers that provide background and advanced reading for many topics in this textbook. This derivation follows from one in a publication included in that collection [16]. "Methods t o calculate coherency stresses in anisotropic materials, and an example calculation for cubic materials, have been published [17].
18.5: COHERENCYSTRAIN EFFECTS
447
where E is Young’s elastic modulus. Therefore, the elastic coherency strainenergy contribution to the total energy is
(18.40)
The final equality in Eq. 18.40 demonstrates that the contribution to coherency energy is independent of wavelength and direction. The coherency energy modifies Eqs. 18.21 and 18.22 as follows:
and the CahnHilliard equation linearized in C B , corresponding to Eq. 18.25, including coherency effects for elastic materials, is
where the first equality gives the isotropic elastic contribution explicitly and the second defines a general coherency modulus, Y ,for anisotropic materials [l,171. The coherency strain energy introduces an additional barrier to spinodal decomposition, which causes a shift on the temperaturecomposition phase diagram of the chemical spinodal, defined by d 2f h o ” / d c i = 0 , to the coherent spinodal, defined by
d2f dCi
+ 2aZY = 0
(18.43)
as in Fig. 18.8 Q
Coexistence
t
T
Figure 18.8:
Relation between chemical and coherent spinodals.
An additional effect of undercooling on the kinetics and microstructure of spinodal decomposition arises from the temperature dependence of d2f which
448
CHAPTER 18: SPINODAL AND ORDERDISORDER TRANSFORMATIONS
is approximately linear near the chemical spinodal temperature [l]. Because 2azY is always positive, the coherent spinodal lies below the chemical spinodal in the TX diagram. The depression AT of the coherent spinodal below the consolute point can be calculated (Eq. 18.43) for various systems. In AlZn, AT is approximately 20 K; in AuNi, it is approximately 400 K. In crystalline solids, only coherent spinodal decomposition is observed. The process of forming incoherent interfaces involves the generation of anticoherency dislocation structures and is incompatible with the continuous evolution of the phaseseparated microstructure characteristic of spinodal decomposition. Systems with elastic misfit may first transform by coherent spinodal decomposition and then, during the later stages of the process, lose coherency through the nucleation and capture of anticoherency interfacial dislocations [18].
18.5.1 Generalizations of the CahnHilliard and AllenCahn Equations Microstructural length scales that initially arise from uniform, but unstable, order parameters are readily understood by the perturbation analyses that lead to the amplification factor R(P) in Eqs. 18.28 and 18.34. When a system is anisotropic such as in a elastically coherent material, the perturbation’s behavior may depend on its direction with respect to the material’s symmetry axes. Orderparameter fluctuations can be generalized by introducing the wavevector p’ in a Fourier representation, (18.44) where

A(P)=
‘S
“(4 
(01
e
$.z
dz
(18.45)
8.
are the amplitudes associated with each Fourier mode Each Fourier mode is independent in a linear case. For example, when Eq. 18.44 is inserted into the linearized CahnHilliard equation, Eq. 18.42,
where
R ( 6 )= Mo
(%+ 2 horn
2 ~ Y(fi) 2
+ 2Kc1612) I6I2
(18.47)
Equation 18.47 indicates how the amplification factor depends on the mode p’ as well as the direction fi = through the anisotropy in Y . The p dependence of the amplification factor in an elastically isotropic crystal (for which R is independent of the direction of 6) is plotted for a temperature inside the coherent spinodal in Fig. 18.9. For p < &.it, the amplification factor R(P) > 0 and the system is unstablethat is, the composition waves in Eq. 18.44 will grow exponentially. The wavenumber pmsx,at which aR(p)/dp= 0, receives maximum amplification and will dominate the decomposed microstructure. Outside the coherent spinodal, where d2fhorn/dc~$2c$Y(fi) > 0, all wavenumbers will have R(P) < 0 and the system will be stable with respect to the growth of composition waves.
18.5: COHERENCYSTRAIN EFFECTS
449
Figure 18.9: Amplification factor vs. wavenumber plot for an elastically isotropic crystal at a temperature inside the coherent spinodal where d2fhorn/dcg 2cy: Y < 0.
+
The solution of Eq. 18.46 is
A ( 6 ,t ) = A($, O)eH("'
(18.48)
which is a generic form for linear perturbation analysis. At leas